PLASTICITY THEORY
Revised Edition (PDF)
Jacob Lubliner University of California at Berkeley
Copyright 1990, 2006 by Jacob Lubliner This book was previously published by Pearson Education, Inc.
Preface When I first began to plan this book, I thought that I would begin the preface with the words “The purpose of this little book is...” While I never lost my belief that small is beautiful, I discovered that it is impossible to put together a treatment of a field as vast as plasticity theory between the covers of a truly “little” book and still hope that it will be reasonably comprehensive. I have long felt that a modern book on the subject — one that would be useful as a primary reference and, more importantly, as a textbook in a graduate course (such as the one that my colleague Jim Kelly and I have been teaching) — should incorporate modern treatments of constitutive theory (including thermodynamics and internal variables), largedeformation plasticity, and dynamic plasticity. By no coincidence, it is precisely these topics — rather than the traditional study of elasticplastic boundaryvalue problems, slipline theory and limit analysis — that have been the subject of my own research in plasticity theory. I also feel that a basic treatment of plasticity theory should contain at least introductions to the physical foundations of plasticity (and not only that of metals) and to numerical methods — subjects in which I am not an expert. I found it quite frustrating that no book in print came even close to adequately covering all these topics. Out of necessity, I began to prepare class notes to supplement readings from various available sources. With the aid of contemporary wordprocessing technology, the class notes came to resemble book chapters, prompting some students and colleagues to ask, “Why don’t you write a book?” It was these queries that gave me the idea of composing a “little” book that would discuss both the topics that are omitted from most extant books and, for the sake of completeness, the conventional topics as well. Almost two years have passed, and some 1.2 megabytes of disk space have been filled, resulting in over 400 pages of print. Naively perhaps, I still hope that the reader approaches this overgrown volume as though it were a little book: it must not be expected, despite my efforts to make it comprehensive, to be exhaustive, especially in the sections dealing with applications; I have preferred to discuss just enough problems to highlight various facets of any topic. Some ofttreated topics, such as rotating disks, are not touched at iii
iv
Preface
all, nor are such general areas of current interest as micromechanics (except on the elementary, qualitative level of dislocation theory), damage mechanics (except for a presentation of the general framework of internalvariable modeling), or fracture mechanics. I had to stop somewhere, didn’t I? The book is organized in eight chapters, covering major subject areas; the chapters are divided into sections, and the sections into topical subsections. Almost every section is followed by a number of exercises. The order of presentation of the areas is somewhat arbitrary. It is based on the order in which I have chosen to teach the field, and may easily be criticized by those partial to a different order. It may seem awkward, for example, that constitutive theory, both elastic and inelastic, is introduced in Chapter 1 (which is a general introduction to continuum thermomechanics), interrupted for a survey of the physics of plasticity as given in Chapter 2, and returned to with specific attention to viscoplasticity and (finally!) rateindependent plasticity in Chapter 3; this chapter contains the theory of yield criteria, flow rules, and hardening rules, as well as uniqueness theorems, extremum and variational principles, and limitanalysis and shakedown theorems. I believe that the book’s structure and style are sufficiently loose to permit some juggling of the material; to continue the example, the material of Chapter 2 may be taken up at some other point, if at all. The book may also be criticized for devoting too many pages to concepts of physics and constitutive theory that are far more general than the conventional constitutive models that are actually used in the chapters presenting applications. My defense against such criticisms is this: I believe that the physics of plasticity and constitutive modeling are in themselves highly interesting topics on which a great deal of contemporary research is done, and which deserve to be introduced for their own sake even if their applicability to the solution of problems (except by means of highpowered numerical methods) is limited by their complexity. Another criticism that may, with some justification, be leveled is that the general formulation of continuum mechanics, valid for large as well as small deformations and rotations, is presented as a separate topic in Chapter 8, at the end of the book rather than at the beginning. It would indeed be more elegant to begin with the most general presentation and then to specialize. The choice I finally made was motivated by two factors. One is that most of the theory and applications that form the bulk of the book can be expressed quite adequately within the smalldeformation framework. The other factor is pedagogical: it appears to me, on the basis of long experience, that most students feel overwhelmed if the new concepts appearing in largedeformation continuum mechanics were thrown at them too soon. Much of the material of Chapter 1 — including the mathematical fundamentals, in particular tensor algebra and analysis — would normally be covered in a basic course in continuum mechanics at the advanced under
Preface
v
graduate or firstyear graduate level of a North American university. I have included it in order to make the book more or less selfcontained, and while I might have relegated this material to an appendix (as many authors have done), I chose to put it at the beginning, if only in order to establish a consistent set of notations at the outset. For more sophisticated students, this material may serve the purpose of review, and they may well study Section 8.1 along with Sections 1.2 and 1.3, and Section 8.2 along with Sections 1.4 and 1.5. The core of the book, consisting of Chapters 4, 5, and 6, is devoted to classical quasistatic problems of rateindependent plasticity theory. Chapter 4 contains a selection of problems in contained plastic deformation (or elasticplastic problems) for which analytical solutions have been found: some elementary problems, and those of torsion, the thickwalled sphere and cylinder, and bending. The last section, 4.5, is an introduction to numerical methods (although the underlying concepts of discretization are already introduced in Chapter 1). For the sake of completeness, numerical methods for both viscoplastic and (rateindependent) plastic solids are discussed, since numerical schemes based on viscoplasticity have been found effective in solving elasticplastic problems. Those who are already familiar with the material of Sections 8.1 and 8.2 may study Section 8.3, which deals with numerical methods in largedeformation plasticity, immediately following Section 4.5. Chapters 5 and 6 deal with problems in plastic flow and collapse. Chapter 5 contains some theory and some “exact” solutions: Section 5.1 covers the general theory of plane plastic flow and some of its applications, and Section 5.2 the general theory of plates and the collapse of axisymmetrically loaded circular plates. Section 5.3 deals with plastic buckling; its placement in this chapter may well be considered arbitrary, but it seems appropriate, since buckling may be regarded as another form of collapse. Chapter 6 contains applications of limit analysis to plane problems (including those of soil mechanics), beams and framed structures, and plates and shells. Chapter 7 is an introduction to dynamic plasticity. It deals both with problems in the dynamic loading of elastic–perfectly plastic structures treated by an extension of limit analysis, and with wavepropagation problems, onedimensional (with the significance of rate dependence explicitly discussed) and threedimensional. The content of Chapter 8 has already been mentioned. As the knowledgeable reader may see from the foregoing survey, a coherent course may be built in various ways by putting together selected portions of the book. Any recommendation on my part would only betray my own prejudices, and therefore I will refrain from making one. My hope is that those whose orientation and interests are different from mine will nonetheless find this wouldbe “little book” useful. In shaping the book I was greatly helped by comments from some out
vi
Preface
standing mechanicians who took the trouble to read the book in draft form, and to whom I owe a debt of thanks: Lallit Anand (M. I. T.), Satya Atluri (Georgia Tech), Maciej Bieniek (Columbia), Michael Ortiz (Brown), and Gerald Wempner (Georgia Tech). An immeasurable amount of help, as well as most of the inspiration to write the book, came from my students, current and past. There are too many to cite by name — may they forgive me — but I cannot leave out Vassilis Panoskaltsis, who was especially helpful in the writing of the sections on numerical methods (including some sample computations) and who suggested useful improvements throughout the book, even the correct spelling of the classical Greek verb from which the word “plasticity” is derived. Finally, I wish to acknowledge Barbara Zeiders, whose thoroughly professional copy editing helped unify the book’s style, and Rachel Lerner and Harry Sices, whose meticulous proofreading found some needles in the haystack that might have stung the unwary. Needless to say, the ultimate responsibility for any remaining lapses is no one’s but mine. A note on crossreferencing: any reference to a number such as 3.2.1, without parentheses, is to a subsection; with parentheses, such as (4.3.4), it is to an equation.
Addendum: Revised Edition Despite the proofreaders’ efforts and mine, the printed edition remained plagued with numerous errors. In the fifteen years that have passed I have managed to find lots of them, perhaps most if not all. I have also found it necessary to redo all the figures. The result is this revised edition.
Contents Chapter 1: Introduction to Continuum Thermomechanics Section 1.1 Mathematical Fundamentals 1.1.1 1.1.2 1.1.3 1.1.4
Notation Cartesian Tensors Vector and Tensor Calculus Curvilinear Coordinates
Section 1.2 Continuum Deformation 1.2.1 1.2.2 1.2.3 1.2.4
Displacement Strain Principal Strains Compatibility Conditions
Section 1.3 Mechanics of Continuous Bodies 1.3.1 1.3.2 1.3.3 1.3.4 1.3.5
Introduction Stress Mohr’s Circle Plane Stress BoundaryValue Problems
Section 1.4 Constitutive Relations: Elastic 1.4.1 Energy and Thermoelasticity 1.4.2 Linear Elasticity 1.4.3 Energy Principles vii
1 1 3 6 9
14 14 15 21 23
26 26 29 33 35 36
44 44 49 54
viii
Contents
Section 1.5 Constitutive Relations: Inelastic 1.5.1 1.5.2 1.5.3 1.5.4
Inelasticity Linear Viscoelasticity Internal Variables: General Theory Flow Law and Flow Potential
59 59 61 65 69
Chapter 2: The Physics of Plasticity Section 2.1 Phenomenology of Plastic Deformation 2.1.1 Experimental StressStrain Relations 2.1.2 Plastic Deformation 2.1.3 Temperature and Rate Dependence
Section 2.2 Crystal Plasticity 2.2.1 Crystals and Slip 2.2.2 Dislocations and Crystal Plasticity 2.2.3 Dislocation Models of Plastic Phenomena
Section 2.3 Plasticity of Soils, Rocks and Concrete 2.3.1 Plasticity of Soil 2.3.2 “Plasticity” of Rock and Concrete
75 76 80 85 89 89 94 100 103 104 108
Chapter 3: Constitutive Theory Section 3.1 Viscoplasticity 3.1.1 InternalVariable Theory of Viscoplasticity 3.1.2 Transition to RateIndependent Plasticity 3.1.3 Viscoplasticity Without a Yield Surface
Section 3.2 RateIndependent Plasticity 3.2.1 Flow Rule and WorkHardening 3.2.2 MaximumDissipation Postulate and Normality 3.2.3 StrainSpace Plasticity
Section 3.3 Yield Criteria, Flow Rules and Hardening Rules 3.3.1 Introduction
111 111 116 118 122 122 127 130 135 135
Contents 3.3.2 3.3.3 3.3.4 3.3.5
ix Yield Criteria Independent of the Mean Stress Yield Criteria Dependent on the Mean Stress Yield Criteria Under Special States of Stress or Deformation Hardening Rules
Section 3.4 Uniqueness and Extremum Theorems 3.4.1 Uniqueness Theorems 3.4.2 Extremum and Variational Principles 3.4.3 Rigid–Plastic Materials
Section 3.5 LimitAnalysis and Shakedown Theorems 3.5.1 Standard LimitAnalysis Theorems 3.5.2 Nonstandard LimitAnalysis Theorems 3.5.3 Shakedown Theorems
137 141 144 146
152 152 154 159
162 162 168 170
Chapter 4: Problems in Contained Plastic Deformation Section 4.1 Elementary Problems 4.1.1 4.1.2 4.1.3 4.1.4
Introduction: Statically Determinate Problems ThinWalled Circular Tube in Torsion and Extension ThinWalled Cylinder Under Pressure and Axial Force Statically Indeterminate Problems
Section 4.2 Elastic–Plastic Torsion 4.2.1 The Torsion Problem 4.2.2 Elastic Torsion 4.2.3 Plastic Torsion
Section 4.3 The ThickWalled Hollow Sphere and Cylinder 4.3.1 4.3.2 4.3.3 4.3.4 4.3.5
Elastic Hollow Sphere Under Internal and External Pressure Elastic–Plastic Hollow Sphere Under Internal Pressure Thermal Stresses in an Elastic–Plastic Hollow Sphere Hollow Cylinder: Elastic Solution and Initial Yield Pressure Elastic–Plastic Hollow Cylinder
177 177 178 181 184
189 189 191 194
205 206 208 213 216 220
x
Contents
Section 4.4 Elastic–Plastic Bending 4.4.1 Pure Bending of Prismatic Beams 4.4.2 Rectangular Beams Under Transverse Loads 4.4.3 PlaneStrain Pure Bending of Wide Beams or Plates
Section 4.5 Numerical Methods 4.5.1 Integration of Rate Equations 4.5.2 The FiniteElement Method 4.5.3 FiniteElement Methods for Nonlinear Continua
229 229 239 245
250 251 256 262
Chapter 5: Problems in Plastic Flow and Collapse I: Theories and “Exact” Solutions Introduction
275
Section 5.1 Plane Problems
276 277 287 291
5.1.1 SlipLine Theory 5.1.2 Simple SlipLine Fields 5.1.3 MetalForming Problems
Section 5.2 Collapse of Circular Plates 5.2.1 Introduction to Plate Theory 5.2.2 Elastic Plates 5.2.3 Yielding of Plates
Section 5.3 Plastic Buckling 5.3.1 Introduction to Stability Theory 5.3.2 Theories of the Effective Modulus 5.3.3 Plastic Buckling of Plates and Shells
298 299 303 308
313 314 319 326
Chapter 6: Problems in Plastic Flow and Collapse II: Applications of Limit Analysis Introduction
337
Contents
xi
Section 6.1 Limit Analysis of Plane Problems 6.1.1 Blocks and Slabs with Grooves or Cutouts 6.1.2 Problems in Bending 6.1.3 Problems in Soil Mechanics
Section 6.2 Beams Under Combined Stresses 6.2.1 6.2.2 6.2.3 6.2.4
Generalized Stress Extension and Bending Combined Extension, Bending and Torsion Bending and Shear
Section 6.3 Limit Analysis of Trusses, Beams and Frames 6.3.1 6.3.2 6.3.3 6.3.4
Trusses Beams Limit Analysis of Frames Limit Design of Frames
Section 6.4 Limit Analysis of Plates and Shells 6.4.1 Limit Analysis of Plates 6.4.2 Limit Analysis of Shells: Theory 6.4.3 Limit Analysis of Shells: Examples
338 338 341 347
355 355 358 364 369
374 374 380 385 390
398 398 404 407
Chapter 7: Dynamic Problems Section 7.1 Dynamic Loading of Structures 7.1.1 Introduction 7.1.2 Dynamic Loading of Beams 7.1.3 Dynamic Loading of Plates and Shells
Section 7.2 OneDimensional Plastic Waves 7.2.1 7.2.2 7.2.3 7.2.4
Theory of OneDimensional Waves Waves in Elastic–Plastic bars Rate Dependence Application of the Method of Characteristics
417 417 419 425
434 434 438 446 448
xii
Contents
Section 7.3 ThreeDimensional Waves 7.3.1 Theory of Acceleration Waves 7.3.2 Special Cases
452 453 459
Chapter 8: LargeDeformation Plasticity Section 8.1 LargeDeformation Continuum Mechanics 8.1.1 Continuum Deformation 8.1.2 Continuum Mechanics and Objectivity
Section 8.2 LargeDeformation Constitutive Theory 8.2.1 8.2.2 8.2.3 8.2.4
Thermoelasticity Inelasticity: Kinematics Inelasticity: Thermomechanics Yield Condition and Flow Rule
Section 8.3 Numerical Methods in LargeDeformation Plasticity 8.3.1 RateBased Formulations 8.3.2 “Hyperelastic” Numerical Methods
465 465 473 478 478 480 485 487
491 492 496
References
501
Index
517
Chapter 1
Introduction to Continuum Thermomechanics Section 1.1 1.1.1.
Mathematical Fundamentals
Notation
Solid mechanics, which includes the theories of elasticity and plasticity, is a broad discipline, with experimental, theoretical, and computational aspects, and with a twofold aim: on the one hand, it seeks to describe the mechanical behavior of solids under conditions as general as possible, regardless of shape, interaction with other bodies, field of application, or the like; on the other hand, it attempts to provide solutions to specific problems involving stressed solid bodies that arise in civil and mechanical engineering, geophysics, physiology, and other applied disciplines. These aims are not in conflict, but complementary: some important results in the general theory have been obtained in the course of solving specific problems, and practical solution methods have resulted from fundamental theoretical work. There are, however, differences in approach between workers who focus on one or the other of the two goals, and one of the most readily apparent differences is in the notation used. Most of the physical concepts used in solid mechanics are modeled by mathematical entities known as tensors. Tensors have representations through components with respect to specific frames or coordinate systems (a vector is a kind of tensor), but a great deal can be said about them without reference to any particular frame. Workers who are chiefly interested in the solution of specific problems — including, notably, engineers — generally use a system of notation in which the various components of tensors appear explicitly. This system, which will here be called “engineering” notation, has as one of its advantages familiarity, since it is the one that is gener1
2
Chapter 1 / Introduction to Continuum Thermomechanics
ally used in undergraduate “strength of materials” courses, but it is often cumbersome, requiring several lines of long equations where other notations permit one short line, and it sometimes obscures the mathematical nature of the objects and processes involved. Workers in constitutive theory tend to use either one of several systems of “direct” notation that in general use no indices (subscripts and superscripts), such as Gibbs’ dyadic notation, matrix notation, and a combination of the two, or the socalled indicial notation in which the use of indices is basic. The indices are used to label components of tensors, but with respect to an arbitrary rather than a specific frame. Indicial notation is the principal system used in this book, although other systems are used occasionally as seems appropriate. In particular, “engineering” notation is used when the solutions to certain specific problems are discussed, and the matrixbased direct notation is used in connection with the study of large deformation, in which matrix multiplication plays an important part. Assuming the reader to be familiar with vectors as commonly taught in undergraduate engineering schools, we introduce indicial notation as follows: for Cartesian coordinates (x, y, z) we write (x1 , x2 , x3 ); for unit vectors (i, j, k) we write (e1 , e2 , e3 ); for the components (ux , uy , uz ) of a vector u we write (u1 , u2 , u3 ). X The summation convention is defined as follows: the symbol may i
be omitted (i.e., it is implied) if the summation (dummy) index (say i) appears exactly twice in each term of a sum. Example: ai bi = a1 b1 + a2 b2 + a3 b3 . The Kronecker delta is defined as (
δij =
1 if i = j 0 if i 6= j
)
= δji .
The LeviCivita “e” tensor or permutation tensor is defined as eijk =
1 if ijk = 123, 231, 312 −1 if ijk = 321, 213, 132 0 otherwise.
There is a relation between the “e” tensor and the Kronecker delta known as the edelta identity: eijk elmk = δil δjm − δim δjl . The fundamental operations of threedimensional vector algebra, presented in indicial and, where appropriate, in direct notation, are as follows.
Section 1.1 / Mathematical Preliminaries
3
Decomposition: u = ui ei . (The position vector in x1 x2 x3 space is denoted x = xi ei .) Scalar (dot) product between unit vectors: ei · ej = δij (orthonormality). Projection: ei · u = ei · ej uj = δij uj = ui . Scalar (dot) product between any two vectors: u · v = ui ei · ej vj = ui vi . Vector (cross) product between unit vectors: ei × ej = eijk ek . Vector (cross) product between any two vectors: u × v = ei eijk uj vk . Scalar triple product: u · (v × w) = (u × v) · w = eijk ui vj wk . Note that the parentheses in the direct notation for the scalar triple product can be omitted without ambiguity, since a product of the form (u · v) × w has no meaning. The notation for matrices is as follows. A matrix with entries αij , where i is the row index and j is the column index, is denoted [αij ] or α. The transpose of α is the matrix [αji ], also denoted αT . The determinant of α is denoted det α, and the inverse of α is α−1 , so that α α−1 = α−1 α = I, where I = [δij ] is the unit matrix or identity matrix .
1.1.2.
Cartesian Tensors
Coordinate Transformation Since our aim is to be able to make statements about physical behavior independently of any choice of coordinate axes, let us see what the relation is between two sets of axes. Limiting ourselves to Cartesian coordinate systems, let us consider a set of axes (xi ), with the corresponding set of unit vectors (ei ) (also known as the basis of the coordinate system), and another set (x∗i ) with the basis (e∗i ). If βij is the cosine of the angle between the x∗i axis and the xj axis, then e∗i · ej = βij . According to this equation, βij is both the xj component of e∗i and the x∗i component of ej , so that e∗i = βij ej and ei = βji e∗j . For any vector u = ui ei = u∗i e∗i , u∗i = βik uk ,
ui = βji u∗j .
4
Chapter 1 / Introduction to Continuum Thermomechanics
If the free index i in the second equation is replaced by k and its righthand side is substituted for uk in the first equation, then u∗i = βik βjk u∗j . Similarly, ui = βki βkj uj . Since u∗i = δij u∗j and ui = δij uj , and since the vector u is arbitrary, it follows that βik βjk = βki βkj = δij , that is, the matrix β = [βij ] is orthogonal . In matrix notation, β β T = β T β = I. The determinant of a matrix equals the determinant of its transpose, that is, det α = det αT , and the determinant of a product of matrices equals the product of the determinants, so that det(αβ) = det α det β. For an orthogonal matrix β, therefore, (det β)2 = det I = 1, or det β = ±1. If the basis (e∗i ) is obtained from (ei ) by a pure rotation, then β is called proper orthogonal , and det β = 1. An example of a proper orthogonal matrix is the matrix describing counterclockwise rotation by an angle θ about the x3 axis, as shown in Figure 1.1.1.
x∗2
x2 6
KA
cos θ sin θ 0 β = − sin θ cos θ 0 0 0 1
A A ∗ A θ * x1 A A A @ K θ @A  x1 @ A
[email protected] @ @ @ @ R x3 , x∗3 @
Figure 1.1.1. Example of a rotation represented by a proper orthogonal matrix.
Linear Operators An operator λ on the space of threedimensional vectors is simply a vectorvalued function of a vector variable: given a vector u, λ(u) uniquely defines another vector. λ is a linear operator if λ(au + bv) = aλ(u) + bλ(v), where a and b are any real numbers, and u and v are any vectors.
Section 1.1 / Mathematical Preliminaries
5
The preceding definitions are independent of any decomposition of the vectors involved. If the vectors are to be represented with respect to a basis (ei ), then the linear operator must also be so represented. The Cartesian components of a linear operator are defined as follows: If v = λ(u), then it follows from the definition of linearity that vi = ei · λ(ej uj ) = ei · λ(ej )uj = λij uj , def
where λij uj = ei · λ(ej ). Thus λ = [λij ] is the component matrix of λ with respect to the basis (ei ). In matrix notation we may write v = λ u, where u (v) is the column matrix whose entries are the components ui (vi ) of the vector u (v) with respect to the basis (ei ). In direct tensor notations it is also customary to omit parentheses: in Gibbs’ notation we would write v = λ · u, and in the matrixbased direct notation, v = λu. In a different basis (e∗i ), where e∗i = βij ej , the component matrix of λ is defined by λ∗ij = βik βjl λkl , or, in matrix notation, λ∗ = β λ β T . If λ∗ = λ, then λ is an isotropic or spherical operator. An example is the identity operator I, whose component matrix is I = [δij ]. The most general isotropic operator is cI, where c is any scalar. If the component matrix of a linear operator has a property which is not changed by transformation to a different basis, that is, if the property is shared by λ and λ∗ (for any β), then the property is called invariant. An invariant property may be said to be a property of the linear operator λ itself rather than of its component matrix in a particular basis. An example is transposition: if λ∗ = β λ β T , then λ∗T = β λT β T . Consequently we may speak of the transpose λT of the linear operator λ, and we may define its symmetric and antisymmetric parts: λS = 12 (λ + λT )
⇔
λSij = λ(ij) = 12 (λij + λji ),
λA = 12 (λ − λT )
⇔
1 λA ij = λ[ij] = 2 (λij − λji ).
If λA = 0 (i.e., λij = λji ), then λ is a symmetric operator. If λS = 0 (i.e., λij = −λji ), then λ is an antisymmetric operator.
Tensors A linear operator, as just defined, is also called a tensor . More generally, a tensor of rank n is a quantity T represented in a basis (ei ) by a component array Ti1 ...in (i1 , ..., in = 1, 2, 3) and in another basis (e∗i ) by the component array Ti∗1 ...in , where Ti∗1 ...in = βi1 k1 ...βin kn Tk1 ...kn .
6
Chapter 1 / Introduction to Continuum Thermomechanics
Thus a scalar quantity is a tensor of rank 0, a vector is a tensor of rank 1, and a linear operator is a tensor of rank 2. “Tensor” with rank unspecified is often used to mean a tensor or rank 2. The tensor whose component array is eijk is an isotropic tensor of rank 3. Tensors of rank 4 are found first in Section 1.4. An array whose elements are products of tensor components of rank m and n, respectively, represents a tensor of rank m + n. An important example is furnished by the tensor product of two vectors u and v (a dyad in the terminology of Gibbs), the tensor of rank 2 represented by u v T = [ui vj ] and denoted u ⊗ v, or more simply uv in the Gibbs notation. Thus an arbitrary tensor λ of rank two, whose components with respect to a basis (ei ) are λij , satisfies the equation λ = λij ei ⊗ ej . Clearly, (u⊗v)w = u(v·w); in the Gibbs notation both sides of this equation may be written as uv · w. An operation known as a contraction may be performed on a tensor of rank n ≥ 2. It consists of setting any two indices in its component array equal to each other (with summation implied). The resulting array, indexed by the remaining indices, if any (the “free indices”), represents a tensor of rank n − 2. For a tensor λ of rank 2, λii = tr λ is a scalar known as the trace of λ. A standard example is u · v = ui vi = tr (u ⊗ v). Note that if n > 2 then more than one contraction of the same tensor is possible, resulting in different contracted tensors; and, if n ≥ 4, then we can have multiple contractions. For example, if n = 4 then we can have a double contraction resulting in a scalar, and three different scalars are possible: Tiijj , Tijij , and Tijji . If u and v are vectors that are related by the equation ui = αij vj , then α necessarily represents a tensor α of rank 2. Similarly, if α and β are tensors of rank 2 related by αij = ρijkl βkl , then the array ρijkl represents a tensor ρ of rank four. The generalization of these results is known as the quotient rule.
1.1.3.
Vector and Tensor Calculus
A tensor field of rank n is a function (usually assumed continuously differentiable) whose values are tensors of rank n and whose domain is a region R in x1 x2 x3 space. The boundary of R is a closed surface denoted ∂R, and
Section 1.1 / Mathematical Preliminaries
7
the unit outward normal vector on ∂R will be denoted n. The partial derivative operator ∂/∂xi will be written more simply as ∂i . A very common alternative notation, which is used extensively here, is ∂i φ = φ,i . If φ is a tensor field of rank n, then the array of the partial derivatives of its components represents a tensor field of rank n + 1. The del operator is defined as ∇ = ei ∂i , and the Laplacian operator as P 2 ∇ = ∂i ∂i = i ∂ 2 /∂x2i . For a scalar field φ, the gradient of φ is the vector field defined by ∇φ = gradφ = ei φ,i . For a vector field v, we use ∇v to denote (∇ ⊗ v)T , that is, ∇v = vi ,j ei ⊗ ej , but this notation is not universal: many writers would call this (∇v)T . There is no ambiguity, however, when only the symmetric part of ∇v is used, or when the divergence of v is defined as the trace of ∇v: div v = ∇ · v = vi ,i . Similarly, the curl of v is defined unambiguously as curl v = ∇ × v = ei eijk vk ,j . For a tensor field φ of rank 2, we define ∇φ as represented by φjk ,i , and ∇ · φ = div φ = φjk ,j ek . These definitions are, again, not universal. The threedimensional equivalent of the fundamental theorem of calculus is Gauss’s theorem: Z
Z
φ,i dV = R
ni φ dS,
(1.1.1)
∂R
where φ is any differentiable field. The particular case where φ is replaced (on both sides of the equation, of course) by vi (the ith component of a vector field v), with summation under the integral signs implied, is known as the divergence theorem. This is the case we use most often. The twodimensional Gauss’s theorem refers to fields defined in an area A in the x1 x2 plane, bounded by a closed curve C on which an infinitesimal element of arc length is ds (positive when it is oriented counterclockwise). It is conventional to use Greek letters for indices whose range is 1, 2; thus the theorem reads Z I φ,α dA = nα φ ds. (1.1.2) A
C
8
Chapter 1 / Introduction to Continuum Thermomechanics
x2
dx2
3 n2 J n Jn1 dsJ J −dx1
x1
Figure 1.1.2. Normal vector to a plane curve Now suppose that the curve C is described parametrically by x1 = x1 (s), x2 = x2 (s). Then, as can be seen from Figure 1.1.2, n1 =
dx2 , ds
n2 = −
dx1 . ds
Thus, for any two functions uα (x1 , x2 ) (α = 1, 2), I
u1 dx1 = −
I
Z
I
I
u2 dx2 = C
u1 ,2 dA A
C
C
and
n2 u1 ds = −
Z
n1 u2 ds = C
u2 ,1 dA. A
Combining these two equations, we obtain Green’s lemma: I
Z
uα dxα = C
(u2 ,1 −u1 ,2 ) dA.
(1.1.3)
A
If there exists a continuously differentiable function φ(x1 , x2 ), defined in A, H H such that uα = φ,α , then uα dxα = dφ = 0 around any closed contour, so that u2 ,1 = u1 ,2 . The converse is also true (i.e., the last equality implies the existence of φ), provided that the area A is simply connected (i.e., contains no holes); otherwise additional conditions are required. The preceding result is known as the twodimensional integrability theorem and will be used repeatedly. There exists an extension of Green’s lemma to a curved surface S in x1 x2 x3 space, bounded by a (not necessarily plane) closed curve C parametrized by xi = xi (s), i = 1, 2, 3. This extension (derived from Gauss’s
Section 1.1 / Mathematical Preliminaries
9
theorem) is known as Stokes’ theorem and takes the form I
Z
ui dxi = C
S
ni eijk uk ,j dS.
(1.1.4)
Clearly, Green’s lemma represents the special case of Stokes’ theorem when n = e3 . From Stokes’ theorem follows the threedimensional integrability theorem: a field φ(x) such that u = ∇φ in a region R exists only if ∇×u = 0, or, equivalently, uj ,i = ui ,j . As in the twodimensional version, this last condition is also sufficient if R is simply connected.
1.1.4.
Curvilinear Coordinates
The study of tensor fields in curvilinear coordinates is intimately tied to differential geometry, and in many books and courses of study dealing with continuum mechanics it is undertaken at the outset. The traditional methodology is as follows: with a set of curvilinear coordinates ξ i (i = 1, 2, 3) such that the position of a point in threedimensional space is defined by x(ξ 1 , ξ 2 , ξ 3 ), the natural basis is defined as the ordered triple of vectors gi = ∂x/∂ξ i , so that dx = gi dξ i ; the summation convention here applies whenever the pair of repeated indices consists of one subscript and one superscript. The basis vectors are not, in general, unit vectors, nor are they necessarily mutually perpendicular, although it is usual for them to have the latter property. One can find, however, the dual basis (gi ) such that gi · gj = δij . A vector v may be represented as vi gi or as v i gi , where vi = v · gi and v i = v · gi are respectively the covariant and contravariant components of v. For tensors of higher rank one can similarly define covariant, contravariant, and several kinds of mixed components. The gradient of a tensor field is defined in terms of the socalled covariant derivatives of its components, which, except in the case of a scalar field, differ from the partial derivatives with respect to the ξ i because the basis vectors themselves vary. A central role is played by the metric tensor with components gij = gi · gj , having the property that dx · dx = gij dξ i dξ j . An alternative approach is based on the theory of differentiable manifolds (see, e.g., Marsden and Hughes [1983]). Curvilinear tensor analysis is especially useful for studying the mechanics of curved surfaces, such as shells; when this topic does not play an important part, a simpler approach is available, based on the socalled “physical” components of the tensors involved. In this approach mutually perpendicular unit vectors (forming an orthonormal basis) are used, rather than the natural and dual bases. We conclude this section by examining cylindrical and spherical coordinates in the light of this methodology.
Cylindrical Coordinates In the cylindrical coordinates (r, θ, z), where r =
q
x21 + x22 , θ = tan−1 (x2 /x1 ),
10
Chapter 1 / Introduction to Continuum Thermomechanics
and z = x3 , the unit vectors are er = e1 cos θ + e2 sin θ,
eθ = −e1 sin θ + e2 cos θ,
ez = e3 ,
so that
d d er = eθ , eθ = −er . dθ dθ Using the chain rule for partial derivatives, we may show the ∇ operator to be given by ∂ 1 ∂ ∂ ∇ = er + eθ + ez . (1.1.5) ∂r r ∂θ ∂z When this operator is applied to a vector field v, represented as v = vr er + vθ eθ + vz ez , the result may be written as 1 ∂ ∂ ∂ + eθ + ez ⊗ (vr er + vθ eθ + vz ez ) ∂r r ∂θ ∂z ∂vr ∂vθ ∂vz = er ⊗ er + eθ + ez ∂r ∂r ∂r ∂vr ∂vθ ∂vz 1 er + eθ vr + eθ − er vθ + ez +eθ ⊗ r ∂θ ∂θ ∂θ ∂vr ∂vθ ∂vz +ez ⊗ er + eθ + ez . ∂z ∂z ∂z
∇⊗v =
er
(1.1.6)
The trace of this secondrank tensor is the divergence of v: ∂vr 1 ∂vθ ∂vz ∇·v = + vr + + ; ∂r r ∂θ ∂z and when v = ∇u, the gradient of a scalar field, then this is 2
∇ u=
∂2 1 ∂ 1 ∂2 ∂2 + + + ∂r2 r ∂r r2 ∂θ2 ∂z 2
!
u.
Lastly, let us consider a symmetric secondrank tensor field λ = er ⊗ er λrr + (er ⊗ eθ + eθ ⊗ er )λrθ + eθ ⊗ eθ λθθ + (er ⊗ ez + ez ⊗ er )λrz + (eθ ⊗ ez + ez ⊗ eθ )λθz + ez ⊗ ez λzz ; its divergence — which we have occasion to use in Section 1.3 — is λrr − λθθ 1 ∂λrθ ∂λrz ∂λrr + + + ∂r r r ∂θ ∂z ∂λrθ 2λrθ 1 ∂λθθ ∂λθz + + + + eθ ∂r r r ∂θ ∂z ∂λrz λrz 1 ∂λθz ∂λzz + ez + + + . ∂r r r ∂θ ∂z
∇ · λ = er
(1.1.7)
Section 1.1 / Mathematical Preliminaries
11
Spherical Coordinates The spherical coordinates (r, θ, φ) are defined by r =
q
x21 + x22 + x23 ,
q
θ = tan−1 (x2 /x1 ), and φ = cot−1 x3 / x21 + x22 . The unit vectors are er = (e1 cos θ+e2 sin θ) sin φ+e3 cos φ, eφ = (e1 cos θ+e2 sin θ) cos φ−e3 sin φ, eθ = −e1 sin θ + e2 cos θ, so that
∂ ∂ ∂ er = eφ , eφ = −er , eθ = 0, ∂φ ∂φ ∂φ ∂ ∂ ∂ er = eθ sin φ, eφ = eθ cos φ, eθ = −er sin φ − eφ cos φ. ∂θ ∂θ ∂θ The ∇ operator is given by ∇ = er
∂ 1 ∂ 1 ∂ + eφ + eθ . ∂r r ∂φ r sin φ ∂θ
For a vector field v we accordingly have ∂vφ ∂vr ∂vθ ∇ ⊗ v = er ⊗ er + eφ + eθ ∂r ∂r ∂r vφ 1 ∂vφ vr 1 ∂vθ 1 ∂vr + eφ ⊗ er ∂φ − + + eφ + eθ r r r ∂φ r r ∂φ vθ 1 ∂vφ cot φ 1 ∂vr − + eφ − vθ + eθ ⊗ er r sin φ ∂θ r r sin φ ∂θ r vr cot φ 1 ∂vθ + + vφ , + eθ r sin φ ∂θ r r (1.1.8) so that ∂vr vr 1 ∂vφ cot φ 1 ∂vθ ∇·v = +2 + + vφ + , ∂r r r ∂φ r r sin φ ∂θ
∂ 2 u 2 ∂u 1 ∂ 2 u cot φ ∂u 1 ∂2u + + + + , ∂r2 r ∂r r2 ∂φ2 r2 ∂φ r2 sin2 φ ∂θ2 and, for a symmetric secondrank tensor field λ, ∇2 u =
2λrr − λφφ − λθθ + λrφ cot φ ∂λrr 1 ∂λrφ 1 ∂λrθ + + + ∂r r ∂φ r sin φ ∂θ r ∂λrφ 1 ∂λφφ 1 ∂λφθ + eφ + + ∂r r ∂φ r sin φ ∂θ λφφ cot φ − λθθ cot φ + 3λrφ + r 3λrθ + 2λφθ cot φ ∂λrθ 1 ∂λφθ 1 ∂λθθ + eθ + + + . ∂r r ∂φ r sin φ ∂θ r (1.1.9)
∇ · λ = er
12
Chapter 1 / Introduction to Continuum Thermomechanics
Exercises: Section 1.1 1. Show that (a) δii = 3 (b) δij δij = 3 (c) eijk ejki = 6 (d) eijk Aj Ak = 0 (e) δij δjk = δik (f) δij eijk = 0 2. Using indicial notation and the summation convention, prove that (s × t) · (u × v) = (s · u)(t · v) − (s · v)(t · u). 3. For the matrix
1 1 0 [aij ] = 1 2 2 , 0 2 3 calculate the values of (a) aii , (b) aij aij , (c) aij ajk when i = 1, k = 1 and when i = 1, k = 2. 4. Show that the matrix β=
12 25 3 5 16 25
9 25 4 − 5 12 25
−
4 5
0
3 5
is proper orthogonal, that is, β β T = β T β = I, and det β = 1. 5. Find the rotation matrix β describing the transformation composed of, first, a 90◦ rotation about the x1 axis, and second, a 45◦ rotation about the rotated x3 axis. 6. Two Cartesian bases, (ei ),√and (e∗i ) are given, with e∗1 = (2e1 + 2e2 + e3 )/3 and e∗2 = (e1 − e2 )/ 2. (a) Express e∗3 in terms of the ei . (b) Express the ei in terms of the e∗i .
Section 1.1 / Mathematical Preliminaries
13
(c) If v = 6e1 − 6e2 + 12e3 , find the vi∗ . 7. The following table shows the angles between the original axes xi and the transformed axes x∗i . x∗1 x∗2 x∗3
x1 135◦ 90◦ 45◦
x2 60◦ 45◦ 60◦
x3 120◦ 45◦ 120◦
(a) Find the transformation matrix β, and verify that it describes a rotation. (b) If a secondrank tensor λ has the following component matrix with the respect to the original axes,
3 −4 0 λ = −4 2 1
2 1 , 3
find its component matrix λ∗ with respect to the rotated axes. 8. (a) Use the chain rule of calculus to prove that if φ is a scalar field, then ∇φ is a vector field. (b) Use the quotient rule to prove the same result. 9. Using indicial notation, prove that (a) ∇×∇φ = 0 and (b) ∇·∇×v = 0. 10. If x = xi ei and r = x, prove that ∇2 (rn ) = n(n + 1)rn−2 . 11. If φ(x1 , x2 , x3 ) = aij xi xj , with aij constant, show that φ,i = (aij + aji )xj and φ,ij = aij + aji . 12. Show that ∇2 (φψ) = φ∇2 ψ + 2(∇φ) · (∇ψ) + ψ∇2 φ. 13. Use Gauss’s theorem to prove that, if V is the volume of a threeR dimensional region R, then V = 31 ∂R xi ni dS. 14. Verify Green’s lemma for the area A bounded by the square with corners at (0, 0), (a, 0), (a, a), (0, a), of u1 (x1 , x2 ) = 0 and u2 (x1 , x2 ) = bx1 , where b is a constant. 15. Find the natural basis (gi ) and the dual basis (gi ) (a) for cylindrical coordinates, with ξ 1 = r, ξ 2 = θ, and ξ 3 = z, and (b) for spherical coordinates, with ξ 1 = r, ξ 2 = φ, and ξ 3 = θ.
14
Chapter 1 / Introduction to Continuum Thermomechanics
16. Starting with the expression in Cartesian coordinates for the gradient operator ∇ and using the chain rule for partial derivatives, derive Equation (1.1.5).
Section 1.2 1.2.1.
Continuum Deformation
Displacement
The first application of the mathematical concepts introduced in Section 1.1 will now be to the description of the deformation of bodies that can be modeled as continua. A body is said to be modeled as a continuum if to any configuration of the body there corresponds a region R in threedimensional space such that every point of the region is occupied by a particle (material point) of the body. Any one configuration may be taken as the reference configuration. Consider a particle that in this configuration occupies the point defined by the vector r = xi ei . When the body is displaced, the same particle will occupy the point r∗ = x∗i ei . (Note that here the x∗i no longer mean the coordinates of the same point with respect to a rotated basis, as in the Section 1.1, but the coordinates of a different point with respect to the same basis.) The difference r∗ − r is called the displacement of the particle and will be denoted u. The reference position vector r will be used to label the given particle; the coordinates xi are then called Lagrangian coordinates. Consequently the displacement may be given as a function of r, u(r), and it forms a vector field defined in the region occupied by the body in the reference configuration. Now consider a neighboring particle labeled by r + ∆r. In the displaced configuration, the position of this point will be r∗ + ∆r∗ = r + ∆r + u(r + ∆r) (see Figure 1.2.1), so that ∆r∗ = ∆r + u(r + ∆r) − u(r), or, in indicial notation, ∆x∗i = ∆xi + ui (r + ∆r) − ui (r). . But if ∆r is sufficiently small, then ui (r + ∆r) − ui (r) = ui ,j (r)∆xj , the error in the approximation being such that it tends to zero faster than ∆r. It is conventional to replace ∆r by the infinitesimal dr, and to write the approximation as an equality. Defining the displacementgradient matrix α def by αij = ui ,j , we may write in matrix notation dx∗ = (I + α)dx.
Section 1.2 / Continuum Deformation
15
x2
BM u(r + ∆r) B j B ∆r CO BP ∗ 7 PPP C ∆r PP qC r + ∆r AK > A r A A u(r) 6 r∗ r∗ + ∆r∗ x3
x1
Figure 1.2.1. Displacement
1.2.2.
Strain
A body is said to undergo a rigidbody displacement if the distances between all particles remain unchanged; otherwise the body is said to be deformed . Let us limit ourselves, for the moment, to an infinitesimal neighborhood of the particle labeled by r; the deformation of the neighborhood may be measured by the extent to which the lengths of the infinitesimal vectors dr emanating from r change in the course of the displacement. The square of the length of dr∗ is dr∗ 2 = dr∗ · dr∗ = dx∗T dx∗ = dxT (I + αT )(I + α) x = dxT (I + 2E) x, where E = 12 (αT + α + αT α), or, in indicial notation, 1 Eij = (uj ,i +ui ,j +uk ,i uk ,j ), 2 which defines the symmetric secondrank tensor E, known as the Green– SaintVenant strain tensor and sometimes called the Lagrangian strain ten
16
Chapter 1 / Introduction to Continuum Thermomechanics
sor .1 Clearly, E(r) describes the deformation of the infinitesimal neighborhood of r, and the tensor field E that of the whole body; E(r) = 0 for all r in R if and only if the displacement is a rigidbody one. The deformation of a region R is called homogeneous if E is constant. It is obvious that a necessary and sufficient condition for the deformation to be homogeneous is that the ui ,j are constant, or equivalently, that u varies linearly with r,
Infinitesimal Strain and Rotation We further define the tensor ε and ω, respectively symmetric and antisymmetric, by 1 1 εij = (uj ,i +ui ,j ), ωij = (ui ,j −uj ,i ), 2 2 so that ui ,j = εij + ωij , and 1 Eij = εij + (εik εjk − εik ωjk − ωik εjk + ωik ωjk ). 2 If εij  1 and ωij  1 for all i, j, then ε is an approximation to E and is known as the infinitesimal strain tensor . The displacement field is then called small or infinitesimal . Moreover, ω can then be defined as the infinitesimal rotation tensor : if ε = 0, then α = ω, and therefore dx∗ = (I + ω) x. Now . (I + ω)T (I + ω) = I + ω T + ω + ω T ω = I + ω T + ω = I; In other words, a matrix of the form I + ω, where ω is any antisymmetric matrix whose elements are small, is approximately orthogonal . The tensor ω, because of its antisymmetry, has only three independent components: ω32 = −ω23 , ω13 = −ω31 , and ω21 = −ω12 . Let these components be denoted θ1 , θ2 , and θ3 , respectively. Then it is easy to show the two reciprocal relations 1 θi = eijk ωkj , 2
ωik = eijk θj .
Since, moreover, eijk εjk = 0 because of the symmetry of ε, the first relation implies that 1 θi = eijk uk ,j , 2 or, in vector notation, 1 θ = ∇ × u. 2 1
As will be seen in Chapter 8, E is only one of several tensors describing finite deformation.
Section 1.2 / Continuum Deformation
17
In a rigidbody displacement, then, dui = eijk θj dxk , or du = θ ×dr. That is, θ is the infinitesimal rotation vector : its magnitude is the angle of rotation and its direction gives the axis of rotation. Note that ∇ · θ = 0; a vector field with this property is called solenoidal . It must be remembered that a finite rotation is described by an orthogonal, not an antisymmetric, matrix. Since the orthogonality conditions are six in number, such a matrix is likewise determined by only three independent numbers, but it is not equivalent to a vector, since the relations among the matrix elements are not linear.
Significance of Infinitesimal Strain Components The study of finite deformation is postponed until Chapter 8. For now, let us explore the meaning of the components of the infinitesimal strain tensor ε. Consider, first, the unit vector n such that dr = ndr, where dr = dr; we find that . dr∗2 = dr∗ · dr∗ = (1 + 2Eij ni nj )dr2 = (1 + 2εij ni nj ) r2 . √ . . But for α small, 1 + 2α = 1 + α, so that dr∗ = (1 + εij ni nj ) r. Hence dr∗ − dr . = εij ni nj dr is the longitudinal strain along the direction n (note that the lefthand side is just the “engineering” definition of strain). Next, consider two infinitesimal vectors, dr(1) = e1 dr(1) and dr(2) = (1) (2) e2 dr(2) . In indicial notation, we have dxi = δi1 dr(1) and dxi = δi2 dr(2) . Obviously, dr(1) · dr(2) = 0. The displacement changes dr(1) to dr(1)∗ and dr(2) to dr(2)∗ , where (1)∗
= (δij + ui ,j ) xj
(2)∗
= (δij + ui ,j ) xj
dxi dxi
(1)
= (δi1 + ui ,1 ) r(1) ,
(2)
= (δi2 + ui ,2 ) r(2) ,
so that (1)∗
dr(1)∗ · dr(2)∗ = dxi But (1)∗
dr
(2)∗
· dr
(2)∗
dxi
. = (u2 ,1 +u1 ,2 ) r(1) dr(2) = 2ε12 dr(1) dr(2) .
π (1)∗ (2)∗ = dr dr cos − γ12 ,
2
where γ12 is the shear angle in the x1 x2 plane (Figure 1.2.2). Consequently, . 2ε12 = (1 + ε11 )(1 + ε22 )γ12 = γ12 for infinitesimal strains.
18
Chapter 1 / Introduction to Continuum Thermomechanics
x2
6 dr(2)
u
dr(2)∗ π − γ12 : + 2 y W dr(1)∗ *
dr(1)
x1
Figure 1.2.2. Shear angle Since the labeling of the axes is arbitrary, we may say in general that, for i 6= j, εij = 21 γij . Both the εij and γij , for i 6= j, are referred to as shear strains; more specifically, the former are the tensorial and the latter are the conventional shear strains. A state of strain that can, with respect to some axes, be represented by the matrix
0 1 ∗ ε = 2γ 0
γ 0 0 0 0 0
1 2
is called a state of simple shear with respect to those axes, and pure shear in general. It cannot be emphasized strongly enough that the tensor ε is an approximation to E, and therefore deserves to be called the infinitesimal strain tensor, only if both the deformation and rotation are infinitesimal, that is, if both ε and ω (or θ) are small compared to unity. If the rotation is finite, then the strain must be described by E (or by some equivalent finite deformation tensor, discussed further in Chapter 8) even if the deformation per se is infinitesimal. As an illustration, we consider a homogeneous deformation in which the x1 x3 plane is rotated counterclockwise about the x3 axis by a finite angle θ, while the the x2 x3 plane is rotated counterclockwise about the x3 axis by the slightly different angle θ − γ, with γ 1. Since all planes perpendicular to the x3 axis deform in the same way, it is sufficient to study the deformation of the x1 x2 plane, as shown in Figure 1.2.3. It is clear that, with respect to axes rotated by the angle θ, the deformation is just one of simple shear,
Section 1.2 / Continuum Deformation
19
x2
C C C θ−γ C C CCWC9 C C C C C M C θ C ?
x1
Figure 1.2.3. Infinitesimal shear strain with finite rotation and can be described by the infinitesimal strain matrix given above. With respect to the reference axes, we determine first the displacement of points originally on the x1 axis, u1 (x1 , 0, x3 ) = −(1 − cos θ)x1 ,
u2 (x1 , 0, x3 ) = sin θx1 ,
and that of points originally on the x2 axis, u1 (0, x2 , x3 ) = − sin(θ − γ)x2 ,
u2 (0, x2 , x3 ) = −[1 − cos(θ − γ)]x2 .
The latter can be linearized with respect to γ: u1 (0, x2 , x3 ) = −(sin θ −γ cos θ)x2 , u2 (0, x2 , x3 ) = −(1−cos θ −γ sin θ)x2 . Since the deformation is homogeneous, the displacement must be linear in x1 and x2 and therefore can be obtained by superposition: u1 (x1 , x2 , x3 ) = −(1 − cos θ)x1 − (sin θ − γ cos θ)x2 , u2 (x1 , x2 , x3 ) = sin θx1 − (1 − cos θ − γ sin θ)x2 . Knowing that u3 = 0, we can now determine the Green–SaintVenant strain tensor, and find, with terms of order γ 2 neglected,
0 1 E = 2γ 0
γ 0 0 0 , 0 0
1 2
that is, precisely the same form as obtained for the infinitesimal strain with respect to rotated axes. Moreover, the result is independent of θ. The reason
20
Chapter 1 / Introduction to Continuum Thermomechanics
is that E measures strain with respect to axes that are, in effect, fixed in the body. Further discussion of the description of finite deformation is postponed until Chapter 8.
Alternative Notations and Coordinate Systems The “engineering” notations for the Cartesian strain components are εx , εy , and εz for ε11 , ε22 , and ε33 , respectively, and γxy for γ12 , and so on. In cylindrical coordinates we find the strain components by taking the symmetric part of ∇ ⊗ u as given by Equation (1.1.6): ∂ur ur 1 ∂uθ ∂uz , εθ = + , εz = , ∂r r r ∂θ ∂z ∂uθ 1 ∂ur uθ ∂uz ∂ur 1 ∂uz ∂uθ γrθ = + − , γrz = + , γθz = + . ∂r r ∂θ r ∂r ∂z r ∂θ ∂z (1.2.1) In spherical coordinates we similarly find, from Equation (1.1.8), εr =
εr =
∂ur , ∂r
γrφ =
εφ =
1 ∂uφ ur + , r ∂φ r
∂uφ 1 ∂ur uφ + − , ∂r r ∂φ r γφθ =
εθ =
γrθ =
1 ∂uθ ur cot φ + + uφ , r sin φ ∂θ r r
∂uθ 1 ∂ur uθ + − , ∂r r sin φ ∂θ r
(1.2.2)
1 ∂uφ cot φ 1 ∂uθ + − uθ . r ∂φ r sin φ ∂θ r
Volumetric and Deviatoric Strain The trace of the strain tensor, εkk = ∇ · u, has a special geometric significance: it is the (infinitesimal) volumetric strain, defined as ∆V /V0 , where ∆V is the volume change and V0 the initial volume of a small neighborhood. An easy way to show this is to look at a unit cube (V0 = 1) whose edges parallel the coordinate axes. When the cube is infinitesimally deformed, the lengths of the edges change to 1 + ε11 , 1 + ε22 , and 1 + ε33 , respectively, . making the volume (1 + ε11 )(1 + ε22 )(1 + ε33 ) = 1 + εkk . The volumetric strain is also known as the dilatation. The total strain tensor may now be decomposed as εij = 31 εkk δij + eij . The deviatoric strain or strain deviator tensor e is defined by this equation. Its significance is that it describes distortion, that is, deformation without volume change. A state of strain with e = 0 is called spherical or hydrostatic.
Section 1.2 / Continuum Deformation
1.2.3.
21
Principal Strains
It is possible to describe any state of infinitesimal strain as a superposition of three uniaxial extensions or contractions along mutually perpendicular axes, that is, to find a set of axes x∗i such that, with respect to these axes, the strain tensor is described by
ε1 0 0 ∗ ε = 0 ε2 0 . 0 0 ε3 Let n be unit vector parallel to such an axis; then the longitudinal strain ¯ is any along n is εij ni nj . By hypothesis, the shear strains εij ni n ¯ j , where n unit vector perpendicular to n, are zero. Consequently the vector whose components are εij nj is parallel to n, and if its magnitude is ε, then εij nj = εni , or εij nj − εni = (εij − εδij )nj = 0. Then, in order that n 6= 0, it is necessary that det(ε − εI) = −ε3 + K1 ε2 + K2 ε + K3 = 0,
(1.2.3)
where K1 = εkk , K2 = 12 (εij εij − εii εkk ), and K3 = det ε are the socalled principal invariants of the tensor ε. Since Equation (1.2.3) is a cubic equation, it has three roots, which are the values of ε for which the assumption holds, namely ε1 , ε2 , and ε3 . Such roots are known in general as the eigenvalues of the matrix ε, and in the particular case of strain as the principal strains. The principal invariants have simple expressions in terms of the principal strains: K1 = ε1 + ε2 + ε3 , K2 = −(ε1 ε2 + ε2 ε3 + ε3 ε1 ), K3 = ε1 ε2 ε3 . To each εI (I = 1, 2, 3) there corresponds an eigenvector n(I) ; an axis directed along an eigenvector is called a principal axis of strain. We must remember, however, that a cubic equation with real coefficients need not have roots that are all real: it may be that one root is real and the other two are complex conjugates. It is important to show that the eigenvalues of a symmetric secondrank tensor — and hence the principal strains — are real (if they were not real, their physical meaning would be dubious). We can also show that the principal axes are mutually perpendicular. Theorem 1 . If ε is symmetric then the εI are real. Proof . Let ε1 = ε, ε2 = ¯ε, where the bar denotes the complex conjugate. (1) (2) Now, if ni = ni , then ni = n ¯ i . Since εij nj = εni , we have n ¯ i εij nj =
22
Chapter 1 / Introduction to Continuum Thermomechanics
ε¯ ni ni ; similarly, εij n ¯ j = ¯εn ¯ i , so that ni εij n ¯ j = ¯εn ¯ i ni . However, εij = εji ; consequently ni εij n ¯j = n ¯ i εij nj , so that (ε − ¯ε)¯ ni ni = 0. Since n ¯ i ni is, for any nonzero vector n, a positive real number, it follows that ε = ¯ε (i.e., ε is real). Theorem 2 . If ε is symmetric then the n(I) are mutually perpendicular. (1)
Proof . Assume that ε1 6= ε2 ; then εij nj (2)
(1)
(1)
(2)
But ni εij nj − ni εij nj
(1)
= ε 1 ni
(2)
and εij nj
(2)
= ε 2 ni .
(1) (2)
= 0 = (ε1 − ε2 )ni ni . Hence n(1) · n(2) = 0.
If ε1 = ε2 6= ε3 , then any vector perpendicular to n(3) is an eigenvector, so that we can choose two that are perpendicular to each other. If ε1 = ε2 = ε3 (hydrostatic strain), then every nonzero vector is an eigenvector; hence we can always find three mutually perpendicular eigenvectors. Q.E.D. If the eigenvectors n(i) are normalized (i.e., if their magnitudes are defined as unity), then we can always choose from among them or their negatives a righthanded triad, say l(1) , l(2) , l(3) , and we define Cartesian coordinates x∗i (i = 1, 2, 3) along them, then the direction cosines βij are given by l(i) · ej , so that the strain components with respect to the new axes are given by (i) (j) εij ∗ = lk ll εkl . But from the definition of the n(i) , we have (i)
(i)
(i)
ll εkl = εi δkl ll = εi lk
(no sum on i),
so that (i) (j)
ε∗ij = εi lk lk = εi δij or
(no sum on i),
ε1 0 0 def ε∗ = 0 ε2 0 = Λ. 0 0 ε3 The same manipulations can be carried out in direct matrix notation. (j) With the matrix Λ as just defined, and with L defined by Lij = li (so that T L = β ), the equations defining the eigenvectors can be written as εL = LΛ, and therefore ε∗ = βεβ T = LT εL = LT LΛ = Λ. If one of the basis vectors (ei ), say e3 , is already an eigenvector of ε, then ε13 = ε23 = 0, and ε33 is a principal strain, say ε3 . The remaining principal strains, ε1 and ε2 , are governed by the quadratic equation ε2 − (ε11 + ε22 )ε + ε11 ε22 − ε212 .
Section 1.2 / Continuum Deformation
23
This equation can be solved explicitly, yielding 1 1q ε1,2 = (ε11 + ε22 ) ± (ε11 − ε22 )2 + 4ε122 . 2 2 In the special case of simple shear, we have ε11 = ε22 = 0 and ε12 = 12 γ. Consequently ε1,2 = ± 21 γ. With respect to principal axes, the strain tensor is represented by 1 γ 0 0 2 ε∗ = 0 − 12 γ 0 , 0 0 0 that is, the strain can be regarded as the superposition of a uniaxial extension and a uniaxial contraction of equal magnitudes and along mutually perpendicular directions. Conversely, any strain state that can be so represented is one of pure shear.
1.2.4.
Compatibility Conditions
If a secondrank tensor field ε(x1 , x2 , x3 ) is given, it does not automatically follow that such a field is indeed a strain field, that is, that there exists a displacement field u(x1 , x2 , x3 ) such that εij = 21 (uj ,i +ui ,j ); if it does, then the strain field is said to be compatible. The determination of a necessary condition for the compatibility of a presumed strain field is closely related to the integrability theorem. Indeed, if there were given a secondrank tensor field α such that αji = uj ,i , then the condition would be just eikm αji ,k = 0. Note, however, that if there exists a displacement field u, then there also exists a rotation field θ such that εij + eijl θl = uj ,i . Consequently, the condition may also be written as eikm (εij + eijl θl ),k = 0. But eikm eijl θl ,k = (δjk δlm − δjm δkl )θl ,k = θm ,j , since θk ,k = 0. Therefore the condition reduces to eikm εij ,k = −θm ,j . The condition for a θ field to exist such that the last equation is satisfied may be found by again invoking the integrability theorem, namely, eikm ejln εij ,kl = 0.
(1.2.4)
The lefthand side of Equation (1.2.4) represents a symmetric secondrank tensor, called the incompatibility tensor , and therefore the equation represents six distinct component equations, known as the compatibility conditions. If the region R is simply connected, then the compatibility
24
Chapter 1 / Introduction to Continuum Thermomechanics
conditions are also sufficient for the existence of a displacement field from which the strain field can be derived. In a multiply connected region (i.e., a region with holes), additional conditions along the boundaries of the holes are required. Other methods of derivation of the compatibility conditions lead to the fourthrank tensor equation εij ,kl +εkl ,ij −εik ,jl −εjl ,ik = 0; the sufficiency proof due to Cesaro (see, e.g., Sokolnikoff [1956]) is based on this form. It can easily be shown, however, that only six of the 81 equations are algebraically independent, and that these six are equivalent to (1.2.4). A sufficiency proof based directly on (1.2.4) is due to TranCong [1985]. The algebraic independence of the six equations does not imply that they represent six independent conditions. Let the incompatibility tensor, whose components are defined by the lefthand side of (1.2.4), be denoted R. Then 1 Rmn ,n = eikm ejln εij ,kln = eikm ejln (ui ,jkln +uj ,ikln ) = 0, 2 regardless of whether (1.2.4) is satisfied, because eikm uj ,ikln = ejln ui ,jkln = 0. The identity Rmn ,n = 0 is known as the Bianchi formula (see Washizu [1958] for a discussion).
Compatibility in Plane Strain Plane strain in the x1 x2 plane is defined by the conditions εi3 = 0 and εij ,3 = 0 for all i, j. The strain tensor is thus determined by the twodimensional components εαβ (x1 , x2 ) (α, β = 1, 2), and the only nontrivial compatibility condition is the one corresponding to m = n = 3 in Equation (1.2.4), namely, eαγ3 eβδ3 εαβ ,γδ = 0. In terms of strain components, this equation reads ε11 ,22 +ε22 ,11 −2ε12 ,12 = 0, or, in engineering notation, ∂ 2 εx ∂ 2 εy ∂2γ + = , ∂y 2 ∂x2 ∂x∂y
(1.2.5)
where γ = γxy . Lastly, an alternative form in indicial notation is εαα ,ββ −εαβ ,αβ = 0.
(1.2.6)
It can easily be shown that, to within a rigidbody displacement, the only displacement field that is consistent with a compatible field of plane
Section 1.2 / Continuum Deformation
25
strain is one of plane displacement, in which u1 and u2 are functions of x1 and x2 only, and u3 vanishes identically. The conditions εi3 = 0 are, in terms of displacement components, u3 ,3 = 0,
u1 ,3 +u3 ,1 = 0,
u2 ,3 +u3 ,2 = 0,
leading to u3 = w(x1 , x2 ),
uα = u0α (x1 , x2 ) − x3 w,α .
The strain components are now εαβ = ε0αβ (x1 , x2 ) − x3 w,αβ , where ε0 is the strain derived from the plane displacement field u0 = u0α eα . The conditions εαβ ,3 = 0 require that w,αβ = 0, that is, w(x1 , x2 ) = ax1 + bx2 + c, where a, b and c are constants. The displacement field is thus the superposition of u0 and of −ax3 e1 − bx3 e2 + (ax1 + bx2 + c)e3 , the latter being obviously a rigidbody displacement. In practice, “plane strain” is synonymous with plane displacement.
Exercises: Section 1.2 1. For each of the following displacement fields, with γ 1, sketch the displaced positions in the x1 x2 plane of the points initially on the sides of the square bounded by x1 = 0, x1 = 1, x2 = 0, x2 = 1. (a) u = 21 γx2 e1 + 12 γx1 e2 (b) u = − 12 γx2 e1 + 21 γx1 e2 (c) u = γx1 e2 2. For each of the displacement fields in the preceding exercise, determine the matrices representing the finite (Green–SaintVenant) and infinitesimal strain tensors and the infinitesimal rotation tensor, as well as the infinitesimal rotation vector. 3. For the displacement field (a) of Exercise √ 1, determine the longitudinal strain along the direction (e1 + e2 )/ 2. 4. For the displacement field given in cylindrical coordinates by u = ar er + brz eθ + c sin θ ez , where a, b and c are constants, determine the infinitesimal strain components as functions of position in cylindrical coordinates.
26
Chapter 1 / Introduction to Continuum Thermomechanics 5. Determine the infinitesimal strain and rotation fields for the displacement field u = −w0 (x1 )x3 e1 + w(x1 )e3 , where w is an arbitrary continuously differentiable function. If w(x) = kx2 , find a condition on k in order that the deformation be infinitesimal in the region −h < x3 < h, 0 < x1 < l. 6. For the displacementgradient matrix
4 −1 α = 1 −4 4 0
0 2 × 10−3 , 6
determine (a) the strain and rotation matrices, (b) the volume strain and the deviatoric strain matrix, (c) the principal strain invariants K1 , K2 , K3 , (d) the principal strains and their directions. 7. For the displacement field u = α(−x2 x3 e1 +x1 x3 e2 ), determine (a) the strain and rotation fields, (b) the principal strains and their directions as functions of position. 8. For the plane strain field εx = Bxy,
εy = −νBxy,
γxy = (1 + ν)B(h2 − y 2 ),
where B, ν and h are constants, (a) check if the compatibility condition is satisfied; (b) if it is, determine the displacement field u(x, y), v(x, y) in 0 < x < L, −h < y < h such that u(L, 0) = 0, v(L, 0) = 0, and ∂v ∂u − (L, 0) = 0. ∂x ∂y
Section 1.3 1.3.1.
Mechanics of Continuous Bodies
Introduction
Global Equations of Motion Mechanics has been defined as the study of forces and motions. It is easy enough to define motion as the change in position of a body, in time, with respect to some frame of reference. The definition of force is more
Section 1.3 / Mechanics of Continuous Bodies
27
elusive, and has been the subject of much controversy among theoreticians, especially with regard to whether force can be defined independently of Newton’s second law of motion. An interesting method of definition is based on a thought experiment due to Mach, in which two particles, A and B, are close to each other but so far away from all other bodies that the motion of each one can be influenced only by the other. It is then found that there exist numbers mA , mB (the masses of the particles) such that the motions of the particles obey the relation mA aA = −mB aB , where a denotes acceleration. The force exerted by A on B can now be defined as FAB = mB aB , and FBA is defined analogously. If B, rather than being a single particle, is a set of several particles, then FAB is the sum of the forces exerted by A on all the particles contained in B, and if A is also a set of particles, then FAB is the sum of the forces exerted on B by all the particles in A. The total force F on a body B is thus the vector sum of all the forces exerted on it by all the other bodies in the universe. In reality these forces are of two kinds: longrange and shortrange. If B is modeled as a continuum occupying a region R, then the effect of the longrange forces is felt throughout R, while the shortrange forces act as contact forces on the boundary surface ∂R. Any volume element dV experiences a longrange force ρb dV , where ρ is the density (mass per unit volume) and b is a vector field (with dimensions of force per unit mass) called the body force. Any oriented surface element dS = n dS experiences a contact force t(n) dS, where t(n) is called the surface traction; it is not a vector field because it depends not only on position but also on the local orientation of the surface element as defined by the local value (direction) of n. If a denotes the acceleration field, then the global force equation of motion (balance of linear momentum) is Z
Z
Z
ρb dV + R
t(n) dS = ∂R
ρa dV.
(1.3.1)
R
When all moments are due to forces (i.e. when there are no distributed couples, as there might be in an electromagnetic field), then the global moment equation of motion (balance of angular momentum) is Z R
ρx × b dV +
Z ∂R
x × t(n) dS =
Z
ρx × a dV,
(1.3.2)
R
where x is the position vector. Equations (1.3.1)–(1.3.2) are known as Euler’s equations of motion, applied by him to the study of the motion of rigid bodies. If a body is represented as an assemblage of discrete particles, each governed by Newton’s laws of motion, then Euler’s equations can be derived from Newton’s laws. Euler’s equations can, however, be taken as axioms describing the laws of motion for extended bodies, independently of any particle structure. They
28
Chapter 1 / Introduction to Continuum Thermomechanics
are therefore the natural starting point for the mechanics of bodies modeled as continua.
Lagrangian and Eulerian Approaches The existence of an acceleration field means, of course, that the displacement field is timedependent. If we write u = u(x1 , x2 , x3 , t) and interpret the xi as Lagrangian coordinates, as defined in Section 1.2, then we have ¨ ; here v = u˙ is the velocity field, and the superposed dot simply a = v˙ = u denotes partial differentiation with respect to time at constant xi (called material time differentiation). With this interpretation, however, it must be agreed that R is the region occupied by B in the reference configuration, and similarly that dV and dS denote volume and surface elements measured in the reference configuration, ρ is the mass per unit reference volume, and t is force per unit reference surface. This convention constitutes the socalled Lagrangian approach (though Lagrange did not have much to do with it) to continuum mechanics, and the quantities associated with it are called Lagrangian, referential, or material (since a point (x1 , x2 , x3 ) denotes a fixed particle or material point). It is, by and large, the preferred approach in solid mechanics. In problems of flow, however — not only fluid flow, but also plastic flow of solids — it is usually more instructive to describe the motion of particles with respect to coordinates that are fixed in space — Eulerian or spatial coordinates. In this Eulerian approach the motion is described not by the displacement field u but by the velocity field v. If the xi are spatial coordinates, then the material time derivative of a function φ(x1 , x2 , x3 , t), defined as its time derivative with the Lagrangian coordinates held fixed, can be found by applying the chain rule to be ∂φ φ˙ = + vi φ,i . ∂t The material time derivative of φ is also known as its Eulerian derivative D and denoted φ. Dt If the displacement field is infinitesimal, as defined in the preceding section, then the distinction between Lagrangian and Eulerian coordinates can usually be neglected, and this will generally be done here until finite deformations are studied in Chapter 8. The fundamental approach is Lagrangian, except when problems of plastic flow are studied; but many of the equations derived are not exact for the Lagrangian formulation. Note, however, one point: because of the postulated constancy of mass of any fixed part of B, the product ρ dV is timeindependent regardless of whether ρ and dV are given Lagrangian or Eulerian readings; thus the relation d dt is exact.
Z
Z
ρψ dV = R
R
ρψ˙ dV
Section 1.3 / Mechanics of Continuous Bodies
1.3.2.
29
Stress
To determine how t depends on n, we employ the Cauchy tetrahedron illustrated in Figure 1.3.1.Assuming b, ρ, a and t(n) to depend continuously on x, we have, if the tetrahedron is sufficiently small, Z
x2
. ρb dV = ρb ∆V ;
p @ t(−e3 ) ∆A3 @ B n: t(n) ∆A * B
[email protected] @ r b p @ @p x1 b p
t(−e1 ) ∆A1
R
Z
. ρa dV = ρa ∆V ;
MBB
R
Z
. t(n) dS = t(n) ∆A
∂R
+
X
t(−ej ) ∆Aj
j
= [t(n) − tj nj ] ∆A,
t(−e2 ) ∆A2 x3
Figure 1.3.1. Cauchy tetrahedron def
where tj = − t(−ej ). Thus we have, approximately, t(n) − tj nj + ρ(b − a)
∆V . = 0. ∆A
This becomes exact in the limit as the tetrahedron shrinks to a point, i.e. ∆V /∆A → 0, so that t(n) = tj nj , def
that is, t(·) is a linear function of its argument. If we define σij = ei · tj , then ti (n) = σij nj , so that σ = [σij ] represents a secondrank tensor field called the stress tensor. Denoting this tensor by σ, the preceding equation may be rewritten in direct tensor notation as t(n) = σn. The force equation of motion (1.3.1) can now be written in indicial notation as Z Z Z ρbi dV + σij nj dS = ρai dV. R
∂R
R
By Gauss’s theorem we have Z
Z
σij nj dS = ∂R
σij ,j dV ; R
30
Chapter 1 / Introduction to Continuum Thermomechanics
therefore, Z
(σij ,j +ρbi − ρai ) dV = 0.
R
This equation, since it embodies a fundamental physical law, must be independent of how we define a given body and therefore it must be valid for any region R, including very small regions. Consequently, the integrand must be zero, and thus we obtain the local force equations of motion (due to Cauchy): σij ,j +ρbi = ρai . (1.3.3) When the relation between traction and stress is introduced into Equation (1.3.2), this equation becomes, in indicial notation, Z R
Z
ρeijk xj bk dV +
Z
∂R
eijk xj σkl nl dS =
R
ρeijk xj ak dV.
By Gauss’s theorem, Z
Z ∂R
xj σkl nl dS =
R
(xj σkl ),l dV
Z
= R
(δij σkl + xj σkl ,l ) dV
Z
= R
therefore
Z R
(σkj + xj σkl ,l ) dV ;
eijk [xj (ρbk + σkl ,l −ρak ) + σkj ]dV = 0,
which, as a result of (1.3.3), reduces to Z R
eijk σkj dV = 0.
Since this result, again, must be valid for any region R, it follows that eijk σkj = 0, or equivalently, σij = σji .
(1.3.4)
In words: the stress tensor is symmetric. In the usual “engineering” notation, the normal stresses σ11 , σ22 , and σ33 are designated σx , σy , and σz , respectively, while the shear stresses are written as τxy in place of σ12 , and so on. This notation is invariably used in conjunction with the use of x, y, z for the Cartesian coordinates and of ux , uy , and uz for the Cartesian components of a vector u, except that the components of the displacement vector are usually written u, v, w, and the bodyforce vector components are commonly written X, Y, Z rather than
Section 1.3 / Mechanics of Continuous Bodies
31
ρbx , and so on. Thus the local force equations of motion are written in engineering notation as ∂σx ∂τxy ∂τxz + + + X = ρax , ∂x ∂y ∂z and two similar equations. The equations in cylindrical coordinates are obtained from Equation (1.1.7), with the changes of notation selfexplanatory: ∂σr σr − σθ 1 ∂τrθ ∂τrz + + + + R = ρar , ∂r r r ∂θ ∂z ∂τrθ 2τrθ 1 ∂σθ ∂τθz + + + + Θ = ρaθ , ∂r r r ∂θ ∂z ∂τrz τrz 1 ∂τθz ∂σz + + + + Z = ρaz . ∂r r r ∂θ ∂z The corresponding equations in spherical coordinates are obtained from Equation (1.1.9): 2σr − σφ − σθ + τrφ cot φ ∂σr 1 ∂τrφ 1 ∂τrθ + + + + R = ρar , ∂r r ∂φ r sin φ ∂θ r σφ cot φ − σθ cot φ + 3τrφ ∂σφ 1 ∂τφθ + + + Φ = ρaφ , ∂φ r sin φ ∂θ r 3τrθ + 2τφθ cot φ ∂τrθ 1 ∂τφθ 1 ∂σθ + + + + Θ = ρaθ . ∂r r ∂φ r sin φ ∂θ r
Projected Stresses If n is an arbitrary unit vector, the traction t = σn has, in general, a component parallel to n and one perpendicular to n. These are the projected stresses, namely, normal stress : σ(n) = n · t(n) = σij ni nj , shear stress :
τ (n) =
p
t(n)2 − [σ(n)]2 ;
note that this is the magnitude of the shearstress vector τ (n) = t(n) − nσ(n) = n × (t × n).
Principal Stresses As in the case of strains, it is possible to find directions n such that τ (n) = 0, so that t(n) = σ(n)n, or σij nj − σni = (σij − σδij )nj = 0.
32
Chapter 1 / Introduction to Continuum Thermomechanics
Then, for n 6= 0, we need det(σ − σI) = −σ 3 + I1 σ 2 + I2 σ + I3 = 0, where I1 = σkk , I2 = 12 (σij σij − σii σkk ), and I3 = det σ are the principal invariants of σ. The principal stresses can now be defined exactly like the principal strains; by Theorem 1 of 1.2.31 they are real, and by Theorem 2 the principal axes of stress are mutually perpendicular. The principal invariants of stress can be expressed in the form I1 = σ1 + σ2 + σ3 , I2 = −(σ1 σ2 + σ2 σ3 + σ3 σ1 ), I3 = σ1 σ2 σ3 . The mean stress or hydrostatic stress is defined as σm = 31 I1 .
Stress Deviator def
The stress deviator or deviatoric stress tensor s is defined by sij = σij − σm δij . The principal invariants of the stress deviator are denoted J1 = skk , which vanishes identically, J2 (= 21 sij sij ), and J3 . The principal axes of s are the same as those of σ, and the principal deviatoric stresses are sI = σI − 13 I1 . J2 and J3 may be expressed in terms of the principal stresses through the principalstress differences σ1 − σ2 etc., namely, 1 J2 = [(σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 ], 6 J3 =
1 [(σ1 − σ2 )2 (σ1 − σ3 + σ2 − σ3 ) + (σ2 − σ3 )2 (σ2 − σ1 + σ3 − σ1 ) 27 +(σ3 − σ1 )2 (σ3 − σ2 + σ1 − σ2 )].
Octahedral Stresses Let the basis vectors (ei ) be directed along the principal axes, and suppose that n is one of the eight vectors 1 n = √ (±e1 ± e2 ± e3 ); 3 a regular octahedron can be formed with planes perpendicular to these vectors. The traction on such a plane (called an octahedral plane) is 1 t(n) = √ (±σ1 e1 ± σ2 e2 ± σ3 e3 ). 3 1
Any crossreference such as 1.2.3, not enclosed in parentheses, refers to a subsection, unless it is specified as a figure or a table. With parentheses, for example (1.2.3), the reference is to an equation.
Section 1.3 / Mechanics of Continuous Bodies
33
The normal stress is 1 1 σ(n) = (σ1 + σ2 + σ3 ) = I1 = σm (mean stress), 3 3 and the shear stress is given by [τ (n)]2
= = def
=
1 2 1 (σ + σ22 + σ32 ) − (σ1 + σ2 + σ3 )2 3 1 9 2 2 (σ + σ22 + σ32 − σ1 σ2 − σ2 σ3 − σ3 σ1 ) 9 1 2 τoct ,
where τoct is called the octahedral shear stress. By comparing the justderived result with the previously obtained expression for J2 in terms of the principal stresses, it can be shown that 2 2 τoct = J2 . 3
1.3.3.
(1.3.5)
Mohr’s Circle
Let the x3 axis coincide with the principal axis defined by σ3 , that is, let e3 = n(3) . Now any unit vector n that is perpendicular to this axis may be written as n = e1 cos θ + e2 sin θ. It follows that t(n) = e1 (σ11 cos θ + σ12 sin θ) + e2 (σ12 cos θ + σ22 sin θ), since σ13 = σ23 = 0, and σ(n) = σ11 cos2 θ + σ22 sin2 θ + 2σ12 sin θ cos θ, which will be designated σθ . By means of the trigonometric identities cos2 θ = 21 (1 + cos 2θ), sin2 θ = 12 (1 − cos 2θ), and 2 sin θ cos θ = sin 2θ, σθ may be rewritten as 1 1 σθ = (σ11 + σ22 ) + (σ11 − σ22 ) cos 2θ + σ12 sin 2θ. 2 2
(1.3.6)
The projected shearstress vector is τ (n) = [σ12 (cos2 θ − sin2 θ) + (σ22 − σ11 ) sin 2θ cos 2θ](−e1 sin θ + e2 cos θ); the quantity in brackets will be designated τθ , and clearly τθ  = τ (n), since the vector in parentheses is a unit vector. With the help of the trigonometric identities cos 2θ = cos2 θ − sin2 θ, sin 2θ = 2 sin 2θ cos 2θ, we may write 1 τθ = σ12 cos 2θ + (σ22 − σ11 ) sin 2θ. 2
(1.3.7)
34
Chapter 1 / Introduction to Continuum Thermomechanics
From Equation (1.3.7) we may obtain the principal directions n(1) and n(2) directly by finding the values of θ for which τθ vanishes, namely, those that satisfy 2σ12 tan 2θ = , (1.3.8) σ11 − σ22 unless σ12 and σ11 − σ22 are both zero, in which case τθ = 0 for all θ. In the general case, if θ1 is a solution of Equation (1.3.8) (so that n(1) = e1 cos θ1 + e2 sin θ1 ), then so is θ1 ± 21 π, showing the perpendicularity of nondegenerate principal directions. As is readily seen, however, dσθ /dθ = 2τθ . It follows that the principal stresses σ1 and σ2 are the extrema of σθ , one being the maximum and the other the minimum, again with the exception of the degenerate case in which σθ is constant. The principal stresses, with the numbering convention σ1 ≥ σ2 , are given by q 1 2 ; 1 σ1 , 2 = (σ11 + σ22 ) ± (σ11 − σ22 )2 + σ12 4 2 this convention is consistent with defining θ1 in such a way that cos 2θ1 = q
1 2 1 4
(σ11 − σ22 )
2 (σ11 − σ22 )2 + σ12
,
sin 2θ1 = q
σ12 1 4
2 (σ11 − σ22 )2 + σ12
,
so that σθ1 = σ1 . Using the justderived expressions for cos 2θ1 and sin 2θ1 and the trigonometric identities cos 2(θ − θ1 ) = cos 2θ cos 2θ1 + sin 2θ sin 2θ1 , sin 2(θ − θ1 ) = sin 2θ cos 2θ1 − sin 2θ1 cos 2θ, we may rewrite Equations (1.3.6)–(1.3.7) as 1 1 σθ = (σ1 + σ2 ) + (σ1 − σ2 ) cos 2(θ − θ1 ), (1.3.9) 2 2 1 τθ = − (σ1 − σ2 ) sin 2(θ − θ1 ). (1.3.10) 2 Equations (1.3.9)–(1.3.10) are easily seen to be the parametric representation of a circle, known as Mohr’s circle, in the σθ τθ plane, with its center at ( 21 (σ1 + σ2 ), 0) and with radius 21 (σ1 − σ2 ), a value (necessarily positive in view of the numbering convention) equal to the maximum of τθ . Note that this maximum occurs when sin 2(θ − θ1 ) = ±1, that is, when θ = θ1 ± 41 π. The significance of the angle θ1 , and other aspects of Mohr’s circle, can be seen from Figure 1.3.2. It can be shown that the maximum over all n (in three dimensions) of the projected shear stress τ (n) is just the largest of the three maxima of τθ found in the planes perpendicular to each of the principal directions. With no regard for any numbering convention for the principal stresses, we have 1 τmax = max τ (n) = max{σ1 − σ2 , σ2 − σ3 , σ1 − σ3 }. (1.3.11) n 2
Section 1.3 / Mechanics of Continuous Bodies
35
τθ 1 (σ1 −σ2 ) 2
(σ s 11 , σ12 ) 2θ s(σ , τ ) θ θ U 2θ1 σ2 x2 K θ1 ? K A σ1 A A * 1 A σ2 σ1 2 (σ1 +σ2 ) A A A A A σ1 s(σ22 , −σ12 ) A A AU − 21 (σ1 −σ2 ) σ2 x1
Figure 1.3.2. Mohr’s circle.
1.3.4.
Plane Stress
Plane stress is defined by the conditions σi 3 = 0 (i = 1, 2, 3) and σij ,3 = 0, so that the stress field is given by σαβ (x1 , x2 ) (α, β = 1, 2). The summation convention applies to Greek indices ranging over 1, 2. Consequently, the equilibrium equations without body force are σαβ ,β = 0, or (1) σ11 ,1 +σ12 ,2 = 0 and (2) σ12 ,1 +σ22 ,2 = 0, so that there exist functions φα (x1 , x2 ) (α = 1, 2) such that (1) σ11 = φ1 ,2 , σ12 = −φ1 ,1 , and (2) σ22 = φ2 ,1 , σ12 = −φ2 ,2 . Hence φ1 ,1 = φ2 ,2 , and therefore there exists a function Φ(x1 , x2 ) such that φ1 = Φ,2 , φ2 = Φ,1 . Thus σ11 = Φ,22 , σ22 = Φ,11 , σ12 = −Φ,12 , or, in twodimensional indicial notation, σαβ = δαβ Φ,γγ −Φ,αβ . The function Φ is known as the Airy stress function. In planestress problems described in “engineering” notation, the shear stress τxy = τyx is sometimes written simply as τ , and the relation between the stress components and the Airy stress function is accordingly written as σx =
∂2Φ ∂2Φ ∂2Φ , σ = , τ = − . y ∂y 2 ∂x2 ∂x∂y
σθ
36
1.3.5.
Chapter 1 / Introduction to Continuum Thermomechanics
BoundaryValue Problems
The standard boundaryvalue problem of solid mechanics is the following: find the fields u and σ throughout R if the given information consists of, first, the bodyforce field b throughout R, and second, boundary conditions on ∂R, namely, that at every point of ∂R there is a local basis (ei ) such that either ti (n) or ui is prescribed for each i, i = 1, 2, 3. It may be that ∂R consists of two parts, ∂Ru and ∂Rt , such that u is prescribed on the former and t on the latter. This is not the most general case, but it is often cited for convenience. The prescribed ti and ui will be denoted tai and uai , respectively. The boundary conditions may be written as ui = uai on ∂Ru , nj σij = tai on ∂Rt , (1.3.12) even if the boundary is not strictly divided into two parts; points at which both displacement and traction components are prescribed may be regarded as belonging to both ∂Ru and ∂Rt — in other words, ∂Ru and ∂Rt may be thought of as overlapping. The prescribed bodyforce field b and surface tractions tai are together known as the loads, while the generally unknown surface tractions ti at the points where the displacements ui are prescribed are called reactions. Whenever displacements are prescribed, the body is said to be subject to external constraints.1 There may, in addition, exist internal constraints which restrict the displacement field in the interior of R; an example is incompressibility, that is, the inability of a body or any part thereof to change its volume, expressed by εkk = ∇ · u = 0. A displacement field is called kinematically admissible if it is mathematically wellbehaved (for example, continuous and piecewise continuously differentiable) and obeys the external and internal constraints, if any. The boundaryvalue problem is called static if the data are independent of time and the acceleration is assumed to be zero. It is called quasistatic if the acceleration is neglected even though the data depend on time. In static or quasistatic boundaryvalue problems, the equations of motion (1.3.3) may be replaced by the equilibrium equations σij ,j +ρbi = 0.
(1.3.13)
A stress field σ that obeys the equilibrium equations (1.3.13) and the traction boundary conditions (1.3.12)2 is called statically admissible. If the acceleration is not assumed to vanish, then the problem is dynamic, and then 1 More specifically, these are holonomic external constraints. A constraint is nonholonomic if, for example, it is given by an inequality — a displacement component may be required to have less than (or greater than) a specified value. Such a constraint is called unilateral.
Section 1.3 / Mechanics of Continuous Bodies
37
additional data are required, namely, the initial conditions consisting of the displacement and velocity fields throughout R at the initial time.
Virtual Displacements A virtual displacement field is defined as the difference between two neighboring kinematically admissible displacement fields. In other words, it is a vector field δu which is such that, if u is a kinematically admissible displacement field, then so is u + δu. It is furthermore assumed that the virtual displacement field is infinitesimal, that is, δui ,j  1. Corresponding to a virtual displacement field δu we may define the virtual strain field δε by δεij = 21 (δuj ,i +δui ,j ). Note that the operator δ when applied to a field represents taking the difference between two possible fields and is therefore a linear operator which commutes with partial differentiation. Note further that if any displacement components are prescribed on any part of the boundary then the corresponding virtual displacement components vanish there, that is, δu = 0 on ∂Ru .
Virtual Work Given a set of loads and a virtual displacement field δu, we define the external virtual work as1 Z
Z
ρbi δui dV +
δW ext =
∂Rt
R
tai δui dS.
The internal virtual work is defined as Z
σij δεij dV.
δW int = R
Since σij = σji , we have σij δεij = σij δui ,j , and therefore σij δεij = (σij δui ),j −σij ,j δui . Using Gauss’s theorem, we obtain Z
δW int = ∂R
nj σij δui dS −
Z
σij ,j δui dV. R
Since, however, δui = 0 on ∂Ru , the surface integral may be restricted to ∂Rt . It follows that δW ext − δW int =
Z R
(σij ,j +ρbi ) δui dV −
Z ∂Rt
(nj σij − tai ) δui dS.
The righthand side vanishes for all virtual displacement fields δu if and only if the quantities multiplying δui in both integrals vanish identically, that 1
A note on notation: we write δW instead of the more usual δW in order to indicate that this is not a case of an operator δ applied to a quantity W .
38
Chapter 1 / Introduction to Continuum Thermomechanics
is, if and only if the equilibrium equations (1.3.13) and the traction boundary conditions (1.3.12)2 are satisfied. Thus the body is in equilibrium under the applied loads if and only if the principle of virtual work, namely, δW ext = δW int ,
(1.3.14)
is obeyed. The principle of virtual work, also known as the principle of virtual displacements, may be interpreted as an application of the method of weighted residuals, whose essential idea is as follows. Suppose that a certain stress field σ is not exactly statically admissible, and therefore the equations obeyed by it have the form σij ,j +ρbi + ρ ∆bi = 0
nj σij = tai + ∆tai
in R,
on ∂Rt ;
we may think of ∆b and ∆ta as being the residuals of the body force and applied surface traction, respectively. If we cannot make these residuals vanish everywhere (which would make the stress field obey the equations exactly), then we can try to make them vanish in some average sense, namely, by multiplying them with a vectorvalued weighting function, say w, belonging to a suitable family (say W ) of such functions, such that Z
ρ ∆b · w dV +
Z ∂Rt
R
∆tai wi dS = 0
for every w belonging to W . If we identify W with the set of all virtual displacement fields, the principle of virtual work results. An advantage of this point of view is that it permits the application of the principle to dynamic problems as well: since the weighting functions w are not a priori identified with the virtual displacement fields, the inertia force −ρa may be added to b, and ∆b may be interpreted as the residual of ρ(b − a). Viewed in the light of the method of weighted residuals, the principle of virtual work may be represented by the equation Z R
(σij ,j +ρbi )wi dV −
Z ∂Rt
(nj σij − tai )wi dS = 0
(1.3.15)
for any w that obeys the same conditions as a virtual displacement field, that is, wi = 0 on ∂Ru , in addition to any internal constraints. Equation (1.3.15) is also known as the weak form of the equilibrium equations with the traction boundary conditions, and forms the foundation for many approximate methods of solution, based on different choices of the family W to which the weighting functions w belong. If W contains only a finite number of linearly independent functions, then the body is said to be discretized . Discretization is discussed below. When w is interpreted as a virtual velocity field , then Equation (1.3.15) is called the principle of virtual velocities,
Section 1.3 / Mechanics of Continuous Bodies
39
and, when, in addition, bi is replaced by bi − ai , as the dynamic principle of virtual velocities. A principle of the virtualwork type but different from the one just discussed is the principle of virtual forces (also called the principle of complementary virtual work). This principle is based on the notion of a virtual stress field δσ, defined (by analogy with the definition of a virtual displacement field) as the difference between two statically admissible stress fields. A virtual stress field therefore obeys δσij ,j = 0 in R and nj δσij = 0 on ∂Rt . The external and internal complementary virtual work are defined respectively by c
Z
δW ext =
∂Ru
uai nj δσij dS
and
c
δW int =
Z
εij δσij dV. R
An analysis similar to the one for virtual displacements leads to c δW int
−
c δW ext
Consequently
Z
= ∂Ru
(ui −
uai )nj δσij
c
Z
dS + R
[εij − 12 (ui ,j +uj ,i )]δσij dV.
c
δW int − δW ext = 0
(1.3.16)
for all virtual stress fields δσ if and only if the strain field ε is compatible with a kinematically admissible displacement field u.
Discretization Approximate treatments of continuum mechanics are often based on a procedure known as discretization, and virtual work provides a consistent framework for the procedure. A displacementbased discretized model of the body may be formulated as follows. Let q1 , ..., qN , qN +1 , ..., qN +K denote an ordered set of N + K scalars, called generalized coordinates. The displacement field u(x) is assumed to be given by u(x) =
NX +K
φn (x)qn ,
(1.3.17)
n=1
where φn (n = 1, ..., N + K) is a given set of vectorvalued functions of position. For given values of the qn , n = N + 1, ..., N + K, the displacement field given by (1.3.17) is kinematically admissible for all values of the qn , n = 1, ..., N . The qn for n = 1, ..., N are called the free generalized coordinates, and those for n = N + 1, ..., N + K, to be denoted qna (n = 1, ..., K), are called the constrained generalized coordinates. The former will be assembled in the 1 × N matrix q, and the latter in the 1 × K matrix q a . The integer N
40
Chapter 1 / Introduction to Continuum Thermomechanics
is called the number of degrees of freedom, and K the number of constraints. In particular, any or all of the qna may be zero. The straindisplacement relation for infinitesimal deformation may be written in direct vector notation as ε = (∇u)S , and consequently the strain tensor at x is ε(x) =
NX +K
(∇φn )S (x)qn .
(1.3.18)
n=1
Before inserting the discretized displacement and strain fields into the principle of virtual work, it is convenient to express them in matrix notation. Matrix notation for vectorvalued quantities such as displacement and force is obvious. The column matrices representing stress and strain are, respectively, σ11 ε11 σ22 ε22 σ ε 33 33 σ= , ε= , (1.3.19) σ23 2ε23 σ13 2ε13 σ12 2ε12 so that ε4 , ε5 , and ε6 represent conventional shear strains, and, most important, σ T ε = σij εij . In certain simpler problems, the dimension of the column matrices σ, ε may be less than six. In problems of plane stress or plane strain in the xyplane, with the component εz or σz ignored (because it does not participate in any virtual work), the matrices are σ=
σx
σ
y τ xy
,
ε=
εx
ε
y γ xy
.
(1.3.20)
In problems with only one component each of normal stress and shear stress (or longitudinal strain and shear strain) they are (
σ=
σ τ
)
(
,
ε=
ε γ
)
.
(1.3.21)
In every case, the stress and strain matrices are conjugate in the sense that the internal virtual work is given by Z
δW int =
σ T δε dV.
(1.3.22)
R
Equations (1.3.17) and (1.3.18) may now be rewritten in matrix notation as u(x) = Φ(x)q + Φa (x)q a ,
ε(x) = B(x)q + B a (x)q a ,
(1.3.23)
Section 1.3 / Mechanics of Continuous Bodies
41
where x and u are the columnmatrix representations of position and displacement, respectively, that is, for threedimensional continua, x=
x1
x
2 x 3
,
u=
u1
u
2 u 3
.
Since q a is prescribed, virtual displacement and strain fields are defined only in terms of the variations of q: δu(x) = Φ(x) δq,
δε(x) = B(x) δq.
(1.3.24)
We may now apply the principle of virtual work to these fields. Since σ T δε = σ T Φ δq = (ΦT σ)T δq, we obtain, using (1.3.24), the internal virtual work in discrete form: δW int = QT δq, where
Z
Q=
B T σ dV
R
is the internal generalized force matrix conjugate to q. Similarly, with the body force per unit volume f = ρb and the prescribed surface traction ta represented by matrices f and ta , the external virtual work is δW ext = F T δq, where
Z
T
Z
Φ f dV +
F = R
ΦT ta dS
∂Rt
is the (known) external generalized force matrix conjugate to q. If the residual force matrix is defined by R = Q − F , then the equilibrium condition may be written as R = 0, (1.3.25) a matrix equation representing N independent scalar equations.
Exercises: Section 1.3 1. If the acceleration field a is the material derivative v˙ of the velocity field v, find the acceleration at the point (1, 1, 0) at the time t = 0 if the velocity field in the Eulerian description is v = C[(x31 + x1 x22 )e1 − (x21 x2 + x32 )e2 ]e−at , where C and a are constants.
42
Chapter 1 / Introduction to Continuum Thermomechanics 2. With respect to a basis (ei ), a stress tensor is represented by the matrix
0.1 0.6 0.0 σ = 0.6 1.2 0.0 MPa 0.0 0.0 0.3 (a) Find the traction vector on an element of the plane 2x1 − 2x2 + x3 = 1. (b) Find the magnitude of the traction vector in (a), and the normal stress and the shear stress on the plane given there. (c) Find the matrix representing the stress tensor with respect to a basis e∗i , where e∗i = βij ej with β given in Exercise 4 of Section 1.1. 3. For the stress tensor in Exercise 2, find (a) the principal invariants I1 , I2 , I3 , (b) the principal stresses and principal directions, (c) the octahedral shear stress, (d) the component matrix of the stress deviator s with respect to the basis (ei ), (e) the principal deviatoric invariants J2 and J3 . 4. Draw the three Mohr’s circles for each of the following states of stress (units are MPa; stress components not given are zero). (a) Uniaxial tension, σ11 = 150 (b) Uniaxial compression, σ22 = −100 (c) Biaxial stress, σ11 = 50, σ22 = 100 (d) Biaxial stress, σ11 = 50, σ22 = −50 (e) Triaxial stress, σ11 = 80, σ22 = σ33 = −40 (f) σ11 = 50, σ22 = −10, σ12 = σ21 = 40, σ33 = 30 5. Find the maximum shear stress τmax for each of the stress states of the preceding exercise. 6. Derive Equation (1.3.11) for τmax as follows: fix a Cartesian basis (ei ) coinciding with the principal stress directions, and form [τ (n)]2 for all possible directions n by identifying n with the spherical unit vector er , so that [τ (n)]2 is a function of the spherical surface coordinates φ and θ. Lastly, show that this function can become stationary only in the planes formed by the principal stress directions.
Section 1.3 / Mechanics of Continuous Bodies
43
7. For the plane stress field given in engineering notation by σx = Axy,
τ=
A 2 (h − y 2 ), 2
σy = 0,
where A and h are constants, (a) show that it is in equilibrium under a zero body force, (b) find an Airy stress function Φ(x, y) corresponding to it. 8. Show that the equilibrium equations in the absence of body force (i.e. Equation (1.3.13) with bi = 0) are satisfied if σij = eikm ejln φkl ,mn , where φ is a symmetric secondrank tensor field. 9. If a stress field is given by the matrix
x21 x2 A (a2 − x22 )x1 0
(a2 − x22 )x1 0 3 2 1 (x2 − 3a x2 ) 0 , 3 0 2ax23
where A and a are constants, find the bodyforce field necessary for the stress field to be in equilibrium. 10. The following displacement field is assumed in a prismatic bar with the x1 axis being the longitudinal axis, and the crosssection defined by a closed curve C enclosing an area A in the x2 x3 plane, such that the x1 R axis intersects the crosssections at their centroids, so that A x2 dA = R A x3 dA = 0. u1 = u(x1 ) − v 0 (x1 )x2 ,
u2 = v(x1 ),
u3 = 0.
Show that the internal virtual work is Z
δW int =
L
(P δu0 + M δv 00 ) dx1 ,
0
where P =
R
A σ11 dA
and M = −
R
A x2 σ11 dA.
11. If the bar described in Exercise 10 is subject to a body force and a surface traction distributed along its cylindrical surface, show that the external virtual work can be written as Z
δW ext =
L
(p δu + q δv + m δv 0 ) dx1 .
0
Find expressions for p, q, and m.
44
Chapter 1 / Introduction to Continuum Thermomechanics
Section 1.4
Constitutive Relations: Elastic
1.4.1.
Energy and Thermoelasticity
Energy As discussed in Section 1.3, the solution of a boundaryvalue problem in solid mechanics requires finding the displacement field u and the stress field σ, that is, in the most general case, nine component fields. Thus far, the only field equations we have available are the three equations of motion (or of equilibrium, in static and quasistatic problems). In certain particularly simple problems, the number of unknown stress components equals that of nontrivial equilibrium equations, and these may be solved to give the stress field, though not the displacement field; such problems are called statically determinate, and are discussed further in Section 4.1. In general, however, constitutive relations that relate stress to displacement (more particularly, to the strain that is derived from the displacement) are needed. Such relations are characteristic of the material or materials of which the body is made, and are therefore also called simply material properties. In this section a simple class of constitutive relations, in which the current value of the strain at a point depends only on the stress at that point, is studied; a body described by such relations is called elastic. The influence of the thermal state (as given, for example, by the temperature) on the stressstrain relations cannot, however, be ignored. In order to maintain generality, instead of introducing elasticity directly a more basic concept is first presented: that of energy. The concept of energy is fundamental in all physical science. It makes it possible to relate different physical phenomena to one another, as well as to evaluate their relative significance in a given process. Here we focus only on those forms of energy that are relevant to solid mechanics. The kinetic energy of a body occupying a region R is K=
1 2
Z
ρv · v dV
R
(v = u˙ = velocity field), so that d K˙ = K = dt
Z
ρv · a dV
R
(a = v˙ = acceleration field), because, even though the mass density ρ and the volume element dV may vary in time, their product, which is a mass element, does not (conservation of mass). The external power acting on the body is Z
P = R
ρb · v dV +
Z ∂R
t(n) · v dS =
Z
Z
ρbi vi dV + R
ti (n)vi dS. ∂R
Section 1.4 / Constitutive Relations: Elastic
45
But ti (n) = σij nj , and the divergence theorem leads to Z
P =
[(σij ,j +ρbi )vi + σij vi ,j ] dV. R
In infinitesimal deformations, the difference between Eulerian and Lagrangian . . coordinates can be ignored, so that 12 (vi ,j +vj ,i ) = ε˙ ij , and hence σij vi ,j = σij ε˙ ij . In addition, σij ,j +ρbi = ρai , so that P − K˙ =
Z
σij ε˙ ij dV R
def
= Pd (deformation power).
˙ More generally, if Pd can be If ε˙ ≡ 0 (rigidbody motion), then P = K. ˙ then the body may approximately neglected in comparison with P and K, be treated as rigid. If, on the other hand, it is K˙ that is negligible, then the problem is approximately quasistatic. A problem of free vibrations may arise if the external power P is neglected. The heat f low into the body is Z
ρr dV −
Q=
Z
h(n) dS ∂R
R
(r = body heating or radiation, h(n) = heat outflow per unit time per unit surface area with orientation n). The first law of thermodynamics or principle of energy balance asserts that there exists a state variable u (internalenergy density) such that d dt
Z R
ρu dV = Q + Pd .
If we apply this law to the Cauchy tetrahedron, we obtain h(n) = h · n (h = heat flux vector), so that Z
Q= R
ρr dV −
Z ∂R
h · n dS =
Z
(ρr − div h) dV
R
by Gauss’s theorem, and we obtain the local energybalance equation, ρu˙ = σij ε˙ ij + ρr − div h.
(1.4.1)
Thermoelasticity The local deformation, as defined by the strain tensor ε, may be assumed to depend on the stress tensor σ, on the internalenergy density u, and on additional variables ξ1 , . . . , ξN (internal variables). By definition, a body is called thermoelastic if ε everywhere depends only on σ and u. The
46
Chapter 1 / Introduction to Continuum Thermomechanics
dependence is not arbitrary; it must be consistent with the second law of thermodynamics. We assume for the time being that at a fixed value of u, the relation between strain and stress is invertible, so that σ may be regarded as a function of ε and u. Possible restrictions on this assumption, resulting from internal constraints, are discussed later. The second law of thermodynamics for a thermoelastic body can be stated as follows: there exists a state function η = η¯(u, ε) (entropy density) such that η˙ = 0 in an adiabatic process, that is, in a process in which ρr −div h = 0. As a consequence, the two equations ∂ η¯ ∂ η¯ ε˙ ij = 0 and ρu˙ − σij ε˙ ij = 0 u˙ + ∂u ∂εij must be satisfied simultaneously. If we now define the absolute temperature T by ∂ η¯ T −1 = , (1.4.2) ∂u then, upon eliminating u˙ between the two equations, ∂ η¯ σij + T ρ ∂εij
!
ε˙ ij = 0.
If, moreover, the ε˙ ij are independent (i.e. if there are no internal constraints as discussed in Section 1.3), then their coefficients must vanish, since any five of the six independent components ε˙ ij may be arbitrarily taken as zero. The vanishing of the coefficients yields σij = −T ρ
∂ η¯ , ∂εij
an equation that gives an explicit form to the assumed dependence of σ on u and ε. The fact that this relation was derived on the basis of an adiabatic process is irrelevant, since, by hypothesis, the relation is only among the current values of σ, ε, and u and is independent of process. It follows further that T ρη˙ = ρu˙ − σij ε˙ ij = ρr − div h. def
If the total entropy of the body is defined by S = S˙ =
Z
Z
ρη˙ dV = R
R
R ρη dV
(1.4.3) , then
T −1 (ρr − div h) dV
R
r h + h · ∇T −1 dV = ρ − div T T R Z Z Z r h(n) = ρ dV − dS + h · ∇T −1 dV. R T ∂R T R Z
Section 1.4 / Constitutive Relations: Elastic
47
We can now bring in the experimental fact that heat flows from the hotter to the colder part of a body. The mathematical expression of this fact is h · ∇T −1 ≥ 0, so that S˙ −
r ρ dV − R T
Z
h(n) dS T
Z ∂R
def
= Γ ≥ 0.
(1.4.4)
Inequality (1.4.4), known as the global Clausius–Duhem inequality, is usually taken to be the general form of the second law of thermodynamics for continua, whether thermoelastic or not, though its physical foundation in the general case is not so firm as in the thermoelastic case (see, e.g., Woods [1981]). The quantity in parentheses is called the external entropy supply, and Γ is the internal entropy production. In the thermoelastic case, clearly, Z
Γ=
h · ∇T −1 dV.
R
R
More generally, Γ may be assumed to be given by R ργ dV , where γ is the internal entropy production per unit mass, and ργ contains, besides the term h · ∇T −1 , additional terms representing energy dissipation. These are discussed in Section 1.5. With the help of the divergence theorem, (1.4.4) may be transformed into the equation Z
ρη˙ − ρ
R
r +∇· T
h T
− ργ dV = 0.
The local Clausius–Duhem inequality is obtained when it is assumed, as usual, that the equation must apply to any region of integration R, however small, and, in addition, that γ is nonnegative: ρη˙ − ρ
r +∇· T
h T
= ργ ≥ 0.
(1.4.5)
The assumptions underlying the derivation of (1.4.5) have been severely criticized by Woods [1981]. The criticisms do not, however, apply to thermoelastic bodies, to which we now return. Given the definition (1.4.2) of the absolute temperature T and the fact that T is always positive, it follows from the implicit function theorem of advanced calculus that we can solve for u as a function of η and ε [i.e. u = u ˜(η, ε)], and we can use η as a state variable. Since, by Equation (1.4.3), u˙ = T η˙ + ρ−1 σij ε˙ ij , we have T = ∂ u ˜/∂η and ∂u ˜ σij − ρ ∂εij
!
ε˙ ij = 0.
(1.4.6)
Again, in the absence of internal constraints, the ε˙ ij can be specified independently. The coefficients in Equation (1.4.6) must therefore all vanish, yielding the relation ∂u ˜ σij = ρ , ∂εij
48
Chapter 1 / Introduction to Continuum Thermomechanics
in which the specific entropy η is the other variable. The equation thus gives the stressstrain relation at constant specific entropy and is accordingly known as the isentropic stressstrain relation. It is also called the adiabatic stressstrain relation, since in a thermoelastic body isentropic processes are also adiabatic. We must remember, however, that the relation as such is independent of process. We now drop the assumption that the body is free of internal constraints. In the presence of an internal constraint of the form cij ε˙ ij = 0, a term pcij , with p an arbitrary scalar, may be added to the the stress without invalidating Equation (1.4.6). This equation is therefore satisfied whenever σij = ρ
∂u ˜ − pcij . ∂εij
The stress, as can be seen, is not completely determined by the strain and the entropy density. As noted in 1.3.5, a commonly encountered internal constraint is incompressibility. In an incompressible body the volume does not change, so that δij ε˙ ij = 0 and thus cij may be identified with δij . The stress is, accordingly, determinate only to within a term given by pδij , where p is, in this case, a pressure. The use of the entropy density η as an independent state variable is not convenient. A far more convenient thermal variable is, of course, the temperature, since it is fairly easy to measure and to control. If the Helmholtz free energy per unit mass is defined as def
ψ = u − T η = ψ(T, ε), then ψ˙ = −η T˙ + ρ−1 σij ε˙ ij , so that η = −∂ψ/∂T and, in the absence of internal constraints, ∂ψ σij = ρ . (1.4.7) ∂εij Equation (1.4.7) embodies the isothermal stressstrain relation. In addition to the stressstrain relations, the properties of a thermoelastic continuum include the thermal stress coefficients and the specific heat. The former are the increases in the stress components per unit decrease in temperature with no change in the strain, that is, ∂σij ∂2ψ ∂η βij = − = −ρ =ρ . ∂T ε=const ∂T ∂εij ∂εij
Clearly, β is a secondrank tensor. The specific heat (per unit mass) at constant strain is ∂u ∂ ∂ψ ∂η ∂η ∂2ψ C= = (ψ + ηT ) = + η + T = T = −T . ∂T ε=const ∂T ∂T ∂T ∂T ∂T 2
Section 1.4 / Constitutive Relations: Elastic
49
Linearization For sufficiently small deviations in strain and temperature from a given reference state, the stressstrain relation, if it is smooth, can be approximated by a linear one. Let us consider a reference state “0” at zero strain and temperature T0 , and let us expand ψ(T, ε) in a Taylor series about this state:
1 ∂ 2 ψ ∂ψ ∂ψ ε + ψ(T, ε) = ψ0 + (T − T ) + (T − T0 )2 ij 0 2 ∂T 0 ∂εij 0 2 ∂T 0 1 ∂ 2 ψ ∂ 2 ψ + (T − T0 )εij + εij εkl + . . . ∂T ∂εij 0 2 ∂εij ∂εkl 0
Now, ∂ψ/∂T 0 = −η0 (η0 = specific entropy in the reference state) and ∂ψ 0 (σ 0 = initial stress). Furthermore, = ρ−1 σij ∂εij 0
∂ 2 ψ 1 = − C0 , 2 ∂T 0 T0 and
∂ 2 ψ 0 , = −ρ−1 βij ∂T ∂εij 0
∂ 2 ψ ∂σij 0 0 ρ = Cijkl = Cklij , = ∂εij ∂εkl 0 ∂εkl 0
the isothermal elastic modulus tensor (of rank 4) at the temperature T0 . Thus 1 0 εij η = η0 + C0 (T − T0 ) + ρ−1 βij T0 and 0 0 0 σij = σij − βij (T − T0 ) + Cijkl εkl
are the constitutive relations of linear thermoelasticity. 0ε . In an isentropic process, η ≡ η0 , so that T − T0 = −(T0 /ρC0 )βij ij Consequently, T0 0 0 0 0 + Cijkl + σij = σij βij βkl εkl , ρC0 which defines the isentropic or adiabatic elastic modulus tensor.
1.4.2.
Linear Elasticity
Elasticity The dependence of the stressstrain relation on the thermal state is often ignored, and the simple relation σ = σ(ε) is assumed. It is then that a body is called simply, in the traditional sense, elastic. The internalenergy density
50
Chapter 1 / Introduction to Continuum Thermomechanics
or the freeenergy density, as the case may be, may be replaced by the strainenergy function W (ε) (per unit volume), so that the stressstrain relation, again in the absence of internal constraints, is σij =
∂W . ∂εij
This relation is exact in an isentropic process, with η at a fixed value, if W (ε) is identified with u ˜(η, ε), and in an isothermal process, with T at a fixed value, if W (ε) is identified with ψ(T, ε). The introduction of the strainenergy function into elasticity is due to Green, and elastic solids for which such a function is assumed to exist are called Greenelastic or hyperelastic. Elasticity without an underlying strainenergy function is called Cauchy elasticity. Throughout this book, “elasticity” means hyperelasticity as a matter of course.
Generalized Hooke’s Law Linearization for an elastic continuum will be carried out with respect to a reference configuration which is stressfree at the reference temperature T0 , so that σ 0 = 0. We may now let C denote either the isothermal or the isentropic modulus tensor, as appropriate, and under isothermal or isentropic conditions we obtain the generalized Hooke’s law σij = Cijkl εkl . The Cijkl , called the elastic constants (recall that they depend on the temperature), are components of a tensor of rank 4, likewise symmetric with respect to the index pairs ij and kl; this symmetry reduces the number of independent components from 81 to 36. But there is an additional symmetry: since ∂ 2 W ∂ 2 W Cijkl = = , (1.4.8) ∂εij ∂εkl ε=0 ∂εkl ∂εij ε=0 we also have Cijkl = Cklij , and thus the number of independent components is further reduced to 21. This number may be reduced even more by material symmetries. Of these, only isotropy is considered here. If stress and strain are represented in matrix notation as given by Equation (1.3.19), then the stressstrain relation may be written as σ = C ε,
(1.4.9)
where the symmetric square matrix C = [CIJ ] (we use capital letters as indices in the sixdimensional space of stress and strain components) is defined as follows: C11 = C1111 , C12 = C1212 , C14 = C1123 , C44 = C2323 , etc.
Section 1.4 / Constitutive Relations: Elastic
51
Assuming the matrix C to be invertible, we also have the strainstress relations ε = C −1 σ. Reverting to tensor component notation, we may write these relations as −1 εij = Cijkl σkl ,
where the compliance tensor C−1 is given as follows: −1 −1 −1 −1 −1 −1 −1 −1 C1111 , C1212 , etc. = C11 = 14 C66 , C1122 = C12 , C1123 = 12 C14
The complementaryenergy function is defined for a general elastic material as W c = σij εij − W. Note that if we assume W c = W c (ε, σ), then ∂W ∂W c = σij − = 0, ∂εij ∂εij so that W c is in fact a function of σ only, and εij =
∂W c . ∂σij
For the linear material we have 1 1 −1 σij σkl = σ T C −1 σ, W c = Cijkl 2 2 and therefore εI =
∂W c . ∂σI
Isotropic Linear Elasticity The most general isotropic tensor of rank 4 has the representation λδij δkl + µδik δjl + νδil δjk . If Cijkl has this form, then, in order to satisfy the symmetry condition Cijkl = Cjikl (symmetry of the stress tensor) we must have µ = ν. The symmetry condition Cijkl = Cklij (existence of strainenergy function) is then automatically satisfied. Thus Cijkl = λδij δkl + µ(δik δjl + δil δjk ), so that the isotropic linear elastic stressstrain relation is σij = λδij εkk + 2µεij .
(1.4.10)
52
Chapter 1 / Introduction to Continuum Thermomechanics
λ and µ are known as the Lam´e coefficients. In particular, µ = G, the shear modulus. The matrix C takes the form C=
λ + 2µ λ λ λ λ + 2µ λ λ λ λ + 2µ 0 0 0 0 0 0 0 0 0
0 0 0 µ 0 0
0 0 0 0 µ 0
0 0 0 0 0 µ
.
Inverting this matrix, we obtain
C −1
1 = µ(3λ + 2µ)
λ + µ −λ/2 −λ/2 0 0 0 −λ/2 λ + µ −λ/2 0 0 0 −λ/2 −λ/2 λ + µ 0 0 0 0 0 0 3λ + 2µ 0 0 0 0 0 0 3λ + 2µ 0 0 0 0 0 0 3λ + 2µ
.
If we define the Y oung 0 s modulus as E = µ(3λ + 2µ)/(λ + µ) and the Poisson’s ratio as ν = 21 λ/(λ + µ), then
C −1
1 = E
1 −ν −ν 0 0 0 −ν 1 −ν 0 0 0 −ν −ν 1 0 0 0 0 0 0 2(1 + ν) 0 0 0 0 0 0 2(1 + ν) 0 0 0 0 0 0 2(1 + ν)
.
Note that the determinant of C −1 is 8(1 + ν)5 (1 − 2ν)E −6 , so that when ν = 12 (incompressible material), the compliance matrix is singular. In that case there exists no matrix C, that is, stress cannot be given as a function of strain, as we already know. From the nonzero elements of C −1 we can obtain the corresponding components of the compliance tensor C−1 : 1 −1 = C1111 , etc., E ν −1 −1 C12 = − = C1122 , etc., E 2(1 + ν) 1 1 −1 = = = = 4C1212 , etc. E µ G −1 C11 =
−1 C44
Consequently the isotropic linearly elastic strainstress relation in indicial notation is 1 εij = [(1 + ν)σij − νσkk δij ]. (1.4.11) E
Section 1.4 / Constitutive Relations: Elastic
53
If the only nonzero stress component is σ11 = σ, and if we denote ε11 by ε, then Equation (1.4.11) gives the uniaxial stressstrain relation σ = Eε.
(1.4.12)
When σ33 = 0, then Equation (1.4.11), with the indices limited to the values 1 and 2, reads 1 εαβ = [(1 + ν)σαβ − νσγγ δαβ ], E which may be inverted to yield σαβ =
E [(1 − ν)εαβ + νεγγ δαβ ]. 1 − ν2
(1.4.13)
In plane problems, with σ and ε defined by Equations (1.3.20), C is given by
1 ν E ν 1 C= 1−ν 2 0 0
0 0 1 (1−ν) 2
for plane stress and by
1−ν ν E ν 1−ν C= (1+ν)(1−2ν) 0 0
0 0 1 (1−2ν) 2
for plane strain. In a stress state composed of uniaxial stress and simple shear, with stress and strain matrices given by (1.3.21), we have "
C=
E 0 0 G
#
.
If E, ν are interpreted as representing the isothermal elastic stiffness, then for small changes in temperature from the reference temperature T0 we may add to the elastic strain given by Equation (1.4.11) the thermal strain α(T − T0 )δij , where α is the familiar coefficient of thermal expansion, obtaining εij =
1 [(1 + ν)σij − νσkk δij ] + α(T − T0 )δij . E
(1.4.14)
The thermal stress coefficients βij are accordingly given by 3Kαδij , where 2 1 E K =λ+ µ= 3 3 1 − 2ν is the bulk modulus, which appears in the volumetric constitutive relation σkk = 3K[εkk − 3α(T − T0 )].
54
Chapter 1 / Introduction to Continuum Thermomechanics We may also derive the deviatoric or distortional constitutive relation sij = 2µeij ,
which includes, in particular, Hooke’s law in shear: τ = Gγ.
(1.4.15)
It is characteristic of an isotropic material that the volumetric and deviatoric stressstrain relations are uncoupled . The uncoupling can also be seen from the strainenergy function, 1 1 W = λ(εkk )2 + µεij εij = K(εkk )2 + µeij eij , 2 2
(1.4.16)
and of the complementaryenergy function, Wc =
1.4.3.
1 1 (σkk )2 + sij sij . 18K 4G
(1.4.17)
Energy Principles
Internal Potential Energy, Variations R
Let Πint = R W dV be the total strain energy or internal potential energy of the body. Given a virtual displacement field δu and the corresponding virtual strain field δε, the first variation of Πint , denoted δΠint , is defined as follows. We let Πint denote, more specifically, the internal potential energy evaluated at the displacement field u, while Πint +∆Πint denotes the internal potential energy evaluated at the varied displacement field u+δu. Assuming the dependence of Πint on u to be smooth, we can write 1 ∆Πint = δΠint + δ 2 Πint + . . . , 2 where δΠint is linear in δu (and/or in its derivatives, and therefore also in δε), δ 2 Πint (the second variation of Πint ) is quadratic, and so on. From the definition of Πint , Z
∆Πint =
[W (ε + δε) − W (ε)]dV
R
Z
= R
1 ∂W δεij dV + ∂εij 2
Z R
∂2W δεij δεkl dV + . . . . ∂εij ∂εkl
According to our definition, the first integral in the last expression is δΠint , while the second integral is δ 2 Πint . Even in the presence of internal constraints, σij δεij =
∂W δεij . ∂εij
Section 1.4 / Constitutive Relations: Elastic
55
In view of the definition of internal virtual work as given in 1.3.5, therefore, δW int = δΠint .
Total Potential Energy, Minimum Principle For a fixed set of loads b, ta , let the external potential energy be defined as Πext = −
Z
Z
ρbi ui dV −
R
∂Rt
tai ui dS;
then the external virtual work over a virtual displacement field δu is δW ext = −δΠext . If we now define the total potential energy as Π = Πint + Πext , then we have δW int − δW ext = δΠ, the first variation of Π. The principle of virtual work, (1.3.15), then tells us that an elastic body is in equilibrium if and only if δΠ = 0;
(1.4.18)
that is, at equilibrium the displacement field makes the total potential energy stationary with respect to virtual displacements. It can further be shown that for the equilibrium to be stable, the total potential energy must be a minimum, a result known as the principle of minimum potential energy. If Π is a local minimum, then, for any nonzero virtual displacement field δu, ∆Π must be positive. Since the first variation δΠ vanishes, the second variation δ 2 Π must be positive. Πext is, by definition, linear in u, and therefore, in the absence of significant changes in geometry,1 δ 2 Πext = 0. Hence 2
Z
2
δ Π = δ Πint = R
Cijkl δεij δεkl dV.
An elastic body is thus stable under fixed loads if Cijkl εij εkl > 0, or, in matrix notation, εT C ε > 0, for all ε 6= 0. A matrix having this property is known as positive definite, and the definition can be naturally extended to the fourthrank tensor C. The positivedefiniteness of C is assumed henceforth. If the loads b and ta are not fixed but depend on the displacement, then the justderived principle is still valid, provided that the loads are derivable from potentials, that is, that there exist functions φ(u, x) and ψ(u, x) defined on R and ∂R, respectively, such that ρbi = −∂φ/∂ui and tai = −∂ψ/∂ui (examples: spring support, elastic foundation). In that case, Z
Πext =
φ dV + R
1
Z
ψ dS, ∂R
It is the changes in geometry that are responsible for unstable phenomena such as buckling, discussed in Section 5.3.
56
Chapter 1 / Introduction to Continuum Thermomechanics
and the second variation δ 2 Πext does not, in general, vanish, even in the absence of significant geometry changes.
Complementary Potential Energy From the principle of virtual forces we may derive a complementary energy principle for elastic bodies. If the prescribed displacements are uai (assumed independent of traction), and if the external and internal complementary potential energies for a given stress field σ are defined as Πcext
=−
Z ∂R
and Πcint
Z
uai nj σij dS
W c (σ) dV,
= ∂R
respectively, then, analogously, c
c
δW int − δW ext = δΠc , where Πc = Πcext + Πcint is the total complementary potential energy. According to the virtualforce principle, then, Πc is stationary (δΠc = 0) if and only if the stress field σ is related by the stressstrain relations to a strain field that is compatible — both with internal constraints (if any) and with the prescribed displacements or external constraints. Since Πc can also be shown to be a minimum at stable equilibrium, this principle is the principle of minimum complementary energy.
Discretized Elastic Body If an elastic continuum is discretized as in 1.3.5, then the stressstrain relation (1.4.9) implies σ(x) = C[B(x)q + B a (x)q a ], and therefore Q = Kq + K a q a , where
Z
K=
B T C B dV
(1.4.19)
R
and Ka =
Z
B T C B a dV.
R
The symmetric matrix K is generally referred to as the stiffness matrix of the discretized model. The equilibrium equation Q = F can now be solved for the qn in terms of prescribed data as q = K −1 (F − K a q a ),
Section 1.4 / Constitutive Relations: Elastic
57
provided that the stiffness matrix is invertible. It is easy to extend the preceding result to include the effects of initial and thermal stresses. The new result is q = K −1 (F − K a q a − Q0 + F T ), where 0
Z
Q =
T
0
B σ dV, R
Z
FT =
B T β(T − T 0 ) dV,
R
σ 0 denoting the initial stress field, T 0 and T respectively the initial and current temperature fields, and β the 6 × 1 matrix form of the the thermalstress coefficient tensor β defined in 1.4.1. The invertibility requirement on K is equivalent to the nonvanishing of its eigenvalues. Note that T
Z
δq K δq =
δεT C δε dV,
R
so that since the elastic strain energy cannot be negative, the lefthand side of the preceding equation also cannot be negative — that is, K must be positive semidefinite. The invertibility requirement therefore translates into one of the positive definiteness of the stiffness matrix. This condition means that any variation in q implies deformation, that is, that the model has no rigidbody degrees of freedom.
Exercises: Section 1.4 1. Assume that the internalenergy density can be given as u = u ¯(ε, T ), that the heat flux is governed by the Fourier law h = −k(T )∇T , and that r = 0. Defining the specific heat C = ∂ u ¯/∂T , write the equation resulting from combining these assumptions with the local energybalance equation (1.4.1). 2. Let the complementary internalenergy density be defined by κ = σij εij /ρ − u. Neglecting density changes, assume that the entropy density can be given as η = ηˆ(σ, κ). (a) Show that T −1 = −∂ ηˆ/∂κ. (b) Assuming ε = ε(σ, η) and κ = κ ˆ (σ, η), show that T = −∂ˆ κ/∂η and εij = ρ∂ˆ κ/∂σij . (c) Defining the complementary freeenergy density χ(σ, T ) = κ + T η, show that η = ∂χ/∂T and the isothermal strainstress relation is εij = ρ∂χ/∂σij . 3. Expand the complementary free energy χ (Exercise 2) in powers of σ and T − T0 , and find the linearized expressions for η and ε.
58
Chapter 1 / Introduction to Continuum Thermomechanics 4. A solid is called inextensible in a direction n if the longitudinal strain along that direction is always zero. Find an isothermal relation for the stress in an inextensible thermoelastic solid, and explain the meaning of any undetermined quantity that may appear in it. 5. Show that, in an isotropic linearly elastic solid, the principal stress and principal strain directions coincide. 6. Write the elastic modulus matrix C for an isotropic linearly elastic solid in terms of the Young’s modulus E and the Poisson’s ratio ν. 7. Combine the stressstrain relations for an isotropic linearly elastic solid with the equations of motion and the straindisplacement relations in order to derive the equations of motion for such a solid entirely in terms of displacement, using (a) λ and µ, (b) G and ν. 8. Derive the forms given in the text for C in plane stress and plane strain. 9. Find the relation between the isothermal and adiabatic values of the Young’s modulus E in an isotropic linearly elastic solid, in terms of the linearexpansion coefficient α and any other quantities that may be necessary.
10. Derive an explicit expression for the strainenergy function W (ε) in terms of the “engineering” components of strain εx , . . . , γxy , ..., using E and ν. 11. Show that, if the bar described in Exercise 10 of Section 1.3 is made of a homogeneous, isotropic, linearly elastic material, then its internal potential energy is Πint
1¯ = E 2
Z
L
2
0
where A is the crosssectional area, I = ¯= E
2
(Au0 + Iv 00 ) dx1 , R
2 A x2 dA,
and
E(1 − ν) . (1 − 2ν)(1 + ν)
¯ in Exercise 11 by E. 12. Give a justification for replacing E 13. Combining the results of Exercise 11, as modified by Exercise 12, with those of Exercise 10 of Section 1.3, show that P = EAu0 and M = EIv 00 .
Section 1.5 / Constitutive Relations: Inelastic
59
14. For the quantity Ξ defined by Z
{W (ε) − ρbi ui − σij [εij − 12 (ui ,j +uj ,i )]} dV
Ξ= R
−
Z ∂Rt
tai ui dS −
Z ∂Ru
ti (ui − uai ) dS,
show that, if u, ε, σ and (on ∂Ru ) t can be varied independently of one another, then δΞ = 0 leads to six sets of equations describing a static boundaryvalue problem in linear elasticity. The result is known as the Hu–Washizu principle.
Section 1.5
Constitutive Relations: Inelastic
In this section a theoretical framework for the description of inelastic materials is presented, building on the discussion of elasticity in the preceding section. The concepts introduced here are applied to the development of the constitutive theory of plasticity in Chapter 3, following a brief survey of the physics of plasticity in Chapter 2.
1.5.1.
Inelasticity
Introduction If we return to the weak (Cauchy) definition of an elastic body as one in which the strain at any point of the body is completely determined by the current stress and temperature there, then an obvious definition of an inelastic body is as one in which there is something else, besides the current stress and temperature, that determines the strain. That “something else” may be thought of, for example, as the past history of the stress and temperature at the point. While the term “past history” seems vague, it can be defined quite precisely by means of concepts from functional analysis, and a highly mathematical theory, known as the theory of materials with memory, has been created since about 1960 in order to deal with it. The dependence of the current strain on the history of the stress (and its converse dependence of stress on strain history, whenever that can be justified) can be expressed explicitly when the behavior is linear. The relevant theory is known as the theory of linear viscoelasticity and is briefly reviewed later in this section. One way in which history affects the relation between strain and stress is through rate sensitivity: the deformation produced by slow stressing is different — almost invariably greater — than that produced by rapid stressing.
60
Chapter 1 / Introduction to Continuum Thermomechanics
A particular manifestation of rate sensitivity is the fact that deformation will in general increase in time at constant stress, except possibly under hydrostatic stress; this phenomenon is called flow in fluids and creep in solids. Rate sensitivity, as a rule, increases with temperature, so that materials which appear to behave elastically over a typical range of times at ordinary temperatures (at least within a certain range of stresses) become markedly inelastic at higher temperatures. For this reason creep is an important design factor in metals used at elevated temperatures, while it may be ignored at ordinary temperatures. If strain and stress can be interchanged in the preceding discussion, then, since a slower rate implies a greater deformation at a given stress, it accordingly implies a lower stress at a given strain. Consequently, the stress will in general decrease in time at a fixed strain, a phenomenon known as relaxation. The rate sensitivity of many materials, including polymers, asphalt, and concrete, can often be adequately described, within limits, by means of the linear theory. The inelasticity of metals, however, tends to be highly nonlinear in that their behavior is very nearly elastic within a certain range of stresses (the elastic range) but strongly historydependent outside that range. When the limit of the elastic range (the elastic limit) is attained as the stress is increased, the metal is said to yield . When the elastic range forms a region in the space of the stress components, then it is usually called the elastic region and its boundary is called the yield surface.
Internal Variables An alternative way of representing the “something else” is through an array of variables, ξ1 , ..., ξn , such that the strain depends on these variables in addition to the stress and the temperature. These variables are called internal (or hidden) variables, and are usually assumed to take on scalar or secondrank tensor values. The array of the internal variables, when the tensorial ones, if any, are expressed in invariant form, will be denoted ξ. The strain is accordingly assumed as given by ε = ε(σ, T, ξ). The presence of additional variables in the constitutive relations requires additional constitutive equations. The additional equations that are postulated for a ratesensitive or ratedependent inelastic body reflect the hypothesis that, if the local state that determines the strain is defined by σ, T, ξ, then the rate of evolution of the internal variables is also determined by the local state: ξ˙α = gα (σ, T, ξ). (1.5.1) Equations (1.5.1) are known as the equations of evolution or rate equations for the internal variables ξα .
Section 1.5 / Constitutive Relations: Inelastic
61
The relation ε = ε(σ, T, ξ) cannot always be inverted to give σ = σ(ε, T, ξ), even when there are no internal constraints governing the strain. As an illustration of this principle of nonduality, as it was called by Mandel [1967], let us consider the classical model known as Newtonian viscosity. When limited to infinitesimal deformation, the model can be described by the equation 1 εij = σkk δij + εvij , 9K where εv is a tensorvalued internal variable, called the viscous strain, whose rate equation is 1 ε˙ v = s, 2η where s is the stress deviator. The elastic bulk modulus K and the viscosity η are functions of temperature; if necessary, a thermal strain α(T − T0 )δij may be added to the expression for εij . It is clearly not possible to express σ as a function of ε, T , and a set of internal variables governed by rate equations. Instead, the stress is given by σij = Kεkk δij + 2η e˙ ij . If it is possible to express the stress as σ(ε, T, ξ), then this expression may be substituted in the righthand side of (1.5.1), resulting in an alternative form of the rate equations: ξ˙α = gα (σ(ε, T, ξ), T, ξ) = g¯α (ε, T, ξ).
Inelastic Strain For inelastic bodies undergoing infinitesimal deformation, it is almost universally assumed that the strain tensor can be decomposed additively into an elastic strain εe and an inelastic strain εi : εij = εeij + εiij , −1 where εeij = Cijkl σkl (with thermal strain added if needed). Newtonian viscosity, as discussed above, is an example of this decomposition, with εi = εv .
1.5.2.
Linear Viscoelasticity
The aforementioned theory of linear viscoelasticity provides additional examples of the additive decomposition. For simplicity, we limit ourselves to states that can be described by a single stress component σ with the conjugate strain ε; the extension to arbitrary states of multiaxial stress and strain
62
Chapter 1 / Introduction to Continuum Thermomechanics
is made later. The temperature will be assumed constant and will not be explicitly shown.
“Standard Solid” Model Suppose that the behavior of a material element can be represented by the mechanical model of Figure 1.5.1(a) (page 63), with force representing stress and displacement representing strain. Each of the two springs models elastic response (with moduli E0 and E1 ), and the dashpot models viscosity. The displacement of the spring on the left represents the elastic strain εe , and the displacement of the springdashpot combination on the right represents the inelastic strain εi . Equilibrium requires that the force in the lefthand spring be the same as the sum of the forces in the other two elements, and therefore we have two equations for the stress σ: σ = E0 ε e ,
σ = E1 εi + η ε˙ i ,
where η is the viscosity of the dashpot element. For the total strain ε we may write σ ε= + εi , E0 ε˙ i =
E1 i 1 σ− ε. η η
The inelastic strain may consequently be regarded as an internal variable, the last equation being its rate equation (E1 and η are, of course, functions of the temperature). Given an input of stress as a function of time, the rate equation for εi is a differential equation that can be solved for εi (t): 1 ε (t) = η i
Z
t
0
e−(t−t )/τ σ(t0 ) dt0 ,
−∞
where the reference time (at which εi = 0) is chosen as −∞ for convenience, and τ = η/E1 is a material property having the dimension of time. In particular, if σ(t) = 0 for t < 0 and σ(t) = σ0 (constant) for t > 0, then εi (t) = (1/E1 )(1 − e−t/τ )σ0 ; this result demonstrates a form of creep known as delayed elasticity. The limiting case represented by E1 = 0 is known as the Maxwell model of viscoelasticity. Note that in this case τ is infinite, so that the factor exp[−(t − t0 )/τ ] inside the integral becomes unity, and the creep solution is just εi (t) = (t/η)σ0 , displaying steady creep.
Generalized Kelvin Model If models of viscoelasticity with more than one dashpot per strain component are used — say a number of parallel springdashpot combinations in
Section 1.5 / Constitutive Relations: Inelastic E1 E0
63
E1
E2
η1
η2
En
E0

pppp
η
ηn
(b)
(a) 6 E1
E2
η1
η2
p p p p p p p
En
E∞
ηn
? (c) 6
6 E0
E∞
η
η
?
?
(d)
(e)
Figure 1.5.1. Models of linear viscoelasticity: (a) “standard solid” model; (b) generalized Kelvin model; (c) generalized Maxwell model; (d) Maxwell model; (e) Kelvin model. series with a spring, the socalled generalized Kelvin model shown in Figure 1.5.1(b) — then the inelastic strain is represented by the sum of the dashpot displacements, and every dashpot displacement constitutes an internal variable. Designating these by ξα , we have εi =
n X
ξα .
α=1
By analogy with the previous derivation, the rate equations for the ξα are, if τα = ηα /Eα , σ ξα ξ˙α = − . ηα τα As before, for a given stress history σ(t0 ), −∞ < t0 < t (where t is the current time), the rate equations are ordinary linear differential equations for the ξα that can be integrated explicitly: Z
ξα (t) =
t
−∞
1 −(t−t0 )/τα 0 0 e σ(t ) dt . ηα
64
Chapter 1 / Introduction to Continuum Thermomechanics
The current strain ε(t) can therefore be expressed as 1 ε(t) = σ(t) + E0
t
n X 1
−∞
η α=1 α
Z
−(t−t0 )/τα
e
!
σ(t0 ) dt0 .
With the uniaxial creep function J(t) defined by J(t) =
n X 1 1 + 1 − e−t/τα , E0 α=1 Eα
the current strain can, with the help of integration by parts [and the assumption σ(−∞) = 0], also be expressed as t
Z
ε(t) = −∞
J(t − t0 )
dσ 0 dt . dt0
If the stress history is given by σ(t0 ) = 0 for t0 < 0 and σ(t0 ) = σ (constant) for t0 > 0, then, for t > 0, the strain is ε(t) = σJ(t). The creep function can therefore be determined experimentally from a single creep test, independently of an internalvariable model (unless the material is one whose properties change in time, such as concrete). Similarly, in a relaxation test in which ε(t0 ) = 0 for t0 < 0 and ε(t0 ) = ε (constant) for t0 > 0, the measured stress for t > 0 has the form σ(t) = εR(t), where R(t) is the uniaxial relaxation function. Under an arbitrary strain history ε(t0 ), the stress at time t is then Z
t
σ(t) = −∞
R(t − t0 )
dε 0 dt . dt0
An explicit form of the relaxation function in terms of internal variables can be obtained by means of the generalized Maxwell model [Figure 1.5.1(c)]. It can be shown that, in general, R(0) = 1/J(0) = E0 (the instantaneous elastic modulus), and R(∞) = 1/J(∞) = E∞ (the asymptotic elastic modulus), with E0 > E∞ except in the case of an elastic material. In particular, E∞ may be zero, as in the Maxwell model [Figure 1.5.1(d)], while E0 may be infinite, as in the Kelvin model [Figure 1.5.1(e)]. The relaxation function of the Kelvin model is a singular function given by R(t) = E∞ + ηδ(t), where δ(t) is the Dirac delta function. A generalization of the preceding description from uniaxial to multiaxial behavior is readily accomplished by treating J(t) and R(t) as functions whose values are fourthrank tensors. For isotropic materials, the tensorial form of these functions is analogous to that of the elastic moduli as given in 1.4.2: Jijkl (t) = J0 (t)δij δkl + J1 (t)(δik δjl + δik δjl ), Rijkl (t) = R0 (t)δij δkl + R1 (t)(δik δjl + δik δjl ).
Section 1.5 / Constitutive Relations: Inelastic
65
By analogy with Newtonian viscosity, it is frequently assumed (not always with physical justification) that the volumetric strain is purely elastic, that is, εkk = σkk /3E. It follows that the creep and relaxation functions obeying this assumption must satisfy the relations 3J0 (t) + 2J1 (t) =
1 , 3K
3R0 (t) + 2R1 (t) = 3K.
The use of creep and relaxation functions makes it possible to represent the strain explicitly in terms of the history of stress, and vice versa, with no reference to internal variables. Indeed, the concept of internal variables is not necessary in linear viscoelasticity theory: once the creep function is known, the assumption of linear response is by itself sufficient to determine the strain for any stress history (the Boltzmann superposition principle). As was mentioned before, a mathematical theory of materials with memory, without internal variables, exists for nonlinear behavior as well. The theory, however, has proved too abstract for application to the description of real materials. Virtually all constitutive models that are used for nonlinear inelastic materials rely on internal variables.
1.5.3.
Internal Variables: General Theory
Internal Variables and Thermomechanics An equilibrium state of a system is a state that has no tendency to change with no change in the external controls. In the thermomechanics of an inelastic continuum with internal variables, a local state (σ, T, ξ) may be called a local equilibrium state if the internal variables remain constant at constant stress and temperature, or, in view of Equation (1.5.1), if gα (σ, T, ξ) = 0,
α = 1, ..., n.
In an elastic continuum, every local state is an equilibrium state, though the continuum need not be globally in equilibrium: a nonuniform temperature field will cause heat conduction and hence changes in the temperature. The existence of nonequilibrium states is an essential feature of ratedependent inelastic continua; such states evolve in time by means of irreversible processes, of which creep and relaxation are examples.1 The thermomechanics of inelastic continua consequently belongs to the domain of the thermodynamics of irreversible processes (also known as nonequilibrium thermomechanics). The fundamental laws of thermodynamics 1 A process is reversible if the equations governing it are unaffected when the time t is replaced by −t; otherwise it is irreversible. In the rateindependent plastic continuum, which forms the main subject of this book, irreversible processes occur even in the absence of nonequilibrium states, as is seen in Chapter 3.
66
Chapter 1 / Introduction to Continuum Thermomechanics
discussed in 1.4.1 are assumed to be valid in this domain as well, but there is no full agreement in the scientific community about the meaning of such variables as the entropy and the temperature, which appear in the second law, or about the range of validity of this law (there is no comparable controversy about the first law). Entropy and temperature were defined in 1.4.1 for thermoelastic continua only; in other words, they are intrinsically associated with equilibrium states. The assumption that these variables are uniquely defined at nonequilibrium states as well, and obey the Clausius–Duhem inequality at all states, represents the point of view of the “rational thermodynamics” school, most forcefully expounded by Truesdell [1984] and severely criticized by Woods [1981]. For continua with internal variables, another point of view, articulated by Kestin and Rice [1970] and Bataille and Kestin [1975] (see also Germain, Nguyen and Suquet [1983]), may be taken. According to this school of thought, entropy and temperature may be defined at a nonequilibrium state if one can associate with this state a fictitious “accompanying equilibrium state” at which the internal variables are somehow “frozen” so as to have the same values as at the actual (nonequilibrium) state. If we follow this point of view, then we are allowed to assume the existence of a freeenergy density given by ψ(ε, T, ξ) such that the entropy density and the stress may be derived from it in the same way as for elastic continua, with the internal variables as parameters. Consequently the stress is given by Equation (1.4.7) if it is entirely determined by ε, T, ξ, and the entropy density is given by η = −∂ψ/∂T . In any statement of the second law of thermodynamics, however, the internal variables must be “unfrozen,” since this law governs irreversible processes. Let us assume that the second law is expressed by the local Clausius–Duhem inequality (1.4.5), and let us rewrite this inequality as ρη˙ − T −1 (ρr − ∇ · h) + h · ∇T −1 = ργ ≥ 0. With the help of the local energybalance equation (1.4.1), the expression in parentheses may be replaced by ρu˙ − σij ε˙ ij , and, since the definition of the ˙ the lefthand side of the freeenergy density ψ leads to T η˙ − u˙ = −(η T˙ + ψ), inequality becomes 1 h · ∇T −1 − ρT −1 (ψ˙ + η T˙ − σij ε˙ ij ). ρ Furthermore, ∂ψ ∂ψ ˙ X ∂ψ ˙ ψ˙ = ε˙ ij + ξα . T+ ∂εij ∂T α ∂ξα With η and σ expressed in terms of ψ, the lefthand side of (1.4.5) — that
Section 1.5 / Constitutive Relations: Inelastic
67
is, the internal entropy production — becomes h · ∇T −1 − ρT −1
X ∂ψ ξ˙α . α
∂ξα
(1.5.2)
This quantity must be nonnegative in any process and at any state, and in particular when the temperature gradient vanishes. The Clausius–Duhem inequality is therefore obeyed if and only if, in addition to the already mentioned heatconduction inequality h · ∇T −1 ≥ 0, the material also obeys the dissipation inequality (Kelvin inequality) D=
X
pα ξ˙α ≥ 0,
(1.5.3)
∂ψ ∂ξα
(1.5.4)
α
where pα = −ρ
is the “thermodynamic force” conjugate to ξα . The preceding results must be generalized somewhat if the material possesses viscosity in the sense that generalizes the Newtonian model: the stress depends continuously1 on the strainrate tensor ε˙ in addition to the thermodynamic state variables ε, T, ξ. The definition of a local equilibrium state now requires the additional condition ε˙ = 0. The stress in the accompanying equilibrium state is still given (by definition) by ρ ∂ψ/∂εij , but it is not ˙ Instead, it equals equal to the actual stress σ(ε, T, ξ; ε). def
σ(ε, T, ξ; 0) = σ e (ε, T, ξ) (equilibrium stress or elastic stress). If the viscous stress is defined as σ v = vε σ − σ e , then the additional term T −1 σij ˙ ij must be added to the internal vε entropy production as expressed by (1.5.2). The quantity σij ˙ ij is the viscous dissipation, and must also be nonnegative. If the decomposition of the strain into elastic and inelastic parts is assumed to take the form ε = εe (σ, T ) + εi (ξ), then, as was shown by Lubliner [1972], such a decomposition is compatible with the existence of a freeenergy density ψ(ε, ξ, T ) if and only if ψ can be decomposed as ψ(ε, T, ξ) = ψ e (ε − εi (ξ), T ) + ψ i (ξ, T ). 1
(1.5.5)
The continuity of the dependence of the stress on the strain rate is what distinguishes viscosity from, say, dry friction.
68
Chapter 1 / Introduction to Continuum Thermomechanics
The Kelvin inequality then takes the special form D = Di − ρ
X ∂ψ i ξ˙α ≥ 0, α
∂ξα
def
where Di = σij ε˙ iij is the inelastic work rate per unit volume. Note that this rate may be negative, without violating the second law of thermodynamics, if ψ i decreases fast enough, that is, if enough stored inelastic energy is liberated. The contraction of muscle under a tensile force, driven by chemical energy, is an example of such a process.
The Nature of Internal Variables What are internal variables in general? In principle, they may be any variables which, in addition to the strain (or stress) and temperature, define the local state in a small2 neighborhood of a continuum. As we have seen, the components of εi themselves may or may not be included among the internal variables. As a general rule, internal variables may be said to be of two types. On the one hand, they may be “physical” variables describing aspects of the local physicochemical structure which may change spontaneously; for example, if the material can undergo a chemical reaction or a change of phase, then a quantity describing locally the extent of the reaction or the relative density of the two phases may serve as an internal variable. Other internal variables of this type include densities of structural defects, as discussed in Chapter 2. On the other hand, internal variables may be mathematical constructs; they are then called phenomenological variables. The inelastic strain εi itself is of this type, as are the dashpot displacements in viscoelastic models. Here the form of the functional dependence of the stress (or strain) on the internal variables, and of their rate equations, is assumed a priori. In the simplest constitutive models describing nonlinear inelastic materials, the internal variables are often assumed to consist of the εiij and an additional variable κ, called a hardening variable. The rate equation for κ is further assumed to be related to the rate equations for the εiij in such a way κ˙ = 0 whenever ε˙ i = 0, but, in a cyclic process at the end of which the εiij return to their original values (see Figure 1.5.2), κ will have changed. Usually, κ is defined so that κ˙ > 0 whenever ε˙ i 6= 0. Two commonly used definitions of κ are, first, the inelastic work , defined as Z
κ= 2
def
Di dt = Wi ,
(1.5.6)
“Small” means small enough so that the state may be regarded as uniform, but large enough for the continuum viewpoint to be valid.
Section 1.5 / Constitutive Relations: Inelastic
69
σ
ε
Figure 1.5.2. Closed stressstrain cycle with inelastic deformation: the inelastic strain returns to zero at the end of the cycle, but the internal state may be different, so that internal variables other than the inelastic strain may be necessary. and second, the equivalent (or effective) inelastic strain, Z r
κ=
2 i i def ε˙ ij ε˙ ij dt = ¯εi . 3
(1.5.7)
The reason for the traditional factor of 23 in the latter definition (which is due to Odqvist [1933]) is the following: if a specimen of a material that is (a) isotropic and (b) characterized by inelastic incompressibility (so that ε˙ ikk = 0) is subjected to a uniaxial tensile or compressive stress, then the inelastic strainrate tensor must be given by
0 0 ε˙ i i 0 , ε˙ = 0 − 12 ε˙ i i 0 0 − 12 ε˙ q
so that 23 ε˙ iij ε˙ iij is just equal to ˙εi . In practice there is little difference in the way the two types of internal variables are used.1 Whether the functions involved are provided by physical theory or by hypothesis, they contain parameters that must be evaluated by comparison of theoretical predictions with experimental results. It is seen in Chapter 2 that in the case of metal plasticity, physical theory has been remarkably successful in providing a qualitative understanding of the phenomena, but attempts to generate constitutive equations in terms of physical variables have not met with success.
1.5.4.
Flow Law and Flow Potential
Regardless of whether the inelastic strain components are directly included among the internal variables, it is always possible to define a flow law , that 1
As is seen in Section 3.1, phenomenological variables are sometimes given physicalsounding names.
70
Chapter 1 / Introduction to Continuum Thermomechanics
is, a rate equation for εi , by applying the chain rule to the basic assumption εi = εi (ξ). The result is ε˙ iij = gij (σ, T, ξ), where gij =
X ∂εiij α
∂ξα
gα ,
the gα being the righthand sides of Equation (1.5.1). Mainly for convenience, it is often assumed that the gij can be derived from a scalar function g(σ, T, ξ), called a flow potential , by means of gij = φ
∂g , ∂σij
φ(σ, T, ξ) being a positive scalar function. The flow potential g is commonly assumed to be a function of the stress alone, the most frequently used form being g(σ, T, ξ) = J2 , where J2 is the second stressdeviator invariant defined in 1.3.2. Since ∂ ∂skl ∂ J2 = ∂σij ∂σij ∂skl
1 1 smn smn = δik δjl − δij δkl skl = sij , 2 3
it follows that the flow law has the form ε˙ iij = φ(σ, T, ξ)sij .
(1.5.8)
One consequence of this flow law is that inelastic deformation is volumepreserving, or, equivalently, that volume deformation is purely elastic — a result that is frequently observed in real materials.
Generalized Potential and Generalized Normality A stronger concept of the flow potential is due to Moreau [1970] and Rice [1970, 1971] (see also Halphen and Nguyen [1975]). A function Ω of σ, T, ξ is assumed to depend on stress only through the thermodynamic forces pα , defined by (1.5.4), conjugate to the internal variables ξα , that is, def Ω = Ω(p, T, ξ)r, where p = {p1 , ..., pn }. It is further assumed that the rate equations are ∂Ω ξ˙α = . (1.5.9) ∂pα Equations (1.5.9) represent the hypothesis of generalized normality, and Ω is called a generalized potential . The thermodynamic forces pα can be obtained as functions of σ by means of the complementary freeenergy density χ(σ, T, ξ) (also called the freeenthalpy density or Gibbs function), defined by χ = ρ−1 σij εij − ψ,
Section 1.5 / Constitutive Relations: Inelastic
71
where ψ is the Helmholtz freeenergy density. It can easily be shown that pα = ρ and εij = ρ
∂χ ∂ξα
∂χ . ∂σij
It follows that ε˙ iij =
X ∂pα ∂2χ ˙ ξα = ξ˙α . ∂σij ∂ξα α ∂σij
X ∂εij X ξ˙α = ρ α
∂ξα
α
Combining with (1.5.9), we find ε˙ iij =
X ∂Ω ∂pα
∂pα ∂σij
α
or ε˙ iij =
,
∂Ω . ∂σij
(1.5.10)
A sufficient condition for the existence of a generalized potential was found by Rice [1971]. The condition is that each of the rate functions gα (σ, T, ξ) depends on the stress only through its own conjugate thermodynamic force pα : ∂Ωα ξ˙α = gˆα (pα , T, ξ) = , ∂pα where, by definition, pα
Z
gˆα (pα , T, ξ) dpα .
Ωα (pα , T, ξ) = 0
If we now define Ω(p, T, ξ) =
X
Ωα (pα , T, ξ),
α
then Equations (1.5.9)–(1.5.10) follow. The preceding results are independent of whether the inelastic strain components εiij are themselves included among the internal variables. For mathematical reasons, the generalized potential Ω is usually assumed to be a convex function of p, that is, with the remaining variables not shown, Ω(tp + (1 − t)p∗ ) ≤ tΩ(p) + (1 − t)Ω(p∗ ) for any admissible p, p∗ and any t such that 0 ≤ t ≤ 1. It follows from this definition that (∂Ω/∂p) · (p − p∗ ) ≥ Ω(p) − Ω(p∗ ), (1.5.11)
72
Chapter 1 / Introduction to Continuum Thermomechanics
where ∂Ω/∂p is evaluated at p, and the dot defines the scalar product in ndimensional space. Thus, for any p∗ such that Ω(p∗ ) ≤ Ω(p), (p−p∗ )· ξ˙ ≥ 0. The hypothesis of generalized normality has often been invoked in constitutive models formulated by French researchers, though not always consistently. An example is presented when constitutive theories of plasticity and viscoplasticity are discussed in detail. Before such a discussion, however, it is worth our while to devote a chapter to the physical bases underlying the theories. We return to theory in Chapter 3.
Exercises: Section 1.5 1. Consider a model of linear viscoelasticity made up of a spring of modulus E∞ in parallel with a Maxwell model consisting of a spring of modulus E 0 and a dashpot of viscosity η 0 . (a) If the dashpot displacement constitutes the internal variable, find the relation among the stress σ, the strain ε, and ξ. (b) Find the rate equation for ξ (i ) in terms of ε and ξ and (ii ) in terms of σ and ξ. (c) Show that a model of the type shown in Figure 1.5.1(a) can be found that is fully equivalent to the present one, and find the relations between the parameters E0 , E1 , η of that model and those of the present one. 2. For a standard solid model with creep function given by 1 J(t) = − E∞
1 1 − e−t/τ , E∞ E0
find an expression for the strain as a function of stress when the stress history is such that σ = 0 for t < 0 and σ = ασ0 t/τ , α being a dimensionless constant and σ0 a reference stress. Assuming E0 /E∞ = 1.5, sketch plots of σ/σ0 against E∞ ε/σ0 for α = 0.1, 1.0, and 10.0. 3. Show that the relation between the uniaxial creep function J(t) and relaxation function R(t) of a linearly viscoelastic material is Z
t
J(t0 )R(t − t0 ) dt0 = t.
0
4. Show that if the freeenergy density is as given by Equation (1.5.5), and if the inelastic strain components εiij are themselves used as internal variables, then the conjugate thermodynamic forces are just the stress components σij .
Section 1.5 / Constitutive Relations: Inelastic
73
5. Show that if the freeenergy density is as given by Equation (1.5.5), and if in addition the specific heat C is independent of the internal variables, then the freeenergy density reduces to the form ψ(ε, T, ξ) = ψ e (ε − εi (ξ)) + ui (ξ) − T η i (ξ). Discuss the possible meaning of ui and η i . 6. Find the flow law derived from a flow potential given by g(σ, T, ξ) = f (I1 , J2 , J3 ). 7. Show that if χ(σ, T, ξ) is the complementary freeenergy density and pα is the thermodynamic force conjugate to ξα , then pα = ρ ∂χ/∂ξα .
74
Chapter 1 / Introduction to Continuum Thermomechanics
Chapter 2
The Physics of Plasticity Section 2.1
Phenomenology of Plastic Deformation
The adjective “plastic” comes from the classical Greek verb πλ ασσιν, ´ meaning “to shape”; it thus describes materials, such as ductile metals, clay, or putty, which have the property that bodies made from them can have their shape easily changed by the application of appropriately directed forces, and retain their new shape upon removal of such forces. The shaping forces must, of course, be of sufficient intensity — otherwise a mere breath could deform the object — but often such intensity is quite easy to attain, and for the object to have a useful value it may need to be hardened, for example through exposure to air or the application of heat, as is done with ceramics and thermosetting polymers. Other materials — above all metals — are quite hard at ordinary temperatures and may need to be softened by heating in order to be worked. It is generally observed that the considerable deformations which occur in the plastic shaping process are often accompanied by very slight, if any, volume changes. Consequently plastic deformation is primarily a distortion, and of the stresses produced in the interior of the object by the shaping forces applied to the surface, it is their deviators that do most of the work. A direct test of the plasticity of the material could thus be provided by producing a state of simple shearing deformation in a specimen through the application of forces that result in a state of shear stress. In a soft, semifluid material such as clay, or soil in general, this may be accomplished by means of a direct shear test such as the shearbox test, which is discussed in Section 2.3. In hard solids such as metals, the only experiment in which uniform simple shear is produced is the twisting of a thinwalled tube, and this is not always a simple experiment to perform. A much simpler test is the tension test. 75
76
2.1.1
Chapter 2 / The Physics of Plasticity
Experimental StressStrain Relations
Tension Tests Of all mechanical tests for structural materials, the tension test is the most common. This is true primarily because it is a relatively rapid test and requires simple apparatus. It is not as simple to interpret the data it gives, however, as might appear at first sight. J. J. Gilman [1969] The tensile test [is] very easily and quickly performed but it is not possible to do much with its results, because one does not know what they really mean. They are the outcome of a number of very complicated physical processes. . . . The extension of a piece of metal [is] in a sense more complicated than the working of a pocket watch and to hope to derive information about its mechanism from two or three data derived from measurement during the tensile test [is] perhaps as optimistic as would be an attempt to learn about the working of a pocket watch by determining its compressive strength. E. Orowan [1944] Despite these caveats, the tension test remains the preferred method of determining the material properties of metals and other solids on which it is easily performed: glass, hard plastics, textile fibers, biological tissues, and many others.
StressStrain Diagrams The immediate result of a tension test is a relation between the axial force and either the change in length (elongation) of a gage portion of the specimen or a representative value of longitudinal strain as measured by one or more strain gages. This relation is usually changed to one between the stress σ (force F divided by crosssectional area) and the strain ε (elongation divided by gage length or straingage output), and is plotted as the stressstrain diagram. Parameters that remain constant in the course of a test include the temperature and the rate of loading or of elongation. If significant changes in length and area are attained, then it is important to specify whether the area used in calculating the stress is the original area A0 (nominal or “engineering” stress, here to be denoted simply σe ) or the current area A (true or Cauchy stress, σt ) — in other words, whether the Lagrangian or the Eulerian definition is used — and whether the strain plotted is the change in length ∆l divided by the original length l0 (conventional or “engineering” strain, εe ) or the natural logarithm of the ratio of the current length l (= l0 + ∆l) to l0 (logarithmic or natural strain, εl ). Examples of stressstrain diagrams, both as σe versus εe and as σt versus εl , are shown in Figure 2.1.1. It is clear that the Cauchy stress, since it does not depend on the initial configuration, reflects the actual state in the specimen better than the nominal stress, and while both definitions of strain involve the initial length, the rates (time derivatives) of conventional and
Section 2.1 / Phenomenology of Plastic Deformation
77
˙ 0 and l/l, ˙ so that it is the latter that is logarithmic strain are respectively l/l independent of initial configuration. In particular, in materials in which it is possible to perform a compression test analogous to a tension test, it is often found that the stressstrain diagrams in tension and compression coincide to a remarkable degree when they are plots of Cauchy stress against logarithmic strain [see Figure 2.1.1(b)]. The rate of work done by the force is F l˙ = σe A0 l0 ε˙ e = σt Alε˙ l , so that σe ε˙ e and σt ε˙ l are the rates of work per unit original and current volume, respectively. While the calculation of Cauchy stress requires, strictly speaking, measurement of crosssectional area in the course of the test, in practice this is not necessary if the material is a typical one in which the volume does not change significantly, since the current area may be computed from the volume constancy relation Al = A0 l0 . As is shown in Chapter 8, the logarithmic strain rate ε˙ l has a natural and easily determined extension to general states of deformation, but the logarithmic strain itself does not, except in situations (such as the tension test) in which the principal strain axes are known and remain fixed. The use of the logarithmic strain in largedeformation problems with rotating principal strain axes may lead to erroneous results.
Compression Tests As seen in Figure 2.1.1(b), the results of a simple compression test on a specimen of ductile metal are virtually identical with those of a tensile test if Cauchy stress is plotted against logarithmic strain. The problem is that a “simple compression test” is difficult to achieve, because of the friction that is necessarily present between the ends of the specimen and the pressure plates. Compression of the material causes an increase in area, and therefore a tendency to slide outward over the plates, against the shear stress on the interfaces due to the frictional resistance. Thus the state of stress cannot be one of simple compression. Lubrication of the interface helps the problem, as does the use of specimens that are reasonably slender — though not so slender as to cause buckling — so that, at least in the middle portion, a state of simple compressive stress is approached. Unlike ductile metals, brittle solids behave quite differently in tension and compression, the highest attainable stress in compression being many times that in tension. Classically brittle solids, such as cast iron or glass, fracture almost immediately after the proportional limit is attained, as in Figure 2.1.1(c). Others, however, such as concrete and many rocks, produce stressstrain diagrams that are qualitatively similar to those of many ductile materials, as in Figure 2.1.1(d). Of course, the strain scale is quite different: in brittle materials the largest strains attained rarely exceed 1%. The stress peak represents the onset of fracture, while the decrease in slope of the stressstrain curve represents a loss in stiffness due to progressive crack
78
Chapter 2 / The Physics of Plasticity
σe (MPa) Nickelchrome steel
σ (MPa)
Mediumcarbon steel, heattreated
1200
1500
1500
(b0 )
1200
900
Coldrolled steel
Mediumcarbon steel, annealed Hard bronze + Lowcarbon steel Soft brass
900
600 300
Points having equal true strain
Compression, σe vs. εe
H ACj r CAUCW rr
600
Tension and compression, σt vs. εl Tension, σe vs. εe
r
300
Fracture
H Y H Annealed copper 10
20
30
40
50
εe (%)
10
20
30
40
50
ε (%)
(b)
(a) σ (MPa)
σ (MPa) 1200
r Glass, compression 30
900
r
600 300
Gray cast iron, compression
15
Compression
r Gray cast iron, tension r Tension
r Glass, tension 1
2
3
4
ε (%)
0.25
0.5
0.75
ε (%)
(d)
(c) σ1 − σ3
σ1 − σ3 (MPa)
Insensitive clay Dense sand, undisturbed sensitive clay
900 1000
)
800
600
A K A 6 A Confining pressure r400 300 r 200 (MPa) r 100 9
Loose sand, remolded sensitive clay
600
10
20 (e)
ε
ε (%) (f)
Figure 2.1.1. Stressstrain diagrams: (a) ductile metals, simple tension; (b) ductile metal (lowcarbon steel), simple tension and compression; (b’) yieldpoint phenomenon; (c) cast iron and glass, simple compression and tension; (d) typical concrete or rock, simple compression and tension; (e) rock (limestone), triaxial compression; (f) soils, triaxial compression.
Section 2.1 / Phenomenology of Plastic Deformation
79
ing. The postpeak portion of the curve is highly sensitive to test conditions and specimen dimensions, and therefore it cannot be regarded as a material property. Moreover, it is not compression per se that brings about fracture, but the accompanying shear stresses and secondary tensile stresses. Nevertheless, the superficial resemblance between the curves makes it possible to apply some concepts of plasticity to these materials, as discussed further in Section 2.3. Unless the test is performed very quickly, soils are usually too soft to allow the use of a compression specimen without the application of a confining pressure to its sides through air or water pressure. This confined compression test or triaxial shear test is frequently applied to rock and concrete as well, for reasons discussed in Section 2.3. The specimen in this test is in an axisymmetric, threedimensional stress state, the principal stresses being the longitudinal stress σ1 and the confining pressure σ2 = σ3 , both taken conventionally as positive in compression, in contrast to the usual convention of solid mechanics. The results are usually plotted as σ1 −σ3 (which, when positive — as it usually is — equals 2τmax ) against the compressive longitudinal strain ε1 ; typical curves are shown in Figure 2.1.1(e) and (f).
Elastic and Proportional Limits, Yield Strength Some of the characteristic features of tensile stressstrain diagrams for ductile solids when rate sensitivity may be neglected will now be described. Such diagrams are characterized by a range of stress, extending from zero to a limiting stress (say σo ) in which the stress is proportional to strain (the corresponding strains are normally so small that it does not matter which definitions of stress and strain are used); σo is called the proportional limit. Also, it is found that the same proportionality obtains when the stress is decreased, so that the material in this range is linearly elastic, described by the uniaxial Hooke’s law given by Equation (1.4.12), that is, σ = Eε. The range of stressstrain proportionality is thus also essentially the elastic range, and the proportional limit is also the elastic limit as defined in Section 1.5. When the specimen is stressed slightly past the elastic limit and the stress is then reduced to zero, the strain attained at the end of the process is, as a rule, different from zero. The material has thus acquired a permanent strain. Rate effects, which are more or less present in all solids, can distort the results. The “standard solid” model of viscoelasticity discussed in 1.5.1, for example, predicts that in a test carried out at a constant rate of stressing or of straining, the stressstrain diagram will be curved, but no permanent strain will be present after stress removal; the complete loadingunloading diagram presents a hysteresis loop. The curvature depends on the test rate; it is negligible if the time taken for the test is either very long or very short compared with the characteristic time τ of the model.
80
Chapter 2 / The Physics of Plasticity
Even in the absence of significant rate effects, it is not always easy to determine an accurate value for the elastic or proportional limit. Some materials, such as soft copper, present stressstrain curves that contain no discernible straight portions. In others, such as aluminum, the transition from the straight to the curved portion of the diagram is so gradual that the determination of the limit depends on the sensitivity of the strainmeasuring apparatus. For design purposes, it has become conventional to define as the “yield strength” of such materials the value of the stress that produces a specified value of the “offset” or conventional permanent strain, obtained by drawing through a given point on the stressstrain curve a straight line whose slope is the elastic modulus E (in a material such as soft copper, this would be the slope of the stressstrain curve at the origin). Typically used values of the offset are 0.1%, 0.2% and 0.5%. When this definition is used, it is necessary to specify the offset, and thus we would speak of “0.2% offset yield strength.”
2.1.2
Plastic Deformation
Plastic Strain, WorkHardening The strain defined by the offset may be identified with the inelastic strain as defined in 1.5.1. In the context in which rate sensitivity is neglected, this strain is usually called the plastic strain, and therefore, if it is denoted εp , it is given by σ εp = ε − . (2.1.1) E The plastic strain at a given value of the stress is often somewhat different from the permanent strain observed when the specimen is unloaded from this stress, because the stressstrain relation in unloading is not always ideally elastic, whether as a result of rate effects or other phenomena (one of which, the Bauschinger effect, is discussed below). Additional plastic deformation results as the stress is increased. The stressstrain curve resulting from the initial loading into the plastic range is called the virgin curve or flow curve. If the specimen is unloaded after some plastic deformation has taken place and then reloaded, the reloading portion of the stressstrain diagram is, like the unloading portion, approximately a straight line of slope E, more or less up to the highest previously attained stress (that is, the stress at which unloading began). The reloading then follows the virgin curve. Similar results occur with additional unloadings and reloadings. The highest stress attained before unloading is therefore a new yield stress, and the material may be regarded as having been strengthened or hardened by the plastic deformation (or coldworking). The increase of stress with plastic deformation is consequently called workhardening or strainhardening.
Section 2.1 / Phenomenology of Plastic Deformation
81
The virgin curve of workhardening solids, especially ones without a sharply defined yield stress, is frequently approximated by the Ramberg– Osgood formula σ σR σ m , (2.1.2) ε= +α E E σR where α and m are dimensionless constants,1 and σR is a reference stress. If m is very large, then εp remains small until σ approaches σR , and increases rapidly when σ exceeds σR , so that σR may be regarded as an approximate yield stress. In the limit as m becomes infinite, the plastic strain is zero when σ < σR , and is indeterminate when σ = σR , while σ > σR would produce an infinite plastic strain and is therefore impossible. This limiting case accordingly describes a perfectly plastic solid with yield stress σR . If the deformation is sufficiently large for the elastic strain to be neglected, then Equation (2.1.2) can be solved for σ in terms of ε: σ = Cεn ,
(2.1.3)
where C = σR (E/ασR )n , and n = 1/m is often called the workhardening exponent. Equation (2.1.3), proposed by Ludwik [1909], is frequently used in applications where an explicit expression for stress as a function of strain is needed. Note that the stressstrain curve representing (2.1.3) has an infinite initial slope. In order to accommodate an elastic range with an initial yield stress σE , Equation (2.1.3) is sometimes modified to read σE ε≤ , Eε, E n σ= (2.1.4) σE σE Eε , ε≥ . σE E
Ultimate Tensile Strength It must be emphasized that when the strain is greater than a few percent, the distinction between the different types of stress and strain must be taken into account. The decomposition (2.1.1) applies, strictly speaking, to the logarithmic strain. The nature of the stressstrain curve at larger strains is, as discussed above, also highly dependent on whether the stress plotted is nominal or true stress [see Figure 2.1.1(b)]. True stress is, in general, an increasing function of strain until fracture occurs. Since the crosssectional area of the specimen decreases with elongation, the nominal stress increases more slowly, and at a certain point in the test it begins to decrease. Since, very nearly, σe = σt exp(−εl ), it follows that dσe = (dσt − σt dεl )exp(−εl ), 1
If m is a number other than an odd integer, then size − 2(σ/σR )m may be replaced by size − 2σ/σR m−1 (σ/σR ) if the curve is the same for negative as for positive stress and strain.
82
Chapter 2 / The Physics of Plasticity
and therefore the nominal stress (and hence the load) is maximum when dσt = σt . dεl If Equation (2.1.3) is assumed to describe the flow curve in terms of Cauchy stress and logarithmic strain, then the maximum nominal stress can easily be seen to occur when εl = n. The maximum value of nominal stress attained in a tensile test is called the ultimate tensile strength or simply the tensile strength. When the specimen is extended beyond the strain corresponding to this stress, its weakest portion begins to elongate — and therefore also to thin — faster than the remainder, and so a neck will form. Further elongation and thinning of the neck — or necking — proceeds at decreasing load, until fracture.
Discontinuous Yielding The stressstrain curves of certain impuritycontaining metals, such as mild steel and nitrogencontaining brass, present a phenomenon known as discontinuous yielding. When the initial elastic limit is reached, suddenly a significant amount of stretching (on the order of 1 or 2%, and thus considerably larger than the elastic strain achieved up to that point) occurs at essentially constant stress, of a value equal to or somewhat lower than the initial elastic limit. If the value is the same, then it is called the yield point of the material. If it is lower, then it is called the lower yield point, while the higher value is called the upper yield point. The portion of the stressstrain diagram represented by the constant stress value is called the yield plateau, and the drop in stress, if any, that precedes it is called the yield drop. Following the plateau, workhardening sets in, as described above. Figure 2.1.1(b’) shows a typical stressstrain diagram for a material with a yield point. As shown in the figure, the stress on the plateau is not really constant but shows small, irregular fluctuations. They are due to the fact that plastic deformation in this stage is not a homogeneous process but concentrated in discrete narrow zones known as L¨ uders bands, which propagate along the specimen as it is stretched, giving rise to surface marks called stretcher strains. When a specimen of a material with a yield point is loaded into the workhardening range, unloaded, and reloaded soon after unloading, the virgin curve is regained smoothly as described previously. If, however, some time — of the order of hours — is allowed to elapse before reloading, the yield point recurs at a higher stress level (see Figure 2.1.2). This phenomenon is called strain aging.
Bauschinger Effect, Anisotropy
Section 2.1 / Phenomenology of Plastic Deformation
83
σ
E First loading 0
Immediate reloading
E Reloading after aging
ε
Figure 2.1.2. Strain aging
specimen of a ductile material that has been subjected to increasing tensile stress and then unloaded (“coldworked”) is different from a virgin specimen. We already know that it has a higher tensile yield stress. If, however, it is now subjected to increasing compressive stress, it is found that the yield stress in compression is lower than before. This observation is known as the Bauschinger effect [see Figure 2.1.3(a)]. The Bauschinger effect can be observed whenever the direction of straining is reversed, as, for example, compression followed by tension, or shearing (as in a torsion test on a thinwalled tube) followed by shearing in the opposite direction. More generally, the term “Bauschinger effect” can be used to describe the lowering of the yield stress upon reloading that follows unloading, even if the reloading is in the same direction as the original loading (Lubahn and Felgar [1961]) [see Figure 2.1.3(b)]. Note the hysteresis loop which appears with large strains, even at very slow rates of straining at which the viscoelastic effects mentioned above may be neglected. Another result of plastic deformation is the loss of isotropy. Following coldworking in a given direction, differences appear between the values of the tensile yield strength in that direction and in a direction normal to it. These differences may be of the order of 10%, but are usually neglected in practice.
Annealing, Recovery The term “coldworking” used in the foregoing discussions refers to plastic deformation carried out at temperatures below the socalled recrystallization temperature of the metal, typically equal, in terms of absolute temperature, to some 35 to 50% of the melting point (although, unlike the melting point, it is not sharply defined); the reason for the name is explained in the next section. The effects of coldworking, such as workhardening, the Bauschinger effect, and induced anisotropy, can largely be removed by a process called annealing, consisting of heating the metal to a relatively high tem
84
Chapter 2 / The Physics of Plasticity σ
1 6 Tension
? ε Compression
) σ (psi) 4000 σ
(103 30 28 26 24 22 20 18 16 14 12 10 8 6 4 2 0
psi)
3000 2000
(a)
a a a qa q q q a q qaq
0.04
qq
0.07
q
ε (%)
a
a
a qqa
q a a a a a qq qq q qq a qq a a aaqa q q a a a qqqqqqqqq 5.04 5.12 aaaaaaaqaaq l 0.22aqa 0.30a a aq a aaq a a
0.02
0.10 0.84
a
a
a
0.96
q
q
q q q q
q
q q q
q q a q a
qa
Copper, tension
a q
Initial loading and unloading Reloading
5.20 13.50
13.58
13.66
13.74
εe (%)
(b)
Figure 2.1.3. Bauschinger effect: (a) classical; (b) generalized (from Lubahn and Felgar [1961]).
perature (above the recrystallization temperature) and holding it there for a certain length of time before slowly cooling it. The length of time necessary for the process decreases with the annealing temperature and with the amount of cold work. Plastic deformation that takes place at temperatures in the annealing range (i.e., above the recrystallization temperature) is known as hotworking, and does not produce workhardening, anisotropy, or the Bauschinger effect. For metals with low melting points, such as lead and tin, the recrystallization temperature is about 0◦ C and therefore deformation at room temperature must be regarded as hotworking. Conversely, metals with very high melting points, such as molybdenum and tungsten (with recrystallization tempera
Section 2.1 / Phenomenology of Plastic Deformation
85
tures of 1100 to 1200◦ C can be “coldworked” at temperatures at which the metal is redhot. The recrystallization temperature provides a qualitative demarcation between stressstrain diagrams that show workhardening and those that do not. Within each of the two ranges, however, the stress needed to achieve a given plastic deformation at a given strain rate also depends on the temperature. In particular, it decreases with increasing temperature (see Figure 2.1.4). σt
T
@ R
((( εl
Figure 2.1.4. Temperature dependence of flow stress A characteristic of some metals (including mild steel), with important implications for design, is a change of behavior from ductile to brittle when the temperature falls below the socalled transition temperature. Softening (that is, a spontaneous decrease in yield strength) of workhardened metals also occurs at temperatures below recrystallization. This process, whose rate is considerably slower than that of annealing, is called recovery. The rate of recovery decreases with decreasing temperature, and is negligible at room temperature for such metals as aluminum, copper and steel. These metals may accordingly be regarded for practical purposes as workhardening permanently.
2.1.3
Temperature and Rate Dependence
The preceding discussion of the rates of annealing and recovery shows the close relationship between temperature and rate. A great many physicochemical rate processes — specifically, those that are thermally activated — are governed by the Arrhenius equation, which has the general form rate ∝ e−∆E/kT ,
(2.1.5)
86
Chapter 2 / The Physics of Plasticity
where k is Boltzmann’s constant (1.38 × 10−23 J/K), T is the absolute temperature, and ∆E is the activation energy of the process. The rate sensitivity of the workhardening stressstrain curve itself increases with increasing temperature. In a good many metals, the dependence on the plastic strain rate of the stress required to achieve a given plastic strain can be approximated quite well by ε˙ r , where the exponent r (sometimes called simply the rate sensitivity) depends on the plastic strain and the temperature, increasing with both. Some typical results for r, obtained from tests at strain rates between 1 and 40 per second, are shown in Table 2.1.1.
Table 2.1.1 Metal Aluminum
Copper
Mild steel
Temperature (◦ C) 18 350 550 18 450 900 930 1200
Value 10% 0.013 0.055 0.130 0.001 0.001 0.134 0.088 0.116
of r for a compression of 30% 50% 0.018 0.020 0.073 0.088 0.141 0.155 0.002 0.010 0.008 0.031 0.154 0.190 0.094 0.105 0.141 0.196
Source: Johnson and Mellor [1973]. The Arrhenius equation (2.1.5) permits, in principle, the simultaneous representation of the rate sensitivity and temperature sensitivity of the stressstrain relation by means of the parameter ε˙ exp(∆E/RT ), or, more generally, ε˙ f (T ), where f (T ) is an experimentally determined function, since the activation energy ∆E may itself be a function of the temperature.
Creep The preceding results were obtained from tests carried out at constant strain rate (since the strains are large, total and plastic strain need not be distinguished). Following Ludwik [1909], it is frequently assumed that at a given temperature, a relation exists among stress, plastic (or total) strain, and plastic (or total) strain rate, independently of the process, and therefore this relation also describes creep, that is, continuing deformation at constant stress. Such a relation is reminiscent of the “standard solid” model of viscoelasticity, in which this relation is linear. It will be recalled that this model describes both the rate dependence of the stressstrain relation (discussed above in this section) and the increasing deformation at constant stress known as creep, which in this case asymptotically attains a finite value (bounded creep), though in the limiting case of the Maxwell model it becomes steady creep. In fact, all linear springdashpot models of viscoelasticity lead
Section 2.1 / Phenomenology of Plastic Deformation
87
εc Creep curve at high stress and temperature Tertiary creep Secondary creep Standard creep curve
Primary creep Creep curve at low stress and temperature
t Figure 2.1.5. Typical creep curves for metals. to creep that is either bounded or steady. For metals, the relation, if it exists, is nonlinear — many different forms have been proposed — and therefore the resulting creep need not belong to one of the two types predicted by the linear models. Typical creep curves for a metal, showing the creep strain εc (equal to the total strain less the initial strain) as a function of time at constant stress and temperature, are shown in Figure 2.1.5. The standard curve is conventionally regarded as consisting of three stages, known respectively as primary (or transient), secondary (or steady), and tertiary (or accelerating) creep, though not all creep curves need contain all three stages. At low stresses and temperatures, the primary creep resembles the bounded creep of linear viscoelasticity, with a limiting value attained asymptotically, and secondary and tertiary creep never appear. At higher stress or temperature, however, the primary creep shows a logarithmic or a power dependence on time: εc ∝ ln t or εc ∝ tα , where α is between 0 and 1, a frequently observed value being 31 (Andrade’s creep law). The logarithmic form is usually found to prevail below, and the power form above, the recrystallization temperature. Creep described by the power law can be derived from a formula relating stress, creep strain and creepstrain rate that has the form (due to Nadai [1950]) σ = C(εc )n (˙εc )r , (2.1.6) where C, n, and r depend on the temperature; this formula reduces to the Ludwik equation (2.1.3) at constant strain rate, and implies a rate sensitivity
88
Chapter 2 / The Physics of Plasticity
that is independent of the strain. At constant stress, the equation can be integrated, resulting in a power law with α = r/(n + r). Tertiary (accelerating) creep is generally regarded as resulting from structural changes leading to a loss of strength and, eventually, fracture. Whether secondary (steady) creep really takes place over a significant time interval, or is merely an approximate description of creep behavior near an inflection point of the creep curve, is not certain (see Lubahn and Felgar [1961], pp. 136–141). In either case, however, one may speak of a minimum creep rate characteristic of the metal at a given stress and temperature, if these are sufficiently high. At a given stress, the temperature dependence of this minimum creep rate is usually found to be given fairly closely by the Arrhenius equation. Its dependence on stress at a given temperature can be approximated by an exponential function at higher stresses, and by a power function of the form ε˙ cmin ∝ σ q , where q is an exponent greater than 1 (the frequently used Bailey–Norton–Nadai law), at lower stresses. (Note that Equation (2.1.6) describes the Bailey–Norton law if n = 0 and r = 1/q.) A commonly used approximation for the creep strain as a function of time, at a given stress and temperature, is εc (t) = εc0 + ε˙ cmin t, where ε˙ cmin is the minimum creep rate, and εc0 is a fictitious initial value defined by the εc intercept of the straight line tangent to the actual creep curve at the point of inflection or in the steadycreep portion. In many materials at ordinary temperatures, ratedependent inelastic deformation is insignificant when the stress is below a yield stress. A simple model describing this effect is the Bingham model: σ < σY , 0, i ε˙ = σ σ 1− Y , σ ≥ σY ,
σ
(2.1.7)
η
where η is a viscosity, and the yield stress σY may depend on strain. The Bingham model is the simplest model of viscoplasticity. Its generalizations are discussed in Section 3.1.
Exercises: Section 2.1 1. Show that the relation between the conventional strain εe and the logarithmic strain εl is εl = ln(1 + εe ). 2. It is assumed that the stressstrain relations of isotropic linear elasticity, with Young’s modulus E and Poisson’s ratio ν, are exact in terms of true stress and logarithmic strain. For uniaxial stress, find the relation (parametric if necessary) between the conventional stress and the
Section 2.2 / Crystal Plasticity
89
conventional strain. Show that the secondorder approximation to the relation is σe = E[εe − ( 12 + 2ν)ε2e ]. 3. A uniaxial tension test produces a curve of true stress against logarithmic strain that is fitted by σt = 2 × 105 εl in the elastic range and 1/6 σt = 635εl in the plastic range, with stresses in MPa. Determine (a) the elasticlimit stress, (b) the logarithmic and conventional strains at maximum load, and (c) the true and conventional stresses at maximum load, assuming negligible volume change. 4. If the reference stress σR in the Ramberg–Osgood formula (2.1.2) is the offset yield strength for a given permanent strain εR , find α in terms of σR , εR , and E. 5. Find a formula describing a stressstrain relation that (a) is linear for σ < σE , (b) asymptotically tends to ε ∝ σ m , and (c) is smooth at σ = σE . 6. Suppose that in Equation (2.1.6) only C depends on the temperature. Show that, for a given stress, the creep curves corresponding to different temperatures are parallel if they are plotted as creep strain against the logarithm of time. 7. Determine the form of the creep law resulting from Equation (2.1.6). 8. Assuming ε = σ/E + εc , and letting n = 0 in Equation (2.1.6), determine the resulting relaxation law, i. e. σ as a function of t when a strain ε is suddenly imposed at t = 0 and maintained thereafter. 9. To what does the Bingham model described by Equation (2.1.7) reduce when σY = 0? When η = 0?
Section 2.2 2.2.1
Crystal Plasticity
Crystals and Slip
Crystal Structure Plasticity theory was developed primarily in order to describe the behavior of ductile metals. Metals in their usual form are polycrystalline aggregates, that is, they are composed of large numbers of grains, each of which has the structure of a simple crystal. A crystal is a threedimensional array of atoms forming a regular lattice; it may be regarded as a molecule of indefinite extent. The atoms vibrate
90
Chapter 2 / The Physics of Plasticity
about fixed points in the lattice but, by and large, do not move away from them, being held more or less in place by the forces exerted by neighboring atoms. The forces may be due to ionic, covalent, or metallic bonding. Ionic bonds result from electron transfer from electropositive to electronegative atoms, and therefore can occur only in compounds of unlike elements. Ionic crystal structures range from very simple, such as the sodium chloride structure in which Na+ and Cl− alternate in a simple cubic array, to the very complex structures found in ceramics. Covalent bonds are due to the sharing of electrons, and are found in diamond and, to some extent, in crystalline polymers. In a metallic crystal, the outer or valence electrons move fairly freely through the lattice, while the “cores” (consisting of the nucleus and the filled shells of electrons) vibrate about the equilibrium positions. The metallic bond is the result of a rather complex interaction among the cores and the “free” electrons. It is the free electrons that are responsible for the electrical and thermal conductivity of metals. s X X XX sX s X X s X X XX Xs s X XXX s c cX X X c c X X X s c X X Xc X X X s sX XXX s (a)
s s , \ , @ , s , , , \@ \
[email protected] s , \, l l @
[email protected] c l @ l @ls c ls @ , @\ , , @\c ,, @ s s , @ \ , (b)
s ,
s ,
, , s , c
c
, , s , s ,
, s,
, , s ,
,
(c)
Figure 2.2.1. Crystal structures: (a) hexagonal closepacked (hcp); (b) facecentered cubic (fcc); (c) bodycentered cubic (bcc). The most common crystal structures in metals are the hexagonal closepacked (hcp), facecentered cubic (fcc) and bodycentered cubic (bcc), shown in Figure 2.2.1. Because of the random orientation of individual grains in a typical metallic body, the overall behavior of the aggregate is largely isotropic, but such phenomena as the Bauschinger effect and preferred orientation, which occur as a result of different plastic deformation of grains with different orientations, demonstrate the effect of crystal structure on plastic behavior. It is possible, however, to produce specimens of crystalline solids — not only metals — in the form of single crystals of sufficiently large size to permit mechanical testing.
Crystal Elasticity The linear elastic behavior of a solid is described by the elastic modulus matrix C defined in 1.4.2. The most general anisotropic solid has 21 inde
Section 2.2 / Crystal Plasticity
91
pendent elements of C. For the isotropic solid, on the other hand, the only nonzero elements of C are (a) C11 = C22 = C33 , (b) C44 = C55 = C66 , and (c) C12 = C13 = C23 (the symmetry CIJ = CJI is not explicitly shown). But only two of the three values are independent, since C11 = λ + 2µ, C44 = µ, and C12 = λ, so that 1 C44 = (C11 − C12 ). 2 In a crystal with cubic symmetry (such as simple cubic, fcc or bcc), with the Cartesian axes oriented along the cube edges, the nonzero elements of C are the same ones as for the isotropic solid, but the three values C11 , C12 and C44 are independent. It may, of course, happen fortuitously that the isotropy condition expressed by the preceding equation is satisfied for a given cubic crystal; this is the case for tungsten. A crystal with hexagonal symmetry is isotropic in the basal plane. Thus, if the basal planes are parallel to the x1 x2 plane, C66 = 21 (C11 − C12 ). The following elements of C are independent: (a) C11 = C22 , (b) C33 , (c) C12 , (d) C13 = C23 , and (e) C44 = C55 . The anisotropy of crystals is often studied by performing tension tests on specimens with different orientations, resulting in orientationdependent values of the Young’s modulus E. If the maximum and minimum values are denoted Emax and Emin , respectively, while Eave denotes the polycrystalline average, the anisotropy index may be defined as (Emax − Emin )/Eave . Values range widely: 1.13 for copper, 0.73 for αiron, 0.2 for aluminum, and, as indicated above, zero for tungsten.
Crystal Plasticity Experiments show that plastic deformation is the result of relative motion, or slip, on specific crystallographic planes, in response to shear stress along these planes. It is found that the slip planes are most often those that are parallel to the planes of closest packing; a simple explanation for this is that the separation between such planes is the greatest, and therefore slip between them is the easiest, since the resistance to slip as a result of interatomic forces decreases rapidly with interatomic distance. Within each slip plane there are in turn preferred slip directions, which once more are those of the atomic rows with the greatest density, for the same reason. A slip plane and a slip direction together are said to form a slip system. In hcp crystals, which include zinc and magnesium, the planes of closest packing are those containing the hexagons, and the slip directions in those planes are parallel to the diagonals. Hexagonal closepacked crystals therefore have three primary slip systems, although at higher temperatures other, secondary, slip systems may become operative. Facecentered cubic crystals, by contrast, have twelve primary slip systems: the closepacked planes are the four octahedral planes, and each con
92
Chapter 2 / The Physics of Plasticity
tains three face diagonals as the closestpacked lines. As a result, fcc metals, such as aluminum, copper, and gold, exhibit considerably more ductility than do hcp metals. In bodycentered cubic crystals there are six planes of closest packing and two slip directions in each, for a total of twelve primary slip systems. However, the difference in packing density between the closestpacked planes and certain other planes is not great, so that additional slip systems become available even at ordinary temperatures. Consequently, metals having a bcc structure, such as αiron (the form of iron found at ordinary temperatures), tungsten, and molybdenum, have a ductility similar to that of fcc metals. The preceding correlation between ductility and lattice type is valid in very broad terms. Real metal crystals almost never form perfect lattices containing one type of atom only; they contain imperfections such as geometric lattice defects and impurity atoms, besides the grain boundaries contained in polycrystals. In fact, these imperfections are the primary determinants of crystal plasticity. Ductility must therefore be regarded as a structuresensitive property, as are other inelastic properties. It is only the thermoelastic properties discussed in 1.4.1 — the elastic moduli, thermal stress (or strain) coefficients, and specific heat — that are primarily influenced by the ideal lattice structure, and are therefore called structureinsensitive.
Slip Bands In principle, slip in a single crystal can occur on every potential slip plane when the necessary shear stress is acting. Observations, however, show slip to be confined to discrete planes.1 When a slip plane intersects the outer surface, an observable slip line is formed, and slip lines form clusters called slip bands. In a given slip band, typically, a new slip line forms at a distance of the order of 100 interatomic spacings from the preceding one when the amount of slip on the latter has reached something of the order of 1,000 interatomic spacings. It follows from these observations that slip does not take place by a uniform relative displacement of adjacent atomic planes.
Critical Resolved Shear Stress It was said above that slip along a slip plane occurs in response to shear stress on that plane. In particular, in a tensile specimen of monocrystalline metal in which the tensile stress σ acts along an axis forming an angle φ with the normal to the slip plane and an angle λ with the slip direction, then the relation between σ and the resolved shear stress on the slip plane and in the slip direction, τ , is σ = (cos φ cos λ)−1 τ. (2.2.1) It was found by Schmid [1924], and has been confirmed by many experiments, 1
Or, more generally, surfaces (slip surfaces), since slip may transfer from one slip plane to another which intersects it in the interior of the crystal, especially in bcc metals.
Section 2.2 / Crystal Plasticity
93
that slip in a single crystal is initiated when the resolved shear stress on some slip system reaches a critical value τc , which is a constant for a given material at a given temperature and is known as the critical resolved shear stress. This result is called Schmid’s law. The critical resolved shear stress is, as a rule, very much higher for bcc metals (iron, tungsten) than for fcc metals (aluminum, copper) or hcp metals (zinc, magnesium).
Theoretical Shear Strength A value of the shear stress necessary to produce slip may be calculated by assuming that slip takes place by the uniform displacement of adjacent atomic planes. Consider the twodimensional picture in Figure 2.2.2: two d * τ h h h h6
?h
h
h
x h 
h
h h

h h

d 2
h
h
h h
h h
)τ Figure 2.2.2. Slip between two neighboring rows of atoms neighboring rows of atoms, the distance between the centers of adjacent atoms in each row being d, and the distance between the center lines of the two rows being h. Suppose the two rows to be in a stable equilibrium configuration under zero stress. If one row is displaced by a distance d relative to the other, a new configuration is achieved that is indistinguishable from the first. A displacement of d/2, on the other hand, would lead to an unstable equilibrium configuration at zero stress. As a first approximation, then, the shear stress necessary to produce a relative displacement x may be assumed to be given by τ = τmax sin
2πx , d
(2.2.2)
and slip would proceed when τ = τmax . When the displacement x is small, the stressdisplacement relation is approximately linear: τ = 2πτmax x/d. But a small displacement x between rows a distance h apart corresponds to a lattice shear of γ = x/h, and Hooke’s law in shear reads τ = Gγ [Equation (1.4.15)]. Consequently, Gd τmax = . 2πh Since h ≡ d, the value G/6 is a first, structureinsensitive approximation to the socalled theoretical shear strength of a crystal. More refined calculations that take actual crystal structures into account reduce the value of the theoretical shear strength to about G/30. In reality, however, the shear strength of single crystals is less than this by one to three orders of magnitude, that is, it is of order 10−3 G to 10−5 G. Only in
94
Chapter 2 / The Physics of Plasticity
socalled whiskers, virtually perfect crystals about 1 µm in diameter, is a shear strength of the theoretical order of magnitude observed.
2.2.2.
Dislocations and Crystal Plasticity
The discrepancy between theoretical and observed shear strength, as well as the observation of slip bands, have led to the inevitable conclusion that slip in ordinary crystals must take place by some mechanism other than the movement of whole planes of atoms past one another, and that it is somehow associated with lattice defects. A mechanism based on a specific defect called a dislocation was proposed independently by G. I. Taylor [1934] and E. Orowan [1934].
Defects in Crystals All real crystals contain defects, that is, deviations from the ideal crystal structure. A defect concentrated about a single lattice point and involving only a few atoms is called a point defect; if it extends along a row of many atoms, it is called a line defect; and if it covers a whole plane of atoms, a planar defect. Point defects are shown in Figure 2.2.3. They may be purely structural, such as (a) a vacancy or (b) an interstitial atom, or they may involve foreign atoms (impurities): (c) a substitutional impurity, (d) an interstitial impurity. As shown in the figure, point defects distort the crystal lattice locally, hhhhhhhhhhh h h hhh h h h h h h h h h h h h hh hh h hh h h h h h h h h hhh hhhhhhhhhhh (a)
(b)
hhhhhhhh h h h h hh hh w h h zh h h h h hhhhhhhh hhhhhhhh (c)
(d)
Figure 2.2.3. Point defects: (a) vacancy; (b) interstitial atom; (c) substitutional impurity; (d) interstitial impurity. the distortion being significant over a few atomic distances but negligible farther away. Planar defects, illustrated in Figure 2.2.4, include (a) grain boundaries in polycrystals, and within single crystals, (b) twin boundaries and (c) stacking faults.
Dislocations The most important line defects in crystals are dislocations. The concept of a dislocation has its origin in continuum mechanics, where it was introduced by V. Volterra. Consider a hollow thickwalled circular cylinder in which a radial cut, extending through the wall, is made [see Figure
Section 2.2 / Crystal Plasticity d d P d d P Ad P d dP d d d A d P Ad P d P Pd d P A P AA d d d d d P P A P d d d P d d d P d Ad P A Ad P d d P d dP P A P P d d d A A d P P d d Pd d A P P d d A Ad P d d d Pd P d P d Ad P d dP A A dPd P d dP d Ad d P d A A Pd P d A P d P A dPd (a) d Z Zd d d Zd dZ Zd Z Zd d Zd d Z Z d Z Z d d Z dd d d Z Z Z d d Z dZ d d d d Z ZdZ d Z dZ d d d d d Z dd d d d d d d d d d d (b)
95
(i)
C 4 B 4 A 4 C 4 B 4 A 4 C
B 4 A 4 C (ii) 4 B 4 A 4 C
C 4B
4C
4 4 4 4 4 4
B 4A 4C 5A 5B 4A 4C
4 4 4 4 4
4A 5B 4A
Stacking faults in a facecentered cubic lattice. The normal stacking sequence of (111) planes is denoted by ABCA... Planes in normal relation to one another are separated by 4, those with a stacking error by 5; (i) intrinsic stacking fault, (ii) extrinsic stacking fault.
(c) (from Hull and Bacon [1984])
Figure 2.2.4. Planar defects: (a) grain boundary; (b) twin boundary; (c) stacking fault.
2.2.5(a)]. The two faces of the cut may be displaced relative to each other by a distance b, either in the (b) radial or (c) axial direction, and then reattached. The result is a Volterra dislocation, with Figures 2.2.5(b) and (c) X X (a)
b X z y X . . . . . . . . . . . . . .. . ....... . . . . . . ..... .... . ....... .. . . . . . . .... ... . ....... ... . . . . . .. b . .. . .. .. X ........ .. X . XX X .. X = X X X X > (b) (c)
Figure 2.2.5. Volterra dislocation: (a) Volterra cut; (b) edge dislocation; (c) screw dislocation. representing respectively an edge and a screw dislocation. When the rough edges are smoothed, the result is a cylinder looking much as it did before the operation, but containing a selfequilibrating internal stress field. If the material is isotropic and linearly elastic, then the stress and displacement fields can be calculated by means of the theory of elasticity. In particular,
96
Chapter 2 / The Physics of Plasticity
the strain energy per unit length of cylinder is found to be W0 =
Gb2 R ln − 1 4π(1 − ν) a
(2.2.3a)
for an edge dislocation and W0 =
R Gb2 ln − 1 4π a
(2.2.3b)
for a screw dislocation, where G is the shear modulus, ν is the Poisson’s ratio, and R and a are respectively the outer and inner radii of the cylinder. An edge dislocation in a crystal can be visualized as a line on one side of which an extra halfplane of atoms has been introduced, as illustrated in Figure 2.2.6(a) for a simple cubic lattice. At a sufficient number of atomic distances away from the dislocation line, the lattice is virtually undisturbed. Consider, now, a path through this “good” crystal which would be closed if the lattice were perfect. If such a path, consisting of the same number of atomtoatom steps in each direction, encloses a dislocation, then, as shown in the figure, it is not closed; the vector b needed to close it is called the Burgers vector of the dislocation, and the path defining it is called the Burgers circuit.
b
b
b
b
b
b
b
b
b
b b b b b b
b
b
b
b
b b Burgers circuit 9 b b b
b
b
b
b
b
b
b
b
b
b
b
b
b
b
b
b
b
b
b
b
b ?b b b
b
b
b
b
b
b
b 6b b b
b
b b
(a)
b 6b b r r b b b b
b
cq
cq
cq
cq
cq
cq
q Atoms above
the slip plane
cAtoms below
qEc qEc qEc qEc qEc qEc the slip plane E E E E E E q c q c q c q c q c q c E E E E E E CO E E E E E q cq cq cq cq cq E c Dislocation line  b E E E E E q cq cq cq cq cq c (b)
Figure 2.2.6. Dislocation in a crystal: (a) edge dislocation; (b) screw dislocation. Note that, for an edge dislocation, the Burgers vector is necessarily perpendicular to the dislocation line. Indeed, this can be used as the defining property of an edge dislocation. Similarly, a screw dislocation can be defined as one whose Burgers vector is parallel to the dislocation line [see Figure 2.2.6(b)]. A dislocation in a crystal need not be a straight line. However, the Burgers vector must remain constant. Thus, a dislocation can change from edge
Section 2.2 / Crystal Plasticity
97
to screw, or vice versa, if it makes a rightangle turn. It cannot, moreover, terminate inside the crystal, but only at the surface of a crystal or at a grain boundary. It can form a closed loop, or branch into other dislocations (at points called nodes), subject to the conservation of the Burgers vectors: the sum of the Burgers vectors of the dislocations meeting at a node must vanish if each dislocation is considered to go into the node (Frank [1951]).
Dislocations and Slip It is now universally accepted that plastic deformation in crystals results from the movement of dislocations. As can be seen from Figure 2.2.7, in order sAtoms before motion cAtoms after motion
s
s
s
s
s
s
s
s
s
s
s
s
cs
cs
s
s
s
s
s
s
s
cs
cs
s
s
s
s
s
s
s
cs
cs
s
s
s
s
s
s
s
sc
s
s
s
s
s
s
s
s
sc
s
s
s
s
s
s
s
s
sc
s
s
s
s
s
s
s
s
s
s
s
s
s
s
b
Figure 2.2.7. Slip by means of an edge dislocation. for an edge dislocation to move one atomic distance in the plane containing it and its Burgers vector (the slip plane), each atom need move only a small fraction of an atomic distance. Consequently, the stress required to move the dislocation is only a small fraction of the theoretical shear strength discussed in 2.2.1. An approximate value of this stress is given by the Peierls–Nabarro stress, 2G 2πh τPN = exp − , 1−ν d(1 − ν) where h and d denote, as before, the distances between adjacent planes of atoms and between atoms in each plane, respectively. The Peierls–Nabarro stress is clearly much smaller than the theoretical shear strength. Its value, moreover, depends on h/d, and the smallest value is achieved when h/d is largest, that is, for closepacked planes that are as far apart as possible;√this result explains why such planes are the likeliest slip planes. When h = 2d, τPN is of the order 10−5 G, consistent with the observed shear strength of pure single crystals. If the stress is maintained, the dislocation can move to the next position, and the next, and so on. As the dislocation moves in its slip plane, the
98
Chapter 2 / The Physics of Plasticity
portion of the plane that it leaves behind can be regarded as having experienced slip of the amount of one Burgersvector magnitude b = b. When the dislocation reaches the crystal boundary, slip will have occurred on the entire slip plane. Suppose that the length of the slip plane is s, and that an edge dislocation moves a distance x in the slip plane; then it contributes a displacement bx/s, so that n dislocations moving an average distance x ¯ produce a displacement u = nb¯ x/s. If the average spacing between slip planes is l, then the plastic shear strain is γp =
u nb¯ x = . l ls
However, n/ls is just the average number of dislocation lines per unit perpendicular area, or, equivalently, the total length of dislocation lines of the given family per unit crystal volume — a quantity known as the density of dislocations, usually denoted ρ. Since only the mobile dislocations contribute to plastic strain, it is their density, denoted ρm , that must appear in the equation for the plastic strain, that is, γ p = ρm b¯ x, and the plastic shearstrain rate is γ˙ p = ρm b¯ v, where v¯ is the average dislocation velocity.
Forces on and Between Dislocations A shear stress τ acting on the slip plane and in the direction of the Burgers vector produces a force per unit length of dislocation that is perpendicular to the dislocation line and equal to τ b. To prove this result, we consider an infinitesimal dislocation segment of length dl; as this segment moves by a distance ds, slip of an amount b occurs over an area dl ds, and therefore the work done by the shear stress is (τ dl ds)b = (τ b) dl ds, equivalent to that done by a force (τ b)dl, or τ b per unit length of dislocation. Equations (2.2.3) for the strain energy per unit length of a dislocation in an isotropic elastic continuum may be used to give an orderofmagnitude estimate for the strain energy per unit length of a dislocation in a crystal, namely, W 0 = αGb2 , (2.2.4) where α is a numerical factor between 0.5 and 1. Two parallel edge dislocations having the same slip plane have, when they are far apart, a combined energy equal to the sum of their individual energies, that is, 2αGb2 per unit length, since any interaction between them is negligible. When they are very close together, then, if they are unlike
Section 2.2 / Crystal Plasticity
99
(that is, if their Burgers vectors are equal and opposite), they will annihilate each other and the resulting energy will be zero; thus they attract each other in order to minimize the total energy. Like dislocations, on the other hand, when close together are equivalent to a single dislocation of Burgers vector 2b, so that the energy per unit length is αG(2b)2 , and therefore they repel each other in order to reduce the energy.
Frank–Read Source The number of dislocations typically present in an unstressed, annealed crystal is not sufficient to produce plastic strains greater than a few percent. In order to account for the large plastic strains that are actually produced, it is necessary for large numbers of dislocations to be created, and on a relatively small number of slip planes, in order to account for slip bands. The Frank–Read source is a mechanism whereby a single segment of an edge dislocation, anchored at two interior points of its slip plane, can produce a large number of dislocation loops. The anchor points can be point defects, or points at which the dislocation joins other dislocations in unfavorable planes. If α in Equation (2.2.4) is constant along the dislocation, independently of its orientation, then an increase ∆L in dislocation length requires an energy increment W 0 ∆L, that is, work in that amount must be done on it. This is equivalent to assuming that a line tension T equal to W 0 is acting along the dislocation. In order to deform an initially straight dislocation segment into a circular arc subtending an angle 2θ, equilibrium requires a restoring force F = 2T sin θ perpendicular to the original dislocation segment. If the length of the segment is L, then the force per unit length is F/L and can be produced by a shear stress τ = F/bL, or τ=
2αGb r sin θ. L
When θ = π/2, that is, when the dislocation segment forms a semicircle, the shear stress is maximum and equal to τmax =
Gb L
if α = 0.5, as it is frequently taken. If the maximum necessary shear stress is acting on a dislocation segment pinned at two points, as in Figure 2.2.8, the semicircular form is soon attained, whereupon the dislocation becomes unstable and expands indefinitely. The expanding loop doubles back on itself, as in (c) and (d), until two sections meet and annihilate each other, since they have the same Burgers vector but opposite line sense, forming a closed outer loop that continues to expand and a new dislocation segment that will repeat the process.
100
Chapter 2 / The Physics of Plasticity 6 @ I @
6 @ I @ r
6 6 6 r
r
r
r
r
@ R @ (a)
(b)
(c)
6
6 @ I @
r
r
JJ ]
@ I @

r
MB B
S w / S
S w / S
(d)
(e)
r

Figure 2.2.8. Frank–Read source (after Read [1953]).
Other mechanisms for the multiplication of dislocations that are similar to the Frank–Read source involve screw dislocations and include crossslip and the Bardeen–Herring source (see, e.g., Hull and Bacon [1984]).
2.2.3.
Dislocation Models of Plastic Phenomena
W. T. Read, Jr., in his classic Dislocations in Crystals (Read [1953]), offered the following caution: “Little is gained by trying to explain any and all experimental results by dislocation theory; the number of possible explanations is limited only by the ingenuity, energy, and personal preference of the theorist.” Indeed, much theoretical work has been expended in the past halfcentury in attempts to explain the phenomena of metal plasticity, discussed in Section 2.1, by means of dislocation theory. No comprehensive theory has been achieved, but numerous qualitative or semiquantitative explanations have been offered, and some of these are now generally accepted. A few are described in what follows.
Section 2.2 / Crystal Plasticity
101
Yield Stress If the loops generated by Frank–Read sources or similar mechanisms could all pass out of the crystal, then an indefinite amount of slip could be produced under constant stress. In reality, obstacles to dislocation movement are present. These may be scattered obstacles such as impurity atoms or precipitates, extended barriers such as grain boundaries, or other dislocations that a moving dislocation has to intersect (“forest dislocations”). In addition, if a dislocation is stopped at a barrier, then successive dislocations emanating from the same Frank–Read source pile up behind it, stopped from further movement by the repulsive forces that like dislocations exert on one another. The yield stress is essentially the applied shear stress necessary to provide the dislocations with enough energy to overcome the shortrange forces exerted by the obstacles as well as the longrange forces due to other dislocations. The mechanisms are many and complex, and therefore there is no single dislocation theory of the yield strength but numerous theories attempting to explain specific phenomena of metal plasticity. This is especially true for alloys, in which the impurity atoms may present various kinds of obstacles, depending on the form they take in the host lattice — for example, whether as solutes or precipitates (for a general review, see, e.g., Nabarro [1975]).
Yield Point Under some conditions, solute atoms tend to segregate in the vicinity of a dislocation at a much greater density than elsewhere in the lattice, forming socalled Cottrell atmospheres. In order to move the dislocation, an extra stress is required to overcome the anchoring force exerted on it by the solutes. Once the dislocation is dislodged from the atmosphere, however, the extra stress is no longer necessary, and the dislocation can move under a stress that is lower than that required to initiate the motion. This is the explanation, due to Cottrell and Bilby [1949], of the yieldpoint phenomenon discussed in 2.1.2 [see Figure 2.1.1(b’)]. Strainaging (Figure 2.1.2) is explained by the fact that the formation of atmospheres takes place by diffusion and is therefore a rate process. Thus if a specimen is unloaded and immediately reloaded, not enough time will have passed for the atmospheres to form anew. After a sufficient time, whose length decreases with increasing temperature, the solutes segregate once more and the upper yield point returns.
WorkHardening As plastic deformation proceeds, dislocations multiply and eventually get stuck. The stress field of these dislocations acts as a back stress on mobile dislocations, whose movement accordingly becomes progressively more difficult, and an ever greater applied stress is necessary to produce additional
102
Chapter 2 / The Physics of Plasticity
plastic deformation. This is the phenomenon of workhardening. In a first stage, when only the most favorably oriented slip systems are active, the back stress is primarily due to interaction between dislocations on parallel slip planes and to the pileup mechanism. In this stage workhardening is usually slight, and the stage is therefore often called easy glide. Later, as other slip systems become activated, the intersection mechanism becomes predominant, resulting in much greater workhardening. In a final stage, screw dislocations may come into play. Since the number of possible mechanisms producing forces on dislocations is great, there is as yet no comprehensive theory of workhardening that would permit the formulation of a stressstrain relation from dislocation theory. For reviews of workhardening models, see Basinski and Basinski [1979] or Hirsch [1975].
Yield Strength of Polycrystals The plastic deformation of polycrystals differs from that of single crystals in that, in the former, individual crystals have different orientations and therefore, under a given applied stress, the resolved shear stress varies from grain to grain. The critical value of this stress is therefore attained in the different grains at different values of the applied stress, so that the grains yield progressively. Furthermore, the grain boundaries present strong barriers to dislocation motion, and therefore the yield stress is in general a decreasing function of grain size, other factors being the same; the dependence is often found to be described by the Hall–Petch relation, kY σY = σY ∞ + √ , d where d is the grain diameter, and σY ∞ and kY are temperaturedependent material constants. The stress σY ∞ , corresponding (theoretically) to infinite grain size, may be interpreted as the yield stress when the effects of grain boundaries can be neglected. As such it should be determinable, in principle, from the singlecrystal yield stress by a suitable averaging process, on the assumption of random orientation of the grains. Such a determination was made by Taylor [1938], who obtained the result that, if the stressstrain curve for a single crystal in shear on an active slip system is given by τ = f (γ p ), then for the polycrystal it is given by σ = mf ¯ (mε ¯ p ), where m ¯ is the average value of the factor (cos φ cos λ)−1 in Equation (2.2.1), a value that Taylor calculated to be about 3.1 for fcc metals.
Bauschinger Effect A fairly simple explanation of the Bauschinger effect is due to Nabarro [1950]. The dislocations in a pileup are in equilibrium under the applied
Section 2.3 / Plasticity of Soils, Rocks and Concrete
103
stress σ, the internal stress σi due to various obstacles, and the back stress σb due to the other dislocations in the pileup; σi may be identified with the elastic limit. When the applied stress is reduced, the dislocations back off somewhat, with very little plastic deformation, in order to reduce the internal stress acting on them. They can do so until they are in positions in which the internal stress on them is −σi . When this occurs, they can move freely backward, resulting in reverse plastic flow when the applied stress has been reduced by 2σi .
Exercises: Section 2.2 1. For a crystal with cubic symmetry, find the Young’s modulus E in terms of C11 , C12 , and C44 for tension (a) parallel to a cube edge, (b) perpendicular to a cube edge and at 45◦ to the other two edges. 2. Show the closepacked planes and slip directions in a facecentered cubic crystals. 3. Derive Equation (2.2.1). 4. For what range of R/a do Equations (2.2.3) give Equation (2.2.4) with the values of α given in the text?
Section 2.3
Plasticity of Soils, Rocks, and Concrete
In recent years the term “geomaterials” has become current as one encompassing soils, rocks, and concrete. What these materials have in common, and in contrast to metals, is the great sensitivity of their mechanical behavior to pressure, resulting in very different strengths in tension and compression. Beyond this common trait, however, the differences between soils on the one hand and rocks and concrete on the other are striking. Soils can usually undergo very large shearing deformations, and thus can be regarded as plastic in the usual sense, although soil mechanicians usually label as “plastic” only cohesive, claylike soils that can be easily molded without crumbling. Rock and concrete, on the other hand, are brittle, except under high triaxial compression. Nevertheless, unlike classically brittle solids, which fracture shortly after the elastic limit is attained, concrete and many rocks can undergo inelastic deformations that may be significantly greater than the elastic strains, and their stressstrain curves superficially resemble those of plastic solids.
104
2.3.1.
Chapter 2 / The Physics of Plasticity
Plasticity of Soil
The Nature of Soil The essential property of soils is that they are particulate, that is, they are composed of many small solid particles, ranging in size from less than 0.001 mm (in clays) to a few millimeters (in coarse sand and gravel). Permanent shearing deformation of a soil mass occurs when particles slide over one another. Beyond this defining feature, however, there are fundamental differences among various types of soils, differences that are strongly reflected in their mechanical behavior. The voids between the particles are filled with air and water; the ratio of the void (air and water) volume to the solid volume is known as the void ratio of the soil. While much of the water may be in the usual liquid form (free water ), and will evaporate on drying, some of the water is attached to the particle surfaces in the form of adsorbed layers, and does not evaporate unless the solid is heated to a temperature well above the boiling point of water. A soil is called saturated if all the voids are filled with water. If both water and air are present, the soil is called partially saturated , and if no free water is present, the soil is called dry. Clay was mentioned at the beginning of this chapter as a prototype of a plastic material. Clays are finegrained soils whose particles contain a significant proportion of minerals known as clay minerals. The chemistry of these minerals permits the formation of an adsorbed water film that is many times thicker than the grain size. This film permits the grains to move past one another, with no disintegration of the matrix, when stress is applied. It is this property that soil mechanicians label as plasticity. Claylike soils are also generally known as cohesive soils. In cohesionless soils, such as gravels, sands, and silts, the movement of grains past one another is resisted by dry friction, resulting in shear stresses that depend strongly on the compression. Materials of this type are sometimes called frictional materials.
Soil Compressibility If soil that is prevented from expanding laterally is loaded in compression between layers, at least one of which is permeable to water, an irreversible decrease in void ratio occurs, a result of the seepage of water from the voids. The process, known as consolidation, takes time, and sometimes goes on indefinitely, though at an everdiminishing rate, much like creep. As a rule, though, something very near the ultimate compression is attained in a finite time which depends on the properties of the soil layer. A typical compression curve is shown in Figure 2.3.1(a). The figure shows both the virgin curve and the hysteresis loop resulting from decompression followed by recompression. A soil that has been decompressed is called overconsolidated . The curves
Section 2.3 / Plasticity of Soils, Rocks and Concrete
Void ratio, e
1.2
105
σ ¯ (MPa)
0.50
Virgin curve Recompression
1.0
0.8
0.25
HH HH
Decompression 0.6 0
0.25
0.50 (a)
σ ¯ (MPa)
0.1
0.2
ε=
e0 − e 1 + e0
(b)
Figure 2.3.1. Compression curve for soil: (a) consolidation curve; (b) compressive stressstrain diagram [(b) is (a) replotted]. are replotted in Figure 2.3.1(b) as a compressive stressstrain diagram. It is seen that except for the upward convexity of the virgin curve, the diagram resembles that of workhardening metals.
Shearing Behavior As in ductile metals, failure in soils occurs primarily in shear. Unlike metals, the shear strength of soils is, in most circumstances, strongly influenced by the compressive normal stress acting on the shear plane and therefore by the hydrostatic pressure. Since soils have little or no tensile strength, the tension test cannot be applied to them. Other means are necessary in order to determine their shear strength. Direct Shear Test. A traditional test of the shear strength of soft clays and of dry sands and gravels is the direct shear test or shearbox test. A sample of soil is placed in a rectangular box whose top half can slide over the bottom half and whose lid can move vertically, as shown in Figure 2.3.2(a). A normal load is applied to the lid, and a shear force is applied to the top half of the box, shearing the soil sample. Simple Shear Test. In this test, developed by Roscoe [1953], it is the strain that is maintained as one of simple shear [see Figure 2.3.2(b)]. The two tests just described, along with others like them, provide simple means of estimating the shear strength. However, the stress distribution in the sample is far from uniform, so that these tests do not actually measure stress, and no stressstrain diagrams can result from them. Triaxial Test. This is generally regarded as the most reliable test of the shearing behavior of soils. As we shall see, it is used to test rock and concrete as well. This test was discussed in 2.2.1; a normal compressive stress σ3 (= σ2 ) is applied to the sides of a cylindrical sample by means of air or
106
Chapter 2 / The Physics of Plasticity N
N = normal load S = shear load N
?
..............................................................................S ...................................................................................................................... Stress ................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................................ ............................................................................................................................................................................................................................................................................................................................................................................................................................................................... ............................................................................................................................................................................................................................................................................................................................................................................................................................................................... . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . ..... ........ ............................................................................................................................................................................................................................................................................................................................................................................................................................................................... ...................................................................................................... . ....................................... ................ ....... ....... ....... ...................................................................... ............................................. ................................................ . .............................. . ........................................ ......................................... ............................................. ......................................... .......................................... ......................................... ...................................... .......................................... Soil sample ....................................... ........................................ .......................................... ........................................ ..................... ......................................... . .................................................. ............................................... . . . . . . . . . . . . . . ....... . . . . . . . ............................. ....... . . . . . . . ....... .................................................................. ....... .......................................................................... ........................................................................... .......................................................................... ........................................................................... ............. .......................................................................... ........................................................................... .......................................................................... ............... . ........................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... .......................................................................... .......................................................................... ........................................................................... .......................................................................... ........................................................................... Hinge ........................................................................... .......................................................................... ...........................................................................
S

? q q
q q
q
q
q q
q
! !! L L L LL q L LL L L L !L 7 L!!
q
......................................................... ......................................................... ......................................................... ......................................................... ......................................................... .........................................................
(a)
q
q
q
q
q
transducers ! !! L q q q L L L q L LL q q q LL L q L !!L L! YH H H Sliding contact
(b)
Figure 2.3.2. Shear tests: (a) direct shear test; (b) simple shear test (after Roscoe [1953]).
water pressure, and an axial compressive stress σ1 , numerically greater than σ3 , is applied at the ends (Figure 2.3.3). The results are commonly plotted σ1
? ) Piston Confining Soil sample P PP fluid ) Membrane P .................... P q P > P ..... .. q P ................................. σ=2 Cell P q P ............................................. σ3 Porous stone XX ....................................
XX z. . .
Ol Pore pressure
Cell pressure
Figure 2.3.3. Triaxial test apparatus. as graphs of σ1 − σ3 against the axial shortening strain ε1 , with σ3 as a parameter. (Alternatively, the mean stress (σ1 + 2σ3 )/3 or the normal stress on the maximumshear plane (σ1 + σ3 )/2 may be used as a parameter.) Note that σ1 − σ3 is a measure both of the maximum shear stress given by shear Equation (1.3.11), namely, τmax = 12 σ1 − σ3 , and of the octahedral √ stress, given in accordance with Equation (1.3.5) as τoct = ( 2/3)σ1 − σ3 . If σ3 = 0 then the test is called an unconfined compression test, used most commonly on hard materials such as rock and concrete, but occasionally on clay if it is performed fast enough (“quick test”). Some typical stressstrain curves for soils are shown in Figure 2.1.1(f) (page 78). The dependence of the shear strength of soils on the normal stress acting on the shearing plane varies with the type and condition of the soil. It is sim
Section 2.3 / Plasticity of Soils, Rocks and Concrete
107
plest in dry cohesionless soils (gravels, sands, and silts), in which resistance to shear is essentially due to dry friction between the grains, and therefore is governed by the Coulomb law of friction: τ = σ tan φ,
(2.3.1)
where τ and σ are respectively the shear and normal stresses on the shearing plane, and φ is the angle of internal friction, a material property. In wet cohesionless soils, the applied stress is the sum of the effective stress in the grains and the neutral stress due to water pressure and possibly capillary tension. If the latter stress is denoted σw (like σ, positive in compression), then the Coulomb law is expressed by τ = (σ − σw ) tan φ,
(2.3.2)
since the water pressure provides a counterthrust on potential sliding surfaces, and therefore it is only the effective stress that governs frictional resistance. The concept of effective stress is due to Terzaghi. Cohesionless soils also undergo significant volume changes when sheared. They tend to swell if they are dense, since closely packed grains must climb over one another in the course of shearing, and shrink if they are loose, since grains fall into the initially large voids and thus reduce the void volume. A granular soil thus has a critical density which remains essentially constant as shearing proceeds, and the soil is termed dense or loose, respectively, if its density is above or below critical. In a sample of fine sand or silt that is dense and saturated, and which has no source of additional water, the swelling that accompanies shearing produces surface tension on the water which acts as a negative neutral stress. Consequently, in accord with Equation (2.3.2), such a sample has shear strength under zero applied stress. In clays, the stresses in the adsorbed water layers play an important role in determining strength, and in partially saturated clays this role is predominant. The shear strength of such clays is given approximately by τ = c + σ tan φ,
(2.3.3)
where φ is the angle of internal friction and c is a material constant called the cohesion, representing the shear strength under zero normal stress. The shear response of a saturated clay depends on whether it is in a drained or undrained condition. The former condition is achieved in a slow application of the stresses, so that the neutral stresses are not changed during the loading and therefore play little part in determining the shear strength. Equation (2.3.1) is consequently a good approximation to the relation between shear stress and normal stress in this condition. In the undrained
108
Chapter 2 / The Physics of Plasticity
condition, on the other hand, the loading is quick and the applied stress is carried by the neutral stress. In this condition the shear strength is independent of the applied normal stress, and is therefore given by Equation (2.3.3) with φ = 0; the cohesion c is then called the undrained strength and denoted cu . Volume changes accompanying shearing are negligible in saturated clays. The shearstrength response of undrained clays thus resembles that of metals. Much of soil engineering practice is based on this model, though it is not universally accepted; see Bolton [1979], Section 5.1, for a survey of the criticisms.
2.3.2.
“Plasticity” of Rock and Concrete
Unlike soils, materials such as rock, mortar and concrete are generally not plastic in the sense of being capable of considerable deformation before failure. Instead, in most tests they fracture through crack propagation when fairly small strains (on the order of 1% or less) are attained, and must therefore be regarded as brittle. However, concrete, mortar, and many rocks (such as marble and sandstone) are also unlike such characteristically brittle solids as glass and cast iron, which fracture shortly after the elastic limit is attained. Instead, they attain their ultimate strength after developing permanent strains that, while small in absolute terms, are significantly greater than the elastic strains. The permanent deformation is due to several mechanisms, the foremost of which is the opening and closing of cracks.
StrainSoftening Following the attainment of the ultimate strength, concrete and many rocks exhibit strainsoftening, that is, a gradual decrease in strength with additional deformation. The nature of this decrease, however, depends on factors associated with the testing procedure, including sample dimensions and the stiffness of the testing machine. The effect of machine stiffness can be described as follows. Let P denote the load applied by the machine to the sample, and u the sample displacement. In the course of a small change ∆u in the displacement, the sample absorbs energy in the amount P ∆u. If the machine acts like an elastic spring with stiffness k, then a change ∆P in the load implies a change P ∆P/k in the energy stored in the machine. This change represents release of energy if P ∆P < 0, that is, once softening takes place. The energy released by the machine is greater than that which can be absorbed by the sample if k < ∆P/∆u, resulting in an unstable machinesample system in the case of a “soft” machine; the sample breaks violently shortly after the ultimate strength is passed. A “stiff” machine, on the other hand, makes for a system that is stable under displacement control. It is only with a stiff machine, therefore, that a complete loaddisplacement (or stressdisplacement) curve
Section 2.3 / Plasticity of Soils, Rocks and Concrete
109
can be traced. It is not certain, however, whether the stressdisplacement curve may legitimately be converted into a stressstrain curve, such as is shown in Figure 2.1.1(d) (page 78), that reflects material properties, since specimen deformation is often far from homogeneous. Experiments by Hudson, Brown and Fairhurst [1971] show a considerable effect of both the size and the shape of the specimens on the compressive stressstrain curve of marble, including as a particular result the virtual disappearance of strainsoftening in squat specimens. Read and Hegemier [1984] conclude that no strainsoftening occurs in specimens of soil, rock and concrete that are homogeneously deformed. A similar conclusion was reached by Kotsovos and Cheong [1984] for concrete. It should be remarked that some rocks, such as limestone, exhibit classically brittle behavior in unconfined compression tests even with stiff testing machines — that is, they fracture shortly after the elastic limit is reached.
The Effect of Pressure An important feature of the triaxial behavior of concrete, mortar and rocks (including those which are classically brittle in unconfined tests) is that, if the confining pressure σ3 is sufficiently great, then crack propagation is prevented, so that brittle behavior disappears altogether and is replaced by ductility with workhardening. Extensive tests were performed on marble and limestone by von K´arm´an [1911] and by Griggs [1936]; some results are shown in Figure 2.1.1(e). Note that the strains attained in these tests can become quite large. The relation between hydrostatic pressure and volumetric strain also exhibits ductility with workhardening; the curves resemble those of Figure 2.3.1(b). It can be said, in general, that rocks and concrete behave in a ductile manner if all three principal stresses are compressive and close to one another.
Dilatancy If the transverse strain ε2 = ε3 is measured in uniaxial compression tests of rock and concrete specimens in addition to the axial strain ε1 , then, as discussed in 1.2.2, the volumetric strain εV equals ε1 +ε2 +ε3 . If the stress σ1 is plotted against εV (positive in compression), it is found that εV begins to decrease from its elastic value at stresses greater than about half the ultimate strength, reaches zero at a stress near the ultimate strength, and becomes negative (signifying an increase in volume) in the strainsoftening range (see Figure 2.3.4, showing both a σ1 ε1 and a σ1 εV diagram). Similar results are obtained in triaxial tests under low confining pressures. This volume increase, which results from the formation and growth of cracks parallel to the direction of the greatest compressive stress, is known as dilatancy. This term is sometimes also applied to the swelling of dense granular soils,
110
Chapter 2 / The Physics of Plasticity σ Volume strain
Longitudinal strain
ε
Figure 2.3.4. Compression tests on concrete or rock: stress against longitudinal strain and volume strain. although the mechanism causing it is unrelated.
Tensile Behavior Uniaxial tension tests are difficult to perform on rock and concrete, and the results of such tests vary considerably. The most reliable direct tension tests are those in which the ends of the specimen are cemented with epoxy resin to steel plates having the same crosssection as the specimen, with the tensile force applied through cables in order to minimize bending effects. The uniaxial tensile strength of rock and concrete is typically between 6 and 12% the uniaxial compressive strength. Strainsoftening, associated with the opening of cracks perpendicular to the direction of tension, is observed in tests performed in stiff machines.
Chapter 3
Constitutive Theory Section 3.1
Viscoplasticity
We saw in the preceding chapter that while “yielding” is the most striking feature of plastic behavior, the existence of a welldefined yield stress is the exception rather than the rule. It so happens, however, that mild steel, which belongs to this exceptional class, is one of the most commonly used of metals, and attempts at a theoretical description of its behavior preceded those for other metals; such attempts naturally incorporated a criterion as an essential feature of what came to be known as plasticity theory, as well as of a later development, known as viscoplasticity theory, which takes rate sensitivity into account. It should be pointed out that while most workers in solid mechanics use “viscoplasticity” in its classical meaning (see Prager [1961]), that is, to denote the description of ratedependent behavior with a welldefined yield criterion, this usage is not universal. Others, following Bodner [1968], use the term for models of highly nonlinear viscoelastic behavior, without any elastic range, that is characteristic of metals, especially at higher temperatures. Such models are discussed in 3.1.3. 3.1.1 is limited to models of classical viscoplasticity. Both classes of models are subclasses of the internalvariable models presented in Section 1.5. In 3.1.2, rateindependent plasticity, the foundation for most of the remainder of this book, is derived as a limiting case of classical viscoplasticity.
3.1.1.
InternalVariable Theory of Viscoplasticity
Yield Surface As in Section 1.5, let ξ denote the array of internal variables ξ1 , ..., ξn . If there is a continuous function f (σ, T, ξ) such that there exists a region in the space of the stress components in which (at given values of T, ξ) 111
112
Chapter 3 / Constitutive Theory
f (σ, T, ξ) < 0, and such that the inelastic strainrate tensor ε˙ i vanishes in that region but not outside it, then this region constitutes the aforementioned elastic range, and f (σ, T, ξ) = 0 defines the yield surface in stress space; the orientation of the yield surface is defined in such a way that the elastic range forms its interior. A material having such a yield function f (·) is viscoplastic in the stricter sense. This definition, it should be noted, does not entail the simultaneous vanishing of all the internalvariable rates ξ˙α in the elastic region; if such were the case, strainaging as described in the preceding chapter would not be possible, since it requires an evolution of the local structure while the material is stressfree. However, this proviso is of significance only for processes whose time scale is of the order of magnitude of the relaxation time for strainaging, which for mild steel at ordinary temperatures is of the order of hours. Thus, for a process lasting a few minutes or less, the internal variables governing strainaging are essentially constant and their rates may be ignored. For the sake of simplicity, we adopt a somewhat more restricted definition of viscoplasticity, according to which all the internalvariable rates vanish in the elastic region, that is, the functions gα (σ, T, ξ) constituting the righthand sides of the rate equations (1.5.1) are assumed to vanish whenever f (σ, T, ξ) ≤ 0. In particular, this definition includes all those models (such as that of Perzyna [1971]) in which the rates of the internal variables depend linearly on ε˙ i . In view of this definition it now becomes convenient to redefine the gα as gα = φhα , where φ is a scalar function that embodies the rate and yielding characteristics of the material, with the property that φ = 0 when f ≤ 0 and φ > 0 when f > 0. Such a function was introduced by Perzyna [1963] in the form γ(T ), where γ(T ) is a temperaturedependent “viscosity coefficient” (actually an inverse viscosity, or fluidity), and the notation is defined — somewhat misleadingly — as (
=
0 for f ≤ 0 Φ(f ) for f > 0
(the more usual definition of the operator < · > is given below). Note that our definition of φ is determinate only to within a multiplicative scalar; that is, if λ is a positive continuous function of the state variables, then φ may be replaced by φ/λ and the hα by λhα without changing the rate equations.
Hardening The dependence of the yield function f on the internal variables ξα describes what are usually called the hardening properties of the material. The relationship between this dependence and the behavior of the material can be understood by considering a stress σ that is close to the yield surface but outside it, that is, f (σ, T, ξ) > 0. In particular, let us look at a case of
Section 3.1 / Viscoplasticity
113
uniaxial stress in a specimen of a material whose static stressstrain curve is given by the solid curve of Figure 3.1.1, which shows both rising (“hardening”) and falling (“softening”) portions. If the material is viscoplastic, then its behavior is elastic at points below the curve, and viscoelastic at points above the curve — that is, the curve represents the yield surface. σ
Hardening Creep A

Softening B

 Creep
3
Static curve
ε
Figure 3.1.1. Hardening and softening in viscoplasticity: relation to creep and static curve. If the stress is held constant at a value above the static curve, creep occurs, resulting in increasing strain as shown by the dashed horizontal lines. If the initial point is, like A, above the rising portion of the static stressstrain curve, then the creep tends toward the static curve and is bounded, while if it is, like B, above the falling portion, then the creep tends away from the static curve and is unbounded. Since the points on the static stressstrain curve are in effect those on the yield surface, we may generalize from the uniaxial case as follows: creep toward the yield surface, characterizing hardening, means that at constant stress and temperature, the yield function f decreases from a positive value toward zero, that is, f˙ < 0. Similarly, softening is characterized by f˙ > 0. But
f˙
σ =const,T =const
=
X ∂f X ∂f ξ˙α = φ hα α
∂ξα
α
∂ξα
= −φH, where, by definition, H=−
X ∂f α
∂ξα
hα .
(3.1.1)
Thus H > 0 and H < 0 for hardening and softening materials (or hardening and softening ranges of the same material), respectively. The limiting case H = 0, which in particular occurs when f is independent of the ξα , describes a perfectly plastic material.
114
Chapter 3 / Constitutive Theory
Viscoplastic Potential If a viscoplastic material has a flow potential in the sense of 1.5.3 (not necessarily in the stricter sense of Rice or Moreau), then it may also be shown to have a viscoplastic potential in the following sense. Let hij be defined by X ∂εiij hij = hα . α ∂ξα The flow equations then are ε˙ iij = φhij .
(3.1.2)
If there exists a function g(σ, T, ξ), continuously differentiable with respect to σ wherever f (σ, T, ξ) > 0, such that hij =
∂g , ∂σij
then g is called a viscoplastic potential . (The relation hij = λ∂g/∂σij is not more general, since the factor λ can be absorbed in φ.) Perzyna [1963] and many others have assumed the existence of a viscoplastic potential identical with the yield function f , or at least such that ∂g/σij ∝ ∂f /σij ; this identity is of no great significance in viscoplasticity, but becomes highly important after the transition to rateindependent plasticity.
Specific Models Based on J2 Flow Potential In 1.5.3 a flow potential was discussed that depends on the stress only through J2 , leading to the flow equation ε˙ iij = φsij . A yield criterion having the same stress dependence, that is, one that can be represented by the equation p J2 − k = 0 (where k depends on T and ξ and equals the yield stress in shear) is known as the Mises (sometimes Huber–Mises) yield criterion. A model of viscoplasticity incorporating this yield criterion and a J2 flow potential was first proposed by Hohenemser and Prager [1932] as a generalization to threedimensional behavior of the Bingham model described in 2.1.3. The flow equation is k 1 (3.1.3) ε˙ iij = sij , 2η J2 where η is a temperaturedependent viscosity, and the Macauley bracket is defined by <x> = xH(x), where H(·) is the Heaviside step function:
H(x) =
0, x ≤ 0, 1, x > 0.
Section 3.1 / Viscoplasticity
115
In other words,
<x> =
0, x ≤ 0, x, x > 0.
The previously discussed model of Perzyna [1963] is a generalization of the Hohenemser–Prager model in which is replaced by H(f )Φ(f ), or in Perzyna’s notation. It will be noted that as k → 0, the Hohenemser–Prager and Perzyna models reduce to the Maxwell model of linear viscoelasticity discussed in 1.5.1. A generalized potential Ω, as discussed in 1.5.4, may be associated with the Hohenemser–Prager model if it takes the form Ω(σ) = 2 /(2η), where √ f = J2 − k, and with the Perzyna model if it is Ω(σ) = H(f )Ω0 (f ). Hardening can be included in a simple manner by letting k be a variable. If the generalized potential is viewed as a function Ω(σ, k), then the effective inelastic strain εi defined by (1.5.7) can easily be shown to obey the rate equation 1 ∂Ω . ε˙ i = − √ 3 ∂k √ It is convenient to let k = k0 + R/ 3, where k0 is the initial value of k, and to treat Ω as a function of (σ, R). Then ε˙ i = −∂Ω/∂R, and −R may be regarded as the thermodynamic force conjugate to the internal variable εi . A more sophisticated model developed by Chaboche [1977] uses as internal variables εi and a strainlike symmetric secondrank tensor α. The thermodynamic forces conjugate to these variables are the stresslike variables −R and −ρ, respectively, and the yield surface is assumed to be given by q R f (σ, ρ, R) = J¯2 − √ − k0 = 0, 3 where 1 J¯2 = (sij − ρ0ij )(sij − ρ0ij ), 2 ρ0 being the deviator of ρ. The yield surface is thus again of the Mises type, but capable not only of expansion (as measured by R) but also of translation (as shown by ρ0 , which locates the center of the elastic region). The hardening described by the expansion of the yield surface is called isotropic, while that described by the translation is called kinematic. The significance of the terms is discussed in Section 3.2. If a generalized potential is again assumed in the Perzyna form, Ω(σ, R, ρ) = H(f )Ω0 (f ), then ε˙ iij = ∂Ω/∂σij and ε˙ i = −∂Ω/∂R as before, the flow equations being sij − ρ0ij ∂Ω ε˙ iij = = H(f )Ω00 (f ) p . ∂σij 2 J¯2 ˙ = ε˙ i , so that the kinematichardening variable α, though In addition, α it must be treated as a distinct variable, coincides with the inelastic strain.
116
Chapter 3 / Constitutive Theory
Chaboche, however, assumes the generalized potential in the form Ω(σ, R, ρ) = H(f )Ω0 (f )+Ωr (ρ), where the second term represents recovery (see 2.1.2). Moreover, Chaboche abandons the generalized normality hypothesis for α by introducing an additional term representing a concept called fading strain memory, due to Il’iushin [1954], the better to describe the Bauschinger effect. The rate equation for α is therefore taken as α˙ ij = −
∂Ω ∂Ωr − F (εi )ε˙ i ρij = ε˙ iij − F (εi )ε˙ i ρij − , ∂ρij ∂ρij
where F (εi ) is a function to be specified, along with Ω0 (f ), Ωr (ρ), and the freeenergy density ψ(T, ε, εi , α), from which R and ρ can be derived in accordance with Equation (1.5.4): R = ρ∂ψ/∂εi , ρij = ρ∂ψ/∂αij .
3.1.2.
Transition to RateIndependent Plasticity
Aside from the previously discussed limit of the Hohenemser–Prager model as the yield stress goes to zero, another limiting case is of great interest, namely, as the viscosity η goes to zero. Obviously, if s 6= 0 then the inelastic √ strain rate would become infinite, unless J2 simultaneously tends to k, in √ which case the quantity (1/η) becomes indeterminate but may remain finite and positive. Supposing for simplicity that k in Equation (3.1.3) is constant, for a given input of stress we can solve this equation for εi as a function of time, and the dependence on time is through the variable t/η. In other words, decreasing the viscosity is equivalent to slowing down the process of inelastic deformation, and the limit of zero viscosity is equivalent to the limit of “infinitely slow” processes. Thus a slow process can take place if J2 is slightly larger than k 2 . We can also see this result by forming the scalar product ε˙ iij ε˙ iij from Equation (3.1.3), from which we obtain p
q
J2 = k + η 2˙εiij ε˙ iij ,
ε˙ i 6= 0,
an equation that is sometimes interpreted as a ratedependent yield criterion. Let us return to the more general model of viscoplasticity considered above, and particularly one in which φ increases with f . The rate equations (3.1.2) indicate that, in the same sense as in the Hohenemser–Prager model, the rate of a process in which inelastic deformation takes place increases with distance from the yield surface. If such a process is very slow , then it takes place very near but just outside the yield surface, so that φ is very small. In the limit as f → 0+ we can eliminate φ (and thus no longer need to concern ourselves with the actual rate at which the process takes place) as follows: if f remains equal to zero (or a very small positive constant), then X ∂f ∂f f˙ = σ˙ ij + φhα = 0. ∂σij α ∂ξα
Section 3.1 / Viscoplasticity We define
117
◦
f=
∂f σ˙ ij ∂σij
(3.1.4)
and assume H > 0 (i.e., hardening), with H as defined by Equation (3.1.1); ◦ then the condition f˙ = f − φH = 0 is possible together with φ > 0 only if ◦
f > 0; this last condition is called loading. Thus we have the result φ=
1 ◦ , H
and therefore
1 ◦ (3.1.5) ξ˙α = hα . H Note that both sides of Equation (3.1.5) are derivatives with respect to time, so that a change in the time scale does not affect the equation. Such an equation is called rateindependent. If it is assumed that this equation describes material behavior over a sufficiently wide range of loading rates, then the behavior is called rateindependent plasticity, also called inviscid plasticity (since it corresponds to the zeroviscosity limit of the Hohenemser–Prager model), or just plain plasticity. Rateindependent plasticity constitutes the principal topic of the remainder of this book. The inelastic strain occurring in rateindependent plasticity is usually denoted εp rather than εi , and is called the plastic strain. The flow equation for the plastic strain may be written as 1 ◦ ε˙ pij = hij . (3.1.6) H For purposes of computation, however, it is sometimes advantageous to remain within the framework of viscoplasticity without making the full transition, even when the problem to be solved is regarded as rateindependent. In other words, a fictitious viscoplastic material of very low viscosity is “associated” with a given rateindependent plastic material, with rate equations given, for example (Nguyen and Bui [1974]), by ξ˙α = hα , η
(3.1.7)
with the viscosity η taken as constant. Computations are then performed under timeindependent loads and boundary conditions until all strain rates vanish. It was shown by Zienkiewicz and Cormeau [1974], among others, that the results are equivalent to those of rateindependent plasticity.
Combined Viscoplasticity and RateIndependent Plasticity At extremely high rates of deformation or loading, the internal variables do not have enough time to change and consequently the deformation can be only elastic. However, the various rate processes responsible for plastic
118
Chapter 3 / Constitutive Theory
deformation, corresponding to the generation of dislocations and the many different kinds of obstacles that dislocations must overcome, may have very different characteristic times. This means that not only do metals differ greatly among one another in their ratesensitivity, but different mechanisms in the same metal may respond with very different speeds. Thus, those mechanisms whose characteristic times are very short compared with a typical loading time produce what appears to be instantaneous inelastic deformation, while the others produce ratedependent deformation as discussed so far in this section. If both phenomena occur in a metal over a certain range of loading times, then the total inelastic strain εi may be decomposed as εi = εvp + εp , (3.1.8) where εvp is the viscoplastic strain equivalent to that governed by Equation (3.1.2), and εp is the apparently rateindependent plastic strain, governed by Equation (3.1.6). It is important to note that the yield functions f and flow tensors hij are, in general, different for the two inelastic strain tensors. In particular, the viscoplastic yield surface is always assumed to be inside the rateindependent plastic (or “dynamic”) yield surface.
3.1.3.
Viscoplasticity Without a Yield Surface
As we have seen, in both classical viscoplasticity and rateindependent plasticity the yield surface is a central ingredient; in the latter it is indispensable. The significance of the yield surface has, however, repeatedly been questioned. Consider the following remarks by Bell [1973]: “Among the many matters pertaining to the plastic deformation of crystalline solids, yield surfaces and failure criteria early became subjects of overemphasis... Indeed most of the outstanding 19th century experimentists doubted that such a phenomenon as an elastic limit, let alone a yield surface, existed... well over a halfcentury of experiment, and the study of restricted plasticity theories for the ‘ideal solid,’ have not disposed of most of the original questions.”
“Unified” Viscoplasticity Models According to Bodner [1968], “yielding is not a separate and independent criterion but is a consequence of a general constitutive law of the material behavior.” Since the 1970s several constitutive models for the ratedependent inelastic behavior of metals have been formulated without a formal hypothesis of a yield surface, but with the feature that at sufficiently low rates the resulting stressstrain curves may resemble those of materials with fairly well defined yield stresses. In fact, with yield based on the offset definition (see 2.1.1), these models can predict yield surfaces in accordance with Bodner’s dictum, particularly if offset strains of the order of 10−6 to 10−5 are used, in contrast to the conventional 10−3 to 10−2 .
Section 3.1 / Viscoplasticity
119
In addition to describing the behavior traditionally called plasticity, in both monotonic and cyclic loading, these models also aim to describe creep, especially at higher temperatures, without a decomposition such as (3.1.8). They have consequently come to be known as “unified” viscoplasticity models, and are particularly useful for the description of bodies undergoing significant temperature changes — for example, spacecraft. Perhaps the simplest such model is due to Bodner and Partom [1972, 1975], in which the flow equations are given by Equation (3.1.2) with hij = sij and φ a function of J2 and (in order to describe hardening) of the inelastic work Wi defined by Equation (1.5.6) as the only internal variable. The rate equation is obviously ˙ i = 2J2 φ(Wi , J2 ). W √ The hardening in this case is purely isotropic, since 3J2 is the value of the ˙ i .1 effective stress necessary to maintain a given inelastic work rate W More sophisticated “unified” viscoplasticity models, that describe many features of the behavior of metals at elevated temperatures, have been developed since 1975 by, among others, Miller [1976], Hart [1976], Krieg, Swearengen, and Jones [1978], Walker [1981], and Krieg, Swearengen, and Rohde [1987] (see reviews by Chan, Bodner, Walker, and Lindholm [1984], Krempl [1987], and Bammann and Krieg [1987]). The essential internal variables in these models are the equilibrium stress tensor ρ, and the scalar drag stress or friction stress σD ;2 the terminology is loosely related to that of dislocation theory, and is an example of “physical” nomenclature for phenomenological internal variables. In the “unified” models the stresslike variables σD and ρ are used directly as internal variables, rather than as conjugate thermodynamic forces. The equilibrium stress ρ, like its counterpart in the Chaboche model, describes kinematic hardening. Some writers, following Kochend¨orfer [1938], relate it to the back stress due to stuck dislocations (see 2.2.3), and consequently the equilibrium stress is also termed back stress; see Krempl [1987] for a discussion (the relationship between constitutive theory and crystal behavior has also been discussed by Kocks [1987]). For isotropic behavior ρ is assumed as purely deviatoric, and the rate equation for inelastic strain takes the form 3 φ(Γ/σD ) ε˙ iij = e˙ iij = (sij − ρij ), (3.1.9) 2 Γ √ ˙ i = 3J2 ε˙ i Or, equivalently, a given effective inelastic strain rate, since in this model W is an increasing function of Wi (or of εi ). 2 A model developed by Krempl and coworkers, known as viscoplasticity based on overstress, dispenses with drag stress as a variable (see Yao and Krempl [1985] and Krempl, McMahon, and Yao [1986]). In another model called viscoplasticity based on total strain (Cernocky and Krempl [1979]), the equilibrium stress is not an internal variable but a function of total strain; this model is therefore a nonlinear version of the “standard solid” model of linear viscoelasticity (see 1.5.1). 1
120
Chapter 3 / Constitutive Theory
where Γ = 3J¯2 , with J¯2 as defined in 3.1.1, and φ is a function (whose values have the dimensions of inverse time) that increases rapidly with its argument. The evolution of the equivalent inelastic strain is given by p
ε˙ i = φ(Γ/σD ),
(3.1.10)
and, in uniaxial stress, ε˙ i = φ(σ − ρ/σD ). Typical forms of φ(x) are Axn , A(ex − 1), and A[sinh(xm )]n , where A, m, and n are constants, n in particular being a large exponent. For an extension to initially anisotropic behavior, see, for example, Helling and Miller [1987]. A variety of forms has been proposed for the rate equations for ρ and σD ; a typical set is due to Walker [1981]: ρ˙ ij = a1 ε˙ iij − [a2 ε˙ i + a3 (2ρkl ρkl /3)(m−1)/2 ]ρij , σ˙ D = [a4 − a5 (σD − σD0 )]ε˙ i − a6 (σD − σD0 )p , where ε˙ iij and ε˙ i are substituted from (3.1.9)–(3.1.10), and a1 , ...., a6 , m, p and σD0 are constants.
Endochronic Theory A different “theory of viscoplasticity without a yield surface” is the endochronic theory of Valanis [1971], originally formulated by him (Valanis [1971]) for “application to the mechanical behavior of metals,” though its range of application has recently been extended to other materials, such as concrete (Baˇzant [1978]). The basic concept in the theory is that of an intrinsic time (hence the name) that is related to the deformation history of the material point, the relation itself being a material property. An intrinsic time measure ζ is defined, for example, by dζ 2 = Aijkl dεiij dεikl + B 2 dt2 , where the tensor A and scalar B may depend on temperature. (In the original theory of Valanis [1971], the total strain ε rather than the inelastic strain εi appeared in the definition.) A model in which B = 0 describes rateindependent behavior and thus defines the endochronic theory of plasticity. An intrinsic time scale is next defined as z(ζ), a monotonically increasing function, and the behavior of the material is assumed to be governed by constitutive relations having the same structure as those of linear viscoelasticity, as described in 1.5.2, but with z replacing the real time t. As in linear viscoelasticity, the internal variables can be eliminated, and the stress can
Section 3.1 / Viscoplasticity
121
be related to the strain history by means of a pseudorelaxation function. The uniaxial relation is Z
z
σ= 0
R(z − z 0 )
dε 0 dz , dz 0
(3.1.11)
while the multiaxial relation describing isotropic behavior is Z
σij = 0
z
dεkk dεij R1 (z − z )δij + 2R2 (z − z 0 ) 0 dz 0 . 0 dz dz
0
With a pseudorelaxation function analogous to that of the “standard solid,” that is, R(z) = E1 + E2 e−αz , and with z(ζ) given by z=
1 ln(1 + βζ), β
where α and β are positive constants, Valanis [1971] was able to fit many experimental data on repetitive uniaxial loadingunloading cycles and on coupling between tension and shear. More recently, Valanis [1980] showed that Equation (3.1.11) can be replaced by Z z dεi dεi σ = σ0 ρ(z − z 0 ) 0 dz 0 . + (3.1.12) dz dz 0 For rateindependent uniaxial behavior, dζ = dεi  with no loss in generality. If the last integral is called α, then the stress must satisfy σ − α = σ0 h(z),
(3.1.13)
where h(z) = dζ/dz. Equation (3.1.12) can be used to construct stressstrain curves showing hardening depending both on the effective inelastic strain [through h(z)] and on the strain path (through α). The equation has a natural extension to multiaxial stress states, which for isotropic materials is (sij − αij )(sij − αij ) = [s0 h(z)]2 . This equation represents a yield surface capable of both expansion and translation in stress space, thus exhibiting both isotropic and kinematic hardening. An endochronic model unifying viscoplasticity and plasticity was presented by Watanabe and Atluri [1986].
Exercises: Section 3.1 1. Suppose that the yield function has the form f (σ, T, ξ) = F (σ) − k(T, κ), where κ is the hardening variable defined by either (1.5.6) or (1.5.7), and the flow equations are assumed as in the form (3.1.2). What is the “hardening modulus” H, defined by Equation (3.1.1)?
122
Chapter 3 / Constitutive Theory
2. If the only stress components are σ12 = σ21 = τ , with τ > 0, write the equation for the shear rate γ˙ = 2˙ε12 given by the Hohenemser–Prager model (3.1.3). Discuss the special case k = 0. 3. Generalize the Hohenemser–Prager model to include isotropic and kinematic hardening. Compare with the Chaboche model. 4. Find the flow equation for a viscoplastic solid with a ratedependent yield criterion given by p
1
J2 = k + η(2˙εij ε˙ ij ) 2m .
5. Construct a simple model for combined viscoplasticity and plasticity, with a perfectly plastic Mises yield criterion and associated flow rule in both. 6. Derive (3.1.12) from (3.1.11).
Section 3.2 3.2.1.
RateIndependent Plasticity
Flow Rule and WorkHardening
Flow Rule In keeping with the formulation of rateindependent plasticity as the limit of classical viscoplasticity for infinitely slow processes, we henceforth consider all processes to be “infinitely” slow (compared with the material relaxation time τ ), and correspondingly regard the material as “inviscid plastic,” “rateindependent plastic,” or simply plastic. The inelastic strain εi will from now on be called the plastic strain and denoted εp instead of εi . The flow equations (3.1.6) may be written as ˙ ij , ε˙ pij = λh where λ˙ =
1 H
0,
(3.2.1)
◦
,
f = 0, f < 0,
(3.2.2)
with H as defined by Equation (3.1.1). The rate equations (3.1.5) analogously become ˙ α. ξ˙α = λh If ∂f /∂ξα ≡ 0, then, as mentioned before, the material is called perfectly ◦ ◦ plastic. In this case H = 0, but f = f˙, and therefore the condition f > 0
Section 3.2 / RateIndependent Plasticity
123
is impossible. Plastic deformation then occurs only if (∂f /∂σij )σ˙ ij = 0 (neutral loading), and the definition (3.2.2) of λ˙ cannot be used. Instead, λ˙ is an indeterminate positive quantity when f = 0 and (∂f /∂σij )σ˙ ij = 0, and is zero otherwise. In either case, λ˙ and f can easily be seen to obey the Kuhn–Tucker conditions of optimization theory: ˙ = 0, λf
λ˙ ≥ 0,
f ≤ 0.
The specification of the tensor function h in Equation (3.2.1), at least to within a multiplicative scalar, is known as the flow rule, and if there exists a function g (analogous to a viscoplastic potential) such that hij = ∂g/∂σij , then such a function is called a plastic potential .
Deformation Theory The plasticity theory in which the plastic strain is governed by rate equations such as (3.2.1) is known as the incremental or flow theory of plasticity. A deformation or totalstrain theory was proposed by Hencky [1924]. In this theory the plastic strain tensor itself is assumed to be determined by the stress tensor, provided that the yield criterion is met. Elastic unloading from and reloading to the yield surface are in principle provided for, although a contradiction is seen as soon as one considers reloading to a stress other than the one from which unloading took place, but located on the same yield surface; clearly, no plastic deformation could have occurred during the unloadingreloading process, yet the theory requires different values of the plastic strain at the two stress states. The deformation theory, which is mathematically much simpler than the flow theory, gives results that coincide with those of the latter only under highly restricted circumstances. An obvious example is the uniaxial case, provided that no reverse plastic deformation occurs; the equivalence is implicit in the use of relations such as (2.1.2). A more general case is that of a material element subject to proportional or radial loading, that is, loading in which the ratios among the stress components remain constant, provided the yield criterion and flow rule are sufficiently simple (for example, the Mises yield criterion and the flow rule with hij = sij ). A rough definition of “nearly proportional” loading, for which the deformation theory gives satisfactory results, is discussed by Rabotnov [1969]. It was shown by Kachanov [1954] (see also Kachanov [1971]) that the stress states derived from the two theories converge if the deformation develops in a definite direction. Another example of a range of validity of the deformation theory, discussed in separate developments by Budiansky [1959] and by Kliushnikov [1959], concerns a material whose yield surface has a singular point or corner, with the stress point remaining at the corner in the course of loading.
124
Chapter 3 / Constitutive Theory
For a simplified discussion, see Chakrabarty [1987], pp. 91–94. The deformation theory has recently been the subject of farreaching mathematical developments (Temam [1985]). It has also been found to give better results than the incremental theory in the study of the plastic buckling of elements under multiaxial stress, as is shown in Section 5.3.
WorkHardening The hardening criterion H > 0, and the corresponding criteria H = 0 for perfect plasticity and H < 0 for softening, were formulated in 3.1.1 for viscoplastic materials on the basis of ratedependent behavior at states outside the yield surface. An alternative derivation can be given entirely in the context of rateindependent plasticity. For given ξ, f (σ, ξ) = 0 is the equation describing the yield surface in stress space. If f (σ, ξ) = 0 and f˙σ=const < 0 (i.e. H > 0) at a given time ˙ t, then at a slightly later time t + ∆t we have f (σ, ξ + ξ∆t) < 0; the yield surface is seen to have moved so that σ is now inside it. In other words, H > 0 implies that, at least locally, the yield surface is expanding in stress space. The expansion of the yield surface is equivalent, in uniaxial stress, to a rising stressstrain curve (see Figure 3.2.1).
r
σspace
y X X f (σ, ξ + ξ∆t) ˙ = 0 if H > 0 PP f (σ, ξ) = 0 i Q k Q Q f (σ, ξ + ξ∆t) ˙ = 0 if H < 0
Figure 3.2.1. Hardening and softening in rateindependent plasticity: motion of yield surface in stress space Conversely, a contracting yield surface denotes worksoftening, and a stationary yield surface perfect plasticity. The description of worksoftening materials is best achieved in strain space rather than stress space, and is discussed later. For now, we treat workhardening materials only, with perfectly plastic materials as a limiting case. In the simplest models of plasticity the internal variables are taken as (1) the plastic strain components εpij themselves, and (2) the hardening variable κ, defined by either Equation (1.5.6) or (1.5.7) (in rateindependent plasticity, εp is written in place of εi ). When the yield function is taken to have
Section 3.2 / RateIndependent Plasticity
125
the form f (σ, εp , κ) = F (σ − ρ(εp )) − k(κ), both isotropic and kinematic hardening, as discussed in Section 3.1, can be described; the hardening is isotropic if ρ ≡ 0 and dk/dκ > 0, and purely kinematic if dk/dκ ≡ 0 and ρ 6= 0. The condition dk/dκ ≡ 0 and ρ ≡ 0 represents perfect plasticity. The simplest model of kinematic hardening — that of Melan [1938] — has ρ(εp ) = cεp , with c a constant. More sophisticated hardening models are discussed in Section 3.3.
Drucker’s Postulate A more restricted definition of workhardening was formulated by Drucker [1950, 1951] by generalizing the characteristics of uniaxial stressstrain curves. With a single stress component σ, the conjugate plastic strain rate ε˙ p clearly satisfies [see Figure 3.2.2(a)] σ˙ ε˙ p
≥ 0,
hardening material, = 0, perfectly plastic material, ≤ 0, softening material.
The inequalities are unchanged if the stress and plasticstrain rates are multiplied by the infinitesimal time increment dt, so that they hold equally well for dσ dεp . This product has the dimensions of work per unit volume, and was given by Drucker the following interpretation: if a unit volume of an elasticplastic specimen under uniaxial stress is initially at stress σ and plastic strain εp , and if an “external agency” (one that is independent of whatever has produced the current loads) slowly applies an incremental load resulting in a stress increment dσ (which causes the elastic and plastic strain increments dεe and dεp , respectively) and subsequently slowly removes it, then dσ dε = dσ (dεe + dεp ) is the work1 performed by the external agency in the course of incremental loading, and dσ dεp is the work performed in the course of the cycle consisting of the application and removal of the incremental stress. (Note that for dεp 6= 0, σ must be the current yield stress.) Since dσ dεe is always positive, and for a workhardening material dσ dεp ≥ 0, it follows that for such a material dσdε > 0. Drucker accordingly defines a workhardening (or “stable”) plastic material as one in which the work done during incremental loading is positive, and the work done in the loadingunloading cycle is nonnegative; this definition is generally known in the literature as Drucker’s postulate (see also Drucker [1959]). Having defined hardening in terms of work, Drucker naturally extends the definition to general threedimensional states of stress and strain, such that dσij dεij > 0 and dσij dεpij ≥ 0, 1
Actually it is twice the work.
126
Chapter 3 / Constitutive Theory
σ
σspace
ε˙p > 0 σr

σ˙ = 0
σ˙ > 0 σ˙ < 0 σ˙ > 0 =0 k σ˙
s
σ˙ < 0
ε
7
z rσ + dσ
=
r
σ∗ Elastic region
ε˙p < 0 (a)
(b)
Figure 3.2.2. Drucker’s postulate: (a) illustration in the uniaxial stressstrain plane; (b) illustration in stress space. the equality holding only if dεp = 0. For perfectly plastic (“neutrally stable”) materials Drucker’s inequalities are dσij dεij ≥ 0 and dσij dεpij = 0. It can be seen that the inequality σ˙ ij ε˙ pij ≥ 0, (3.2.3) sometimes known simply as Drucker’s inequality, is valid for both workhardening and perfectly plastic materials. Because it uses the concept of work, Drucker’s postulate is often referred to as a quasithermodynamic postulate, although it is quite independent of the basic laws of thermodynamics. Drucker’s inequality (3.2.3) may also be given an interpretation that is free of any considerations of incremental work: the lefthand side represents the scalar product σ˙ · ε˙ p , and the inequality therefore expresses the hypothesis that the plastic strain rate cannot oppose the stress rate. We should note, lastly, that Drucker’s definition of workhardening is in a sense circular. The definition assumes an external agency that is capable of applying arbitrary stress increments. But as can readily be seen from stressstrain diagrams, this assumption is not valid for softening or perfectly plastic materials; for example, in a tension test no increase in stress is possible. In other words, such materials are unstable under stress control . On the other hand, they are stable under strain control (or displacement control1 ), since arbitrary strain increments that do not violate internal constraints may, in principle, be applied. This fact points to the applicability of strainspace plasticity, to be discussed later, to a wider class of materials. Drucker’s statement of his workhardening postulate is broader than summarized above, in that the additional stress produced by the external 1
Stability under strain control and displacement control are equivalent when deformations are infinitesimal, but not when they are finite.
Section 3.2 / RateIndependent Plasticity
127
agency need not be a small increment. In particular, the initial stress, say σ ∗ , may be inside the elastic region, or at a point on the yield surface far away from σ, and the process followed by the external agency may consist of elastic loading to a stress σ on the current yield surface, a small stress increment dσ producing an incremental plastic strain dε, and finally, elastic unloading back to σ ∗ ; the path is illustrated in Figure 3.2.2(b). With dσ neglected alongside σ − σ ∗ , the work per unit volume done by the external ∗ ) dεp . Drucker’s postulate, consequently, implies agency is (σij − σij ij ∗ (σij − σij ) ε˙ pij ≥ 0.
3.2.2.
(3.2.4)
MaximumPlasticDissipation Postulate and Normality
MaximumPlasticDissipation Postulate Inequality (3.2.4) is, as we have just seen, a necessary condition for Drucker’s postulate, but it is not a sufficient one. In other words, its validity is not limited to materials that are workhardening in Drucker’s sense. Its significance may best be understood when we consider its uniaxial counterpart, (σ − σ ∗ )˙εp ≥ 0. As is seen in Figure 3.2.3, the inequality expresses the property that the σ
rσ
ε˙p ≥ 0
r
σ∗
rσ∗
ε
ε˙p
≤0 σ
r
Figure 3.2.3. Maximumplasticdissipation postulate: illustration in the uniaxial stressstrain plane. plastic strain rate is positive (negative) only if the current stress σ is not less than (not greater than) any stress σ ∗ in the current elastic range — in other words, if σ equals the current tensile (compressive) yield stress.
128
Chapter 3 / Constitutive Theory
Clearly, worksoftening and perfectly plastic materials have this property as well. Inequality (3.2.4) thus constitutes a postulate in its own right, called the postulate of maximum plastic dissipation. It was proposed independently by Mises [1928], Taylor [1947] and Hill [1948a]; it was derived from considerations of crystal plasticity by Bishop and Hill [1951], and is shown later to follow also from Il’iushin’s postulate of plasticity in strain space.
Consequences of MaximumPlasticDissipation Postulate Inequality (3.2.4) has consequences of the highest importance in plasticity theory. To examine them, we represent symmetric secondrank tensors as vectors in a sixdimensional space, as in 1.3.5, but using boldface rather than underline notation, and using the dotproduct notation for the scalar product. Our inequality may thus be written as (σ − σ ∗ ) · ε˙ p ≥ 0. We suppose at first that the yield surface is everywhere smooth, so that a welldefined tangent hyperplane and normal direction exist at every point. It is clear from the twodimensional representation in Figure 3.2.4(a) that if (3.2.4) is to be valid for all σ ∗ to the inward side of the tangent to the yield surface at σ, then ε˙ p must be directed along the outward normal there; this consequence is known as the normality rule. But as can be seen in Figure 3.2.4(b), if there are any σ ∗ lying to the outward side of the tangent, the inequality is violated. In other words, the entire elastic region must lie to one side of the tangent. As a result, the yield surface is convex. S Q S S rXX > XXXS z X r :σ 6 S r S : σ−σ ∗ r S r σ∗
ε˙ p
ε˙ p
Q Q
ε˙ p
Q
rX QX y XXr σ∗ σ Q Q Q Q
X
3 :
r σ C
Q
S
(a)
(b)
(c)
Figure 3.2.4. Properties of yield surface with associated flow rule: (a) normality; (b) convexity; (c) corner. Let us define Dp (ε˙ p ; ξ) by ∗ p Dp (ε˙ p ; ξ) = max σij ε˙ ij , ∗ σ
Section 3.2 / RateIndependent Plasticity
129
the maximum being taken over all σ ∗ such that f (σ ∗ , ξ) ≤ 0. It follows from (3.2.4) that σij ε˙ pij = Dp (ε˙ p ; ξ). (3.2.5) To make it clear that Dp (ε˙ p ; ξ) depends only on ε˙ p and ξ and not on σ, we note that, if the yield surface is strictly convex at σ (whether this point is regular or singular), then this is the only stress that corresponds to a given normal direction in stress space and hence to a given ε˙ p . If the yield surface has a flat portion, then all points on this portion have the same normal, that is, different stresses correspond to the same ε˙ p , but the scalar product σ · ε˙ p = σij ε˙ pij is the same for all of them. Dp (ε˙ p ; ξ) will be called simply the plastic dissipation. Inequality (3.2.4) may now be rewritten as ∗ p Dp (ε˙ p ; ξ) ≥ σij ε˙ ij ,
(3.2.6)
giving explicit meaning to the name “principle of maximum plastic dissipation.”
Normality The normality rule is now discussed in more detail. At any point of the yield surface f (σ, ξ) = 0 where the surface is smooth, the outward normal vector is proportional to the gradient of f (in stress space), and therefore, reverting to indicial notation, we may express the normality rule as hij =
∂f , ∂σij
(3.2.7)
where hij is the tensor function appearing in the flow equation (3.2.1). Equation (3.2.7) expresses the result that the function f defining the yield surface is itself a plastic potential, and therefore the normality rule is also called a flow rule that is associated with the yield criterion, or, briefly, an associated (sometimes associative) flow rule. A flow rule derivable from a plastic potential g that is distinct from f (more precisely, such that ∂g/∂σij is not proportional to ∂f /∂σij ) is accordingly called a nonassociated flow rule. In the French literature, materials obeying an associated flow rule are usually called standard materials, and this term will often be used here. We are now in a position to say that Drucker’s postulate applies to standard workhardening (or, in the limit, perfectly plastic) materials. The frequently expressed notion that Drucker’s postulate is required for the convexity of the yield surface and for the normality rule is clearly erroneous, as is the idea that workhardening materials are necessarily standard. If the yield surface is not everywhere smooth but has one or more singular points (corners) at which the normal direction is not unique, then at such a point ε˙ p must lie in the cone formed by the normal vectors meeting there [see Figure 3.2.4(c)]. The argument leading to the convexity of the yield surface
130
Chapter 3 / Constitutive Theory
is not affected by this generalization. As will be seen, Equation (3.2.7) can still be formally used in this case, provided that the partial derivatives are properly interpreted. In a rigorous treatment, the concept of gradient must be replaced by that of subgradient, due to Moreau [1963]; its application in plasticity theory was formulated by Moreau [1976]. Another treatment of singular yield surfaces was proposed by Koiter [1953a], who supposed the yield surface to be made of a number — say n — of smooth surfaces, each defined by an equation fk (σ, ξ) = 0 (k = 1, ..., n); the elastic region is the intersection of the regions defined by fk (σ, ξ) < 0, and σ is on the yield surface if at least one of the fk vanishes there, it being a singular point only if two or more of the fk vanish. Equation (3.2.7) is replaced by X ∂fk hij = αk , ∂σ ij k the summation being over those k for which fk (σ, ξ) = 0, and the αk are nonnegative numbers that may, with no loss of generality, be constrained so P that k αk = 1.
3.2.3.
StrainSpace Plasticity
As we noted above, it is only in workhardening materials, which are stable under stress control, that we may consider processes with arbitrary stress increments, and therefore it is only for such materials — with perfect plasticity as a limiting case — that a theory in which stress is an independent variable may be expected to work. No such limitation applies to theories using strain as an independent variable. Surprisingly, such theories were not proposed until the 1960s, beginning with the pioneering work of Il’iushin [1961], followed by papers by Pipkin and Rivlin [1965], Owen [1968], Lubliner [1974], Nguyen and Bui [1974], Naghdi and Trapp [1975], and others. To see that strainspace yield surfaces have the same character whether the material is workhardening or worksoftening, let us consider one whose stressstrain diagram in tension/compression or in shear is as shown in Figure 3.2.5(a); such a material exemplifies Melan’s linear kinematic hardening if E 0 > 0, and is perfectly plastic if E 0 = 0. The stress σ is on the yield surface if σ = E 0 ε ± (1 − E 0 /E)σE , and therefore the condition on the strain ε is E(ε − εp ) = E 0 ε ± (1 − E 0 /E)σE , or, equivalently, ε = [E/(E − E 0 )]εp ± εE , where εE = σE /E [see Figure 3.2.5(b)]. A yield surface in εspace is thus given by the pair of points corresponding to a given value of εp , and the εεp diagram has a “stable” form (i.e., a positive slope) for all E 0 < E, even if negative.
Yield Criterion and Flow Rule in Strain Space To formulate the threedimensional yield criterion in strain space, let C
Section 3.2 / RateIndependent Plasticity
131 ε
σ
σE
0 E 1 1
E 1 ) −σE ) 1 0 E
1
E/(E−E 0 )
? εE
εp
ε −εE
(a)
(b)
Figure 3.2.5. Material with linear hardening: (a) stressstrain diagram; (b) εεp diagram. denote the elastic modulus tensor, so that the σεεp relation may be written def σ = C · (ε − εp ) [i.e., σij = Cijkl (εkl − εpkl )]. If fˆ(ε, ξ) = f (C · (ε − εp ), ξ), then the strainspace yield criterion is just fˆ(ε, ξ) = 0. Since ∂ fˆ ∂f = Cijkl ∂εij ∂σkl σ=C·(ε−εp )
,
the same logic that led to (3.2.1)–(3.2.2) produces the flow equations ε˙ pij =
1
L
hij , f = 0, ∂σij f < 0,
(3.2.8)
∂f hkl . ∂σij
(3.2.9)
where L=−
X ∂ fˆ α
∂ξα
hα = H + Cijkl
The normality rule (3.2.7), when translated into the strainspace formulation, takes the form ˆ −1 ∂ f hij = Cijkl . ∂εkl Note that L may very well be, and normally may be assumed to be, positive even when H is zero or negative, that is, for perfectly plastic or worksoftening materials. It is thus not necessary to distinguish between these material types, the only restriction being L > 0. This condition describes
132
Chapter 3 / Constitutive Theory
stability under strain control in the same sense that the workhardening criterion H > 0 describes stability under stress control; it will here be called kinematic stability. The flow equation given by (3.2.8)–(3.2.9), when combined with the relation σ˙ ij = Cijkl (˙εkl − ε˙ pkl ), yields σ˙ ij = Cijkl ε˙ kl −
1
L
Cijmn hmn , ∂σpq
0,
f = 0,
(3.2.10)
f < 0.
˙ which may be regarded This is an explicit expression for σ˙ in terms of ε, −1 as an inversion of ε˙ ij = Cijkl σ˙ kl + ε˙ pij with ε˙ p given by Equation (3.2.1). In this sense the result, which was first derived by Hill [1958] [for standard materials, i.e. with h given by (3.2.7)], is not necessarily based on strainspace plasticity.
Workhardening (Plastic) Modulus It is easy to show that when ε˙ p 6= 0, H = (Cijkl fij hkl )
fij σ˙ ij , Cijkl fij ε˙ kl
where fij = ∂f /σij . Thus H may be related to the socalled workhardening modulus or plastic modulus dσ/dεp obtained in a simple tension test. If the material has (a) elastic isotropy, (b) plastic incompressibility, and (c) sufficient plastic symmetry so that σij = σδi1 δj1 implies that ε˙ p22 = ε˙ p33 = − 12 ε˙ p11 and ε˙ pij = 0 for i 6= j, then (with εp = εp11 ) H = h11 f11
dσ . dεp
Il’iushin’s Postulate It can also be shown that the normality rule follows from a “postulate of plasticity” in strain space first proposed by Il’iushin [1961], namely, that in any cycle that is closed in strain space, I
σij dεij ≥ 0,
(3.2.11)
where the equality holds only if the process is elastic; we show this by proving that (3.2.11) implies the maximumplasticdissipation postulate (3.2.4). Consider a state (ε1 , ξ 1 ) with ε1 on the yield surface, and any strain ε∗ on or inside both the current yield surface and the subsequent yield surface obtained after a brief plastic process of duration ∆t from (ε1 , ξ 1 ) to (ε1 + ˙ ˙ ε∆t, ξ 1 + ξ∆t), that is, fˆ(ε1 , ξ 1 ) = 0,
˙ ˙ fˆ(ε1 + ε∆t, ξ 1 + ξ∆t) = 0,
Section 3.2 / RateIndependent Plasticity
133
and fˆ(ε∗ , ξ 1 ) ≤ 0,
˙ fˆ(ε∗ , ξ 1 + ξ∆t) ≤ 0.
In the cycle 1 2 3 ˙ ˙ ˙ (ε∗ , ξ 1 ) → (ε1 , ξ 1 ) → (ε1 + ε∆t, ξ 1 + ξ∆t) → (ε∗ , ξ 1 + ξ∆t),
segments 1 and 3 are elastic, so that, if the process is isothermal,
σij ε˙ ij =
ρψ˙ ρψ˙ + D
in 1 and 3 in 2,
where ψ(ε, ξ) is X the free energy per unit mass at the given temperature and ˙ = −ρ (∂ψ/∂ξ ) ξ˙α is the dissipation per unit volume. Now D(ε, ξ, ξ) α α
I
I
σij dεij =
Z
D dt;
ρ dψ + 2
but I
. ˙ ˙ ρ dψ = ρψ(ε∗ , ξ 1 + ξ∆t) − ρψ(ε∗ , ξ 1 ) = −D(ε∗ , ξ 1 , ξ)∆t,
. ˙ and size − 1int2 D dt = D(ε1 , ξ 1 , ξ)∆t, the approximations being to within o(∆t). It follows that ˙ ≥ D(ε∗ , ξ, ξ) ˙ D(ε, ξ, ξ)
(3.2.12)
(the superscripts 1 can now be dropped) if (ε, ξ) is a state with ε on the ˙ and ε∗ is any strain on or inside current yield surface with corresponding ξ, the yield surface. With the freeenergy density decomposed as in Equation (1.5.5) (and εp written in place of εi ), D = σij ε˙ pij − ρψ˙ i and therefore, if σ ∗ = C · (ε∗ − εp ) is any stress on or inside the yield surface, inequality (3.2.12) is equivalent to (3.2.4), which is thus seen to be a consequence of Il’iushin’s postulate. It remains to be investigated whether the converse holds. Consider an arbitrary process that is closed in strain space, going from (ε∗ , ξ 1 ) to (ε∗ , ξ 2 ), with ξ 2 not necessarily infinitesimally close to ξ 1 . At any state of the process, ˙ σij ε˙ ij = ρψ˙ + D(ε, ξ, ξ), with D = 0 whenever the process is instantaneously elastic, and therefore I
I
σij dεij =
˙ − D(ε∗ , ξ, ξ)] ˙ dt. [D(ε, ξ, ξ)
According to the principle of maximum plastic dissipation, the integrand is nonnegative whenever ε∗ is on or inside the strainspace yield surface at the
134
Chapter 3 / Constitutive Theory
current value of ξ, and therefore Il’iushin’s postulate is satisfied for processes in which the original yield surface is inside all subsequent yield surfaces. The last condition is satisfied in materials with isotropic hardening, but not in general. Consequently Il’iushin’s postulate is a stronger (i.e. less general) hypothesis than the principle of maximum plastic dissipation.
Nguyen–Bui Inequality On the other hand, an inequality first explicitly stated by Nguyen and Bui [1974] may be shown to be weaker than the maximumplasticdissipation principle. It is readily seen that this principle, as expressed in the form (3.2.12), is equivalent to Cijkl (εkl − ε∗kl )˙εpij ≥ 0
(3.2.13)
for any strain ε∗ that is on or inside the current yield surface in strain space. Suppose, in particular, that ε∗ is close to ε and is given by ε∗ = ε ± ε˙ dt, with dt > 0 and ε˙ the strainrate tensor in a possible process. With the plus sign chosen, the process goes from ε to ε∗ and is necessarily elastic, so that ε˙ p = 0 and therefore Inequality (3.2.13) is satisfied as an equality. Thus ε˙ 6= 0 only if the minus sign is taken, and therefore (3.2.13) takes the local form Cijkl ε˙ pij ε˙ kl ≥ 0, (3.2.14) or the equivalent form given by Nguyen and Bui, σ˙ ij ε˙ pij ≥ Cijkl ε˙ pij ε˙ pkl . Inequality (3.2.14), like Drucker’s inequality (3.2.3), may be interpreted as a stability postulate, this time in strain space: if we take Cijkl aij bkl as defining a scalar product between two tensors a and b in strainincrement space, then (3.2.14) expresses the notion that the plastic strain rate cannot oppose the total strain rate. Inequality (3.2.14) is by itself sufficient for the associated flow rule to follow, and consequently describes standard kinematically stable materials.
Exercises: Section 3.2 1. A workhardening plastic solid is assumed to obey√the Mises yield criterion with isotropic hardening, that is, f (σ, ξ) = J2 − k(εp ), and the flow rule hij = sij . Show that √ 3sij <skl s˙ kl > p ε˙ ij = . 4k 2 k 0 (εp ) 2. Show that the solid described in Exercise 1 obeys Drucker’s inequality (3.2.3) if and only if k 0 (εp ) > 0.
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
135
3. If σ and σ ∗ are stresses such that J2 = k 2 and J2∗ ≤ k 2 , show that (sij − s∗ij )sij ≥ 0, and hence that the solid of Exercise 1 obeys the maximumplasticdissipation postulate (3.2.4) independently of k 0 (εp ), that is, whether the solid hardens or softens. 4. For a workhardening solid with the yield criterion of Exercise 1, but with the nonassociated flow rule hij = sij + tij , where sij tij = 0, show that for some σ˙ Drucker’s inequality (3.2.3) is violated. 5. For the standard isotropically hardening Mises solid of Exercise 1, show that sij <skl ε˙ kl > ε˙ pij = . k 0 (εp ) 2 2k 1 + √ 3G 6. Show that the standard Mises solid obeys the Nguyen–Bui inequality (3.2.14) whether it hardens or softens.
Section 3.3 3.3.1.
Yield Criteria, Flow Rules and Hardening Rules
Introduction
The yield function f in stress space may be written with no loss of generality in terms of the stress deviator and the first invariant of stress, that is, f (σ, ξ) = f (s, I1 , ξ), where I1 = σkk = δij σij , so that ∂I1 /∂σij = δij . Since 1 1 skl = σkl − I1 δkl = δik δjl − δij δkl σij , 3 3
it follows that ∂skl /∂σij = δik δjl − 13 δij δkl . Consequently, ∂f ∂f ∂skl ∂f ∂f ∂I1 = + = (f ij − 13 δij f kk ) + δij , ∂σij ∂skl ∂σij ∂I1 ∂σij ∂I1 where f ij = ∂f /∂sij . Accordingly, in a standard material plastic volume change (“dilatancy”) occurs if and only if the yield criterion depends on I1 , i.e. on the mean stress, and, conversely, plastic incompressibility obtains if and only if the yield criterion depends on s but not on I1 . If the yield criterion of a plastically incompressible material is significantly affected by mean stress, then the material is necessarily nonstandard.
Isotropic Yield Criteria
136
Chapter 3 / Constitutive Theory
If the yield criterion is initially isotropic, then the dependence of f on σ must be through the stress invariants I1 , I2 , and I3 , or, equivalently, on the principal stresses σI (I = 1, 2, 3), provided this dependence is symmetric, that is, invariant under any change of the index I. Similarly, the dependence of f on s must be through the stressdeviator invariants J2 and J3 ; the equivalent dependence on the principal stresses may be exhibited in the socalled principal stressdeviator plane or πplane, namely, the plane in σ1 σ2 σ3 space given by σ1 + σ2 + σ3 = 0, shown in Figure 3.3.1. J J
σ3
σ2
6 ........................................... J . . . . ........................................................................... .... .... .... .... . ........... J .................................................................................................................................................................................. ... ... ... ... ... ... ... PH .......................................................................................................................... Y .. .. .. .. .. H ........................J J ................... . . ....................................... . . . . . . . . H ........................................................................................................................... .s..O ...................................... ..... σ1 ...........................J .............................H ..........J . . .. ... .... .... ........................... ................................................................................................................ ..........................J ....... ... ... ............... .......................................................J ........ ...........0.............................J . ...................... ...............................P ......................................................................................................... . πplane ......................................................................... J .................................................... ......................... J σ1 =σ2 =σ3 J J
Figure 3.3.1. πplane. Indeed, if a point P (σ1 , σ2 , σ3 ) in σ1 σ2 σ3 space (the Haigh–Westergaard →
→
space) is represented by the vector OP , then its projection OP 0 onto the πplane is the vector whose components are the principal stress deviators s1 , s2 , s3 . The magnitude of this projection — that is, the distance from P √ to the axis σ1 = σ2 = σ3 — is just 2J2 . A yield surface that is independent of I1 has, in this space, the form of a cylinder perpendicular to the πplane, and therefore may be specified by a single curve in this plane. A yield surface that depends on I1 may be described by a family of curves in the πplane, each corresponding to a different value of I1 and forming the intersection of the yield surface in σ1 σ2 σ3 space with a plane I1 = constant, that is, a plane parallel to the πplane. A curve√in the πplane can also be described in terms of the polar coordinates ( 2J2 , θ), where the polar angle θ may defined as that measured from the projection of the σ1 axis toward the projection of the σ2 axis, and can be shown to be given by √
tan θ =
3(σ2 − σ3 ) s2 − s3 = √ . 2σ1 − σ2 − σ3 3s1
Using some trigonometric identities and the fact that s1 + s2 + s3 = 0, it is also possible to define θ in terms of the deviatoric stress invariants J2 and
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules J3 :
137
√ 3 3J3
. 3/2 2J2 A point with θ = 0 corresponds to σ1 > σ2 = σ3 ; the locus of such points on the yield surface is said to represent one of the three tensile meridians of the surface. A point with θ = π/3 corresponds to σ1 = σ2 > σ3 , and lies on a compressive meridian. cos 3θ =
3.3.2.
Yield Criteria Independent of the Mean Stress
Since the concept of plasticity was first applied to metals, in which the influence of mean stress on yielding is generally negligible (Bridgman [1923, 1950]), the oldest and most commonly used yield criteria are those that are independent of I1 . Such criteria have an alternative twodimensional representation: since their dependence on the principal stresses must be through the differences σ1 − σ2 , σ1 − σ3 and σ2 − σ3 , and since σ1 − σ2 = (σ1 −σ3 )−(σ2 −σ3 ), the yield criterion can be plotted in a plane with σ1 −σ3 and σ2 − σ3 as coordinate axes.
Tresca Criterion The Tresca yield criterion is historically the oldest; it embodies the assumption that plastic deformation occurs when the maximum shear stress over all planes attains a critical value, namely, the value of the current yield stress in shear, denoted k(ξ). Because of Equation (1.3.11), this criterion may be represented by the yield function f (σ, ξ) =
1 max (σ1 − σ2 , σ2 − σ3 , σ3 − σ1 ) − k(ξ), 2
(3.3.1)
or, equivalently, 1 f (σ, ξ) = (σ1 − σ2  + σ2 − σ3  + σ3 − σ1 ) − k(ξ). 4
(3.3.2)
The projection of the Tresca yield surface in the πplane is a regular hexagon, shown in Figure 3.3.2(a), whose vertices lie on the projections of the positive and negative σ1 , σ2 and σ3 axes, while in the (σ1 − σ3 )(σ2 − σ3 )plane it takes the form of the irregular hexagon shown in Figure 3.3.2(b). Of course, the forms (3.3.1) and (3.3.2) for the Tresca yield function are not unique. The form f (σ) = [(σ1 − σ2 )2 − 4k 2 ][(σ2 − σ3 )2 − 4k 2 ][(σ1 − σ3 )2 − 4k 2 ] (with the dependence on ξ not indicated) has the advantage of being analytic and, moreover, expressible in terms of the principal stressdeviator invariants J2 and J3 : f (σ) = 4J2 3 − 27J32 − 36k 2 J2 2 + 96k 4 J2 − 64k 6 .
138
Chapter 3 / Constitutive Theory
σ2 −σ3
Tresca
σ3 2k
?
Tresca
Mises
Mises 0
σ1
√
0 k
σ1 +σ2 +σ3 =0
3k
σ1 −σ3 2k
σ2
(a)
(b)
Figure 3.3.2. Projections of Tresca and Mises yield surfaces: (a) πplane; (b) σ1 −σ3 σ2 −σ3 plane.
Tresca Criterion: Associated Flow Rule Although the Tresca yield surface is singular, we can nonetheless derive its associated flow rule by means of a formal application of Equation (3.2.7) to the second form, Equation (3.3.2). We write d x = sgn x, dx where
(3.3.3)
+1, x > 0 −1, x < 0 defines the signum function for x 6= 0. It is conventional to define sgn 0 = 0, but in the present context it is more convenient if sgn x does not have a unique value at 0 but can have any value between −1 and 1. Strictly speaking, then, it is not a function in the usual sense but a setvalued function or multifunction, a concept with considerable use in convex analysis.1 In this way we obtain sgn x = 2H(x) − 1 =
1˙ ε˙ p1 = λ[sgn (σ1 − σ2 ) + sgn (σ1 − σ3 )], 4 where, in accordance with Equations (3.2.1)–(3.2.2), for workhardening ma◦ terials λ˙ = /H, with H=
X ∂k α
1
∂ξα
hα ,
In fact, our use of Equation (3.3.3) comes rather close to the subdifferential calculus of Moreau.
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
139
while for the perfectly plastic material λ˙ is indeterminate. Similar expressions are obtained for ε˙ p2 and ε˙ p3 . Thus, if the principal stresses are all distinct, ˙ ε˙ p = 0, ε˙ p = − 1 λ. ˙ If, on and ordered such that σ1 > σ2 > σ3 , then ε˙ p1 = 12 λ, 2 3 2 p p p ˙ ˙ ˙ ε˙ = 1 λ(1−β), ε˙ = − 1 λ, the other hand, σ1 = σ2 > σ3 , then ε˙ = 1 λ(1+β), 1
4
2
4
3
2
where β is any real number between −1 and 1. Analogous expressions can be obtained for all other combinations of principal stresses. The Tresca flow rule can also be obtained by the method due to Koiter, discussed in 3.2.2. It can be seen that for every combination of principal stresses, ˙εp1  + ˙ and therefore the plastic dissipation is given by ˙εp2  + ˙εp3  = λ, ˙ Dp (ε˙ p ; ξ) = λk(ξ) = k(ξ)(˙εp1  + ˙εp2  + ˙εp3 ). If it is desired to use an effective plastic strain εp as an internal variable in conjunction with the Tresca criterion and its associated flow rule, then the definition Z 1 p ε = (˙εp1  + ˙εp2  + ˙εp3 ) dt 2 is more appropriate than (1.5.7). In Rfact, if it is assumed that k is a function of εp as thus defined, then Wp = 2 k dεp , so that a onetoone correspondence can be established between Wp and εp .
L´evy Flow Rule and Mises Yield Criterion In the nineteenth century SaintVenant and others used the Tresca yield criterion together with the (nonassociated) flow rule derived from the J2 potential (see 1.5.4) whose general form was first proposed (for total rather than plastic strain) by L´evy, namely, ˙ ij , ε˙ pij = λs with λ˙ defined as above. As seen in Section 3.1 in connection with viscoplasticity, and as first pointed out by Mises [1913], the yield criterion with which this flow rule is associated is the Mises criterion, represented by the yield function p f (σ, ξ) = J2 − k(ξ), where k(ξ) is again the yield stress in shear at the current values of ξ. In view of the relation (1.3.5) between J2 and the octahedral shear stress, the Mises criterion is also known as the maximumoctahedralshearstress criterion, and as a result of Equation (1.4.17), which shows the complementary energy of an isotropic, linearly elastic material to be uncoupled into volumetric and distortional parts, it is also called the maximumdistortionalenergy criterion. An alternative — and analytic — form of the Mises yield function (with the dependence on ξ not shown explicitly) is f (σ) = J2 − k 2 .
140
Chapter 3 / Constitutive Theory
Expressing J2 in terms of the principal stresses (see Section 1.3), we may formulate the Mises yield criterion in the form (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ1 − σ3 )2 = 6k 2 or σ12 + σ22 + σ32 − σ2 σ3 − σ3 σ1 − σ1 σ2 = 3k 2 . The form √ taken by the Mises yield surface in the πplane is that of a circle of radius 2k, and in the (σ1 − σ3 )(σ2 − σ3 )plane that of an ellipse. Both forms are shown, along with those for the Tresca criterion, in Figure 3.3.2 (page 138). The plastic dissipation for the Mises criterion and associated flow rule is given by ˙ ij sij = Dp (ε˙ p ; ξ) = σij ε˙ pij = λs
q
2J2 ε˙ pij ε˙ pij
p
q
= k(ξ) 2˙εpij ε˙ pij . If k is a function of εp as defined by (1.5.7), then Wp is in onetoone correspondence with εp . As mentioned above, L´evy and Mises formulated the flow rule bearing their name for the total, rather than merely the plastic, strain rate; in this form it is valid as an approximation for problems in which elastic strains are vanishingly small, or, equivalently, for materials whose elastic moduli are infinite — the socalled rigidplastic materials (see Section 3.4). The generalization allowing for nonvanishing elastic strains is due to Prandtl [1924] and Reuss [1930]; expressed in terms of total strain rate, with isotropic linear elasticity, the result is known as the Prandtl–Reuss equations: 1 σ˙ kk , 3K 1 ˙ ij . e˙ ij = s˙ ij + λs 2G
ε˙ kk =
(3.3.4)
Some generalizations of the Mises yield function have been proposed so that dependence on J3 is included. A typical form is f (σ) =
J2 1 − c 33 J2
!α
J2 − k 2 .
The exponent α has variously been taken as 13 and 1, k is as usual the yield stress in simple shear, and c is a parameter that is to be determined so as to optimize the fit with experimental data.
Anisotropic Yield Criteria
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
141
Anisotropy in yielding may be of two types: initial anisotropy and induced anisotropy. The former exists in materials that are structurally anisotropic, even before any plastic deformation has taken place; the latter appears, even in initially isotropic materials, as a result of workhardening (Section 2.1). An example of an initially anisotropic yield criterion is Schmid’s law (Section 2.2), according to which yielding in single crystals occurs when the shear stress on certain preferred planes (the slip planes) reaches a critical value; in the special case when every plane is a slip plane, Schmid’s law reduces to the Tresca criterion. An anisotropic generalization of the Mises criterion is due to Hill [1950]; it replaces J2 with a general quadratic function of σ and therefore has the form 1 Aijkl σij σkl = k 2 , 2 where A is a fourthrank tensor which has the same symmetries as the elasticity tensors (Aijkl = Ajikl = Aklij ). If the yield criterion is independent of mean stress, then A also obeys Aijkk = 0, so that it has at most fifteen independent components (like a symmetric 5 × 5 matrix); the isotropic (Mises) case corresponds to Aijkl = δik δjl − 31 δij δkl . A special case considered by Hill [1948b] refers to a material with three mutually perpendicular planes of symmetry; if a Cartesian basis is chosen so that the coordinate planes are parallel to the planes of symmetry, then in this basis the components of A coupling normal stresses with shear stresses (e.g. A1112 , A1123 , etc. — nine independent components altogether) are zero, and A is given by Aijkl σij σkl = A(σ22 − σ33 )2 + B(σ11 − σ33 )2 + C(σ11 − σ22 )2 2 2 2 + 4Dσ23 + 4Eσ13 + 4F σ12 ,
where A, . . . , F are constants; clearly A1111 = B + C, A1122 = −C, A1133 = −B, A1212 = F , and so on.
3.3.3.
Yield Criteria Dependent on the Mean Stress
A yield criterion depending on the mean stress becomes necessary when it is desired to apply plasticity theory to soils, rocks, and concrete, as discussed in Section 2.3. One such criterion has its origin in the Mohr theory of rupture, according to which failure (rupture) occurs on a plane in a body if the shear stress and normal stress on that plane achieve a critical combination. Since the strength properties of an isotropic material are unchanged when the direction of the shear stress is reversed, the critical combination may be expressed by the functional equation τ = ±g(σ). This equation represents a pair of curves (each being the other’s reflection through the σaxis) in the Mohr plane, and a state of stress, as determined by the three Mohr’s circles, is safe if all three circles lie between the curves, while it is a critical state if
142
Chapter 3 / Constitutive Theory
one of the three is tangent to the curves. These curves are thus the envelopes of the Mohr’s circles representing failure and are therefore called the Mohr failure (rupture) envelopes. The point (σ, τ ) is a point of tangency — say the upper one — if it obeys (1) the equation τ = g(σ), (2) the equation of the Mohr’s circle [centered at (σm , 0) and of radius τm ], and (3) the tangency condition. If σ and τ are eliminated between these three equations, there remains an equation in terms of σm and τm , which constitutes the failure criterion.1 Concretely, if a point in principalstress space is located in the sextant σ1 > σ2 > σ3 , then σm = 12 (σ1 + σ3 ) and τm = 12 σ1 − σ3 ; the equation consequently represents a cylindrical surface parallel to the σ2 axis, and the failure surface is formed by six such surfaces.
Mohr–Coulomb Criterion The equations can be reduced explicitly if the Mohr envelopes are straight lines, that is, if g(σ) = c − µσ. This is just Equation (2.3.3), with the sign of σ changed to the usual convention whereby it is positive in tension; c is the cohesion, and µ = tan φ is the coefficient of internal friction in the sense of the Coulomb model of friction. The resulting criterion is consequently known as the Mohr–Coulomb criterion. It is convenient to represent the Mohr’s circle parametrically: σ = σm + τm cos 2α,
τ = τm sin 2α,
where α is the angle between the failure plane and the axis of the least tensile (greatest compressive) stress. The tangency condition is then µ = cot 2α, so that α = 14 π − 12 φ, sin 2α = cos φ, and cos 2α = sin φ. The equation in terms of σm and τm becomes τm + σm sin φ = c cos φ, from which it is seen that the failure stress in simple shear is c cos φ. (Needless to say, when φ = 0 the Mohr–Coulomb criterion reduces to that of Tresca.) In terms of the principal stresses the criterion takes the form max[σi − σj  + (σi + σj ) sin φ] = 2c cos φ, i6=j
so that the yield stresses in tension and compression are respectively 2c cos φ/(1+ sin φ) = 2c tan α and 2c cos φ/(1 − sin φ) = 2c cot α. The associated plastic dissipation was shown by Drucker [1953] to be Dp (ε˙ p ; ξ) = c cot φ(˙εp1 + ε˙ p2 + ε˙ p3 ). 1
It is pointed out by Hill [1950] that tangency between the Mohr envelope and Mohr’s circle does not necessarily occur at real (σ, τ ), and that it is the failure criterion and not the envelope that is fundamental.
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
143
The failure surfaces in σ1 σ2 σ3 space are obviously planes that intersect to form a hexagonal pyramid; the plane in the sextant σ1 > σ2 > σ3 , for example, is described by σ1 − σ3 + (σ1 + σ3 ) sin φ = 2c cos φ. A form valid in all six sextants is σmax − σmin + (σmax + σmin ) sin φ = 2c cos φ, where σmax and σmin denote respectively the (algebraically) largest and smallest principal stresses. The last equation may be rewritten as 2 1 σmax − σmin + [(σmax − σint ) − (σint − σmin )] sin φ = 2c cos φ − I1 sin φ, 3 3 where σint denotes the intermediate principal stress. The lefthand side, being an isotropic function of the stress deviator, is therefore a function of J2 and J3 . The Mohr–Coulomb criterion is therefore seen to be a special case of the family of criteria based on Coulomb friction and described by equations of the form F¯ (J2 , J3 ) = c − λI1 , where c and λ are constants.
Drucker–Prager Criterion Another yield criterion of this family, combining Coulomb friction with the Mises yield criterion, was proposed by Drucker and Prager [1952] and has become known as the Drucker–Prager criterion. With the Mises criterion interpreted in terms of the octahedral shear stress, it may be postulated that p yielding occurs on the octahedral planes when τoct = 23 k − 13 µI1 , so that, in view of Equation √ criterion may be represented by the yield func√ (1.3.5), the tion f (s, I1 ) = J2 + µI1 / 6 − k. The yield surface in Haigh–Westergaard space is a right √ circular cone about the meanstress axis, subtending the −1 angle tan ( 3µ). The yield tension, √ stresses in √ simple shear, √ √and compression are respectively k, 3k/(1 + µ/ 2) and 3k/(1 − µ/ 2); note √ that for this criterion to be physically meaningful, µ must be less than 2. The associated plastic dissipation is q
k 2˙εpij ε˙ pij
Dp (ε˙ p ; ξ) = p
1 + µ2
.
Projections of the yield surfaces corresponding to the Mohr–Coulomb and Drucker–Prager criteria onto a plane parallel to the πplane (i.e. one with σ1 + σ2 + σ3 = constant) are shown in Figure 3.3.3(a).
144
Chapter 3 / Constitutive Theory σ2 σ3
Mohr–Coulomb @ @ + Drucker–Prager @ @
σ1
σ1
σ3 =0 Y H H Drucker–Prager Mohr–Coulomb
σ1 +σ2 +σ3 = const.
σ2
(a)
(b)
Figure 3.3.3. Mohr–Coulomb and Drucker–Prager criteria: (a) plane parallel to πplane; (b) plane stress.
Mises–Schleicher Criterion A yield criterion that takes into account the difference between the yield strengths in tension and compression was discussed by Mises [1926] and Schleicher [1926]. If σT and σC denote, respectively, the tensile and compressive yield stresses, then the criterion may be expressed in the form 3J2 + (σC − σT )I1 − σT σC = 0. The associated plastic dissipation is p p σC − σT e˙ ij e˙ ij σC σT Dp (ε˙ ; ξ) = + ε˙ p . p 2 ε˙ kk 3(σC − σT ) kk p
3.3.4.
Yield Criteria Under Special States of Stress or Deformation
Equibiaxial Stress A state of stress is called equibiaxial if two of the principal stresses are equal, as, for example, in the triaxial soil test described in Section 2.3. If σ2 = σ3 , then q q p J2 = 13 σ1 − σ3  = 2 13 τm , so that the Mises and Tresca yield criteria are formally equivalent, as are the Mohr–Coulomb criterionMohr–Coulomb and Drucker–Prager criteria.
Plane Stress
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
145
The criteria for plane stress are obtained simply by setting σ3 = 0. Thus the Tresca and Mises criteria are just as they appear in Figure 3.3.2(b) (page 138). In a state of plane stress in the x1 x2 plane with σ22 = 0 (i.e., a state of stress that may be represented as a superposition of simple tension or compression and shear), it can further be shown that both the Mises and the Tresca yield criteria can be expressed in the form
σ σY
2
+
τ τY
2
= 1,
(3.3.5)
where σ = σ11 , τ = σ12 , and σY and τY are respectively the yield stresses √ in simple tension or compression and in shear, that is, τY = k, and σY = 3k or 2k, depending on the criterion. The Mohr–Coulomb criterionMohr– Coulomb and Drucker–Prager criteria in plane stress are shown in Figure 3.3.3(b). In general, an isotropic yield criterion with σ3 = 0 may be written (with dependence on ξ not indicated explicitly) as f0 (σ1 , σ2 ) = 0, or equivalently, upon transforming the independent variables, as f1 [n, 21 (σ1 − σ2 )] = 0, def
where n = 12 (σ1 + σ2 ). Because of isotropy, the dependence of f1 on its second argument must be through the absolute value r = 12 σ1 − σ2 . The preceding equation can then be solved for r as a function of n: r = h(n).
(3.3.6)
In particular, h(n) takes the form h(n) =
q
k 2 − 31 n2
for the Mises criterion and
h(n) =
k, n < k 2k − n, n > k
for the Tresca criterion.
Plane Strain In plane strain, as defined, for example, by ε˙ 3 = 0, the situation is more complicated, since the planestrain condition requires ε˙ p3 = −˙εe3 , in turn involving the stress rates. If, however, the elastic strain rates may be equated to zero (the condition for this is discussed later), then we have
146
Chapter 3 / Constitutive Theory
ε˙ 3 = ε˙ p3 = 0. Assuming a plastic potential g(σ1 , σ2 , σ3 ), we obtain the equation ∂ g(σ1 , σ2 , σ3 ) = 0, ∂σ3 which when combined with the yield criterion in terms of the principal stresses, permits the elimination of σ3 and hence the formulation of a yield criterion in terms of σ1 and σ2 , leading once more to Equation (3.3.6). Consider, for example, the Mises criterion with its associated flow rule ˙ which requires s3 = 2 [σ3 − 1 (σ1 + σ2 )] = 0, that is, σ3 = 1 (σ1 + σ2 ). ε˙ p = λs, 3 2 2 Substituting this into the Mises yield criterion yields 34 (σ1 − σ2 )2 = 3k 2 , or σ1 − σ2  = 2k. According to the Tresca flow rule, on the other hand, for ε˙ p3 to be zero, σ3 must be the intermediate principal stress, that is, either σ1 > σ3 > σ2 or σ1 < σ3 < σ2 , so that max (σ1 − σ3 , σ2 − σ3 , σ1 − σ2 ) = σ1 − σ2  = 2k. Consequently the two criteria coincide, and may be expressed by Equation (3.3.6) with h(n) = k. Consider next the Mohr–Coulomb criterionMohr–Coulomb criterion, with a nonassociated flow rule that is governed by a plastic potential having the same form as the yield function, that is, g(σ) = σmax − σmin + (σmax + σmin ) sin ψ, where ψ is known as the angle of dilatancy, since ψ = 0 describes a plastically incompressible solid; the special case ψ = φ represents the associated flow rule. The planestrain condition ε˙ p3 = 0 again requires that σ3 be the intermediate principal stress. The criterion therefore may be described by Equation (3.3.6) with h(n) = c cos φ − n sin φ.
3.3.5.
Hardening Rules
A specification of the dependence of the yield criterion on the internal variables, along with the rate equations for these variables, is called a hardening rule. In this subsection we first review in more detail the significance of the two models of hardening — isotropic and kinematic — previously discussed for viscoplasticity in Section 3.1. Afterwards we look at some more general hardening rules.
Isotropic Hardening The yield functions that we have studied so far in this section are all reducible to the form f (σ, ξ) = F (σ) − k(ξ).
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
147
Since it is only the yield stress that is affected by the internal variables, no generality is lost if it is assumed to depend on only one internal variable, say ξ1 , and this is invariably identified with the hardening variable κ, defined as either the plastic work Wp by Equation (1.5.6) or as the effective plastic strain εp by Equation (1.5.7). The function h1 corresponding to ξ1 [see p Equation (3.1.5)] is given by σij hij or 23 hij hij , respectively, for each of the two definitions of κ, so that the workhardening modulus H is (
H=
k 0 (Wq p )σij hij ,
k 0 (εp )
2 3
hij hij .
As was pointed out in Section 3.2, workhardening in rateindependent plasticity corresponds to a local expansion of the yield surface. The present behavior model (which, as we said in Section 3.1, is called isotropic hardening) represents a global expansion, with no change in shape. Thus for a given yield criterion and flow rule, hardening behavior in any process can be predicted from the knowledge of the function k(κ), and this function may, in principle, be determined from a single test (such as a tension test). The most attractive feature of the isotropic hardening model, which was introduced by Odqvist [1933], is its simplicity. However, its usefulness in approximating real behavior is limited. In uniaxial stressing it predicts that when a certain yield stress σ has been attained as a result of workhardening, the yield stress encountered on stress reversal is just −σ, a result clearly at odds with the Bauschinger effect (Section 2.1). Furthermore, if F (σ) is an isotropic function, then the yield criterion remains isotropic even after plastic deformation has taken place, so that the model cannot describe induced anisotropy.
Kinematic Hardening In Sections 3.1 and 3.2 we saw, however, that if f can be written in the form f (σ, ξ) = F (σ − ρ) − k(ξ), (3.3.7) then more general hardening behavior can be described. Isotropic hardening is a special case of (3.3.7) if ρ ≡ 0 and if k depends only on κ, while purely kinematic hardening corresponds to constant k but nonvanishing variable ρ. Kinematic hardening represents a translation of the yield surface in stress space by shifting its reference point from the origin to ρ, and with uniaxial stressing this means that the the length of the stress interval representing the elastic region (i.e., the difference between the current yield stress and the one found on reversal) remains constant. This is in fairly good agreement with the Bauschinger effect for those materials whose stressstrain curve in the workhardening range can be approximated by a straight line (“linear hardening”), and it is for such materials that Melan [1938] proposed the
148
Chapter 3 / Constitutive Theory
model in which ρ = cεp , with c a constant. A similar idea was also proposed by Ishlinskii [1954], and a generalization of it is due to Prager [1955a, 1956a], who coined the term “kinematic hardening” on the basis of his use of a mechanical model in explaining the hardening rule (Figure 3.3.4). A kinematic H H HH HH H HH .. .. ............ .. ....H .. .. .. .. .. .. .. .. .. HH .......... .. .. .. H .. . .. . H . . ....... ...... H...H . H ..... ...... ........ ..... ...... . . . . ... H . ... ...... . . Pin . .... H...... ....... ...... .. . ........ ........ . .. . . .. . . HH ..... ............ ...... ........ H ........ ..H H . ............ . H .............. . ..H .. ... H .H ............ ...... ................. H..H ...... H ... ... .H ........ H ................. ............ H..H .. ........ ..H ..H H ........ ................... ...... ............ H . . . . . ..... H..H .... ................... ............ H..H .... ....... ..H H ................... ...... ............ H..H ...... . ..H ........ .H H ...H ................... ........ H ... ............ . . . . . . . . H.H ................. .... H... ...... ..H H ................... ... ... ..H H ................... πplane ............ ............. ..H . . H . . ............. ...... H.....H ............... .......... H H ........... .. . H
Figure 3.3.4. Prager’s mechanical model of kinematic hardening. hardening model is also capable of representing induced anisotropy, since a function F (σ − ρ) that depends only on the invariants of its argument stops being an isotropic function of the stress tensor as soon as ρ differs from zero. It should be pointed out that, since ρ is a tensor in stress space (sometimes called the back stress, as discussed in 3.1.3), the equation ρij = cεpij does not imply proportionality between the vectors representing ρ and εp in any space other than the ninedimensional space of secondrank tensors, and particularly not in the sixdimensional space in which symmetric tensors are represented, since the mappings of stress and strain into this space must be different [see Equations (1.4.9)] in order to preserve the scalar product σ · ε = σij εij ; consequently, as was pointed out by Hodge [1957a], the translation of the yield surface for a material with an associated flow rule is not necessarily in the direction of the normal to the yield surface, as was assumed by Prager in constructing his model. In more sophisticated kinematic hardening models, internal variables other than εp and κ are included; in particular, the back stress ρ may be treated as a tensorial internal variable with its own rate equation. Indeed, the Melan–Prager model falls into this category when its equation is rewritten as ρ˙ ij = c˙εpij ;
(3.3.8)
here c need not be a constant but may itself depend on other internal variables. In the model described by Backhaus [1968], for example, c depends on the effective plastic strain εp . Lehmann [1972] replaces the isotropic relation
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
149
(3.3.8) between ρ˙ and ε˙ p by a more general one, ρ˙ ij = cijkl (σ, ρ)˙εpkl . Another example of a kinematic hardening model is that due to Ziegler [1959], ρ˙ ij = µ(σ ˙ ij − ρij ), where µ˙ =
∂f σ˙ > < ∂σ kl kl
∂f /∂σmn (σmn − ρmn )
in order to satisfy the consistency condition f˙ = 0. A modification of Equation (3.3.8) that better reproduces the real Bauschinger effect consists of including in its righthand side a term representing “fading strain memory,” so that the rate equation takes the form ρ˙ ij = c˙εpij − aρij ε˙ p . The more general kinematic hardening models can be similarly modified.
Generalized Hardening Rules The hardening represented by Equation (3.3.7) with both ρ and k variable seems to have been first studied by Kadashevich and Novozhilov [1952]; it is called combined hardening by Hodge [1957a]. The combined hardening model proposed for viscoplasticity by Chaboche [1977], presented in Section 3.1, has been applied by Chaboche and his collaborators to rateindependent plasticity as well. A model with a family of back stresses ρ(l) (l = 1, 2, ..., n) is due to Mr´oz [1967]; a similar model is due to Iwan [1967]. Both models describe materials whose stressstrain curves are piecewise linear. For materials whose stressstrain curves in the workhardening range are smooth with straightline asymptotes, a class of models known as twosurface models have been proposed by Dafalias [1975] (see also Dafalias and Popov [1975]), Krieg [1975], and others. In these models the yield surface in stress space is constrained to move inside an outer surface, known variously as bounding surface, loading surface, or memory surface, given by, say, f (σ, ξ) = 0. The workhardening modulus H at a given state is assumed to be an increasing function of a suitably defined distance, in stress space, between the current stress σ and a stress σ on the outer surface, called the image stress of σ. When this distance vanishes, the workhardening modulus attains its minimum value, and further hardening proceeds linearly, with the two surfaces remaining in contact at σ = σ. The various twosurface models differ from one another in the definition of the bounding surface, in the way the image stress depends on the current
150
Chapter 3 / Constitutive Theory
state, and in the variation of workhardening modulus. In the model of Dafalias and Popov, both surfaces are given similar combinedhardening structures, with a “back stress” β playing the same role for the outer surface that ρ plays for the yield surface, and σp = c(σ − ρ) + β, where c is a constant. H is assumed to depend on δ = (σ − σ) : (σ − σ) in such a way that H = ∞ at initial yield, producing a smooth hardening curve. Experiments by Phillips and Moon [1977] showed that when yield surfaces are defined on the basis of a very small offset strain, they undergo considerable distortion, in addition to the expansion and translation considered thus far. In order to describe such distortion in initially isotropic materials, Equation (3.3.7) must be modified to f (σ, ξ) = F (σ − ρ, ξ) − k(ξ), where F is initially an isotropic function of its first argument but becomes anisotropic as plastic deformation takes place. An example of such a function is that proposed by Baltov and Sawczuk [1965] for a Misestype yield surface: 1 F (σ − ρ, ξ) = Aijkl (ξ)(σij − ρij )(σkl − ρkl ), 2 where
1 Aijkl (ξ) = δik δij − δij δkl + Aεpij εpkl , 3 A being a constant. Other proposals are reviewed by Bergander [1980]. Extensive experimental investigation of the hardening of metals were carried out by Phillips and coworkers; their work, along with that of others, is reviewed by Phillips [1986].
Exercises: Section 3.3 1. Show that the forms (3.3.1) and (3.3.2) for the Tresca yield function are equivalent. 2. Derive the associated flow rule for the Tresca yield criterion by means of Koiter’s method (see 3.2.2). 3. Show that for any combination of principal stresses, the associated flow rule for the Tresca yield criterion gives ˙εp1  + ˙εp2  + ˙εp3  = φ. 4. An elastic–perfectly plastic solid with a uniaxial yield stress of 300 MPa is assumed to obey the Tresca yield criterion and its associated flow rule. If the rate of plastic work per unit volume is 1.2 MW/m3 , find the principal plastic strainrate components when (a) σ1 = 300 MPa, σ2 = 100 MPa, σ3 = 0,
Section 3.3 / Yield Criteria, Flow Rules and Hardening Rules
151
(b) σ1 = 200 MPa, σ2 = −100 MPa, σ3 = 0, (c) σ1 = 200 MPa, σ2 = −100 MPa, σ3 = −100 MPa. 5. Derive the associated flow rule for the general isotropic yield criterion given by F (J2 , J3 ) − k 2 = 0, and in particular (a) for the one given by the equation following (3.3.4) and (b) for the analytic form of the Tresca criterion. 6. A workhardening elasticplastic solid is assumed to obey the Mises criterion with the associated flow rule and isotropic hardening. If the virgin curve in uniaxial tension can be described in the smalldeformation range by σ = F (εp ), state the rate equations (3.2.1)–(3.2.2) explicitly when k is assumed to depend (a) on εp and (b) on Wp . 7. Derive the MohrCoulomb criterion as follows. (a) Using the theory of Mohr’s circles in plane stress, in particular Equations (1.3.9)–(1.3.10), find the direction θ such that τθ − µ(−σθ ) is maximum. p
(b) Show that this maximum value is 1 + µ2 σ1 − σ2 /2 + µ(σ1 + σ2 )/2, and that the MohrCoulomb criterion results when this value is equated to the cohesion c, with µ = tan φ. (c) Show that the Mohr circles whose parameters σ1 , σ2 are governed by this criterion are bounded by the lines ±τθ = σθ tan φ − c. 8. Derive the associated flow rule and plastic dissipation for the DruckerPrager yield criterion. 9. Given the yield stresses σT and σC in uniaxial tension and compression, respectively, find the yield stress in shear resulting from the following yield criteria: (a) Mohr–Coulomb, (b) Drucker–Prager, (c) Mises– Schleicher. 10. Show that in a state of plane stress with σ11 = σ, σ12 = τ and σ22 = 0, both the Tresca and the Mises yield criteria can be expressed in the form (3.3.5). 11. Derive the form of Equation (3.3.6) for the MohrCoulomb criterion in plane stress. 12. If the function F in Equation (3.3.7) equals J¯2 , with J¯2 defined as in 3.1.1, while k is constant, and if the evolution of ρ is governed by (3.3.8), show that the rate equation of ρ is p
ρ˙ ij = (sij − ρij )
(skl − ρkl )s˙ kl . 2k 2
152
Chapter 3 / Constitutive Theory
13. Generalize the preceding result to the case where k depends on εp , obtaining rate equations for both ρ and εp .
Section 3.4 3.4.1.
Uniqueness and Extremum Theorems
Uniqueness Theorems
Uniqueness Theorems in Elastic Bodies Consider a body made of a linearly elastic material with no internal constraints, occupying a region R and subject to prescribed tractions ta on ∂Rt , prescribed displacements ua on ∂Ru , and a prescribed bodyforce field b in R. For convenience, the body force per unit volume is defined as f = ρb. We suppose that a stress field σ and a displacement field u in R have been found such that σij = Cijkl εkl (where ε is the strain field derived from u) and σij ,j +fi = 0 in R, nj σij = tai on ∂Rt , and u = ua on ∂Ru . In other words, (σ, u) constitutes a solution of the static boundaryvalue problem. Is this solution unique? As a result of the classical uniqueness theorem due to Kirchhoff, the answer is “yes” as regards the stress field and “almost” as regards the displacement field. For, if (σ (1) , u(1) ) and (σ (2) , u(2) ) are two different solutions, and if we write φ = φ(1) − φ(2) for any φ, then σ ij = Cijkl εkl , σ ij ,j = 0 in R, and nj σ ij u ¯i = 0 on ∂R. Consequently, by the divergence theorem, Z
0=
(σ ij u ¯i ),j dV ZR
=
(σ ij ,j u ¯i + σ ij u ¯i ,j ) dV ZR
=
σ ij εij dV ZR
= R
Cijkl εij εkl dV.
It follows from the positivedefiniteness of C (see 1.4.3) that ε must vanish ¯ may have at throughout R. Consequently, σ must vanish as well, while u most the form of a rigidbody displacement; full uniqueness of the displacement field depends on having sufficient external constraints. If the material were nonlinearly elastic, the same method could be applied, but incrementally. Suppose that the stress field σ and displacement field u have been found under the current f , ta and ua . We may then prove the uniqueness of infinitesimal increments dσ resulting from increments df , dta and dua , provided that C is interpreted as the tangent elastic modulus
Section 3.4 / Uniqueness and Extremum Theorems
153
tensor as defined by Equation (1.4.8), so that dσij = Cijkl dεkl . Incremental uniqueness implies global uniqueness, since any state of loading can be attained by the successive imposition of small incremental loads. Consequently, the stress and strain fields are uniquely determined (and the displacement field determined to within a rigidbody displacement) so long as C is positive definite.
Uniqueness of Stress Field in an Elastic–Plastic Body The positivedefiniteness of C means that, for an elastic material, dσij dεij > 0 whenever dσ 6= 0. The last inequality is equivalent to Drucker’s first inequality for a workhardening plastic material (see Section 3.2). Indeed, we know that as long as no unloading occurs, no distinction can be made between plastic and nonlinearly elastic materials. It was shown by Melan [1938] that incremental uniqueness of stress and strain can be established for workhardening standard materials when unloading has taken place, provided that the hypothesis of infinitesimal strains is valid. The reason for the proviso is that, with finite deformations, a distinction must be made between increments at a fixed material point and those at a fixed point in space (see Hill [1950] and Chapter 8 of the present book). By analogy with the proof for elastic bodies, it can be shown that a sufficient condition for the uniqueness of the stress field in a plastic body is that if dσ (1) and dσ (2) are two possible incremental stress fields and dε(1) and dε(2) are the associated incremental strain fields, then (1)
(2)
(1)
(2)
(dσij − dσij )(dεij − dεij ) > 0
(3.4.1)
unless dσ (1) = dσ (2) . It was shown by Valanis [1985] that condition (3.4.1) applies in dynamic as well as in quasistatic problems. Consider next an elasticplastic body made of standard material, occupying the region R. Let Re and Rp denote the parts of R where f < 0 and f = 0, respectively. With linear elasticity assumed, the inequality is clearly satisfied in Re , while in Rp we may use the general flow equation (3.2.1) together with (3.2.2) and the normality rule (3.2.7). Converting rates into increments by multiplying them by the infinitesimal time increment dt, we obtain, at any point in Rp , (α)
(α)
−1 dεij = Cijkl dσkl +
∂f , H ∂σij
where df (α) =
∂f (α) dσ . ∂σkl kl
α = 1, 2,
(3.4.2)
154
Chapter 3 / Constitutive Theory
Hence (1)
(2)
(1)
(2)
(1)
(2)
(1)
(2)
−1 (dσij − dσij )(dεij − dεij ) = Cijkl (dσij − dσij )(dσkl − dσkl ) 1 + (df (1) − df (2) )( − ). H
It is easy to see that any two real numbers a, b satisfy − = β(a − b) for some β, 0 ≤ β ≤ 1, and that therefore the second term on the righthand side is never negative. Since the first term is positive unless dσ (1) = dσ (2) , the uniqueness of dσ (and therefore of dε) is proved, and hence the uniqueness of the stress and strain fields under a given history of f , ta , and ua . If the material is perfectly plastic, then Equation (3.4.2) for the strain increments at points where f = 0 must be replaced by (α)
(α)
−1 dεij = Cijkl dσkl + dλ(α)
∂f , ∂σij
α = 1, 2,
(3.4.3)
where dλ(α) = 0 if df (α) < 0, and dλ(α) > 0 only if df (α) = 0 but is otherwise undetermined. Thus (1)
(2)
(1)
(2)
(1)
(2)
(1)
(2)
−1 (dσij − dσij )(dεij − dεij ) = Cijkl (dσij − dσij )(dσkl − dσkl )
+(dλ(1) − dλ(2) )(df (1) − df (2) ). The second term evidently vanishes either if both df (1) and df (2) vanish, or if both are negative (leading to dλ(1) = dλ(2) = 0). If df (1) = 0 and df (2) < 0, then the term equals −dλ(1) df (2) and is positive, as it is when (1) and (2) are interchanged. The uniqueness of dσ — and hence that of the stress field — follows, but not that of dε. If normality is not obeyed, then workhardening (i.e. the positiveness of H) is not sufficient for uniqueness. The corresponding sufficient condition is, instead, H > Hcr , where Hcr is a critical value of the hardening modulus given by Raniecki [1979] as Hcr
1 = 2
s
∂f ∂f q ∂f Cijkl Cijkl hij hkl − Cijkl hij ∂σij ∂σkl ∂σkl
!
.
Clearly, Hcr = 0 when the normality rule (3.2.7) is obeyed.
3.4.2.
Extremum and Variational Principles
In Section 1.4 we derived the two fundamental variational principles of elastostatics, which form a dual pair. The principle of minimum potential energy
Section 3.4 / Uniqueness and Extremum Theorems
155
teaches that in a body in stable equilibrium the correct displacement field — that is, the one that, with its associated stress field, forms the solution of the boundaryvalue problem — is the one which, among all the kinematically admissible displacement fields that are close to it, minimizes the total potential energy Π. Similarly, the principle of minimum complementary energy asserts that the correct stress field is the one which, among all the neighboring stress fields that are statically admissible, minimizes the total complementary energy Πc . If the material is linear, then unless large displacements come into play, the respective energies depend at most quadratically on their variables, and it is easy to see that the restriction to admissible fields that are close to the correct one may be removed. Indeed, it can be shown directly that, if Π∗ is the total potential energy evaluated at the arbitrary kinematically admissible displacement field u∗ , and if Π = Π∗ u∗ =u , where u is the correct displacement field, then Π∗ > Π
unless u∗ = u.
For 1 Π −Π = 2 ∗
Z R
Cijkl (ε∗ij ε∗kl −εij εkl ) dV
−
Z R
fi (u∗i −ui ) dV
−
Z ∂Rt
tai (u∗i −ui ) dS;
but the surface integral may be changed into one over all of ∂R, since u∗ = u on ∂Ru , and consequently, by the divergence theorem, into Z R
[σij ,j (u∗i − ui ) + σij (ε∗ij − εij )] dV,
∗ = C ∗ where σij = Cijkl εkl is the correct stress field. If we define σij ijkl εkl then with the help of the equilibrium equations, we obtain
1 2
Π∗ − Π =
Z R
∗ ∗ (σij εij + σij εij − 2σij ε∗ij ) dV.
The integrand, however, is Cijkl (εij εkl + ε∗ij ε∗kl − 2ε∗ij εkl ) = Cijkl (ε∗ij − εij )(ε∗kl − εkl ), and is positive except when ε∗ = ε. Similarly, Πc∗ − Πc =
1 2
Z R
−1 ∗ ∗ Cijkl (σij σkl − σij σkl ) −
Z ∂Ru
∗ nj (σij − σij )uai dS,
and with the help of analogous transformations, we obtain Πc∗ − Πc =
1 2
Z R
−1 ∗ ∗ ∗ Cijkl [σij σkl − σij σkl − 2(σij − σij )εij ] dV,
156
Chapter 3 / Constitutive Theory
−1 where εij = Cijkl σkl , so that the integrand is −1 ∗ ∗ Cijkl (σij − σij )(σkl − σkl ),
also positive except when σ ∗ = σ. In view of the resemblance between the uniqueness proof and the proofs of the extremum principles, it appears reasonable that such principles may be derived for displacement and stress increments (or, equivalently, velocities and stress rates) in elasticplastic bodies that are either workhardening or perfectly plastic. Such is indeed the case. The theorems to be presented have been derived by Handelman [1944], Markov [1947], Greenberg [1949], and Hill [1950];1 the proofs are Hill’s.
Extremum Principle for Displacement Let du∗ denote a kinematically admissible displacement increment, that is, one which obeys the internal constraints, if any, and which satisfies du∗ = dua on ∂Ru . The corresponding incremental strain and stress field are dε∗ and dσ ∗ , where dσ ∗ is not in general statically admissible, but is related to dε∗ through the associated flow rule; we thus use Equation (3.2.10) with hij = ∂f /∂σij , to obtain Hill’s [1958] result
σ˙ ij =
Cijkl ε˙ kl , Cijkl
f < 0,
ε˙ kl −
1 ∂f ∂f L ∂σpq ∂σkl
!
, f = 0.
Here L is given by Equation (3.2.9) for a standard material, namely, L = H + Cijkl
∂f ∂f , ∂σij ∂σkl
and the perfectly plastic case corresponds to H = 0. Let the functional Λ∗ be defined by Λ∗ =
1 2
Z R
∗ dσij dε∗ij dV −
Z R
dfi du∗i dV −
Z ∂Rt
dtai du∗i dS,
with Λ = Λ∗ du∗ =du . Note that the form of Λ is essentially that of the potential energy Π of the linear elastic body, with incremental rather than total displacements and with the total (elasticplastic) tangent modulus tensor in place of C. By 1
Some extensions have been proposed by, among others, Ceradini [1966], Maier [1969, 1970] and Martin [1975].
Section 3.4 / Uniqueness and Extremum Theorems
157
means of the transformations used in the elastic case, we can therefore show that Z 1 ∗ Λ∗ − Λ = (dσij dε∗ij + dσij dεij − 2dσij dε∗ij ) dV, 2 R and it remains to be shown that the integrand is positive unless dσ ∗ = dσ. With the decomposition dε = C−1 dσ + dεp , the integrand becomes p∗ −1 ∗ ∗ ∗ Cijkl (dσij − dσij )(dσkl − dσkl ) + dσij dεp∗ ij + dσij dεij − 2dσij dεij .
The term in C−1 is clearly nonnegative, and vanishes only if dσ ∗ = dσ. As for the remaining terms, in the case of a workhardening material their sum becomes φ=
1 (df ∗ + df − 2df ), H
∗ . Clearly, φ vanishes where df = (∂f /∂σij ) dσij and df ∗ = (∂f /∂σij ) dσij if df ∗ and df are both nonpositive, and equals H −1 (df ∗ − df )2 if both are positive. If df ∗ > 0 and df ≤ 0, φ = H −1 df ∗ (df ∗ − 2df ) > 0, while in the opposite case φ = H −1 (df )2 . For the perfectly plastic material, we replace H −1 by dλ, with dλ related to df as in the uniqueness proof, and similarly H −1 by dλ∗ , so that
φ = df ∗ dλ∗ + df dλ − 2df dλ∗ . The first two terms always vanish, as does the last term except when df < 0 and df ∗ = 0, in which case dλ∗ > 0, so that φ = −2df dλ∗ > 0. Consequently φ is never negative, so that Λ∗ > Λ (3.4.4) except when dσ ∗ = dσ. For the workhardening (but not the perfectly plastic) material this also means that dε∗ = dε and therefore du∗ = du if sufficient constraints exist.
Extremum Principle for Stress The complementary extremum principle concerns a statically admissible incremental stress field dσ ∗ . In the case of a workhardening material this determines an incremental strain field dε∗ , related to dσ ∗ through the associated flow rule — Equation (3.4.2) with the superscript (α) replaced by ∗ — but not, in general, derivable from a continuous displacement field. Clearly, 1 −1 ∗ ∗ ∗ dσij dε∗ij = Cijkl dσij dσkl + 2 . H −1 ∗ + If the material is perfectly plastic, on the other hand, then dε∗ij = Cijkl dσkl p∗ p∗ ∗ ∗ dεp∗ ij , with dε not determined by dσ . However, in such a material dσij dεij = 0, and therefore −1 ∗ ∗ ∗ dσij dε∗ij = Cijkl dσij dσkl .
158
Chapter 3 / Constitutive Theory We now define the functional 1 Ω = 2 ∗
Z R
∗ dσij
dε∗ij
dV −
Z ∂Ru
∗ nj dσij duai dS,
∗ dε∗ defined by the appropriate formula above. We also define, as with dσij ij before, Ω = Ω∗ dσ∗ =dσ .
Note that the form of Ω is, mutatis mutandis, that of Πc , and also that Ω = −Λ. The surface integral in Ω∗ is transformed into Z R
∗ dσij dεij dV,
and therefore Ω∗ − Ω =
1 2
Z R
∗ ∗ (dσij dε∗ij + dσij dεij − 2dσij dεij ) dV.
The integrand differs from the one in Λ∗ − Λ only in the interchange of starred and unstarred quantities, and may by the same method be shown to be nonnegative and to vanish only if dσ ∗ = dσ, so that Ω∗ > Ω
unless dσ ∗ = dσ.
(3.4.5)
We furthermore have the double inclusion −Λ∗ ≤ −Λ = Ω ≤ Ω∗ .
Variational Principles As mentioned earlier, an extremum principle is stronger than a variational principle because it asserts an extremum over all admissible functions of a certain class, not only over those that are infinitesimally close to the extremal. Going further, we see that a variational principle need not assert an extremum at all, even a local one, but only the condition that the functional obeying it is stationary. For example, the function f (x) = x3 is stationary at x = 0, since f 0 (0) = 0, but has neither a minimum nor a maximum there. Likewise, f (x, y) = x2 − y 2 is stationary at (0, 0); the point is a saddle point — a maximum when viewed along the xaxis and a minimum along the yaxis. Extremum principles are useful for many reasons, one of them being that they allow us to evaluate approximate solutions when the exact solution is unknown: between two incremental displacement fields du∗ , in the absence
Section 3.4 / Uniqueness and Extremum Theorems
159
of other information we choose the one that produces the smaller value of Λ∗ . But variational principles are useful even when they are not extremum principles: they permit compact statements of boundaryvalue problems, and they are useful in formulating the “weak form” of such problems, which is necessary for consistent discretization, as shown in 1.3.5 and as further shown in Section 4.5 which deals with numerical methods. The extremum principles derived above clearly imply the corresponding variational principles: δΛ = 0, δΩ = 0. We should remember, however, that the extremum principles rely on the positivedefiniteness of certain local quantities, whose proof requires that the material be nonsoftening. Consider, on the other hand, the following functional: Θ=
1 2
Z R
Cijkl ε˙ ij ε˙ kl dV − −
Z
1 2
Z
b˙ i u˙ i dV −
R
Rp
1 ∂f 2 dV L ∂σkl
Z ∂Rt
t˙ai u˙ i dV.
It is easy to see that Θ is just Λ with rates in place of increments; the change is made to avoid mixing the differential operator d with the variation operator δ. Clearly, with σ˙ given in terms of ε˙ by the strainspace flow rule, Z
δΘ = R
σ˙ ij δ ε˙ ij dV −
Z
b˙ i δ u˙ i dV −
R
Z ∂Rt
t˙ai δ u˙ i dV,
and δΘ = 0 for an arbitrary kinematically admissible δ u˙ only if σ˙ is statically admissible.
3.4.3.
Rigid–Plastic Materials
In discussing the SaintVenant–L´evy–Mises flow rule in the preceding section, we mentioned in passing that these authors equated ε˙ with ε˙ p , in effect neglecting the elastic strain rate — a treatment tantamount to treating the nonvanishing elastic moduli as infinite. Any solutions obtained on this basis are, theoretically, valid for idealized materials called rigidplastic.1 Practically, however, they are useful approximations for two classes, not mutually exclusive, of problems: (a) those in which the elastic strain rates may be neglected, and (b) those in which the elastic strains are significantly smaller than the plastic ones. Problems of class (a) include those of impending collapse or incipient plastic flow of elastic–perfectly plastic bodies, for which it 1
In many references, the theory of rigidplastic materials obeying the Mises yield criterion and the associated flow rule is called the Mises theory, while the corresponding theory of elasticplastic materials is called the Prandtl–Reuss theory.
160
Chapter 3 / Constitutive Theory
is shown later in this section that, when deformation proceeds at constant loads, the elastic strain rates vanish identically. In order to accommodate problems of class (b), the hypothesis of infinitesimal deformations should be abandoned in formulating any general theorems for this theory. Since the problems are frequently those of flow, it appears natural to use an Eulerian formulation, in which R is the region currently occupied by the body and σ is the true (Cauchy) stress tensor. No reference configuration is used in this approach, and therefore no displacement field u appears; in its place we have the velocity field v. The boundary ∂R is accordingly partitioned into ∂Rt and ∂Rv , with v = va on ∂Rv . No strain tensor is introduced, but rather the Eulerian deformationrate tensor (also called stretching tensor ) d, defined by dij = 21 (vi ,j +vj ,i ). ˙ With infinitesimal deformations, of course, d approximates ε.
Uniqueness of Stress Field In general plasticity theory, the decomposition of the deformation rate into elastic and plastic parts is far from unequivocal, as is shown in Chapter 8. In a rigidplastic material, however, d may be identified with the plastic strain rate, and thus the plastic dissipation per unit volume, Dp , defined in Section 3.2, satisfies Dp (d) = σij dij . (3.4.6) The maximumplasticdissipation principle may therefore be written ∗ (σij − σij )dij ≥ 0.
(3.4.7)
If d 6= 0, then the equality holds only if σ and σ ∗ are plastically equivalent, that is, if d is related to both of them through the associated flow rule. In a Mises material, plastically equivalent stresses differ at most by a hydrostatic pressure, but in a Tresca material two stresses are plastically equivalent if they lie on the same facet of the hexagonal cylinder in principalstress space. If, now, (σ (α) , v(α) ), α = 1, 2, represent two admissible states of a rigidplastic body, corresponding to the same body force and boundary conditions, then (1) (2) (1) (2) nj (σij − σij )(vi − vi ) = 0 on ∂R, and therefore Z ∂R
(1) nj (σij
−
(2) (1) σij )(vi
−
(2) vi ) dS
Z
= R
(1)
(2)
But the last integrand may be written as (1)
(2)
(1)
(1)
(2)
(σij − σij )(dij − dij ) dV = 0.
(2)
(1)
(2)
(σij − σij )dij + (σij − σij )dij ,
Section 3.4 / Uniqueness and Extremum Theorems
161
and this is positive unless either d(1) and d(2) both vanish, or σ (1) and σ (2) are plastically equivalent. The general conclusion is thus that two admissible stress fields σ (1) and σ (2) must be plastically equivalent everywhere except in their common rigid region, that is, at points where f (σ (α) ) < 0, α = 1, 2. If the body is made of a Mises material (or any other material whose yield surface in stressdeviator space is strictly convex) and deforms plastically in its entirety, then the two stress fields can differ at most by a hydrostatic pressure field, which must be uniform in order to satisfy equilibrium, and must vanish if a surface traction is prescribed anywhere on ∂R. Thus there is not more than one admissible stress field for which the whole body is plastic (Hill [1948a]), unless ∂R = ∂Rv , in which case the stress field is determined only to within a uniform hydrostatic pressure. On the other hand, uniqueness of the velocity field is not established.
Extremum Principle for Velocity The degree to which the velocity field is determined may be learned from the kinematic extremum principle to be shown next, first proposed by Markov [1947] for a Mises material. Given a kinematically admissible velocity field v∗ , we define a functional Γ∗ by Γ∗ =
Z
Dp (d∗ ) dV −
Z R
R
fi vi∗ dV −
Z ∂Rt
tai vi∗ dS,
and, as usual, Γ = Γ∗ v∗ =v . Using the standard transformations we can show that Z
Γ= ∂Rv
and that Γ∗ − Γ =
Z R
nj σij via dS
(3.4.8)
[Dp (d∗ ) − Dp (d) − σij (d∗ij − dij )] dV.
Because of (3.4.6), the integrand is just Dp (d∗ ) − σij d∗ij , and this is nonnegative as a result of the maximumplasticdissipation principle, Equation (3.4.7), since the actual stress σ necessarily obeys the yield criterion. Consequently, Γ∗ ≥ Γ. (3.4.9) It is not possible, in general, to strengthen the inequality by asserting that the equality holds only when v∗ = v. The most we can say is that if Γ∗ = Γ, then v∗ is kinematically admissible, and d∗ is associated with a stress field σ ∗ that is statically admissible and obeys the yield criterion everywhere. More particularly, however, if the body is one for which the stress field is unique (see above) and if the stress determines the deformation rate to within a scale factor (as is true of the Mises material, or any other material with a
162
Chapter 3 / Constitutive Theory
smooth yield surface), then the entire deformationrate field is determined to within a scale factor. The indeterminacy may be eliminated if a nonzero velocity is prescribed anywhere on ∂Rv .
Principle of Maximum Plastic Work Given a statically admissible stress field σ ∗ which nowhere violates the yield criterion, then, if σ and v are the actual stress and velocity fields, respectively, we clearly have Z R
(σij −
∗ σij )dij
Z
dV = ∂Rv
∗ nj (σij − σij )via dS.
From the principle of maximum plastic dissipation there immediately follows the result Z Z ∗ a nj σij via dS ≥ nj σij vi dS, ∂Rv
∂Rv
due to Hill [1948a] and dubbed by him the principle of maximum plastic work. Here, again, the equality holds only if σ ∗ and σ are plastically equivalent, and therefore only if σ ∗ = σ whenever σ is unique. Note that the lefthand side of the inequality is equal to Γ, Equation (3.4.8), and is therefore bounded both above and below. Many results relating to variational principles in both elasticplastic and rigidplastic solids are contained in Washizu [1975].
Exercises: Section 3.4 1. Show that for any two real numbers a, b, − = β(a − b) for some β, 0 ≤ β ≤ 1. 2. Show that the Hu–Washizu principle (Exercise 14 of Section 1.4) may be extended to elasticplastic materials if W (ε) is replaced by W (ε − εp ). 3. Derive Equation (3.4.8) and the one following it.
Section 3.5 3.5.1.
LimitAnalysis and Shakedown Theorems
Standard LimitAnalysis Theorems
The extremum principles for standard rigidplastic materials that were discussed in the preceding section can be reformulated as the theorems of
Section 3.5 / LimitAnalysis and Shakedown Theorems
163
limit analysis, which give upper and lower bounds on the loads under which a body that may be approximately modeled as elastic–perfectly plastic reaches a critical state. By a critical state we mean one in which large increases in plastic deformation — considerably greater than the elastic deformation — become possible with little if any increase in load. In the case of perfectly plastic bodies this state is called unrestricted plastic flow ,1 and the loading state at which it becomes possible is called ultimate or limit loading. It will be shown that, in a state of unrestricted plastic flow, elasticity may be ignored, and therefore a theory based on rigidplastic behavior is valid for elasticplastic bodies. The proof of the limitanalysis theorems is based on the principle of maximum plastic dissipation, and consequently they are valid only for standard materials; a limited extension to nonstandard materials is discussed in 3.5.2. It should be noted that the “loads” in the present context include not only the prescribed surface tractions ta but all the surface tractions t operating at points at which the displacement (or velocity) is not constrained to be zero. In other words, the loads include reactions that do work ; the definition of ∂Rt is accordingly extended. The reason for the extension is that the velocity fields used in the limitanalysis theorems are kinematically admissible velocity fields, not virtual velocity fields. The latter is, as we recall, the difference between two kinematically admissible velocity fields, and must therefore vanish wherever the velocity is prescribed, whereas a kinematically admissible velocity field takes on the values of the prescribed velocity. We begin by defining a state of impending plastic collapse or incipient plastic flow as one in which a nonvanishing strain rate (ε˙ 6= 0) occurs under constant loads (f˙ = 0, t˙ = 0). The qualification “impending” or “incipient” is important: we are looking at the very beginning of such a state, which means that (1) all prior deformation has been of the same order of magnitude as elastic deformation, so that changes of geometry can be neglected, and (2) acceleration can be neglected and the problem can be treated as quasistatic.
Vanishing of Elastic Strain Rates In addition to the preceding assumptions, it is assumed that the equations of equilibrium and the traction boundary conditions can be differentiated with respect to time with no change in form; consequently, the principle ˙ f˙ , and t˙ replacing σ, f , and t. For a virtual of virtual work is valid with σ, 1
A rigorous formulation of the theorems in the context of convex analysis is due to Fr´emond and Friaˆ a [1982], who show that the concept of unrestricted plastic flow is too general for materials whose elastic range is unbounded in the appropriate stress space, and must be replaced by the weaker concept of “almost unrestricted” plastic flow (´ecoulement presque libre).
164
Chapter 3 / Constitutive Theory
displacement field we take v δt, where v is the actual velocity field and δt is a small time increment. The virtual strain field is, accordingly, ε˙ ij δt, where ε˙ ij = 12 (vi ,j +vj ,i ). At impending collapse, then, Z
0=
f˙ · v dV +
R
Z
t˙ · v dS =
∂Rt
Z
Z
σ˙ ij ε˙ ij dV = R
R
−1 σ˙ ij (˙εpij + Cijkl σ˙ kl ) dV.
The positive definiteness of the elastic complementary energy implies −1 Cijkl σ˙ ij σ˙ kl ≥ 0 unless σ˙ = 0. This fact, combined with Drucker’s inequality (3.2.3), implies that at impending collapse or incipient plastic flow the stress rates vanish, so that ε˙ e = 0 and ε˙ = ε˙ p . In other words, a body experiencing plastic collapse or flow behaves as though it were rigidplastic rather than elasticplastic. This result, first noted by Drucker, Greenberg, and Prager [1951], makes possible the rigorous application to elasticplastic bodies of the theorems of limit analysis that had previously been formulated for rigidplastic bodies. The following presentation of the theorems follows Drucker, Greenberg and Prager.1
LowerBound Theorem Suppose that at collapse the actual loads are f , t and the actual stress, ˙ Suppose velocity and strainrate fields (in general unknown) are σ, v and ε. further that we have somehow determined a stress field σ ∗ which does not violate the yield criterion anywhere and which is in equilibrium with the loads f ∗ = (1/s)f , t∗ = (1/s)t, where s is a numerical factor. By virtual work, we have Z
∗ σij ε˙ ij dV
R
1 f · v dV t · v dS + s ∂R R Z Z 1 1 ˙ dV. σij ε˙ ij dV = Dp (ε) s R s R Z
= =
Z
∗ε ˙ ≥ σij But, by the principle of maximum plastic dissipation, Dp (ε) ˙ ij , so that s ≥ 1. In other words, the factor s (the socalled “static multiplier”) is in fact a safety factor.
UpperBound Theorem Let us suppose next that instead of σ ∗ , we somehow determine a velocity field v∗ (a collapse mechanism), with the corresponding strainrate field ε˙ ∗ , and loads f ∗ = cf , t∗ = ct that satisfy Z ∂Rt 1
t∗ · v∗ dS +
Z R
f ∗ · v∗ dV =
Z
Dp (ε˙ ∗ ) dV,
R
See also Drucker, Prager and Greenberg [1952], Hill [1951, 1952], and Lee [1952].
Section 3.5 / LimitAnalysis and Shakedown Theorems
165
provided the righthand side (the total plastic dissipation) is positive;2 then, again by virtual work, Z
Dp (ε˙ ∗ ) dV = c
R
Z R
σij ε˙ ∗ij dV,
where σ is, as before, the actual stress field at collapse. The principle of maximum plastic dissipation, however, also implies that Dp (ε˙ ∗ ) ≥ σij ε˙ ∗ij . Consequently c ≥ 1, that is, c (the “kinematic multiplier”) is an overload factor.
Alternative Formulation for OneParameter Loading Rather than using multipliers, the theorems can also be expressed in terms of a single reference load to which all the loads on the body are proportional. Let this reference load be denoted P , and let the loading (consisting of applied loads and working reactions) be expressed as f = P ˜f ,
t = P ˜t,
where ˜f and ˜t are known functions of position in R and on ∂Rt , respectively. Let, further, PU denote the value of P at collapse. If a plastically admissible stress field σ ∗ is in equilibrium with P ˜f and P ˜t for some value of P , say PLB ∗ , then this value is a lower bound, that is, PLB ∗ ≤ PU . An upper bound PU B ∗ can be found explicitly for a kinematically admissible velocity field v∗ : ˙ ∗ )dV R Dp (ε . PU ≤ PU B = R R ˜ ∗ ˜ ∗ R f · v dV + ∂Rt t · v dS ∗
R
(3.5.1)
For loading governed by a single parameter, therefore, the two theorems may also be expressed as follows: The loads that are in equilibrium with a stress field that nowhere violates the yield criterion do not exceed the collapse loads, while the loads that do positive work on a kinematically admissible velocity field at a rate equal to the total plastic dissipation are at least equal to the collapse loads. If the loads produced by the application of the two theorems are equal to each other, then they equal the collapse loads. In particular, if one has succeeded in finding both (a) a statically and plastically admissible stress field, and (b) a kinematically admissible velocity field such that the strain rate produced by it is everywhere1 associated to the stress, then a complete solution is said to have been found. This solution is not necessarily unique and hence cannot be called an exact solution, but, as a result of the theorems of limit analysis, it predicts the correct collapse load. Some applications of this concept are given in Chapter 5. In Chapter 2 If the total plastic dissipation is negative, v∗ can be replaced by −v∗ ; if it is zero, v∗ does not represent a collapse mechanism. 1 If the velocity field involves regions that move as rigid bodies (rigid regions), then the strain rate there is of course zero and the question of association does not arise.
166
Chapter 3 / Constitutive Theory
6 the theorems are used to obtain estimates of collapse loads in problems for which no complete solutions have been found.
Multiparameter Loadings We now consider loadings that are governed by several parameters that can vary independently. These parameters will be called generalized loads; some of them may be applied loads, and others may be reactions that do work. Let them be denoted PI (I = 1, ..., N ), so that f=
N X
PI ˜f (I) ,
t=
I=1
N X
PI ˜t(I) ,
I=1
the ˜f (I) and ˜t(I) again being known functions. For a kinematically admissible velocity field v, generalized velocities p˙I can be defined by Z
p˙I =
˜f (I) · vdR +
R
Z
˜t(I) · vdS,
∂Rt
so that, by virtual work, Z
σij ε˙ ij dV = R
N X
def
˙ PI p˙I = P · p,
(3.5.2)
I=1
where P and p˙ are the N dimensional vectors representing the PI and p˙I . Any combination of generalized loads PI thus represents a point in Pspace (a load point), while a fixed proportion among the PI represents a direction in this space (a loading direction). A combination of PI at which unrestricted plastic flow occurs represents a limit point (or flow point or yield point — the last designation makes sense only in terms of a rigidplastic material), and the set of all such points is the limit locus (or flow locus or yield locus), given by, say, Φ(P) = 0. It follows from Equation (3.5.2) and the principle of maximum plastic dissipation that if P and P∗ are on or inside the limit locus, and if p˙ is a generalized velocity vector that is possible under a load vector P, then (P − P∗ ) · p˙ ≥ 0.
(3.5.3)
By arguments identical with those of 3.2.2 for the maximumplasticdissipation principle in terms of stresses and strain rates, it follows from inequality (3.5.3) that the limit locus is convex, and that the generalized velocity vector is normal to the limit locus, that is, ∂Φ p˙I = λ˙ ∂PI
Section 3.5 / LimitAnalysis and Shakedown Theorems
167
wherever Φ(P) is regular. The appropriate generalization, following either the Koiter or the Moreau formalism, may be formed for singular limit loci. A fixed loading direction is described by N − 1 parameters, and keeping these constant is equivalent to oneparameter loading. Consequently, along any direction lowerbound and upperbound load points can be found, and since they depend on the N − 1 parameters, they form parametric representations of upperbound and lowerbound loci. A simple illustration of multiparameter loading is provided by an “ideal sandwich beam,” composed of two equal, very thin flanges of crosssectional area A, separated by a distance h that is spanned by a web of negligible area [see Figure 3.5.1(a)]. The beam is subject to an axial force P , whose line of M/MU 1
@ @
SS o
6 h
A
@
1
@ @ @
/
?
P/PU
(a) (b)
Figure 3.5.1. Ideal sandwich beam: (a) crosssection; (b) flow locus. action is defined as midway between the flanges, and a bending moment M ; P and M may be treated as generalized loads, and the conjugate generalized ˙ and the rotation velocities are respectively the average elongation rate ∆ ˙ The stresses in the flanges may be assumed to be purely axial, and rate θ. equilibrium requires that they be σ=
P M ± . 2A Ah
If the yield stress is σY , then the yield inequality σ ≤ σY in each flange is equivalent to P M ± ≤ 1, P MU U where PU = 2σY A, MU = σY Ah. The limit locus, shown in Figure 3.5.1(b), is thus given by P M P M Φ(M, P ) = max + , − − 1 = 0. PU M U PU MU
Since this locus was found on the basis of a stress distribution, it is strictly speaking a lowerbound locus. The stress distribution is, of course, unique, and therefore the lower bound must in fact give the true limit locus.
168
Chapter 3 / Constitutive Theory
It can easily be shown that the same limit locus results from an application of the upperbound theorem. Consider a velocity field in which only one of the flanges elongates while the other remains rigid. In order for the mean ˙ that of the deforming flange must be elongation rate of the beam to be ∆, ˙ ˙ 2∆, and the rotation rate, to within a sign, is θ˙ = 2∆/h. For the sake ˙ ˙ of definiteness, let us take both ∆ and θ as positive. The strain rate in ˙ the deforming flange is 2∆/L, so that the total plastic dissipation — the ˙ ˙ numerator on the righthand side of (3.5.1) — is σY (2∆/L)(AL) = PU ∆. We take P as the reference load, and pick a loading direction by letting M = ˙ + (αh/2)(2∆/h) ˙ ˙ αP h/2. The denominator in (3.5.1) is thus ∆ = (1 + α)∆, and the upper bound for P is PU /(1 + α). Since MU = PU h/2, the upper bound for M is αMU /(1 + α). The upperbound values satisfy M/MU + P/PU = 1, an equation describing the first quadrant of the previously found ˙ limit locus. The remaining quadrants are found by varying the signs of ∆ ˙ and θ. A velocity field with both flanges deforming leads to an upperbound load point lying outside the limit locus just found, with two exceptions: one where the elongation rates of the flanges are the same, and one where they are equal and opposite. Details are left to an exercise.
3.5.2.
Nonstandard LimitAnalysis Theorems
The theorems of limit analysis can be stated in a form that does not directly refer to any concepts from plasticity theory: A body will not collapse under a given loading if a possible stress field can be found that is in equilibrium with a loading greater than the given loading. A body will collapse under a given loading if a velocity field obeying the constraints (or a mechanism) can be found that so that the internal dissipation is less than the rate of work of the given loading. In this form, the theorems appear intuitively obvious. In fact, the concepts underlying the theorems were used long before the development of plasticity theory. Use of what is essentially the upperbound theorem goes back to the eighteenth century: it was used in 1741 by a group of Italian mathematicians to design a reinforcement method for the crumbling dome of Saint Peter’s Church, and in 1773 by Coulomb to investigate the collapse strength of soil. The latter problem was also studied by Rankine in the midnineteenth century by means of a technique equivalent to the lowerbound theorem. The simple form of the theorems given above hides the fact that the postulate of maximum plastic dissipation (and therefore the normality of the flow rule) is an essential ingredient of the proof. It was therefore necessary to find a counterexample showing that the theorems are not universally applicable to nonstandard materials. One such counterexample, in which
Section 3.5 / LimitAnalysis and Shakedown Theorems
169
plasticity is combined with Coulomb friction at an interface, was presented by Drucker [1954a]. Another was shown by Salen¸con [1973].
Radenkovic’s Theorems A theory of limit analysis for nonstandard materials, with a view toward its application to soils, was formulated by Radenkovic [1961, 1962], with modifications by Josselin de Jong [1965, 1974], Palmer [1966], Sacchi and Save [1968], Collins [1969], and Salen¸con [1972, 1977]. Radenkovic’s first theorem may be stated simply as follows: The limit loading for a body made of a nonstandard material is bounded from above by the limit loading for the standard material obeying the same yield criterion. The proof is straightforward. Let v∗ denote any kinematically admissible velocity field, and P∗ the upperbound load point obtained for the standard material on the basis of this velocity field. If σ is the actual stress field at collapse in the real material, then, since this stress field is also statically and plastically admissible in the standard material, Dp (ε˙ ∗ ) ≥ σij ε˙ ij ∗ , and therefore, by virtual work, P∗ · p˙ ∗ ≥ P · p˙ ∗ . Since v∗ may, as a special case, coincide with the correct collapse velocity field in the fictitious material, P∗ may be the correct collapse loading in this material, and the theorem follows. Radenkovic’s second theorem, as modified by Josselin de Jong [1965], is based on the existence of a function g(σ) with the following properties: 1. g(σ) is a convex function (so that any surface g(σ) = constant is convex); 2. g(σ) = 0 implies f (σ) ≤ 0 (so that the surface g(σ) = 0 lies entirely within the yield surface f (σ) = 0); 3. to any σ with f (σ) = 0 there corresponds a σ 0 such that (a) ε˙ p is normal to the surface g(σ) = 0 at σ 0 , and (b) 0 (σij − σij )˙εij ≥ 0.
(3.5.4)
The theorem may then be stated thus: The limit loading for a body made of a nonstandard material is bounded from below by the limit loading for the standard material obeying the yield criterion g(σ) = 0. The proof is as follows. Let σ denote the actual stress field at collapse, P the limit loading, v the actual velocity field at collapse, ε˙ the strainrate
170
Chapter 3 / Constitutive Theory
field, and p˙ the generalized velocity vector conjugate to P. Thus, by virtual work, Z P · p˙ = σij ε˙ ij dV. R
Now, the velocity field v is kinematically admissible in the fictitious standard material. If σ 0 is the stress field corresponding to σ in accordance with the definition of g(σ), then it is the stress field in the fictitious material that is ˙ and, if P0 is the loading that is in equilibrium plastically associated with ε, 0 with σ , then Z P0 · p˙ =
R
0 σij ε˙ ij dV.
It follows from inequality (3.5.4) that ˙ P0 · p˙ ≤ P · p. Again, σ 0 may, as a special case, coincide with the correct stress field at collapse in the standard material, and therefore P0 may be the correct limit loading in this material. The theorem is thus proved. In the case of a Mohr–Coulomb material, the function g(σ) may be identified with the plastic potential if this is of the same form as the yield function, but with an angle of dilatation that is less than the angle of internal friction (in fact, the original statement of the theorem by Radenkovic [1962] referred to the plastic potential only). The same is true of the Drucker– Prager material. It should be noted that neither the function g, nor the assignment of σ 0 to σ, is unique. In order to achieve the best possible lower bound, g should be chosen so that the surface g(σ) = 0 is as close as possible to the yield surface f (σ) = 0, at least in the range of stresses that are expected to be encountered in the problem studied. Since the two surfaces do not coincide, however, it follows that the lower and upper bounds on the limit loading, being based on two different standard materials, cannot be made to coincide. The correct limit loading in the nonstandard material cannot, therefore, be determined in general. This result is consistent with the absence of a uniqueness proof for the stress field in a body made of a nonstandard perfectly plastic material (see 3.4.1).
3.5.3.
Shakedown Theorems
The collapse discussed thus far in the present section is known as static collapse, since it represents unlimited plastic deformation while the loads remain constant in time. If the loads are applied in a cyclic manner, without ever reaching the static collapse condition, other forms of collapse may occur. If the strain increments change sign in every cycle, with yielding on both sides of the cycle, then alternating plasticity is said to occur; the net plastic
Section 3.5 / LimitAnalysis and Shakedown Theorems
171
deformation may remain small, but weakening of the material may occur nevertheless — a phenomenon called lowcycle fatigue — leading to breaking of the most highly stressed points after a certain number of cycles. It may also happen that plastic deformation in each cycle accumulates so that after enough cycles, the displacements are large enough to be equivalent to collapse; this is called incremental collapse. On the other hand, it may happen that no further plastic deformation occurs after one or a few cycles — that is, all subsequent unloadingreloading cycles are elastic. In that case the body is said to have experienced shakedown or adaptation. It is obvious that for bodies subject to repeated loading, shakedown is more relevant than static collapse, and that criteria for shakedown are of great importance.
Residual Stresses: Example If an initially stressfree body has been loaded into the plastic range, but short of collapse, and the loads are then reduced to zero, then the stress field in the unloaded body does not in general vanish. As an example, consider the fourflange sandwich beam shown in Figure 3.5.2, subject to a bending moment M only. If the flanges behave similarly in tension and compression, 2
6 h
? 6 O
h
? 6 h
?
J ] J J J J J 1 YH H H JJ HH JA H O
10
20
Figure 3.5.2. Ideal fourflange beam: geometry. then the stresses in the flanges satisfy σ10 = −σ1 and σ20 = −σ2 , and the moment is M = −σ1 Ah − 3σ2 Ah. In accordance with elementary beam theory (which is discussed further in Section 4.4), the longitudinal strain in the flanges varies linearly with distance from the socalled neutral plane, which in the present case may be shown to be the plane OO. Thus ε2 = 3ε1 , with ε10 = −ε1 and ε20 = −ε2 . As long as all flanges are elastic, stress is proportional to strain, and therefore
172
Chapter 3 / Constitutive Theory
σ2 = 3σ1 . It follows that σ1 = −
M def e = σ1 , 10Ah
σ2 = −
3M def e = σ2 . 10Ah
By definition, the notation σ e will be used for stresses calculated on the basis of assumed elastic behavior of a body, or elastic stresses. def
The outer flanges will yield when M  = (10/3)σY Ah = ME . Provided that the web holds, however, the deformation will remain contained so long as the inner flanges remain elastic. Collapse occurs when all four flanges yield, that is, when σ1 = σ2 = −σY , so that M  = 4σY Ah = MU . The range ME ≤ M  ≤ MU is called the range of contained plastic deformation. Suppose, for example, that M = (11/3)σY Ah = M ∗ . The actual stresses are σ1 = −(2/3)σY , σ2 = −σY , while the elastic stresses are σ1e = −(11/30)σY , σ2e = −(11/10)σY . When the moment is removed, the flanges will unload elastically, a process equivalent to subtracting the elastic stresses from the actual stresses. The resulting residual stresses are σ1r = −(3/10)σY and σ2r = (1/10)σY . Their resultant moment is, of course, zero. If the beam is now repeatedly reloaded with a bending moment of the same sign as before, the response will be elastic provided that M ≤ M ∗ . Consequently, for the given load amplitude, shakedown takes place in the first cycle.
Residual Stress and Displacement A stress field ρ that is in equilibrium with zero body force and zero prescribed surface tractions is called selfequilibrated , or, more simply, a field of selfstress. Such a field must clearly satisfy ρij ,j = 0 in R,
ρij nj = 0 on ∂Rt .
In an elasticplastic body under given loads f , ta , the stress field can always be written as σ = σ e + ρ, (3.5.5) where σ e is the elastic stress field corresponding to the given loads, and ρ is the selfequilibrated field of residual stresses. The strain field can accordingly be written as −1 e −1 εij = Cijkl σkl + Cijkl ρkl + εpij . (3.5.6) The first term, which will be written ε0ij , represents the strain field in the hypothetical elastic body under the prescribed loads. This strain field is compatible with a displacement field that will be denoted ue , that is, 1 ε0ij = (uei ,j +uej ,i ). 2 Since the total strain field ε is also compatible, the remaining terms of (3.5.6) are also derivable from a displacement field ur (the residual displacement
Section 3.5 / LimitAnalysis and Shakedown Theorems
173
field): 1 −1 Cijkl ρkl + εpij = (uri ,j +urj ,i ), 2
(3.5.7)
and u = ue + ur . It may be shown that the plastic strain field εp uniquely determines the residual stress field ρ and, with sufficient constraints to prevent rigidbody displacement, also the residual displacement field ur . The method of proof is analogous to that of the elastic uniqueness theorem of 3.4.1. If ρ and ρ + ρ are two different residual stress fields, then, from the principle of virtual work, Z R
−1 ρij (Cijkl ρkl
Z
= R
+
εpij ) dV
Z
= R
−1 ρkl + εpij ) dV (ρij + ρij )(Cijkl
−1 (ρij + ρij )[Cijkl (ρkl + ρkl ) + εpij ] dV = 0.
Rearrangement of terms leads to Z R
−1 ρij Cijkl ρkl dV = 0,
and hence to ρ = 0 in view of the positivedefiniteness of C−1 . With ρ uniquely determined by εp , it follows from (3.5.7) that ur is determined to within a rigidbody displacement.
QuasiStatic Shakedown Theorem Suppose that an elasticplastic body has already shaken down under a loading that is varying in time (but sufficiently slowly so that inertia may be neglected) within a certain range of the generalized loads. It follows from the definition of shakedown that the plastic strain field εp remains constant in time and defines a timeindependent residual stress field ρ such that the total stress field σ, given by (3.5.5), does not violate the yield criterion anywhere: f (σ e + ρ) ≤ 0. Clearly, the existence of such a residual stress field is a necessary condition for shakedown. It was shown by Melan [1938], however, that this is also a sufficient condition: shakedown will occur in the given load range if a timeindependent selfstress field ρ∗ , not necessary equal to the actual residual stress field ρ, can be found such that f (σ e + ρ∗ ) < 0 for all elastic stress fields σ e corresponding to loadings within the given range.
174
Chapter 3 / Constitutive Theory To prove the theorem, we consider the nonnegative quantity 1 Y = 2
Z R
−1 Cijkl (ρij − ρij ∗ )(ρkl − ρkl ∗ ) dV.
Since the body may not yet have shaken down, the actual residual stress field ρ, and hence Y , may be timedependent, with Y˙ =
Z R
−1 Cijkl (ρij − ρij ∗ )ρ˙ kl dV.
Since ρ and ρ∗ are both selfequilibrated, and since the lefthand side of (3.5.7) forms a compatible strain field, it follows from the principle of virtual work that Z −1 (ρij − ρij ∗ )(Cijkl ρ˙ kl + ε˙ pij )dV = 0. R
Consequently Y˙ = −
Z R
σ∗
(ρij − ρij ∗ )˙εpij dV = −
ρ∗ .
σe
Z R
(σij − σij ∗ )˙εpij dV,
σ∗
where = + By hypothesis, does not violate the yield criterion, and therefore, as a result of the maximumplasticdissipation postulate (3.2.4), Y˙ ≤ 0, where the equality holds only in the absence of plastic flow. Since Y ≥ 0, the condition Y˙ = 0 must eventually be reached, and this condition corresponds to shakedown. An extension of the theorem to workhardening materials is due to Mandel [1976] (see also Mandel, Zarka, and Halphen [1977]). The yield surface is assumed to be of the form f (σ, ξ) = F (σ − cεp ) − k 2 (κ), where F is a homogeneous quadratic function of its argument, and k is a nondecreasing function of κ. A body made of such a material will shake down if, in addition to a timeindependent residual stress field ρ∗ , there exist timeindependent internalvariable fields ξ ∗ = (εp∗ , κ∗ ) such that f (σ e + ρ∗ , ξ ∗ ) < 0 everywhere.
Kinematic Shakedown Theorem A kinematic criterion for shakedown was derived by Koiter [1956, 1960]. A strong version of Koiter’s theorem states that shakedown has not taken place if a kinematically admissible velocity field v∗ , satisfying v∗ = 0 on ∂Rv , can be found so that Z R
∗
f · v dV +
Z ∂Rt
a
∗
t · v dS >
Z R
Dp (ε˙ ∗ ) dV.
Section 3.5 / LimitAnalysis and Shakedown Theorems
175
This inequality, with the principle of virtual work applied to its lefthand side, can be transformed into Z R
e σij ε˙ ij ∗ dV
Z
Dp (ε˙ ∗ ) dV.
>
(3.5.8)
R
Suppose, now, that shakedown has taken place, with a timeindependent residual stress field ρ. From the maximumplasticdissipation postulate, e D(ε˙ ∗ ) ≥ (σij + ρij )˙εij ∗ ,
and therefore Z
D(ε˙ ∗ )dV ≥
Z
R
R
e σij ε˙ ij ∗ dV +
Z
ρij ε˙ ij ∗ dV.
(3.5.9)
R
An application of the virtualwork principle to the last integral shows that it vanishes, since ρ is selfequilibrated and v∗ = 0 on ∂Rv . Inequalities (3.5.8) and (3.5.9) are therefore in contradiction, that is, shakedown cannot have taken place. A weaker version of the theorem requires only that a strain rate ε˙ ∗ be found during a time interval (0, T ) such that the strain field ∗
Z
ε =
T
ε˙ ∗ dt
0
is compatible with a displacement field u∗ that satisfies u∗ = 0 on ∂Ru , and Z 0
T
Z
∗
f · u˙ dV + R
Z ∂Rt
a
∗
t · u˙ dS
Z
T
Z
dt > 0
Dp (ε˙ ∗ ) dV dt.
R
With these conditions met, the body will not shake down during the interval. Recent developments in shakedown theory have included taking into account the effects of temperature changes, creep, inertia, and geometric nonlinearities. For a review, see the book by K¨onig [1987]
Exercises: Section 3.5 1. Find the ultimate load FU for the structure shown in Figure 4.1.2(a) (page 185), assuming that all the bars have the same crosssectional area, are made of the same elastic–perfectly plastic material with uniaxial yield stress σY , and act in simple tension. 2. Using both the lowerbound and the upperbound theorems, find the limit locus for the beam having the idealized section shown in Figure 3.5.2 (page 171) subject to combined axial force P and bending moment M .
176
Chapter 3 / Constitutive Theory
3. In a body made of a standard Mohr–Coulomb material with cohesion c and internalfriction angle φ under a load P , lower and upper bounds to the ultimate load PU have been found as PU− = ch− (φ) and PU+ = ch+ (φ). Show how the results can be used to find the best bounds on PU if the material is nonstandard but has a plastic potential of the same form as the yield function, with a dilatation angle ψ 6= φ. 4. For the beam of Figure 3.5.2 subject to a bending moment M only, find the range of M within which shakedown occurs on the basis of the following assumed selfstress distributions. (a) ρ1 ∗ = 21 σY = −ρ01 ∗ , ρ2 ∗ = − 16 σY = −ρ02 ∗ (b) ρ1 ∗ = − 12 σY = −ρ01 ∗ , ρ2 ∗ = 16 σY = −ρ02 ∗ (c) ρ1 ∗ = 34 σY = −ρ01 ∗ , ρ2 ∗ = − 14 σY = −ρ02 ∗ 5. For the beam of Figure 3.5.2 under combined axial force P and bending moment M , (a) find the elastic stresses σ e in each flange; (b) given the selfstress distribution ρ1 ∗ = − 35 σY , ρ2 ∗ = 54 σY , ρ01 ∗ = 15 σY , ρ02 ∗ = − 52 σY find the range of P and M moments under which shakedown occurs by ensuring that ρ∗ + σ e  ≤ σY in each flange. 6. Using the result of Exercise 2 for the beam of Figure 3.5.2 under combined axial force and bending moment, find, if possible, loading cycles between pairs of points on the limit locus such that there occurs (a) incremental plastic deformation, (b) alternating plastic deformation, and (c) shakedown.
Chapter 4
Problems in Contained Plastic Deformation Section 4.1 4.1.1.
Elementary Problems
Introduction: Statically Determinate Problems
There are a few static or quasistatic boundaryvalue problems in solid mechanics that are approximately statically determinate. That is, much of the stress field may be determined from the applied loading (whether prescribed tractions or initially unknown reactions), independently of the material properties. These problems include the following: (a) Uniaxial tension or compression of a straight rod or tube with an axial force P . (b) Torsion of a thinwalled tube with a torque T . (c) Simultaneous tension or compression and torsion of a thinwalled tube. (d) Axially symmetric loading of a thinwalled shell of revolution. The solution of these problems, as regards stress, is the stuff of elementary solid mechanics. In problem (a), away from the ends the only significant stress component is the axial stress σ = P/A, where A is the crosssectional area, and this stress is uniform if A is constant, that is, if the bar is prismatic. This solution constitutes the basis of the simple tension or compression test discussed in Section 2.1; the loadelongation diagram essentially reproduces the conventional stressstrain diagram. Similarly, in problem (b) the only significant stress component is the shear stress τ = T /2Ah, where A is the area enclosed by the curve tracing the midpoints of the wall, and h is the wall thickness. This stress is constant if the wall thickness is uniform. If the tube, moreover, is circular, with radius 177
178
Chapter 4 / Problems in Contained Plastic Deformation
c, then τ = T /2πc2 h, while the shear strain is given by γ = cφ/L, where φ is the relative angle of twist between the ends of the tube, and L is its length. The T φ diagram of the tube thus reproduces the τ γ diagram of the material. The torsion of a thinwalled circular tube is consequently a simple means of determining the pure shearing behavior of solids that are sufficiently strong in tension, such as metals and hard plastics. As discussed in Section 2.3, geomaterials require different tests of shear behavior. A complication of the torsion test on thinwalled tubes is that if the thickness is too small in relation to the radius, the induced compressive stress may provoke buckling. It is characteristic of these two problems that if the material is taken as perfectly plastic, then the applied load (force or torque) cannot exceed the value at which yielding first occurs. When this value is reached, the body continues to deform under constant load — a process that, depending on the field of application, is called plastic flow or plastic collapse — until significant changes in geometry take place, or until inertial effects become important. The solution of problem (c) for stresses is the superposition of those of (a) and (b). The resulting stress field forms, locally, a state of plane stress determined by σ and τ , so that if the material yields according to either the Mises or the Tresca criterion, the yielding is described by Equation (3.3.5). Measurements of changes in elongation and twist angle provide a test of the flow rule, and the movement of the yield curve in the στ plane may elucidate the hardening rule. Tests based on this problem were first performed by Taylor and Quinney [1931]. The solution of problem (d) is particularly simple when the shell is a sphere (or a portion of a sphere), of radius c and wall thickness h, under uniform internal and external pressure. This loading produces a state of uniform, essentially plane stress, with both principal stresses equal to σ = pc/2h, p being the pressure difference (internal less external). Another important case is that of a cylindrical tube under a combination of uniform pressure and an axial force P ; in this case the principal stresses are σ1 = pc/h (circumferential) and σ2 = pc/2h+P/2πch (axial). Since arbitrary combinations of principal stresses can be produced by varying the axial force and the pressure, this case has formed the basis of numerous experiments, beginning with those of Lode [1925], to study yield criteria, flow rules, and hardening.
4.1.2.
ThinWalled Circular Tube in Torsion and Extension
We consider, as a special case of problem (c), a circular tube made of a rateindependent plastic material governed by either the Mises or the Tresca yield criterion, given in terms of σ and τ by Equation (3.3.5). We furthermore assume isotropic hardening based on a hardening variable κ. The criterion
Section 4.1 / Elementary Problems
179
may therefore be written in the form f (σ, τ, κ) = σ ¯ − σY (κ) = 0,
(4.1.1)
√ where σ ¯ = σ 2 + ατ 2 , and α = (σY /τY )2 is a constant equal to 3 for Mises criterion and 4 for the Tresca criterion. Note that f inte = σ ¯˙ . The flow rule will be assumed to be associated and hence derivable from a plastic potential which may be identified with σ ¯ . The associated flow rule is equivalent to the postulate of maximum plastic dissipation, Equation (3.2.4), which in the present state of stress reduces to (σ − σ ∗ )ε˙p + (τ − τ ∗ )γ˙ p >= 0 for any σ ∗ and τ ∗ such that f (σ ∗ , τ ∗ , κ) ≤ 0. Thus the plastic elongation rate ε˙p and shearing rate γ˙ p are the strain rates conjugate to the stresses σ and τ , respectively, and are given by σ ε˙p = λ˙ , σ ¯
ατ γ˙ p = λ˙ . σ ¯
If the hardening variable κ is defined by r
κ˙ =
(ε˙p )2 +
1 p 2 (γ˙ ) , α
˙ and therefore the hardening modulus H, as defined by Equation then κ˙ = λ, (3.1.1), is just σ 0 Y (κ). In view of Equation (4.1.1), H is a function of σ ¯ in any plastic loading process. In particular, H(¯ σ ) is the slope of the σεp curve obtained from a simple tension or compression test at a point where σ = σ ¯ ; it is also α1 times the slope of the τ γ p curve obtained from the √ simple torsion test, problem (b), at a point where τ  = σ ¯ / α. Equations (3.2.1)–(3.2.2) for this problem thus reduce to σ˙ σ + , E Hσ ¯ τ˙ ατ γ˙ = + . G Hσ ¯
ε˙ =
(4.1.2)
When a stress path σ(t), τ (t) is prescribed, Equations (4.1.2) can be used to find the corresponding strain path ε(t), γ(t) by integration, in general numerical. An explicit form may be obtained when the stress path is radial, that is, when σ = a¯ σ and τ = b¯ σ , a and b being constants constrained by 2 2 the requirement a + αb = 1. With ε¯(¯ σ ) defined by Z
ε¯(¯ σ) =
d¯ σ H(¯ σ)
180
Chapter 4 / Problems in Contained Plastic Deformation
(note that this describes the σεp curve in simple tension and compression), the strains are given by a σ ¯ + a¯ ε(¯ σ ), E b γ= σ ¯ + αb¯ ε(¯ σ ). G ε=
When the strain path is given, Equations (4.1.2) form a pair of coupled nonlinear differential equations for the stresses; they must in general be solved numerically. If, however, the workhardening is very slight (this includes the limit of perfect plasticity), then σY may be regarded, at least over a certain range of strain, as a constant, and σ and τ are no longer independent but are coupled through the yield criterion. The quantity σ ¯˙ /H σ ¯ may be eliminated between the two equations, resulting in the single equation ατ σ˙ σ τ˙ − = ατ ε˙ − σ γ. ˙ E G Suppose, for example, that the tube is stretched until it just yields (σ = σY , τ = 0); thereafter, it is twisted, with further axial deformation prevented, that is, ε˙ = 0. After σ is eliminated, the equation becomes dγ 1 ατ 2 = + , dτ G E(τY2 − τ 2 ) and may be integrated to yield 1 α τY τY + τ γ= τ+ ln −τ G 2(1 + ν) 2 τY − τ
.
This result can also be in terms of the ratio of plastic to elastic shear strain: γp α τY 1 + τ /τY = ln −1 . e γ 2(1 + ν) 2τ 1 − τ /τY
It is clear that the shear strain, and therefore the angle of twist, grows indefinitely as the torque approaches its ultimate value 2πc2 hτY . Unlike the simple problems (a) and (b), however, in this case the growth is asymptotic. Indeed, so long as the shear stress is less than, say, 99its yield value, the plastic strain remains of the same order of magnitude as the elastic strain. The tube can then be said to be in a state of contained plastic deformation. In the present chapter we concentrate on problems of this type; problems in plastic flow and collapse are considered in Chapter 5. As the shear stress approaches the yield value, the axial stress approaches zero, and a state of virtually pure torsion is attained. The constant axial strain σY /E changes, in the process, from purely elastic to plastic. Since these changes take place over a rather narrow range of strain, the validity of
Section 4.1 / Elementary Problems
181
the assumption of negligible workhardening, which was necessary to obtain the solution, may be limited to this range. It therefore follows that the τ γ curve for this problem will asymptotically attain the curve for simple shear. If desired, the remaining strainrate components ε˙r and ε˙θ may be found through the flow rule. Since σr = σθ = 0, and therefore sr = sθ = − 12 sz , the Mises flow rule (α = 3) implies ε˙r = ε˙θ = − 21 ε˙z . Since, however, σr = 0 is the intermediate principal stress, the Tresca flow rule (α = 4) implies ε˙r = 0, ε˙θ = −ε˙z . A completely analogous result is produced if the twist is held constant while extension proceeds. For this and related problems, see Hill [1950], pp. 71–75, or Chakrabarty [1987], Section 3.3(i). Hill’s results relating to large deformation must be taken with caution, because, as was pointed out in 2.1.1, the use of logarithmic strains is inappropriate when the principal strain axes rotate. Moreover, the results are based on the use of nonobjective stress rates; this matter is discussed further in Chapter 8.
4.1.3.
ThinWalled Cylinder Under Pressure and Axial Force
In a cylindrical shell under a uniform internal pressure p and a tensile axial force P , the principal stresses are σ1 = pc/h (circumferential) and σ2 = 1 σ + σa (axial), where σa = P/2πch. If the material is governed by the 2 1 Mises criterion with isotropic hardening, this criterion can once more be q 2 written in the form (4.1.1), but this time with σ ¯ = σa + 43 σ12 . It is convenient to use σa and σ1 as the variables defining the stress state, since the yield function is defined in terms of these stresses. The associated flow rule will be assumed, and its form may again be derived from the postulate of maximum plastic dissipation. Let εz denote the axial and εθ the circumferential strain. Since the plastic dissipation takes the form Dp = σ1 ε˙p1 + σ2 ε˙p2 = σ1 (ε˙pθ + 21 ε˙pz ) + σa ε˙pz , it follows that
σa , Hσ ¯ where H is again the uniaxial hardening modulus, and ε˙pz =
3 σ1 1 ε˙pθ + ε˙pz = , 2 4 Hσ ¯ from which ε˙pθ =
3 4
σ1 − 12 σa . Hσ ¯
182
Chapter 4 / Problems in Contained Plastic Deformation
The equations for the total strain rates are therefore σa σ˙ a + ( 12 − ν)σ˙ 1 + , ε˙z = E H σ ¯ 3 (1 − 12 ν)σ˙ 1 − ν σ˙ a σ1 − 12 σa ε˙θ = + 4 . E Hσ ¯
(4.1.3)
The calculations may now proceed as in the previous example. However, since in the present case the principal axes of strain do not rotate, there is no difficulty in extending the results into the largedeformation range by interpreting the strains as logarithmic. The strain rates are given by l˙ ε˙z = , l
c˙ ε˙θ = . c
The volume enclosed by the shell is πc2 l (if h is neglected next to c), and its change is given by V˙ l˙ 2c˙ 5 3σ1 σ ¯˙ 1 = + = ε˙z + 2ε˙θ = (1 − 2ν)σ˙ a + − 2ν σ˙ 1 + . V l c E 2 2H σ ¯
When the deformations are sufficiently great, the elastic strains may be neglected. The shell material may then be regarded as incompressible, so that the solid volume 2πchl remains constant, and the thickness h may be determined from this condition. Consider, for example, a closed cylindrical tank containing gas under pressure and undergoing an axial extension at a constant absolute temperature T . It follows from the idealgas law, pV = nRT, where n is the number of moles of gas and R is the universal gas constant (Avogadro’s number × Boltzmann’s constant), that plc2 is constant. But plc2 =
pc lch = σ1 lch, h
and therefore σ1 is also a constant, given by the initial value of pc/h. We may now write V˙ 1 − 2ν 3σ1 σ ¯˙ = σ˙ a + . V E 2H σ ¯ We assume, first, linear workhardening (H = constant) after an initial yield stress σE . We further suppose that the √ gas pressure alone is not sufficient to cause yielding, that is, σ1 < 2σE / 3. We may then integrate the preceding equation to obtain V 1 − 2ν 3σ1 ln = σa + < ln V0 E 2H
s
σa2 + 34 σ12 >. σE
Section 4.1 / Elementary Problems
183
If, on the other hand, the workhardening is described by the Ramberg– Osgood equation (2.1.2), then !(m−1)/2 !m √ 2 3 22 V 1 − 2ν 3mσ1 σa + 4 σ1 3σ1 ln = σa + − 1 . − V0 E 2(m − 1)E σ 2σR R Note that the elastic part of the volumetric strain has the same sign as σa , but the plastic part is never negative, whether the tank undergoes extension or compression. Note also that the expression for the volume becomes infinite in the limit as H− > 0 for the linear workhardening case and as m− > inf for the Ramberg–Osgood case; both of these limits represent perfect plasticity. In this example, then, contained plastic deformation cannot occur if the material is perfectly plastic. The difference between the present problem and the preceding one does not lie in the fact that one involves torsion and extension, and the other extension and gas pressure. Rather, the crucial difference is that the twisted tube was subject to the kinematic constraint of no axial extension; it is this constraint that prevented unrestricted plastic deformation immediately upon yielding. Had the axial force, rather than the length, been held constant, contained plastic deformation would not have taken place. In the case of linear workhardening an explicit expression can also be found for the axial extension and the radial expansion. The former is governed by l˙ σ˙ a σ 2 σ˙ a = + 2 a3 2 , (4.1.4) l E (σa + 4 σ1 )H which may be integrated to give " # √ r q σa 1 2σ l 3 3σ a 1 + . l0 E H 2 2σY 3σ1 The axial force at a given value of l may then be found from l0 P = 2πc0 h0 σa . l
(4.1.5)
A similar integration for the radius change leads to s
c νσa 3σ1 σa2 + 34 σ12 ln = − + < ln > c0 E 4H σE r " # √ q 3 2σ 3 σ 1 a 1 −1 −1 . − − cos 2H 2 2σY 3 σ1 The force P given by Equation (4.1.5) becomes stationary (P˙ = 0), indicating an instability, when l˙ σ˙ a = . l σa
184
Chapter 4 / Problems in Contained Plastic Deformation
Equating the righthand side of this equation to that of (4.1.4), and assuming that H E so that the elastic strain rate can be neglected, we find a critical value of the hardening modulus above which instability will not occur, namely σ3 Hc r = a2 . σ ¯ Note that this is positive only when σa > 0, that is, when the axial force is tensile; when this force is compressive, any nonnegative value of H is sufficient for stability. Note further that, in the absence of pressure, Hc r = σa ; this is just the necking condition discussed in 2.1.2. The pressure tends to lower the critical value of the hardening modulus, so that it is a stabilizing factor. Different values of Hc r are found for problems in which the ratio σa /σ1 or the ratio P/p is held fixed (see, e.g., Chakrabarty [1987], Section 3.3(iii)].
4.1.4.
Statically Indeterminate Problems
In contrast to the statically determinate problems just discussed, in statically indeterminate problems contained plastic deformation occurs even without kinematic constraints. Consider the simple pinconnected threebar assemblage shown in Figure 4.1.1(a). Since a pin joint cannot transfer moments, the bars carry axial forces only and each bar can be assumed to be in a state of uniaxial tension or compression, the stress being σ = P/A, where P is the axial force in the bar. If all three bars have the same crosssectional area A and are made of the same elastic–perfectly plastic material, with Young’s modulus E and yield stress σY , the elastic solution for the bar forces P0 and P1 ( = P10 ) is P0 =
F , 1 + 2 cos3 θ
P1 =
F cos2 θ , 1 + 2 cos3 θ def
and is valid while P0 ≤ PU (where PU = σY A), or F ≤ (1+2 cos3 θ)PU = FE ; here FE denotes, as usual, the elasticlimit value of the load F . When def F = FE , the downward displacement ∆ of the joint equals σY L/E = ∆E . The range 0 < F < FE , or 0 < ∆ < ∆E , represents the elastic range. When F > FE , P0 remains constant at PU , and P1 may be determined by statics alone to be 21 (F − PU ) sec θ, provided that this value does not reach def
PU . The latter condition occurs when F = (1 + 2 cos θ)PU = FU . In the range FE < F < FU , the displacement ∆ is determined by the deformation of bars 1 and 10 alone, a deformation that remains purely elastic. It is this elastic deformation that also determines the plastic deformation of bar 0. The range in question is thus the range of contained plastic deformation. Contained plastic deformation ends when ∆ = ∆E sec2 θ. Beyond this value, the displacement grows indefinitely while F remains at the value FU ,
Section 4.1 / Elementary Problems
185 F
sf s f s f 1 TT 10 0 TT TT + θ s θ TT T T TT f s
FU
FE
∆
?
F
∆E
(a)
(b)
∆E sec2 θ
Figure 4.1.1. Threebar assemblage: (a) structure; (b) loaddeflection diagram. precisely the definition of plastic collapse given in Section 3.4, and the load FU is the ultimate load of the structure. The complete F ∆ diagram is shown in Figure 4.1.1(b). It is not difficult to see that if the number of bars in the assemblage is multiplied, as in Figure 4.1.2(a), the loaddeflection diagram has the form shown in Figure 4.1.2(b). The range of contained plastic deformation is now represented by numerous segments, whose initial and final points must be calculated step by step. F
f s.......................................... f s f s f s sf sf f s ........................................... l.................n........0.................................................A...A.. 20 CC 10 0 1 2............................................................................., , l n . l...................................................A. CC z ...................................................., , l ......................... Y H .. jH , l.......................................A........... C . . . . . . . , l .................. ....................H k l...........................A...A....... C C .... ., Q , l Q ..............., .... H θ1 ......w l...............A......A.... C C .
[email protected] Q , l . . . I . . . . . . . l......A...A...A.C C .........., @ Q θ2 , l . , l l.A.C f , @θ l s, , l
FU
(
FE
n
∆
?
F
∆E
(a)
(b)
Figure 4.1.2. Multibar assemblage: (a) structure; (b) loaddeflection diagram. It can be shown that in the elastic range, the bar forces (if all bar areas are equal) are given by F
P0 = 1+2
n X k=1
, 3
cos θk
Pk =
F cos2 θk 1+2
n X k=1
. 3
cos θk
(4.1.6)
186
Chapter 4 / Problems in Contained Plastic Deformation
Note that the bar forces decrease with distance from the central bar. It can thus be assumed that the order of yielding of the bars is outward from bar 0. If bar 0 and m − 1 bars on either side of it have yielded (so that Pk = PU , k = 0, ..., m − 1), then it can be shown that for k = m, ..., n, cos2 θk
Pk = 2
n X
"
F − PU
1+2
3
m−1 X
!#
cos θl
,
(4.1.7)
l=1
cos θl
l=m
provided that Pm ≤ PU , that is, F ≤ PU
m−1 X
n X 2 1+2 cos θk + cos3 θk . 2θ cos m k=1 k=m
!
When all but the last pair of bars have yielded, that is, when m = n, the upper bound on F is just the ultimate load FU , given by FU = PU
1+2
n X
!
cos θk .
k=1
Of course, as we learned in 3.4.1, this value could easily have been determined without going through the stepbystep process. If, on the other hand, the structure were reduced to bar 0 only, then it would be statically determinate and naturally there would be no contained plastic deformation; the elastic range would be followed immediately by unrestricted plastic flow. Contained plastic deformation, therefore, is due either to constraints or to the introduction of redundant elements that make the structure statically indeterminate. A thinwalled tube under torsion or pressure forms, as we have seen, a statically determinate problem. A thickwalled tube may be thought of as the limit of an assemblage of a large number of concentric thinwalled tubes, all but one of which are redundant. The range of contained plastic deformation is therefore characterized by a torquetwist or pressureexpansion diagram which is the limit of that of Figure 4.1.2(b) as the segments become infinitesimal — that is, a smooth curve in which the ultimate load may be attained asymptotically, as in the problem of 4.1.2 [see Figure 4.1.3(a)] or at a finite displacement, as in Figure 4.1.3(b).
ElasticPlastic Boundary At any stage of contained plastic deformation in the problem of Figure 4.1.2, the spaces between the plastic and elastic groups of bars may be said to form the elasticplastic boundary. As the load is increased and an additional pair of bars yields, the boundary moves to the next pair of spaces. In a relatively simple problem such as this one, the elasticplastic boundary is defined by a single parameter, for example the integer m. Problems
Section 4.1 / Elementary Problems T or p
187 T or p
φ or u (a)
φ or u (b)
Figure 4.1.3. General loaddisplacement diagrams: (a) ultimate load reached asymptotically; (b) ultimate load reached at a finite displacement.
with radial symmetry, as shown in the next two sections, are similarly simple: the elastic and plastic zones can be separated only by a spherical or a cylindrical surface, and the boundary is determined by its radius. It is the simplicity of the elasticplastic boundary that makes problems of this nature tractable analytically. In general, the elasticplastic boundary is one of the unknown quantities of a problem, and when it is not defined by a small number of parameters then it can only be determined by trial and error, step by step, in the course of an incremental solution. Typically, the given loading is scaled down until it is small enough so that the whole body is elastic. Since the elastic problem is linear, the stresses are directly proportional to the load (in the case of oneparameter loading). With the help of the elastic solution it is therefore possible to find the value of the load at which the body first yields, such as FE in the preceding example, as well as the point or points where yielding first occurs. The elasticplastic boundary originates at these points. Following the initiation of yielding, the loading must be increased by small increments, and a trial solution is found for a statically admissible stressincrement field dσ. The resulting stress f atσ must then be tested to determine whether it is plastically admissible for the current yield surface. If it is not, then the trial solution must be corrected so as to bring all stress values inside or on the yield surface; the procedure is usually an iterative one. The points at which σ is inside the yield surface constitute the current elastic domain, while those where σ is on the yield surface form the plastic domain. The elasticplastic boundary is thus a part of the solution at each step. The solution must usually be carried out numerically, and methods are discussed in Section 4.5. Sections 4.2, 4.3, and 4.4 deal with problems that can be treated analytically.
188
Chapter 4 / Problems in Contained Plastic Deformation
Another feature of the problem of Figure 4.1.2, as well as of thickwalled tubes under pressure or torsion, is that when the ultimate load is reached, the entire body is plastic; in other words, the elasticplastic boundary passes out of the body. In the case of our bar assemblage, this is a result of the symmetry of the problem, with respect to both geometry and loading. In the absence of such symmetry it is not necessary for all the bars of an assemblage of this type to be plastic at collapse: one bar may remain elastic, since it can rotate rigidly as the other bars deform. There are other problems as well in which an elasticplastic boundary is present at collapse. An example is the cantilever beam studied in Section 4.4, and other examples are given in Section 5.1.
Exercises: Section 4.1 1. Solve Equations (4.1.2) for the stressstrain relation in tension when the tube is twisted until it just yields, and thereafter it is stretched with further twisting prevented. Assume negligible workhardening. 2. If the load on the assemblage of Figure 4.1.1(a) is not vertical but has both a vertical component V directed downward and a horizontal load H directed to the right, the problem is no longer symmetric and the three bar forces must be assumed to be distinct. Discuss the behavior of the assemblage when (a) V = cH, with c constant and H increasing, and (b) V is held constant at a value at which the assemblage is elastic, and then H is gradually increased from zero. 3. Suppose the assemblage of Figure 4.1.1(a) to carry no load but to be subject to a monotonically increasing temperature change, the temperature being the same in all bars. If the Young’s modulus E, the thermal expansion coefficient α, and the yield stress σY (equal in tension and compression) are independent of temperature, find the temperature change ∆T at which yielding begins. 4. Do Exercise 3 when σY is a linearly decreasing function of temperature; that is, σY = σY 0 − a(T − T0 ), where a is a constant and T0 is the initial temperature. 5. Show that Equations (4.1.6) describe the elastic state of the assemblage of Figure 4.1.2(a). 6. Show that Equations (4.1.7) give the forces in the bars of the assemblage of Figure 4.1.2(a) that have remained elastic when the central bar and m − 1 bars on either side of it have yielded. Find the value attained by the load F so that bars m are just about to yield.
Section 4.2 / Elastic–Plastic Torsion
189
7. When the load F has attained the value found in Exercise 6 and is then removed, find the residual bar forces. Which of the bars go into compression?
Section 4.2 4.2.1.
ElasticPlastic Torsion
The Torsion Problem
The twisting of prismatic bars under the action of equal and opposite torques applied at the ends is one of the classical topics of solid mechanics. For elastic bars of circular crosssection, the relation between torque and twist was first derived by Coulomb in 1784. A general theory for bars of arbitrary crosssection was published by SaintVenant in 1855; this theory makes it possible to predict where the stress is maximum, and therefore where, and at what values of the torque and twist, yielding will first occur. SaintVenant’s theory is based on the semiinverse method originated by him. An inverse method is one in which a solution (a stress field or a displacement field) is assumed, while the boundary conditions that it satisfies, and in particular the resulting surface tractions, are determined afterwards. In a semiinverse method, a part of the solution is assumed, and the rest is left to be determined by solving appropriate differential equations. In the torsion problem, assumptions can be made on both the stress and displacement fields. It is important to note that the value of the torque is not a part of the boundary data; instead, it is the angle of twist that is prescribed, and the torque results as a reaction to the imposed twist, not a load.
The BoundaryValue Problem We consider a prismatic bar whose longitudinal axis (e.g., the centroidal axis) is the x3 axis and whose crosssection (assumed simply connected) is defined by a closed curve C in the x1 x2 plane (see Figure 4.2.1). The bar is defined as being in a state of torsion or twist if one end section, viewed in its plane (i.e., with any warping ignored), rotates rigidly with respect to the other. The end sections are assumed to be free to warp, so that there is no normal traction on them. The lateral surface is tractionfree. Consequently, if the rotation of the section at x3 = 0 is defined as zero and if the relative angle of rotation between the two end sections is θL, then the boundary conditions are at x3 = 0 : at x3 = L :
u1 = u2 = 0, σ33 = 0; u1 = −θLx2 , u2 = θLx1 , σ33 = 0;
on C, 0 < x3 < L : Ti = σij nj = σiα nα = 0, where n1 =
dx2 dx1 , n2 = − . ds ds
190
Chapter 4 / Problems in Contained Plastic Deformation x2
6 H HH
C
H HH  x1 H H HH HH H H HH H HH H Y H HH H HH HH H H HH H HH HH L HH H j HH H H H j H
x3
Figure 4.2.1. Prismatic shaft: geometry.
Stress Assumptions If we assume that σ11 = σ22 = σ33 = σ12 = 0, then the equilibrium equations (with zero body force) reduce to τα ,3 = 0
(α = 1, 2),
τα ,α = 0,
where τα = σα3 . The first two equations imply that τ1 and τ2 are functions of x1 and x2 only, so that the problem is mathematically (though not physically) twodimensional. The third equation implies that there exists a function φ(x1 , x2 ) such that τ1 = φ,2 and τ2 = −φ,1 . To satisfy the traction boundary conditions, we need
dxα dφ τα nα = φ,α = = 0, ds C ds C so that φ must be constant on C. With no loss of generality we may let the constant be 0. If the section is multiply connected, with interior contours C1 , C2 ,..., then we can set φ = 0 on the exterior boundary curve C, but on each of the interior curves we can only set it equal to some unknown constant. The torque T is given by Z
T
(x1 τ2 − x2 τ1 ) dA = −
=
AZ
[(xα φ),α −2φ] dA = −
A
= 2
xα φ,α dA AI
= −
Z
Z Z
nα xα φ dA + 2 C
φ dA A
φ dA, A
since φ vanishes on C. We may think of the surface formed by the stress function φ(x1 , x2 ) as a “tent” pitched over the base formed by the boundary curve C; then the torque is twice the volume enclosed by the tent. The contour lines of the tent (curves along which φ has a constant value) are also significant: if at a given point of the crosssection, a local Cartesian
Section 4.2 / Elastic–Plastic Torsion
191
coordinate system is established so that the x1 axis is parallel to the contour, then locally τ1 = φ,2 and τ2 = 0. Thus every point of the shaft is stresswise in a state of simple shear, and the shear stress is everywhere directed along the contour, while its magnitude is just the slope of the tent surface. If the shaft is made of an elasticplastic material, then the yield criterion may be expressed in terms of the stress function φ as ∇φ = k, where k = τY is the yield stress in shear.
Displacement Assumptions If the material is isotropic, then regardless of whether it is elastic, plastic, or whatever, the only nonvanishing strain components (under the assumption of infinitesimal deformation) consistent with the stress assumptions can be def def the shear strains γ1 = 2ε13 and γ2 = 2ε23 . A displacement field consistent with this condition and with the displacement boundary conditions is u1 = −θx2 x3 ,
u2 = θx1 x3 ,
u3 = θψ(x1 , x2 ),
where ψ is known as the warping function; the factor θ is placed in front of it for convenience. Note that θ, which is simply called the twist, is the angle of twist per unit length, assumed uniform. The dependence of u3 on θ is not linear in all situations, but it is so in many of the ones that we are going to study. The strain components are γ1 = θ(ψ,1 −x2 ),
4.2.2.
γ2 = θ(ψ,2 +x1 ).
Elastic Torsion
The isotropic linear elastic stressstrain relations τα = Gγα translate to τ1 = φ,2 = Gθ(ψ,1 −x2 ), τ2 = −φ,1 = Gθ(ψ,2 +x1 ).
(4.2.1)
These are two equations in the two unknown functions φ and ψ. We may eliminate either one and be left with one differential equation in one unknown function.
The Stress Method If we eliminate ψ, so that φ is the unknown of the problem, we obtain ∇2 φ = −2Gθ,
(4.2.2)
which, together with the boundary condition φ = 0 on C, constitutes a standard mathematical problem. The conventional method of solution consists of, first, finding a particular solution φ1 which satisfies the differential equation but not necessarily the boundary conditions, and next, assuming that
192
Chapter 4 / Problems in Contained Plastic Deformation
φ = φ1 + φ2 , so that φ2 is the solution of the differential equation ∇2 φ2 = 0 (the Laplace equation) with the boundary condition φ2 = −φ1 on C — a classical problem known as the Dirichlet problem. Equation (4.2.2) together with the boundary condition is mathematically identical with the problem of the deflection of a membrane, tightly stretched in a frame occupying the contour C by an isotropic tension H and subject to a transverse pressure p; if this deflection is denoted w(x1 , x2 ), then the equation governing it is p ∇2 w = − , H and the correspondence, first discussed by Prandtl [1903], is known as the membrane or soapfilm analogy. With appropriate numerical scaling, it is possible to use the results of experiments on soap films in order to calculate the torsional properties of shafts (see, e.g., Timoshenko and Goodier [1970], pp. 324–325]. Even without actual experiments, the analogy is useful in helping to visualize the nature of the solution. In particular, it is often intuitively obvious where the slope of the membrane deflection, and hence the stress, is maximum. Typically, this maximum occurs at the points on the exterior boundary nearest the axis. For some crosssections, such as an ellipse and an equilateral triangle, a complete solution φ can be found in closed form. Using the conventional notation x, y in place of x1 , x2 , we may write the solution for an ellipse described by (x/a)2 + (y/b)2 = 1 as a2 b2 φ = Gθ 2 a + b2
x2 y 2 1− 2 − 2 a b
!
.
The torque on a shaft made of an isotropic, linearly elastic material with shear modulus G always has the form T = GJθ, where J has dimensions of length4 and depends on the geometry of the crosssection alone; the product GJ is known as the torsional stiffness. For the ellipse, we have J = πa3 b3 /(a2 + b2 ). The maximum stress is τmax =
2T max(a, b). πa2 b2
The circle is, of course, a special case of the ellipse with a = b. For the equilateral triangle, a stress function having the form φ(x, y) = Cf1 (x, y)f2 (x, y)f3 (x, y), where f1 (x, y) = 0,
f2 (x, y) = 0,
f3 (x, y) = 0
are the equations of the three lines forming the triangle, obviously satisfies the boundary condition φ = 0, and can easily be shown to satisfy the differential equation (4.2.2) with a suitable value of the constant C. If c denotes
Section 4.2 / Elastic–Plastic Torsion
193
the side of the triangle, then the torsional stiffness is maximum shear stress is τmax = 20T /c3 .
√
3Gc4 /80, and the
Rectangular Shaft A closedform solution does not exist for any other polygonal shaft. A Fourier series solution can be obtained for a rectangular shaft. Consider the rectangle bounded by x = + − a/2, y = + − b/2, with b >= a. If we assume that ! a2 φ1 = Gθ − x2 , 4 then this satisfies the boundary condition on the longer sides but not on the shorter sides; it is reasonable to expect that the larger b/a, the closer φ1 will be to φ. The “correction” φ2 may be assumed in the form of a Fourier series in x that is even in x and vanishes on x = + − a/2, and whose coefficients depend on y: ∞ X (2m + 1)πx fm (y) cos . φ2 = Gθ a m=0 Now ∞ X
2
∇ φ2 = Gθ
m=0
"
#
00 fm (y)
(2m + 1)2 π 2 (2m + 1)πx − fm (y) cos , 2 a a
00 = [(2m+1)π/a]2 f ; the solution and if this is to vanish for all (x, y), then fm m that is even in y is fm (y) = Am cosh(2m + 1)πy/a, where the coefficients Am must be such that φ2 = −φ1 on y = + − b/2. To satisfy this condition we need the appropriate Fourier series expansion for φ1 , that is, we need ∞ X a2 (2m + 1)πx − x2 = Bm cos ; 4 a m=0
then the solution is complete if Am cosh [(2m + 1)πb/2a] = −Bm . In accordance with the theory of Fourier series, Bm
4 = a
Z
a/2
0
!
(2m + 1)πx 8(−1)m a2 a2 − x2 cos dx = . 4 a (2m + 1)3 π 3
Hence, finally, φ2 = −Gθ
∞ 8a2 X (−1)m cosh (2m + 1)πy/a (2m + 1)πx cos . 3 π m=0 (2m + 1)3 cosh (2m + 1)πb/2a a
Integration leads to ∞ 1 64a X 1 (2m + 1)πb − 5 tanh . J =a b 5 3 π b m=0 (2m + 1) 2a
"
3
#
194
Chapter 4 / Problems in Contained Plastic Deformation
Since the hyperbolic tangent function approaches unity as its argument increases, the series converges very rapidly. The maximum shear stress occurs at (± 12 a, 0) and is given by ∞ (2m + 1)πb 1 8 X sech . = Gaθ 1 − 2 2 π m=0 (2m + 1) 2a
#
"
τmax
It is seen from the formula for J that as b/a → ∞, J → a3 b/3, which is the result based on φ1 alone. For such infinitely narrow rectangles we also obtain τmax = Gθa = T a/J. These results are often applied to the torsion of shafts of open thinwalled section made up of several rectangles (possibly even curved) of dimensions ai , bi (i = 1, ..., n) with bi ai . For such sections we have the approximations n . 1X 3 J= a bi , 3 i=1 i
. T amax τmax = . J
The Displacement Method If we choose the warping function ψ rather than the stress function φ as the unknown function of the problem, the governing differential equation is the Laplace equation ∇2 ψ = 0. The traction boundary conditions in terms of ψ are n1 (ψ,1 −y) + n2 (ψ,2 +x) =
∂ψ dy dx −y −x = 0, ∂ν ds ds
or
1 d 2 ∂ψ = r (r2 = x2 + y 2 ). ∂ν 2 ds This result makes it clear that the warping vanishes if and only if the crosssection is circular. For an ellipse, we find that ψ = [(b2 −a2 )/(b2 +a2 )]xy is an exact solution of the problem, but in general this problem is more difficult to work with than the one with φ as the unknown. Moreover, as is shown next, it is only with φ that a boundaryvalue problem for elasticplastic shafts can be formulated.
4.2.3.
Plastic Torsion
It is clear that in the elastic range the stress function is of the form φ(x1 , x2 ) = Gθ × f (x1 , x2 ), where f (x1 , x2 ) is determined by the crosssection geometry alone. As the twist θ is increased, the stresses grow proportionately, until at one or more points of the crosssection the yield criterion is met; these are the points — necessarily located on C — where ∇f  attains its maximum
Section 4.2 / Elastic–Plastic Torsion
195
value, and the value of θ when this occurs is θE = τE /(G∇f max ), where τE is the elasticlimit shear stress. As the twist is further increased beyond θE , one or more plastic regions form and expand, while the elastic regions shrink. If the shaft material is elastic–perfectly plastic, with τE = τY = k, then the equation satisfied by the stress function in the plastic regions is ∇φ = k. Eventually this equation becomes valid everywhere, a condition known as fully plastic torsion. In a solid (simply connected) shaft, this state is attained in the limit as θ → ∞, while in a hollow (multiply connected) shaft it may occur at a finite value of θ. The torsion of elasticplastic shafts with workhardening has generally been studied by means of deformation theory, it being argued that under monotonic loading such a treatment would provide a good approximation to the solutions of the incremental theory,1 although the two coincide exactly only when the shaft is circular. A formulation according to Prandtl–Reuss theory is due to Prager [1947]. In either case, the governing equations must be solved numerically.
Fully Plastic Torsion The mathematical problem given by ∇φ = k in A,
φ = 0 on C,
(4.2.3)
has a unique solution (Ting [1966a]), which will be denoted φp . The solution describes a roof of constant slope, and φp (x1 , x2 ) is simply k times the distance from (x1 , x2 ) to the nearest point on C. A point (x1 , x2 ) is a ridge point whenever there is more than one such nearest point. The ridge points represent the remnants of the elastic zone as it shrinks to zero area, so that the plastic strain rates vanish there. At a ridge point, therefore, γ˙ 1 = γ˙ 2 = 0 even in the limit as θ → ∞. A line consisting of ridge points is called a ridge line. Since a ridge point is the meeting place of contours having different directions, a ridge line is the locus of a discontinuity in ∇φ, and therefore the stress is discontinuous across the plane formed by the x3 axis and the ridge line. A stress discontinuity does not, by itself, violate equilibrium: consider an element ∆S of a surface perpendicular to the page and a very thin volume element containing it, as shown in Figure 4.2.2. In the limit as the thickness goes to zero, the element is in equilibrium if the traction is continuous, that is, if the stress components σn (the normal stress) and τ (the shear stress) are continuous; the lateral stress σt , on the other hand, may be discontinuous. Now, if n is a unit vector normal to a ridge line, then the traction on the plane normal 1
See, e.g., Mendelson [1968], Section 116; Kachanov [1971], Section 30; Chakrabarty [1987], Section 3.6(vi).
196
Chapter 4 / Problems in Contained Plastic Deformation
t(n)
6 @ @ σn τ @ I @@ @ @@ @ n ∆S @ @@ @ @@ @ @ @ @ @ @ R
[email protected] ? σt (may be discontinuous) t(−n)
Figure 4.2.2. Stress discontinuity
to n is e3 (n1 τ1 + n2 τ2 ), but n1 τ1 + n2 τ2 is just the component of ∇φ parallel to the ridge line, and this is continuous if the ridge line bisects the angle between the two φ contours that meet there. An experimental method for finding the solution is furnished by the sandheap analogy: if sand is piled onto a horizontal table having the shape of the crosssection, the slope of the resulting heap cannot exceed the angle of internal friction of the sand, and the maximal heap is formed when the critical slope obtains everywhere except at a vertex or on ridge lines; any additional sand poured will just slide off. If C is a regular polygon, then the φp surface takes the form of a pyramid. The limit of a regular polygon as the number of sides becomes infinite is a circle; the corresponding surface is a cone. For any other convex polygon, it is formed by ridge lines which bisect the angles between nearest sides, as seen in Figure 4.2.3.
A A A A A A A A A A A A A
Figure 4.2.3. Ridge lines and contours in a convex polygon. R
The torque given by 2 A φp dA is the ultimate torque TU . Thus, for a circle of radius a, TU = 32 πka3 . For a rectangle of sides a and b, with b > a, TU = 61 ka2 (3b − a). In a nonconvex polygon, that is, one with reentrant corners, the ridge
Section 4.2 / Elastic–Plastic Torsion
197
lines and contours are not all straight. Consider the crosssection shown in Figure 4.2.4. For a point (x, y) with x > y > 0, the nearest point on the y
@ @
Ridge lines
@ @ r(x,y)
r(a,y) XXX y X x
Contour lines
@ @
a
@ @ 
Figure 4.2.4. Ridge lines and contours in a nonconvex polygon. side with the reentrant corner is just the corner, while the pnearest point on the other side is (a, y); (x, y) is therefore a ridge point if x2 + y 2 = a − x, that is, if it lies on the parabola described by y 2 = a2 − 2ax. To the left of this parabola, the φp contours are circular arcs centered about the corner, and to the right they are straight lines parallel to the yaxis. The structure is, of course, symmetric about the line y = x.
Contained Plastic Torsion For values of the twist θ such that θE < θ < ∞, the crosssectional area A consists of elastic and plastic regions, with Equation (4.2.2) governing the stress function φ in the former and Equation (4.2.3) in the latter. The boundary of each region consists of those parts of C (if any) that belong to it, and of the elasticplastic boundary Γ, which is in general unknown and whose determination, as discussed in Section 4.1, constitutes a part of the problem. Moreover, values of φ on Γ are unknown. However, Equation (4.2.2) is an elliptic partial differential equation, and such an equation requires the specification of boundary data on a known, closed boundary. Consequently, the solution in the elastic region cannot be constructed. Equation (4.2.3), on the other hand, is parabolic, and its solution can be obtained by working inward from the plastic part of C. This solution is therefore the same as the solution for the fully plastic crosssection, provided that the plastic region
198
Chapter 4 / Problems in Contained Plastic Deformation
lies entirely between the normals to C at the points where Γ meets C (see Prager and Hodge [1951], Section 3.2); this result was proved by T. W. Ting [1966a]. We are thus led to the membraneroof analogy due to Nadai [1923]: we imagine a rigid roof having the shape of the surface of the ultimate sand heap, and a membrane stretched underneath it and subjected to a uniform upward pressure. Under sufficiently low pressures the membrane does not touch the roof, a state corresponding to elastic torsion. As the pressure is increased, parts of the membrane become tangent to the roof and remain there, representing the plastic regions, while those parts of the membrane that are still free represent the elastic region. The membraneroof analogy was used by Nadai [1950] for the experimental solution of elasticplastic torsion problems. It is clear from the analogy that the elastic region consists of those points where φ < φp and ∇φ < k. It was shown by Ting [1966b] that the correct solution is the one that minimizes the functional def
K[φ∗ ] =
Z
(∇φ∗ 2 − 4Gθφ∗ ) dA,
A
the minimum being taken either over all those functions φ∗ that satisfy φ∗ ≤ φp or those that satisfy ∇φ∗  ≤ k, in addition to satisfying φ∗ = 0 on C. The properties of the solution for various crosssections were further investigated in a series of papers by T. W. Ting [1967, 1969a,b, 1971]. Ting’s minimum principle also permits the application of numerical methods based on discretization, similar to that discussed for elastic bodies in 1.4.3, except for the presence of inequality constraints.
Elastic–Plastic Warping An important feature of the elasticplastic solution is that once a point of the crosssection has become plastic, the stress state there remains constant. Any strain increment in the plastic region is therefore purely plastic. The ˙ α , which follows from isotropy, implies that in the plastic flow rule γ˙ αp = λτ zone, γ˙ 1 ψ,1 −x2 φ,2 = =− . γ˙ 2 ψ,2 +x1 φ,1 Let the normal to the boundary subtend an angle χ with the x1 axis; then, in the plastic zone, φ,1 = −k cos χ,
φ,2 = −k sin χ.
Consequently, ψ,1 cos χ + ψ,2 sin χ = x2 cos χ − x1 sin χ, or
∂ψ = d, ∂n
Section 4.2 / Elastic–Plastic Torsion
199
where n denotes the directed distance, measured outward, along a line normal to the boundary, and d denotes the distance from this line to the origin (see Figure 4.2.5). If n is measured from the intersection point R of the x2
χ *Ar K? n P A r R
r
R0
K A
d
C
Γ
0
x1
AU
Figure 4.2.5. Elasticplastic warping: illustration of the notation used in the theory. given normal line with the elasticplastic boundary, then at a point P on the line such that n is the distance from R to P , ψ(P ) = ψ(R) + nd. To obtain ψ(R), we solve Equations (4.2.1) for the ψ,α . Along Γ, dψ = ψ,α dxα = x2 dx1 − x1 dx2 + so that Z
R
(x2 dx1 − x1 dx2 ) +
ψ(R) =
Z
R0
1 τα dxα , Gθ R
τα dxα , R0
where R0 is a point on Γ such that ψ(R0 ) = 0 — for example, the intersection of Γ with a line of symmetry, if such a line exists, or else an arbitrary point.
Warping of a Fully Plastic Rectangular Shaft The warping of a fully plastic rectangular shaft can be obtained more simply. Because of symmetry, it is sufficient to consider only the quadrant 0 < x < 21 a, 0 < y < 12 b, shown in Figure 4.2.6, which we divide into the regions I and II, respectively above and below the ridge line whose equation is y = [(b − a)/2] + x. In region I, τ2 = 0 and therefore ˙ 2 +x) = 0. γ˙ 2 = θ(ψ, The general solution of the partial differential equation ψ,2 +x = 0 is
200
Chapter 4 / Problems in Contained Plastic Deformation
y b 2 I Ridge line
b−a 2
II a 2
0
x
Figure 4.2.6. Fully plastic rectangular shaft: first quadrant, regions separated by ridge line. ψ(x, y) = −xy + f (x), f being an arbitrary continuously differentiable function. Symmetry requires zero warping on the yaxis, so that f (0) = 0. The ˙ nonvanishing shearingrate component is γ˙ 1 = θ[−2y + f 0 (x)], but since the shearing rate must vanish on the ridge line, it follows that f 0 (x) = b − a + 2x ˙ − a + 2(x − y)], and, consequently, f (x) = (b − a)x + x2 . (so that γ˙ 1 = θ[b In region II the warping function is governed by ψ,1 −y = 0, so that ˙ ψ = xy + g(y) with γ˙ 2 = θ[2x + g 0 (y)]. For this to vanish on the ridge line, we must have g 0 (y) = b − a − 2y for y > 21 (b − a), and if we integrate g 0 in the form g(y) = −[y − 21 (b − a)]2 , then the warping function is also continuous on the ridge line. For y < 12 (b − a), however, the vanishing of ψ on the yaxis requires g(y) = 0, and therefore the complete solution for g is g(y) = −2 , < · > being the Macauley bracket, and the ˙ − ]. shearing rate is γ˙ 2 = 2θ[(x 2 The results may be used to obtain the value of the ultimate torque by means of the upperbound theorem (Section 3.4). The plastic dissipation is
˙ = Dp (ε)
a 0 pY is applied to the interior of the tube and then reduced back to zero, the unloading process is elastic if p is not too great. The resulting field of residual stresses is obtained by subtracting the elastic stresses given by (4.3.19) and (4.3.22), with p given by (4.3.27), from the elasticplastic stresses given, in the case of the Tresca criterion, by (4.3.29)–(4.3.30). Using, furthermore, Equation (4.3.23), we obtain the residual stresses in the form " ! # p a2 r2 σr = −k 1 − 2 − ln 2 , p r ! a " E # 2 p a r2 σθ = −k a σr and the Tresca yield criterion and flow rule, but assume that the yield stress k is a function of a hardening variable κ, defined, say, by (1.5.6) (“plastic work”); in the present case, this definition reduces to κ˙ = k(κ)(ε˙pθ  + ε˙pr ) = 2k(κ)ε˙pθ , since ε˙pr = −ε˙pθ . As long as ε˙pθ ≥ 0 (no reverse yielding), the preceding relation can be integrated to give Z 0
κ
dκ0 = 2εpθ , k(κ0 )
so that κ is in a onetoone relation with εpθ , and k can also be viewed as a function of εpθ .
228
Chapter 4 / Problems in Contained Plastic Deformation A similar relation in uniaxial tension, with σ1 = σ, σ2 = σ3 = 0, gives κ˙ = k(κ)(ε˙p1  + ε˙p2  + ε˙p3 ) = 2k(κ)(ε˙p1 ),
since ε˙p2 = ε˙p3 = − 12 ε˙p1 . The relation between κ and εpθ in the tube is thus the same as between κ and εp1 in uniaxial tension. If σ1 = σY (εp1 ) describes the uniaxial relation between stress and plastic strain, then, in the tube, k = 21 σY (εpθ ). In the elastic zone the stress field is given by Equations (4.3.29), with k replaced by 12 σE , where σE = σY (0) is the initial yield stress. In the plastic zone the equilibrium equation (4.3.18) becomes dσr 1 = σY (εpθ ), (4.3.35) dr r with the boundary conditions σr = −p at r = a and σr = 21 σE (1 − c2 /b2 ) at r = c. The elastic relations for εeθ = εθ − εpθ and εer = εr + εpθ , together with the straindisplacement relations εθ = u/r and εr = du/dr, lead to u 1 = εpθ − νεz + [(1 − 2ν)(1 + ν)σr + (1 − ν 2 )σY (εpθ )] r E and
1 du = −εpθ − νεz + [(1 − 2ν)(1 + ν)σr − ν(1 + ν)σY (εpθ )]. dr E Eliminating u between these equations, with the substitution from (4.3.35), leads further to dεp dεp 1 − ν2 +r θ =− 2σY (εpθ ) + rH(εpθ ) θ , dr E dr "
2εpθ
#
where H = dσY /dεpθ is the hardening modulus. The last equation can be integrated, subject to the boundary condition that εpθ = 0 at r = c, to yield "
εpθ
#
c2 1 − ν2 σE 2 − σY (εpθ ) , = E r
With the help of the last equation, r can be eliminated as a variable in favor of εpθ , so that (4.3.32) can be integrated into a relation between σr and εpθ . If εp0 denotes the value of εpθ at r = a, then the pressure is given by 1 c2 p= 1− 2 2 b
!
1 σE + 2
Z 0
εp0
E + (1 − ν 2 )H(εpθ ) σY (εpθ ) dεpθ , Eεpθ + (1 − ν 2 )σY (εpθ )
(4.3.36)
with c given by c2 1 E = σY (εp0 ) + εp . 2 a σE 1 − ν2 0 The two last equations provide the relation between p and c through the parameter εp0 . The integration is in general carried out numerically, but an explicit relation is easily obtained if the hardening is linear, that is, if H is constant. Details are left to an exercise.
Section 4.4 / ElasticPlastic Bending
229
Exercises: Section 4.3 1. Discuss the behavior of an elasticplastic spherical shell under both external and internal pressure in comparison with its behavior under internal pressure only. 2. Evaluate Equation (4.3.10) for the case of linear workhardening, the uniaxial relation being σY = Hεp , where the plastic modulus H is constant. 3. A spherical shell of initial inner and outer radii a0 , b0 is made of a material whose stressstrain curve is given by σ = f (ε) with no elastic range. (a) Find an equation to replace (4.3.12). (b) Find the condition for plastic instability. 4. A hollow cylinder of initial inner and outer radii a0 , b0 is assumed to be in plane strain and made of an isotropically hardening Mises material that is both plastically and elastically incompressible. (a) Show that if the uniaxial stressstrain curve is given by σ = f (ε), √ √ then σθ − σr = (2/ 3)f (2εθ / 3). (b) Assuming large strains, with εθ = ln(r/r0 ), find the analogues of Equations (4.3.10) and (4.3.12). (c) Determine the criterion for plastic instability. 5. Discuss how Equation (4.3.36) would be integrated for a cylinder made of a material with no elastic range. 6. Integrate Equation (4.3.36) and thus find an explicit pc relation for the case of linear workhardening [i. e., σY (εp ) = σE + Hεp , with H constant].
Section 4.4 4.4.1.
ElasticPlastic Bending
Pure Bending of Prismatic Beams
General Concepts A straight bar is said to be in a state of pure bending if the end sections are subject to normal tractions whose resultants are equal and opposite moments about an axis perpendicular to the longitudinal axis of the bar. It
230
Chapter 4 / Problems in Contained Plastic Deformation
follows from equilibrium requirements that the stresses on every transverse section add up to the same moment (constant bending moment). In practice a condition of pure bending can be achieved by placing a bar on symmetrically located supports, with equal overhangs of length, say, a; if equal transverse forces F are applied at the ends of the bar, then the portion between the supports is in a state of constant bending moment F a [see Figure 4.4.1(a)].
y
E
a


g
4 ?
F
a
?
F
(a)
Center of curvature C
E ((( ( ( E r ( ( ] Neutral plane J zX ( y (y ,z ) XXX 0 0 EX X (0,0) XX M E XXXXX E y X X Plane of bending EX E E E
C
(b) P/\/P/\C
Q/\\/\
1/κ
C C 9 D CC @9 D εx @ : :
[email protected] Neutral plane
(c)
Figure 4.4.1. Pure bending: (a) possible beam geometry and loading; (b) local geometry in the crosssection plane; (c) local geometry in the plane of bending. If the bar is prismatic (of uniform crosssection, in terms of both geometry and material properties) and sufficiently long in comparison with crosssectional dimensions, then it can be assumed, as with the cylinder discussed in Section 4.3, that the stresses are independent of the longitudinal coordinate, except in the vicinity of the end sections. Let this coordinate be denoted x; then the preceding assumption, as well as the equilibrium equations and the boundary conditions of zero traction on the lateral surface, is satisfied if σx = σ(y, z),
Section 4.4 / ElasticPlastic Bending
231
with all other stress components equal to zero. If the moment components about the y and zaxes are My and Mz , respectively, then equilibrium is satisfied if Z
Z
σ(y, z) dA = 0, A
Z
zσ(y, z) dA = My ,
−
A
yσ(y, z) dA = Mz . A
(4.4.1) Since every crosssection of the bar has the same stress distribution, it can be expected to have the same strain distribution as well. When the strain components are infinitesimal and independent of x, three of the compatibility conditions (1.2.4) reduce to ∂ 2 εx ∂ 2 εx ∂ 2 εx = = = 0, ∂y 2 ∂z 2 ∂y∂z so that the longitudinal strain εx must be of the form a + by + cz, with a, b and c constant. It will be written as εx = −κ[(y − y0 ) cos α + (z − z0 ) sin α].
(4.4.2)
Here (y0 , z0 ) are the coordinates of the intersection of the crosssection with a fiber that does not elongate (a neutral fiber ), α is the angle between the plane of bending and the xyplane, and κ is the curvature (the reciprocal of the radius of curvature) of the neutral fibers in the plane of bending. For an illustration of the geometry, see Figure 4.4.1(b) and (c). The identical vanishing of the shear stresses τxy and τxz implies, if the material properties are isotropic, the vanishing of the corresponding strains γxy and γxz , so that the displacements satisfy ∂v ∂u + = 0, ∂x ∂y
∂w ∂u + = 0. ∂x ∂z
Consequently, ∂2v ∂2u ∂εx = − =− = κ cos α, 2 ∂x ∂x∂y ∂y ∂2w ∂2u ∂εx = − =− = −κ sin α. 2 ∂x ∂x∂z ∂z Combining, we find that κ=
∂2 (v cos α − w sin α). ∂x2
The quantity in parentheses is the displacement of a fiber from its reference position in the plane of bending. Supposing this to be the xyplane (α = 0), we may write κ = ∂ 2 v/∂x2 . Strictly speaking, the curvature of the bent fiber is given by ∂ 2 v/∂x2 , [1 + (∂v/∂x)2 ]3/2
232
Chapter 4 / Problems in Contained Plastic Deformation
and consequently the infinitesimaldeformation theory is valid as long as the slope of bent fibers with respect to the longitudinal axis is small, or, equivalently, as long as the radius of curvature remains large compared with the length of the bar.
Elastic Bending If the bar is made of a single linearly elastic material with Young’s modulus E, then Equation (4.4.2) can be combined with the stressstrain relation σx = Eεx to give σ(y, z) = −Eκ[(y − y0 ) cos α + (z − z0 ) sin α].
(4.4.3)
It is convenient to place the origin of the yzplane at the centroid of the crosssection, that is, Z Z y dA = z dA = 0. A
A
Inserting (4.4.3) into the first of Equations (4.4.1) yields y0 cos α+z0 sin α = 0 as the equation governing the coordinates of the neutral fibers — that is, they lie in the plane (the neutral plane) that is perpendicular to the plane of bending and that contains the centroidal fiber. Equation (4.4.3) can accordingly be simplified to σ(y, z) = −Eκ(y cos α + z sin α).
(4.4.4)
It is also convenient to make the y and zaxes the principal axes of area, that is, Z yz dA = 0. A
Inserting (4.4.4) into the remaining Equations (4.4.1) leads to My = −EIy κ sin α, where
Z
Iy =
2
z dA, A
Mz = EIz κ cos α, Z
Iz =
(4.4.5)
y 2 dA
A
are the principal second moments of area (often called the principal moments of inertia) of the crosssection. The inclination of the bending plane is given, from (4.4.5), by tan α = My Iz /Mz Iz . The bending plane is perpendicular to the moment vector, whatever that may be, if Iy = Iz ; this equality occurs whenever the crosssection has two or more nonperpendicular axes of symmetry, as in the case of a circle or a regular polygon (equilateral triangle, square, etc.). Otherwise, the moment vector is normal to the bending plane only if it is itself directed along a principal axis, that is, if My = 0 or Mz = 0.
Section 4.4 / ElasticPlastic Bending
233
Combining Equations (4.4.4) and (4.4.5) gives the stress distribution σx = −
M z y My z + . Iz Iy
(4.4.6)
All the preceding results are valid as long as the extreme values of the stress given by (4.4.6) remain in the elastic range. More generally, we may assume a nonlinear stressstrain relation σ = f (ε). The function f , with the righthand side of (4.4.2) as its argument, defines σ(y, z), which when inserted in (4.4.1) furnishes three coupled, nonlinear equations for the parameters κ, α, and y0 cos α + z0 sin α, the last of which is the displacement between the neutral plane and the centroidal axis. Coupled nonlinear equations are generally difficult to solve. A simplification is achieved if the bending is symmetric.
Symmetric Bending An axis of symmetry is necessarily a principal axis of the crosssection. Let the section be symmetric about the yaxis, and let My = 0, Mz = M . Then α = 0, and Equations (4.4.5)–(4.4.6) simplify to M = EIκ, σx = −M y/I, where I = Iz , in the elastic range. However, symmetry alone dictates α = 0, independently of material properties, and this condition may be assumed to hold under nonlinear material behavior as well. With the stressstrain relation σ = f (ε) as above, the parameters κ and y0 are governed by Z
Z
f (−κ(y − y0 )) dA = 0,
A
f (−κ(y − y0 ))y dA = −M.
(4.4.7)
A
If y0 can be eliminated between these equations, then the result is the momentcurvature relation M = Φ(κ).
(4.4.8)
Doubly Symmetric Sections An even greater simplification is achieved if the zaxis, also, is an axis of symmetry and if the stressstrain relation is the same in tension and compression, that is, if f is an odd function. In that case y0 = 0 by symmetry, and the function Φ is given explicitly by Z
Φ(κ) =
f (κy)y dA. A
Consider, for example, a bar of rectangular section of width b and depth 2c (so that I = 2bc3 /3), made of an elastic–perfectly plastic material. The elastic momentcurvature relation and stress distribution are valid as long
234
Chapter 4 / Problems in Contained Plastic Deformation
as σmax = 3M /2bc2 ≤ σY , or M  ≤ ME , where ME = 2σY bc2 /3 is the initial yield moment. When M > ME , the elastic relation σ = −Eκy holds at values of y at which this quantity does not exceed σY in magnitude, that is, for def y ≤ y ∗ = σY /Eκ; this range forms the elastic core. The plastic zones are −c < y < −y ∗ and y ∗ < y < c, where σ = σY sgn κ and σ = −σY sgn κ, respectively; the stress distribution is shown graphically in Figure 4.4.2(a). Because of symmetry, the moment is given by M = −2b
Z
"
c
Z
y∗
Z
2
y dy + σY sgn κ
σy dy = 2b Eκ 0
0
#
c
y∗
y dy .
Upon integration and substitution for y ∗ , this becomes "
1 M = MU sgn κ 1 − 3
κE κ
2 #
,
κ > κE ,
(4.4.9)
where κE = σY /Ec is the absolute value of the curvature corresponding to M  = ME , and MU = σY bc2 is the ultimate moment which is attained asymptotically as κ → ∞. The momentcurvature relation given by (4.4.9) is shown in Figure 4.4.2(b), and is quite similar to the torquetwist relation (4.2.4) for an elastic–perfectly plastic shaft of solid circular crosssection. The difference is that while the ratio TU /TE between the ultimate and initial yield torques is 4/3 in the torsion of a circular shaft, in the bending of a rectangular beam the corresponding ratio MU /ME , known as the shape factor , is 3/2. M y
y c
c MU
y∗
@ @ −σY
σY
@ @ @ @ −y ∗ −c
ME σ
σY
−σY
κ
κE
(a)
(b)
−c
(c)
Figure 4.4.2. Elasticplastic beam: (a) stress distribution; (b) momentcurvature relation; (c) ultimate stress distribution. Suppose, now, that the material workhardens according to the law (2.1.4), with 0 < n < 1; the limiting cases n = 0 and n = 1 represent perfect plasticity and unlimited elasticity, respectively. The momentcurvature
σ
Section 4.4 / ElasticPlastic Bending
235
relation can easily be shown to be "
κ n κE ME M= sgn κ 3 − (1 − n) 2+n κE κ
2 #
,
κ > κE ,
(4.4.10)
where κE = σE /Ec, ME = 2σE bc2 /3. Note that there is no ultimate moment when n > 0. Elasticplastic momentcurvature relations analogous to (4.4.9) can be found for other doubly symmetric sections, although the integration often gets cumbersome. It is fairly easy, however, to determine the ultimate moment and hence the shape factor. In the limit as κ → ∞, the stress distribution becomes as shown in Figure 4.4.2(c), that is, consisting of two blocks of constant stress of value σY and −σY , respectively, each distributed over onehalf the area, and statically equivalent to equal and opposite forces of magnitude σY A/2, each acting at the centroid of the halfarea. The ultimate moment is therefore 1 MU = σY Ad, (4.4.11) 2 where d is the distance between the centroids of the halfareas. Since ME = σY I/c, where c is onehalf the depth, the shape factor is Acd/2I. The quantity 21 Ad is often called the plastic modulus of the section and denoted Z. For a bar of solid circular crosssection with radius c, we have I = πc4 /4, A = πc2 , and d/2 = (4/3π)c; hence the shape factor is 16/3π ≈ 1.7. For a thinwalled circular tube of wall thickness t, I = πc3 t, A = 2πct, and d/2 = (2/π)c, so that MU /ME = 4/π ≈ 1.27. As a rule, the shape factor is greater the more material is concentrated near the center, and the smaller (closer to 1) the more material is concentrated near the extreme fibers. For rolled structural shapes, typical values are near 1.2 for Ibeams and between 1.1 and 1.15 for wideflange beams. The ideal sandwich beam (or ideal Ibeam) discussed in 3.5.1 has a shape factor of 1. The momentcurvature relation for such a beam is (
M=
EIκ, κ ≤ MU /EI, MU sgn κ, κ ≥ MU /EI,
(4.4.12)
analogous to the torquetwist relation for a thinwalled circular tube, discussed in 4.1.1.
Sections Without Double Symmetry For sections without symmetry about the zaxis the determination of a momentcurvature relation is more complicated, since y0 as a function of κ must first be found from the first of Equations (4.4.7) and then inserted in the second. For an elastic–perfectly plastic material it is easy, however, to find the asymptotic value of y0 in the limit of infinite curvature, since the
236
Chapter 4 / Problems in Contained Plastic Deformation
6
h
?
6 A A A √ A a = h/ 2 A A A A ? A A A b
Figure 4.4.3. Isosceles triangle: ultimate neutral plane.
neutral plane must then divide the crosssection area into equal halves, as in the case of sections with double symmetry. Unlike this special case, in general this plane does not go through the centroid. The ultimate moment is still given by (4.4.11), with d = d1 + d2 , where d1 and d2 are the distances from the centroids of each of the halfareas to the ultimate neutral plane. The relations κE = σY /Ec, ME = σY I/c, and the expression 12 Acd/I for the shape factor, are valid if c is interpreted as the distance from the centroid to the farthest fiber in the xyplane. When κ exceeds κE somewhat, a plastic zone forms on the side of the farthest fiber, but the rest of the section remains elastic as long as the magnitude of the stress at the opposite extreme fiber does not attain σY . It is only when this last condition is reached that the second plastic zone forms. The calculations are often involved. Consider, for example, an isosceles triangle of base b and height h. For a section of this shape, A = bh/2, c = 2h/3, and I = bh3 /36. To determine d, we must first find the location of the ultimate neutral plane. If the distance from this plane to the apex is a (see Figure 4.4.3), then the area of the isosceles triangle of height a and base ba/h must equal onehalf the area √ 2 1 1 of the whole √ triangle, that is, 2 ba /h = 4 bh; hence a = h/ √ 2, while d1 = a/3 = h/3 2. For a trapezoid of√height h − a = (1 − 1/ 2)h and major and minor bases b and ba/h = b/ 2, respectively, it √ can be shown that the distance from √ the centroid to the minor base is (8 − 5 2)h/6. Consequently √ d = 2(2− 2)h/3, and the shape factor is easily calculated to be 4(2− 2) ≈ 2.34. The elasticplastic solution for the isosceles triangle can be found, for example, in Nadai [1950], Volume I, page 358.
Unloading and Residual Stresses Consider a symmetrically bending elasticplastic beam whose momentcurvature relation has the general form M = Φ(κ), of which (4.4.9), (4.4.10) and (4.4.12) are special cases. Suppose, in particular, that initial loading has produced a curvature κ0 . If the moment M = Φ(κ0 ) is removed, then
Section 4.4 / ElasticPlastic Bending
237
the residual stress distribution can be calculated on the assumption that the unloading is elastic, that is, stresses equal to Φ(κ0 )y/I are added to those produced by the initial loading. The assumption is justified if the resulting stresses are in the elastic range. The springback, described by the change in curvature, is likewise elastic, and given by −Φ(κ0 )/EI. The residual curvature, which defines the permanent deformation of the beam, is κres = κ0 −
Φ(κ0 ) . EI
If, for example, the momentcurvature relation is (4.4.10), the ratio of residual to initial curvature is (if κ0 > 0) "
1 κE κres =1− 3 κ0 2+n κ0
1−n
−
κE κ0
3 #
.
(4.4.13)
In the perfectly plastic case (n = 0), half of the curvature is recovered when κ0 = 2.88κE . The calculation of residual stresses is particularly simple for doubly symmetric sections, since there is then no need to find y0 , and the residual stresses are given by y σres = Φ(κ0 ) − f (κ0 y). I A typical residualstress distribution is shown in Figure 4.4.4. Note that the y (mm)
60 40 @ @ 240 @ −240 @ @ @ −40 −60
y (mm)
+ σ (MPa)
60
% % 40 % % % σ 204.5 306.7 % % % % % −60
y (mm)
= (MPa)
60 % % 40 E E E −35.5 E 66.7 E E −40 % % −60
σ (MPa)
Figure 4.4.4. Residualstress distribution in an elastic–perfectly plastic rectangular beam. stresses near the center of the section keep their sign, while near the extreme fibers the loading is reversed. If the material is perfectly plastic, then the residual stresses at the extreme fibers are ±(1 − M/ME )σY . Reverse yielding can occur only if the shape factor is greater than 2, a condition unlikely to occur in doubly symmetric sections.
238
Chapter 4 / Problems in Contained Plastic Deformation
Asymmetric Plastic Bending When the moment is not perpendicular to an axis of symmetry, the elasticplastic solution becomes exceedingly difficult even for a simple crosssection. The initial yield condition can be determined by finding, for given My and Mz , the maximum absolute value of the righthand side of (4.4.6) and equating it to σY , a procedure that gives a relation between My and Mz . For a rectangle, this relation is Mz  +
2c My  = ME b
if ME is defined for symmetric bending in the xyplane as before; the relation is represented by the rhombus shown in Figure 4.4.5(a). The fully plastic condition can be studied according to the following procedure, illustrated in Figure 4.4.5(b). y My Ultimate neutral
0 =(b/h)M MU U
Ultimate yield locus
(b/h)ME "b
" b " b
"
b b
" " b b
b "ME
" "
b
MU
Mz
b "Initial b "yield b" locus
r plane B β BMB B) B B B Oα B B z Bd B Br B * BN Centroids
of halfareas (a)
(b)
Figure 4.4.5. Asymmetric plastic bending: (a) initial and ultimate yield loci for a rectangular beam; (b) ultimate neutral place and centroids of halfareas. The ultimate neutral plane is assumed to form an angle α with the zaxis. Since this plane divides the crosssection into two equal areas, its location can be determined by geometry, as can the locations of the centroids of the halfareas. If the distance between these centroids is once more denoted d, then the magnitude of the fully plastic moment is again σY Ad/2. It must be kept in mind, however, that d depends on α. The line joining the centroids of the halfareas forms an angle β with the yaxis, which depends on α. The moment vector is perpendicular to this line, and its components are, if the halfarea below the neutral plane is in tension, 1 My = − σY Ad sin β, 2
1 Mz = σY Ad cos β. 2
Section 4.4 / ElasticPlastic Bending
239
Since both d and β depend on α, the preceding equation forms a parametric representation, in terms of α, of a closed curve in the My Mz plane called the interaction diagram. For a rectangle of width b and depth h, it can be shown that !
h b2 d cos β = 1 − 2 tan2 α , 2 3h
d sin β =
b2 tan α, 3h
tan α ≤
h b
and !
b h2 d sin β = 1 − 2 cot2 α , 2 3b
h2 d cos β = cot α, 3b
tan α ≥
h . b
It is easy to eliminate α between the expressions for My and Mz to obtain the interaction relation directly. If we define MU = σY bh2 /4 as before, MU0 = σY b2 h/4 = (b/h)MU , my = My /MU0 , and mz = Mz /MU , then the relation is given by the two equations
my 3 ≤ 1, mz  + m2y = 1, 4 mz
my 3 ≥ 1. my  + m2z = 1, 4 mz
and
The relation is represented by the outer curve of Figure 4.4.5(a). The interaction curves for many other sections with double symmetry are found to lie fairly close to this curve.
4.4.2.
Rectangular Beams Under Transverse Loads
EndLoaded Cantilever: Elastic Solution The elastic theory of beams under transverse loads has its origin in SaintVenant’s research on the bending of a prismatic cantilever carrying a concentrated force F = jFy + kFz at its free end. SaintVenant began by assuming that Equation (4.4.6) for the longitudinal stress σx remains valid, along with σy = σz = τyz = 0. If the beam spans 0 < x < L, with x = 0 denoting the builtin end, the moment acting on the crosssection at x is (L − x)i × F, or Mz = (L − x)Fy , My = −(L − x)Fz . Since σx depends on x, equilibrium requires the presence of shear stresses τxy , τxz , independent of x, that satisfy Z
Z
τxy dA = Fy , A
τxz dA = Fz . A
Since the problem is linear, it may be treated as a superposition of the two problems corresponding to Fz = 0 and Fy = 0, and since the labeling of the principal axes as y or z is arbitrary, only one of these problems need be treated — for example, Fz = 0, Fy = F . It must be kept in mind that τxz cannot be assumed to vanish. The application of the one nontrivial
240
Chapter 4 / Problems in Contained Plastic Deformation
equilibrium equation to the stresses, and of the compatibility conditions to the strains resulting from them, reduces the problem to one of solving the Laplace equation in the yzplane subject to certain boundary conditions, in addition to that of finding the stress function of the elastic torsion problem (see 4.2.2); the latter is unnecessary if the yaxis is a symmetry axis of the crosssection and is the line of action of the force, as will be assumed. Details of the theory, along with solutions for circular, elliptic, rectangular and other crosssections can be found in most books on elasticity.1 In particular, for any crosssection the deflection satisfies ∂ 2 v/∂x2 = F (L − x)/EIz , so that within the limitations of smalldeformation theory, the local momentcurvature relation is the same as in pure bending. The results for the rectangular beam show that the zaverage of τxz vanishes, while that of τxy is given by τ¯xy
1 = b
def
Z
b/2
−b/2
τxy dz =
3F 2 (c − y 2 ), 4bc2
where b and c are the width and halfdepth of the crosssection, respectively, as before. Moreover, the shear stresses τxy become independent of z in the limit of both infinitely narrow (b/c → 0) and infinitely wide (b/c → ∞) rectangles, corresponding respectively to solutions for plane stress and plane strain. For such beams, then, the stress distribution is σ=
F (L − x)y , I
τ=
F 2 (c − y 2 ), 2I
(4.4.14)
where σ = σx , τ = τxy , and I = Iz = 2bc3 /3.
EndLoaded Cantilever: ElasticPlastic Solution For the state of stress just derived, both the Mises and the Tresca yield criteria are given by Equation (3.3.5). It is not difficult to see that in the cantilever under study, the lefthand side of this equation attains its maximum wherever σ is greatest, that is, at the corners (0, ±c). Consequently, def plasticity begins when F = FE = 2σY bc2 /3L. If the load F is increased beyond this value, plastic zones develop at the top and bottom faces of the beam, spreading from the corners, as shown in Figure 4.4.6. In the plastic zones the yield criterion requires that the stresses obey σ ∂σ τ ∂τ + = 0, σY2 ∂x τY2 ∂x
σ ∂σ τ ∂τ + 2 =0 σY2 ∂y τY ∂y
in addition to the equilibrium equations ∂σ ∂τ + = 0, ∂x ∂y 1
∂τ = 0. ∂x
For example, Love [1927], Chapter 15; Timoshenko and Goodier [1970], Chapter 11; or Boresi and Chong [1987], Chapter 7.
Section 4.4 / ElasticPlastic Bending
241 F
y
3 Plastic zones Q Q
ξ
c

6
H Y H y = y∗ (x)
0
L
x
y = −y ∗ (x)
Q s Q
−c
Figure 4.4.6. Elastic and plastic zones in an endloaded cantilever. These equations can be satisfied simultaneously only if σ and τ are both constant in each plastic zone, and since τ must vanish on the top and bottom faces, it must vanish everywhere in the plastic zones, and therefore σ = ±σY . In particular, if the elasticplastic boundary at x is located at y = ±y ∗ (x), then σ = σY in −c ≤ y ≤ −y ∗ (x) and σ = −σY in y ∗ (x) ≤ y ≤ c. In the elastic core −y ∗ (x) ≤ y ≤ y ∗ (x) the ydistribution of σ is linear as in the elastic case, that is, σ = −σY y/y ∗ (x). The resultant moment about the zaxis at x is ! Z c y ∗2 2 yσ dy = σY b c − M = −b , 3 −c and since for equilibrium this must equal F (L−x), it follows that the elasticplastic boundary is given by ∗
s
y (x) =
3
c2
F (L − x) − b . σY
(4.4.15)
def
In particular, y ∗ (x) = c at x = L − 2σY bc2 /3F = L − ξ; the length ξ represents the extent of the elastic zone at the given value of F . We can accordingly write, more simply, s
y ∗ (x) = c 3 −
2(L − x) . ξ
The elasticplastic boundary shown in Figure 4.4.6 is thus given by two symmetrically located segments of a parabola whose vertex is on the extension of the beam axis beyond the builtin section. As in the case of the twisted shaft, the deformation in the plastic zone is contained by the elastic deformation as long as the elastic core is of nonvanishing thickness. The regime of contained plastic deformation ends when y ∗ (0) = 0, that is, when the vertex of the parabola reaches the builtin secdef tion of the beam. The corresponding value of the load is F = σY bc2 /L = FU , the ultimate load . When it is attained, unrestrained plastic flow may begin, taking the form of a rigid rotation of the remaining elastic region about the
242
Chapter 4 / Problems in Contained Plastic Deformation
point (0, 0), with an attendant stretching and shrinking of the xfibers in the upper and lower plastic zones, respectively. The resulting mechanism is known as a plastic hinge. Plastic hinges are used extensively in the plastic analysis of beams and framed structures under various loadings, as is shown later in this book. The preceding derivation of the ultimate load neglects the growth of the shear stress in the elastic core. In fact, since τ = 0 in the plastic zones, the transverse force must be balanced by the shear stress in the elastic core only. This shear stress has a parabolic distribution in −y ∗ (x) ≤ y ≤ y ∗ (x), with a maximum value, at (x, 0), of 3F/4by ∗ (x), so that the maximum shear stress in the beam is τmax = 3F/4by ∗ (0). As the elastic core shrinks, this maximum shear stress grows until it attains τY , when a secondary plastic zone forms. With the help of Equation (4.4.15), the value of the force F at which this occurs is found to be given by
F FU
2
+
16 F 16 − 2 = 0, 2 3β FU 3β
where β = σY c/τY L. The only positive root of the equation is F 8 = FU 3β 2
r
!
3 1 + β2 − 1 . 4
For spantodepth ratios greater than 3, we have √ c/L < 1/6, so that in a beam made of a Mises material (σY /τY = 3), β 2 will be no greater than 1/12. The secondary plastic zone will therefore not form before F = 0.985FU , and the effect of the shear stress in the elastic core on the formation of the plastic hinge may accordingly be neglected. As a further refinement we note that since the shear stress in the elastic core varies with x, a transverse normal stress σy must develop there as well. However, the effect of this stress on the criterion for the initiation of the inner plastic zone, and consequently on the ultimate load for reasonably long beams, is negligible for sufficiently great spantodepth ratios.1 In order to determine the deflection, it will be assumed that the momentcurvature relation derived for pure bending holds locally in the elasticplastic def portion of the beam as well. Letting κ = v¯00 (x), where v¯(x) = v(x, 0), and using Equation (4.4.9) with the relevant substitutions, we obtain p
1 , x < L − ξ, σ Y 3 − 2(L − x)/ξ v¯00 (x) = x Ec x > L − ξ. L− , ξ 1
For a “stubby” cantilever whose span is comparable to its depth, beam theory cannot be used; the problem of the collapse load for such a beam is studied as a limitanalysis problem in 6.1.2.
Section 4.4 / ElasticPlastic Bending
243
Note that v¯00 (0) → ∞ as F → FU ; this is consistent with the notion of a plastic hinge, since infinite curvature at a point on a curve corresponds to a slope discontinuity. Rather than determine the whole function v¯(x), we calculate only the tip deflection ∆ = v¯(L) − v¯(0) by means of the fundamental relation v¯(L) − v¯(0) =
Z
L
v¯0 (x) dx,
0
which by integration by parts becomes Z
∆=
L
(L − x)¯ v 00 (x) dx,
(4.4.16)
0
since v¯0 (0) = 0 and v¯0 (L) = 0L v¯00 (x) dx. Hence, for 2L/3 L − ξ. ξ2 p
The tip deflection is therefore ∆=−
ξ2
s
L2
σY 3 − 2 3 − 2 . Ec 4 ξ2
As ξ decreases from L (q = qE ) to seen to double.
√
2/3L (q = qU ), the deflection may be
Uniformly Loaded Simply Supported Beam A uniformly loaded beam of span 2L that is simply supported at its ends is equivalent to a uniformly loaded cantilever of length L carrying, in addition, an end load that is opposed to the distributed load and equal in magnitude to the resultant of the latter (see Figure 4.4.7). The moment distribution at any state, as well as all other quantities while the beam is completely elastic, can therefore be obtained by superposing the solutions of the two previously treated problems, with F = qL. The moment at x is 1 1 M (x) = qL(L − x) − q(L − x)2 = q(L2 − x2 ). 2 2
Section 4.4 / ElasticPlastic Bending
245
y
y
??????????????????????? g 4
x
⇐⇒
F=qL
6 ????????????
x
Figure 4.4.7. Uniformly loaded simply supported beam, equivalence with cantilever. The maximum moment occurs at x = 0 and equals qL2 /2. Consequently, qE = 2ME /L2 and, as expected, qU = 3qE /2. Whenpq > qE , the elasticplastic portion extends over 0 < x < η, where η = 1 − q/qE L, and the boundary is described by
y∗ c
2
2
− 3ρ
x L
= 3(1 − ρ),
where ρ = q/qU . The boundary is thus given by portions of hyperbolas √ whose asymptotes are y = ± 3(c/L)x. At collapse, the boundary attains the asymptotes. The curvature distribution is 1 p , x < η, 3(1 − ρ + ! ρx2 /L2 ) σY 00 v¯ (x) = 3 x2 Ec ρ 1 − , x > η. 2
2
L
The deflection is once more given by Equation (4.4.16), namely, σY ∆= Ec
"Z 0
η
L−x 3 p dx + ρ 2 3(1 − ρ + ρx2 /L2 )
Carrying out the integration and inserting η = "
1 σY 2 ∆= L √ sinh−1 Ec 3ρ
s
3ρ − 2 + 3(1 − ρ)
s
L
Z η
x2 (L − x) 1 − 2 L
!
#
dx .
p
1 − 2ρ/3L, we obtain
ρ 1 3ρ + 1 1− √ ρ+ρ− − 2ρ 3 3
s
In this case the deflection tends to infinity as ρ → 1, but remains of the order of ∆E = (5/12)σY L2 /Ec until q gets quite close to qU ; for example, ∆ ≈ 2.0∆E when ρ = 0.95.
4.4.3.
PlaneStrain Pure Bending of Wide Beams or Plates
Initially Flat Plates
#
2 1− . 3ρ
246
Chapter 4 / Problems in Contained Plastic Deformation
If the width b of a rectangular beam is considerably greater than its depth 2c, then it is better to regard is as a plate, and, in the problem of bending, replace the assumption of plane stress with that of plane strain; the assumption can be justified everywhere except near the sides z = ±b/2. The solutions to elastic problems in plane stress are formally identical to those in plane strain if the Young’s modulus E and the Poisson’s ratio ν in the planestress solution is replaced by E 0 = E/(1 − ν 2 ) and ν 0 = ν/(1 − ν), respectively; in addition, a stress σz = ν(σx + σy ) must be present in order to maintain the state of plane strain. In fact, the planestrain solutions are “exact” in the sense that all the compatibility conditions are satisfied, while in all but the simplest planestress solutions some of the conditions are violated, except in the limit of infinitely thin sheets (see, e.g., Timoshenko and Goodier [1970], Article 98). The elastic momentcurvature relation in the pure bending of a wide plate is accordingly M = E 0 κ, while the distribution of bending stress is again given by σx = −M y/I. If the stress σz = νσx is taken into account, yielding occurs wherever σx  = σY 0 , where σY 0 =
σY ,
Tresca, σY , Mises. √ 1 − ν + ν2
A similar relation relates the elasticlimit stress in plane strain, σE 0 , to σE for a workhardening material. With E replaced by E 0 and σY (or σE ) by σY 0 (or σE 0 ), the results obtained for narrow rectangular beams in 4.4.1 apply to wide plates. For example, Equation (4.4.13) for the residual curvature upon unloading holds if κE = σY 0 /E 0 c.
Initially Curved Plates: Elastic State A section of a wide plate of constant curvature, subject to a constant bending moment M , is shown in Figure 4.4.8(a). The state of stress at each point may be assumed to be independent of θ and to consist of the components σr , σθ , and σz , with σz = ν(σr + σθ ) to maintain plane strain. The only equilibrium equation is therefore (4.3.18): σr − σθ dσr + = 0. dr r Unlike the expansion of a cylindrical tube, however, the bending of a plate requires a tangential displacement uθ = v(r, θ) in addition to the radial displacement ur = u(r, θ). In view of the straindisplacement relations (1.2.1), the strainstress relations may be written as 1 ∂u = 0 (σr − ν 0 σθ ), ∂r E
u 1 ∂v 1 , 1 ∂u ∂v v + = 0 (σθ − ν 0 σr ) + − = 0. r r ∂θ E r ∂θ ∂r r
Section 4.4 / ElasticPlastic Bending
σθ a2 /M 8.0 7.755
3JJ M J
σr a2 /M 1.2 1.070 0.9
6.0
Mk
OCC C
247
b
J
J C a J
J CC
JC
JC
4.0
σr
σθ
2.0 0 1.0 −2.0 −4.0 −4.917 −6.0
0.6
1.360 1.443 1.2
1.4
0.3 1.6
b = 2a
1.8
r/a 2.0
(b)
(a)
Figure 4.4.8. Curved wide plate or bar in pure bending: (a) geometry; (b) elastic stress distribution for b = 2a. Eliminating u, v and σθ between these equations and (4.3.18) results in d3 σr 5 d 2 σr 3 dσr + + 2 = 0. 3 2 dr r dr r dr The general solution is σr = A ln r + B +
C , r2
and (4.3.18) immediately gives σθ = A(ln r + 1) + B −
C . r2
The condition that the curved boundary, r = a and r = b, is tractionfree requires that σr vanish there, that is, Ab2 ln b + Bb2 + C = 0,
Aa2 ln a + Ba2 + C = 0.
The couple M is given by M =−
Z
b
a
B b A σθ r dr = − [b2 (1 + 2 ln b) − a2 (1 + 2 ln a)] − (b2 − a2 ) − C ln . 4 2 a
Solving the three equations for A, B, and C in terms of M , we obtain the stresses M σr = 4 ∆ M σθ = 4 ∆
!
b r a2 b2 b b2 ln + a2 ln − 2 ln r a r a ! a2 b2 b b r 2 2 2 2 ln + b ln + a ln − b + a , r2 a r a
(4.4.17)
248
Chapter 4 / Problems in Contained Plastic Deformation
where 2
2 2
2 2
∆ = (b − a ) − 4a b
b ln a
2
.
The variation of the stresses with r is shown in Figure 4.4.8(b). The maximum value of σr − σθ  occurs at r = a, where it equals σθ (a). Initial yielding according to the Tresca criterion takes place when M = ME , where b k∆ 2 2 2 2b ln − b + a , ME = 2 a k being the yield stress in shear. For b = 2a, ME = 0.258ka2 .
Initially Curved Plates: ElasticPlastic State The state of stress in an initially curved plate or wide beam in plane strain under a bending moment M > ME was studied by Shaffer and House [1955]. At first the plastic zone spans a ≤ r ≤ c1 , while c1 ≤ r ≤ b is elastic. In the plastic zone the equilibrium equation (4.3.18), together with the Tresca yield condition σθ − σr = 2k and the boundary condition σr (a) = 0, gives the stresses r σr = 2k ln , a
r σθ = 2k ln + 1 . a
In the elastic region the stresses are still given by (4.4.17), but the constants A, B, and C must be determined to satisfy continuity with the plastic stresses at r = c1 , in addition to σr (b) = 0. As the moment is increased further, at a certain value, say M1 , σθ (b) attains the value −2k. For b = 2a, M1 = 0.387ka2 . When M > M1 , a second plastic zone forms in c2 ≤ r ≤ b, in which stresses are given by b σr = 2k ln , r
b σθ = −2k 1 − ln . r
The stresses in the elastic core c1 ≤ r ≤ c2 are still given by (4.4.17). The four continuity conditions for σr and σθ at r = c1 and r = c2 furnish the three constants A, B, and C, and in addition, a relation between c1 and c2 , namely, ! c22 ab 2 2 c1 1 + ln = c2 1 − ln 2 . ab c1 √ The fully plastic state is attained when c1 = c2 = ab. The ultimate moment is "
MU = 2k −
√
Z a
ab
r ln + 1 r dr + a
For b = 2a, MU = 0.5κ2 .
Z
b
√
ab
#
b k 1 − ln r dr = (b − a)2 . r 2
Section 4.4 / ElasticPlastic Bending
249
As in the thickwalled tube in plane strain, both the elastic and plastic parts of εz vanish as long as σz is the intermediate principal stress, so that σz = ν(σr + σθ ) in the plastic regions as well. In the inner plastic zone, the condition that σr < σz < σθ is (1 − 2ν) ln(c1 /a) < ν, while in the outer plastic zone the corresponding condition σθ < σz < σr is (1 − 2ν) ln(b/c2 ) < 1 − ν. Clearly, these √ conditions are satisfied at all stages if they are satisfied when c1 = c2 = ab, and the second condition is satisfied whenever the first one is, since ν ≤ 1 − ν. The results are consequently valid provided ln(b/a) ≤ 2ν/(1 − 2ν). For ν = 0.3, the limiting value of b/a is e1.5 = 4.48. The displacement field in the elasticplastic pure bending of wide bars was derived by Shaffer and House [1957] for an incompressible material and by Eason [1960a] for compressible materials. The overall change in geometry can be measured by the fractional change in the angle subtended by the bar, ∆α/α, and this is found to remain of the elastic order of magnitude until M reaches about 0.95MU , similar to the case of initially straight bars. The corresponding planestress problem was treated by Eason [1960b].
Exercises: Section 4.4 1. Find the shape factor MU /ME for the elastic–perfectly plastic Ibeam having the crosssection shown in Figure 6.2.2. 2. Find the momentcurvature relation of an elastic–perfectly plastic beam of square crosssection that is bent about a diagonal. 3. Derive Equation (4.4.10). 4. Find the momentcurvature relation analogous to (4.4.10) for a rectangular beam made of a linearly workhardening material with initial yield stress σE and workhardening modulus H. 5. Find the shape factor for an elastic–perfectly plastic Tbeam made of two equal rectangles of length d and thickness t. Calculate for d/t = 8 and for the limiting case as d/t → ∞. 6. Find the equations of the interaction diagram for pure bending of an elastic–perfectly plastic beam of ideal angle section composed of two narrow rectangles of length a and b, respectively, having the same thickness t. Sketch the diagram for b = 0.6a. 7. Derive an equation analogous to (4.4.13) for the residual curvature in the beam of Exercise 4. 8. Discuss the behavior of an elastic–perfectly plastic rectangular beam that is bent by means of a uniform bending moment to a curvature κ0 > κE , and then unloaded and reloaded by a bending moment in the
250
Chapter 4 / Problems in Contained Plastic Deformation opposite direction until plastic deformation again takes place. Plot the momentcurvature diagram.
9. Discuss the development of a secondary plastic zone due to shear stresses in a uniformly loaded cantilever beam and a uniformly loaded simply supported beam of rectangular crosssection. 10. Discuss the planestress elasticplastic solution, including the secondary plastic zone, for a simply supported beam of rectangular crosssection carrying a concentrated load at x = αL, with 0 < α < 21 .
Section 4.5
Numerical Methods
The problems discussed in the preceding sections of this chapter, for which solutions were often presented in closed form, have been extremely simple: highly regular shapes, simple boundary conditions, and idealized material behavior. Real bodies whose mechanical behavior we wish to study are rarely characterized by such simplicity. But models that approximate the behavior of real bodies involve complex computations which have become feasible only with the development of highspeed digital computers over the past thirty years. A computer can perform only a finite number of calculations in a finite time. The description of the mechanical state of a body, if it is to be achieved numerically, must therefore be defined by a finite number of variables. In the simple problems discussed in Section 4.1, stress and strain were assumed to be essentially constant throughout the body, and therefore each such problem is governed by the rate equations alone, constituting a set of one or more ordinary differential equations. For example, Equations (4.1.2) and (4.1.3) each represent a set of two coupled nonlinear ordinary differential equations. In the more general problems studied in Sections 4.2 to 4.4, stress and displacement are unknown functions of position, with the former required to satisfy the equilibrium equations and the latter related to them through constitutive relations. Knowledge of the values of these functions at all points of the body amounts to an infinity of data. For the problem to be numerically tractable, this infinity must be reduced to a finite amount. That is, the stress and displacement fields must be determined, at least approximately, by a finite number of parameters. The process whereby this reduction is accomplished is the discretization of the problem, which was discussed in general terms in 1.3.5. The discretized problem is again governed by a coupled set of nonlinear ordinary differential equations. Their number,
Section 4.5 / Numerical Methods
251
however, can be quite large, and therefore special techniques are required in order to economize on computer time. Numerical techniques of time integration of the differential equations arising in elasticplastic problems are discussed in 4.5.1. In 4.5.2 we present an overview of the most usual discretization scheme, namely, the finiteelement method (other methods are mentioned in passing). Finally, in 4.5.3 we discuss, in summary form, the combination of the two topics, that is, the formulation of finiteelement methods for elasticplastic and elasticviscoplastic continua. Matrix notation is used throughout this section, but with boldface rather than underline notation. For a columnmatrixvalued function of a columnmatrixvalued variable — say φ(ξ) — the rectangular matrix [∂φi /∂ξj ] is denoted ∂φ/∂ξ, ∂ξ φ or φξ . In particular, if φ(ξ) is scalarvalued, then ∂φ/∂ξ = φξ = ∂ξ φ is a row matrix.
4.5.1.
Integration of Rate Equations
Viscoplasticity For viscoplasticity, including viscoplasticity without a yield surface as given by the “unified” models (i.e., ratedependent behavior with internal variables), the governing equations are σ = C(ε − εi )
(4.5.1)
ξ˙ = φh,
(4.5.2)
and where φ and h are functions of (σ, ξ, T ) or of (ε, ξ, T ), and the internalvariable matrix ξ includes εi . When the temperature and the stress or strain are prescribed functions of time, the viscoplastic rate equations (4.5.2) are just a set of coupled firstorder ordinary differential equations, which may be written in matrix notation as ξ˙ = φ(ξ, t). (4.5.3) A rather general method of integrating Equation (4.5.3) is the generalized Euler method, according to which, if ξ(t) is known and ∆ξ = ξ(t + ∆t) − ξ(t), then, approximately, ∆ξ = ∆t [(1 − β)φ(ξ, t) + βφ(ξ + ∆ξ, t + ∆t)],
(4.5.4)
where ξ = ξ(t), and β is a parameter between 0 and 1 to be chosen in accordance with the solution algorithm followed. The choice β = 0 represents the forward Euler method (sometimes called simply Euler’s method),
252
Chapter 4 / Problems in Contained Plastic Deformation
one that is fully explicit in the sense that the unknown quantity ∆ξ appears only on the lefthand side of the equation. While this method is simple, the error accumulates rather rapidly unless very small time increments are used. With 0 < β ≤ 1, the procedure is implicit. In particular, the choice β = 1 represents the backward Euler method. A common choice is β = 21 , representing the Crank–Nicholson method. With β > 0, Equation (4.5.4) constitutes a set of coupled nonlinear equations for the ∆ξα . An iterative scheme is required, as a rule, in order to achieve a solution. In the direct iteration method or method of successive approximations, an initial guess ∆ξ (0) (e.g., ∆ξ (0) = 0) is made and substituted for ∆ξ in the righthand side of (4.5.4). The result of computing the righthand side is then called ∆ξ (1) , is substituted again, and so forth. The iteration stops when two successive approximations are sufficiently close, that is, when an appropriately defined magnitude (or norm) of ∆ξ (k+1) − ∆ξ (k) , denoted ∆ξ (k+1) − ∆ξ (k) , is less than some prescribed error tolerance. The magnitudesξ may be defined in a variety of ways, for example, max ξα , α
X
ξα , or
α
X
ξα2 .
α
An iteration method that usually produces faster convergence than the direct iteration method is the Newton–Raphson method. The righthand side of Equation (4.5.4) is subtracted from its lefthand side, and the result is rewritten as ψ(∆ξ) = 0, it being understood that ψ also depends on ξ, t and ∆t. The initial guess ∆ξ (0) (which may again be zero, or which may be calculated from an explicit scheme) is introduced; this is the predictor phase of the solution. Next, ψ at ∆ξ (1) is evaluated by the approximation . ψ(∆ξ (1) ) = ψ(∆ξ (0) ) + J(∆ξ (1) − ∆ξ (0) ), where J = (∂ψ/∂∆ξ)∆ξ(0) = I − β ∆t (∂φ/∂ξ)ξ+∆ξ(0) . By treating the approximation as an equality and setting ψ(∆ξ (1) ) = 0, we obtain ∆ξ (1) = ∆ξ (0) + J−1 ψ(∆ξ (0) ); this is the corrector phase. The process may be continued with ∆ξ (1) replacing ∆ξ (0) in order to produce ∆ξ (2) , and so on, until ψ(∆ξ (k) ) is sufficiently small. With a reasonably good guess for ∆ξ (0) , it is usually not necessary to recalculate J at each iteration
RateIndependent Plasticity The incremental stressstrain relations of rateindependent plasticity are σ˙ = C(ε˙ − ε˙ p ).
(4.5.5)
Section 4.5 / Numerical Methods
253
The flow equations (3.2.1) are written in matrix notation as ˙ ε˙ p = λg,
(4.5.6)
where g is the columnmatrix representation of the flow tensor with components hij , defined in 3.1.1. If f (σ, ξ) = 0 is the equation of the yield surface, then, in accordance with Equation (3.2.8), λ˙ =
1
L
< fσ C ε˙ >, f = 0,
(4.5.7)
0, f < 0,
where L is given by Equation (3.2.9), or, in matrix notation, L = H + fσ Cg, with H denoting the workhardening modulus as before. Equations (4.5.5)–4.5.7) can be combined symbolically in the form ˙ σ˙ = Cep ε,
(4.5.8)
where it must be understood that in view of (4.5.7), the elasticplastic modulus matrix Cep is a nonlinear operator, since it depends on the direction of ε˙ in addition to depending on the current state as specified by (σ, ξ, T ) or by (ε, ξ, T ) (recall that εp is included in ξ). The rate equations for ξ, ˙ ξ˙ = λh,
(4.5.9)
when combined with (4.5.7) will symbolically be written in the form ˙ ξ˙ = Λε,
(4.5.10)
where Λ is a nonlinear operator like Cep . Note that the governing equations, (4.5.5)–4.5.7) and (4.5.9), have here been chosen in their strainspace form, while the statically determinate problems studied in Section 4.1, in particular those described by Equations (4.1.2) and (4.1.3), were formulated under stress control. The reason for the choice of strain control as the basis for the development of numerical methods is twofold: first, because strain control, not being limited to workhardening materials, is more general than stress control; and second, because the strainspace formulation is naturally associated with a displacementbased spatial discretization scheme, such as the most usual versions of the finiteelement method. The predictor/corrector scheme described for the viscoplastic rate equations can be applied to rateindependent plasticity as well. An effective method consists of an elastic predictor followed by a plastic corrector. It is
254
Chapter 4 / Problems in Contained Plastic Deformation
supposed that σ and ξ (which includes εp ) have been determined with sufficient accuracy, with f (σ, ξ) ≤ 0 satisfied, at a certain value of the strain tensor ε. The elastic predictor/plastic corrector scheme is used to determine the effect of a small strain increment ∆ε: it is initially guessed that the effect is purely elastic, so that the stress will change to σ (1) = σ + C ∆ε, and the internalvariable matrix will remain as ξ = ξ (1) . For simplicity, the superscript (k) is applied to quantities evaluated at σ (k) , ξ (k) . If f (1) ≤ 0, then the elastic prediction is correct, and the process is repeated for the next strain increment. If, however, f (1) > 0, then the strain increment must include some plastic strain, and a correction must be applied to σ (1) and ξ (1) . The stress correction is ∆σ (2) = −C ∆εp(2) , and ∆εp(2) is given, in principle, by integrating 4.5.6) over the increment. In practice, it will be defined by an approximation: ∆εp(2) = ∆λ g(1) . Likewise, ∆ξ (2) = ∆λ h(1) , and ∆λ is defined so that the state defined by σ (2) = σ (1) + ∆σ (2) and ξ (2) = ξ (1) +∆ξ (2) lies on the yield surface, at least in the first approximation. To within an error that is of an order higher than the first in ∆λ, . f (2) = f (1) + (∂f /∂σ)(1) ∆σ (2) + (∂f /∂ξ)(1) ∆ξ (2) = f (1) − L(1) ∆λ, where L(1) is the value at σ (1) , ξ (1) of the quantity L defined by (3.2.9). The satisfaction of the yield criterion at σ (2) , ξ (2) , to this approximation, requires that f (1) ∆λ = (1) . L In fact, it can be shown that the state at (2) is on or outside the yield surface if the yield function f is a convex function of its arguments,1 since convexity implies [see Equation (1.5.11)] that f (2) − f (1) − (∂f /∂σ)(1) ∆σ (2) − (∂f /∂ξ)(1) ∆ξ (2) ≥ 0, and the definitions of ∆σ (2) , ∆ξ (2) , ∆λ and L reduce the lefthand side of the inequality to its first term. Usually, f (2) is close enough to zero so that this correction is sufficient. Otherwise, the plastic correction process can be repeated until the state obtained is on the yield surface to a sufficient degree of accuracy (for fairly simple yield surfaces and flow rules, the final 1 A yield function f is convex if it is, for example, of the combinedhardening type (3.3.7), with F and −k convex functions of their arguments. The convexity of F is necessary for the yield surface to be convex, while the convexity of −k means essentially that the isotropic hardening rate is at most linear.
Section 4.5 / Numerical Methods
255
state may be obtained by scaling). The next strain increment can then be applied. Under stress control, the effect of a stress increment ∆σ on the yield function is examined. If f (1) = f (σ + ∆σ, ξ) ≤ 0, then ∆ε = C−1 ∆σ, and the next increment can be applied. If f (1) > 0, then ξ is corrected by . ∆ξ (2) = ∆λ h(1) , where ∆λ = f (1) /H (1) in order that f (2) = 0. As under strain control, the correction is repeated as needed. The preceding scheme, called the returnmapping algorithm, is a generalization of the radialreturn algorithm, so called because, according to the Mises flow rule, Cg is proportional to the stress deviator s, and therefore ∆σ (2) ∝ −s(1) , that is, the stress correction is directed toward the origin of the stressdeviator space. Other predictor/corrector algorithms have been proposed, for example the initialstress algorithm of Zienkiewicz, Valliappan, and King [1969]. More generally, the elastic predictor/plastic corrector method may be thought of as a split of the elasticplastic problem into an elastic problem governed by 1 ∆εij = (∆ui ,j +∆uj ,i ), 2
∆εpij = 0,
∆ξα = 0,
and a plastic problem governed by the differential equations d σ(λ) = −Cg(σ(λ), ξ(λ)), dλ
d ξ(λ) = h(σ(λ), ξ(λ)), dλ
(4.5.11)
constrained by the yield criterion f (σ(λ), ξ(λ)) = 0,
(4.5.12)
and subject to the initial condition {σ(λ), ξ(λ)}λ=0 = {σ (1) , ξ}, where σ (1) is, as defined above, the stress tensor in the trial elastic state and ξ is the internalvariable array at the end of the preceding time step. The problem formed by Equations (4.5.11)–4.5.12) may be solved either by direct iteration or by the Newton–Raphson method. Some general methods, applicable to any yield criterion and hardening rule, have been developed, including the general closestpoint projection method and the cuttingplane algorithm (see Simo and Hughes [1988]). For example, in the closestpoint projection method, the equations of the backward Euler method for perfect plasticity with an associated flow rule, which may be written as f (σ + ∆σ) = 0, def
ψ(∆σ, ∆ξ) = ∆εp − ∆λ ∂σ f (σ + ∆σ)T = 0,
256
Chapter 4 / Problems in Contained Plastic Deformation
are linearized by means of a Newton–Raphson scheme with ∆εp = −C−1 ∆σ (since ∆ε = 0 in the corrector phase), yielding ψ (0) − [C−1 + ∆λ(0) ∂σσ f (σ + ∆σ (0) )](∆σ (1) − ∆σ (0) ) − (∆λ(1) − ∆λ(0) ) ∂σ f (σ + ∆σ (0) )T = 0 and f (σ + ∆σ (0) ) + ∂σ f (σ + ∆σ (0) )(∆σ (1) − ∆σ (0) ) = 0. These equations may be solved for ∆λ(1) and ∆σ (1) , and hence for ∆εp(1) . The accuracy and stability of integration algorithms for rate equations are discussed by Ortiz and Popov [1985].
4.5.2.
The FiniteElement Method
In statically indeterminate problems, the equilibrium equations must be solved simultaneously with the constitutive relations. When the latter are represented by nonlinear rate equations, the resulting problem is one of nonlinear partial differential equations, and must be solved numerically, that is, the differential equations must be replaced by algebraic equations, and this is accomplished by means of a spatially discretized model of the continuum, as discussed in 1.3.5.
Generalities The most commonly used spatial discretization method nowadays is the finiteelement method, originally developed as a method of analysis of complex framed structures (such as aircraft structures) in which the “elements” are simple elastic members such as truss bars, straight and curved beams, and the like. The method was soon extended to inelastic behavior and to bodies modeled by one, two, and threedimensional domains of arbitrary shape, the elements being small subdomains having a relatively simple geometry. In the case of onedimensional domain (which may be straight or curved), finite elements are necessarily line segments. In twodimensional and threedimensional domains, a particular division into subdomains is known as a finiteelement mesh, and the elements are typically polygons and polyhedra, respectively. Some meshes are shown in Figure 4.5.1. In order to maintain the simplicity of the element geometry, it may be necessary to approximate the boundary of the domain — typically, a curved boundary by one that is piecewise straight, as in Figure 4.5.1(b). Occasionally, elements with curved boundaries may be used advantageously, as for example in a domain with circular geometry, in which the elements may be partly bounded by arcs of circles [see Figure 4.5.1(c)]. Associated with each element are a number of points known as nodes, usually located on the boundary (but occasionally in the interior) of the
Section 4.5 / Numerical Methods
257
Q Q H @HH H @ @ @ @ l DD @ l D l l D l T
T
T
Q Q Q Q Q Q @ @ @
(a)
(c)
(b)
Figure 4.5.1. Finiteelement meshes: (a) general mesh; (b) approximation of curved boundary; (c) domain with circular geometry using curvilinear elements. element. The nodes usually include, at the very least, the vertices of the polygon. It is generally most convenient to use, as the generalized coordinates of the model, the values at the nodes of the functions describing the displacement field; these may simply be the nodal displacements, although in finiteelement models for beams, plates and shells the nodal rotations may be included as well. It is often convenient to include, among the nodal displacements, initially even those that are prescribed, and to eliminate them after the global formulation. A finite element is characterized, then, by its shape, by the nodes associated with it, and by the assumed variation of displacement within the element, which is described by means of shape functions or interpolation functions.1 These functions are ordinarily taken as polynomial in terms of a local set of rectilinear coordinates. The simplest finite element is one having the shape of a triangle in two dimensions, or of a tetrahedron in three dimensions, and in which the nodes are the vertices only [see Figure 4.5.2(ab)]. The variation of displacement is r "T " " " T " " " r"X X XXX
T T T XXX T XXXT Tr X (a)
Figure 4.5.2. Constantstrain elements: dimensional.
r
r r L L L L L Lr (b)
(a) twodimensional; (b) three
taken as linear. It is easy to see that the number of parameters necessary to 1
If the shape functions describing the variation of displacement in terms of the nodal displacements are the same as those describing the geometry of the element in terms of the global coordinates, then the element is called isoparametric.
258
Chapter 4 / Problems in Contained Plastic Deformation
describe the variation of each displacement component in such an element is just equal to the number of vertices. Since the partial derivatives of the displacement field are constant within the element, the strain is likewise constant, and the element is called a constantstrain element. Since the displacement in a constantstrain element varies linearly along the edges (or sides), it is continuous between adjacent elements. Furthermore, a rigidbody displacement of all the nodes produces a rigidbody displacement field in each element and therefore in the whole domain. The linear variation of the displacement also means that the strain within each element is constant, so that a combination of nodal displacements representing a global state of constant strain does in fact produce such a state. An element that meets these criteria is known as a conforming element. It has been shown that the approximate solutions obtained by successive refinements of conforming finiteelement meshes converge monotonically to the exact solution of the corresponding elasticity problem. The constantstrain element has, as its principal advantage, its simplicity. On the other hand, since the displacement field is represented by a piecewiselinear approximation, it is clear that a rather fine mesh is required in order to obtain reasonably accurate results. More refined elements permit the use of coarser meshes and thus reduce computational time and storage. Some twodimensional examples are shown in Figure 4.5.3 (while they are shown as rectilinear, they may also be curvilinear): (a) The sixnode triangular element (T6 ), with a general quadratic variation of the displacement. (b) The fournode quadrilateral element (Q4 ), with a bilinear variation of the displacement; that is, when one local coordinate is held fixed, then the variation with respect to the other coordinate is linear. (c) The ninenode quadrilateral element (Q9 ), with a biquadratic variation of the displacement.
r`` r ``` "T " C ``` " `r " T C r " C T " r " C T " r X X C T XXX CX r X XrXX T XXX XXXT Tr X Xr (a) (b)
((r E E E Er r E E E E r Er (c)
r r(((( r r
Figure 4.5.3. Higherorder twodimensional elements: (a) sixnode triangle (T 6); (b) fournode quadrilateral (Q4); (c) ninenode quadrilateral (Q9).
Section 4.5 / Numerical Methods
259
Other elements in use include the sevennode triangular element (T7 ), like T6 but with an additional node at the center, and the eightnode quadrangular element (Q8 ), like Q9 but without the central node. Each element of Figure 4.5.3 has a threedimensional counterpart: (a) the tennode tetrahedron, (b) the eightnode hexahedron, and (c) the twentysevennode hexahedron. In addition, wedgetype elements are sometimes used, as in Figure 4.5.4. Elements used for the analysis of plates and shells generally have the same shapes as the twodimensional elements of Figure 4.5.2 (flat for plates, curved for shells), but as mentioned above, the generalized coordinates may include nodal rotations in addition to nodal displacements. r X , XXXr , ,l , l , , l , r X r , X l XXr,, lr
Figure 4.5.4. Wedge element. The finiteelement method is not the only technique for the numerical solution of boundaryvalue problems in solid mechanics. An older technique is the finitedifference method; see, for example, Mendelson [1968] for its application to plasticity problems. A relatively new technique is the boundaryelement method, based on certain fundamental solutions in elasticity theory; for its application to elasticplastic bodies, see Telles and Brebbia [1979] and Maier [1983]. For torsion problems, a “cellular analogy,” in which solid shafts are idealized as multicelled structures, was developed by Johnson [1988].
Displacement Formulation The most common formulation of the finiteelement method is as a displacementbased discretization of the type discussed in 1.3.5. In order to simplify the discussion, it will be assumed that all constrained generalized coordinates are zero. Let the number of unknown nodal displacements associated with a given element be N e (in general in this section, the superscript e denotes a reference to the given element). The column matrix of these displacements will be denoted qe , and may be derived from the global nodaldisplacement matrix q by means of the relation qe = Ae q,
(4.5.13)
where Ae is an N e × N matrix. If the local description of the nodal displacements is in the same frame as the global one, then Ae is what is known as a Boolean matrix: Aemn = 1 if the mth elemental degree of freedom corresponds to the nth global degree of freedom, and Aemn = 0 otherwise.
260
Chapter 4 / Problems in Contained Plastic Deformation
For a given element occupying the subdomain Ωe , the interpolation functions φn of Equation (1.3.17), when assembled in a 3 × N e matrix, will be denoted Ne . Similarly, the functions (∇φn )S of Equation (1.3.18), when assembled in a 6 × N e matrix, will be denoted Be ; this matrix is constant in a constantstrain element. The finiteelement analogues of Equations (1.3.17)– (1.3.18) accordingly are
uh (x)
Ωe
= Ne (x)qe ,
εh (x)
Ωe
= Be (x)qe .
Here the superscript h designates the discretization, and Ωe denotes the restriction of a function to Ωe . The element internalforce matrix Qe is analogously obtained by the virtualwork method discussed in 1.3.5 as Qe =
Z
BeT σ dΩ,
Ωe
where dΩ denotes an infinitesimal element of area or volume as appropriate. In a constantstrain element, with constant material properties assumed, the stress and internal variables are also constant, so that the preceding integral reduces to a product. In a higherorder element the values of the state variables must be specified at certain points within the element known as Gauss points, and numerical integration must be carried out in terms of these values. By the principle of virtual work, QT δq =
X
QeT δqe ,
e
P
where e denotes summation over all the elements. In view of (4.5.13), the global internalforce matrix is immediately obtained as Q=
X
AeT Qe .
e
Let F denote the column matrix representing the global discretized external loads, that is, F=
X e
A
eT
"Z
eT
N
Z
f dΩ +
Ωe
∂Ωet
# eT a
N
t dΓ ,
where ∂Ωet is that portion (if there is any) of the boundary of Ωe that forms a part of ∂Rt , and dΓ is an infinitesimal (surface or line) element of such a boundary. The equilibrium equation is then Q = F.
Section 4.5 / Numerical Methods
261
For an elastic body, this equation becomes Kq = F, where K=
X
AeT Ke Ae ,
e
is the global stiffness matrix, with e
Z
K =
BeT CBe dΩ,
Ωe
being the element stiffness matrix. The corresponding equations for nonlinear continua with ratetype constitutive equations are discussed in 4.5.3.
Mixed Formulation In inelastic (and some elastic) problems it is sometimes advantageous to base finiteelement methods on a mixed formulation, in which the approximations for displacement, strain and stress are by means of distinct functions; one instance of the advantage is the treatment of incompressibility. According to this point of view, the straindisplacement relations and the constitutive relations are constraints, with the stress and strain, respectively, as the corresponding Lagrange multipliers. Consequently, these relations are to be satisfied in a weak way, rather than pointwise, and the corresponding weak forms may be derived from the Hu–Washizu principle (see Exercise 14 of Section 1.4 and Exercise 2 of Section 3.4). Since the variations δu, δε, and δσ are independent of one another, the principle furnishes three separate variational equations, written (for consistency with the rest of the present section) in matrix notation: Z
T
S
T
(σ ∇ δu − f δu) dV −
Z
taT δu dS = 0,
(4.5.14)
∂Rt
R
Z
[σ − C(ε − εi )]T δε dV = 0,
(4.5.15)
R
Z
(∇S u− ε)T δσ dV = 0,
(4.5.16)
R
where ∇S u is the appropriate columnmatrix representation of (∇u)S , and Equation 4.5.1) is assumed as the constitutive relation (εi may be replaced by εp ). Equations (4.5.14)–4.5.16) are the weak forms, respectively, of the equilibrium equations, of the stressstrain relations and of the straindisplacement relations. When the straindisplacement and stressstrain relations are enforced pointwise, the displacement formulation is recovered.
262
Chapter 4 / Problems in Contained Plastic Deformation
In the mixed finiteelement formulation, stress and strain have distinct discretizations: σ h (x) e = Se (x)ce , (4.5.17) Ω
ε (x) h
Ωe
= Ee (x)ae ,
(4.5.18)
where in general Se ! = Ee . Since the interpolations of stress and strain are in general assumed discontinuous between the elements, the variational equations (4.5.15)–4.5.16) hold for each element Ωe . Substituting (4.5.17)– 4.5.18) into (4.5.15) and 4.5.16), respectively, gives σ (x) h
Ωe
εh (x)
eT −1
e
Ωe
Z
EeT C(ε − εi ) dΩ,
= S (x)H
(4.5.19)
Ωe
= Ee (x)He−1
Z
def ¯ S u, SeT ∇S u dΩ = ∇
(4.5.20)
Ωe
where e
Z
H =
SeT Ee dΩ,
Ωe
¯ S is a discrete approximation to the operator ∇S . Equation (4.5.14), and ∇ with the aid of Equations 4.5.19)–4.5.20), now yields def
G(u, δu) =
X Z e
Ωe
where Geext =
¯ S u − εi )T C ∇ ¯ S δu dΩ − Geext = 0, (∇
Z
f T δu dΩ +
Ωe
Z ∂Ωet
(4.5.21)
taT δu dΓ.
Equation (4.5.21) is a variational equation in the displacements, to be used in place of the virtualwork equation in the discretization process discussed in 1.3.5.
4.5.3.
FiniteElement Methods for Nonlinear Continua
Nonlinear Problems: Incremental Solution As long as inertia effects can be ignored and the deformation remains infinitesimal, the discretization procedure described above can be applied in nonlinear problems when the displacement, strain, and stress fields are replaced by their respective time derivatives, that is, the velocity, strainrate, ˙ and σ. ˙ and stressrate fields v, ε, We consider a problem in which the discretized externalload matrix F is a given function of time. One approach is to insert F in the timedifferentiated equilibrium equation ˙ = F. ˙ Q
Section 4.5 / Numerical Methods
263
This equation can be integrated over a time interval ∆t to yield ∆R = ∆Q − ∆F = 0.
Viscoplastic Problems As has already been said, as the temperature goes up, the behavior of metals becomes significantly ratedependent and is therefore much better described by viscoplasticity theory (whether with or without a yield surface) than by rateindependent plasticity. In addition, it was pointed out in 3.1.2 that the solutions of problems in classical viscoplasticity under constant loads attain asymptotically the equivalent rateindependent plasticity solutions, and are often easier to achieve. To simplify the writing, the factor φ in Equation (4.5.2) is taken as unity, and the yield criterion, if any, is assumed to be embodied directly in h. The rate equations are thus ξ˙ = h(σ, ξ); (4.5.22) these equations include the flow equation ε˙ i = g(σ, ξ).
(4.5.23)
When Equation (4.5.1) is differentiated with respect to time and combined with (4.5.23), the displacementbased discretization leads to ˙ = Kq˙ − G, Q where G=
X e
A
eT
Z
(4.5.24)
BeT Cg dΩ,
Ωe
and K is the previously defined elastic global stiffness matrix. The problem, then, is to integrate Equations (4.5.22) and (4.5.24) for ξ and q, with σ given h by (4.5.1) together with ε e = Be qe , subject to the equilibrium equation Ω Q = F. As with the previously considered integration of the rate equation alone, the simplest technique is the Euler method, expressed by ∆ξ = ∆t h
(4.5.25)
∆σ = C(∆ε − ∆t g),
(4.5.26)
and where h (which includes g) is evaluated at the beginning of the time step. Applying the discretization process to Equation (4.5.26) gives ∆q = K−1 (∆F + ∆t G).
(4.5.27)
264
Chapter 4 / Problems in Contained Plastic Deformation
The method is effective only with small time increments, not only because of the accumulation of discretization error, but because roundoff error may produce unstable results — that is, small changes in the initial conditions may produce large differences in the solution after a certain time. The Euler method is conditionally stable in the sense that stability holds only if the time increment ∆t is less than some critical value ∆tcr . The generalized Euler method discussed previously has been shown to be unconditionally stable when β ≥ 12 . The initial values of h and g in Equations (4.5.25–26) are replaced by linear approximations to their values at t + β ∆t, where t denotes the beginning of the time step. These approximations are h + β(hσ ∆σ + hξ ∆ξ)
and
g + β(gσ ∆σ + gξ ∆ξ),
respectively. Hence Equations (4.5.25–26) are replaced by (I − β ∆t hξ ) ∆ξ = DT (h + βhσ ∆σ) and (I + β ∆t Cgσ ) ∆σ = C[∆ε − DT (g + βgξ ) ∆ξ] (note that the dimension of the identity matrices I in these equations is not in general the same). Eliminating ∆ξ between the two equations, we obtain ¯ ¯ ), ∆σ = C(∆ε − ∆t g where ¯ = [C−1 + β ∆t gσ + β 2 DT gξ (I − β ∆t h )−1 hσ ]−1 C ξ and ¯ = g + βgξ (I − β ∆t hξ )−1 h. g By analogy with (4.5.27), we obtain the discretized equation ¯ −1 (∆F + ∆t G), ¯ ∆q = K where ¯ = K
X
A
eT
Z
B
¯ e dΩ Ae CB
Ωe
e
and ¯ = G
eT
X e
A
eT
Z
BeT C¯ g dΩ.
Ωe
The improved accuracy and stability of the generalized Euler method is achieved at the cost of computing and inverting a new stiffness matrix at each time step. If desired, several iterations may be performed in each time step in order to improve the results.
Section 4.5 / Numerical Methods
265
ElasticPlastic Problems The finiteelement solution of elasticplastic problems has been the subject of intense development since the 1960s, and a number of different approaches have been proposed. Differences persist over such issues as the use of many constantstrain elements against fewer higherorder elements, the use of local constitutive equations in rate form against that of variational inequalities in the derivation of the discrete equations, and others. In this section a brief outline of some of the most common approaches is presented. Much of the theory can be found in textbooks such as Oden [1972] and Zienkiewicz [1977] (see also Zienkiewicz and Taylor [1989]), while computer implementation is treated by Owen and Hinton [1980]. More recent developments based on a mixed formulation are discussed by Simo and Hughes [1988]. A finiteelement model may be regarded as successful if it achieves convergence of the solutions obtained under successive refinements of the mesh. It is especially so if, in those cases where a closedform solution (or another reliable solution) is available, the convergence is to this solution. The strainspace formulation of the rate equations of plasticity permits, in principle, the application of any solution method to problems involving bodies that may be workhardening, perfectly plastic, or strainsoftening. However, the finiteelement method has been successful only for workhardening and perfectly plastic bodies. Attempts to solve problems involving strainsoftening behavior have almost invariably led to meshsensitivity, that is, lack of convergence under mesh refinement. This result should not be too surprising. Our study of uniqueness criteria (Section 3.4) showed that no such criteria exist for softening bodies (if a body is nonstandard, then it must even have some hardening). Furthermore, our discussion of the physical nature of softening behavior in 2.3.2 showed that such behavior may be caused by a localization of strain rather than by pointwise strainsoftening. Several schemes that account for localization (or a size effect) have been formulated in order to permit successful finiteelement solutions of problems involving strainsoftening bodies. Such schemes are beyond the scope of the present introductory treatment, which is consequently confined to workhardening and perfectly plastic bodies. We begin with an introduction to displacementbased methods. We suppose that the current global displacement matrix q and the current local state (σ, ξ) at each point are known.1 The constitutive relation can be taken in the form (4.5.8), and, if the sign of λ˙ is assumed to be known at all
1
Points in the present context means elements if these are constantstrain, and Gauss points in the case of higherorder elements.
266
Chapter 4 / Problems in Contained Plastic Deformation
points, then the tangent stiffness Cε is Cε =
f < 0 or λ˙ ≤ 0, 1 C − Cgfσ C, f = 0 and λ˙ > 0. L C,
A possible initial assumption is that λ˙ has the same sign at the current state as it did at the preceding state. The global tangent stiffness Kt may be defined in terms of Cε in the same way as K in terms of C, that is, Kt =
X
A
eT
Z
B Ωe
e
eT
e
Cep B dΩ Ae .
The problem of determining the state at successive discrete points in time when the externalload history is prescribed2 may be broken down, at each time point, into two phases. The first phase constitutes the rate problem: the generalized velocities are obtained from ˙ q˙ = K−1 t F,
(4.5.28)
and, with q˙ known, ε˙ may be determined from the interpolation ε˙ h e = Ω Be q˙ e , and the assumption on λ˙ may be checked. If it is verified, then the rate problem has been solved, since q˙ and ε˙ are now known, as are ξ˙ through Equation (4.5.9) or (4.5.10), and σ˙ through (4.5.5) or (4.5.8). Otherwise, an (0) iteration scheme may be used: If Kt denotes Kt evaluated on the basis of ˙ then the solution the initial assumption on λ, (k−1) −1
q˙ (k) = Kt
˙ F,
k = 1, 2, ...,
permitting the evaluation of a new distribution of λ˙ and hence the calculation (k) of a new tangent stiffness matrix Kt . The process normally converges after a small number of iterations. Once the rate problem is solved, the second phase of the solution is the determination of the state resulting from the imposition of an incremental load ∆F. An explicit method begins with ∆q(0) = K−1 t ∆F, from which ∆ε(0) is computed, and hence ∆ξ (1) and ∆σ (1) as in 4.5.1, with a single implementation of the returnmapping algorithm. In general, the incremental nodal forces ∆Q(1) resulting from ∆σ (1) do not equal ∆F, creating residual forces ∆R(1) that may be added to ∆F in the next step of the iteration, which yields ∆q(1) from the general algorithm (k) ∆q(k) = ∆q(k−1) + K−1 t ∆R , 2
(4.5.29)
It is assumed, for simplicity, that any prescribed boundary velocities are zero.
Section 4.5 / Numerical Methods
267
where the stiffness matrix Kt may or may not be modified at each iteration according to the new values of σ and ξ. In the tangentstiffness method, which is equivalent to the Newton–Raphson method, the stiffness matrix Kt is recomputed at each iteration, providing faster convergence of the iteration process at the expense of more computation at each iteration. These computation costs are reduced in the socalled modified tangentstiffness methods, in which Kt is computed only once for each load increment, for example in the first or in the second iteration. In the initialstiffness method the elastic stiffness K is used throughout the process, greatly decreasing the need for matrix inversion but increasing the number of iterations. Convergence occurs when the residual forces are sufficiently small, based on some appropriate norm. The next load increment can then be applied, and the iteration procedure can begin again.
Algorithmic Tangent Moduli When the returnmapping algorithm is used in conjunction with the tangent stiffness defined by Cε , the result is a loss of the quadratic rate of asymptotic convergence, particularly important for large time steps (Nagtegaal [1982], Simo and Taylor [1985]). A procedure that preserves the quadratic rate of asymptotic convergence replaces Cep in the expression for Kt by the socalled algorithmic (or consistent) tangent moduli, defined as follows: given an algorithm that produces ∆σ when σ, ε, ξ and ∆ε are given, or formally, if ∆σ = ∆σ(σ, ε, ξ, ∆ε), then Calg = ∂∆σ/∂∆εt+∆t . While Calg coincides with the elasticplastic tangent modulus tensor Cε in problems with only one independent stress component, it does not do so in general. For more details, see Simo and Taylor [1985] and Simo and Hughes [1988]. The definition of Calg given above is consistent with the incremental form of the equilibrium equations, ∆Q = ∆F. Other forms may be associated with the total form, Q = F, and with the mixed formulation, given by Equation (4.5.21). The derivation for the case of the mixed formulation is shown next.
Application of Mixed Formulation In the mixed formulation, the finiteelement discretization may be written as uh (x) e = Ne (x)qe , Ω S h ∇ u (x)
εh (x)
Ωe
=
= Be (x)qe ,
Ωe ¯ S uh (x) ∇
Ωe
¯ e (x)qe , =B
(4.5.30)
268
Chapter 4 / Problems in Contained Plastic Deformation
where1 ¯ e (x) = Ee (x)He−1 B
Z
SeT Be dΩ.
Ωe
Substitution of (4.5.30) into Equation (4.5.21), the reduced weak form of the equilibrium equation, gives Q=
X e
AeT
Z
¯ eT C(∇ ¯ S u − εp ) dΩ B
Ωe
for the global internalforce matrix, where εp is evaluated by integration of the rate equations. An application of the Newton–Raphson method again yield Equation (4.5.29), with the tangent stiffness matrix now given by Kt = ∂Q/∂q =
X
AeT
X e
¯ eT {∂[C(∇ ¯ S u − εp )]/∂(∇ ¯ S u)} [∂(∇ ¯ S u)/∂q] dΩ B
Ωe
e
=
Z
A
eT
Z Ωe
¯ eT Calg B ¯ e dΩ Ae , B
since ¯ e Ae , ¯ S u)/∂q = [∂(∇ ¯ S u)/∂qe ] (∂qe /∂q) = B ∂(∇ and
¯ S u − εp )]/∂(∇ ¯ S u) Calg = ∂[C(∇
t+∆t
is the tensor of algorithmic (consistent) tangent moduli obtained by differentiation of the algorithmic (discrete) flow law.
Examples As one example of the application of the finiteelement method to the solution of elasticplastic problems, we examine the thickwalled elastic– perfectly plastic cylindrical tube in plane strain, with the material assumed to obey the Mises criterion and its associated flow rules; the corresponding problem for the Tresca criterion was treated analytically in 4.3.5. If the material is plastically and elastically incompressible (Poisson’s ratio equal to onehalf), then the Mises and Tresca results coincide. Two cases are presented. In both, the ratio b/a of the outer to the inner radius is 2, and k/G = 0.003. The finite elements used are concentric rings (toroids) of rectangular crosssection, so that the mesh in any rzplane is a rectangular one; fournoded (Q4) elements are chosen for their simplicity. It was shown by Nagtegaal, Parks and Rice [1974] that in a nearly incompressible body in plane strain represented by Q4 elements, an unrealistically stiff response (“locking”) is obtained unless special precautions are taken. 1
¯ e has given the procedure the name “Bbar”. The use of the matrix function B
Section 4.5 / Numerical Methods
r0
oo
.1
oo
.
269
e3
e5
e7
e9
4 e
6 e
8 e
10 e
11
e 26
40
2 8


8

8

8

12 e 8
?

(a)
r0
.1 .2 .3
oo oo
40
e4
e7
e10
e13
e16
e19
e22
e25
e28
e31
5 6 e
8 9 e
11 12 e
14 15 e
17 18 e
20 21 e
23 24 e
26 27 e
29 30 e
32 33 e
6 ? 6 ?
          10 @ 4 each
(b)
oo
e1
e4
e7
e10
e13
e16
e19
e22
e25
0.25
6 4
r
0.50 2
5
8
11
14
17
20
23
26
? 6 4
oo
0.25 3
e
6 e
9 e
12 e
15 e
18 e
21 e
24 e
27 e
?
      
8
8 @ 1 each 8


(c)
Figure 4.5.5. Meshes used in analysis of elasticplastic cylinder: (a) coarse mesh, displacement control, equal radial displacements applied at nodes 1 and 2; (b) fine mesh, displacement control, equal radial displacements applied at nodes 1, 2, and 3; (c) fine mesh, force control, forces applied at nodes 1, 2, and 3 in the proportions shown.
270
Chapter 4 / Problems in Contained Plastic Deformation
The previously discussed Bbar procedure, in which the volume strain is independently approximated by a discontinuous interpolation, is one way out, and such a procedure is used in the present analysis. The program used is FEAP (Finite Element Analysis Program), developed by R. L. Taylor (for an introductory treatment, see Zienkiewicz [1977], Chapter 24). In the first case the cylinder is virtually incompressible (ν = 0.4999) and is analyzed under displacement control, with the radial displacement of the inner surface, u(a), monotonically increased up to 4ka/3G and then decreased until the pressure turns negative. Two meshes are used, a coarser and a finer one, shown respectively in Figure 4.5.5(a) and (b). The mesh represents a 1radian sector of the cylinder, and therefore, at each value of P P u(a) the pressure is calculated according to p = ( R)/ah, where R is the sum of the radial reactions at nodes 1 and 2 in mesh (a) and at nodes 1, 2, and 3 in mesh (b). The results of the computations are shown in Table 4.5.1 as p(a) and p(b) , respectively, and they are compared with the exact values pex obtained according to the theory of Section 4.3. The convergence is evident. Table 4.5.1. PressureDisplacement Relation for Incompressible Cylinder: Computed and Exact Values 3G u(a)/ka 1 2 3 4 3 2
p(a) /k 0.5010 0.9578 1.1973 1.3192 0.8184 0.3177
p(b) /k 0.5000 0.9562 1.1937 1.3156 0.8162 0.3160
pex /k 0.4996 0.9539 1.1928 1.3139 0.8143 0.3147
In the second case, the cylinder is analyzed under pressure control, with the mesh shown in Figure 4.5.5(c), and both compressible (ν = 0.3) and incompressible behavior are examined. For the former, the computed results for the stress distributions σr , σθ , and σz , and for the displacements u(a) and u(b), are shown for various values of c/a (where c is the radius of the elasticplastic boundary) in Figure 4.5.6, where they are compared with the numerical solution of Hodge and White [1950];1 the graph of p/k against c/a in Figure 4.5.6(d) was used to obtain c/a for the imposed values of p/k. Finally, the distributions of σz for both compressible and incompressible behavior when c/a = 1.5, and a plot of p/k against 2Gu(b)/ka for the incompressible case, are shown in Figure 4.5.7. 1
The graphs are taken from Prager and Hodge [1951].
Section 4.5 / Numerical Methods
σr /2k 0 –0.1 –0.2 –0.3 –0.4 –0.5 –0.6
271
rr rr r
r r r r r rr h c/a = r hhhh 1.8 r r r hh h h hrrhhhhhh 1.6 r rh r hhh hh hhhh r hhhhhh 1.4 h h r r r r hhhhhh 1.2 h 1.0 r r r r r r r r r
–0.7
σz /2k 0.30 0.25
rr
0.20 0.15 0.10
r r
0.05 0
1.2
1.4
1.6
r/a 2.0
1.8
(a)
r @ c/a = @ 1.8 r h hr h 1.6 (r ( 1.4 r ( 1.2 r r 1.0 r r
rrr
r
r
r r
r r
r r
r
r
–0.05
–0.8 1.0
r r r r
r r r
r
r r
r r
–0.10 –0.15
σθ /2k 1.0
–0.20 1.0
1.2
1.4
1.6
1.8
r/a 2.0
(b) 0.9
r r
0.8 0.7 0.6 0.5 0.4
r r r r r r
r r rr
r
rr r
r r
r
r
r
1.2
1.4
1.6
(c)
r r
r
1.8
2Gu/ka 5
p/k 2.5
1.6
r
0.3 0.2 1.0
r
r
r rr
r
r r
c/a =
r r r 1.8
r
1.4
1.2 1.0 r r r r/a 2.0
4 2Gu(a)/ka
r
3
r
2
r r r
0 1.0
r r
1.0
2Gu(b)/ka
r
1.2
2.0
1.5
p/k
r
1
r
0.5
1.4
1.6
1.8
0.0 c/a 2.0
(d)
Figure 4.5.6. Compressible cylinder (ν = 0.3), results of finiteelement calculations: (a)–(c) stress distributions at various values of c/a; (d) displacements of inner and outer curfaces, and internal pressure, against c/a.
272
Chapter 4 / Problems in Contained Plastic Deformation
σz /k 0.6
r r r r r
0.4
r r
r r r r
p/k 1.5
r
0.2
r
r
r r
r
1.0
r
0
r r
r
0.5
r
–0.2
1.0
1.5
(a)
r/a 2.0
0 0
1.0
2.0
2Gu(b)/ka 3.0
(b)
Figure 4.5.7. Compressible and incompressible cylinder, results of finiteelement analysis (dots) and of Hodge and White [1950] or exact analysis (curves): (a) axial stress distributions at c/a = 1.5 (dashed line, incompressible [exact]; solid line, compressible [Hodge and White]; (b) pressure against displacement of outer surface (incompressible only).
Another example is the endloaded elastic–perfectly plastic cantilever beam in plane stress, discussed in 4.4.2. Computations, based on the returnmapping algorithm for plane stress formulated by Simo and Taylor [1986], were performed with a 4 × 40 and an 8 × 80 mesh of Q4 elements, covering half the beam (above or below the middle line). Numerical and analytical results for the load–deflection relation are shown in Figure 4.5.8. Lastly, an example is given of a problem for which no analytical solution is known. Figure 4.5.9 shows the torquetwist relation for an elastic–perfectly plastic Ibeam having the crosssection shown in the figure. The computed results, due to Baba and Kajita [1982], are shown along with the ultimate torque calculated by means of the sandheap analogy (see 4.2.3). As we saw in 4.2.1, in a displacement formulation of the torsion problem the warping function ψ(x1 , x2 ) is the only unknown; fournoded rectangular elements are used, with a cubic interpolation for ψ, and with the values of ψ, ψ,1 , and ψ,2 at the nodes as the nodal variables. A comparison of the results with those obtained by the “cellular analogy” was made by Johnson [1988].
Section 4.5 / Numerical Methods
273
F/FE 1.5
+ ×
++ ××
+
+ ×
+ × + × + ×
1.0
+ Coarser mesh × Finer mesh Analytical F 40
+ ×
0.5
?
4
?6
+ ×
0.0 0.0
σY = 2 × 10−3 E
0.5
1.0
1.5
2.0
∆/∆E 2.5
Figure 4.5.8. Endloaded rectangular cantilever beam in plane stress: finiteelement and analytical results for the forcedeflection diagram.
Exercises: Section 4.5 1. Find the elasticplastic tangentmodulus tensor Cep for the solid obeying the associated flow rule with the yield function f (σ, ρ, ε¯p ) =
q
2J¯2 −
√
2/3 (σE + βH ε¯p ),
where σE , β, and H are constants, 1 J¯2 = (sij − ρij )(sij − ρij ), 2 and ρ and ε¯p are governed respectively by 2 ρ˙ ij = (1 − β)H ε˙pij , 3
p ε¯˙ =
q
2 3
ε˙pij ε˙pij .
2. (a) Formulate the radialreturn algorithm for the elasticplastic solid of Exercise 1. (b) By differentiating the algorithm, find the consistent tangentmodulus tensor, and compare with the result of Exercise 1. 3. Provide the details of the derivation of Equation (4.5.21) from Equation (4.5.14) by using the relations (4.5.19–20).
274
Chapter 4 / Problems in Contained Plastic Deformation
T /TE 4 Sandheap analogy 3
b
2
b
b
b
b
b b b b bb
b
?
4
T
1

6 12
 3
? 0
0
1
2
3
4
20
5
θ/θE
Figure 4.5.9. Torsion of an Ibeam: finiteelement results for the torquetwist diagram (Baba and Kajita [1982]). The ultimate load obtained by the sandheap analogy is shown for comparison.
Chapter 5
Problems in Plastic Flow and Collapse I Theories and “Exact” Solutions Introduction In Chapter 4 the concepts of plastic flow and plastic collapse were regarded as essentially equivalent, representing a state in which a body continues to deform under constant applied forces. In practical applications, however, the two concepts have quite different meanings. Plastic collapse describes undesirably large deformations of an already formed body (a structure) that result from excessive forces; the calculation of collapse loads of simple structures was studied in Section 4.1. The concept of plastic flow, on the other hand, is usually applied to the deliberate forming of a mass of solid (such as metal or clay) into a desired shape through the application of appropriate forces.1 It is remarkable that these two large classes of problems, of fundamental importance in mechanical and civil engineering, can be attacked by the same methodology — the theory of rigid–perfectly plastic bodies, with the help of the theorems of limit analysis. A particularly extensive body of theory, filling entire books, exists for problems of plane strain; a summary of the theory, with some applications, is presented in Section 5.1. In Section 5.2 we deal with the plastic collapse of circular plates. Apart from plastic collapse, collapse of a elasticplastic body may also be due to structural instability. Such collapse (e.g., the buckling of a column) may begin when the body is still fully elastic, and plastic deformation occurs as a part of postbuckling behavior . Buckling that follows yield is covered by the theory of plastic instability, which is treated in Section 5.3. 1
The plastic flow of soil constitutes an exception, since substantial movement of a soil mass supporting a building or forming an earth dam is generally regarded as failure.
275
276
Section 5.1
Chapter 5 / Problems in Plastic Flow and Collapse I
Plane Problems
In Section 4.3 we found the stress field in a pressurized elastic–perfectly plastic hollow cylinder in a state of plane strain by solving the equilibrium equations together with, on the one hand, the compatibility condition in the elastic region and, on the other hand, the yield criterion in the plastic region, and by satisfying the boundary conditions on the outer and inner surfaces and continuity conditions at the elasticplastic boundary. The solution is valid for all pressures up to the ultimate pressure pU . When the ultimate pressure is reached, the tube becomes fully plastic. The compatibility and continuity conditions then become irrelevant. The equilibrium equation (4.3.18) and the yield criterion now constitute equations for the two unknown stress components σr and σθ , which may be solved so that the traction boundary conditions are satisfied. For both the Mises and Tresca yield criteria (which are equivalent in plane plastic flow), the solution produces the stresses given by Equations (4.3.30)1,2 with c = b. Since the fully plastic tube problem is formulated entirely in terms of the stresses, it is often said to be statically determinate, though in a looser sense than that of Section 4.1, since it is not equilibrium (“statics”) alone that determines the stress field, but the yield criterion as well. The fully plastic torsion problem of 4.2.3 can similarly be characterized as statically determinate, since once again there is one nontrivial equilibrium equation which, together with the yield criterion, can be used to determine the two unknown stress components subject to the traction boundary conditions. The same notion of static determinacy can be applied, in principle, to a body of arbitrary shape that is assumed to be undergoing plane plastic deformation, or to be in a state of plane stress: there are, in general, three unknown stress components (σ11 , σ22 , σ12 in Cartesian coordinates) and two plane equilibrium equations, plus the yield criterion. However, static determinacy in this sense is effective in producing a unique stress field only in special cases, namely those in which (a) only traction boundary conditions are relevant, and (b) the entire body must become plastic for unrestricted plastic flow to occur. As we saw in the beam problems studied in Section 4.5, it is in general possible to have unrestricted flow in a plastic region that occupies only a part of the body, the rest of the body remaining in the elastic range and hence behaving as though it were rigid (recall, from 3.5.1, the vanishing of the elastic strain rates at incipient plastic flow). Even when the aforementioned conditions (a) and (b) are satisfied, there may occur situations in which the traction boundary are not by themselves sufficient to choose between two possible stress tensors at a point (see Figure 5.1.4, which is discussed later). Since, in the general case, some of the boundary conditions may be kinematic (velocity boundary conditions), it becomes necessary to find a
Section 5.1 / Plane Problems
277
kinematically admissible velocity field such that the strain rates derived from it obey the flow rule. Consequently, the stress and velocity problems are coupled. In the special cases where a unique stress field can be found directly, then the velocity field can be found afterwards, as was done with the warping of a fully plastic rectangular shaft (see 4.2.3). In the axisymmetric planestrain problem, the only velocity component is the radial velocity v, and the flow rule is equivalent to the incompressibility constraint dv v + = 0, dr r which may be solved to give v(r) = v(a)(a/r). If, in addition, elastic regions remain in the course of plastic flow, then a solution of the problem requires the determination of the elasticplastic boundary and of a stress field in the elastic regions which is continuous with the plastic stress field at the boundary. While this was accomplished for the beam problems of Section 4.5, it is in general an exceedingly difficult task. In many problems, the main objective is to find the load that produces plastic flow or collapse, and a complete elasticplastic solution is not necessary to achieve this objective: we know from the theorems of limit analysis (Section 3.5) that the correct critical load is obtained from a plastically and statically admissible stress field and a kinematically admissible velocity field that is associated with it in the plastic region. Thus a rigidplastic boundary may be established on a purely kinematic basis, and the plastic stress field needs to be extended into the rigid region only so that is statically and plastically admissible. With this extension, the solution becomes a complete rigid–plastic solution, usually known simply as a complete solution (Bishop [1953]). A systematic method of determining stress fields and associated velocity fields in perfectly plastic bodies obeying the Mises (or Tresca) yield criterion in plane strain was developed in the 1920s by Prandtl, Hencky, Mises and others, and generalized by Mandel [1962] to include other yield criteria and plane stress. This method, generally known as slipline theory, is discussed in the next subsection. Some applications are presented in succeeding subsections.
5.1.1.
SlipLine Theory
Shear Directions A convenient way to establish the necessary relations for the stress field in a plastic region is with the help of the definitions n = 12 (σ1 + σ2 ) and r = 12 σ1 − σ2 , as given in 3.3.4, in conjunction with the yield condition (3.3.6). We introduce the Mohr’s circle relations σ11 = n + r sin 2θ,
σ22 = n − r sin 2θ,
σ12 = −r cos 2θ,
(5.1.1)
278
Chapter 5 / Problems in Plastic Flow and Collapse I
τθ
x2
6 6
II
σ22

Ib
Yb
6
σ12
S
?b
2θ
b
S S r
nP i
S b  II
n σ11
 σθ 6 σ 12
Sb
X
?
(a)
A AA r A σ22 i θ 6  σ12 P PP n PP P q P Pr @ θ I @ σ12 @6 @  σ11 X
Y
 x1 (b)
Figure 5.1.1. First (I) and second (II) shearline directions in the (a) Mohr’scircle and (b) physical planes. where θ is the angle from the x1 axis to one of the principal shear directions, namely the one along which the maximum shear stress r is directed to the left when one is facing the outer normal (see Figure 5.1.1). This direction will be called the second shear direction, and a line having this direction locally everywhere will be called a second shear line. The other shear direction (shear line) will be called the first. When equations (5.1.1) are substituted into the equilibrium equations σ11 ,1 +σ12 ,2 = 0,
σ12 ,1 +σ22 ,2 = 0,
the resulting equations are, upon substitution of r = h(n), [1 + h0 (n) sin 2θ]n,1 −h0 (n) cos 2θ n,2 +2r(θ,1 cos 2θ + θ,2 sin 2θ) = 0, −h0 (n) cos 2θ n,1 +[1 − h0 (n) sin 2θ]n,2 +2r(θ,1 sin 2θ − θ,2 cos 2θ) = 0. (5.1.2) Equations (5.1.2) constitute a pair of nonlinear partial differential equations for n, θ. A useful method of numerical solution for these equations is the method of characteristics.
Method of Characteristics In order to understand how this method can be used to solve the system, it is simpler to consider first a single firstorder partial differential equation of the form Av,1 + Bv,2 = C, where A, B and C are functions of x1 , x2 and v. The equation can be
Section 5.1 / Plane Problems
279
multiplied by an infinitesimal increment dx1 and rewritten as B v,2 dx1 = C dx1 . A
A( v,1 dx1 +
The quantity in parentheses becomes a perfect differential dv = (v,1 ) dx1 + (v,2 ) dx2 if dx2 = m dx1 , where m = B/A. The direction defined by dx2 /dx1 = m is called a characteristic direction, and a curve that is everywhere tangent to a characteristic direction is known as a characteristic curve or simply a characteristic. Along such a curve, then, dx1 dx2 dv = = . A B C If v is known at one point of a characteristic curve, then dv can be calculated for a neighboring point on this curve, and continuing this operation allows v to be determined at all points on the curve. If v is known at all points of a curve Σ that is nowhere tangent to a characteristic, then its values may be calculated along all the characteristics that intersect Σ. If two characteristics emanating from different points of Σ should intersect at some point Q of the x1 x2 plane, then in general two different values of v will be obtained there. The point Q is therefore the locus of a discontinuity in v. Consider, now, a curve Σ that is nowhere tangent to a characteristic, and suppose that a discontinuity (jump) in v,1 or v,2 occurs at a point P of Σ. Since the only information necessary to determine the characteristic curve through P and the values of v along this curve is the value of v at P , the directional derivative of v along the characteristic will have the same value on either side of it. Consequently, if any jump in v,2 or v,1 is propagated through the x1 x2 plane, it must occur across the characteristic through P . In order to apply the method of characteristics to a system of several firstorder partial differential equations, the number of real characteristic directions at each point must equal the number of unknown variables. The system is then called hyperbolic. The system (5.1.2) is consequently hyperbolic if it has two real characteristic directions. It is called parabolic if there is one such direction, and elliptic if there are none.
Characteristics of Equations (5.1.2) In order to determine whether Equations (5.1.2) constitute a hyperbolic system, we begin by solving them for n,1 , n,2 in terms of θ,1 , θ,2 : n,1 =
−2r (θ,1 cos 2θ + θ,2 sin 2θ − h0 θ,2 ), 1 − h02
n,2 =
−2r (θ,1 sin 2θ − θ,2 cos 2θ + h0 θ,1 ). 1 − h02
280
Chapter 5 / Problems in Plastic Flow and Collapse I
Note that the solutions break down when h0 (n) = 1. Assuming that this breakdown does not occur, we attempt to determine the characteristics by assuming that, along a characteristic, dn = λ dθ. Now dn = n,1 dx1 + n,2 dx2 −2r = {θ,1 [cos 2θ dx1 + (sin 2θ + h0 ) dx2 ] + θ,2 [(sin 2θ − h0 ) dx1 − cos 2θ dx2 ]} 1 − h02 = λ dθ = θ,1 (λ dx1 ) + θ,2 (λ dx2 ). Equating the coefficients of θ,1 and θ,2 , respectively, in the second and fourth lines leads to the system of equations [(1 − h02 )λ + 2r cos 2θ] dx1 + 2r(sin 2θ + h0 ) dx2 = 0, 2r(sin 2θ − h0 ) dx1 + [(1 − h02 )λ − 2r cos 2θ] dx2 = 0, which constitute a secondorder eigenvalue problem. equation is
The characteristic
(1 − h02 )2 λ2 − 4r2 cos2 2θ − 4r2 sin2 2θ + 4r2 h02 , yielding the eigenvalues λ = ±√
2r . 1 − h02
The roots are real if and only if h0  ≤ 1; the problem is hyperbolic if h0  < 1, parabolic when h0  = 1, and elliptic when h0  > 1. Referring to the examples of the yield condition (3.3.6) discussed following its formulation, we note that the planestress problem for the Mises criterion is hyperbolic only when n < 3k/2, parabolic when n = 3k/2, and elliptic when n > 3k/2; this last condition occurs when 1 σ1 < < 2. 2 σ2 For the Tresca criterion, the problem is hyperbolic when n < k and parabolic when n ≥ k; the elliptic case does not arise. In plane strain, on the other hand, h0 ≡ 0 for both criteria with the associated flow rule when the elastic strains can be neglected, and therefore the problem is hyperbolic throughout the plastic domain. The same is true for the Mohr–Coulomb criterion with the appropriate (not necessarily associated) flow rule, since h0 = − sin φ, where φ is the angle of internal friction. More generally, for any yield criterion given by Equation (3.3.6) with h0  < 1, it is convenient to define a variable angle of internal friction, φ(n), by sin φ(n) = −h0 (n); this is just the inclination of the Mohr envelope with respect to the σaxis at the point of tangency. The eigenvalues λ are correspondingly given by ±2r sec φ.
Section 5.1 / Plane Problems
281
From the trigonometric identity tan(a + b) =
sin 2a + sin 2b cos 2a + cos 2b
we may derive the directions of the eigenvectors. The eigenvector corresponding to λ = 2r sec φ is given by dx2 /dx1 = − cot(θ − 12 φ), and will be called the first or α characteristic, while the eigenvector corresponding to λ = −2r sec φ is given by dx2 /dx1 = tan(θ + 21 φ), and will be called the second or β characteristic. In the case of the Mises and Tresca criteria in plane strain (the classical case), the characteristic directions coincide with the shear directions and are orthogonal. In general the characteristics of the two families intersect at an angle 21 π ± φ; they coalesce into a single family when φ = 12 π, that is, in the parabolic case. Defining the dimensionless variable ω by Z
ω=
cos φ(n) dn, 2h(n)
we may write the characteristic relations, following Mandel [1962], as dω = dθ along a first characteristic, dω = −dθ along a second characteristic.
(5.1.3)
Note that ω = n/2k in the classical case, and cot φ n ln 1 − tan φ 2 c
ω=−
for the Mohr–Coulomb material, yielding the preceding value in the limit as φ → 0, with c = k. If we introduce a curvilinear coordinate system α, β such that first and second characteristics are given respectively by β = constant and α = constant, then we can write the canonical equations ∂ (ω − θ) = 0, ∂α
∂ (ω + θ) = 0, ∂β
which have the general solution ω = ξ(α) + η(β),
θ = ξ(α) − η(β),
ξ and η being arbitrary functions. In the following discussion of the geometric properties of the characteristic network we shall limit ourselves to the case with φ constant — that is, the Mohr–Coulomb criterion — so that a change in θ is also a change in the direction of the characteristic. This case includes the classical case, φ = 0, and
282
Chapter 5 / Problems in Plastic Flow and Collapse I
the characteristic network is then called a Hencky–Prandtl network . Among its properties are the following: 1. Suppose that one α characteristic is straight, that is, for a given β, ∂θ/∂α = 0. It follows that ξ 0 (α) = 0, and consequently all the α characteristics are straight. Obviously, the same result holds for β characteristics. 2. Consider a pair of α characteristics, defined by β and β 0 , respectively, and a pair of β characteristics defined by α and α0 , the points of intersection being labeled A = (α, β), B = (α0 , β), C = (α, β 0 ), and D = (α0 , β 0 ), as in Figure 5.1.2. It follows from the solution above that χAC = θ(α, β) − θ(α, β 0 ) = η(β 0 ) − η(β), χBD = θ(α0 , β) − θ(α0 , β 0 ) = η(β 0 ) − η(β), and consequently the two angles χAC and χBD are equal. It can similarly be shown that χAB equals χCD . This result is due to Hencky [1923] and is known as Hencky’s theorem. In words: the angle formed by the tangents of two given characteristics of one family at their points of intersection with a characteristic of the other family does not depend on the choice of the intersecting characteristic of the other family.
D r(α0 , β 0 ) rC hh (α, β 0 ) h
( χBD (((( hhhh (((((( h( ( hhhh 0 , β) (((( h hhhh B (α r((( χAC h hhhh
(α, β)
rA
Figure 5.1.2. Characteristics of Equations (5.1.2). 3. Now take (α0 , β 0 ) in Figure 5.1.2 infinitesimally close to (α, β). If Rβ (α, β) denotes the radius of curvature of the β characteristics at (α, β) and if dsα and dsβ denote infinitesimal arc lengths along the α and β characteristics, respectively, then dsβ(AC) = Rβ (α, β)χAC = [Rβ (α0 , β) + dsα ]χBD . Since Rβ (α0 , β) = Rβ (α, β) + dRβ , it follows that dRβ = −dsα along an α characteristic. Similarly, dRα = dsβ along a β characteristic. This result is due to Prandtl [1923].
Traction Boundary Conditions Traction boundaryvalue problems may be of three types, with the construction of characteristics corresponding to each type shown in Figure 5.1.3.
Section 5.1 / Plane Problems
283
Problem 1. The boundary is nowhere tangent to a characteristic. Problem 2. The boundary is composed of characteristics of both families. Problem 3. The boundary is of mixed type.
@ X @
[email protected] [email protected] X @ XX XX
[email protected] [email protected] X X @
` ` ``` `` ` ` ``` `` ` `` ` `` ` `
(a)
AA P P P A P PP A PP PPP A P P A PP A
(b)
(c)
Figure 5.1.3. Traction boundaryvalue problems: (a) Problem 1; (b) Problem 2; (c) Problem 3. If the relation between ω and n is invertible, then the state of stress at a point is determined by (ω, θ). Referring to Figure 5.1.4, we note that, along an arc whose normal forms an angle χ with the x1 axis, the normal stress, shear stress and transverse (interior) normal stress are respectively given by σ = n + r sin 2(θ − χ),
τ = r cos 2(θ − χ),
σ 0 = n − r sin 2(θ − χ), (5.1.4)
where n and r are determined by ω. If the arc forms a part of the boundary, however, then at most σ and τ will be given there (traction boundary con√ ditions); σ 0 can then have either of the values σ ± 2 r2 − τ 2 . Usually the right value of σ 0 can be chosen by physical intuition.
HH σ h h Hh h H τ h YH H hhh σH 0 Hh hh H Yh H H h h h hhhh H H h h h h Hh H hhh hH Hh jH hhh H h H y hhh h Hh h H θ Yχ
Figure 5.1.4. Stresses at a boundary. In the classical case, the two choices for σ 0 give the respective explicit expressions for θ and ω 1 τ θ = χ ± cos−1 , 2 k
σ 1 ω= ± 2k 2
s
1−
τ2 . k2
284
Chapter 5 / Problems in Plastic Flow and Collapse I
Stress Discontinuities An arc such as that of Figure 5.1.4 may also be located in the interior of the plastic domain and be part of a line of stress discontinuity. To satisfy equilibrium, σ and τ must be continuous across such a line, but ω (and therefore n) and θ are discontinuous, so that the directions of the characteristics of each family change abruptly. In the general case r is also discontinuous, 0 but in the classical case r equals k and √ is therefore continuous; σ then takes 2 2 each of the two possible values ±2 k − τ on either side of the discontinuity line. Note that there is no discontinuity if and only if τ  = k, that is, if the arc is along a characteristic (which in the classical case is a shear line). When τ  < k, θ changes by cos−1 (τ /k). It can be seen from a Mohr’scircle construction that the line of stress discontinuity must bisect the angles formed by the characteristics of each family on either side of it. It can also be seen that if the discontinuity line is thought of as the limit of a narrow zone of continuous but rapid change in σ 0 while σ and τ remain constant, all the intermediate Mohr’s circles must be of radius less than k, showing that this zone is elastic and that the discontinuity line is therefore the remnant of an elastic zone (just like the ridge lines in the torsion problem). As a result of this property, it was shown by Lee [1950] that a line of stress discontinuity acts like an inextensible but perfectly flexible filament. If the two regions separated by a line of stress discontinuity are denoted 1 and 2, and if the inclination of the line is χ, then σ and τ as given by the first two Equations (5.1.4) are continuous across this line. Specializing to the classical case, with n = 2ωk and r = k, leads to 2ω1 + sin 2(θ1 − χ) = 2ω2 + sin 2(θ2 − χ), cos 2(θ1 − χ) = cos 2(θ2 − χ). These equations may be solved for θ2 and ω2 in terms of θ1 and ω1 , yielding the jump conditions due to Prager [1948]: θ2 = 2χ − θ1 ± nπ,
ω2 = ω1 ± sin 2(θ1 − χ),
(5.1.5)
n being an integer, and the appropriate sign being taken as indicated by the problem. It was shown by Winzer and Carrier [1948] that if several straight lines of stress discontinuity separating domains of constant stress meet at a point, then these lines must number at least four. Winzer and Carrier [1949] also discussed stress discontinuities between fields of variable stress. The preceding arguments can be carried over from the classical to the general case (see Salen¸con [1977]). In particular, the jump conditions may be written directly in terms of the variables in Equations (5.1.4), n1 + r1 sin 2(θ1 − χ) = n2 + r2 sin 2(θ2 − χ), r1 cos 2(θ1 − χ) = r2 cos 2(θ2 − χ).
(5.1.6)
Section 5.1 / Plane Problems
285
Velocity Fields If a traction boundaryvalue problem is solved by constructing a characteristic network, as described above, over a part of the region representing the body, then the loading forms an upper bound to that under which plastic flow becomes possible, since, as will be shown below, a kinematically admissible velocity field can then be found. As mentioned before, the exact flow load is found when the stress field can be extended in a statically and plastically admissible manner into the rigid region. The following discussion will be limited to the classical case; for a more general discussion, see, for example, Salen¸con [1977]. The equations governing the velocity components v1 , v2 are found by combining the associated flow rule, ε˙11 ε˙22 ε˙12 = = , σ11 − σ22 σ22 − σ11 2σ12 with the strainrate–velocity relations ε˙11 = v1 ,1 ,
ε˙22 = v2 ,2 ,
1 ε˙12 = (v1 ,2 +v2 ,1 ) 2
and with Equations (5.1.1) to obtain v1 ,1 +v2 ,2 = 0,
v1 ,2 +v2 ,1 −2 cot 2θ v2 ,2 = 0.
(5.1.7)
The characteristics of Equations (5.1.7) are found by assuming dv1 = λ dv2 . Thus dv1 = v1 ,1 dx1 + v1 ,2 dx2 = v2 ,1 (−dx2 ) + v2 ,2 (2 cot 2θ dx2 − dx1 ) = λ dv2 = v2 ,1 (λ dx1 ) + v2 ,2 (λ dx2 ), so that the characteristic directions are the eigenvectors of the system λ dx1 + dx2 = 0, dx1 + (λ − 2 cot 2θ) dx2 = 0. The eigenvalues λ are the roots of λ2 − 2λ cot 2θ − 1 = 0, namely, (
λ = cot 2θ ± csc 2θ =
cot θ − tan θ.
For λ = cot θ we have dx2 /dx1 = − cot θ (i.e., the first shear direction) while for λ = − tan θ we have dx2 /dx1 = tan θ (i.e., the second shear direction).
286
Chapter 5 / Problems in Plastic Flow and Collapse I
We see therefore that the characteristics of the velocity equations are the same as those of the stress equations. The characteristic relations are thus dv1 = cot θ dv2 along an α characteristic, dv1 = − tan θ dv2 along a β characteristic. A plane whose coordinates are v1 and v2 is known as the hodograph plane, and a diagram in this plane showing the velocity distribution is called a hodograph. If P and Q are two neighboring points in the x1 x2 plane (the physical plane) lying on the same shear line, and if P 0 and Q0 are the points in the hodograph plane representing the respective velocities, then as shown by Geiringer [1951] and Green [1951], it follows from the characteristic relations that the line element P 0¯Q0 is perpendicular to P¯Q. Consequently the Hencky–Prandtl properties apply to the hodograph as well. A rigid region, if it does not rotate, is represented by a single point in the hodograph plane. It is also instructive to express the characteristic relations in terms of the velocity components along the characteristic directions, given respectively by vα = v1 sin θ −v2 cos θ and vβ = v1 cos θ +v2 sin θ. The relations were derived by Geiringer [1931] and are known as the Geiringer equations: dvα = vβ dθ along an α characteristic, dvβ = −vα dθ along a β characteristic.
(5.1.8)
It can be seen that these relations express the condition that the longitudinal strain rates ε˙11 and ε˙22 vanish when the x1 and x2 axes coincide locally with the characteristic directions, in other words, that the shear lines are inextensible. This result also follows directly from the flow rule, since with respect to such axes we have σ11 − σ22 = 0. It must be remembered, however, that the flow rule actually gives only the ratios among the strain rates, and the preceding result must strictly be written as ε˙11 /ε˙12 = ε˙22 /ε˙12 = 0. Another interpretation of this result is that ε˙12 is infinite, meaning that either v1 ,2 or v2 ,1 is infinite. This happens if the tangential velocity component is discontinuous across a characteristic (the normal component must be continuous for material continuity), that is, if slip occurs. The characteristics are thus the potential loci of slip and are therefore also called slip lines. Kinematically admissible velocity fields with discontinuities across slip lines are often used in the construction of solutions. In particular, slip may occur along a characteristic forming the boundary between the plastic and rigid regions. If slip occurs along an α characteristic, with the tangential velocity having the values vα and vα∗ on either side of it, then, since vβ has the same value on both sides, an application of Equation (5.1.8)1 along the two sides of the slip line gives dvα = dvα∗ , or d(vα∗ − vα ) = 0. An analogous result applies to a β characteristic. Thus the discontinuity in the tangential velocity
Section 5.1 / Plane Problems
287
remains constant along a slip line. It follows further that the curves in the hodograph plane that form the images of the two sides of a line of velocity discontinuity are parallel.
5.1.2.
Simple SlipLine Fields
A great many practical problems can be solved by means of slipline fields containing straight slip lines. As we have seen, if one slip line (characteristic) of a given family is straight, then all the slip lines of that family must be straight. Families of straight slip lines, as can be seen in Figure 5.1.5, may be of three types: (a) parallel, (b) meeting at a point, and (c) forming an envelope. b A A A AA A A A A AA A AA A A A A A A A A AA A (a)
EA EA E A E A E AA E (b)
b b l b l b el b Le l bb b L e ll L e L e (c)
Figure 5.1.5. Families of straight slip lines: (a) constantstate field; (b) centered fan; (c) noncentered fan with envelope. (a) If all the slip lines of one family are straight and parallel, then those of the other family must be likewise. Since θ is constant, it follows from Equations (5.1.3) that ω is constant as well, and therefore that the state of stress is uniform. A region in which the slip lines are of this type is called a region of constant state; this term is taken from wavepropagation theory and is not strictly applicable here, because, while the stress components are constant, the velocity components are not necessarily so; Equations (5.1.8), with dθ = 0, yield the solutions vα = f (β), vβ = g(α). The functions f and g are arbitrary except as constrained by boundary conditions. (b) If the slip lines of one family are straight and meet at a point, then those of the other family must be concentric circular arcs. Such a system of slip lines is called a centered fan. A number of problems may be solved by inserting a centered fan between two regions of constant state, in such a way that the bounding radial lines of the fan are also the bounding parallel lines of the constantstate regions. ω is constant along all the straight lines, while along the circular arcs of the fan, dω = ±dθ, depending on whether the arcs are α or β characteristics. If the θ difference between the two constantstate regions is ∆θ, then this is just the angle subtended by the bounding lines of the fan, and ∆ω = ±∆θ. (c) An envelope of slip lines is also called a limiting line, and a family
288
Chapter 5 / Problems in Plastic Flow and Collapse I
of straight slip lines forming an envelope is called a noncentered fan; the envelope is called the base curve of the fan. A limiting line cannot be in the interior of the plastic region, and therefore must form a part of either the boundary of the body or of the rigidplastic boundary. Other properties of limiting lines are discussed by Prager and Hodge [1951], Section 25.
Some Applications We now consider some simple applications of slipline fields consisting of constantstate regions and centered fans, illustrated in Figure 5.1.6. These results are of considerable importance in soil mechanics, where they are used to study the stability of slopes and the carrying capacity of foundations made of clays for which the hypothesis of constant shear strength (the undrained strength discussed in 2.3.1) can be justified. (a) Consider, first, a wedge of angle 2γ with a uniform pressure on one side and no traction on the other. A possible shearline net consists of two regions of constant state, separated by a line of stress discontinuity bisecting the wedge. With the principal stresses 2k − p, −p on one side and 0, −2k on the other, continuity of the normal stress across the discontinuity line is possible only if p = 4k sin2 γ. This value is therefore a lower bound to the pressure causing incipient plastic flow. As can be seen in Figure 5.1.6(a), when the wedge is acute (γ < 14 π) a velocity field may be constructed such that regions ABC and AEF slip along the slip lines AB and AF , respectively, while ACDE flows perpendicular to the stressdiscontinuity line AD, so that slip also occurs along AC and AE. The material below BAF may be rigid. (b) When the wedge is obtuse (γ > 41 π) no such velocity field is possible. On the other hand, it is now possible to insert a centered fan of angle 2γ − 12 π between two constantstate regions, producing the pressure p = 2k(1 + 2γ − 1 π), which exceeds the previously obtained lower bound for all γ > 14 π. 2 (c) Now consider a truncated wedge with pressure on the top face. At each corner we can construct a plastic zone consisting of a centered fan between two triangular regions of constant state, and plastic flow can occur when the two plastic regions meet, so that the top face can have a downward velocity. The angle subtended by each fan is just γ, so that p = 2k(1 + γ). (d) The limit of the preceding case as γ → 21 π represents a halfplane carrying a rigid block, and therefore the limiting pressure on the interface between the halfplane and the block is k(2 + π). This result was obtained by Prandtl [1920] by assuming a single triangular region of constant state under the block, with a centered fan on either side and another constantstate region outside each fan [see Figure 5.1.6(f)]. Prandtl’s solution was criticized by Hill, who pointed out that, since the elastic solution of the problem leads to infinite stresses at the corners of the block, plastic zones must be there from the outset. As the pressure is increased, these zones will
Section 5.1 / Plane Problems
D A B A B P PAr r E B C B A P p B P P B BP A P B P A P BP P A B B B B BP P B A B A PP P PA F B Rigid AA jγ
289
p BHH P H P H P B B P P HH PP P B BB B P P U P B HH γ PP BBBBB P Rigid
(b)
(a)
p ??????????? A @ @ @ @ B
[email protected] @ HB @ H γ@ A B AA * H Rigid H HBB (c)
@ @ @
@ @ @
@
@ @
@
@ @
Rigid
(d)
p A
????? B S A A S S AH O S H HH S HH D SC 66666666 6 6 6 6 6 6 6 66 q (e)
@ @ @ @
[email protected] @ @ @
[email protected] @ @ @ @ @ @
[email protected] @ @
[email protected] @ @ @ L @ L @ L L Rigid
(f)
Figure 5.1.6. Simple slipline fields: (a) acute wedge; (b) obtuse wedge; (c) truncated wedge loaded on the top edge; (d) rigid block on a halfplane, Hill solution; (e) finite truncated wedge, discontinuous stress field; (f) rigid block on a halfplane, Prandtl solution.
290
Chapter 5 / Problems in Plastic Flow and Collapse I
grow until they meet, as in case (c). In the last two examples, no stress field outside the plastic regions has been presented, so that the resulting pressures must be regarded as upper bounds only. For example (c), Drucker and Chen [1968] have shown how to construct a statically admissible stress field, leading to a lower bound equal to the upper bound on the pressure. The following example shows that for a finite truncated wedge, a lower pressure than that obtained in (c) above can be found. (e) A solution for a finite truncated wedge, uniformly loaded on its top and bottom faces, is based on a fully plastic stress distribution, with the four triangular constantstate regions separated by the stressdiscontinuity lines OA, . . . , OD, which bisect the angles at the corners. In order for these bisectors to meet at one point, the ratio of the bottom to the top face of the trapezoid must be (1+sin γ)/(1−sin γ). Because of symmetry, only the right half of the wedge need be considered. Since the flank BC is tractionfree, region 2 is in a state of simple compression parallel to BC, and the values of θ and ω there are θ2 = γ + π/4 and ω2 = − 12 , respectively. In region 1, by symmetry, θ = θ1 = π/4. By Equation (5.1.5)2 , ω1 = − 21 − sin γ. Equation (5.1.1)2 then gives, in region 1, σy = −2k(1 + sin γ) = −p, where p is the pressure on the top face; note that this value is less than that obtained in (c) above. The pressure on the bottom face can similarly be found as q = 2k(1 − sin γ). It can be seen that the aforementioned geometric restriction is necessary for equilibrium.
Problems with Circular Symmetry In classical problems with axial symmetry, the slip lines are along the shear directions and therefore at 45◦ to the radial and tangential directions. They are therefore given by logarithmic spirals, r ∝ e±θ . These slip lines can be used to construct velocity fields in hollow prisms with a circular bore under internal pressure. In Figure 5.1.7, for example, an axisymmetric stress field — the same as in the hollow cylinder under internal pressure — is assumed in the region inside the largest circle, with a vanishing stress field outside this circle. Plastic flow is assumed to occur only in the curved triangular regions bounded by the slip lines that meet the sides of the square at their midpoints. The remaining regions move diagonally outward as rigid bodies. A statically admissible stress field and an associated kinematically admissible velocity field are thus found, and the pressure must be that for the cylinder, namely, p = 2k ln b/a.
Section 5.1 / Plane Problems
291
b
b


P i PP
Slip lines
a
B BN
0
Figure 5.1.7. Hollow prism with a circular cutout.
5.1.3.
MetalForming Problems
A number of problems representing metalforming processes can be solved approximately by means of the theory of plane plastic strain, if the metal is idealized as a material that is rateindependent and rigid–perfectly plastic, and if the thermal stresses that result from the temperature gradients induced by the forming process can be neglected. In a metalforming problem — unlike a structural problem — unrestricted plastic flow is the desired condition. The solution is intended to furnish the smallest applied force under which the metal will flow, rather than the largest load under which the structure will not collapse. For this reason an upper bound to the force is a “safe” answer. Metalforming processes that closely approximate planestrain conditions (and for which slipline theory can be used to generate upper bounds on the forming forces) include forging, indentation, and cutting of wide strips, as well as continuous processes such as extrusion, drawing and rolling. In problems representing the latter category of processes, it is not the initiation of the process that is studied, but a state of steady plastic flow in which a large amount of plastic deformation has already taken place, and the stress and velocity fields are taken as constant in time in an Eulerian sense, much as in steadyflow problems of fluid mechanics. An extensive bibliography of slipline fields for metalforming processes can be found in Johnson, Sowerby and Venter [1982]. Many examples are also to be found in Johnson and Mellor [1973], Chapters 11 and 14, and Chakrabarty [1987], Chapters 7 and 8. Only a few selected problems will be
292
Chapter 5 / Problems in Plastic Flow and Collapse I
treated here.
Indentation The problem of the halfplane carrying a rigid block, illustrated in Figure 5.1.6(d), can also be interpreted as describing the beginning of indentation of a halfplane by a flat punch. The Hill solution, which requires slip between the plastic zones and the punch, implies smooth contact. In the Prandtl solution, on the other hand, the triangular region directly under the punch moves rigidly downward with it, corresponding to rough contact. This material in this region is often called dead metal . The solution shown in Figure 5.1.6(c) for the truncated wedge of halfangle γ with uniform pressure on its top face can be adapted to the problem of indentation by a flat indenter at the bottom of a flat trench (Figure 5.1.8) if γ is replaced by π − γ. The indentation pressure is thus p = 2k(1 + π − γ).
Tγ? T C T X X C X T X X X @ C @
[email protected] @ @ @ C C @ π−γ
Figure 5.1.8. Flat indenter at the bottom of a flat trench. A solution for the frictionless indentation of a halfplane by an acute wedgeshaped indenter of halfangle α (α < π/4) was proposed by Hill, Lee and Tupper [1947]. This problem is one of pseudosteady plastic flow , in which the geometry of the slipline field (and therefore the stress and velocity fields) changes as penetration proceeds, but in a geometrically similar manner — that is, the angles remain the same, and only the scale changes. As shown in Figure 5.1.9, the slipline field covers Zone 1. Zone 3 is that in which the material is elastic and therefore treated as rigid, while the intermediate Zone 2 contains material that has yielded but is restrained from moving. As can be seen, the solution allows for the piling up of material (the formation of a “coronet”) about the indenter, although in practice such piling up is observed only in workhardening materials. The angle θ subtended by the centered fan between the two constantstate triangles can be determined from the wedge halfangle α by means of the condition that the volume of piledup material (shown as shaded in the figure) equals the volume of that portion of the indenter that has penetrated the work (shown crosshatched). The slipline field is equivalent to that in Figure 5.1.6(b), with θ = 2γ − π/2, and therefore the contact pressure q is q = 2k(1 + θ).
Section 5.1 / Plane Problems
293
J
ppp` pppppppp ppppppppppppppp α A B ppppppppppppp pppp pJ ``` ppppppppppppppppppp ppppppppppppppppppppppppp 3 Q k ppppppppppppppppppppppppppppppp ppppppppppppppppppppppppppppppppppppp p p pQ p p p p p p p pppppppppQ pppppppppppppppppppppppppp
pp ppJ ppppp+
` D J J Q ` Q Q
J Q
J `
D J Q Q Q
JJ1 J D Zone DD J 3 ` Q `` ` D H J
θ P ` hZone 2 ( Zone 3
Figure 5.1.9. Indentation of a halfplane by an acute wedgeshaped indenter. The indenter force, at a given state of indentation, is thus F = 4k(1 + θ)AB. Because of geometric similarity, the indenter force is consequently proportional to indentation depth.
Forging and Cutting The simultaneous application of identical flat punches to a strip of finite thickness, Figure 5.1.10(a), may be used to model forging, with the bottom punch representing the anvil and the top punch the forging tool. Similarly, the cutting of a strip of metal with a wirecutterlike tool can be described as the simultaneous indentation by a pair of identical wedgeshaped indenters located opposite each other [Figure 5.1.10(b)]. Because of symmetry, in each case only the top half of the strip needs to be considered, and the middle plane may be regarded as a frictionless foundation. The solution of both problems was studied by Hill [1953].
?
? TT`
6
`TT 6
(a)
(b)
Figure 5.1.10. Forging and cutting: (a) forging; (b) cutting. For the cutting problem Hill showed that when the plastic region has not yet reached the foundation, the slipline field is the same as for the
294
Chapter 5 / Problems in Plastic Flow and Collapse I
semiinfinite domain. When, however, the plastic region extends through the thickness of the strip, a different mode of deformation takes over: piling up ceases, and the material on either side of the plastic region moves rigidly outward; the slipline field is shown in Figure 5.1.11(a).
? TT`
6 
`TT 6 (a)
2h
?
? ............... .............. ............. ............ ........... .......... ......... ........ ....... ...... ..... .... ... @ .. @. AA AA

... ... .... ..... ...... ....... ........ ......... .......... ........... ............ ............. .............. ...............
@ @ 6 2a(b)
Figure 5.1.11. Slipline fields: (a) forging; (b) cutting. For the forging problem, the slipline field is shown in Figure 5.1.11(b). A triangular deadmetal region attaches itself to the punch, and indentation proceeds as in the cutting problem, provided that h < 8.74a, where h is the halfthickness of the strip and a the halfwidth of the punch. When h = 8.74a, it can be shown that the punch pressure is p = 2k(1 + π/2), as for the semiinfinite domain. It follows that for h > 8.74a the zone of plastic deformation does not go through the strip and the pressure remains at this value.
Drawing and Extrusion Drawing and extrusion are processes in which a billet of material is forced to flow through a die shaped to produce the required crosssection. In drawing, as the name suggests, the material is pulled. Extrusion involves pushing. In direct extrusion the die is stationary with respect to the container holding the billet, and a ram moves in the container, pushing the billet outward with the help of a pressure pad. In reverse extrusion the container is closed at one end, and the die is pushed inside the container. The three processes are shown in Figure 5.1.12. The technologically important applications of these processes are predominantly threedimensional — drawing produces wire, and extrusion is used to make lightweight structural shapes, trim and the like. In the absence of threedimensional solutions, however, the solutions of the corresponding plane problems provide qualitative information on the nature of the plastic regions and hence allow estimates for the required forces. Figure 5.1.13(a) illustrates a solution due to Hill [1948c] describing frictionless extrusion through a square die with 50% reduction. The slipline field consists the two centered fans OAB and OA0 B 0 ; because of symmetry,
Section 5.1 / Plane Problems
295
Die holder ........................................... ................................................... .......................................................... ................................................................................ ................................................................................ ................................................................................. ................................................................................. ................................................................................ ................................................................................. ................................................................................ ................................................................................. ................................................................................ ................................................................................. ................................................................................ ................................................................................ ................................................................................ .............................................................. ........................................................ ....................................................
@ R
[email protected] JJJJJJJ .............................
[email protected] .............................. ............................. ............................. .. .............................. ............................. .............................. ........................................................ ........................................................ ........................................................ ........................................................ ........................................................ ........................................................ ........................................................ ........................................................ .............................. ............................. .............................. ............................. .............................. ............................. .............................. ............................. ..............................

XX Die y
JJJ
JJJ
Extruding metal
Container +
.... @ @ @ @ @ @ @ .... @ @ @
[email protected] @ @ @ @ @ @ @ I @ A @ Ram A A
Die
Pressure pad
(a)
(b) Container + @ Closure plate @ ......................... @ .. ......................... ......................... ......................... @ .. ......................... ......................... @ ......................... ......................... + ............................................................... ............................................................... ............................................................... @@ ............................................................... @ ............................................................... ............................................................... ............................................................... ......................... ......................... @ ......................... ......................... @ ......................... .. .........................
[email protected] @ ........................... @@
@@
@@ Die (c)
Figure 5.1.12. Drawing and extrusion: (a) drawing; (b) direct extrusion; (c) reverse extrusion.
only OAB need be considered. Since the exit slip line OA is a line of constant stress, σ11 must vanish identically on it in order for the extruded metal to its left to be in equilibrium, and σ12 = 0 because the line forms an angle of 45◦ with the xaxis. The yield criterion requires σ22  = 2k, and, since the sheet is being compressed, it follows that σ22 = −2k. Equations (5.1.1), with n = 2kω and r = k, accordingly require that ω = − 12 and θ = π/4 on OA. The characteristic relations can now be used to determine the state along AB. Since the fan subtends 90◦ , θ = 3π/4, and Equation (5.1.3)2 shows that ω = 21 (1 + π) there. By Equations (5.1.1), then, we have σ11 = −(2 + π)k, σ22 = −πk, and σ12 = 0 on AB. The average value of −σ11 along OAB is thus equal to the extrusion pressure,
p= 1+
π k. 2
A statically admissible extension of the stress field into the rigid region due to Alexander [1961] shows this to be the exact pressure, not merely an upper bound. The stress field on OB is extended into the deadmetal region ABC, while that on OA is extended into OAP ; the extruded metal to the left of AP is stressfree, so that AP is a line of stress discontinuity. The extension to the right of the arc OB is achieved analytically. A simple slipline field for a reduction of 32 is shown in Figure 5.1.13(b),
296
Chapter 5 / Problems in Plastic Flow and Collapse I
.......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... ........................................................................................................................... .......................................................................................................................... ................................... ........................................................................................................................... ............................................................. .......................................... .......................................... C B .......................................... .......................................... ....... .......................................... ............................................................... (2+π)k .......................................... .......................................... .......................................... .................... . .......................................... πk ............................................................... .......................................... ....... ............................................................... .......................................... .......................................... ........................................................ ....... . ....................... .............................................................. .......................................... .................... . A ............................................................... .......................................... ....... ............................................................... .......................................... .......................................... ....... ............................................................... 0 .......................................... ....... O . P 2k .............................................................. .......................................... .......................................... .......................................... .......................................... ........................................................ ........................................................ .......................................... .......................................... .......................................... ....... ............................................................... A.0.. . .......................................... . . . ............................................................. .......................................... .......................................... ........................................................ .......................................... .......................................... ................................... .......................................... ................................... .......................................... .......................................... .......................................... .......................................... .......................................... ................................... ................................... .......................................... .......................................... .......................................... 0 ....... .......................................... C 0 B . . . ................................... . . . ........................................................................................................................... . . . . . . ........................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... .......................................................................................................................... ..........................................................................................................................
? 6 (((( ( ( Ph ( h H @Hhhhhh @HHH @ H ? @ H 6 @
........................................................................... ........................................................................... ........................................................................... ........................................................................... ........................................................................... ........................................................................... ........................................................................... ........................................................................... ........................................................................... ........................................................................... ........................................................................... ...... ............................................................................ ........................................................................... ........................................................................... ............................................................................ .............................................................. ............................................................... .......................................... .......................................... .......................................... ....... ............................................................... .......................................... ................................... .......................................... ................................... .................... . .......................................... ............................................................... .......................................... ....... ............................................................... .......................................... .......................................... ........................................................ ....... . .............................................................. ........................................................ .......................................... .......................................... ................................. .......................................... ..................... .......................................... ......... .......................................... ....... ............................................................... .......................................... .......................................... ....... ............................................................... .......................................... .......................................... .......
@ @
@
@
@
@ @
@ @
(b)
(((( ( ( ( h Hhhhh hh @HH @ HH @ H H @ @
(a)
Figure 5.1.13. Extrusion: (a) frictionless extrusion through a square die with 50% reduction; (b) slipline field for twothirds reduction. and leads to an extrusion pressure of 4 π 1+ k. 3 2
p=
Figures 5.1.14(a) and (b) illustrate both drawing and extrusion through a tapered die. If the container walls in the extrusion problem are smooth, then the slipline fields are identical if the die angle α and the reduction ratio r are the same; the stress fields in the regions covered by the slipline field differ only by a hydrostatic stress. A particularly simple slipline field due to Hill and Tupper [1948], valid for a smooth die when r = 2 sin α/(1 + 2 sin α), is shown in Figure 5.1.14(c). In the extrusion problem, ω and θ on the exit slip line OA are the same as in the preceding problem, and therefore their values in the constantstate region ABC are ω = − 21 (1 + 2α), θ = π/4 + α. The normal pressure on AC is q = (1 − 2ω)k = 2(1 + α)k, and the tangential stress there is zero. For equilibrium, the extrusion pressure p must be 4(1 + α) sin 2α k. p = rq = 1 + 2 sin 2α
Section 5.1 / Plane Problems
297 ..............................................
..............................................
............................................. ............................................. .................................................... ............................................. .............................................. ............................................. ............................................................... ...." " .................................... . ..............." ." . . . .... . . " ................ .................................... . . . ..............." ........................ .." .. ." ........................ ........................ .... .................................... ........................
............................................. ............................................. .................................................... ............................................. .............................................. ............................................. ............................................................... ...." " . ..............." ." . . . . . " ................ . . . ..............." " ..." ..
........................ .... .................................... ......... ........................ ................ ........... . .............. .................................... ............ ............ ...................... . ....................................................... . .... ............................................. .............................................. ............................................. .................................................. ............................................. ............................................. .............................................
......... ................ .............. ............ ............ ....................................................... ............................................. .............................................. ............................................. .................................................. ............................................. ............................................. .............................................
b bb bb b b b
b bb bb b b b
(a)
(b)
............................................................................ ........................................................................... ........................................................................... ....................................................................................... ........................................................................... ........................................................................... ............................................................................ ................... ....................... C . . . α ................... ◦ .................. 45 ................... ............. .......... 45◦
" "" 6 "" w"" r "" ? " X
[email protected] B α @ 45◦@ 6
6
1
?
O
CC b bb b b b
......... ................ .............. .......... ...
(c)
Figure 5.1.14. Drawing and extrusion through a tapered die: (a) drawing; (b) extrusion; (c) slipline field for drawing and extrusion through a smooth tapered die with r = 2 sin α/(1 + 2 sin α) (Hill and Tupper [1948]. The corresponding drawing problem is solved by superposing a hydrostatic tension equal in magnitude to this pressure. The drawing stress therefore has the same value as the extrusion pressure. For further solutions of metalforming problems using slipline theory, see the aforementioned references by Johnson and Mellor [1973], Johnson, Sowerby and Venter [1982], and Chakrabarty [1987].1 Additional plane problems, in which complete solutions are not available, are discussed in Section 6.1 in the context of limit analysis.
Exercises: Section 5.1 1. For a Hencky–Prandtl network in which the values of ω − θ on any two neighboring first characteristics and the values of ω + θ on any two neighboring second characteristics differ by the same small constant, show that the diagonals of the network are lines of constant ω or of constant θ (use Figure 5.1.2). 1
Finiteelement methods for metalforming problems are treated by Kobayashi, Oh, and Altan [1989].
298
Chapter 5 / Problems in Plastic Flow and Collapse I
2. Show that when four straight lines of stress discontinuity meet on an axis of symmetry of stress field and separate four regions of constant stress, as in Figure 5.1.6(e), the angles AOD and BOC must be right angles. 3. Show that any velocity field that is associated with the stress field of the preceding exercise represents rigidbody motion. 4. Derive the Geiringer equations (5.1.8). 5. Find the differential equations for the velocity field in plane plastic flow in a standard Mohr–Coulomb material. Determine the characteristics of the velocity field. 6. Show that in classical problems of plane plastic flow with axial symmetry, the slip lines are given in polar coordinates by r ∝ e±θ . 7. Show that the relation between θ and α in the slipline field of Figure 5.1.9 is 1 π θ −1 α= θ + cos tan − . 2 4 2 8. The slipline field of Figure 5.1.6(c) may be regarded as representing a stage in the squashing of an originally pointed wedge of halfangle α (greater than γ) by a lubricated flat plate. (a) Using geometry and volume constancy, find the relation between α and γ. (b) Find the relation between the applied force and the distance moved by the plate. (c) Determine the smallest value of α for which the solution is valid. 9. Discuss how the slipline field of Figure 5.1.6(c) can be used to study the necking of a symmetrically notched tension specimen. 10. Discuss the velocity fields associated with the slipline fields of Figures 5.1.13(a) and (b).
Section 5.2
Collapse of Circular Plates
The goal of this section is derivation of collapse loads for axisymmetrically loaded circular plates made of a perfectly plastic material obeying the Tresca criterion. For such plates, complete solutions exist in closed form, and they are treated in 5.2.3. For the collapse loads of plates without circular symmetry, limit analysis must be used to obtain estimates, and this is done in
Section 5.2 / Collapse of Circular Plates
299
Chapter 6. The introduction to plate theory given in 5.2.1 is general, and not limited to circular plates. Similarly, the presentation of elastic relations and yield criteria at the beginning of 5.2.2 and 5.2.3, respectively, is general, but solutions will be given for axisymmetric problems only.
5.2.1.
Introduction to Plate Theory
Derivation of Plate Equilibrium Equations A plate may be defined as a solid body occupying in the undeformed configuration the region A × [−h/2, h/2], that is, the set of points {(x1 , x2 , x3 )  (x1 , x2 ) ∈ A, −h/2 ≤ x3 ≤ h/2}, where A is a closed domain in the x1 x2 plane bounded by a simple closed curve C (we are assuming no holes in the plate), with h considerably smaller than the typical dimension of A. The plane x3 = 0 is called the middle plane of the plate. The outward normal unit vector to C in the x1 x2 plane has components να (α = 1, 2), and the counterclockwise tangential unit vector has components tα . We shall approach the study of the mechanics of plates by a combined use of the threedimensional equilibrium equations and of virtual work. The plate equilibrium equations will be derived directly from the former. First, we define the stress resultants as follows: Z
Nαβ = Z
Qα =
h/2
−h/2 h/2
−h/2
Mαβ = −
Z
σαβ dx3
(membrane forces),
σα3 dx3
(shear forces),
h/2
−h/2
x3 σαβ dx3 (moments).
The surface loads are pα =
h/2 σα3 −h/2 h/2
Z
q = σ33 −h/2 + h/2
h/2
+ Z
−h/2 h/2
fα dx3 ,
f3 dx3 ,
−h/2 Z h/2
mα = −x3 σα3 −h/2 −
−h/2
x3 fα dx3 ,
where f is the body force per unit volume. Distinguishing the x3 coordinate from the xα (α = 1, 2), we write the local equilibrium equations σαβ ,β +σα3 ,3 +fα = 0,
(5.2.1)
σα3 ,α +σ33 ,3 +f3 = 0.
(5.2.2)
300
Chapter 5 / Problems in Plastic Flow and Collapse I
Integrating these equations through the thickness and performing integration by parts where necessary yields Nαβ ,β +pα = 0
(5.2.3)
Qα ,α +q = 0.
(5.2.4)
and When Equations (5.2.1) are multiplied by x3 and then integrated through the thickness, the result is Mαβ ,β +Qα + mα = 0.
(5.2.5)
We can eliminate Qα between Equations (5.2.4) and (5.2.5), and obtain Mαβ ,αβ = q − mα ,α .
(5.2.6)
Equations (5.2.3) and (5.2.4–5) or (5.2.6) are the plate equilibrium equations, the former for inplane or membrane forces and the other for bending forces. Note that the two modes of behavior — inplane deformation and bending — are statically uncoupled. In the elementary theory they are also kinematically uncoupled, and therefore can be studied separately.
Displacement Assumptions and Virtual Work The elementary displacement model for plate behavior is described by the following displacement field: uα (x1 , x2 , x3 ) = u ¯α (x1 , x2 ) − x3 w,α (x1 , x2 ),
u3 (x1 , x2 , x3 ) = w(x1 , x2 );
here the u ¯α are the inplane displacements and w is the deflection. It follows that εi3 = 0, i = 1, 2, 3, so that σij δεij = σαβ δεαβ , and εαβ = ε¯αβ −x3 w,αβ , where ε¯αβ = 21 (¯ uα ,β +¯ uβ ,α ). It is important to check whether the assumption of infinitesimal strain is valid. The Green–SaintVenant strain tensor (Section 1.2) has the inplane components 1 1 Eαβ = εαβ + uγ ,α uγ ,β + w,α w,β . 2 2 If we neglect the contributions of the inplane displacements u ¯α , then the righthand side reduces to 1 1 −x3 w,αβ + x23 w,αγ w,βγ + w,α w,β . 2 2 If δ is a typical deflection and l a typical dimension of A, then the first term is of order hδ/l2 , the second of order (hδ/l2 )2 , and the third of order (δ/l)2 . While the second term is negligible in comparison to the third whenever h/l is sufficiently small, as is normal in plate theory, for the third term to be
Section 5.2 / Collapse of Circular Plates
301
negligible in comparison to the first term it is necessary for the deflection to be small compared to the plate thickness. Otherwise, the Green–SaintVenant strain tensor must be used, given in general by ¯αβ − x3 w,αβ , Eαβ = E with
¯αβ = ε¯αβ + 1 w,α w,β . E (5.2.7) 2 Equation (5.2.7) will be used in the next section when the buckling of plates is studied. Under the hypothesis of infinitesimal strain, the internal virtual work becomes Z δW int = (Nαβ δ ε¯αβ + Mαβ δw,αβ ) dA. A
This equation may be rewritten as (1)
(2)
δW int − δW ext = δW ext , (1)
where δW ext denotes the part of the external virtual work due to the body (2) force and the surface tractions on the planes x3 = +−h/2, and δW ext is that due to applied forces and moments along the edge. The first part accordingly is given by (1) δW ext
Z "Z
= −h/2
A
#
h/2
fi δui dx3 +
h/2 (σi3 δui ) −h/2
dA.
Now fi δui = fα δ u ¯α − x3 fα δw,α +f3 δw and h/2
h/2
h/2
h/2
(σi3 δui ) −h/2 = σα3 −h/2 δ u ¯α − (x3 σα3 ) −h/2 δw,α +σ33 −h/2 δw, so that (1)
δW ext =
Z
(pα δ u ¯α + q δw + mα δw,α ) dA. A
Since Nαβ is symmetric, it follows that Nαβ δ ε¯αβ = Nαβ δ u ¯α ,β , and (1)
δW int −δW ext =
Z A
[(Nαβ δ u ¯α ,β −pα δ u ¯α )+(Mαβ δw,αβ −mα δw,α −q δw)] dA.
Now Nαβ δ u ¯α ,β = (Nαβ δ u ¯α ),β −Nαβ ,β δ u ¯α , and Mαβ δw,αβ − mα δw,α = (Mαβ δw,α ),β −[(Mαβ ,β +mα ) δw],α +(Mαβ ,αβ +mα ,α ) δw,
302
Chapter 5 / Problems in Plastic Flow and Collapse I
so that upon applying the twodimensional divergence theorem we obtain δW int −
(1) δW ext
I
=
[νβ Nαβ δ u ¯α + νβ Mαβ δw,α +να (Mαβ ,β +mα ) δw]ds
CZ
−
A
[(Nαβ ,β +pα ) δ u ¯α + (Mαβ ,αβ +mα ,α −q) δw] dA.
(5.2.8) However, by the equilibrium equations (5.2.3) and (5.2.6) the area integral vanishes. In the remaining contour integral, the expression in parentheses may be replaced by −Qα as a result of Equation (5.2.5). Moreover, the three functions w, w,1 and w,2 are not independent on C, because, if w,α is decomposed as w,α = να ∂w/∂n + tα ∂w/∂s, then the normal derivative ∂w/∂n (which represents the local rotation of the plate) can be prescribed independently of w, but the tangential derivative ∂w/∂s is entirely determined by w. Performing the aforementioned decomposition and defining Mn = να νβ Mαβ (the normal bending moment), Mnt = να tβ Mαβ (the twisting moment), and Qn = να Qα , we obtain δW int −
(1) δW ext
I
= C
∂δw ∂δw νβ Nαβ δ u ¯ α + Mn + Mnt + Qn δw ds. ∂n ∂s
By integration by parts, I
Mnt C
∂ δw ds = − ∂s
I C
∂Mnt δw ds, ∂s
and therefore δW int −
(1) δW ext
I
= C
∂w νβ Nαβ δ u ¯ α + Mn δ + Vn δw ds, ∂n
where Vn = Qn − ∂Mnt /∂s is the effective shear force along the edge. A graphic illustration of the equivalence between a varying twisting moment and a distributed transverse force may be seen in Figure 5.2.1. ? ? ? ? z } { z } { z } { z } { 6 6 6 6 6? ? ? ? ?
Figure 5.2.1. Effective shear force along a plate edge. Finally, let the applied inplane forces along the edge be Fαa , the applied bending moment (acting about the tangent to C) Mna , and the applied transverse force Vna , all per unit length. Then (2) δW ext
I
= C
Fαa δ u ¯α
+
∂w Mna δ ∂n
+
Vna δw
ds,
Section 5.2 / Collapse of Circular Plates
303
so that the boundary conditions are either νβ Nαβ = Fαa or u ¯α prescribed, ∂w either Mn = Mna or prescribed, ∂n a either Vn = Vn or w prescribed. Leaving aside the inplane forces and displacements, we see that at every point of the edge two conditions must be specified. For example, along a clamped edge the conditions are w = 0 and ∂w/∂n = 0; along a simply supported edge, w = 0 and Mn = 0; and along a free edge, Vn = 0 and Mn = 0. The condition Vn = 0 was first derived by Kirchhoff, and consequently the theory of plates that has thus far been outlined is known as Kirchhoff plate theory. In the original plate theory formulated by Sophie Germain, a free edge was assumed to be subject to the three boundary conditions Qn = 0, Mnt = 0, and Mn = 0, resulting in an improperly posed boundaryvalue problem for elastic plates. In the present treatment the principle of virtual work was used to derive the boundary conditions that are consistent with the displacement model adopted, while the equilibrium equations (5.2.3)–(5.2.6) were derived from the threedimensional ones — that is, they were shown to be necessary, but not sufficient. However, it can easily be seen that the principle of virtual work also implies the equilibrium equations (5.2.3) and (5.2.8), and as the only necessary ones: since the displacement components u ¯α , w can vary independently in A, and since the area integral in Equation (5.2.8) must vanish, it follows that the coefficients of δ u ¯α and δw must vanish. Equation (5.2.5) may then be used as the definition of Qα . Before introducing constitutive equations, it must be noted that although the displacement model is one in which ε33 = 0, this constraint is not realistic. Actually, it is the stress σ33 which is very nearly zero, or at least, its maximum value is very small in comparison to those of the stresses σαβ (α, β = 1, 2). Similarly, the shear stresses σ3α , though important in the equilibrium equations, are generally of small magnitude. Consequently, most points of the plate are nearly in a state of plane stress. The elastic behavior of isotropic plates should therefore be described by Equations (1.4.13), and plasticity by a planestress yield criterion.
5.2.2.
Elastic Plates
Elastic Relations Equations (1.4.13), σαβ =
E [(1 − ν)εαβ + νεγγ δαβ ]. 1 − ν2
304
Chapter 5 / Problems in Plastic Flow and Collapse I
lead to Nαβ =
Eh [(1 − ν)¯ εαβ + ν ε¯γγ δαβ ] 1 − ν2
and Mαβ = D[(1 − ν)καβ + νκγγ δαβ ], where D = Eh3 /[12(1 − ν 2 )] is the plate bending modulus, and καβ = w,αβ is the curvature tensor . It can be seen that the problem of the inplane forces is identical with the planestress problem, with Nαβ , Fαa , u ¯α and ε¯αβ corresponding to σαβ , Tαa , uα , and εαβ , respectively. For the flexure problem, the equilibrium equation, when combined with the momentcurvature and curvaturedeflection relations, becomes q¯ ∇4 w = , D where q¯ = q − mα ,α is the effective transverse load per unit area. In what follows we shall assume, as is the case in most problems, that mα = 0 and therefore q¯ will be replaced by q.
Axisymmetrically Loaded Circular Plates Given a circular plate of radius a, if the load q is a function (in polar coordinates) of r only and if the edge conditions are uniform, then the deflection w can likewise be assumed to be a function of r only, the only nonzero shear force is Qr = Q, and the only moments are Mr and Mθ . Equation (5.2.4) then reduces to 1 d (rQ) + q = 0, r dr which can be integrated to yield 1 Q=− r
r
Z
rq dr, 0
and Equation (5.2.5) becomes dMr Mr − M θ + + Q = 0. dr r The curvature tensor components are κr =
d2 w , dr2
κθ =
1 dw , r dr
and therefore the elastic relations take the form Mr = D
d2 w 1 dw +ν 2 dr r dr
!
,
Mθ = D
1 dw d2 w +ν 2 r dr dr
!
.
Section 5.2 / Collapse of Circular Plates
305
Substituting this result in the momentshear equations results in D
d3 w 1 d2 w 1 dw + − 2 3 2 dr r dr r dr
!
= −Q.
But the lefthand side is just dw d 1 d r D dr r dr dr
,
so that the differential equation can be solved by integration. The simplest problem is the one where the load is uniform, that is, q = constant. Then Q = −qr/2, and the integration for w results in w(r) =
qr4 + Ar2 + B ln r + C, 64D
where A, B, C are constants of integration. For the deflection to be finite at the center we must have B = 0, and it is convenient to set C = 0, that is, measure the deflection relative to the center rather than relative to the edge. The remaining constant, A, is then determined from the edge condition. Clamped Edge. Here the edge condition is w0 (a) = 0, leading to A = −qa2 /32D. The deflection of the edge relative to the center is thus qa4 /64D, or equivalently, the center deflection relative to the edge is qa4 /64D. The moments are Mr (r) =
q [(3 + ν)r2 − (1 + ν)a2 ], 16
Mθ (r) =
q [(1 + 3ν)r2 − (1 + ν)a2 ]. 16
Simply Supported Edge. We have Mr (r) =
(3 + ν)qr2 + 2(1 + ν)DA, 16
and therefore the condition Mr (a) = 0 leads to A = −(3 + ν)qa2 /32(1 + ν)D. The deflection is therefore w(r) =
q [(1 + ν)r4 − 2(3 + ν)a2 r2 ], 64(1 + ν)D
the maximum deflection being (5+ν)qa4 /64(1+ν)D, or, with ν = 0.3, about four times as large as for the clamped plate. The moments are Mr (r) =
(3 + ν)q 2 (r − a2 ), 16
Mθ (r) =
q [(1 + 3ν)r2 − (3 + ν)a2 ]. 16
As a preliminary step to determining the deflection due to an arbitrary axisymmetric load q(r), we consider the case of a force F concentrated on a
306
Chapter 5 / Problems in Plastic Flow and Collapse I
circle of radius b. This may be viewed as the limit as c → b of the annular loading 0, 0 < r < b, F q(r) = , b < r < c, 2 π(c − b2 ) 0, c < r < a. It follows that rQ is constant for r < b and for r > c (with Q = 0 in the former region), and that rQcb
=−
Z
c
q(r)r dr = −
b
F . 2π
Consequently, in the limit as c → b we have d 1 d dw r dr r dr dr
=
0,
r < b,
F , r > b. 2πDr
Denoting the deflections in r < b and r > b by w1 and w2 , respectively, and setting w1 (0) = 0 for convenience, we have w1 (r) = A1 r2 , w2 (r) = A2 r2 + B2 b2 ln
r F 2 r + C2 b2 + r ln . b 8πD b
The continuity conditions w1 (b) = w2 (b), w10 (b) = w20 (b), and w100 (b) = w200 (b) yield F F , B2 = C2 = . A2 = A1 − 8πD 8πD Thus F r 2 2 2 2 2 w2 (r) = A1 r + (r + b ) ln + b − r , 8πD b w20 (r)
F = 2A1 r + 8πD
!
r b2 2r ln + −r , b r
and in r > b, "
F r b2 Mr (r) = 2(1 + ν)DA1 + 2(1 + ν) ln + (1 − ν) 1 − 2 8π b r If the edge r = a is clamped, then w20 (a) = 0 and therefore "
F a 1 b2 A1 = − ln − 1− 2 8πD b 2 a
!#
,
!#
.
Section 5.2 / Collapse of Circular Plates
307
while if the edge is simply supported, then Mr (a) = 0 and "
F a 1−ν b2 A1 = − ln + 1− 2 8πD b 2(1 + ν) a
!#
.
These results may be combined by writing "
a b2 F ln + λ 1 − 2 A1 = − 8πD b a
!#
,
where λ equals − 21 for the clamped plate and (1 − ν)/2(1 + ν) for the simply supported plate. Since we have set w(0) = 0, the center deflection relative to the edge is a F b2 ln − (1 + λ)(a2 − b2 ) . −w(a) = 8πD b
Let the solution derived above be written as w(r) = −
F g(r, b; λ), 8πD
where, by definition, " !# a ρ2 r2 , ln ρ + λ 1 − a2 g(r, ρ; λ) = r a 2 2 2 r ln r − ρ ln ρ + (1 + λ)r −
r < ρ, 1+λ
r2 a2
!
ρ2 , r > ρ.
Now consider an arbitrary load distribution q(r). The total load contained in the infinitesimal annulus ρ < r < ρ + dρ is 2πq(ρ)ρ dρ, and consequently the deflection due to this load alone is −(1/4D)q(ρ)g(r, ρ; λ)ρ dρ. The deflection due to the entire load is obtained by superposition: w(r) = −
1 4D
Z
a
q(ρ)g(r, ρ; λ)ρ dρ, 0
and for the center deflection, in particular, we have 1 −w(a) = 4D
Z 0
a
a q(ρ) (1 + λ)(a − ρ ) − ρ ln ρ dρ. ρ
2
2
2
Consider, for example, a downward load F uniformly distributed over an inner circle of radius b; then b F a (1 + λ)(a2 − ρ2 ) − ρ2 ln ρ dρ 2 4πb D ρ " 0 ! # F a2 b2 b2 a b2 = (1 + λ) − − ln + . 4πD 2 4 4 b 16
Z
w(a) =
308
Chapter 5 / Problems in Plastic Flow and Collapse I
When b = a, we obtain w(a) = [4(1 + λ) − 1]
F a2 , 64πD
from which we obtain the previous results for the clamped and simply supported cases (with q = −F/πa2 ) by inserting the appropriate values of λ. With b = 0 we obtain the solution for a load concentrated at the center. The deflection at any r is obtained by evaluating w(r) by superposition, with r > b, and then taking the limit as b → 0: 1 F w(r) = lim · 2 b→0 4D πb
Z
b
"
0
a r r2 r ln − ρ2 ln + (1 + λ)r2 − 1 + λ 2 r ρ a 2
!
#
ρ
2
ρ dρ
a F r2 ln + (1 + λ)r2 . = 8πD r
The maximum deflection is
1, clamped, w(a) = 3+ν 16πD , simply supported. 1+ν F a2
The bending moments are F a 2(1 + ν) ln − (1 − ν) + 2(1 + ν)λ , 8π r
Mr =
a F 2(1 + ν) ln + (1 − ν) + 2(1 + ν)λ . Mθ = 8π r The logarithmic singularity at the center indicates that the assumptions of elementary plate theory do not hold near the point of application of a concentrated load. For more details, see Timoshenko and WoinowskyKrieger [1959], Section 5.1.
5.2.3.
Yielding of Plates
Plate Yield Criteria A plate will be said to yield in bending at a point (x1 , x2 ) if the stress tensor there obeys the yield criterion at every x3 except x3 = 0; points in the middle plane are regarded as remnants of the elastic core. If the stresses σi3 are assumed negligible in magnitude next to the σαβ (this does not mean that they can be neglected in the equilibrium equations, because derivatives occur there), then we may apply a planestress yield criterion, say f
σαβ σy
!
= 0,
Section 5.2 / Collapse of Circular Plates
309
in every plane x3 6= 0. Equilibrium is satisfied if σαβ = −
4 Mαβ sgn x3 . h2
(5.2.9)
If the ultimate moment is defined as MU = σy h2 /4, then the plate yield criterion is given by f (mαβ ) = 0, where mαβ = Mαβ /MU ; the Mises and Tresca criteria become, respectively, m211 − m11 m22 + m222 + 3m212 = 1 (Mises), max(m1 , m2 , m1 − m2 ) = 1
(Tresca).
A yield criterion that approximates the behavior of doubly reinforced concrete slabs is the Johansen criterion, max(m1 , m2 ) = 1. Problems in contained plastic bending of plates may be studied by means of numerical methods analogous to those of Section 4.5.1 The plastic collapse of perfectly plastic plates may in general be investigated by means of limit analysis, as is done in Section 6.4. If such plates are, however, circular and axisymmetrically loaded and supported, then exact solutions may be obtained for the collapse state.
Fully Plastic Axisymmetrically Loaded Circular Plates If the loading and support are axisymmetric, then the only nonvanishing moments are Mr and Mθ , and the equilibrium equation is (rMr )0 − Mθ =
Z
r
qr dr.
(5.2.10)
0
This equation and the yield condition constitute two equations for Mr and Mθ . Equivalently, if the yield condition is solved for Mθ in terms of Mr and the resulting expression for Mθ is substituted in (5.2.10), the result is a nonlinear firstorder differential equation for Mr (r). At the center of the plate, Mr = Mθ and consequently, if the curvature there is positive (concave upward), Mr (0) = MU constitutes an initial condition with which the differential equation may be solved. In addition, a boundary condition at the edge r = a must be satisfied; this yields the ultimate load. Let us recall that for a simply supported plate, the edge conditions are w = Mr = 0 ; thus Mr = 0 is a boundary condition with which the differential equation may be solved. For a clamped plate, the edge must form a hinge circle, 1
For an introduction to finiteelement methods for plates, see Zienkiewicz [1977], Chapter 10.
310
Chapter 5 / Problems in Plastic Flow and Collapse I
that is, a locus of slope discontinuity (a special case of the hinge curve discussed in Section 6.2). As we shall √ see, the edge condition there becomes Mr (a) = −MU or Mr (a) = −2MU / 3 for the Tresca or Mises material, respectively. Figure 5.2.2 shows the Mises and Tresca yield criteria for axisymmetrically loaded circular plates. It follows from the preceding discussion that the center of the plate is in the moment state corresponding to point B, and that a simply supported edge corresponds to point C. A simply supported plate may thus be assumed to be entirely in the regime BC. For the the Tresca material, this means that Mθ = MU everywhere, and the problem to be solved is therefore linear. Mθ
Mises = B
C
Tresca 9
A D
O
MU Mr
D0 s E Figure 5.2.2. Mises and Tresca yield criteria for axisymmetrically loaded circular plates
Solution for Tresca Plate Let us consider, for example, a downward load F uniformly distributed over a circle of radius b, the plate being unloaded outside this circle. The equilibrium equation is then
(rMr )0 − MU =
F r2 − , r < b, 2
2πb
F − ,
2π
r > b.
The solution for r < b satisfying the condition at r = 0 is Mr = M U −
F r2 , 6πb2
while the solution for r > b satisfying the condition at r = a is
Mr =
F − MU 2π
a −1 . r
Section 5.2 / Collapse of Circular Plates
311
Continuity at r = b requires that
F = 2π
MU . 1 − 2b/3a
This result includes the extreme cases F = 6πMU for the uniformly loaded plate (b = a) and F = 2πMU for a plate with concentrated load. This last case could not have been treated directly because the moments would have to go to infinity at the center —a condition incompatible with plasticity. On segment BC of the Tresca hexagon, the flow rule yields κ˙ r /κ˙ θ = 0, that is, w˙ 00 /(w˙ 0 /r) = 0. Consequently the velocity field obeying the edge condition must be w(r) ˙ = (1 − r/a)v0 , where v0 is the center velocity (i.e., the plate deforms in the shape of a cone). It is shown in Chapter 6 that the upperbound load obtained with this velocity field equals the one obtained here, as indeed it must, since the solution is complete. In order to study the clamped plate, we must know the velocity fields associated with the other sides of the Tresca hexagon. On CD we have κ˙ r + κ˙ θ = 0, that is, w˙ 00 + w˙ 0 /r = 0, a differential equation whose solution is w˙ = C +D ln r. Neither this velocity field nor the preceding (conical) one can possibly meet a condition of zero slope at a clamped edge, and this is why a hinge circle is necessary there. Finally, on AB and DE the flow rule gives κ˙ θ /κ˙ r = 0. If this is interpreted as κ˙ θ = w˙ 0 /r = 0, then the velocity field is w˙ = constant (i.e., rigidbody motion). Alternatively, we may interpret it as κ˙ r = inf ; this would be the state at a hinge circle, and from this follows the clampededge condition Mr = −MU . On the Mises√ellipse, the only relevant point where κ˙ θ /κ˙ r = 0 is D0 , where Mr = −2MU / 3. It follows from these considerations that a clamped plate must be in regime BC near the center and in CD near the edge; point C gives the state at r = c for some c such that 0 < c < a. With the same loading as assumed for the simply supported plate above, we have to solve the problem both for c > b and c < b. Case 1 : c > b. The equilibrium equation is F r2 , 0 < r < b, 2πb2 F (rMr )0 = MU − , b < r < c, 2π F , c < r < a. rMr0 = MU − 2π (rMr )0 = MU −
Let m = Mr /MU and p = F/2πMU ; then the solution satisfying the condi
312
Chapter 5 / Problems in Plastic Flow and Collapse I
tions at r = 0 and r = c is m(r) = 1 −
pr2 3b2
0 < r < b,
c − 1 , b < r < c, r r c < r < a. m(r) = −(p − 1) ln , c
m(r) = (p − 1)
The additional conditions to be met are continuity at r = b and m = −1 at r = a, producing the two equations 1 c 1 − p = (p − 1) −1 , 3 b
(p − 1) ln
a = 1. c
The assumption c > b requires 1 < p < 3, and the limiting case c = b, p = 3 corresponds to b/a = e−1/2 . Consequently, the present case represents the range 0 < b/a < e−1/2 . Eliminating c between the two equations, we obtain 1 3(p − 1) − p−1 b = e , p < 3. a 2p
For example, p = 2 corresponds to b/a = 0.276, p = 1.5 to b/a = 0.068, and p = 1.286 to b/a = 0.01. The ultimate concentrated load is 2πMU (p = 1, b = 0), the same as for the simply supported plate. This limit is approached, however, only at extremely small values of b/a. Case 2 : b > c. The equilibrium equation is F r2 2πb2 F r2 rMr0 = MU − 2πb2 F rMr0 = MU − 2π
(rMr )0 = MU −
0 < r < c, c < r < b, b < r < a.
An analysis similar to that in Case 1 leads to 5−p+ln(p/3) b − 2(p−1) =e , p > 3. a
The extreme case b = a (uniformly loaded plate) corresponds to p = 5.63, an increase of 88% over the ultimate load of the simply supported case. Much of the preceding theory is due to H. G. Hopkins and various collaborators. For more details and other solutions, see, for example, Hopkins and Prager [1953], Hopkins and Wang [1954], and Drucker and Hopkins [1955].
Section 5.3 / Plastic Buckling
313
For plates without circular symmetry, complete solutions are not available. Estimates of collapse loads will be found with the help of the upperbound theorem of limit analysis — and exceptionally of the lowerbound theorem — in 6.4.1. The effect of large deflections on the collapse load of a simply supported circular plate was studied by Onat and Haythornthwaite [1956]; the analysis is based on the deformation of the plate into a conical shell (see also Hodge [1959], Section 117). Approximate methods for determining collapse loads of shells are studied in 6.4.3.
Exercises: Section 5.2 1. Derive the plate equilibrium equations (5.2.6) by means of virtual work. Discuss the significance of the shear forces Qα in this formulation. 2. A uniformly loaded circular plate made of an elastic–perfectly plastic material with yield stress σY is assumed to obey the Tresca criterion. If the total load is F , determine the value FE at which yielding begins when the plate is (a) simply supported and (b) clamped. Compare with the corresponding ultimate loads. 3. Determine the velocity field in a fully plastic clamped circular Tresca plate of radius a carrying a load F that is uniformly distributed over an inner circle of radius b. Use the upperbound theorem to determine the relation between the load and the ratio b/a. Compare with the results in the text. 4. A simply supported circular Tresca plate of radius a carries a load F that is uniformly distributed over the perimeter of the circle r = b. Find the value of F and the moment distribution when the plate is fully plastic. 5. A simply supported circular Tresca plate of radius a carries a load F that is uniformly distributed over the entire plate. The ultimate moment is MU inside the circle b = a/2 and 21 MU outside this circle. Find the value of F and the moment distribution when the plate is fully plastic.
Section 5.3
Plastic Buckling
While Sections 5.1 and 5.2 dealt with the plastic collapse of bodies whose material behavior may be idealized as perfectly plastic, the present section
314
Chapter 5 / Problems in Plastic Flow and Collapse I
is devoted to the study of the buckling collapse of bodies made of workhardening material. The elementary theory of elastic column buckling is part of the knowledge of all students of mechanics. It is worthwhile, however, to begin this section, in 5.3.1, with a general introduction to stability theory and to use the buckling of bars as an illustration of the theory. In 5.3.2 we discuss theories of the modulus that must be used in the determination of critical loads. Finally, in 5.3.3 the plastic buckling of plates and shells is studied.
5.3.1.
Introduction to Stability Theory
Elastic Stability In 1.4.3 it was shown that an elastic body under conservative loads is in equilibrium if and only if the total potential energy Π is stationary with respect to virtual displacements, a condition expressed by Equation (1.4.18): δΠ = 0. It was further stated without proof that the equilibrium is stable only if Π is a minimum. An intuitive, though not strictly rigorous proof can be based on the following observation: if the configuration of the body is to change slightly from the one at equilibrium, and if the potential energy at the altered configuration is greater than at equilibrium, then additional work must be done on the body in order to effect the change, and therefore the change cannot take place spontaneously. The proof can be easily made rigorous for discrete systems (those with a finite number of degrees of freedom), and the result is known as the Lagrange–Dirichlet theorem. The proof for continua runs into technical difficulties, but these will be ignored here, and the result will be accepted. Mathematically, the condition that Π is a minimum at equilibrium can be expressed as follows: let Π denote the potential energy evaluated at the displacement field u, and Π + ∆Π the potential energy evaluated at the varied displacement field u + δu. Assuming the dependence of Π on u to be smooth, we can write 1 ∆Π = δΠ + δ 2 Π + . . . , 2 where δΠ (the first variation defined in 1.4.3) is linear in δu (and/or in its derivatives, and therefore also in δε), δ 2 Π is quadratic, and so on. We may limit ourselves to virtual displacements that are small enough so that terms beyond the quadratic can be neglected. Since δΠ vanishes if Π is stationary at u, clearly Π is a minimum only if δ 2 Π is nonnegative for all δu that are compatible with the constraints (i.e., for all virtual displacements).
Section 5.3 / Plastic Buckling
315
We may therefore say that the equilibrium is stable only if δ 2 Π > 0 for all virtual displacements. The criterion for the onset of instability, known as the Trefftz criterion, is thus δ 2 Π = 0. Since Π = Πint + Πext , we have δ 2 Π = δ 2 Πint + δ 2 Πext . An equivalent statement of the Trefftz criterion is therefore δ 2 Πint + δ 2 Πext = 0. In a linearly elastic body, Πint
1 = 2
Z R
Cijkl εij εkl dV,
and therefore 1 Cijkl [(εij + δεij )(εkl + δεkl ) − εij εkl ] dV 2Z R Z Z
∆Πint =
= R
Cijkl εij δεkl dV +
1 2
R
Cijkl δεij δεkl dV.
As a result of the definitions of the first and second variations, the first integral in the last expression is δΠint , and the second integral is δ 2 Πint , that is, Z δ 2 Πint =
R
Cijkl δεij δεkl dV.
(5.3.1)
Generalization to QuasiElastic Materials A general theory of stability in elastic–plastic solids capable of large deformations was formulated by Hill [1958]. Here, we shall limit our consideration to infinitesimal deformations. We can then immediately generalize the preceding result for linearly elastic bodies to nonlinearly elastic ones if we interpret C as the tangent modulus tensor defined by Cijkl = ∂σij /∂εkl . Since δσij = Cijkl δεkl , the integrand of (5.3.1) can be rewritten as δσij δεij . Since it is a given equilibrium state that is examined as to its stability, the past history of the body is irrelevant to this examination, and therefore the result can be further extended to materials that are quasielastic in the sense that, at a given state, a small stress variation δσ can be uniquely associated with a small strain variation δε. As we have seen, rateindependent plastic materials have this property. We may therefore state, as a generalization to quasielastic bodies of the Trefftz criterion, the energy criterion for the stability of such bodies subject to conservative loads: Z R
δσij δεij dV + δ 2 Πext = 0.
(5.3.2)
316
Chapter 5 / Problems in Plastic Flow and Collapse I
Furthermore, the first term on the lefthand side will be written as δ 2 Πint without thereby implying the existence of an internal potential energy Πint . In other words, we shall define def
δ 2 Πint =
Z
δσij δεij dV. R
In the absence of internal constraints, the quantity δσij δεij is positive for all nonvanishing δε if the material is linearly elastic. It is so likewise for rateindependent plastic materials that are stable in the sense of Drucker (see 3.2.1), that is, workhardening and obeying an associated flow rule. For bodies made of such materials, then, instability can occur only if it is possible for δ 2 Πext to be negative. If the loads f and ta are independent of displacement, the external potential energy is Z Z fi ui dV −
Πext = −
R
∂R
tai ui dS,
as given in 1.4.3. We see, then, that ∆Πext = δΠext (i.e. δ 2 Πext = 0) unless the virtual displacement significantly alters the region occupied by the body, thereby introducing terms that are quadratic in δu into ∆Π.
Buckling of QuasiElastic Bars The classic example of this occurrence is the buckling of a bar (column, strut) under a compressive axial load P acting through the neutral axis. If the bar is initially straight, with length L, and then bends, with the deflection of the neutral axis given by p v(x) (0 < x < L), then the chord spanned by RL the neutral axis becomes 0 1 − v 0 2 dx, so that the work done by the load P is ! Z Lq Z L . 1 2 2 0 P L− 1 − v dx = P v 0 dx. 2 0 0 If the only other load is a distributed transverse load q, then the external potential energy is Z
Πext = −
0
L
1 qv dx − P 2
Z
L
2
v 0 dx,
0
and the first and second variations are, respectively, δΠe = −
L
Z
q δv dx − P
0
Z
= 0
L
Z
L
v 0 δv 0 dx
0
L
00
(P v − q) δv dx − P v 0 δv 0
(the last form having been obtained by integration by parts), and δ 2 Πext = −P
Z 0
L
(δv 0 )2 dx.
(5.3.3)
Section 5.3 / Plastic Buckling
317
If the bar is subject to a distributed axial compressive load of intensity p per unit length in addition to end loads P0 and PL at x = 0 and x = L, respectively, then the external potential energy can be written as Πext = −
L
Z
qv dx −
Z
L
ps dx + P0 s(0) − PL s(L),
0
0
where s(x) is the shortening of the bar due to bending at point x, given by s(x) = s(0) +
1 2
Z
x
2
v 0 dx.
0
If P (x) now denotes the internal axial force at x (positive in compression), then equilibrium requires P 0 + p = 0, and therefore −
Z
L
Z
L
P sL 0
0
P s dx =
ps dx = 0
0
1 + 2
L
Z
2
P v 0 dx.
0
Equation (5.3.3) for Πext needs to be changed only by placing P under the integral sign, and δ 2 Πext = −
L
Z
P (δv 0 )2 dx.
0
In accordance with elementary beam theory, the state of stress at each point will be approximated as uniaxial, so that δσij δεij = δσx δεx . Furthermore, δεx = −y δv 00 , so that δ 2 Πint =
L Z
Z 0
(−y) δσx dA δv 00 dx =
Z
L
δM δv 00 dx,
0
A
where M is the bending moment. The energy criterion for bars therefore takes the form Z Z L
0
L
δM δv 00 dx −
P (δv 0 )2 dx = 0.
(5.3.4)
0
Integration by parts of the first integral leads to Z 0
L
L
(δM 0 + P δv 0 ) δv 0 dx = δM δv 0 0 .
Since the end conditions on beams are usually such that either the rotation v 0 or the bending moment M cannot be varied, the righthand side of this equation vanishes. ¯ such that δM = EI ¯ δv 00 ; in Finally, we assume an effective modulus E a linearly elastic material, of course, this is just the Young’s modulus E. ¯ may be assumed to be determined by the average In nonlinear materials E
318
Chapter 5 / Problems in Plastic Flow and Collapse I
stress in the bar, σ = P/A. Theories of the effective modulus are discussed in 5.3.2. In problems in which constraints on the deflection v itself can be disregarded, the virtual rotation δv 0 may be taken as the unknown variable. Writing this variable as θ, we obtain, upon observing that the rotation is not constrained in the interior of the bar, the differential equation ¯ 0 )0 + P θ = 0. (EIθ
(5.3.5)
More generally, the first integral in (5.3.4) must be integrated by parts twice, so that the energy criterion becomes Z 0
L
L
(δM 0 + P δv 0 )0 δv dx = (δM 0 + P δv 0 ) δv 0 .
(5.3.6)
The quantity in parentheses may be interpreted as the virtual shear force, and therefore either it or the virtual displacement can be expected to vanish at each end. The differential equation expressing the energy criterion is therefore ¯ 0 )00 + (P θ)0 = 0. (EIθ (5.3.7)
EndLoaded Prismatic Bars If the bar is prismatic then A and I are constant. If, moreover, it is subject to an axial end load only, then P is constant. In such a bar, then, the average stress P/A and therefore, by hypothesis, the effective modulus are constant. Equation (5.3.7) thus becomes ¯ 000 + P θ0 = 0, EIθ
(5.3.8)
and can be immediately solved as θ = B cos λx + C sin λx + D, where B, C, and D are constants, and λ is defined by P λ2 = ¯ . EI If the bar is pinned at both ends, then θ0 (0) = 0 and θ0 (L) = 0. The first condition requires C = 0, and the second λB sin λL = 0. For a nontrivial solution,1 λ and B must both be different from zero, and instability occurs only if sin λL = 0, 1
Note that D is irrelevant since it represents a rigid rotation.
Section 5.3 / Plastic Buckling
319
that is, if λ = nπ/L, where n is a positive integer. The fundamental mode of buckling corresponds to n = 1, that is, λ = π/L, and the load producing it (the critical load ) obeys P I = π2 2 . ¯ L E ¯ = E, and If the bar is elastic, E P = π2
EI def = PE , L2
where PE is known as the Euler load . For other end conditions, the equation governing the critical load can be written as P I = π2 2 , (5.3.9) ¯ Le E where Le is known as the effective length of the bar, given by Le = π/λ1 , λ1 being the smallest nonzero value of λ. For a cantilever column, for example, the characteristic equation is cos λL = 0, leading to a fundamental mode descibed by λ1 = π/2L, and hence Le = 2L. For a bar that is clamped at x = 0 and pinned at x = RL, the end conditions are θ(0) = θ0 (L) = 0, in addition to the constraint 0L θ dx = 0, describing zero deflection of the pinned end relative to the clamped end. The three conditions lead to the characteristic equation λL = tan λL, whose lowest root is λ1 L = 4.4934. Hence Le /L = π/4.4934 = 0.699. The solution of Equation (5.3.9) for the critical load for inelastic bars will be postponed until after the discussion of the effective modulus.
5.3.2.
Theories of the Effective Modulus
TangentModulus (Engesser–Shanley) Theory The first analysis of inelastic column buckling is due to Engesser [1889], who based the calculation of the critical load on the incremental relation δσx = Et δεx , where Et is the tangent modulus, defined as the slope dσ/dε of the uniaxial compression curve at the current value of σ = P/A. The essential assumption is that, while a bending moment requires a nonuniform stress distribution, the deviation of the stress from the average is, at least initially, sufficiently small so that the stressstrain curve can be locally approximated by straight line with slope Et . Consequently, the effective ¯ is just Et . Since this is a function of σ, it is convenient to modulus E rewrite Equation (5.3.9) in terms of σ rather than P , and to designate the solution as the critical stress σcr = Pcr /A. It is conventional to define the def p “radius of gyration” r = I/A, and to designate Le /r as the slenderness
320
Chapter 5 / Problems in Plastic Flow and Collapse I
ratio. Equation (5.3.9) now reads σ π2 = . Et (σ) (Le /r)2
(5.3.10)
A plot of the solution of this equation, σcr against Le /r, is often called a column curve. When σcr is given explicitly as a function of Le /r, the relation is called a column formula. If the material has a definite elasticlimit stress σE such that Et (σ) = E for σ < σE , then the slenderness ratio at which σ = σE is called the critical slenderness ratio, defined by L r
s
=π cr
E . σE
The critical slenderness ratio is clearly a material property (for mild steel it is about 90), and for supercritically slender bars the critical load is given by the elastic solution. The portion of the column curve for Le /r > (L/r)cr is thus the Euler hyperbola given by σcr =
π2E . (Le /r)2
If the material is perfectly plastic, so that σY = σE , then a stress greater than σE is not possible, and therefore σcr = σE for Le /r ≤ (L/r)cr . For materials without a definite elastic limit, the column curve approaches the Euler hyperbola asymptotically as Le /r → ∞. For a material whose uniaxial stressstrain relation is described by the Ramberg–Osgood equation (2.1.2), the tangent modulus is easily obtained as Et =
E , 1 + αm(σ/σR )m−1
(5.3.11)
and the column curve is obtained from σ σ + αm σR σR
m
=
π 2 E/σR . (Le /r)2
Since such a material hardens indefinitely, no cutoff stress exists for short bars. A formula describing a stressstrain relation with no definite elastic limit that approaches perfect plasticity asymptotically, with an ultimate stress σ∞ , was proposed by Prager [1942] in the form σ = σ∞ tanh
Eε . σ∞
Section 5.3 / Plastic Buckling
321
The asymptote is approached quite fast: when the total strain equals twice the elastic strain (ε = 2σ/E), the stress is already given by σ = 0.9575σ∞ . The tangent modulus can be readily obtained as "
Et = E 1 −
σ σ∞
2 #
.
The preceding formula can be easily generalized to
Et = E 1 −
σ σ∞
n
,
(5.3.12)
where n = 2 corresponds to the Prager formula. The case n = 1 describes an exponential stressstrain curve, σ = σ∞ [1 − exp(−Eε/σ∞ )]. The greater the value of n, the more rapid the approach to perfect plasticity. The column curve for the generalized Prager formula may be plotted from σ/σ∞ π 2 E/σ∞ = . 1 − (σ/σ∞ )n (Le /r)2 Explicit column formulas can be obtained from this equation for n = 1 and n = 2.
The ReducedModulus (K´arm´an) Theory Soon after the publication of Engesser’s theory, it was recognized by engineers, beginning with Consid`ere [1891] and eventually including Engesser himself, that the tangentmodulus theory was in contradiction with the elastic–plastic behavior of metals; a formal theory was proposed by von K´arm´an [1910], based on the following reasoning. When an initially straight bar under a compressive axial load begins to buckle, the fibers on the concave side undergo additional compression, but in those on the convex side the compressive strain, and hence the stress, is reduced. The stress change in the latter fibers is consequently elastic. Writing, for convenience, stress and strain as positive in compression, the incremental stressstrain relation is accordingly (
δσ =
Et δε, E δε,
δε > 0, δε < 0,
)
where Et is, as before, the elastic–plastic tangent modulus at the stress σ. Let y = y0 give the location of the neutral fibers, with y > y0 and y < y0 being the areas of additional and reduced compression, respectively. Since δε = (y − y0 ) δv 00 , the additional bending moment is Z
δM = A
(y − y0 ) δσ dA
322
Chapter 5 / Problems in Plastic Flow and Collapse I
or δM = Er I δv 00 , where 1 Er = E I
Z
2
(y − y0 ) dA + Et
yy0
is the reduced modulus. The value of y0 is determined, as usual, by the constancy of the axial load: Z
0 = δP =
δσ dA, A
or
Z
(y − y0 ) dA + Et
E
Z
yy0
Elimination of y0 permits the expression of Er as a function of σ and of bar geometry. If the bar is rectangular, with width b and depth h, then Equation (5.3.13), with the help of I = bh3 /12, gives 4 (Et h31 + Eh32 ). h3
Er = where
h h − y0 , h 2 = + y0 . 2 2 Equation (5.3.14), with the factor b omitted, then becomes h1 =
Z
y0
E −h/2
(y − y0 ) dy + Et
so that h1 /h2 =
Z
h/2
y0
1 (y − y0 ) dy = (Et h21 − Eh22 ) = 0, 2
p
E/Et , and √ h1 E =√ √ , h E + Et
√ h2 Et √ = √ . h E + Et
Finally, then, Er = √
4EEt √ 2 . E + Et
The reduced modulus is seen to be greater than the tangent modulus by a factor between 1 and 4, and therefore gives a correspondingly greater critical load. Figure 5.3.1 shows column curves based on both the tangentmodulus and reducedmodulus theories, for the Ramberg–Osgood formula with α = 0.1 and m = 10, and for the Prager formula.
Section 5.3 / Plastic Buckling σcr σ0
1.4
323
Ramberg–Osgood RM
TM
Elastic
1.2
1.0
σ0 =
Prager RM
n
σR , Ramberg−Osgood σ∞ , Prager
TM 0.8
0.6
0.4
0.2
0.0 0.0
q 1.0
2.0
3.0
4.0
5.0
6.0
7.0
σ0 Le E r
Figure 5.3.1. Column curves based on tangentmodulus (TM) and reducedmodulus (RM) theories for the Ramberg–Osgood formula with α = 0.1 and m = 10, and for the Prager formula. The elastic column curve is included for comparison.
Comparison of the Two Theories The reducedmodulus theory dominated engineering practice for most of the first half of the twentieth century, since it was rigorously based on elastic–plastic theory. However, experiments in which bars are subjected to increasing axial loads until they buckle have consistently shown the results to be in much better agreement with the tangentmodulus theory. The first explanation of this discrepancy was given by Shanley [1947]. The reducedmodulus theory is based on the assumption that buckling occurs with no firstorder change in the axial load, δP = 0. But, as Shanley wrote, “upon reaching the critical tangentmodulus load, there is nothing to prevent the column from bending simultaneously with increasing axial load.” It is thus possible for the neutral fibers to coincide initially with the extreme fibers on the concave side, all the other fibers undergoing additional compression. Any other possible location of the neutral fibers would correspond to a higher axial load, and therefore the tangentmodulus load Ptm is a lower bound to the elastic–plastic buckling load. The tangentmodulus load is thus not a load at which instability occurs, but bifurcation: when this load is exceeded the bar may be in one of several configurations — it may remain straight, or it may be bent in either direction
324
Chapter 5 / Problems in Plastic Flow and Collapse I
(buckling in one plane only is assumed). If the bar buckles at Ptm , then, as the load is increased, the neutral axis moves inward, tending asymptotically to the position corresponding to the reducedmodulus load. The latter load is therefore an upper bound to the buckling load.
Effect of Imperfections In tests on real bars, imperfections such as initial curvature or eccentricity of the load are inevitable. Some bending moment, however slight, must therefore be present as soon as any load is applied, and consequently bending proceeds from the beginning of loading. Consider a pinned elastic column with the load applied at a small distance e from the centroidal axis. The deflection v can easily be shown to be governed by EIv 00 + P v = P e, and the maximum deflection is found to be "
vmax
π = e sec 2
s
P PE
!
#
−1 .
The deflection remains of the order of e until the load gets close to the Euler load, when it begins to grow large. A similar conclusion holds for a column with an initial deflection v0 of amplitude e. The equation governing the total deflection v under an axial load P is EI(v 00 − v000 ) + P v = 0, and if the column is pinned while v0 is assumed as v0 (x) = e sin(πx/L), then the maximum deflection is vmax =
e . 1 − P/PE
For an imperfect column, then, the buckling load may be interpreted as the load in the vicinity of which the imperfections become significantly amplified. It is for this reason that the tangentmodulus load must necessarily appear as the buckling load of workhardening elastic–plastic columns, since the possibility of remaining straight when this load is exceeded is open only to perfect columns. In columns made of an elastic–perfectly plastic material, both the reduced and tangent moduli are zero, and therefore a perfect column, as discussed previously, will buckle elastically or yield in direct compression at supercritical and subcritical slenderness ratios, respectively. Such a sharp transition is, in fact, hardly ever observed in real columns made of structural steel, a material that is fairly well represented as elastic–perfectly plastic.
Section 5.3 / Plastic Buckling
325
The deviation from theoretical behavior can also be ascribed to imperfections. An approximate theory, developed by several nineteenthcentury authors and recently reviewed by Mortelhand [1987], results in the formula (1 − σ/σY )σ/σY π2E = , 1 − (1 + η)σ/σY σY (Le /r)2 where η = Ahe/2I, h being the beam depth and e, as before, the amplitude of the initial deflection. The effect of imperfections is of even greater significance in the analysis of postbifurcation behavior. This topic has been extensively reviewed by Calladine [1973] and Hutchinson [1974].
Other Uniaxial Buckling Problems: Rings and Arches From the preceding arguments we can infer that in all buckling problems in which uniaxial stress is assumed, the elastic solution can be used to give the buckling load with E replaced by Et , provided that Et can be taken as constant. Take, for example, a circular ring under an external pressure q per unit length of center line, the radius of the center line being R. The compressive force in the ring is thus qR, and the stress is σ = qR/A, where A is the crosssectional area. The wellknown solution is due to Bresse (see Timoshenko and Gere [1961]). The fundamental buckling mode is shown in Figure 5.3.2(a), with the ring deformed into an ellipse, and the critical pressure is 3EI qcr = 3 , R where I is the second moment of area of the crosssection for bending in the plane of the ring. q
C AA U CW @ R H j H X z X : *
?
q
3 9 R y X X H Y H
@ I
es e
CCW BMB B
AAU
?
B
R
e e
s % %
% 2α
R BB e B % eB % eB% (b)
%
K A 6 OCC A (a)
Figure 5.3.2. Buckling of a ring or arch: (a) complete ring; (b) hingeended arch. The four points on the buckled ring whose radial displacement is zero are the nodes of the buckling modes. Any half of the ring between two opposite
326
Chapter 5 / Problems in Plastic Flow and Collapse I
nodes is equivalent to a semicircular arch that is hinged at both ends, and therefore Bresse’s formula furnishes the critical buckling pressure for such an arch. More generally, for a hingedended arch subtending an angle 2α the fundamental buckling mode can be expected to be as shown in Figure 5.3.2(b), and the result for the critical pressure is !
qcr =
π2 EI −1 . 2 α R3
These results may be immediately converted to the inelastic case. Limiting ourselves to the ring, we obtain σ 3 = , Et (σ) (R/r)2 p
where r = I/A as before. If the stressstrain relation is given by the generalized Prager formula with n = 1, an explicit formula for the stress, and hence for the critical pressure, is obtained: qcr =
σ∞ A/R . 1 + (σ∞ /3E)(R/r)2
For a ring of rectangular crosssection, with depth h (in the radial direction) and width b (in the axial direction), we have A = bh and r2 = h2 /12. Defining p = q/b as the pressure in the usual sense (per unit area), we obtain σ∞ h/R , pcr = 1 + 4(σ∞ /E)(R/h)2 a formula that coincides with that derived by Southwell [1915] when σ∞ is identified with the yield stress. Southwell’s result was actually intended for cylindrical tubes rather than rings, but based on an assumption of uniaxial stress — a highly questionable assumption for a shell, as shown in the next subsection.
5.3.3.
Plastic Buckling of Plates and Shells
Introduction Consider a flat plate subject to an applied inplane force per unit length Fαa around its edge and a distributed inplane force per unit area pa . The membraneforce field Nαβ obeys the equilibrium equation (5.2.3) and the boundary condition νβ Nαβ = Fαa . The equilibrium becomes unstable if it is possible for the plate to undergo a deflection w(x1 , x2 ) with no additional forces applied. The membrane forces Nαβ can be assumed to be related to ¯αβ given by Equation (5.2.7), and the average Green–SaintVenant strains E
Section 5.3 / Plastic Buckling
327
if the former do not change, then neither do the latter. The middle plane will therefore undergo a secondorder displacement u ¯α such that 2¯ εαβ = u ¯α ,β +¯ uβ ,α = −w,α w,β . The work done by the applied forces on this displacement is I C
Fαa u ¯α ds
Z
I
+
pα u ¯α dA = A
ZC
= A
Z
νβ Nαβ u ¯α ds +
pα u ¯α dA A
[(Nαβ ,β +pα )¯ uα + Nαβ u ¯α ,β ] dA
with the help of the twodimensional divergence theorem. The quantity in parentheses vanishes as a result of (5.2.3). Since Nαβ is symmetric, Nαβ u ¯α ,β = Nαβ ε¯αβ = − 21 Nαβ w,α w,β , and the second variation of the external potential energy can finally be obtained as δ 2 Πext =
Z A
Nαβ δw,α δw,β dA.
(5.3.15)
δMαβ δw,αβ dA.
(5.3.16)
For δ 2 Πint we have δ 2 Πint =
Z A
Since δMαβ δw,αβ = (δMαβ δw,α ),β −δMαβ ,β δw,α , and since the edge conditions are usually such that νβ δMαβ δw,α = 0 on C, the equation expressing the energy criterion becomes Z A
(δMαβ ,β −Nαβ δw,β ) δw,α dA = 0.
Support conditions on a plate are rarely such that the deflection itself is unconstrained; another integration by parts is usually necessary, leading to the differential equation δMαβ ,αβ −(Nαβ δw,β ),α = 0.
(5.3.17)
Let the incremental relation between strain and stress for an isotropic material in a state of plane stress be written in the form 1 ε˙αβ = ¯ [(1 + ν¯)σ˙ αβ − ν¯σ˙ γγ δαβ ], E ¯ is the instantaneous where ν¯ is the instantaneous contraction ratio, and E modulus, in general not equal to the uniaxial tangent modulus discussed
328
Chapter 5 / Problems in Plastic Flow and Collapse I
before. If the tangentmodulus theory is applied to the plate problem, then an incremental momentcurvature relation can be written in the form ¯ δMαβ = D[(1 − ν¯) δw,αβ +¯ ν δw,γγ δαβ ],
(5.3.18)
¯ = Eh ¯ 3 /12(1 − ν¯2 ) is the effective plate modulus. The parameters where D ¯ and ν¯, and hence also D, ¯ are functions of Nαβ , and the general form E of (5.3.17) when the relations (5.3.18) are substituted is complicated. In what follows, only examples with a uniform membraneforce field will be considered.
Circular Plate Under Radial Load A simple example is that of a circular plate under a uniformly distributed compressive radial load applied around its edge. Let a be the radius of the plate, h its thickness, and N the magnitude of the applied load per unit length of circumference. It is easy to see that a uniform state of plane stress, σr = σθ = −N/h, is in equilibrium, satisfies the compatibility conditions if the plate is elastic, and obeys the yield criterion everywhere if it obeys it anywhere when the plate is plastic. If the buckling is assumed axisymmetric, the deflection of the middle plane being w(r), then the second integration by parts leading to (5.3.17) may be dispensed with, and the energy criterion can be expressed by the differential equation 1 [(r δMr )0 − δMθ ] + N φ = 0, r where φ = δw0 is the virtual rotation of the radial lines, with the prime denoting differentiation with respect to r. The axisymmetric form of (5.3.18) is ¯ φ0 + ν¯ φ , δMθ = D ¯ φ + ν¯φ0 , δMr = D r r and the equation governing φ is thus 1 φ00 + φ0 + r
N 1 − 2 φ = 0, ¯ D r
(5.3.19)
a Bessel equation of order 1. The q general solution that is regular at r = 0 ¯ and J1 is the Bessel function of the is φ(r) = J1 (λr), where λ = N/D first kind of order 1. Let λ = k/a be the smallest nonzero root for which φ satisfies the boundary condition. The critical load is then Ncr = σcr h, where ¯ the solution of the nonlinear equation σcr is, in view of the definition of D, ¯ h 2 k2 E , σ= 12 1 − ν¯2 a ¯ and ν¯ being, as noted above, functions of σ. E
(5.3.20)
Section 5.3 / Plastic Buckling
329
If the edge of the plate is clamped, then the edge condition φ(a) = 0 leads to the characteristic equation J1 (k) = 0, whose smallest nonzero root is k = 3.832. If the edge of the plate is free to rotate, then Mr must vanish there, so that the edge condition is φ0 (a) + ν¯φ(a)/a = 0. The characteristic equation then becomes J0 (k) −
1 − ν¯ J1 (k) = 0. k
Except in the case of the elastic plate, for which ν¯ = ν (the Poisson’s ratio), this equation must be solved simultaneously with (5.3.20) in order to find σcr . ¯ and ν¯ as functions of σ. We assume It is now necessary to evaluate E the plate material to be workhardening and governed by the Mises criterion and its associated flow rule. The plastic strain rate can then be written as ε˙pij =
9 skl s˙ kl sij , 4 HσY2
where σY is the current value of the uniaxial yield stress and H is the uniaxial plastic modulus (related to the tangent modulus by Hinv = Et inv − Einv), as can easily be verified by the substitutions s11 = 23 σ, s22 = s33 = − 31 σ, and σ = σY . In a state of plane stress, 1 skl s˙ kl = σαβ σ˙ αβ − σαα σ˙ ββ , 3 and therefore, if currently σ1 = σ2 = σ, ε˙p1 = ε˙p2 =
1 (σ˙ 1 + σ˙ 2 ). 4H
The complete incremental stressstrain relations are therefore
ε˙1 =
ε˙2 = Thus
1 1 + E 4H
1 1 + E 4H
σ˙ 1 −
σ˙ 2 −
ν 1 − E 4H
ν 1 − E 4H
σ˙ 2 , σ˙ 1 .
1 1 1 1 3 = + = + ¯ E 4H 4Et 4E E
and ν¯ =
1 + 4ν − E/Et . 3 + E/Et
. It should be noticed that for small values of Et /E, ν¯ = −1 + 4(1 + ν)Et /E . ¯ ¯ = 4Et , so that the factor E/(1 and E − ν¯2 ) in Equation (5.3.20) tends to a 1 constant fraction, 2 (1−ν), of the elastic value. This result, which is similar to
330
Chapter 5 / Problems in Plastic Flow and Collapse I
what occurs in other plate and shell buckling problems, is quite unreasonable when compared with the uniaxial case, and indeed with experimental data. Furthermore, the result is not limited to the Mises criterion but would also be produced by any isotropic yield criterion that is smooth at σ1 = σ2 = ±σY , since all such yield loci must be tangent there. We are left with the conclusion that incremental plasticity with a smooth yield surface may not be applicable to the analysis of multiaxial instability problems. Considerable improvement is obtained when the deformation theory of plasticity discussed in 3.2.1 is used. The Hencky theory, in particular, is based on the Mises criterion, and gives the plastic strain as εpij = where
3¯ εp sij , 2¯ σ
(5.3.21) r
r
3 2 p p σij σij , ε¯p = ε ε σ ¯= 2 3 ij ij are the equivalent stress and plastic strain, related to each other by the uniaxial relation. The incremental form of (5.3.21) is dεpij
3 = 2¯ σ
ε¯p d¯ ε − d¯ σ sij + ε¯p dsij . σ ¯
p
Upon introducing the uniaxial secant and tangent moduli Es and Et , defined by 1 1 ε¯p 1 1 d¯ εp = + , = + , Es E σ ¯ Et E d¯ σ the incremental relation may be written as dεpij =
3 2
1 1 − Et Es
d¯ σ sij + σ ¯
1 1 − Es E
dsij .
Applying the relation to the planestress case with σ1 = σ2 leads to the instantaneous modulus and contraction ratio 1 1 3 ¯ = 4Et + 4Es E and ν¯ = −
E/Et + 2(1 − 2ν) − 3E/Es . E/Et + 3E/Es
For a gradually flattening uniaxial stressstrain curve, when Et Es E . . ¯= we have E 4Et as in the incremental theory, but ν¯ = −(1 − 6Et /Es ), and . ¯ therefore E/(1 − ν¯2 ) = Es /3. To the first approximation, then, it is the secant modulus, rather than the elastic modulus, that governs the buckling, resulting in a much smaller critical load than that given by the incremental theory.
Section 5.3 / Plastic Buckling
331
An explanation of the failure of incremental theory based on an isotropic yield criterion to predict a reasonable buckling load is due to Phillips [1972], who points out that the yield criteria of workhardening materials become anisotropic almost immediately upon plastic loading.
Torsional Buckling of a Cruciform Column If a column is made up of thin plate sections that do not form a closed tube and is sufficiently short, then under the action of a compressive axial load it will buckle by twisting rather than bending. Consider, for example, the crossshaped column shown in Figure 5.3.3, and in particular the flange whose middle plane is the xyplane with y positive. If the virtual twist angle per unit length of the crosssection at x is φ(x), then the virtual deflection at (x, y) is δw(x, y) = yφ(x). The axial load P may be assumed to be uniformly distributed with intensity P/4b per unit width of flange. The secondorder external potential energy on a fiber of width dy is therefore P d(δ Πext ) = − dy y 2 4b 2
Z
L
φ02 dx,
0
and, for the whole flange, 2
Z
y=b
δ Πext = y=0
P b2 d(δ Πext ) = − 12 2
Z
L
φ02 dx.
0
The energy criterion may be expressed by adding this quantity to δ 2 Πint as given by (5.3.16) and equating the result to zero. Now δw,11 = yφ00 ,
δw,12 = φ0 ,
δw,22 = 0,
so that ¯ 2 φ002 + (1 − ν¯)φ02 ]. δMαβ δw,αβ = D[y However, φ00 is of order φ0 /L, and, if L b, then the first term in brackets may be neglected in comparison with the second. Consequently, independently of the form taken by φ0 , Pcr =
¯ − ν¯) 12D(1 , b
¯ we can define σcr = Pcr /4bh as the solution or, because of the definition of D, of 2 h ¯ σ=G , b ¯ = E/2(1 ¯ where G + ν¯) is the instantaneous shear modulus, dτ /dγ. Note that the result is independent of the column length L. In any incremental theory with a yield criterion of the form (3.3.5) and an associated flow rule, when τ = 0 the normal to the yield locus is directed
332
Chapter 5 / Problems in Plastic Flow and Collapse I
x
?? " ?? " ? "????? ????? ?? " ?? " ? " ?
b
6
L
# "# " "# "# " " ## " φ# q k 0
?
z
66 "" 666666 " 66 " " 666
" y
""
Figure 5.3.3. Cruciform (crossshaped) column: initial and buckled geometry. ¯ = G, so that the in the σdirection, and therefore dγ p = 0. Consequently G buckling load is unaffected by plasticity — again an untenable result. On the other hand, in the Hencky theory we have dγ p = 3
1 1 − Es E
dτ,
so that ¯= G
Es . 3 + (1 − 2ν)Es /E
Once again, it is primarily the secant modulus that determines the critical load. Experiments by Gerard and Becker [1957] on aluminum columns show very good agreement with the prediction of deformation theory for ν = 21 (see Figure 5.3.4).
Shell Under External Pressure The behavior of shells is in general much more complicated than that of plates. However, the buckling behavior of certain thinwalled shells may be studied by means of a simplified theory, known as the Donnell–Mushtari– Vlasov (DMV) theory, whose structure is essentially the same as that of plate theory (see Niordson [1985], Chapter 15). It must be kept in mind,
Section 5.3 / Plastic Buckling
333
1.2
r r r rr rrr rrrr rrr
1.0 .8
r rrrrr rr rr rr rr rr r rrr
(a)
(b)
σcr G(h/b)2.6
rr
.4
r r rr r
.2 0
0
10
20
30 40 σcr (ksi)
50
60
Figure 5.3.4. Torsional buckling of a crossshaped column: predictions of (a) incremental and (b) deformation theories with ν = 1/2. Dots represent experimental results (Gerard and Becker [1957]). though, that shells are far more imperfectionsensitive than bars or plates; even the slightest imperfections can greatly reduce the buckling load. For an elastic thinwalled cylindrical tube of mean radius R and thickness h, subject to an external pressure p, the critical pressure can be found from the Bresse formula for the ring by substituting D for EI, resulting in pcr
E = 4(1 − ν 2 )
h R
3
.
The substitution is equivalent to assuming that the axial strain is zero. In other words the tube, when viewed axially, is in a state of plane strain as opposed to the planestress state of the ring. The axial stress is thus σz = νσθ , where σθ = −pR/h is the circumferential stress, and the circumferential stressstrain relation is σθ = Eεθ /(1 − ν 2 ). In an elastic–plastic tube governed by incremental theory, the planestrain condition can only be enforced incrementally, that is, dσz = ν¯ dσθ . If buckling occurs after yielding, then the state of stress just before buckling is not known a priori , but must be determined by integrating the incremental relation, and checking at each step whether the buckling criterion is met. The situation is somewhat simpler with deformation theory. The condition εz = 0 results in 1 Es σz = 1 − (1 − 2ν) σθ . 2 E
334
Chapter 5 / Problems in Plastic Flow and Collapse I
The incremental relation is Es 1 − 2ν dEs 1 1 − (1 − 2ν) dσθ − dσz = d¯ σ. 2 E 2E d¯ σ But
dEs Es =− d¯ σ σ ¯
Es −1 Et
and (2σθ − σz ) dσθ + (2σz − σθ ) dσz . 2¯ σ Thus both d¯ σ and dσz can be expressed as multiples of dσθ , and the expressions can be substituted in 1 1 2σθ − σz 1 1 dεθ = (dσθ − ν dσz ) + − d¯ σ, E 2 Es E σ ¯ q
d¯ σ = d σθ2 − σθ σz + σz2 =
resulting in d¯ εθ =
1 dσ , ˜ θ E
˜ is in general a complicated function of σθ ; it is this E ˜ that replaces where E 1 ˜ E in the Bresse formula. When ν = 2 , however, E turns out to be just 4Et /3, where Et is the uniaxial tangent modulus. In this case the same result is given by incremental plasticity theory. The problem of the spherical shell is easier, since the state of stress before buckling is σθ = σφ = −σ, where σ = pR/2h. The critical value of σ for elastic buckling is given by E h σcr = p . 2 3(1 − ν ) R The value for plastic buckling can be obtained by solving ¯ h E , 3(1 − ν¯2 ) R
σ=p
¯ and ν¯ are the same functions of σ as are used for the circular plate where E under radial force. Figure 5.3.5 shows the critical stress for the buckling of a spherical shell, based on both the incremental and deformation theories, using the Ramberg–Osgood formula with α = 0.1 and m = 6. For comparison, the stressstrain curve is also shown.
Exercises: Section 5.3 1. Find the reduced modulus Er in terms of the elastic modulus E and the tangent modulus Et for (a) an ideal sandwich section and (b) for a thinwalled square tube section. Compare with the result for a rectangular section when Et /E = 0.1 and when Et /E = 0.02.
Section 5.3 / Plastic Buckling
335
2.0 1.8 (a) 1.6
(c) (b)
1.4 σcr σR 1.2 or σ σR 1.0 0.8
(a) Incremental theory (b) Deformation theory (c) Stressstrain curve
0.6 0.4 0.2 0
0
1
2
3
p 1 3(1 − ν 2 )
4
Eh σR R
5
6
Eε or σ R
7
Figure 5.3.5. Buckling of a spherical shell under internal pressure: critical stress based on (a) incremental and (b) deformation theories, with (c) stressstrain curve included (from Hutchinson [1972]). 2. Plot column curves based on both the tangentmodulus and the reducedmodulus theories (for a rectangular section) for (a) the generalized Prager formula with n = 1, (b) the generalized Prager formula with n = 4, (c) the Ramberg–Osgood formula with α = 0.3 and m = 4. 3. For a ring under radial pressure, plot suitably nondimensionalized buckling curves (qcr against R/r) on the basis of (a) the Prager formula and (b) the Ramberg–Osgood formula with α = 0.2 and m = 6. ¯ and a con4. Is it possible to find an instantaneous plate modulus D traction ratio ν¯ for the buckling problem of a circular plate under a compressive radial load when the plate material obeys the incremental theory of plasticity with the Tresca criterion and its associated flow rule? Explain. 5. Perform the analysis leading to the results shown in Figure 5.3.5.
336
Chapter 5 / Problems in Plastic Flow and Collapse I
Chapter 6
Problems in Plastic Flow and Collapse II Applications of Limit Analysis Introduction The theorems of limit analysis for standard elastic–perfectly plastic threedimensional continua in arbitrary states of deformation were proved in 3.5.1. The proof, due to Drucker, Prager, and Greenberg [1952],1 was the final link in a chain of development of the theory, which began with proofs for beams and frames by Gvozdev [1938], Horne [1950], and Greenberg and Prager [1951], followed by a proof for bodies in plane strain by Drucker, Greenberg, and Prager [1951]. In this chapter applications of the theorems are presented. Section 6.1 deals with plane problems in both plane strain and plane stress. Section 6.2 deals with beams under combined loading (including arches), Section 6.3 with trusses and frames, and Section 6.4 with plates and shells. It is shown that as a rule, plausible velocity fields are easier to guess than stress fields, and therefore in many cases only upperbound estimates are available. Of particular importance are velocity fields called mechanisms, in which deformation is concentrated at points, lines, or planes, with the remaining parts of the system moving as rigid bodies. The use of mechanisms for estimating collapse loads antedates the development of plasticity theory. Examples include Coulomb’s method of slip planes for studying the collapse strength of soil, the plastichinge mechanism due to Kazinczy [1914] for steel frames, and the yieldline theory of Johansen [1932] for reinforcedconcrete slabs, later extended to plates in general. 1
But already given in the book by Prager and Hodge [1951].
337
338
Chapter 6 / Problems in Plastic Flow and Collapse II
Section 6.1
Limit Analysis of Plane Problems
As pointed out in Section 5.1, slipline theory as a rule gives only upper bounds, unless an admissible extension of the stress field from the region covered by the slipline field to the rest of the body is found. A convenient method for finding lower bounds is by means of discontinuous stress fields, some examples of which were studied in Section 5.1.
6.1.1.
Blocks and Slabs with Grooves or Cutouts
Among the earliest applications of limit analysis to plane problems are studies of the effects of cutouts on the yielding of rectangular slabs or blocks subject to tension perpendicular to a side. In the absence of cutouts, the slab may be assumed to collapse under a uniform state of tensile stress σ = σY = 2k, the Tresca criterion being assumed in plane stress. The cutouts may be expected to reduce the average or nominal tensile stress σ required for collapse to 2ρk (0 < ρ < 1), where ρ is called the cutout factor . Limit analysis may be used to find bounds on the cutout factor.
Tension of a Grooved Rectangular Block The following example, illustrated in Figure 6.1.1, is discussed by Prager and Hodge [1951]. A statically admissible stress field is shown in Figure 6.1.1(a). The trapezoidal regions on either side of the line of symmetry OO correspond to the truncated wedge of Figure 5.1.6(e) (page 289), except that the stresses are tensile rather than compressive. The rectangular regions beyond the trapezoids are in simple tension with stress σ = 2k(1 − sin γ), where γ is the wedge semiangle. In order to produce the best lower bound, γ should be as small as possible, subject to the geometric restriction discussed in connection with Figure 5.1.6(e) and the evident additional restriction that the flanks of the wedge be tangent to the cutout circles. It can be shown, the details being left to an exercise, that these restrictions require that 2 sin 2γ = 1 + sin γ. The smallest angle obeying this equation is 0.379 radian, so that sin γ = 0.370, and the lower bound to the cutout factor is 0.630. A simple kinematically admissible velocity field is shown in Figure 6.1.1(b). The portion above the line AB slides rigidly along this line with respect to the portion below. If the sliding speed is v, then the plastic √ dissipation per unit area along AB is kv, while the length of √ the line is 3a 2. The external rate of work per unit thickness is σ · 4a · v/ √2. Equating this rate to the total internal dissipation per unit thickness, 3 2kva, yields the upper bound σ = 3k/2, or ρ = 3/4. Figure 6.1.1(c) shows a slipline field in which the region bounded by the slip lines AB and A0 B (as well as its mirror image) is in a state of
Section 6.1 / Limit Analysis of Plane Problems
339
B
Q L Q L
J Q
J
Q JJJJJ J L
QJJJJ J
J
JJ J J L
J
J JJJJJ
J
L
J
J a J Ia
J L
b J b O O J J
L
JJJ
J
J L
J
J
L j JJJ JJ
J γ J
J
J J
J Q J Q J
J
JJJJ L
Q J
J J
L J Q QL
2a

2a
I 45◦ A0
B
b
b
b
A
AAU q
C
bO
A
(c)
(b)
(a)
Figure 6.1.1. Tension of a grooved rectangular block: (a) statically admissible stress field; (b) kinematically admissible velocity field; (c) slipline field. axisymmetric stress as studied in Section 4.4. The stress σθ in this region is
r , a
σθ = 2k 1 + ln
where r is measured from the center O of the circle. The resultant axial force per unit thickness is therefore Z
2a
F =2 a
Z
σθ dr = 4k
2a
a
r 1 + ln dr a
= 8ka ln 2. The nominal stress is thus σ = F/4a = 2k ln 2, corresponding to a cutout factor of ln 2 = 0.693. Since the stress field has not been extended to the regions outside the slipline field, this value cannot be a lower bound. On the other hand, the slipline field implies a solution for the velocity field, which, together with the rigid axial motion of the regions outside it, forms a kinematically admissible velocity field for the body as a whole, and therefore the result gives an improved upper bound for the cutout factor. The bounds on the cutout factor are therefore 0.630 ≤ ρ ≤ 0.693.
Tension of a Square Slab With a Slit A thin square slab with a narrow slit perpendicular to the direction of the load is shown in Figure 6.1.2(a). The slit width is assumed to be of
340
Chapter 6 / Problems in Plastic Flow and Collapse II
the same order of magnitude as the slab thickness, both being much smaller than the sides of the square. A kinematically admissible velocity field may be based on a shearing failure mode as shown in Figure 6.1.2(b). If the shearing plane makes an angle α with the load direction then the total area of the surface of sliding is (1 − β)ah csc α, where h is the slab thickness; and if the relative velocity of motion of the two parts of the slab is v, then the plastic dissipation per unit area is kv sec α. The total internal dissipation is therefore 2k(1 − β)ahv csc 2α. The external work rate is σahv, and therefore an upper bound to the cutout factor is (1 − β) csc 2α. The best upper bound is obtained for α = π/4, and gives ρ = 1 − β. 666666666666666666
666
α

(1 − β)a
2βa


(1 − β)a
?????????????????? ???  h 2a (a)
# c T # Tcc # 1 T c # #2 T 2c # c c# ? T H ξa T 4 HH 3 H 4 6 3 H H T 2 #c 2 #c T c # T 1 c T ## c # cT c T # (c)
(b)
Figure 6.1.2. Tension of a square slab with a narrow slit: (a) geometry and loading; (b) kinematically admissible velocity field; (c) statically admissible stress field. A discontinuous stress field for the determination of a lower bound was constructed by Hodge [1953] (see Hodge [1959], Section 122), and is shown in Figure 6.1.2(c). Since the problem is one of plane stress and not plane strain, it is not the Prager jump conditions (5.1.5) but the more general jump conditions (5.1.6), together with the yield criterion, that must be used. There being four distinct regions, the total number of unknown stress variables (ni , ri , θi ) (i = 1, 2, 3, 4) is 12. The equations for these variables are furnished by, first, two traction boundary conditions each on two sides of the square and on the face of the slit, and second, by two jump conditions each on the boundaries between regions 1 and 2, 2 and 3, and 2 and 4. In particular, the fact that τxy vanishes on the external boundaries of regions 1, 3 and 4 means that it vanishes throughout these regions. Regions 3 and 4 can reasonably be assumed to be in a state of simple tension and compression, respectively, so that θ3 = θ4 = 3π/4. In region 1, θ is either 3π/4 or
Section 6.1 / Limit Analysis of Plane Problems
341
π/4; it will be assumed that σy ≥ σx there, so that θ1 = π/4. The remaining boundary conditions accordingly give n1 − r1 = σ,
n3 − r3 = 0,
n4 + r4 = 0,
so that n1 , n3 and n4 can be eliminated. The jump conditions are n2 + r2 sin 2(θ2 − χ12 ) = σ + r1 cos 2χ12 , n2 + r2 sin 2(θ2 − χ23 ) = r3 (1 − cos 2χ23 ), n2 + r2 sin 2(θ2 − χ24 ) = −r4 (1 + cos 2χ24 ), r2 cos 2(θ2 − χ12 ) = r1 sin 2χ12 , r2 cos 2(θ2 − χ23 ) = −r3 sin 2χ23 , r2 cos 2(θ2 − χ24 ) = −r4 sin 2χ24 , where the angles χ12 , χ23 and χ24 , giving the inclinations of the normals to the boundary lines with the xaxis, can be expressed in terms of β and ξ. Once the equations are solved, satisfaction of the yield inequality 2r + n − r + n − r ≤ 4k in each region produces four inequalities on the cutout factor ρ = σ/2k: ρβ ≤ 1 − ξ,
ρ ≤ 1 − β,
ρβ ≤ ξ,
q
ρ [ξ + β(1 − β)]2 + 4β 2 ≤ β + ξ(1 − β). If the second inequality were satisfied as an equality, then the result β = 1−ρ would coincide with the upper bound. It turns out that if the equality is assumed, then the remaining inequalities are obeyed if ξ = 1 − β + β 2 . In this problem, then, the exact cutout factor has been found. Other problems involving slabs with cutouts were treated by Hodge and various coworkers (see Hodge [1959], Chapter 12, for a survey).
6.1.2.
Problems in Bending
Pure Bending of a Notched Bar The notched bar shown in Figure 6.1.3(a) is of rectangular crosssection and subject to equal and opposite couples M applied at its ends. The discontinuous stress field shown is statically admissible, and plastically admissible in classical plane strain as well as for the Tresca criterion in plane stress. It is, of course, equivalent to the limiting stress distribution in a perfect beam, limited to the material below the notch, and gives a lower bound of 12 kba2 for the ultimate moment, where b is the width of the beam.
342
Chapter 6 / Problems in Plastic Flow and Collapse II
Stressfree
M
% % e e%  2k 2k e
Stressfree
O M
6
a
? (a)
M
Rotating rigid regions e % A ω % e Iω e ...% .. ... r...... II I .... ..... ...... ..... ....... R , ...... ....... ........ ....... α C D ........ ....... ,........ ........ ....... ....... ...... ....... ...... ....... ...... ..... .... ..... ll .... ... 6 .... B I @ @ Static rigid Thin zones in which shearing occurs
O M
“hinge”
(b)
Figure 6.1.3. Pure bending of a notched bar: (a) statically admissible stress field; (b) mechanism. An upper bound can be found on the basis of a mechanism, shown in Figure 6.1.3(b), in which the outer portions of the bar rotate rigidly by sliding along the arcs ACB and ADB, the inner region ACBD remaining stationary; the arcs must accordingly be circular. The mechanism resembles the plastic hinge discussed in 4.4.2. If the angular velocity of rotation is ω and the radius of the arcs is r, then the plastic dissipation per unit area of sliding surface is krω. If the angle subtended by the arcs is 2α, then the total area of the sliding surfaces is 4brα. But r = 21 a csc α, so that the total internal dissipation is kωba2 α csc2 α. Equating this to the external work rate 2M ω gives the upper bound M = 21 kba2 α csc2 α. The smallest value of this occurs when tan α = 2α, and gives the upper bound of M = 0.69kba2 . For a bar that is wide enough to be regarded as bending in plane strain, A. P. Green [1953] found a slipline field that gives the improved upper bound of M = 0.63kba2
EndLoaded Cantilever in Plane Strain and Plane Stress Another problem studied by Green [1954a] by means of slipline theory concerns the impending collapse of an endloaded wide tapered cantilever, shown in Figure 6.1.4.1 If the taper is not extreme and if the ratio L/h of the length to the least depth is sufficiently great, it is reasonable to suppose that the collapse mechanism is of the plastichinge type. The slipline fields shown in Figures 6.1.4(a) and (b) produce deformations similar to those 1
For the prismatic beam, the problem was also studied by Onat and Shield [1955].
Section 6.1 / Limit Analysis of Plane Problems
343
corresponding to a hinge mechanism. In (a), the rigid portion to the right of the slipline field rotates about point Y ; in (b) it slides over the circular arc P Y Q, as in the preceding problem, and AP Y QB is a continuous slip line that is a locus of velocity discontinuity.
L
A
A
?θ
D
P
6 Y
C
O h
D
Y
C
O
Q E
B
?
6θ
?
B
E
?
F
F
(b)
(a) XX XXX
XXX
0
1
y
z 2k Tension
k
Unstressed
–2k9 3
XXX X
4
F
◦ 75
XXX
2
O :
L
? 6
@ @
h
I Rk @ @
Compression
O ◦
W 0

75
?
? (d)
F
(c)
Figure 6.1.4. Endloaded tapered cantilever: (a)–(b) slipline fields; (c) statically admissible stress field. (d) Weakly supported prismatic cantilever. A complete solution is found, with the help of the discontinuous but statically and plastically admissible stress field shown in Figure 6.1.4(c), for the beam with 15◦ taper (θ = 75◦ ), in which case FU = kbh for all values of L/h. For greater values of θ, no extension of the stress field into the rigid regions is given and therefore the calculated value of F is an upper bound to FU , though, as Green argues, it is likely to be very close, since the proposed slipline field shows remarkable similarity with the plastically deformed region observed in experiments. For θ ≥ 75◦ the load is given, in accordance with the slipline field in (a), by F = 2kbh sin 2θ
for
L 1 ≥ tan θ(sin 2θ − cos 2θ). h 2
344
Chapter 6 / Problems in Plastic Flow and Collapse II
For a given θ, as L/h is decreased below the limiting value, F increases. For prismatic beams, Green [1954a,b] also constructed solutions for uniformly distributed loading, and for other boundary conditions, including “weakly” supported cantilevers (see Figure 6.1.4(d)) as well as beams fixed at both ends. A much simpler velocity field for a prismatic beam is shown in Figure 6.1.5(a). In this picture region 1 undergoes simple shearing, regions 2 and 3 rotate rigidly, and regions 4 and 5 undergo tension or compression. In the lastnamed regions the vertical velocity does not vanish, so that the condition of no motion at the wall is not satisfied. A modification of the mechanism that satisfies this condition, shown in Figure 6.1.5(b), was proposed by Drucker [1956a]; here region 6 does not displace. The mechanism of Figure 6.1.5(a) is equivalent (with the direction of the force reversed) to that of Figure 6.1.5(c) for a centerloaded simply supported beam. Calculations are done here only for mechanism (a). y 4
π/4
I ?
π/4 2
6
@4
2
6
1
@4
@
@
I ?
2
6 x
1
d h
1
5
@ @
5
?
3 L

3
[email protected] @
?
L
?
F
(a)
6
?
L
F
F
@ @  ? 2F
(b)
3 L
6 F
(c)
Figure 6.1.5. Velocity fields for a prismatic beam: (a) simple velocity field for a cantilever; (b) Drucker’s modification; (c) centerloaded simply supported beam. The velocity components vx and vy will be denoted u˙ and v, ˙ respectively, with the subscripts referring to the regions. The mechanism implies the following velocity field: ˙ 1− x , u˙ 1 = 0, v˙ 1 = ∆ L ˙ ∆ d x ˙ u˙ 2 = y− , v˙ 2 = ∆ 1 − , L 2 L ˙ ˙ 1 − x , v˙ 4 = ∆ y − d . u˙ 4 = ∆ L L 2
The velocities in regions 3 and 5 are analogous to those in 2 and 4, respectively. Note that the velocity field is continuous. Note further that ε˙x + ε˙y = 0 in every region, so that the mechanism applies to plane strain
Section 6.1 / Limit Analysis of Plane Problems
345
as well as to plain stress. For either the Mises or the Tresca criterion, the ˙ ˙ ˙ equals τY ∆/L in regions 4 and 5. in region 1 and 2τY ∆/L dissipation Dp (ε) Equating the external work rate to the total internal dissipation, ˙ ˙ ∆ ∆ h−d 2 ˙ F ∆ = τY · bLd + 2τY · b , L L 2
leads to the upper bound "
d d h F = τY bh 1− + h 2L h
2 #
.
(6.1.1)
The upper bound can be optimized by minimizing with respect to d. The minimum occurs at d = h − L and leads to F = τY bh(1 − L/2h); but this result is valid only for L < h. For L ≥ h, d = 0, that is, the mechanism is a plastic hinge consisting of two deforming triangles, and F = τY bh2 /2L — a result that, in plane stress, agrees with that of elementary beam theory for the Tresca criterion.
EndLoaded Cantilever in Plane Stress: Lower Bound Drucker [1956a] also constructed a lower bound for the problem by means of the following statically admissible stress field: F x 2α2 2y cos α 1 − bh h 1 − cos α h
σx =
F α 2y = sin α 1 − bh 1 − cos α h
τxy
sgn y,
,
σy = 0,
with α ≤ π/2. The yield criterion (3.3.5)1 is met at x = L if α=
hσY 2LτY
and
F = τY bh
1 − cos α . α
(6.1.2)
In accordance with the limitation on α, the result is limited to h/L ≤ πτY /σY . It can easily be ascertained that for small values of h/L, the result for F approaches σY bh2 /4L as in the beamtheory approach. For h/L > πτY /σY , the stress field is σx = 0, and
τxy = τY
x π 2y − d cos 1− L 2 h−d
σx = σY 1
σy = 0,
for y
d . 2
The stress field is in equilibrium if d = h − πτY L/σY . The load is then 2 d F = τY bh 1 + π h
π −1 2
τY L . = τY bh 1 − (π − 2) σY h
(6.1.3)
The upper and lower bounds are compared in Figure 6.1.6. 2F L τY bh2 1.0 0.8 0.6
1 Lower bound
σY =2 τY (Tresca)
Upper
bound )
0.4 0.2 0 0.02
0.04
0.1
0.2
0.4
1.0
2.0
4.0
10.0
20.0
h L
Figure 6.1.6. Upper and lower bounds for an endloaded prismatic cantilever beam
IBeams Green [1954b] extended his results for prismatic beams to Ibeams by assuming that the slipline fields derived for rectangular beams in plane stress prevail in the web, while the flanges are in pure tension or compression. The shear force is thus carried entirely by the web, while the bending moment is the sum of that provided by the web and the couple formed by the flange forces. The simple velocity fields shown in Figure 6.1.5 were proposed for short Ibeams by Leth [1954] with d as the actual web depth. The upperbound load based on the field in (a) or (c) is
F = τY
h−d Aw + 2Af , L
where Aw = tw d is the web area and Af = bf (h − d) is the flange area, tw and bf being respectively the web thickness and flange width. Since Af and Aw are typically of the same order of magnitude, the second term in parentheses may usually be neglected, and the upperbound loaded may be approximated as τY Aw .
Section 6.1 / Limit Analysis of Plane Problems
347
For sufficiently long Ibeams, however, it is reasonable to assume that . failure is by a plastichinge mechanism, with F = MU /L as given by elementary beam theory. For an Ibeam, MU =
σY . σY h [Aw d + 2Af (h + d)] = (Aw + 4Af ), 4 4
the approximate expression being based on the assumption that h − d h. Comparing the two upper bounds, then, we find that the plastichinge mechanism furnishes the lower one for L σY ≥ h 4τY
1+4
Af Aw
,
approximately, or about 5/2 for a beam made of Tresca material with Af = Aw . Additional results in the limit analysis of beams, derived on the basis of local behavior, are discussed in Section 6.2 (see 6.2.4).
6.1.3.
Problems in Soil Mechanics
Yield Criterion and Flow Rule The most commonly used yield criterion for soils is the Mohr–Coulomb criterion discussed in 3.3.3, σmax − σmin + (σmax + σmin ) sin φ = 2c cos φ, where c is the cohesion and φ is the angle of internal friction. The Mohr– Coulomb criterion includes, as limiting cases, (1) the Tresca criterion (with φ = 0 and c = k), used to describe, for example, saturated clays, and (2) the cohesionless friction model (c = 0) for cohesionless soils (dry sands and gravels). If the material is taken as standard, then the flow rule at a regular point of the yield surface is ˙ + sin φ), ε˙pmax = λ(1
˙ − sin φ), ε˙pmin = −λ(1
ε˙pint = 0.
p The flow rule implies a constant dilatancy ratio, defined as (ε˙p1 +ε˙p2 +ε˙p3 )/γ˙ max , p p p p which at a regular point is given by (ε˙max + ε˙min )/(ε˙max − ε˙min ) and is therefore equal to sin φ. The measured dilatancy of most soils (as well as rocks and concrete) is usually significantly less than this,1 except in the case of undrained clays in which both internal friction and dilatancy are negligible. Most such materials, therefore, cannot be modeled as standard. In a nonstandard model, the flow rule may be taken in the same form as above, but with the dilatancy angle ψ replacing φ. 1
The dilatancy ratio rarely exceeds 0.1, while the angle of internal friction may be as high as 45◦ in dense, wellgraded soils with angular particles.
348
Chapter 6 / Problems in Plastic Flow and Collapse II
The plastic dissipation in a standard Mohr–Coulomb material was shown by Drucker [1953] to be Dp (ε˙ p ) = c cot φ(ε˙p1 + ε˙p2 + ε˙p3 ) at any point of the yield surface, including the corners. In plane plastic flow with ε˙3 = 0, as was pointed out in 3.3.4, σ3 is the intermediate principal stress, even if ψ 6= φ. The criterion therefore takes the form σ1 − σ2  + (σ1 + σ2 ) sin φ = 2c cos φ.
Mechanisms A Coulomb mechanism in plane strain is one in which polygonal blocks of material move rigidly relative to one another. The interfaces between the blocks may be regarded as very narrow zones in which the strain rates are very large. In a nondilatant material, only shearing takes place in such a zone, so that the movement is one of sliding, and the interfaces are just slip lines, as discussed in Section 5.1. In the presence of dilatancy, dilatation as well as shearing takes place, and the movement involves separation in addition to sliding.1 In fact, it can easily be shown (the details are left to an exercise) that the velocity discontinuity forms an angle equal to ψ with the interface – that is, if the magnitude of the discontinuity is v then the sliding speed is v cos ψ and the separation speed is v sin ψ. If the thickness of the zone is h, then the average longitudinal strain rate perpendicular to the interface is (v sin ψ)/h and the average shearing rate is (v cos ψ)/h, so that the principal strain rates are 21 (±1 + sin ψ)v/h. In the standard material, then, the plastic dissipation per unit area of interface is cv cos φ. In another type of mechanism, introduced by Petterson and developed by Fellenius, the velocity discontinuities are along circular arcs, with the material inside an arc rotating rigidly about the center of the circle and thus sliding past the remaining material. This mechanism, known as a slip circle, is clearly appropriate only for a nondilatant (e.g., Tresca) material. Nevertheless, like the Coulomb mechanism with pure sliding, it is often used regardless of material properties. Both the location of the center of the circle and its radius can be chosen so as to minimize the upperbound load predicted by the mechanism. In a standard Mohr–Coulomb material, a velocity discontinuity such that the mass on one side rotates rigidly while that on the other side remains stationary takes the form of a logarithmic spiral rather than a circle. As can be seen from Figure 6.1.7, dr/(r dθ) = tan φ, which can be integrated to give 1 In practice, soil mechanicians often use the Coulomb mechanism with pure sliding regardless of the yield criterion or flow rule assumed. Also, the mechanism is usually analyzed by means of statics rather than kinematics. For the Tresca material, the results are equivalent.
Section 6.1 / Limit Analysis of Plane Problems
349
r = r0 exp[tan φ(θ − θ0 )]. Clearly, for φ = 0, the curve becomes the circle r = r0 .
AA Q QA r dθ Q A r H j dθ H } Z dr* φ A
Figure 6.1.7. Velocity discontinuity in a standard Mohr–Coulomb material.
In accordance with Radenkovic’s theorems (see 3.5.1), any upper bound found for a standard Mohr–Coulomb material is also an upper bound for a nonstandard material with the same yield criterion, while any lower bound for a standard Mohr–Coulomb material whose angle of internal friction equals the dilatancy angle of the nonstandard material is also a lower bound for the latter. The following examples illustrate the procedure. The examples are limited to soils that can be modeled as homogeneous, a condition rarely encountered in real soil masses. For an extensive survey of applications of limit analysis to soil mechanics, including numerical results, see Chen [1975].
Stability of a Vertical Bank A vertical bank of height h occupies the halfstrip 0 ≤ y ≤ h, x ≥ 0. We wish to determine the maximum height so that the bank does not collapse. Since the weight of the bank per unit horizontal area is wh, where w is the specific weight, we may regard h as the equivalent of a load, and denote its greatest safe value by hU . A lower bound to hU may be found by assuming, with Drucker and Prager [1952], the stress field σx = τxy = 0, σy = −w(h − y), which satisfies the equilibrium equations and leaves the vertical and horizontal surfaces of the bank tractionfree. The greatest numerical value of σy , equal to wh, must not exceed the yield stress in uniaxial compression for the standard Mohr–Coulomb material with internalfriction
350
Chapter 6 / Problems in Plastic Flow and Collapse II
angle ψ, namely 0 σC
π ψ 2c cos ψ . = 2c tan + = 1 − sin ψ 4 2
If necessary — that is, if the bank is not situated atop a hard stratum — the stress field may be extended into the halfspace y ≤ 0 without violating the yield criterion as follows: (
σx = αwy,
τxy = 0,
σy =
−w(h − y), x > 0, wy, x < 0,
)
where α = (1 − sin ψ)/(1 + sin ψ). The stress field thus contains admissible discontinuities that separate it into three zones. For the standard Tresca √ material, the lower bound may be written as 2k/w. An improvement to 2 2k/w is achieved by means of an admissible stress field consisting of seven zones, proposed by Heyman [1973], who also discusses incomplete stress fields leading to somewhat higher lower bounds. A numerical solution by Pastor [1976] yields a lower bound of 3.1k/w. However, the stress fields producing these improvements include tensile stresses in some regions, while the Drucker–Prager stress field does not. Indeed, for a material that cannot take tension it was shown by Drucker [1953], on the basis of a mechanism including a tension crack , that 2k/w is an upper bound as well. y
6
h
?
r
)N v φ
k
β
k
x
Figure 6.1.8. Coulomb mechanism in a vertical bank. An upper bound for a Mohr–Coulomb material may be found with the help of the Coulomb mechanism shown in Figure 6.1.8, in which a wedge of angle β separates from the remainder of the bank. The weight (per unit thickness perpendicular to the page) of the wedge is W = 12 wh2 tan β, and if the magnitude of the velocity of the wedge is v, then its downward component is v cos(β + φ). Equating the external work rate to the internal dissipation, 1 2 wh tan β cos(β + φ)v = chv cos φ sec β, (6.1.4) 2
Section 6.1 / Limit Analysis of Plane Problems
351
produces the upper bound h=
2c cos φ . w sin β cos(β + φ)
The least upper bound is obtained by maximizing the denominator with respect to β: d [sin β cos(β + φ)] = cos β cos(β + φ) − sin β sin(β + φ) = 0, dβ or
π −β . tan(β + φ) = cot β = tan 2 The equation is obeyed if β = 14 π − 12 φ. But
π φ π φ cos sin − + 4 2 4 2
1 = (1 − sin φ), 2
and therefore hU ≤ 2σC /w (= 4k/w for a Tresca material). We are thus left with the wide limits, 2c π ψ tan + w 4 2
4c π φ tan + . w 4 2
≤ hU ≤
The mechanism based on the logarithmic spiral produces a slight improvement over that of Coulomb: the optimal spiral reduces the factor in the upper bound from 4 to 3.83.
Stability of a Simple Slope The improvement in the upper bound obtained by using a curved rather than a planar slip surface is significantly greater for inclined banks, known as simple slopes. It is conventional in soil mechanics to define the stability factor 1 Ns = whU /c, a function of the slope α as well as of the internalfriction angle φ. The optimal Coulomb wedge gives Ns =
4 sin α cos φ . 1 − cos(α − φ)
It was shown by Taylor [1937] that limitequilibrium calculations based on the logarithmic spiral are so close to those based on the slip circle as to be undistinguishable. Chen [1975] showed further that there is no significant difference between the results of the limitequilibrium method and upperbound limit analysis. Some examples are shown in Table 6.1.1. Very little work has to date been done on lower bounds in the limit analysis of slope stability. 1
Some authorities, including D. W. Taylor [1948], use the stability number m = 1/Ns instead.
352
Chapter 6 / Problems in Plastic Flow and Collapse II
Table 6.1.1. Stability Factors of Homogeneous Simple Slopes Failure Surface Plane Curved 4.00 3.83 6.28 6.03
α 90◦
φ 0◦ 25◦
75◦
0◦ 25◦
5.21 9.80
4.56 6.03
60◦
0◦ 25◦
6.93 17.36
5.24 12.74
Thrust on Retaining Walls If a vertical bank of soil is too high for stability — and in a cohesionless soil, any height is too great — then it must be held back by a retaining wall. The soil and the wall exert on each other a mutual thrust, equal to the resultant of the horizontal stress σx in the soil. Failure of the soil may occur when it is in one of two states, active and passive. In a passive failure, the wall moves into the soil, increasing the horizontal pressure until the yield criterion is reached in the soil. The thrust P is thus an increasing load on the soil mass, doing positive work, and its limiting value, known as the passive thrust and denoted Pp , is an ultimate load in the usual sense. In an active failure, the wall is pushed outward as a result of the horizontal pressure, and this pressure is reduced until the soil yields. In the process the thrust decreases and does negative work. If the limiting thrust (the active thrust) is denoted Pa , then the upper and lower bounds are bounds on −Pa , and the usual nomenclature of limit analysis must be reversed: the upperbound theorem gives a lower bound to Pa , and the lowerbound theorem gives an upper bound. The static analysis is due to Rankine. The geometry is taken as the same as in the preceding problem, Figure 6.1.8, and the wall is assumed smooth. Equilibrium is satisfied if σy = −w(h − y), τxy = 0, and σx depends on y only. The Mohr–Coulomb criterion is assumed to be met everywhere, that is, σx − σy  + sin φ (σx + σy ) = 2c cos φ. Two solutions exist for σx : 1 − sin φ cos φ − 2c 1 + sin φ 1 + sin φ φ π φ 2 π = σy tan − − 2c tan − , 4 2 4 2
σx = σy
Section 6.1 / Limit Analysis of Plane Problems
353
representing active failure, and 1 + sin φ cos φ + 2c 1 − sin φ 1 − sin φ π π φ φ 2 = σy tan + 2c tan , + + 4 2 4 2
σx = σy
representing passive failure. Introducing σy = −w(h − y) and integrating over 0 ≤≤ h gives the limiting thrusts, 1 π φ Pa = wh2 tan2 − 2 4 2
and
1 π φ Pp = wh2 tan2 + 2 4 2
π φ − 2ch tan − 4 2
+ 2ch tan
π φ . + 4 2
The preceding formulas, known as Rankine’s formulas, are widely used in soil mechanics. In view of Radenkovic’s second theorem, however, it must be recognized that they are not true lower bounds (in the usual sense for Pp , in the reverse sense for Pa ) unless the friction angle φ is replaced by the dilatancy angle ψ. Upper bounds can be obtained by means of the Coulomb mechanism, following Coulomb’s own analysis of 1776, but making sure that a kinematic approach with an associated flow rule is taken; Coulomb assumed pure sliding, and analyzed the wedge statically. For active failure, the mechanism is the same as for the freestanding vertical bank. With the wall again assumed to be smooth, the external rate of work is given by the lefthand side of (6.1.4) with the additional term −P v sin(β + φ), and the internal dissipation equals the righthand side. Consequently, 1 P = wh2 tan β cot(β + φ) − ch cos φ sec β csc(β + φ). 2 Both terms on the righthand side can be shown to be stationary at β = 1 π − 12 φ, so that the largest P (corresponding to the smallest upper bound 4 on −P ) is given by π φ 1 Pa = wh2 tan2 − 2 4 2
− ch cos φ sec
2
π φ − . 4 2
But π π φ cos φ = sin − φ = sin 2 − 2 4 2
so that cos φ sec
2
π φ − 4 2
π φ π φ = 2 sin − cos − , 4 2 4 2
π φ = 2 tan − , 4 2
354
Chapter 6 / Problems in Plastic Flow and Collapse II
and the Rankine formula for the active thrust is recovered. An analogous result is obtained for the passive thrust. Here the wedge moves upward and to the right, the velocity forming an angle β − φ with the vertical (details are left to an exercise). We thus see that the Rankine formulas give the correct limiting thrusts on a smooth wall for the standard Mohr–Coulomb material. For the nonstandard material, they furnish the Radenkovic bounds. The kinematic approach may be extended to obtain upper bounds in the presence of friction between the soil and the wall, by adding the term µP vy  to the internal dissipation, µ being an average coefficient of friction and vy the vertical component of velocity; it is assumed that the wall moves horizontally. While no analytical solutions exist, the wedge angle β giving the lowest upper bound can easily be found numerically for given µ, φ, and wh/c.
Exercises: Section 6.1 1. Find the best value of the wedge angle γ for the stress field of Figure 6.1.1(a). 2. Assume that the velocity discontinuity in Figure 6.1.1(b) is inclined at an arbitrary angle α. Find the upper bound to the cutout factor, and show that α = 45◦ gives the best upper bound. 3. Show that for a rectangular slab of sides 2a and 2b (b > a) with a slit of length 2βa parallel to the shorter side, the cutout factor for simple tension perpendicular to the slit is still 1 − β. 4. Find lower and upper bounds on the cutout factor for the slab in Exercise 1 when b < a. 5. Find the value of the load F corresponding to the slipline fields of Figure 6.1.4(a) for θ ≥ 75◦ . 6. Determine the velocity fields corresponding to the mechanisms of Figure 6.1.5(b) and (c) and the corresponding upper bounds to the collapse load F . 7. Derive Equation (6.1.2) for beams with h/L ≤ πτY /σY . 8. Derive Equation (6.1.3) for beams with h/L ≥ πτY /σY . 9. Find an upper bound to the critical height h of the bank of Figure 6.1.8 when the straight velocitydiscontinuity line is replaced by a logarithmic spiral (Figure 6.1.7).
Section 6.2 / Beams Under Combined Stresses
355
10. Derive the equations governing the upper bound to the passive thrust and the lower bound to the active thrust on a retaining wall in the presence of friction between the soil and the wall. 11. Assuming plane strain, use a stress field like that of Figure 5.1.5(e) to find a lower bound to the ultimate tensile force carried by the symmetrically notched tension specimen of Exercise 9, Section 5.1. Compare with the result of that exercise.
Section 6.2 6.2.1.
Beams Under Combined Stresses
Generalized Stress
Introduction A concept of great usefulness in the limit analysis of beams, arches, frames, plates and shells was introduced by Prager [1955b, 1956b, 1959]. It is that of generalized stress and strain. Consider the ideal sandwich beam as shown in Figure 3.5.1(a) (page 155), but subject to distributed loading so that the axial force P and bending moment M vary along its length. While M and P can no longer be regarded as generalized loads, they may be regarded as generalized stresses in the following sense. At any section of the beam, the stresses in the flanges are σ = P/2A ± M/Ah. The local values of the elongation and rotation obey the relations d∆ dθ = ε, = κ, dx dx where ε is the mean longitudinal strain and κ is the curvature. The strains in the flanges are ε ± hκ/2, and the internal virtual work can easily be shown to be Z L
(P δε + M δκ)dx,
δW int = 0
the span of the beam being 0 < x < L. The local axial force P and bending moment M may now be regarded as the generalized stresses, with ε and κ, respectively, as their conjugate generalized strains. Figure 3.5.1(a), in addition to representing the limitload locus for the beam under external axial force and moment, thus also represents the yield locus for the ideal sandwich beam. Such yield loci are also called interaction diagrams; an example was already studied in 4.4.1 (see Figure 4.4.5(a), page 224). The ideal sandwich beam is statically determinate in the sense of 4.1.1, since it has no range of contained plastic deformation: if the material is
356
Chapter 6 / Problems in Plastic Flow and Collapse II
perfectly plastic, then the beam can undergo unlimited deformation as soon as either flange yields. In any real beam, as we already know, the ultimate moment MU is greater than the elasticlimit moment ME , and therefore two distinct yield loci exist: the elasticlimit (or initial yield) locus and the ultimate yield locus [again, see Figure 4.4.5(a)]. Under the hypothesis of rigid–plastic behavior, however, only the ultimate yield locus is relevant.
Generalized Stress and Strain: Definitions Generalized stresses may coincide with the actual stresses, or they may be local stress resultants integrated over one or (as in the present example) two dimensions, or even over a whole finite element of the body (such as a bar in a truss). If the generalized stresses are denoted Qj (j = 1, ..., n), then the conjugate generalized strains qj are in general defined by δW int =
Z X n
Qj δqj dΩ,
Ω j=1
R
where Ω (·) dΩ describes integration over the entire body with respect to volume, area, or length, as appropriate, or summation over all finite elements.1 Let Q and q denote the generalized stress and strain vectors, respectively. As illustrated by the ideal sandwich beam, a yield locus in terms of generalized stresses, say Φ(Q) = 0, may be derived in exactly the same way as the limit locus in terms of generalized loads was derived in 3.5.1. For rigid–plastic materials, the generalized plastic dissipation is thus ¯ p = Q · q, ˙ D
(6.2.1)
and the principle of maximum plastic dissipation may be written as (Q − Q∗ ) · q˙ ≥ 0 or ¯ p (q) ˙ ≥ Q∗ · q˙ D
(6.2.2)
for any Q∗ such that Φ(Q∗ ) ≤ 0. Finally, the theorems of limit analysis may be restated as follows. LowerBound Theorem. A load point P is on or inside the limit locus if a generalized stress field Q∗ can be found that is in equilibrium with P and obeys Φ(Q∗ ) ≤ 0 everywhere. UpperBound Theorem. A load point P is on or outside the limit locus if a kinematically admissible velocity field, yielding the generalized velocity 1
In technical mathematical language, dΩ is a measure in a space of three, two, one or zero dimensions.
Section 6.2 / Beams Under Combined Stresses
357
vector p˙ ∗ conjugate to P and the generalized strainrate field q˙ ∗ , can be found so that Z ¯ p (q˙ ∗ ) dΩ. P · p˙ ∗ = D (6.2.3) Ω
Elastic and Plastic Generalized Strain When it is desired to describe elastic–plastic behavior in terms of generalized stress and strain, then it is necessary to decompose the generalized strain into elastic and plastic parts: q = qe + qp . But with the exception of some simple cases, there is in general no onetoone correspondence between qe and εe or between qp and εp . Consider, for example, a real (as distinct from ideal) beam subject to symmetric bending only; the moment M is the only generalized stress, and the curvature κ is the only generalized strain. The actual strain at a point is given by ε = −κy. In the elastic range, the momentcurvature relation is M = EIκ, and therefore the elastic part of the curvature is κe =
M . EI
The plastic strain is σ E 1 My p = −κ y − σ+ . E I
εp = ε − εe = −(κe + κp )y −
Thus, while 1 yεp dA, I A there is no inverse relation by which κp determines εp . The quantity σ + M y/I does not vanish in the range of contained plastic deformation, and neither does its time derivative. Consequently, κp = −
Z
Z
σ ε˙p dA 6= M κ˙ p ,
A
except when σ˙ = 0, a condition that implies that M˙ = 0 and hence κ˙ e = 0, and therefore holds only on the ultimate yield locus. It follows that the principle of maximum plastic dissipation in terms of generalized stress and generalized plastic strain is in general valid only under ˙ The exceptional cases are those in unrestricted plastic flow, with q˙ p = q. which no contained plastic deformation occurs locally, as at a section of an ideal beam, or in a bar carrying axial force only (truss member).
358
6.2.2.
Chapter 6 / Problems in Plastic Flow and Collapse II
Extension and Bending
Introduction The theory of symmetric pure bending of elastic–plastic beams, discussed in 4.4.1, can easily be extended to beams subject to an axial force P in addition to the bending moment M , provided the deflection is so small that the additional bending moment resulting from the axial force acting over the deflection (the socalled P∆ effect) is negligible. With this proviso satisfied, and with the uniaxial stressstrain relation given by σ = f (ε), the first of Equations (4.4.7) needs only to have its righthand side changed from 0 to P . As seen in 4.4.1, the problem of asymmetric bending is difficult even in the absence of axial force. An analysis of rectangular beams subject to axial force and bending moments about both axes was carried out by ShakirKhalil and Tadros [1973]. In the present subsection, only symmetric bending is considered. Consider a beam whose centroidal fiber coincides with the zaxis, whose crosssection is symmetric about the yaxis, and which is made of an elastic– perfectly plastic material. In bending in the yzplane, the strain is given as by Equation (4.4.2) with α = 0 (but with the axes renamed): ε = −κ(y−y0 ), so that κy0 = ε0 is the strain of the centroidal fibers or, equivalently, the average strain over the crosssection. In the elastic range, this strain is elastically related to the average stress P/A, that is, κy0 = P/AE. Since κ = M/EI regardless of the value of P , it follows that the coordinate y0 of the neutral axis is given by y0 = P I/M A, and the stress distribution is σ=
P My − . A I
Let the ycoordinates of of the extreme bottom and top fibers be y = −c1 and y = c2 , respectively. The magnitudes of the extreme values of the stresses are P P M c1 M c2 σ1 = + , σ = − , 2 A A I I and the elastic limit corresponds to max(σ1 , σ2 ) = σY , that is, P M M P max + , − = 1, PU ME1 ME2 PU
where PU = σY A,
ME1 = σY
I , c1
ME2 = σY
I . c2
If the section is doubly symmetric, then c1 = c2 = h/2 and ME1 = ME2 = ME = 2σY I/h. The elasticlimit locus is then simply P/PU  +
Section 6.2 / Beams Under Combined Stresses
359
M/ME1 1
@
ME2 /ME1
@ @
@ @ @
–1
@ @ 1
@ @ @
P/PU
@
@ @
@ –ME2 /ME1 @ –1
Figure 6.2.1. Elasticlimit locus for an asymmetric beam under combined bending and extension. M/ME  = 1, that is, it has exactly the same form as the yield locus of the ideal sandwich beam [Figure 3.5.1(b)] but with the elasticlimit moment ME replacing the ultimate moment MU .1 For a section without double symmetry, the elasticlimit locus is as shown in Figure 6.2.1 if c2 > c1 (so that ME1 > ME2 ). Note that for a certain ratio of P to M , namely P/M = (c2 − c1 )A/2I, yielding occurs simultaneously at the top and bottom fibers, and two plastic zones form as the generalized stress (M, P ) moves outside the elasticlimit locus. Otherwise only one plastic zone forms at first. As the point (M, P ) moves farther from the origin, the stress at the extreme fiber opposite the plastic zone increases until it, too, reaches the yieldstress value, creating a second plastic zone. Further loading results in the shrinking of the elastic core, exactly as in pure bending, until it becomes negligibly thin, indicating that the ultimate yield locus has been reached.
Yield Locus for Symmetric Bending In order to determine the ultimate yield locus, let us assume for the sake of definiteness that M > 0, so that the bottom fibers are in tension, with σ = σY , and the top fibers are in compression, with σ = −σY . If y0 is the 1
For the ideal sandwich beam, of course, ME = MU .
360
Chapter 6 / Problems in Plastic Flow and Collapse II
ycoordinate of the vanishing elastic core, then Z
y=y0
y dA −
M = −σY
Z
y=c2
and
Z
y dA
y dA = 2σY
y=y0
dA −
P = σY
(6.2.4)
y=y0
y=y0
y=−c1
y=c2
Z
y=−c1
Z
y=c2
dA
(6.2.5)
y=y0
y=c2 y dA = 0. For a given crosssection, the integrals in Equations since y=−c 1 (6.2.4)–(6.2.5) can be evaluated in terms of y0 , so that these equations furnish a parametric representation of the ultimate yield locus in the M P plane in terms of the parameter y0 , the range of y0 being −c1 ≤ y0 ≤ c2 .
R
Associated Flow Rule The principle of maximum plastic dissipation holds in states of uniaxial stress regardless of the yield criterion and flow rule obeyed by the material under multiaxial stress. Consequently the generalized strain rate (ε˙0 , κ) ˙ must be perpendicular to the yield locus in the M P plane, that is, ε˙0 dP + θ˙ dM = 0. Now consider Equations (6.2.4)–(6.2.5). If b(y) denotes the width of the beam at the level y, then dA = b(y)dy, and therefore dM = −2σY b(y0 )y0 dy0 ,
dP = 2σY b(y0 )dy0 ,
so that normality is equivalent to ε˙0 − y0 κ˙ = 0 — precisely the definition of ε˙0 .
Examples of Yield Loci In order to compare the behavior of different crosssections, it is convenient to describe the yield locus in terms of the dimensionless generalized stresses m = M/MU and p = P/PU , where PU = σY A (A being the total crosssectional area) and MU is given by Equation (4.4.11). The parameter can also be made dimensionless by defining, for example, η = 2y0 /h, where h = c1 + c2 is the depth of the beam; the range of η is thus −η1 ≤ η ≤ η2 , where ηi = 2ci /h, i = 1, 2. Equations (6.2.4)–(6.2.5) can therefore be written symbolically as m = m(η), ¯ p = p¯(η). (6.2.6) As an example, consider a rectangular beam of width b and depth h. It is easy to see that Equations (6.2.4)–(6.2.5) become h2 M = σY b − y02 4
!
Section 6.2 / Beams Under Combined Stresses
361
and P = 2σY by0 In dimensionless form, m = 1 − η2,
p = η,
so that in this case the yield locus can be described in explicit form, m = 1 − p2 , and forms a parabola. For a circular bar of radius a, it is more convenient to define η by η = −1 sin (y0 /a), so that its range is − 12 π ≤ η ≤ 12 π. The yield locus is given by p=
1 (2η + sin 2η), π
m = cos3 η.
If M is negative, it need only be replaced by −M (and m by −m) in all the results for doubly symmetric sections. Without double symmetry, P must also be replaced by −P (and p by −p). The yield loci for the rectangular and circular bars are shown as curves 1 and 2 in Figure 6.2.2. It is seen that they differ only slightly over the entire range. The yield locus for an Ibeam, on the other hand, can be expected to lie between the loci for the rectangular beam and for the ideal sandwich beam, and closer to the latter. Figure 6.2.2 also shows, as curve 3, the locus for the Ibeam shown in the adjacent picture. In practice, curved yield loci such as the one for the rectangular bar are often replaced, following Onat and Prager [1954], by piecewise linear approximations such as the one shown with dashed lines in Figure 6.2.2.1 Such approximations may also be regarded as the exact yield loci for certain idealized sections, which are in turn approximations to the true sections. The advantage of this point of view (see Hodge [1959], Section 73) is that a velocity field that gives generalized strain rates associated with the approximate yield locus may be easily visualized in the context of the idealized section. A frequently used yield locus for wideflange steel sections is given by 0.85m + p = 1, p ≥ 0.15, (6.2.7) m = 1, p ≤ 0.15.
Application: Collapse of a Semicircular Arch As an illustration of the use of the yield locus in terms of moment and axial force, we consider the pinnedended semicircular arch of radius a, loaded by a concentrated vertical force 2F at midspan, shown in Figure 6.2.3(a). 1
A general theory of plasticity with piecewise linear yield loci is due to Hodge [1957a].
362
Chapter 6 / Problems in Plastic Flow and Collapse II m 1.0 H
? H
6 16
H H H H H
0.8
 1
H
20
H J J 0.6
J1 J 1J 3
10
1
? 
2 ) J
0.4
J J J 0.2
J J J
0
0.2
0.4
0.8
0.8
J
1.0
p
Figure 6.2.2. Yield loci under combined bending and extension for rectangular beams (curve 1), circular beams (curve 2), and the Ibeam shown (curve 3). Dashed lines represent a piecewise linear approximation for rectangular beams. The vertical reactions at the supports are each equal to F by symmetry, but the horizontal reactions ±H are unknown. Let χ denote the angle between the resultant reaction and the vertical, so that tan χ = H/F . A freebody diagram of a segment of the arch is shown in Figure 6.2.3(b), and equilibrium shows that the axial force and moment are P (φ) = −F sin φ − H cos φ = −F (sin φ + tan χ sin φ) F =− sin(χ + φ), cos χ M (φ) = F a(1 − sin φ) − Ha cos φ Fa [cos χ − sin(χ + φ)]. = cos χ With the moment and axial force varying along the arch, it must be assumed that the yield criterion (whichever is chosen) is met only at certain critical sections. As in the case of transversely loaded beams discussed in 4.4.2, plastic hinges form at those sections. If a single hinge were to form in the arch, it would necessarily, because of symmetry, be at midspan. A threehinged arch, however, is a stable structure. Consequently, plastic collapse of the arch requires the formation of two additional plastic hinges, located
Section 6.2 / Beams Under Combined Stresses
363
symmetrically about the midpoint of the arch. The collapse mechanism is shown by the dashed curves in Figure 6.2.3(a); the arch segments between the hinges move as rigid bodies. 2F
? b
P (φ)
b
e
7 a q
S  M (φ) o S
b
φ
w e
4
4
(a)
(b)
H } Z χ 6 Z R Z/ P Z
Figure 6.2.3. Pinended circular arch: (a) initial geometry and loading (solid line) and collapse mechanism (dashed line); (b) freebody diagram of a segment. The location of the offcenter hinges can easily be determined by noting that both moment and axial force have local maxima only at φ = π/2 − χ, and therefore any convex combination of them also has a local maximum there. Collapse is thus determined by the requirement that the yield criterion Φ(M, P ) = 0 is met at φ = 0 and φ = π/2 − χ. Assuming a section with double symmetry so that Φ(M, P ) = Φ(M , P ), we can find χ and the value of F at collapse by solving simultaneously Φ(F tan χ, F a1 − tan χ) = 0
and Φ(F sec χ, F a(sec χ − 1)) = 0.
The choice of a nonlinear yield criterion necessitates the simultaneous solution of two nonlinear equations, a task that may be unpleasant. With a piecewise linear yield criterion, on the other hand, once the side of the polygon is chosen that is appropriate for each equation, the equations are linear in F . Eliminating F , a quadratic equation in cos χ or sin χ is obtained. For simplicity, the square yield locus corresponding to the ideal sandwich section will be used. With the help of the dimensionless quantity η = MU /PU a, the equations to be solved are [1 − tan χ + η tan χ]F a = MU , [(1 + η) sec χ − 1]F a = MU . Consequently χ satisfies 1 − tan χ + η tan χ = (1 + η) sec χ − 1. It can immediately be seen that if tan χ > 1, then tan χ = secχ, or χ = π/2, so that the additional plastic hinges coincide with the central
364
Chapter 6 / Problems in Plastic Flow and Collapse II
hinge, and no collapse is possible. It is necessary, then, that tan χ < 1. For . η negligibly small, tan χ is very nearly 3/4 and therefore FU = 4MU /a — a result equivalent to neglecting the influence of axial forces. For η small but not negligible, a firstorder approximation in η may be effected, leading . . to tan θ = 3/4 − 5η/16 and FU = (4MU /a)/(1 + 4.25η). Other examples of arch collapse based on piecewise linear yield loci were studied by Onat and Prager [1953, 1954]; see also Hodge [1959], Section 74.
6.2.3.
Combined Extension, Bending and Torsion
In a bar under a combination of axial force, bending moment, and torque, the nonvanishing stress components are σz , τxz , and τyz , with τxz = ∂φ/∂y and τyz = −∂φ/∂x, φ being the stress function. Any point of the bar is in a state of plane stress in the plane that "is perpendicular to ∇φ; the # σ τ state of stress in that plane can be given by , where σ = σz and τ 0 q
2 + τ 2 . Both the Mises and the Tresca yield criteria are τ = ∇φ = τxz yz given by Equation (3.3.5):
σ σY
2
+
τ τY
2
= 1.
Since σij ε˙ij = σ ε˙ + τ γ, ˙ the associated flow rule may be obtained from the maximumplasticdissipation principle as σ ε˙p = λ˙ 2 , σY
τ γ˙ p = λ˙ 2 , τY
(6.2.8)
and the plastic dissipation is ˙ = Dp (ε)
q
(σY ε) ˙ 2 + (τY γ) ˙ 2.
(6.2.9)
Lower Bound A lowerbound yield locus for combined extension, bending, and torsion can be found by generalizing an approach proposed by Hill and Siebel [1951] for combined bending and torsion only. The approach is based on assuming, on the one hand, the same distribution of normal stress as in 6.2.2, but with σ = ασY , where 0 ≤ α ≤ 1; and on the other hand, √ the same distribution of shear stress as in fully plastic torsion, but with τ = 1 − α2 τY . The second assumption leads immediately to def
t=
p T = 1 − α2 . TU
The first assumption means that the mp relation would be given by (6.2.6) if m and p were defined as M/αMU and P/αPU , respectively. With the
Section 6.2 / Beams Under Combined Stresses
365
standard definitions, the relation is therefore p = p¯(η), α
m = m(η). ¯ α
Eliminating α, we can describe the yield surface in mptspace in terms of the single parameter η: p=
p
1 − t2 p¯(η),
m=
p
1 − t2 m(η). ¯
For the rectangular beam, we have the explicit description m=
p
1 − t2 − √
p2 . 1 − t2
The projections of this surface on both the mt and ptplanes are unit circles.
Upper Bound An upperbound yield curve for combined extension, bending and torsion can be found following the method of Hill and Siebel [1953]. The assumed velocity field is taken so that it results only in an extension rate ε˙0 of the centroidal fiber, a pure curvature rate κ˙ about the centroidal axis, and a rate of twist θ˙ about the centroid; warping is neglected.1 With symmetric bending in the yzplane assumed, the strain rates are ε˙z = ε˙0 − κy, ˙ where r =
˙ γ˙ θz = rθ,
p
x2 + y 2 . The plastic dissipation is therefore q
˙ r2 + (αy − β)2 , Dp (ε˙ ∗ ) = τY θ ˙ and β = (σY /τY )(ε˙0 /θ). ˙ where α = (σY /τY )(κ/ ˙ θ) A simple way of finding the upperbound generalized stresses corresponding to the assumed velocity field is to determine the stresses that are related to it by the associated flow rule and that obey the yield criterion — but that do not, in general, form a statically admissible stress field — and then to calculate their resultants. The associated flow rule (6.2.8) produces the stresses σ2 σ = Y (ε˙0 − κy) ˙ = −µσY (αy − β) λ˙ and τ = µτY r, 1
A correction for warping, resulting in better upper bounds for noncircular sections, is due to Gaydon and Nuttall [1957].
366
Chapter 6 / Problems in Plastic Flow and Collapse II
˙ λ˙ is a function of position where τ = τzθ (so that τrz ≡ 0),1 and µ = τY θ/ that can be determined by requiring that the yield criterion (3.3.5) be obeyed everywhere, resulting in 1 . + (αy − β)2
µ= p
r2
The stress resultants M , P and T are therefore given by M =−
Z
y2 dA, r2 + (αy − β)2
Z
yσ dA = ασY A
p
A
Z
Z
P =
σ dA = βσY A
A
Z
T =
Z
rτ dA = τY A
A
p
r2
1 dA, + (αy − β)2
(6.2.10)
r2 dA. r2 + (αy − β)2
p
The integrations in Equations (6.2.10) may be performed, numerically if necessary, to yield a parametric representation of the upperbound yield surface in mptspace in terms of the parameters α and β. Computed yield curves representing the projections of the lowerbound and upperbound yield surfaces in the mt and ptplanes, are shown in Figure 6.2.4(a) and (b) for a circular and a square bar, respectively.
Extension and Torsion of a Circular Bar For a circular bar, the upperbound solution presented above is, in fact, a complete solution, since an axisymmetric shearstress distribution τθz = τ (r), τrz = 0 is statically admissible. A closedform result can be obtained for extension and torsion alone, that is, for α = 0. We define the dimensionless parameter ζ = β/a, where a is the radius of the bar. Equations (6.2.10)2,3 give p=
2π ζaσY σY πa2
Z 0
and 2π τY 2 τ πa3 3 Y
t= or p = 2ζ
q
ζ2
Z 0
+1−ζ ,
a
a
r dr =ζ ζ 2 a2 + r2
r3 dr 3 = 2 2 2 2 ζ a +r
p
a
Z
p
0
Z 0
dx x + ζ2
p
1
x dx , x + ζ2
p q
t = 2ζ 3 − (2ζ 2 − 1) ζ 2 + 1.
(6.2.11)
The first of Equations (6.2.11) can be rewritten as q
p + 2ζ 2 = 2ζ ζ 2 + 1. 1
Thus the traction boundary conditions are not satisfied for any but a circular bar.
Section 6.2 / Beams Under Combined Stresses
367
m,p
6 Upper bound (exact)
Upper bound
1.0
@ R @
pt
0.8
@ I @
Lower bound
mt
Lower bound
0.6 0.4 0.2
t
1.0
0.8
0.6
0.4
0.2
0 0
0.2
0.4
0.6
0.8
1.0
t
(a) m,p
6 Upper bound pt
1.0
A U A
mt 0.8
@ I @
Lower bound
0.6 0.4 0.2
t 1.2
1.0
0.8
0.6
0.4
0.2
0 0
0.2
0.4
0.6
0.8
1.0
t
1.2
(b)
Figure 6.2.4. Lowerbound and upperbound yield loci under bending, torsion and extension: (a) circular bar; (b) square bar. Squaring both sides, we find 4ζ 4 + 4ζ 2 = 4ζ 4 + 4ζ 2 p + p2 , or 4ζ 2 (1 − p) = p2 , which can immediately be solved for ζ: p ζ= √ . 2 1−p Substituting in the equation for t, we obtain the explicit relation p 1 t = (2 + p) 1 − p. 2
Squaring both sides of this equation, we may rewrite it as t2 + p 2 = 1 +
p2 − p3 , 4
a form that is convenient for determining the extent to which the present upperbound yield curve differs from the previously found lower bound, described by the unit circle. The righthand side of the last equation has its
368
Chapter 6 / Problems in Plastic Flow and Collapse II
maximum at p = 2/3, its value there being 28/27. Consequently the distance of the ppoints on the dimensionless yield curve from the origin lies between 1 and 28/27 = 1.018, and the curve differs only slightly from the circle. The stress distribution giving rise to the resultants just obtained can also be determined as the solution of a constrained extremum problem: find the stresses satisfying (3.3.5) everywhere such that the torque, Z
T =
rτ dA, A
is maximum for a given axial force, Z
P =
σ dA. A
Substituting for τ by solving (3.3.5), the problem may be written as Z
τY δ
q
r 1 − (σ/σY
)2 dA
Z
+νδ
σ dA = 0, A
A
where ν is a Lagrangian multiplier, or Z " A
(σ/σY )r β−p 1 − (σ/σY )2
#
δσ dA = 0,
where β = νσY /τY . There being no further constraint on the distribution of σ, the quantity in brackets under the integral sign must be zero, that is, β σ =p 2 , σY β + r2 and the yield criterion is satisfied everywhere if and only if τ r =p 2 . τY β + r2 Integration leads immediately to p and t given by Equations (6.2.11), with ζ = β/a as before.
Bending and Torsion of a Bar of Arbitrary CrossSection A complete solution for combined bending and torsion of a fully plastic bar of arbitrary crosssection may be obtained by integrating numerically a nonlinear partial differential equation first derived by Handelman [1944]. The stress function φ(x, y) is now regarded as unknown, and it is to be found so that it maximizes the bending moment for a given torque (or vice versa). For doubly symmetric bending in the yzplane, we have M=
σY τY
Z A
q
y τY2 − (∂φ/∂x)2 − (∂φ/∂y)2 dA.
Section 6.2 / Beams Under Combined Stresses
369
The constrained extremum problem may therefore be written as Z A
q
y δ τY2 − (∂φ/∂x)2 − (∂φ/∂y)2 − ν δφ dA = 0,
where ν is again a Lagrangian multiplier. Since φ = 0 and hence δφ = 0 on the boundary, integration by parts leads to Z ∂ y∂φ/∂x q 2 2 2 A ∂x τY − (∂φ/∂x) − (∂φ/∂y) ∂ y∂φ/∂y + ν δφ dA = 0. q + ∂y 2 2 2
τY − (∂φ/∂x) − (∂φ/∂y)
Since φ is unconstrained in the interior of A, the contents of the curly brackets must vanish everywhere, and this furnishes the required partial differential equation for φ, an elliptic equation subject to the boundary condition φ = 0. Different values of ν give different ratios of M to T . The equation was solved numerically for a square crosssection by Steele [1954], and for other crosssections by Imegwu [1960], who showed that the interaction diagram in the mtplane is remarkably insensitive to crosssectional shape.
6.2.4.
Bending and Shear
In the problems involving combinations of bending moments, axial force and torque that have been considered so far in this section, these stress resultants are independent of one another as far as the equilibrium of the beam is concerned, and therefore their interaction may be rigorously studied on a purely local basis. In particular, for the purpose of lowerbound analysis, if a statically admissible stress distribution is found for each such resultant separately, then a linear combination of such stress distributions is also statically admissible. If a beam is subject to transverse loading, then this loading determines both the shear force V and the bending moment M , which are therefore related to each other by the equilibrium equation dM = V. dz Strictly speaking, then, M and V are not generalized stresses that can be specified independently of each other. Indeed, each case of a transversely loaded beam presents a distinct problem of limit analysis. As discussed in 6.1.2, even such closely related cases as the endloaded cantilever and the centerloaded simply supported beam are different. If the spantodepth ratio is sufficiently high, however, the limit
370
Chapter 6 / Problems in Plastic Flow and Collapse II
loads tend to those predicted by the elementary plastichinge mechanism — that is, the overall collapse of the beam is almost completely determined by local behavior at a critical section. It thus becomes reasonable to formulate an approximate local yield locus, in terms of M and V , that governs local behavior, analogous to the local yield loci found above. The problem of limit analysis of an arbitrarily loaded beam then reduces to the determination of the critical section or sections; this problem is studied in 6.3.2. The particular problem of the endloaded cantilever may be used as the test problem for studying the local yield locus, as discussed by Drucker [1956]. Here, the problem has already been investigated from two points of view: in 4.5.2 as the limit of elastic–plastic bending, and in 6.1.2 as a problem in plane limit analysis. The latter approach, as was indicated there, gives both upper and lower bounds for the collapse load of the beam. The former approach, as is shown next, furnishes a lower bound.
Lower Bound as Limit of ElasticPlastic Solution We saw in 4.5.2 that as the elastic core shrinks under the influence of an increasing moment, the maximum shear stress there grows until it also reaches the yield value, after which a secondary plastic zone forms in which τ  = τY , σ = 0. Between this central plastic zone and each of the two outer plastic zones is an elastic zone in which, going from inside to outside, the normal stress increases linearly in magnitude from 0 to σY , and the shear stress decreases (parabolically in a rectangular beam or in the web of an Ibeam) from τY to zero. The limiting state is, of course, one in which the elastic zones shrink to vanishing thickness. This limit does not represent, strictly speaking, a statically admissible stress field, since it includes a discontinuity in τ . Since, however, the discontinuity occurs at two isolated points, equilibrium of any finite element is not violated and the stress distribution is acceptable. If the width of the plastic zone is c, then V = τY bc and M = σY b(h2 − c2 )/4. Defining v = V /VU , where VU = τY A, we immediately obtain the dimensionless interaction curve given by m = 1 − v2. This curve has clearly the same form as the one previously found for the interaction between moment and axial force, with v replacing p. In fact, it can be shown that for any doubly symmetric section the yield locus in the mvplane is given parametrically by m = m(η), ¯
v = p¯(η),
where m ¯ and p¯ are the same functions as in Equation (6.2.6). The proof is based on the observation that the stress distribution for combined bending moment and axial force, shown in Figure 6.2.5(a), is the superposition of those shown in Figure 6.2.5(b) and (c). However, the stress distribution
Section 6.2 / Beams Under Combined Stresses
371
(b) alone produces the same moment as (a), and the stress distribution (c) alone produces the same axial force as (a). If, now, (c) represents a block of shear stress rather than normal stress, then it produces a shear force, rather than an axial force, by exactly the same formula. When suitably nondimensionalized, therefore, the shear force is exactly the same function of the depth of the central zone as is the axial force.

=

+ 
(a)
(b)
(c)
Figure 6.2.5. Fully plastic stress distribution at a beam crosssection under combined bending moment and axial force. In a rectangular cantilever of length L carrying a concentrated transverse force F at its tip, collapse occurs when a plastic hinge forms at the builtin end. At this point M = F L and V = F . Defining f = F L/MU , we find that the lower bound based on Figure 6.2.5(bc) predicts
f =1−
σY h 2τY 2L
2
f 2,
a quadratic equation for f that can be solved explicitly for f . Assuming the Tresca criterion (σY = 2τY ) and defining δ = h/2L, we can write the solution as 1 p 1 + 4δ 2 − 1 . (6.2.12) f= 2 2δ
Upper Bound: Hodge Approach The generalized strain rates conjugate to M and V are the curvature rate κ˙ and the shear rate γ, ˙ respectively. The strainrate components conjugate to the stresses σ and τ are ε˙ = −κy ˙ and γ. ˙ Given κ˙ and γ, ˙ the associated flow rule (6.2.8) produces the stresses σ=−
σY2 κy, ˙ λ˙
τ=
τY2 γ. ˙ λ˙
Satisfaction of the yield criterion (3.3.5) requires λ˙ =
q
q
(τY γ) ˙ 2 + (σy κy) ˙ 2 = τY γ˙ 1 + νy 2 ,
372
Chapter 6 / Problems in Plastic Flow and Collapse II
where ν = σY κ/τ ˙ Y γ. ˙ The stresses are therefore νσY y , 1 + ν 2y2
τY τ=p . 1 + ν 2y2
σ = −p
(6.2.13)
The stress resultants are accordingly given in terms of the parameter ν as y2 dA, 1 + ν 2y2
Z
M = νσY A
Z
V = τY A
p
1 dA. 1 + ν 2y2
p
b

? 6
a
6
h
 c
?
Figure 6.2.6. Ibeam: geometry. Hodge [1957b] evaluated the integrals in the preceding equations for the Ibeam shown in Figure 6.2.6. If c/b and a/h are small, then the parametric form of the yield locus in dimensionless form is, after neglecting terms of order higher than the first in these quantities, m=
2 tanh ω + j(coth ω − ωcsch 2 ω) , 2+j v=
sech ω + jωcsch ω , 1+j
where ω = sinh−1 (νh/2), while j = ch/2ab is a dimensionless shape parameter. The limiting cases j = 0 and j = ∞ correspond, respectively, to the ideal Ibeam (with finite flange thickness but negligible web thickness) and the rectangular beam. The calculated interaction curves are shown in Figure 6.2.7. Hodge also derived the same stress distribution by solving the constrained extremum problem, as in 6.2.3. On this basis Hodge regards the yield locus as also providing a lower bound. However, the shear stress given
Section 6.2 / Beams Under Combined Stresses
373
v 1.0
Rectangular beam (j = ∞)
0.8
Ideal Ibeam (j = 0)

0.6
* Ibeam (j = 1)
0.4
0.2
0 0
0.2
0.4
0.6
0.8
1.0
m
Figure 6.2.7. Interaction curves for Ibeam (Hodge [1959]). by (6.2.13)2 does not vanish at the extreme fibers, and it therefore appears difficult to accept the stress distribution as statically admissible. Plots of the lowerbound curve defined by Equation (6.2.12), the upperbound curve due to Hodge [1957b], and the lowerbound and upperbound curves due to Drucker [1956] (see 6.1.2) are shown in Figure 6.2.8. It can be seen that all the curves have the limit f = 1 as δ → 0, so that the effect of shear is negligible for beams that are not overly deep, and that all tend asymptotically to the hyperbola f = 1/δ for δ large. It must be remembered, however, that values of δ greater than about 0.5 cannot reasonably be regarded as describing beams.
Exercises: Section 6.2 1. Using the assumptions of elementary beam theory, derive an expression for the internal virtual work in a beam of arbitrary crosssection subject to a variable bending moment M and axial force P . 2. Find the ultimate yield locus for a beam having the idealized section of Figure 3.5.2. 3. For a beam whose crosssection is an isosceles triangle, find the ultimate yield loci for combined axial force and bending moment (a) perpendicular and (b) parallel to the axis of symmetry. 4. Analyze the collapse of a semicircular arch of ideal sandwich section
374
Chapter 6 / Problems in Plastic Flow and Collapse II f 1.0 0.8 0.6 0.4 0.2 0 0.01
0.02 0.05 0.1 0.2 0.5 1.0 Upper bound, Hodge Lower bound, Eq. (6.2.12) Twodimensional theory (Fig. 6.1.6)
2.0
5.0
10.0
δ
Figure 6.2.8. Lowerbound and upperbound curves under combined bending and shear of a rectangular beam, load against depthspan ratio. that is built in at the supports and carries a concentrated load 2F at the vertex. 5. Analyze the collapse of a symmetric simply supported arch of ideal sandwich section, forming a circular segment of angle 2α, and loaded by (a) a concentrated load 2F at the vertex, (b) a uniform vertical load of intensity q, and (c) a uniform radial load of intensity q. 6. Show that for combined torsion and axial force or bending moment of a circular bar, the unit circles are lower bounds to the yield loci in both the pt and mtplanes. 7. Find a result analogous to (6.2.12) for an endloaded cantilever of circular crosssection with radius a, letting δ = a/L. 8. Evaluate the integrals following Equation (6.2.13) for a rectangular crosssection. Compare with the cited result of Hodge [1957b] for j = ∞.
Section 6.3 6.3.1.
Limit Analysis of Trusses, Beams and Frames
Trusses
A truss is an assemblage of stiff bars that are more or less flexibly connected to one another at their ends. In an ideal truss, the connection is through frictionless pins, with the center of each pin coinciding with the intersection
Section 6.3 / Limit Analysis of Trusses, Beams and Frames r = −1
>Ar
r=0
rB
>Ar
375
r=0
rB
>
[email protected] rB
@ @
>Dr
rC
>Dr
(a)
rC
fr
D
(b)
r=1 A r
A r
rB
>@
@
@ @
>Dr
(c)
r=1
rB
>@
@ @rC
@ @rC (d)
>Dr
@ @ @rC (e)
Figure 6.3.1. Some simple trusses.
of the centroidal lines of the bars meeting there. Moreover, all the loads are applied at the joints. Consequently, all bars carry axial forces only, and if n is the number of bars, then the bar forces P1 , . . . , Pn in effect constitute the stress field. In order for each pin to be in equilibrium, the vector sum of all the bar forces in the members connected through that pin must be zero. If the number of joints is j, then the total number of joint equilibrium equations is 3j, unless all the bars and loads lie in the same plane, in which case the truss is a plane (or planar ) truss and the number of equations is 2j. A nonplane truss is usually called a space truss. The unknowns of the problem, in addition to the bar forces, are the reaction components, s in number. If n + s = kj (where k = 2 or 3 in the plane truss or space truss, respectively), then the equilibrium equations are precisely enough to determine the unknowns, and the truss is statically determinate (or isostatic). If r = n + s − kj is positive, then the truss is statically indeterminate (or hyperstatic or redundant), and r is called the degree of static indeterminacy (or, more simply, the indeterminacy number or redundancy number ). If this number is negative, then the truss is unstable (or hypostatic) and is, in fact, a mechanism. In a stable truss, the number s of reaction components must be at least equal to the number of equilibrium equations for the truss as a whole, three for the plane truss and six for the space truss. If s is greater than this number, then the truss is externally indeterminate. Some simple trusses, with r equal to 0, −1 and 1 are shown in Figure 6.3.1. In particular, the truss in (e) is statically indeterminate of degree one even though, apparently, r = 6 + 4 − 2·4 = 2. In fact, bar AD cannot deform
376
Chapter 6 / Problems in Plastic Flow and Collapse II
and therefore cannot carry any force. This bar may, as a result, be ignored in any analysis of the truss.
Limit Analysis of Trusses A truss member will be said to fail if it can undergo significant lengthening or shortening with no significant change in the bar force. Failure in this sense can result from yielding, if the material is perfectly plastic or nearly so, or, in the case of a compression member, from buckling. Since the bar force in a failed member is no longer determined by equilibrium but by the failure criterion, it can be presumed as known if the properties of the bar are known, and the number n of unknown bar forces drops by one, as does the indeterminacy number r. The truss therefore becomes unstable if r + 1 bars fail. In particular, a statically determinate truss collapses as soon as one bar fails. Any choice of r+1 bars that fail provides a mechanism with one degree of freedom that can be used with the upperbound theorem. Given a reference ˙ i of the ith failed bar may be determined velocity v, the elongation rates ∆ + by geometry. Let PU i denote the ultimate bar force in tension, and PU−i the magnitude of that in compression; the latter is the lesser of the yield force ˙ i , and the buckling force. The internal dissipation in a failed bar is PU±i ∆ ˙ the superscript sign being that of ∆i . The truss of Figure 4.1.1 has three bars, six reaction components, and four joints, so that r = 1 and two bars must fail for collapse to occur. In 4.1.4 we read, however, that all three bars must fail for this truss to collapse. With PU+ the same in all three bars, the collapse load in this case is FU = PU+ (1 + 2 cos α). If we were to assume a mechanism in which bars AD and CD fail, while BD remains rigid, the external work rate would be zero and the upperbound theorem would fail to give a finite upper bound to FU . Consider, now, an asymmetric mechanism with bars BD and CD only failing. Bar AD then rotates rigidly about its support, and if the downward component of the velocity of pin D is v, then its leftward component is v cot α. The velocity component in the direction of bar CD, equal to its elongation rate, is v(cos α + cot α sin α) = 2v cos α. Equating the external work rate to the total internal dissipation, F v = PU+ v(1 + 2 cos α), leads to the an upper bound equal to FU . The equality can be explained as follows: suppose that the symmetry of the system is disturbed ever so slightly (e.g., by giving the load a small leftward component or by making bar CD just a little bit weaker than AD). The correct collapse mechanism would then, indeed, be the asymmetric one just considered. But a minimal asymmetry should not significantly affect the collapse load calculated on
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
e @ e @
[email protected] [email protected] @ e
e @ e @
[email protected] [email protected] @ e
(i)
(ii)
@ @ @ @ hhhh h @
(iv)
hh @ hhh @ @ @ @ (v)
377
@ @ @ @
[email protected] h (iii)
hhhh h @ @ @ @
[email protected] h (vi)
Figure 6.3.2. Collapse mechanisms for the truss of Figure 6.3.1(d).
the basis of assumed symmetry, and hence the collapse loads given by the symmetric and asymmetric mechanisms should be the same. Let us now look at the possible collapse mechanisms of the truss of Figure 6.3.1(d) under a downward force F applied at joint C. First, it is apparent that any mechanism in which bars AC and CD do not deform does not permit any translation of C, so that the force F cannot do any work; such a mechanism is not admissible. A mechanism in which both AC and CD fail but the other bars remain rigid allows rotation of BC about B, leading to a zero external work rate for the given loading. The only mechanisms to be considered, therefore, are those in which either AC or CD fails, but not both; these mechanisms number six, and are shown in Figure 6.3.2. Dashed lines represent bars that fail. We assume that the bars are of identical crosssection and sufficiently stiff so that PU+ = PU− = PU in every bar. The mechanism (i) in which CD and BC fail presents a rigid rotation of AC about A; if the downward velocity of C is v, then the angular velocity of rotation of AC is v/a, where a is the length of the nondiagonal bars, so that the shortening rate of CD and the lengthening rate of BC are also v. The total internal dissipation is thus 2PU v, and the resulting upper bound on F is 2PU . If (ii) CD and AB fail, then AC rotates about A, BD rotates about D, and BC rotates about its midpoint. The shortening rate of CD is again v, as is the lengthening rate of AB, and the upper bound is once more 2PU . The mechanisms in which AC fails along with either (iii) BC or (iv) AB, and the one √ (v) in which CD and BD fail, all give the same upper bound of (1 + 1/ 2)PU . Finally, in the shear mechanism (vi) in which AC and √ BD fail, these bars lengthen and shorten, respectively, at the rate v/ 2,
378
Chapter 6 / Problems in Plastic Flow and Collapse II
√ leading to the upper bound 2PU . This upper bound, being the smallest, must equal the ultimate load. To confirm this equality, we analyze the truss statically under this value of F , assuming that PAC = PU√and PBD = −PU . We find that all the other bar forces are of magnitude P/ 2, so that the “stress field” (the distribution of bar forces) is plastically admissible. It is clear that if the crosssectional areas of all three nondiagonal bars √ were √ to be reduced by a factor of 2, their ultimate bar forces would fall to 1/ 2 times those of the diagonals, and the stress field would still be — just barely — plastically admissible under the justcalculated collapse load. Collapse would then occur with all bars yielding, indicating the most efficient use of material; such a truss would be an example of minimumweight design. A kinematic analysis of the minimumweight truss shows that all six mechanism based on failure in two bars produce the same upper bound. The most general collapse mechanism, then, is a linear combination of the six. It is easy to see that this mechanism has four degrees of freedom, represented by the horizontal and vertical displacements of joints B and C.
Limit Design of Trusses The design of structures on the basis of limit analysis is known as limit design. Limit design for minimum weight is particularly simple for trusses in which no bars buckle, because the weight of a bar is directly proportional to its area, and hence to its strength. Let the ultimate bar force of the ith bar be PU i , and its length Li . In minimumweight design, the object is then to minimize n X
PU i Li
i=1
subject to inequality constraints on the PU i , ensuring that the truss is strong enough to carry the prescribed load. The problem is one of linear programming; it is discussed in its general form after a study of the present example. Suppose, for simplicity, that PU (AB) = PU (BC) = PU (CD) = PU 1 and PU (AC) = PU (BD) = PU 2 . We are thus led to minimize √ 3PU 1 + 2 2PU 2 subject to the following inequalities: 2PU 1 ≥ F,
PU 2 PU 1 + √ ≥ F, 2
√
2PU 2 ≥ F ;
in this elementary case the six mechanisms furnish only three independent inequalities, and the second of the three is redundant, since it is satisfied
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
379
whenever the other two are. The solution is simple, as √ we already know: all the inequalities are satisfied as equalities when PU 2 = 2PU 1 = F/2.
LinearProgramming Formulation of Limit Design If a truss has n bars, then the number of different combinations of r + 1 bars — that is, the number of different mechanisms — is m=
n! . (n − r − 1)! (r + 1)!
Let v denote a positive reference velocity in the kth mechanism (k = 1, . . . , m), such that the elongation rate of the ith bar in this mechanism is αik v, and the velocity conjugate to the applied force Fj (j = 1, . . . , l) is βjk v. According to the upperbound theorem, then, n X i=1
αik PU i ≥
l X
βjk Fj ,
k = 1, . . . , m.
(6.3.1)
j=1
The problem of minimumweight design of a truss is then one of minimizing the linear function G(PU 1 , . . . , PU n ) =
n X
Li PU i
i=1
subject to the linear constraints (6.3.1); this problem is one of linear programming. The connection between limit design and linear programming was apparently first noted by Heyman [1951]. The standard linearprogramming problem is one of maximizing, rather than minimizing, the objective function cT x, where c and x are 1 × n column matrices, subject to the constraints aTk x ≤ bk ,
k = 1, . . . , m,
(6.3.2)
where the ak are 1 × n column matrices, and the bk are real numbers. Often the additional constraint that the xi be nonnegative is imposed. The problem of minimumweight design of a truss becomes a standard problem if we identify xi with PU i , ci with −Li , ak with the kth column of the matrix −[αik ], and −bk with the righthand side of (6.3.1). By defining the m × n matrix A through AT = [a1 , . . . , am ] and the m × 1 matrix b through b = (b1 , . . . , bm ), inequality (6.3.2) may be rewritten in the short form Ax ≤ b,
(6.3.3)
x ≥ 0.
(6.3.4)
and the additional constraint as
380
Chapter 6 / Problems in Plastic Flow and Collapse II
In an alternative formulation of the linearprogramming problem, the constraint conditions (6.3.3)–(6.3.4) are replaced by Ax = b,
x ≥ 0.
(6.3.5)
An efficient numerical solution method due to Dantzig, called the simplex algorithm, exists for the problem in this form (see Dantzig [1963]). The constraints (6.3.3)–(6.3.4) can be converted to the form (6.3.5) by introducing the slack variables yk (k = 1, . . . , m), which form the m × 1 matrix y, and rewriting (6.3.3) as Ax + y = b,
y ≥ 0.
(6.3.6)
¯ is now defined by x The (n + m) × 1 matrix x ¯i = xi (i = 1, . . . , n) and ¯ is similarly defined by x ¯n+k = yk (k = 1, . . . , m). The m×(n+m) matrix A ¯ ¯ Aki = Aki (i = 1, . . . , n) and Ak,n+j = δjk (j = 1, . . . , m). The constraint inequalities (6.3.4) and (6.3.6) together can now be written as ¯ x = b, A¯
¯ ≥ 0, x
a form identical with (6.3.5).
6.3.2.
Beams
Any transversely loaded beam, except an ideal sandwich beam, is statically indeterminate in the sense of Section 4.1 — that is, the stress field cannot be deduced from the loading independently of unknown properties: at any section, an infinity of stress distributions can be found that give the same resultant moment M and shear force V . It is conventional, however, to call a beam statically determinate (or indeterminate) if it is externally determinate (or indeterminate) in the same sense as a truss, that is, if the number of independent reaction components is the same as (or greater than) the number of equilibrium equations available to determine them. In the absence of internal hinges, this number is three for plane bending. Any hinge, whether frictionless or a plastic hinge, provides an additional equilibrium equation: at a frictionless hinge, M = 0, since such a hinge cannot transmit moment, while at a plastic hinge M = MU+ or M = −MU− . The indeterminacy number of a beam is accordingly r = s − h − 3, where s is the number of reaction components1 and h is the number of hinges. Like a plane truss, the beam collapses when r is reduced to −1, so that if h0 hinges are present initially, the number of plastic hinges required for collapse is s − h0 − 2, and specifically, one if the beam is statically determinate, and two or more if it is statically indeterminate. A plastic hinge may form at any point of the beam at which the condition M  = MU is possible, that is, in the interior of a 1
Provided that these components do not include three collinear forces.
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
381
span, at a builtin end, or at an intermediate support. A collapse mechanism is admissible if it does not violate any support condition (possibly relaxed by the formation of a plastic hinge) and if it produces a positive external work rate. If the effect of shear on the formation of a plastic hinge can be neglected, as will be assumed, then a hinge that has rotated by an angle ∆θ can be thought of as the limit of a small segment, of length, say, ∆x, in which the curvature is ∆θ/∆x and the plastic dissipation per unit length is ˙ ˙ MU ∆θ/∆x. The total internal dissipation in the hinge is therefore MU ∆θ. A moment distribution is statically and plastically admissible if it is in equilibrium with the applied loads, is consistent with all force and moment end conditions and frictionless hinge conditions (if any), and is such that M  ≤ MU everywhere. In the moment distribution at collapse, the points where M = ±MU are precisely the ones where plastic hinges form.
Example: Beam with Point Loads If the beam carries point loads only, then the moment can vary only in straightline fashion between points where concentrated forces (loads or reactions) act, and therefore the actual collapse mechanism must be one in which hinges form at load points, builtin ends, or intermediate supports. Consider the beam shown in Figure 6.3.3(a), indeterminate to the first degree, and requiring two plastic hinges for collapse. The possible mechanisms are (1) with hinges at A and B, (2) with hinges at A and C, and (3) with hinges at B and C. They are shown as Figure 6.3.3(b), (c), and (d), respectively. Let us look first at mechanism 1. If the downward displacement of point ˙ + B is ∆, then that of point C is 21 ∆, so that the external work rate is αF ∆ 1 1 ˙ ˙ (1 − α)F ∆ = 2 (1 + α)F ∆. The angles of rotation of the hinges at A 2 and B, assumed small, are respectively 3∆/L and 9∆/2L; the total internal ˙ dissipation is therefore 15MU ∆/2L, and if this is equated to the external work rate, the resulting upper bound on F L/MU is 15/(1 + α). A similar analysis of mechanisms 2 and 3 leads to the respective upper bounds of 12/(2 − α) and 6/(1 − α); but the second of these is greater than the first for any α between 0 and 1, so that mechanism 3 may be discarded. It can easily be seen that mechanism 1 gives the lesser upper bound when α > 2/3, and mechanism 2 when α < 2/3. The ultimate load is therefore given by 12 2 , α≤ , FU L 2 − α 3 = 2 15 MU , α≤ . 1+α 3
The preceding result may also be cast in the form of two inequalities,
382
Chapter 6 / Problems in Plastic Flow and Collapse II
A
L 3
αF
 ?
L 3
B
(1–α)F
 ?
L 3
∆

fh ? hh? ? h h? hh f h 6 3∆ 6 3∆
fD
C
(a)
L
f
2L
(b)
? fPP PP PP ? f PP f
fh hhhh hhh? hhh f ? hf h hh h (c)
(d) F2 L/MU 10
5
HH
HH H Hq(6, 3) A A A 5
10
F1 L/MU
(e)
Figure 6.3.3. Singlespan beam simply supported at one end and built in at the other, with concentrated loads at the third points: (a) geometry and loading; (b)–(d) collapse mechanisms; (e) interaction diagram. parametrically dependent on α, that the total load F must obey: (2 − α)F L ≤ 12, MU
(1 + α)F L ≤ 15. MU
Yet another way of presenting the result would be to regard the loads at B and C as two independent loads F1 and F2 . The inequalities are accordingly rewritten as MU F1 + 2F2 ≤ 12 , L (6.3.7) MU 2F1 + F2 ≤ 15 , L represented graphically by the interaction diagram shown in Figure 6.3.3(e). The last pair of inequalities, Equations (6.3.7), can also be derived by means of an equilibrium analysis. Suppose that a plastic hinge has already formed at A, with MA = −MU ; the beam is then statically determinate, and the bending moments at B and C can easily be calculated to be, respectively, (2F1 + F2 )L/9 − 2MU /3 and (F1 + 2F2 )L/9 − MU /3. The requirement that these moments not exceed MU gives precisely the inequalities (6.3.7).
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
383
The inequalities are also design criteria: they give the minimum value of MU that the section must have in order to carry a given set of loads F1 , F2 .
Example: Beam with Distributed Load Suppose, now, that the beam just examined carries a uniformly distributed load of intensity F/L rather than the point loads. It can still be assumed with some certainty that one of the plastic hinges necessary for collapse will form at the builtin end, but the other hinge can be, in principle, anywhere along the span of the beam. In fact it will form, of course, at the section where the bending moment has a local extremum. If a hinge has formed at the builtin end (x = 0), then the bending moment at any x, 0 ≤ x ≤ L, is
M (x) = MU − 1 −
x L
fx x 1− 2L L
+
,
where f = F L/MU . The maximum of the quantity in brackets occurs at def x/L = 12 + 1/f , and equals (f − 4 + 4/f )/8 = φ(f ). Any value of f for which φ(f ) does not exceed unity is a lower bound for fU = FU L/MU . For example, φ(10) = 0.8, so that 10 is a lower bound. On the other hand, φ(12) = 1.04, so that fU must be somewhat less than 12. The actual value of fU is obtained by setting φ(f ) equal to unity, giving the quadratic equation f 2 − 12f + 4 = 0. √ This equation has the two roots 6 ± 4 2. Clearly, since what is sought is the greatest lower bound, the larger root must be chosen. We thus obtain fU = 11.657 In a kinematic solution, a mechanism with a plastic hinge at x = 0 and another at x = αL, with α to be determined, is assumed, as in Figure 6.3.4. If the downward displacement of the hinge is ∆, then the average
αL

?X ? ( fX ??? (? (? ( ?? ( XX ? XX? ( ? ?( ( (((( f X ? X?f( ( XX ( ( L
x
Figure 6.3.4. Uniformly loaded singlespan beam, simply supported at one end and built in at the other: collapse mechanisms. displacement of both rigid portions of the beam is ∆/2, so that the external ˙ work rate is F ∆/2. The hinge at the builtin end rotates by an angle ∆/αL,
384
Chapter 6 / Problems in Plastic Flow and Collapse II
and the other hinge by the angle ∆/αL + ∆/(1 − α)L. The total internal dissipation is therefore ˙ ∆ 2−α MU . α(1 − α) L It follows that an upper bound to fU is f=
2(2 − α) . α(1 − α)
The least upper bound is found by minimizing f with respect to α: 1 df 2−α 2−α 1 = − − 2 dα α(1 − α)2 α2 (1 − α) α(1 − α) 1 [α(2 − α) − (1 − α)(2 − α) − α(1 − α)] = 0, = [α(1 − α)]2 leading to the quadratic equation α2 − 4α + 2 = 0. √ Since α must be less than 1, the only √ relevant root is α = 2 − 2 and gives the least upper bound f = 6 + 4 2 = 11.657, which, of course, coincides with the previously found greatest lower bound. Without the analytical solution, assumed values of α give upper bounds that may be satisfactory; for example, α = 0.5 leads to f = 12, and α = 0.6 leads to f = 11.667. Moreover, assumed mechanisms can also be used to give lower bounds without resorting to an analytical solution. Consider, for example, the mechanism with α = 0.5, corresponding to f = 12. The moment distribution corresponding to this mechanism is given by "
M (x) = −MU
2 #
x x 1−7 +6 L L
,
and is not plastically admissible because M max = M (7L/12) = (25/24)MU . If, however, all the moments are multiplied by 24/25, then the distribution becomes plastically admissible, and in equilibrium with a load for which f = (24/25)12 = 11.52, which is thus a lower bound.
Example: Continuous Beam A beam with two or more spans, separated by intermediate supports that exert transverse force reactions, is called a continuous beam. The rule governing the degree of static indeterminacy is the same for continuous as for simple beams. However, collapse of a continuous beam may occur in one span only, and does not in general require r + 1 plastic hinges. The collapse of a span between two intermediate supports, or between an intermediate support and a builtin end support, requires three hinges. A span between
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
385
an intermediate support and a simple end support will collapse with only two hinges. It is thus possible for a continuous beam to remain statically indeterminate at collapse. For this reason the kinematic method is preferable by far for the limit analysis of continuous beams. F1
A
f
L 4
 ?
F2 L 4
 fB
L 4
 ?
L 4
C
Figure 6.3.5. Continuous beam, simply supported at one end, built in at the other, and with an intermediate support, carrying a concentrated load at the midpoint of each span. Looking at the beam shown in Figure 6.3.5, we see immediately that the feasible collapse mechanisms are (a) the one in which span AB collapses like the beam of Figure 6.3.4, and (b) the one in which span BC collapses like a beam with both ends built in. In mechanism (b) hinges develop at B (or rather, just to the right of B), at C, and at midspan. The loads F1 , F2 are governed by the uncoupled inequalities, √ MU F1 ≤ (6 + 2 2) , L
F2 ≤ 16
MU . L
These inequalities also specify the minimum value of MU .
6.3.3.
Limit Analysis of Frames
A rigid frame (or simply a frame) is an assemblage of bars that are joined together rigidly, so that they cannot rotate with respect to one another. The joints transmit bending moment, and the members resist the applied loads primarily through bending; axial force and shear are considered secondary effects. Collapse is assumed to occur when sufficient plastic hinges have formed to produce a mechanism. In a multistory frame, collapse may be limited to a single story, and therefore the overall degree of static indeterminacy is not a relevant parameter for the determination of the necessary number of hinges.
Simple Frame A onestory, onebay frame such as shown in Figure 6.3.6 is statically indeterminate of degree three, and the collapse of the frame as a whole indeed requires four hinges, as shown in Figures 6.3.6(a) and (c). Consider, however, Figure 6.3.6(d), which illustrates the beam mechanism. This mechanism does not entail collapse in the sense of unlimited displacements; the deflection of the beam is limited by that of the columns. In practice, however, a structure
386
Chapter 6 / Problems in Plastic Flow and Collapse II
may be said to collapse when its displacements can become significantly greater than those in the elastic range. If the axial elongation of the beam is neglected, a deflection ∆ of the central hinge requires q that the beamcolumn . 1 joints move laterally inward by a distance 2 L − 14 L2 − ∆2 = ∆2 /L. This distance represents the elastic deflection of the columns, ∆e , which is of the same order of magnitude as the beam deflection when the whole frame is . p elastic. Now ∆/∆e = L/∆e is a large number. We are therefore justified in regarding the beam mechanism as a collapse mechanism. F2 F1 
sB
D hhh? s (( 6C( E E E E E E H E E A Es ? EsE L
(a)
 hhh( ? s ((s s s (b)
s s
?
s s
 shhh? ( s ((s
(c)
(d)
Figure 6.3.6. Onestory, onebay frame: (a)–(c) fourhinge mechanisms; (d) beam mechanism. The only pertinent collapse mechanisms for the frame of Figure 6.3.6 are the beam mechanism (d), the panel or sidesway mechanism (c), and the composite mechanism (b), which is a superposition of (c) and (d) in which the hinge at B is eliminated. The composite mechanism (a) — the mirror image of (b) — in which joint D is rigid, entails negative work done by the horizontal force and therefore is viable only when this force is zero, in which case it is equivalent to (b). When a hinge is assumed to be at a joint such as B or D, it will actually be in the weaker of the two members meeting there — that is, it forms when the bending moment (which, for equilibrium, must be the same in both members as the joint is approached) reaches the smaller of the two values of MU . Let MU 1 , MU 2 , and MU 3 denote the values of MU in AB, BD, and DE, respectively. If it is assumed that the horizontal load F1 is, for example, a wind load which is just as likely to act to the left at D as to the right at B (so that the loading of Figure 6.3.6 represents only one of two mirrorimage cases), then the frame design should be symmetric, and MU 3 = MU 1 . The upperbound theorem applied to the three mechanisms (b)(d) gives the following inequalities: F2 L ≤ 4MU 2 + 4 min(MU 1 , MU 2 ), F1 H ≤ 2MU 1 + 2 min(MU 1 , MU 2 ), 2F1 H + F2 L ≤ 4MU 1 + 4MU 2 + 4 min(MU 1 , MU 2 ).
(6.3.8)
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
387
As before, these inequalities serve both analysis and design. For the purposes of analysis, let us assume equal values of MU for all three members. The interaction diagram between F1 and F2 is then as shown in Figure 6.3.7(a). The design implications of inequalities (6.3.8) are discussed in the following subsection. ¯ M U 2 /M F2 L/MU 3 ........... ........... 8............ ........... ............ ............ ............ ............ .............
..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... Safe region ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ..... ..... ..... .... ......................................... ........................................ ........................................ ....................................... ....................................... ...................................... ..................................... ..................................... ....................................
A
............. .............. .............. ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ..... ...... ..... 4 ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... ..... ...... .....
A
2
A A
A AA
Safe boundary
1
4
8
(a)
F1 H/MU
1
2
3
¯ M U 1 /M
(b)
Figure 6.3.7. Interaction diagrams for the frame of Figure 6.3.6: (a) load plane; (b) design plane (see page 391).
Complex Frames In a frame comprising several stories and bays, the number of possible collapse mechanisms can become quite large. Every transversely loaded member may form a beam mechanism, and each story may produce a panel mechanism. Furthermore, at any joint at which three or more members come together, a plastic hinge may form independently in each member near the joint (if only two members meet, the hinge can form only in the weaker member). It is convenient to establish a basis of independent mechanisms, called elementary mechanisms, such that all mechanisms may be regarded as superpositions of the elementary ones. These elementary mechanisms, as first discussed by Neal and Symonds [1952], consist of all the beam and panel mechanisms, and in addition, of the joint mechanisms constituted by the formation of plastic hinges, at a joint, in every one of the members that come together there, resulting in a rotation of the joint [see Figure 6.3.8(e)]. The joint mechanisms are not in themselves collapse mechanisms, since the external work rate associated with them is zero (unless an external moment acts at the joint), but they are used in combination with beam and/or panel mechanisms in order to cancel superfluous hinges. Let r denote, as before, the degree of redundancy of the frame. A simple method of determining r is to cut the frame at a sufficient number of sections so that it just becomes statically determinate, that is, equivalent to a set of simply supported beams and/or cantilevers; r is then the number of stress
388
Chapter 6 / Problems in Plastic Flow and Collapse II
resultants (moments, axial forces and shear forces) that can arbitrarily be specified at the cuts. Equivalently, r is the number of sections at which the moment can be arbitrarily prescribed. Suppose, now, that the number of critical sections — that is, sections at which a plastic hinge can form — is n. It follows that there are n − r independent relations among the n moments at the critical sections, and these relations are equilibrium equations. Each such equation can be associated, by means of the principle of virtual work, with a mechanism. Consequently, there are n − r independent mechanisms. As an example, consider the twobay frame shown in Figure 6.3.8(a).1 By means of two cuts, the frame can be transformed into three disconnected cantilevers, and therefore r = 2×3 = 6. The critical sections, as shown, number 10. Consequently the frame has four independent mechanisms. In terms of elementary mechanisms, these are (b)–(c) the two beam mechanisms, (d) the panel mechanism, and (e) the joint mechanism. In the method of superposition of mechanisms due to Neal and Symonds [1952], the analysis begins by determining the upper bounds predicted by the elementary beam and panel mechanisms. Because of the symmetry of the structure, the two beam mechanisms give the same upper bounds. We thus obtain the two inequalities ˙ + 2M0 θ˙ = 7M0 θ, ˙ (2F )Lθ˙ ≤ M0 θ˙ + 2M0 (2θ) ˙ F (2L)θ˙ ≤ (4·M0 + 2·1.5M0 )θ˙ = 7M0 θ,
(b, c) (d)
both of which yield the upper bound F = 3.5M0 /L. In order to improve the upper bound, we proceed to study composite mechanisms. Mechanism (f) is a superposition of (c), (d), and (e) in which the hinges at sections 5 and 6 are eliminated, while a hinge is created at 4. The internal dissipation of the mechanisms can therefore be obtained by subracting from the sum of the righthand members of the two preceding ˙ or (7 + 7 − inequalities the quantity (1.5M0 + 2M0 − 2M0 )θ˙ = 1.5M0 θ, ˙ The external work rate is just the sum of the left1.5)M0 θ˙ = 12.5M0 θ. ˙ Mechanism (f) therefore gives the upper bound F = hand sides, or 4F Lθ. 3.125M0 /L. Mechanism (g) is a further superposition of (f) and (b) in which the hinge ˙ at 2 is eliminated. The internal dissipation is (12.5 + 7 − 1)M0 θ˙ = 18.5M0 θ, ˙ while the external work rate is 6F Lθ. We thus obtain the even smaller upper bound of F = 3.083M0 /L. In the present example, it appears that we have run out of reasonable mechanisms, and the result should give us the collapse load. In more complex cases, it may be quite difficult to make sure that all the possible collapse 1
The circled numbers next to the members mean that the value of MU for a member is the given number times a reference moment M0 .
Section 6.3 / Limit Analysis of Trusses, Beams and Frames 2F F
x?
2i 3

2x
1i
2F 4 6 xxx 5
x? i x 8 7 2 6
i 1.5
1x
1i
x10 2L

2L
x9 ? 2L

(a)
r rPPP r
rP PPr r
(b) r
r
r
r
(c) r r r
r r
(d)
r
(e)
r`` `r
r r
(f)
389
r r
r`` `r
```r r
r
r r
(g)
Figure 6.3.8. Twobay frame: (a) geometry and loading; (b)–(c) beam mechanisms; (d) panel mechanism; (e) joint mechanism; (f)–(g) composite mechanisms.
mechanisms have been explored. The only way to check whether the best upper bound that has been found indeed gives the collapse load is to see if it is also a lower bound, that is, to find a statically admissible moment distribution such that M  = MU at all sections corresponding to hinges in the mechanism, and M  ≤ MU elsewhere. In the present example this is easy, since the optimal mechanism represents total collapse and thus involves r+1 = 7 hinges, leaving the structure statically determinate at collapse. The four independent equilibrium equations (which can be formed by applying the principle of virtual work to the elementary mechanisms) and the seven hinge conditions give eleven equations for the ten criticalsection moments and the load F . It turns out that the moments at 2, 5, and 6 do not exceed the local values of MU , and the load is in fact equal to the best upperbound
390
Chapter 6 / Problems in Plastic Flow and Collapse II
value derived above. The situation is more difficult in multistory frames, in which the best mechanism found by the method of superposition of mechanisms often represents partial collapse, with fewer than r+1 plastic hinges and therefore not enough equations for a rigorous moment check. If the degree of redundancy remaining at failure is small (one or two), a trialanderror procedure is usually applied: guesses are made for a sufficient number of criticalsection moments so that the equilibrium equations can be solved. In more complicated cases, the momentdistribution method due to Horne [1954] and English [1954] may be used; for examples of application, see Hodge [1959], Chapter 3. A method of analysis based on the lowerbound theorem is the method of inequalities, due to Neal and Symonds [1951]. The criticalsection moments Mi (i = 1, . . . , n) are governed by the 2n inequalities −MU i ≤ Mi ≤ MU i , and by the n − r equilibrium equations, at least one of which contains the load F . The equilibrium equations can be transformed by means of linear combinations so that only one of them contains F . The problem now is again one of linear programming: the equation containing F serves as the defining equation for F as the function of the Mi that is to be maximized, with the remaining equations, as well as the inequalities, serving as constraints.
6.3.4.
Limit Design of Frames
Limit Design of a Simple Frame The achievement of a minimumweight design is not so simple for frames as it is for trusses, because there is no simple proportionality, or indeed any onetoone relation, between weight and strength. In simple frames, such as the one analyzed in the preceding subsection, a trialanderror approach is usually the easiest (see Heyman [1953]). In complex frames a more systematic approach, based on some simplifying assumptions, is necessary in order that the problem may be converted into one of mathematical (not necessarily linear) programming. As a first example of limit design of a frame, we consider the fixedbase rectangular frame of Figure 6.3.6 (page 386), for which we derived inequalities (6.3.8). Let the design loads (working loads times appropriate def ¯ , where M ¯ is a reference safety factors) be such that F2 L = 3F1 H = 12M quantity having the dimensions of a moment. The sections chosen for the columns and the beam must then satisfy the following inequalities: ¯, MU 2 + min(MU 1 , MU 2 ) ≥ 3M
(a)
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
391
Table 6.3.1. Plastic Moduli of Selected WideFlange Sections Z (in.3 ) 287 260 234
Shape W14×159 W14×145 W14×132
Z (in.3 ) 212 198 175
Shape W14×120 W16×100 W16×89
Z (in.3 ) 150 130 105
Shape W16×77 W16×67 W16×57
¯, MU 1 + min(MU 1 , MU 2 ) ≥ 2M
(b)
¯. MU 1 + MU 2 + min(MU 1 , MU 2 ) ≥ 5M
(c)
The solution of these inequalities is shown in Figure 6.3.7(b) (page 387) as the “safe region” whose polygonal boundary will be called the safe boundary. Any point in the safe region or on the safe boundary will be said to represent a safe design. ¯ and MU 2 to 1.5M ¯ ; but We note that MU 1 must be at least equal to M ¯, if these criteria are met, there is no need for MU 1 to be greater than 2M ¯ or for MU 2 to be greater than 3M . Thus the choice of sections can be made from a rather restricted range. Let the frame dimensions be L = 24 ft. and H = 12 ft., so that the total weight of the frame is proportional to w1 + w2 , where w1 and w2 denote the weight per unit length of the column and beam, respectively. The design loads will be taken as F1 = 1.0 × 105 lb ¯ = 3.6 × 106 lbin. With the usual and F2 = 1.5 × 105 lb, corresponding to M 3 2 value of σY = 36 × 10 lb/in. for A36 structural steel, it follows that that ¯ /σY = 100 in.3 . Then the ranges of the plastic modulus Z = MU /σY for M the columns and the beam are 100 in.3 ≤ Z1 ≤ 200 in.3 ,
150 in.3 ≤ Z2 ≤ 300 in.3 ,
and they must obey the inequalities 2Z1 + Z2 ≥ 500 in.3 ,
Z1 + 2Z2 ≥ 500 in.3 .
It will be assumed that for architectural reasons, the section depth is to be limited to 16 in. The choice will be made from standard wideflange sections, where the designation Wd × w refers to a section whose depth is d (in inches) and whose weight per unit length is w (in pounds per foot). The strength of a wideflange beam, for a given weight, increases sharply with the depth, and therefore the deepest available sections should be chosen for economy. A listing of section properties for selected wideflange sections is shown in Table 6.3.1. Four designs will be tried. 1. In a design with the lightest possible columns, a W16×57 section presents Z1 = 105 in.3 , requiring ZU 2 ≥ 290 in.3 . Unfortunately, no standard
392
Chapter 6 / Problems in Plastic Flow and Collapse II
W16 section has a plastic modulus close to this value. We consequently choose, for the beam, a W14×159 section, giving Z2 = 287 in.3 . If this is assumed to be close enough, we obtain a design with w1 + w2 = 216 lb/ft. 2. The lightest possible beam section is a W16×77, with Z2 = 150 in.3 , . requiring columns with Z1 = 200 in.3 , which is provided by a W16×100 (Z = 198 in.3 ); this choice yields w1 + w2 = 177 lb/ft., a considerable improvement over the first trial. 3. The beam and column sections of design 2 can be reversed, yielding the same weight. 4. A beam section intermediate between those in designs 2 and 3 is a W16×89 and gives Z2 = 175 in.3 ; this requires Z1 ≥ 162.5 in.3 , and the lightest section satisfying this criterion is again W16×89; thus w1 +w2 = 178 lb/ft., virtually the same as designs 2 and 3, and superior to them by virtue of the greater ease of connections resulting from having the same section throughout. The minimum required value of Z1 = Z2 is 167 in.3 , so that this design carries an overdesign factor of 1.05. The additional margin of safety provides an allowance for axial force. If, for example, Equation (6.2.7) is used for the interaction, then each member can carry an axial force up to (1 − 0.85/1.05)PU = 0.19PU with no loss in momentcarrying capacity. On the basis of design 4, MU 1 = MU 2 = 6.3 × 106 lbin. With the overdesign factor included, the collapse forces are F1 = 1.05 × 105 lb and F2 = 1.575 × 105 lb The weight of the beam is about 2000 lb, and we are therefore justified, in retrospect, in having neglected it. Since the structure is statically determinate at collapse, an equilibrium analysis can easily be performed. The moment at the only other critical section, namely B, is found to be of magnitude 3.78 × 106 lbin., so that the yield criterion is nowhere violated, and the correct mechanism was chosen. While this last result is obvious in the present example, in frames in which a large number of possible mechanisms exists, the moment check is a necessity, as in analysis. The same equilibrium analysis shows that the beam and column DE carry compressive axial forces of 0.875 × 105 lb, and that the maximum shear force (in CD and DE) has the same magnitude. We consider, first, the effect of axial force. The slenderness ratio of the columns, even if they are taken as doubly pinned, is about 20, so that they are not expected to buckle elastically. The crosssectional area of a W16 × 89 section is 26.2 in.2 , so that PU = 9.432 × 105 lb, and P/PU  = 0.093 < 0.19. We consider, finally, the effect of shear. The web area of the section is 7.9 in.2 , and therefore the average shear stress in the web is some 11 × 103 lb/in.2 , well below the shear yield stress of about 20 × 103 lb/in.2 for A36 steel. It follows that the frame can be safely designed on the basis of bending alone.
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
393
Foulkes’ Theorems For a complex frame, the time required for a trialanderror method of limit design would be prohibitively long. Any systematic approach is based on the assumption of a functional relation between the weight per unit length and the flexural strength (as measured by MU or Z) of a beam. Clearly, no such relation exists in general, but an approximate relation can be established for a limited range of sections that is used in the design of a frame. If a relation of the form w = a + bMU
(6.3.9)
can be found, then the problem of minimumweight design of a frame can also be transformed into one of linear programming: the total weight is W =a
X
Li + b
i
X
Li MU i ,
i
the summation being over all members, and therefore the objective function is G(MU 1 , . . .) =
n X
Li MU i ,
i=1
independently of the parameters a and b in the approximate representation (6.3.9); this approach was presented by Foulkes [1953]. In the juststudied simple frame, for the three W16 sections considered, the unit weight (in lb/ft.) is very nearly given by . w = 5 + 0.48Z, with Z in cubic inches. The total weight of the frame, to within an additive constant, is therefore proportional to Z1 + Z2 . The theoretical minimumweight design is thus achieved by finding the point (Z1 , Z2 ) on the safe boundary where the constantweight line Z1 + Z2 = const. is tangent to the boundary. This point is Z1 = Z2 = 167 in.3 , and would represent the actual minimumweight design if a section with this value of Z could be found. Note that the point of tangency between the constantweight line and the safe boundary is a vertex of the boundary, that is, an intersection of two of the lines forming this boundary.1 Since each such line represents a particular collapse mechanism, the theoretical minimumweight frame can collapse in either of two mechanisms, or in a linear combination of the two. In particular, a linear combination of the two mechanisms, with nonnegative coefficients, can be found so that the inequality produced by the combined 1
If the constantweight lines are parallel to one of the boundary lines, then any point on the boundary segment of this line, including the two vertices, represents a minimumweight design,
394
Chapter 6 / Problems in Plastic Flow and Collapse II
mechanism is represented by a line that is parallel to the constantweight lines. Such a mechanism is known as a Foulkes mechanism or a weightcompatible mechanism. If n independent values of MU may be used in a design, then the design space is ndimensional. The theoretical minimumweight design is represented by the point of tangency of a constantweight hyperplane with the safe boundary, which is made up of intersecting hyperplanes. If the point is unique, then it is a vertex of the boundary and is therefore an intersection of at least n of the hyperplanes making up the boundary, each representing a distinct collapse mechanism. A Foulkes mechanism can be formed by combining these mechanisms linearly so that the combined mechanism is represented by a hyperplane that is parallel to the constantweight hyperplanes. Consider a frame design for which a Foulkes mechanism can be assumed. Let Li denote the combined length of all the members whose ultimate moment is MU i . In a Foulkes mechanism, the plastic hinges forming in these members have the property that the sum of the absolute values of their angular velocities is proportional to Li . If the proportionality factor is c, then the total dissipation in the mechanism is c
n X
MU i Li = cG.
i=1
If, moreover, a statically and plastically admissible distribution of bending moments compatible with the design can be found, then the design loads Fj are the collapse loads, and therefore, by virtual work X
Fj vj = cG,
j
where the vj are the velocities conjugate to the Fj in the Foulkes mechanism. Consider, now, any other safe frame design, described by values MU∗ i of the ultimate moments. Since the Foulkes mechanism is a kinematically admissible mechanism, it follows from upperbound theorem that X j
Fj vj ≤ c
n X
MU∗ i Li = cG∗ ,
i=1
and therefore G∗ ≥ G. This result, due to Foulkes [1954], may be stated in words as follows: A frame design that admits a Foulkes mechanism and a compatible, statically and plastically admissible distribution of bending moments is a minimumweight design. Upperbound and lowerbound theorems for minimumweight design were also established by Foulkes. The upperbound theorem is obvious, since any
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
395
safe design provides an upper bound to the minimum weight. Conversely, any design based on a Foulkes mechanism, without necessarily satisfying the condition of admissible moments, provides a lower bound to the minimum weight. A general method, based on Foulkes’ theorems, for the mimimumweight design of highly redundant frames was first developed by Heyman and Prager [1958]. The concept of a Foulkes mechanism can be extended to structures other than frames, including those modeled as continua. If, for example, a beam can be designed with an arbitrarily varying crosssection, then a minimumweight design, based on the relation (6.3.9), is one in which the moment distribution at collapse is such that M  = MU everywhere. Plastic flow, in this case, is not localized in hinges but occurs throughout the beam, with a curvaturerate distribution κ. ˙ Since the plastic dissipation in a Foulkes mechanism is proportional to G, it follows that Z 0
L
MU κ ˙ dx = c
Z
L
MU dx, 0
and the Foulkes mechanism is one in which κ ˙ = c. Similarly, a Foulkes mechanism for a plate obeying the Tresca criterion is one in which κ˙ 1  + κ˙ 2  + κ˙ 1 + κ˙ 2  = 2c, where κ˙ 1 and κ˙ 2 are the principal curvature rates. The general criterion for minimumweight design of continua is due to Drucker and Shield [1957]. Applications to plate design were discussed by Hopkins and Prager [1955], Prager [1955b], and Freiberger and Tekinalp [1956], and to shells by Onat and Prager [1955], Freiberger [1956b] and Onat, Schumann, and Shield [1957]. The results for variablesection beams were applied to frame design by Heyman [1959, 1960] and by Save and Prager [1963]. Further contributions are due to Chan [1969], Maier, Srinivasam, and Save [1972], and Munro [1979]. Many of these results are reviewed in the books by Neal [1963], Massonnet and Save [1965], Heyman [1971], Save and Massonnet [1972], Rozvany [1976], Horne [1979], and Borkowski [1988].
Additional Remarks 1. In both the analysis and the design of frames, all loads were assumed to be concentrated, thus fixing in advance the locations of the critical sections. If any span carries a distributed load, then the critical section in that span must be assumed, and therefore any mechanism gives an upper bound to the collapse load; improvements to the upper bound can be achieved by changing the hinge locations. On the other hand, if any distributed load is replaced by a statically equivalent (equipollent) set of concentrated loads, then the collapse load calculated on the basis of the concentrated loads is
396
Chapter 6 / Problems in Plastic Flow and Collapse II
a lower bound on the collapse load for the distributed load. This result, derived by Symonds and Neal [1951], is known as the loadreplacement theorem. 2. Only rectangular frames were studied as examples. Frames with inclined members, such as the gable frame of Figure 6.3.9, can be studied analogously. The frame shown has three independent mechanisms; these can r Q Q
Q ? QQ Q
!r ! r !
Q

(a)
r
Q Qr !!Q HH ! QH !! QH Hr r r
Q r r
Q
(d)
Q
(b)
Q r Q Q
Q QQ Q QQ QQ r QQr r r
Q Q
r Q Q Q Q r Qr (g)
(c) r Z #Q Q # Z Q Z # Q Z r# Q r r
(e)
(f) Q Q H r QH ! QH ! ! QH Hr r r (h)
Figure 6.3.9. Gable frame: (a) geometry and loading; (b) beam mechanism; (c) panel mechanism; (d) gable mechanism; (e)–(f) other panel mechanisms; (h) composite mechanism. be taken as the beam mechanism (b), the panel mechanism (c), and the gable mechanism (d), which may also be regarded as a kind of panel mechanism. Other panel mechanisms, each of which is a combination of (c) and (d) with one hinge eliminated, are shown as (e)–(g), and a composite mechanism as (h). 3. A relation between weight and strength given by (6.3.9) can be a reasonable approximation to the properties of actual sections if their number is small. For a larger range of sections, a better approximation is usually obtained with a nonlinear relation such as w ∝ MUα , where α = 2/3 for . geometrically similar sections, and α = 0.6 gives a good approximation for many standard Ibeam sections. The problem of minimumweight design then becomes one of nonlinear programming. The computational implemen
Section 6.3 / Limit Analysis of Trusses, Beams and Frames
397
tation of nonlinear programming is not yet at a point where it can be readily applied to the plastic design of complex structures.
Exercises: Section 6.3 1. The truss of Figure 6.3.1(d) is subject to equal horizontal forces F acting to the right at B and C, and a downward vertical force 2F acting at B. If the ultimate bar force PU is the same in all bars and is equal in tension and compression, find the smallest upper bound for FU by analyzing mechanisms, and verify that it is also a lower bound. 2. Find a minimumweight design for the truss of the Exercise 1, assuming that PU = ±σY A in every bar. 3. A beam of span L, built in at the left end and simply supported at the right end, carries a load αF uniformly distributed over the left half and a concentrated load (1 − α)F at a distance L/4 from the right end. (a) Find FU as a function of α by means of both a kinematic and a static analysis. (b) Show how some reasonable upper and lower bounds can be found by means of assumed mechanisms. (c) Find the minimum value of MU as a function of α. 4. In a continuous beam like that of Figure 6.3.5, the loads F1 and F2 are uniformly distributed over the respective spans rather than concentrated. Plot an interaction diagram between F1 L/MU and F2 L/MU . 5. If the rate of deflection of a beam is denoted v(x) and the curvature rate is κ˙ = v 00 (x), show how a Foulkes mechanism for a beam built in at both ends can be generated by means of a deflection curve made up of parabolic arcs. Find a minimumweight design for an ideal sandwich beam of uniform depth but variable flange area. 6. An asymmetric frame is shown in the adjacent figure. (a) Assuming MU FU .
2F
 L/2 ? to be the same in all members, find F 6 L/2 6 ? L
(b) Assuming only that the value of MU in the short column is onehalf of that in the long column, find a minimumweight design for the frame.
?
398
Chapter 6 / Problems in Plastic Flow and Collapse II
7. A twostory onebay frame has the geometry and loading shown in the adjacent figure, and is assumed to collapse under the loading. (a) Find the value of MU if this value is the same in all members. (b) Find the value of MU if this is the value of the ultimate moment in the lower columns and beam, while in the upper columns and beam this value is 0.5MU .
3F
 L/2 ? 2F 6 2F
F
?
L
? 6
L L
?
(c) Assuming only that MU has one value (say MU 1 ) in the lower columns and beam and another value (say MU 2 ) in the upper columns and beam, find the minimumweight design, and plot the design diagram relating MU 1 /F L and MU 2 /F L.
Section 6.4
Limit Analysis of Plates and Shells
The concept of plate yielding was already developed in Article 5.2.3, with the yield criterion given in terms of the moments Mαβ . As shown in 6.4.1, these moments serve as the generalized stresses in the limit analysis of plates. In shells (as in arches), the equilibrium of moments is coupled with membrane forces (analogous to axial forces), and therefore both moments and membrane forces appear as generalized stresses. With the greater number of generalized stresses, the yield loci become more difficult to represent and approximations leading to piecewise linear yield criteria often become necessary. The theory is developed in 6.4.2, and examples are studied in 6.4.3. Thorough coverage of the material in this section can be found in the book by Save and Massonnet [1972].
6.4.1.
Limit Analysis of Plates
Plastic Flow of Plates With the stresses given by Equation (5.2.9), the plastic dissipation per unit volume at plastic collapse (or, equivalently, under the hypothesis of rigid–plastic behavior) is 4 4 Mαβ sgn x3 (−x3 κ˙ αβ ) = 2 x3 Mαβ κ˙ αβ , 2 h h where h is the plate thickness. Integrating through the thickness, we obtain the plastic dissipation per unit area, Dp = σαβ ε˙αβ = −
¯ p = Mαβ κ˙ αβ . D
(6.4.1)
Section 6.4 / Limit Analysis of Plates and Shells
399
∗ that does not violate the yield Now consider any stress distribution σαβ ∗ criterion and gives zero membrane forces. If the moments resulting from σαβ ∗ are Mαβ , then the inequality (3.2.4) expressing the principle of maximum plastic dissipation can be integrated through the thickness, giving ∗ (Mαβ − Mαβ )κ˙ αβ ≥ 0.
(6.4.2)
The moments and the curvature rates are thus respectively the generalized stresses and generalized strain rates for the analysis of the bending collapse of plates. Since yield criteria in terms of moments have already been formulated (see 5.2.2), the associated flow rule can be deduced from (6.4.2) to have the form ∂f . καβ = λ˙ ∂Mαβ For the Mises, Tresca, and Johansen criteria, respectively, we obtain the plastic dissipations per unit area as ¯ p (κ) ˙ = D ¯ p (κ) ˙ = D
q
√2 MU κ ˙ 21 + κ˙ 1 κ˙ 2 + κ˙ 22 3 1 ˙ 1  + κ˙ 2  + κ˙ 1 + 2 MU (κ
(Mises), κ˙ 2 )
¯ p (κ) ˙ = MU (κ˙ 1  + κ˙ 2 ) D
(Tresca), (Johansen).
With moments replacing stresses and curvature rates replacing strain rates, the theorems of limit analysis can be applied to the estimation of collapse loads of plates as in any other problems. As with the plane problems studied in the preceding section, much more use can be made of the upperbound theorem than of the lowerbound theorem.
Hinge Curves A hinge curve or yield curve (hinge line or yield line if straight) is a curve in the region A occupied by the middle plane, across which the slope of the deflection w is discontinuous. Let ∆θ denote the change in slope encountered along a line normal to the curve, and suppose that this change takes place uniformly over a narrow zone of width δ. Within this zone, the numerically ˙ larger principal curvature rate, say κ˙ 1 , is given by κ˙ 1  = ∆θ/δ, with κ˙ 1  ¯ ˙ through the width of the zone, we√obtain, for the κ˙ 2 . If we integrate Dp (κ) ˙ for the plastic dissipation per unit length of the hinge curve, (2MU / 3)∆θ ˙ for the Tresca and Johansen criteria. The total Mises criterion and MU ∆θ internal dissipation needed in limit analysis, Dint =
Z
˙ Dp (ε)dV, R
400
Chapter 6 / Problems in Plastic Flow and Collapse II
is therefore Z q Z 2 2 2 ˙ κ˙ 1 + κ˙ 1 κ˙ 2 + κ˙ 2 dA + Dint = √ MU ∆θ ds (Mises), 3 Z A HCZ 1 ˙ ds (Tresca), (κ˙ 1  + κ˙ 2  + κ˙ 1 + κ˙ 2 )dA + ∆θ Dint = MU 2 HC A Z Z ˙ Dint = MU (κ˙ 1  + κ˙ 2 ) dA + ∆θds (Johansen), A
HC
where HC denotes the hinge curve. Comparing the Mises and Tresca results, we note that the expressions inside the square brackets coincide if q 1 (κ˙ 1  + κ˙ 2  + κ˙ 1 + κ˙ 2 ) = κ˙ 21 + κ˙ 1 κ˙ 2 + κ˙ 22 , 2 and this occurs if and only if one of three conditions κ˙ 1 = 0, κ˙ 2 = 0, or κ˙ 1 + κ˙ 2 = 0 is met. Consequently, an upperbound load obtained for a Tresca plate on the basis of a velocity field obeying one of these conditions √ almost everywhere1 serves for a Mises plate as well if multiplied by 2/ 3. Yieldline theory was developed by Johansen [1932] for the ultimateload design of reinforcedconcrete slabs. In a polygonal plate, the yield curves are yield lines and divide the plate into portions that move as rigid bodies, so that all the dissipation takes place on the yield lines. If any edge is clamped, then either the portion of the plate adjacent to it does not move, or the edge itself becomes a yield line. In accordance with the upperbound theorem, the yieldline pattern must be such as to minimize Dint /Dext , where R Dext = A q w˙ dA is the external work rate.
Applications of YieldLine Theory As an example, consider a simply supported rectangular plate of dimensions 2a×2b under a uniform load F/4ab. “Simply supported” is interpreted in the traditional sense, that is, the plate deflection vanishes at the edges; such a plate is called “positionfixed” by Johnson and Mellor [1973]. According to a weaker definition of simple support, used by Johnson and Mellor, only downward deflection is prevented, and the plate is free to lift off. For the traditional definition, the yieldline pattern may be one of the two shown in Figure 6.4.1. Actually, pattern (a) is a special case of pattern (b), with c = a, but because of its relative simplicity it is instructive to study it separately. It can easily be shown that, if v0pis the center velocity, then the slopediscontinuity rate on the yield lines is (v0 /a)2 + (v0 /b)2 , so that, for a Tresca material, Dint = 4MU v0 1
p
a2
r
+
b2
1 1 a b + 2 = 4MU v0 + , 2 a b b a
“Almost everywhere” means everywhere except on a set of points whose total area is zero.
Section 6.4 / Limit Analysis of Plates and Shells
H HH H
HH HH 6 HH b H H ? a 
401
@ @ @ @ @ @
c
(a)
(b)
Figure 6.4.1. Yieldline patterns for a simply supported rectangular plate. Pattern (a) is a special case of pattern (b), with c = a. while Dext = 1thirdF v0 , so that the upper bound on F is 12MU (a/b + b/a). For pattern (b), we have
Dint = 4MU v0 and
c b + b c
v0 a b + 2(a − c)MU ·2 = 4MU v0 + b b c
1 1 1 c F v0 ·4bc + ·4b(a − c) = F v0 3 − . = 4ab 3 2 6 a
Dext
The ratio Dint /Dext is a minimum at c given by s
c b = 3+ a a
2
b a
b − , a
which can be seen to be less than one for all b/a < 1. Consequently, s
8 a F ≤ MU 3 + 3 b
2
b a
2
b + a
which is less than the upper bound given by pattern (a) except in the case of the square, when the two upper bounds are necessarily equal. The preceding results hold for a plate made of a Mises material if MU is replaced √ by 2MU / 3. If the plate is clamped, then the same yieldline pattern as above can be assumed, provided that the edges become yield lines. It can easily be verified that the total dissipation along the edges is just equal to that on the interior yield lines, so that the upperbound load obtained by this method is twice what it is for the simply supported plate. It is shown later, however, that a better upperbound load can be found for clamped plates in general. A lower bound for the simply supported rectangular plate can be obtained by assuming the statically admissible moment field
m11 = 1 −
x1 a
2
,
m22 = 1 −
x2 b
2
,
m12 = −λ
x1 x2 , ab
402
Chapter 6 / Problems in Plastic Flow and Collapse II
where mαβ = Mαβ /MU , and λ is a constant to be determined. It can readily be verified that the center and the midpoints of the edges yield according to all three criteria. The equilibrium condition mαβ ,αβ = −
F 4abMU
gives a b + +λ . F = 8MU b a The best lower bound is therefore obtained with the largest λ such that the yield criterion is not violated anywhere. This occurs, for each of the three yield criteria, if the criterion is satisfied at the corners, where m11 = m22 = 0 and m12  = λ. Thus the largest admissible √ value of λ turns out to be 1 for the Johansen, 21 for the Tresca, and 1/ 3 for the Mises criterion. For a square plate (a = b), we obtain uppertolowerbound ratios of 1, 1.2, and 1.344, respectively, for the three criteria. For the square Johansen plate, we thus have the exact collapse load FU = 24MU . Upper and lower bounds for uniformly loaded rectangular Johansen plates with various combinations of simply supported and clamped edges have been calculated by Manolakos and Mamalis [1986]. A plate in the shape of a regular polygon will, according to yieldline theory, deform plastically into a pyramid, with yield lines on all diagonals. If we think of a circle as the limit as n → ∞ of an nsided polygon, then it becomes clear that for a circular plate to undergo plastic flow (collapse), the entire plate must become plastic — that is, the yield condition must be met everywhere, as was assumed in Section 5.3.
Applications of circularplate results The results for the clamped circular plate derived in 5.2.3 may be applied to finding an upperbound load for a clamped plate of arbitrary shape. Consider the largest circle that can fit into the area A occupied by the plate; we can then assume a velocity field such that this circle is a hinge circle and the material inside it collapses like a clamped circular plate, while the material outside it remains rigid. If, for example, the plate is uniformly loaded and square, then the total load that would make the plate collapse in this mode is 4/π times the load carried by the largest inscribed circle, or (4/π) × 5.63 × 2πMU = 45.04MU ; this is less, and therefore a better upper bound, than the one of 48MU given by yieldline theory. If a clamped plate is carrying a single concentrated load F , then the upperbound collapse load of 2πMU is obtained for any inscribed circle centered at the load. It was shown by Haythornthwaite and Shield [1958] that the moment field Mr = −MU , Mθ = 0 inside the circle can be extended outside it without violating equilibrium or the yield criterion, so that 2πMU is in fact the collapse load.
Section 6.4 / Limit Analysis of Plates and Shells
403
The same hingecircle mechanism may be used to obtain 2πMU as the upper bound for a concentrated load carried by a simply supported plate of arbitrary shape. Since the moment field is Mr = 0, Mθ = MU inside the circle, it can be continued outside it in a discontinuous but statically and plastically admissible manner as Mr = Mθ = 0, so that 2πMU is the collapse load in this case as well (see Zaid [1959]). All the collapse loads for the axisymmetric Tresca plate may be used as bounds on the corresponding loads for the Mises plate, by virtue of the following reasoning: (1) Any moment field that is in equilibrium with the load and that obeys the Tresca criterion represented by the largest hexagon inscribed in the Mises ellipse (as in Figure 5.2.2, page 292), obviously does not violate the Mises criterion, and therefore the load is a lower bound for the Mises collapse load. (2) All the velocity fields associated with the sides of the Tresca hexagon satisfy one of the conditions κ˙ 1 = 0, √κ˙ 2 = 0, κ˙ 1 + κ˙ 2 = 0; consequently, the Tresca collapse load multiplied by 2/ 3 is an upper bound for the Mises collapse load. Therefore, if fM and fT are the ultimate values of f = F/2πMU for the Mises and Tresca plates, respectively, then 2 fT ≤ fM ≤ √ fT . 3 In order to obtain fM exactly, we must solve the quadratic equation Mr2 − Mr Mθ + Mθ2 − MU2 = 0 for Mθ , making sure that the correct root is chosen, and substitute it in the equilibrium equation. Let ρ = r/a, and let φ(ρ) be a function such that the distributed load (assumed to be acting downward) is given by q(ρ) = −(f MU /a2 )φ0 (ρ)/ρ; note that φ(0) = 0 and φ(1) = 1. The differential equation for m = Mr /MU , dm 1 + m− ρ dρ 2
r
3 1 − m2 = −f φ(ρ), 4
must be solved subject to the initial condition m(0) = 1, and fM is the value of f for which the solution satisfies m(1) = 0 for a simply supported plate and m(1) = −1 for a clamped plate. If the plate is uniformly loaded, then φ(ρ) = ρ2 . A numerical solution of the differential equation leads to fM = 3.26 for the simply supported plate and fM = 5.92 for the clamped plate. These values may be compared with the respective lower bounds of 3 and 5.63, and the upper bounds of 3.46 √ (= 2 3) and 6.50. Other results relating to plate collapse may be found in the books by Hodge [1959], Chapter 10; Hodge [1963]; Johnson and Mellor [1973], Chapter 15; and Save and Massonnet [1972].
404
6.4.2.
Chapter 6 / Problems in Plastic Flow and Collapse II
Limit Analysis of Shells: Theory
A shell is to a plate essentially as an arch is to a beam. As we saw in 6.2.2, the use of a nonlinear P M interaction locus makes the collapse analysis of arches difficult, and in practice a piecewise linear locus is needed. This simplification is all the more necessary for shells, in which more than one component of both membrane force and moment must in general be accounted for. As with onedimensional members, a piecewise linear yield locus is generated by giving the shell an ideal sandwich structure. Alternatively, the piecewise linear locus may be viewed as an approximation to the “exact” nonlinear one for a solid (or nonideal sandwich) shell. The geometry of a shell is usually described by its middle surface, analogous to the middle plane of a plate, so that the two free surfaces are at a distance h/2 from it. At any point of the middle surface, a local Cartesian basis (ei ) may be formed such that e3 is perpendicular to the middle surface, while e1 and e2 define its tangent plane. With respect to this basis, the stress resultants Nαβ , Qα , and Mαβ may be defined in the same way as for plates. The equilibrium equations they satisfy are, of course, different; they require a global curvilinear coordinate system. The general theory of shells is not presented here; only some special cases are studied. The deformation of the middle surface can be described by means of the strain tensor with components ε¯αβ , describing stretching, and the curvature tensor with components καβ , describing bending. With shearing deformation neglected, the internal virtual work per unit surface area is Mαβ δκαβ + Nαβ δ ε¯αβ , and consequently, the Mαβ and Nαβ constitute the generalized stresses for the most general shearless theory of limit analysis of shells; the shear forces Qα are reactions and do not enter the yield locus. If the mechanical behavior of the shell is isotropic in the tangent plane, then the yield locus is expressible in terms of the principal moments M1 , M2 , and the principal membrane forces N1 , N2 . If, in addition, symmetry or another constraint require one of the principal strains ε¯1 , ε¯2 or the principal curvatures κ1 , κ2 to be zero, then the conjugate force or moment ceases to be a generalized force and becomes an internal reaction instead; it can therefore be eliminated from the yield locus, further reducing the number of dimensions of the space in which the yield locus must be described.
Piecewise Linear Yield Locus Following Hodge [1959], we derive the piecewise linear yield locus on the basis of the ideal sandwich shell, made up of two thin sheets of thickness t separated by a core of thickness h. The sheets are elastic–perfectly plastic and obey the Tresca yield criterion with a uniaxial yield stress σY . The
Section 6.4 / Limit Analysis of Plates and Shells
405
principal stresses in the two sheets will be denoted σ1+ , σ2+ and σ1− , σ2− , respectively, the sign convention being chosen so that 1 Mα = (σα− − σα+ )ht, 2
α = 1, 2,
and Nα = (σα− + σα+ )t,
α = 1, 2.
Consequently, α ∓ Mα . σα± = N 2t ht
If the principal stresses σα± are not to violate the Tresca yield criterion, they must satisfy the six inequalities σ1±  ≤ σY ,
σ2±  ≤ σY ,
σ1± − σ2±  ≤ σY .
In order to express these inequalities in terms of the Mα and Nα , we define MU = σY ht and NU = 2σY t, as well as the dimensionless quantities mα = Mα /MU , nα = Nα /NU . We thus obtain m1 − n1  ≤ 1,
m1 + n1  ≤ 1,
m2 − n2  ≤ 1,
m2 + n2  ≤ 1,
m1 − m2 + n1 − n2  ≤ 1,
(6.4.3)
m1 − m2 − n1 + n2  ≤ 1.
The six absolutevalue inequalities (6.4.3) are equivalent to twelve algebraic inequalities, so that the yield locus is bounded by twelve hyperplanes in the fourdimensional m1 m2 n1 n2 space. If one of the quantities mα , nα represents an internal reaction rather than a generalized stress, then it can be eliminated from the yield locus. Suppose this quantity to be m2 (i.e., suppose the shell to be constrained so that κ2 = 0); then the inequalities involving m2 may be rewritten as −1 + n2 ≤ m2 ≤ 1 + n2 ,
− 1 − n2 ≤ m2 ≤ 1 − n2 ,
−1 + m1 + n1 − n2 ≤ m2 ≤ 1 + m1 + n1 − n2 ,
(6.4.4)
−1 + m1 − n1 + n2 ≤ m2 ≤ 1 + m1 − n1 + n2 . The actual values of m2 do not matter, as long as some m2 can be found so that all the inequalities (6.4.4) can be satisfied, and this is the case whenever the first member of each inequality is no greater than the third member of every inequality. The first two inequalities give n2  ≤ 1,
(6.4.5a)
n1 − n2  ≤ 1.
(6.4.5b)
and the second two give
406
Chapter 6 / Problems in Plastic Flow and Collapse II
Combining inequalities from the first and second pairs leads to the following additional nontrivial inequalities: 2n2 − n1 + m1  ≤ 2,
2n2 − n1 − m1  ≤ 2.
(6.4.5cd)
Together with (6.4.3)1,2 , we thus have six absolutevalue inequalities involving m1 , n1 and n2 , or a total of twelve algebraic inequalities. The yield locus is therefore a dodecahedron in the threedimensional m1 n1 n2 space, illustrated in Figure 6.4.2. The derivation of this locus is due to Hodge [1954], n2
6 @ n1 @ B @ @ B B B B B B B  m1
@ @ B B B B B B B B
@ @
Figure 6.4.2. Piecewise linear yield locus for a cylindrical shell (from Prager [1959]). who also derived the exact nonlinear yield locus for a solid shell made of uniform material. As discussed previously, the piecewise linear locus may be thought of as an approximation to the exact one when the appropriate values of MU and NU are used, namely MU = σY h2 /4 and NU = σY h, with σY the uniaxial yield stress of the solidshell material. The plastic dissipation per unit area of the ideal sandwich shell, given rigid–plastic behavior, is ¯ p = σY t ε˙+  + ε˙+  + ε˙+ + ε˙+  + ε˙−  + ε˙−  + ε˙− + ε˙−  . D 1 2 1 2 1 2 1 2 2 But h ε˙± ¯˙ α ∓ κ˙ α , α = 1, 2. α =ε 2 Consequently, ¯ p = 1 [NU ε¯˙ 1 + MU κ˙ 1  + NU ε¯˙ 1 − MU κ˙ 1  D 4 + NU ε¯˙ 2 + MU κ˙ 2  + NU ε¯˙ 2 − MU κ˙ 2  + NU (ε¯˙ 1 + ε¯˙ 2 ) + MU (κ˙ 1 + κ˙ 2 ) + NU (ε¯˙ 1 + ε¯˙ 2 ) − MU (κ˙ 1 + κ˙ 2 )] . (6.4.6)
Section 6.4 / Limit Analysis of Plates and Shells
407
(( E E (( iP u0 (z) P E 6 E  E((
E E ((( E E E E u(z) EE (E (( E E E E E E E E E E dθ E a E E E E E E E E E E E(( E (
w(z)
r
z
Figure 6.4.3. Displacements in a radially loaded cylindrical shell. Yield criteria that are appropriate for the approximate treatment of reinforcedconcrete shells are discussed by Save and Massonnet [1972], Chapter 9.
6.4.3.
Limit Analysis of Shells: Examples
Radially Loaded Cylindrical Shell: Basic Equations As a first example of the application of the theory discussed above, we consider a circular cylindrical shell of uniform mean radius a and thickness h, subject to an axisymmetric radial pressure distribution that may vary along the axial coordinate z. Because of axial symmetry the displacement of the middle surface has only the radial component u(z) and the axial component w(z). The displacements throughout the shell are assumed to be governed by the “plane sections remain plane” hypothesis applied to a longitudinal strip subtending a small angle dθ (see Figure 6.4.3): ur (r, z) = u(z),
uθ (r, z) = 0,
uz (r, z) = w(z) − (r − a)u0 (z). In accordance with Equations (1.2.1), the only nonvanishing strain components are u . u εθ = = r a and εz = w0 − yu00 ,
408
Chapter 6 / Problems in Plastic Flow and Collapse II
where y = r − a. The internal virtual work per unit area is Z
h/2
−h/2
(σθ δεθ + σz δεz ) dy = Nθ
δu + Nz δw0 + Mz δu00 , a
where Z
Nθ =
h/2
−h/2
Z
σθ dy,
Nz =
h/2
−h/2
σz dy,
Mz = −
h/2
Z
−h/2
yσz dy.
The generalized stresses are thus three in number. The conjugate generalized strains are ε¯θ = u/a, ε¯z = w0 , and κz = u00 . The fact that κθ = 0 (i.e., circles remain circles) removes Mθ from the rank of generalized stresses. The yield locus is therefore given by Equations (6.4.3)1,2 and (6.4.5a)–(6.4.5d), with M1 = Mz , N1 = Nz , and N2 = Nθ . The plastic dissipation per unit area is ˙ w˙ 0 w˙ 0 ¯ p = 1 2NU u D + NU + MU u˙ 00 + NU − MU u˙ 00 4 a a a u˙ u ˙ 0 00 + w˙ + MU u˙ + NU + w˙ 0 − MU u˙ 00 . + NU a a
(6.4.7)
The equilibrium equations can be obtained by applying the principle of virtual work. If the shell axis occupies the interval −L ≤ z ≤ L, then the internal virtual work is Z
δW int = 2πa
L
−L
(Nθ
δu + Nz δw0 + Mz δu00 ) dz. a
Through integration by parts this becomes n
L
δW int = 2πa (Mz δu0 − Mz0 δu + Nz δw) −L Z
L
+ −L
Mz00
Nθ + a
δu −
Nz0
δw dz .
In addition to the radial pressure p (positive outward), let the shell be loaded by a bending moment Mz+ , an axial force Nz+ , and a shear force Q+ r , all per − − unit length of circumference, at z = L, and similarly, Mz , Nz , and Q− r at z = −L. The external virtual work is therefore "Z
δW ext = 2πa
L
−L
p δu dz + Nz+ δw(L) + Mz+ δu0 (L)
− − 0 − + Q+ r δu(L) −Nz δw(−L) − Mz δu (−L) − Qr δu(−L) .
Equating the internal and external virtual work leads to the equilibrium equations Nθ Nz0 = 0, Mz00 + =p (6.4.8) a
Section 6.4 / Limit Analysis of Plates and Shells
409
and the boundary conditions (Mz − Mz± ) δu0 = 0,
(Mz0 + Q± r ) δu = 0,
(Nz − Nz± ) δw = 0,
z = ±L.
Note that the axial end forces must be equal and opposite for equilibrium. If these are zero, then Nz = 0 everywhere. For the shell without end load, the piecewise linear yield locus reduces to a hexagon in the Mz Nθ plane, formed by the three pairs of parallel lines described by m = 1, 2n + m = 2, 2n − m = 2, (6.4.9) where m = Mz /MU and n = Nθ /NU (see Figure 6.4.4, which also shows the “exact” nonlinear yield locus as well as the simplified square locus given by m ≤ 1, n ≤ 1). n B
G
H
A
C
m
F
D
J
E
I
Exact Approximate
Figure 6.4.4. Yield loci for a cylindrical shell without end load. The plastic dissipation for the yield criterion described by (6.4.9) may be obtained from (6.4.7) by substituting, as in uniaxial stress, ε¯˙ 1 = − 12 ε¯˙ 2 , or w˙ 0 = −u/2a. ˙ The result is ˙ u˙ u˙ ¯ p = 1 NU u + NU + MU u˙ 00 + NU − MU u˙ 00 . D 2 a 2a 2a
(6.4.10)
When the state of generalized stress can be assumed to be represented by points on one of the inclined lines AB, BC, DE, and EF of Figure 6.4.4, then Nθ can be expressed in terms of Mz , and the result substituted in the equilibrium equation (6.4.8)2 . The equation then becomes a linear differential equation for Mz , which can be solved subject to appropriate boundary
410
Chapter 6 / Problems in Plastic Flow and Collapse II
conditions. Since the normality rule gives 2MU u˙ 00 = ±NU u/a ˙ along the aforementioned lines, the dissipation is just NU u/a. ˙ The same result obtains at the vertices B and E. Along the lines AF and CD, normality requires u/ ˙ u˙ 00 = 0. A nonvanishing velocity thus implies u˙ 00 = ±∞, that is, the formation of a plastic hinge circle. A simple case occurs when the pressure p is constant and the ends of the tube are free. Then Mz = 0, and the yield criterion reduces to Nθ  = NU . The ultimate pressure is therefore given by pU  = NU /a. A solution for a pressurized tube with clamped ends was derived by Hodge [1954]. Here the central portion of the tube is in regime DE, and the outer portions in EF ; the boundary is at z = ±ηL. The parameter η and the dimensionless ultimate pressure p¯ = pU a/NU are given implicitly as functions of the dimensionless shell parameter ω, defined by ω2 = The results are sinh ωη = √ p¯ =
NU L2 . 2MU a
sin ω(1 − η) , 2 cos ω(1 − η) + 1
2 − cos ω(1 − η) 2[1 − cos ω(1 − η)]
for ω ≤ 1.65, and tan ω(1 − η) = coth ωη, p¯ = 1 +
1 2(2 cosh ωη − 1)
for ω > 1.65. For more details, see Hodge [1959], Section 112.
Cylindrical Shell with a Ring Load As another example, suppose that a freeended shell is subject to a radially inward ring loading at z = 0, its intensity being F per unit length of circumference; that is, p(z) = −F δ(z), where δ(·) is the Dirac delta function. Note that δ(z) =
1 d 1 d2 sgn z = z. 2 dz 2 dz 2
It is reasonable to assume initially that the hoop stress is compressive, that is, Nθ ≤ 0. If the shell is extremely short, then its collapse should not depend very much on whether the force is applied around a ring or uniformly distributed over the surface in a statically equivalent manner. For very short
Section 6.4 / Limit Analysis of Plates and Shells
411
. shells, then, we should expect FU = 2NU L/a, with bending having little or no effect. When bending is taken into account, it can be seen that at least in a central portion of the tube, Mz ≥ 0. It will be assumed, to begin with, that the entire shell is plastic and in regime AB of Figure 6.4.4. Eliminating Nθ , we obtain the following dimensionless differential equation for m(ζ), using the dimensionless variable ζ = z/L, and the parameters f = F a/(2NU L) and ω as previously defined: m00 (ζ) + ω 2 m(ζ) = 2ω 2 − 4ω 2 f δ(ζ). The general solution of this equation that is even in ζ is m(ζ) = 2 − 2ωf sin(ωζ) + C cos ωζ, with C an arbitrary constant. The freeend condition m(1) = m0 (1) = 0 yields C = −2 cos ω and sin ω f= . (6.4.11) ω The solution may accordingly be written as m(ζ) = 2[1 − cos ω(1 − ζ)]. The requirement that 0 ≤ m ≤ 1 limits the validity of this solution to ω ≤ π/3. For sufficiently short shells, then, Equation (6.4.11) gives a lower bound to the collapse load; in particular, the limit as ω → 0 is f = 1, as previously discussed. An associated kinematically admissible velocity field, however, can easily be found, namely, u(ζ) ˙ = −v0 cos ωζ.
(6.4.12)
It can readily be checked that the generalized strain rates derived from this velocity field satisfy the normality condition for regime AB, and hence Equation (6.4.11) gives the collapse load for ω ≤ π/3. Alternatively, the upperbound theorem can be applied directly to the velocity field (6.4.12), the dissipation per unit length being 2πNU u, ˙ and the external work rate 2πaF v0 . The result is Equation (6.4.11) as an upper bound, as long as u(ζ) ˙ does not change sign; this condition is met for ω ≤ π/2. Equation (6.4.11) is therefore an upper bound for π/3 ≤ ω ≤ π/2. However, a better upper bound can be obtained for this range by assuming a velocity field with a plastic hinge circle at ζ = 0, namely, u(ζ) ˙ = −v0 (cos ωζ + β sin ωζ).
(6.4.13)
The additional dissipation at the hinge circle is 4πaMU βv0 /L = 2πNU Lβv0 /ω 2 . Equating dissipation and external work rate yields f = sin ω −
β (1 − 2 cos ω) 2ω 2
412
Chapter 6 / Problems in Plastic Flow and Collapse II
if u˙ does not change sign, that is, if β ≤ ω cot ω. Choosing this limiting value for β gives the smallest value of f , namely, f=
2 − cos ω , 2ω sin ω
which is less than the righthand side of (6.4.11) for π/3 < ω < π/2. A lower bound for ω > π/3 can be obtained by assuming the solution m(ζ) = 2 − cos ωζ − 2ωf sin(ωζ) valid for ζ < η, where η is such that m(η) = m0 (η) = 0, and continuing it statically as Mz √ = 0, Nθ = 0 for ζ > η. The conditions at η lead to ωη = π/3 and f = 3/(2ω), or, in dimensional form, s
F =
6MU NU , a
a result that can be seen to be independent of the length. As can be seen, however, as the length increases, so does the discrepancy between the upper and lower bounds. For longer shells the solution based on the hexagonal yield locus becomes difficult. For an infinitely long shell, Drucker [1954b] found the collapse load s
F =2 or f =
p
3MU NU a
(6.4.14)
3/2/ω. This load is based on the following moment distribution: √ 6 m(ζ) = 2 − cos ωζ − sin ωζ, 0 ≤ ζ ≤ ζ1 (AB), ω = −2 + cosh ω(ζ − ζ2 ), ζ1 ≤ ζ ≤ ζ3 (BC), = −2 + 2 cos ω(ζ − ζ4 ),
ζ3 ≤ ζ ≤ ζ4 (DE),
= 0,
ζ4 ≤ ζ
(rigid),
where ωζ1 = cos
−1
√ 2+3 2 = 0.469, 7
ω(ζ2 − ζ1 ) = cosh−1 2 = 1.317,
1 1 1 cosh−1 4 = 1.032, ω(ζ4 − ζ3 ) = cos−1 = 0.659. 2 2 4 It follows that ωζ4 = 3.477, and therefore the result is valid for ω ≥ 3.477. Note that m(0) = 1 and m(ζ2 ) = −1, so that plastic hinges develop at those points. At ζ3 the hoop stress Nθ changes abruptly from a negative to a positive value, and at ζ4 back to zero. ω(ζ3 − ζ2 ) =
Section 6.4 / Limit Analysis of Plates and Shells
413
As pointed out by Drucker [1954b], the mathematics is greatly simplified if the the yield locus is replaced by the rectangle Mz  ≤ MU , Nθ  ≤ NU . With this yield criterion, Eason and Shield [1955] found complete solutions for shells of all lengths, and with the load not necessarily at the center. Since the rectangle circumscribes the hexagon, the collapse loads found by Eason and Shield are upper bounds on those that would be found for the hexagonal yield locus. Furthermore, a rectangle with vertices at (±MU0 , ±NU0 ) may be inscribed in the hexagon; then the collapse load for the rectangle is a lower bound for the hexagon when MU and NU are respectively replaced by MU0 and NU0 . The values of MU0 and NU0 may be chosen to as to maximize the lower bound. With the rectangular yield locus, both kinematic and static solutions are quite easy. The sides Mz  = MU of the rectangle (like those of the hexagon) correspond to hinge circles, while the sides Nθ  = NU describe velocities u˙ varying linearly with position. For each side, Mz and Nθ are polynomial functions of z. For the symmetric problem under consideration, Eason and Shield’s results are √ 1 1 f= + 1 , ω ≤ 1 + 2, 2 2 ω √ √ 2 , ω ≥ 1 + 2. f= ω The latter result is equivalent to s
F =4
MU N U , a
(6.4.15)
independent of the length. Equation (6.4.15) also gives the lower bound s
F =4
MU0 NU0 , a
where
MU0 N0 + 2 U ≤ 2, MU0 ≤ MU . MU NU 0 0 1 The p lower bound is maximized for MU = MU , NU = 2 NU , and equals 2 2MU NU /a. The bounds thus bracket Drucker’s collapse load (6.4.14) for the long shell.
Spherical Cap Under Pressure In shells of revolution, as a rule, all four generalized stresses are active. An approximate theory, in which the effects of one of them are ignored, was proposed by Drucker and Shield [1959], but its applicability is limited. It was shown by Hodge [1959] that for a shell of revolution, a point on the fourdimensional piecewise linear yield locus (6.4.3) corresponds to
414
Chapter 6 / Problems in Plastic Flow and Collapse II
plastic deformation only if it lies on the intersection of two of the twelve hyperplanes, one of which represents yielding of the top sheet and the other represents yielding of the bottom sheet. The generalized stresses thus satisfy two yield equations and two equilibrium equations, making the problem “statically determinate.” Furthermore, there are two normality conditions on the generalized strain rates, and since the latter are derived from two velocity components, the problem is “kinematically determinate” as well. We consider here a spherical cap of radius a subtending a halfangle φ0 , clamped around its edge, and carrying a uniform radial pressure p (see Figure 6.4.5). The problem was treated by Onat and Prager [1954] on the basis of a nonlinear yield criterion and by Hodge [1959, Section 116] on the basis of the piecewise linear yield criterion (6.4.3). p
C ? AUA N CW
JJ BMB ^
J
J
B J
B  φ J
Ba φ0 s
J J B
J B
JB
JB
JB
Figure 6.4.5. Spherical cap under uniform external pressure: geometry and loading. If the radial displacement is ur = u and the meridional displacement is uφ = v, then the generalized strains are ε¯θ =
u + v cot φ , a
ε¯φ =
u + v0 , a
u0 − v , a2
κφ =
u00 − v 0 , a2
κθ = cot φ
where (·)0 = d(·)/dφ. To find an upper bound on the collapse pressure, we assume the velocity field u˙ = −v0 (cos φ − cos φ0 ), v˙ = 0. The generalized strain rates are accordingly ε¯˙ θ = ε¯˙ φ = −
v0 (cos φ − cos φ0 ), a
κ˙ θ = κ˙ φ =
v0 cos φ. a2
The plastic dissipation per unit area is then, from Equation (6.4.6), ¯ p = NU v0 [ cos φ0 − (1 − k) cos φ + (1 + k) cos φ − cos φ0 ] D
Section 6.4 / Limit Analysis of Plates and Shells (
=
415
2NU v0 (cos φ − cos φ0 ), 0 ≤ φ ≤ φ∗ , 2kNU v0 cos φ, φ∗ ≤ φ ≤ φ0 ,
where
MU , NU a
k=
cos φ∗ =
cos φ0 . 1−k
The expression for φ > φ∗ is necessary, of course, only if φ0 > φ∗ . In addition, since u˙ 0 does not vanish at the edge φ = φ0 , a plastic hinge circle forms there, necessitating the additional dissipation (per unit length) given by MU v0 sin φ0 /a = kNU v0 sin φ0 . The total internal dissipation is thus Z φ0 ¯ p sin φ dφ + 2πakNU v0 sin2 φ0 . D Dint = 2πa2 0
The external work rate is 2
Dext = 2πa
Z
φ0
pu˙ sin φ dφ = πa2 pv0 (1 − cos φ0 )2 .
0
Setting Dext = Dint yields the upper bound "
NU 1 + cos φ0 k2 p=2 1+k + a 1 − cos φ0 1 − k NU 1 + cos φ0 , p = 4k a 1 − cos φ0
cos φ0 1 − cos φ0
2 #
, cos φ0 ≤ 1 − k, cos φ0 ≥ 1 − k.
A lower bound may be obtained by assuming that the stress field in the shell is one of simple membrane compression, Nθ = Nφ = −NU , with Mθ = Mφ = 0. The corresponding lowerbound pressure is p = 2NU /a. A lower bound that is better for sufficiently small cap angles was found by Hodge [1959] by assuming Nθ , Nφ , Mθ and Mφ to be sinusoidally varying functions of φ, substituting into the equilibrium equations, and choosing the free coefficients so as to maximize the pressure subject to the yield inequalities. The resulting best lower bound is given by
pa 1 1 − =2+ NU 1 − cos φ0
s
1−k 1+k
2
+4
1 − cos φ0 1 + cos φ0
2
.
Clearly, this result is an improvement over the previous one if and only if the quantity under the squareroot sign is less than unity.
Exercises: Section 6.4 1. Using yieldline theory, find upper bounds for a uniformly loaded, simply supported Tresca plate having the shape of (a) an equilateral triangle, (b) a right isosceles triangle, and (c) a regular hexagon.
416
Chapter 6 / Problems in Plastic Flow and Collapse II
2. Repeat Exercise 1 for clamped plates. 3. Find lower bounds for some of the plates in Exercises 1 and 2. 4. Using yieldline theory, find upper bounds for the plates of Exercises 1 and 2 when they carry a single concentrated load at the center or centroid. Compare with the result FU = 2πMU . 5. A square Tresca plate carrying a uniform downward load is simply supported along its edges against downward deflection but is free to lift off. Using yieldline theory, find an upper bound to the collapse load. 6. Using some of the methods of Section 6.2, find lower and upper bounds for the yield locus of an ideal sandwich shell obeying the Mises criterion and its associated flow rule (a) when M2 is not a generalized stress and (b) when, in addition, N1 = 0. 7. Find the complete solution for the clamped pressurized cylindrical shell with clamped ends obeying the “square” yield locus of Figure 6.4.4. Plot the nondimensional ultimate pressure p¯ = pU a/NU against the shell parameter ω. 8. Repeat Exercise 7 for a shell that is (a) clamped at one end and free at the other and (b)simply supported at both ends. 9. Repeat Exercise 8 for the hexagonal yield locus. 10. For a short freeended cylindrical shell subject to a noncentered ring load, find the collapse load based on the “square” yield locus.
Chapter 7
Dynamic Problems Section 7.1 7.1.1
Dynamic Loading of Structures
General Concepts
All the problems studied so far have been static or quasistatic. In any complete solution of such a problem, the stress field satisfies the equilibrium equation with the prescribed body force and the static boundary conditions with the prescribed surface tractions. The effects of inertia are neglected. In a body made of a standard perfectly plastic material, the ultimate loading is the greatest loading under which a solution to the static problem can be found such that the yield criterion is nowhere violated. If a loading in excess of the limit loading is applied, then, obviously, the static problem (in which, by definition, inertia is ignored) has no solution, and inertia effects must be taken into account. If the time of loading is short, enough of the external work may be transformed into kinetic energy so that excessive deformation is prevented; for example, when a nail is struck by a hammer, it may experience a force in excess of its static ultimate load without permanent deformation. The problem of impact or impulsive loading of structural elements such as beams, plates and shells has been most often treated within the constitutive framework of limit analysis: rigid–perfectly plastic behavior, with the yield criterion in terms of generalized stresses. This approach, which has been reasonably successful with regard to the determination of permanent deformations, is presented in this section; it is generally regarded as justified when the energy imparted to the body greatly exceeds the elastic energy that can be stored. If local constitutive equations are used, waves propagate through the body. The propagation of onedimensional and multidimensional waves in elasticplastic bodies is studied in Sections 7.2 and 7.3, respectively. 417
418
Chapter 7 / Dynamic Problems
It must be pointed out at the outset that the solution of dynamic problems on the basis of rateindependent plasticity is in conflict with the definition of rateindependent plastic behavior as the limiting behavior of viscoplastic bodies at very slow rates (see 3.1.2). The use of rateindependent plasticity for such problems is based on the assumption of a “dynamic” yield stress that is independent of rate in the range of rates encountered in the dynamic problem, but not, in general, identical with the static yield stress. The adequacy of this procedure, as opposed to the use of viscoplasticity theory, has long been the subject of debate and is discussed in 7.2.3. Until then, the rateindependent model will be tacitly assumed.
Dynamic Behavior of Rigid–Perfectly Plastic Bodies: General Results Most of the structures for which static collapse loads have been determined on the basis of the rigid–perfectly plastic model have also been subject to dynamic analysis; the solutions have been surveyed by Krajcinovic [1973] and Jones [1975]. A common feature of the solutions is that if the body is restrained against rigidbody motion, then the velocity field eventually takes on a mode form in the sense that its spatial variation becomes independent of time. In other words, the velocity becomes the product of a timedependent amplitude and a function of position: ˙ v(x, t) = ∆(t)w(x). A proof that all solutions must converge to mode form is due to Martin [1980]; it is based on an extremum principle, according to which the final √ mode is the one that minimizes Dint / K, where Dint is the total plastic dissipation and K is the kinetic energy. The fact that at least the final phase of the motion is in mode form means that all points of the body come to rest at once. If the time at which this occurs is ts , then the permanent displacement field up (x) can be found by integrating the velocity over time from t = 0 to t = ts . A theorem due to Martin [1975] gives a lower bound on ts for a body on which all prescribed loads and prescribed surface velocities are zero for t > t0 . Let v∗ be any kinematically admissible velocity field, with a strainrate field ε˙ ∗ derived from it. When the body force, prescribed surface traction and prescribed surface velocity are all zero, the dynamic principle of virtual velocities reduces to −
Z
∗
ρv˙ · v dV =
Z
R
R
σij ε˙∗ij dV,
where v is the actual velocity field and σ is the actual stress field. Combining this result with the maximumplasticdissipation postulate, we obtain −
Z R
ρv˙ · v∗ dV ≤
Z R
Dp (ε˙ ∗ ) dV.
Section 7.1 / Dynamic Loading of Structures
419
The righthand side of this inequality is independent of time, while on the lefthand side only v˙ depends on time. If v0 (x) = v(x, t0 ), then, since v(x, ts ) = 0, integration of both sides from t0 to ts leads to Z
∗
ρv0 · v dV ≤ (ts − t0 )
R
Z
Dp (ε˙ ∗ ) dV.
R
Consequently,
R v0 · v∗ dV R ts − t0 ≥ R . ∗
˙ R Dp (ε
(7.1.1)
) dV
Another result due to Martin [1975] governs the permanent displacement field up (x) = u(x, ts ). If σ ∗ is any statically and plastically admissible stress field, then the static principle of virtual work implies that Z ∂R
∗ σij vi nj dS =
Z R
∗ σij ε˙ij dV,
while the dynamic principle of virtual velocities gives −
Z
ρv˙ · v dV =
Z
σij ε˙ij dV. R
R
Again using the maximumplasticdissipation postulate, we obtain Z ∂R
Z
∗ σij vi nj dS ≤ −
where
1 K= 2
ρv˙ · v dV = −
R
Z
d K, dt
ρv · v dV.
R
Since K(ts ) = 0, integration of both sides of the inequality leads to Z ∂R
∗ σij (upi − u0i )nj dS ≤ K0 ,
(7.1.2)
where u0 is the displacement field at t0 . In the case of impulsive loading lasting a very short time, u0 can be taken as zero. The preceding results can easily be formulated in terms of generalized stresses and strains.
7.1.2
Dynamic Loading of Beams
Equations of Motion for Elastic–Plastic Beams The equations of motion of a beam according to the elementary (Euler– Bernoulli) theory can be obtained by adding inertial forces to the distributed load. We consider only a beam of doubly symmetric crosssection, with the centroidal axis along the xaxis, and with bending confined to the xyplane.
420
Chapter 7 / Dynamic Problems
If the deflection in the positive ydirection is u(x, t), then the inertial force per unit length is −¯ ρ∂ 2 u/∂t2 , where ρ¯ = ρA is the beam mass per unit length, ρ being the mass density and A the crosssectional area. With q denoting the distributed load per unit length, the equation of motion is ∂2u ∂2M = q − ρ ¯ . ∂x2 ∂t2
(7.1.3)
When q = 0, and a functional relation is assumed between the moment M and the curvature κ = ∂ 2 u/∂x2 , it can be shown that the deflection can be expressed as u(x, t) = tf (η), where η = x2 /t, and that κ (and hence M ) as well as the velocity v = ∂u/∂t are functions of the single variable η alone. If, say, κ = Ψ(M ), then the moment is governed by the differential equation d2 √ dM η dη 2 dη
+
ρ¯ 0 √ dM Ψ (M ) η = 0. 16 dη
(7.1.4)
For a linearly elastic beam, Ψ0 (M ) = 1/EI, so that the equation is linear; a general solution is due to Boussinesq. For an elastic–plastic beam, Equation (7.1.4) is in general nonlinear, and must be solved numerically. It is, however, piecewise linear if a momentcurvature relation with linear workhardening is assumed, and an analytic solution can then be obtained. The first such solution was found by Bohnenblust (see Duwez, Clark, and Bohnenblust [1950]), who treated an infinitely long beam in which one point is suddenly given a velocity that remains constant in time — equivalent to being struck by a very heavy concentrated mass traveling at that velocity (so heavy that the resistance of the beam is insufficient to decelerate it), or as in the experiments that were performed by Duwez et al., to the beam itself moving transversely as a rigid body before it impinges on a concentrated rigid obstacle. The deformation remains elastic if the impact velocity p v0 does not exceed vE = κE EI/¯ ρ, where κE is the elasticlimit curvature as defined in 4.4.1. When v0 > vE and the hardening is linear, different deformation patterns develop for vE < v0 < 2.087vE and for v0 > 2.087vE . The analogous problem for rigid–plastic beams, with various types of workhardening and with extensions to variable velocity and to semiinfinite beams, was treated by Conroy [1952, 1955, 1956, 1963]. Equation (7.1.4) for such a beam is valid only in the plastic portions of the beam. In the rigid portions, the moment is governed by Equation (7.1.3) with q = 0 and with the deflection given by a straightline function of x, say u(x, t) = f (t)+g(t)x. The boundary between the rigid and plastic portions is itself an unknown function of time. It was shown by Conroy [1952] how the plastic portions shrink to points, representing plastic hinges, in the limit as the workhardening decreases to zero. For linear hardening, Conroy [1955] showed that certain problems can be solved by means of linear elastic analysis.
Section 7.1 / Dynamic Loading of Structures
421
Impact Loading of a Perfectly Plastic FreeEnded Beam The impact loading of a freeended beam by a suddenly applied force that is a prescribed function of position and time was studied by Lee and Symonds [1952] for a rigid–perfectly plastic beam loaded at the center and by Bleich and Salvadori [1953, 1955] for an elastic–perfectly plastic beam under a loading that is symmetric about the midpoint but is otherwise arbitrary. We consider, first, the problem treated by Lee and Symonds [1952]. A freeended beam of length 2L is suddenly loaded at its midpoint by a concentrated force F (t), which rises to a peak value Fm and declines to zero in a short time. Let ∆(t) denote the midpoint displacement. It can be assumed that at first the beam is accelerated as a rigid body, so that the displacement is ∆ everywhere, and the load F is balanced by a uniformly distributed iner¨ with 2¯ ¨ = F [see Figure 7.1.1(a)]. The bending moment at tial force ρ¯∆, ρL∆ a distance x from the midpoint may be obtained from the freebody diagram of Figure 7.1.1(b), and is M (x, t) =
F (t) (L − x)2 ; 4L
the maximum moment is M (0, t) = F (t)L/4. The assumption of rigidbody motion is therefore valid as long as this moment is less than MU , or F (t) < 4MU /L. F
M
?
x
6666666666666666666
¨ = F ρ¯∆ 2L 2L

?6666666 F 2L
(b)
(a)
F
h ( hhh (( hhh( h ( ((( hhh ( ? ( ( θ w hhh ( (( ? (c)
L–x
F/2
( (( ( ((( ( ? ( ( ( w ( (( E E E E E EE E ¨ ¨ E E ρ¯(∆–xθ)
x
(d)
Figure 7.1.1. Impact loading of a perfectly plastic freeended beam: (a) geometry and loading; (b) freebody diagram; (c) hinge rotation; (d) motion of onehalf of the beam. When F (t) ≥ 4MU /L, a plastic hinge must form at x = 0. Let the halfangle of rotation of the hinge be θ(t), as in Figure 7.1.1(c). Because of symmetry, it is sufficient to study the motion of half the beam, say 0 < x < L
422
Chapter 7 / Dynamic Problems
[see Figure 7.1.1(d)]. Since the deflection is u(x, t) = ∆(t) − xθ(t) as long as θ(t) 1, the global force equation of motion may be obtained by balancing the force F/2 acting on half the beam with the total inertial force: F = ρ¯ 2
L
Z 0
2
¨ ¨ ¨ − xθ)dx ¨ − ρ¯ L θ. (∆ = ρ¯L∆ 2
Similarly, the moment equation of motion is obtained by balancing the moment MU with the moment about x = 0 of the inertial force: Z
MU = ρ¯ 0
L
2
3
¨ dx = ρ¯ L ∆ ¨ ¨ − ρ¯ L θ. ¨ − xθ)x (∆ 2 6
The linear and angular accelerations are, respectively, ¨ = 2MU (φ − 3), ∆ ρ¯L2 3MU θ¨ = (φ − 4), ρ¯L3 where φ(t) = F (t)L/MU . The distribution of bending moment is now
M (x, t) = MU 1 −
x L
2
1 x 1 − [φ(t) − 4] . 2 L
It can easily be shown that this distribution has a local extremum in the interior of the beam when φ(t) > 6, and that this extremum is located at x/L = φ(t)/3[φ(t) − 4] and has the value −2MU [φ(t) − 6]3 /27[φ(t) − 4]2 . This value equals −MU when φ reaches 22.9; an additional plastic hinge then forms in each half of the beam. For F (t) ≥ 22.9MU /L, therefore, the equations of motion must reflect the additional hinges, which move in toward the middle as the load increases. Further results relative to this problem were obtained by Symonds and Leth [1954] and by Cotter and Symonds [1955]. The effect of distributed rather than concentrated loads was studied by Salvadori and DiMaggio [1953] and by Seiler and Symonds [1954] (see also Seiler, Cotter and Symonds [1956]). An extension of the method to elastic–perfectly plastic beams is due to Alverson [1956]. Bleich and Salvadori [1953, 1955] examined the motion of an impulsively loaded elastic–perfectly plastic beam by using the natural modes of vibration of elastic beams — for the entire beam during the initial elastic phase, and for the portions of the beam separated by plastic hinges after the beam yields, provided that the hinges are stationary. Salvadori and DiMaggio [1953] studied the development of hinges for various degrees of concentration of the load, ranging from uniformly distributed to concentrated. For a comparison
Section 7.1 / Dynamic Loading of Structures
423
between the results of Lee and Symonds and those of Bleich and Salvadori, see the discussion by Symonds and by Bleich and Salvadori following the paper by Bleich and Salvadori [1955]. The impact loading of a rigid–perfectly plastic beam that is built in at both ends was studied by Symonds and Mentel [1958], who took into account the axial forces that develop when such a beam deflects.
Cantilever Struck by a Mass at Its Tip The method of Lee and Symonds was applied by Parkes [1955] to study the impact on a cantilever beam of length L by an object of mass m traveling with a velocity v0 . The beam is again assumed to be rigid–perfectly plastic, so that the kinetic energy of the striker can be absorbed only in a plastic hinge. Initially the hinge is at the tip, but it moves in time toward the builtin end. Let x denote distance along the beam measured from the tip and ∆(t) the tip deflection, and let x = x ¯(t) give the position of the hinge at t. The portion x > x ¯(t) remains undisturbed. In the portion x < x ¯(t), the curvature 2 2 rate κ˙ = ∂ v/∂x (where v = ∂u/∂t) vanishes, so that the velocity is given by x ˙ v(x, t) = ∆(t) 1− . x ¯(t) Since the plastic hinge occurs at a maximum of the bending moment, the shear force there is zero, and therefore the net force on the moving portion of the beam is zero. The translational equation of motion for this portion of the beam is therefore ˙ = 0, ¨ + ρ¯ d (¯ x∆) (7.1.5) m∆ 2 dt while the rotational motion can be obtained by taking moments about the tip, yielding ρ¯ d 2 ˙ (¯ x ∆) = MU . (7.1.6) 6 dt Equations (7.1.5)–(7.1.6) can be integrated to give ρ¯ ˙ m+ x ¯(t) ∆(t) = A, 2
ρ¯ ˙ [¯ x(t)]2 ∆(t) − MU t = B, 6
˙ where A and B are constant. Since x ¯(0) = 0 and ∆(0) = v0 , it follows that A = mv0 and B = 0. Hence, if we define β = ρ¯L/2m and ξ = x ¯(t)/L, then ˙ ∆(t) 1 = v0 1 + βξ and t=
mv0 L βξ 2 , 3MU 1 + βξ
(7.1.7)
424
Chapter 7 / Dynamic Problems
provided that ξ < 1. The plastic hinge reaches the builtin end at time ˙ 1 ) = v0 /(1 + β). t = t1 , given by Equation (7.1.7) when ξ = 1. Note that ∆(t For t > t1 , the motion is in mode form:
˙ v(x, t) = ∆(t) 1−
x . L
The equation for ∆(t) can be obtained by taking moments about x = L, namely, ! ρ¯L2 ¨ mL + ∆ = −MU . 3 Integration, with continuity at t = t1 , leads to ˙ 1 ∆(t) 3MU (t − t1 ) 3MU = − = (ts − t), v0 1 + β mv0 L(3 + 2β) mv0 L(3 + 2β) where
mv0 L mv0 L 3 + 2β = 3MU 1 + β MU is the time at which the motion stops. Consequently, the permanent deflection up may be obtained by integrating the velocity over time up to ts . If the mass of the striker is much greater than that of the beam, that is, if β 1, then the permanent deflection is approximately ts = t1 +
x mv02 L 1− . up (x) ≡ 2MU L
Thus the beam remains straight, and the deflection is that which is necessary so that all the kinetic energy is absorbed by the hinge at the builtin end. If, on the other hand, the mass of the striker is much less than that of the beam, the final shape is a superposition of a rotation and a local deformation near the tip. The form is, approximately, given by up (x) =
2m2 v02 L ln 3MU ρ¯ x
with up (0) =
if βx/L 1,
2m2 v02 ln β. 3MU ρ¯
Parkes [1955] also carried out experiments in which mildsteel cantilever beams were subjected to impact by relatively heavy weights dropped on their tips, as well as by bullets. Reasonably good agreement with the theory was obtained when MU was given a “dynamic” value based on the data of Manjoine [1944] for the rate sensitivity of the yield stress of mild steel. A numerical study of the Parkes problem by Symonds and Fleming [1984] shows that when elasticity is taken into account, then the initial phase of
Section 7.1 / Dynamic Loading of Structures
425
the deflection is not even approximately represented by the travelinghinge solution — that is, plastic deformation is not concentrated in a narrow zone in the interior. On the other hand, convergence to mode form is a prominent feature of the solution.
7.1.3
Dynamic Loading of Plates And Shells
Dynamic Loading of Rigid–Plastic Circular Plates The dynamic problem of a simply supported rigid–plastic circular plate that is suddenly loaded by a uniformly distributed pressure — a blast loading — was studied by Hopkins and Prager [1954], as a sequel to the same authors’ static solution (Hopkins and Prager [1953]) discussed in 5.2.3. The equilibrium equation (5.2.10) is replaced by the equation of motion, 0
(rMr ) − Mθ = −
Z
r
(p + µw)r ¨ dr.
(7.1.8)
0
where we write u0 for ∂u/∂r and u˙ for ∂u/∂t, while µ is the mass per unit area and p is the pressure (assumed acting in the negative zdirection). The Tresca yield criterion, as represented by the hexagon of Figure 5.2.2 (page 310), is assumed. As in the static case, the plate is assumed to be in regime BC, with point B corresponding to the center of the plate. A conical deformation can therefore be assumed, given by
w(r, t) = −∆(t) 1 −
r . a
Inserting this expression in the equation of motion (7.1.8) and substituting Mθ = MU , we can integrate the equation to obtain !
r2 r2 r3 ¨ − Mr (r, t) = MU − p + µ∆(t) . 6 6 12a ¨ = 2(p − pU ), where pU = The boundary condition Mr (a, t) = 0 yields µ∆ 2 ¨ we may write the 6MU /a is the static ultimate pressure. Eliminating µ∆, following expression for Mr : r2 r p − (p − pU ) 2 − 6 a
Mr = MU −
.
This result is valid, however, only if the righthand side does not exceed MU , that is, if the quantity in brackets is nonnegative for all r. The necessary and sufficient condition for this is p ≤ 2pU . Pressures satisfying this condition may be called moderate pressures, while pressures greater than 2pU will be called high pressures.
426
Chapter 7 / Dynamic Problems
At high pressures, the deflection may be assumed in the shape of a truncated cone, with a hinge circle of radius r0 separating the outer conical ˙ region from the inner region, which moves rigidly with a velocity w˙ = −∆. The latter region is at point B of the Tresca hexagon, so that Mr = Mθ = MU , and the equation of motion for r < r0 reduces to ¨ = p. µ∆ For r > r0 , the velocity is a−r ˙ w(r, ˙ t) = −∆(t) , a − r0 and the acceleration is therefore given by µw ¨ = −p
a−r . a − r0
The equation of motion (7.1.8) now becomes (rMr )0 = MU −
p (2r3 − 3r0 r2 + r03 ), 6(a − r0 )
which when integrated subject to the initial condition Mr = MU at r = r0 , leads to (r − r0 )3 (r + r0 ) rMr = rMU − p . 12(a − r0 ) Finally, the condition Mr = 0 at r = a gives r0 as the solution of the cubic equation r0 2 r0 2pU 1− 1+ = . (7.1.9) a a p Suppose, now, that the pressure is suddenly removed at time t = t0 . For p ≤ 2pU , the form of the preceding solution is still valid for t > t0 , with p ¨ = −2pU . replaced by zero. The midpoint acceleration is now given by µ∆ The time history of the midpoint deflection is therefore 1 [p(2t0 t − t20 ) − pU t2 ], 0 < t < t0 , µ 1 = (p − pU )t2 , t0 < t < ts , µ
∆(t) =
˙ s ) = 0, so that where ts is the time at which the motion stops, that is, ∆(t ts = (p/pU )t0 . The permanent midpoint deflection is thus ∆p = ∆(ts ) =
p(p − pU ) 2 t0 . µpU
The result for ts coincides with the lower bound given by Martin’s theorem, Equation (7.1.1), when the conical velocity field is used, say w˙ ∗ =
Section 7.1 / Dynamic Loading of Structures
427
˙ ∗ (1 − r/a). The denominator of the righthand side of (7.1.1) is then ∆ ˙ ∗ , while the numerator is 2πMU ∆ Z
2π 0
a
˙ 0 )∆ ˙∗ 1− r µ∆(t a
2
r dr = 2π
2 a2 ˙ ˙ ∗ = 2π a (p − pU )t0 ∆ ˙ ∗. µ∆(t0 )∆ 12 6
Since MU = pU a2 /6, it follows that
ts − t 0 ≥
p − 1 t0 , pU
and the righthand side coincides with the exact value. When p > 2pU , the removal of the pressure means that in the central ¨ = 0, and therefore region the acceleration becomes zero, that is, ∆ ˙ ˙ 0 ) = pt0 . ∆(t) = ∆(t µ ˙ a nonvanishing Since the velocity in the conical region is proportional to ∆, acceleration there requires the radius of the hinge circle to be a function of time, say r¯(t), with r¯(t0 ) = r0 . For r > r¯(t), then, the velocity and the acceleration are, respectively, w(r, ˙ t) = −
pt0 a − r pt0 r¯˙ (t) a − r and w(r, ¨ t) = − , µ a − r¯(t) µ [a − r¯(t)]2
so that the equation of motion is (rMr )0 = MU +
pt0 r¯˙ [3a(r2 − r¯2 ) − 2(r3 − r¯3 )]. 6(a − r¯2 )2
Integrating, with Mr = MU at r = r¯, we obtain rMr = rMU +
pt0 r¯˙ (r − r¯)2 [2a(r + 2¯ r) − (r2 + 2r¯ r + 3¯ r2 )]. 12(a − r¯)2
Setting Mr = 0 at r = a, we obtain for r¯ the differential equation (a2 + 2a¯ r − 3¯ r2 )
d¯ r 2pU a3 =− . dt pt0
The factor on the lefthand side is positive, and therefore the radius of the hinge circle will decrease. The equation can be integrated to give t p =1+ [a2 (r0 − r¯) + a(r02 − r¯2 ) − (r03 − r¯3 )]. t0 2pU a3 Let t1 denote the time at which the radius of the hinge circle goes to zero. Then " 2 3 # t1 p r0 r0 r0 =1+ + − , t0 2pU a a a
428
Chapter 7 / Dynamic Problems
where r0 is given by Equation (7.1.9). For t > t1 , the velocity field (though not the deflection) is fully conical, and is consequently in mode form. Perzyna [1958] studied the effect of different time profiles of the pressure pulse. The corresponding problem for a clamped plate was treated by Florence [1966]. The problem of impact loading of a circular plate, in which a uniform velocity is suddenly imparted to the plate (except the edge), was treated in a similar manner by Wang [1955] for a simply supported plate and by Wang and Hopkins [1954] for a clamped plate. Nonaxisymmetric problems were treated by Hopkins [1957]. For simply supported plates, the results based on the Tresca criterion are immediately transferable to the Johansen criterion, since regime BC of Figure 5.2.2 is common to both. For clamped plates the criteria differ. The blast loading of square clamped plates obeying the Johansen criterion was studied by Cox and Morland [1959].
PressurePulse Loading of a Cylindrical Shell Relatively few dynamic problems have been solved for elastic–plastic or rigid–plastic shells. We consider here a solution due to Hodge [1955] for a circular cylindrical shell, made of a rigid–perfectly plastic material and clamped at both ends, that is suddenly loaded by a uniform radial pressure which does not decrease in time, the initial value of the pressure being greater than the static ultimate pressure pU . For mathematical simplicity, the square yield criterion of Figure 6.4.4 (page 409) is adopted; an analysis by Hodge and Paul [1957] based on the hexagonal locus shows that the solution is not greatly affected by changes in shape of the yield locus. The static ultimate pressure may be obtained by assuming that Nθ = NU throughout. The equilibrium equation (6.4.8)2 is then Mz00 = p −
NU . a
A collapse mechanism may be assumed to consist of hinge circles at the center (z = 0) and at the builtin ends (z = ±L). For generalizedstress points on side GH of the square of Figure 6.4.4, the associated flow rule requires that u˙ 00 = 0. The radial velocity field is accordingly
˙ 1− u(z) ˙ =∆
z . L
(7.1.10)
A moment distribution consistent with this velocity field has Mz (0) = −MU and Mz (±L) = MU , and is given by !
Mz = M U
z2 2 2 −1 , L
Section 7.1 / Dynamic Loading of Structures so that pU =
NU 4MU NU + = 2 a L a
429
2 , ω2
1+
p
where ω = NU L2 /2MU a is the shell parameter defined in 6.4.3. In the dynamic problem it can still be assumed that Nθ = NU , so that the velocity field is z ˙ . u(z, ˙ t) = ∆(t) 1− L The equilibrium equation is replaced by the equation of motion, Mz00 = p −
NU − µ¨ u, a
(7.1.11)
where µ is again the mass per unit area. Integrating the equation of motion subject to the condition Mz = −MU at z = 0 leads to NU Mz = −MU + p − a
2 3 z2 ¨ z − z − µ∆ 2 2 6L
!
.
The end condition Mz = MU at z = ±L then gives ¨ = 3 (p − pU ). µ∆ 2 ¨ from the expression for Mz , we obtain Eliminating µ∆ !
M z = MU
p − pU z2 2 2 −1 − L 4
z3 z − L
!
2
.
This solution is valid only if Mz  ≤ MU everywhere, requiring Mz00 (0) ≥ 0,
Mz0 (L) ≥ 0,
Mz0 (−L) ≤ 0.
The first condition is satisfied if NU MU p ≤ pU + 8 2 = L a
6 1+ 2 ω
def
= p1 .
The last two conditions are fulfilled if MU NU p ≥ pU − 16 2 = L a
6 1− 2 . ω
(7.1.12)
If the pressure has a constant value p0 for 0 < t < t0 and then suddenly drops to zero, then inequality (7.1.12) is obeyed after unloading only if ω 2 ≤ 6; a shell satisfying this criterion may be called, following Hodge [1955], a short shell. For a short shell with pU < p0 < p1 (a moderate pressure), the
430
Chapter 7 / Dynamic Problems
solution thus far derived is valid both for 0 < t < t0 and for t > t0 , with p given by p0 and 0, respectively. The midpoint velocity is 3 ˙ ∆(t) = (p0 − pU )t, 0 < t < t0 , 2µ 3 = (p0 t0 − pU t), t0 < t < ts , 2µ where ts = (p0 /pU )t0 is the time at which the motion stops. The permanent radial expansion at the midsection is ∆(ts ) =
3p0 t2 4µ
p0 −1 . pU
In a long shell (ω 2 > 6) under moderate pressure, the solution is valid during the first phase but not after unloading. In order to obtain a valid solution, we must abandon the hypothesis that the entire shell is in regime GH of Figure 6.4.4. Instead, only a central portion of the shell, say z < z¯(t), will be assumed to be in this regime, with the sections z = ±¯ z (t) at point G, and the remainder of the shell in regime GJ. In the latter regime the flow rule gives u˙ = 0, and therefore the outer portions of the shell undergo no further motion. The velocity field is thus
˙ u(z, ˙ t) = ∆(t) 1− = 0,
z , z < z¯(t), z¯(t) z > z¯(t).
The equation of motion for z < z¯ is Mz00
¨ ˙˙ NU ¨ + µ ∆ − ∆z¯ =− + µ∆ a z¯ zbar2
!
z.
Since Mz0 (0, t) = 0, a first integration gives Mz0
˙˙ NU ¨ z+µ ∆ ¨ − ∆z¯ =− + µ∆ a z¯
!
zz . 2¯ z
Furthermore, Mz0 = 0 at z = z¯, so that ˙ z¯˙ ∆ ¨ µ +∆ z¯
!
= −2
NU . a
(7.1.13)
Integrating again yields, upon elimination of NU by means of Equation (7.1.13) and with Mz (0, t) = −MU , ˙ z¯˙ ∆ ¨ Mz = −MU + µ −∆ z¯
!
z 2 z3 − 4 6¯ z
!
.
Section 7.1 / Dynamic Loading of Structures
431
Finally, since Mz = MU at z = z¯, we obtain ˙ z¯˙ ∆ ¨ µ −∆ z¯
!
= 24
MU . z¯2
(7.1.14)
Combining Equations (7.1.13) and (7.1.14) produces ¨ =− µ∆
NU MU − 12 2 , a z¯
(7.1.15)
˙ z¯˙ = − µ∆
NU MU z¯ + 12 . a z¯
(7.1.16)
¨ from Differentiating (7.1.16) with respect to time and substituting for µ∆ (7.1.15), we find that ˙ z¨¯ = 0. µ∆ ˙ cannot be zero while the shell is in motion, it follows that z¨¯ = 0, Since ∆ ˙ so that z¯ is a constant. We obtain its value from Equation (7.1.16) at t = t0 , ˙ = 3(p0 − pU )t0 /2µ. Hence when z¯ = L and ∆ z¯˙ = −
2L NU 1 − ω62 , 3t0 a p0 − pU
which is always negative for a long shell (ω 2 > 6); consequently, the hinge circles move toward the center, and their location is given by z¯(t) = L + (t − t0 )z¯˙ .
(7.1.17)
The √ motion stops when the righthand side of (7.1.16) vanishes, that is, when z¯ = 6L/ω. The time when this occurs is " # √ ! 3 p0 − pU 6 L √ 1− = t0 1 + . ts = t0 + z¯˙  ω 2 (1 + 6/ω)(NU /a) The permanent radial expansion at the midsection can be obtained by inte˙ grating ∆(t), as given by (7.1.16) and with z¯ given by (7.1.17), from t0 to ts , and adding the result to ∆(t0 ) = 3(p0 − pU )t20 /4µ. Under high pressures, that is, p0 > p1 , during the initial phase hinge circles may be assumed at z = ±z0 and at z = ±L, with M = −MU and N = NU for z ≤ z0 , and the velocity given by ˙ u(z, ˙ t) = ∆(t),
z < z0 ,
L−z ˙ = ∆(t) , z > z0 . L − z0 Equation (7.1.11) for z < z0 gives ¨ =p− µ∆
NU . a
432
Chapter 7 / Dynamic Problems
For z > z0 , therefore, the equation of motion may therefore be written as Mz00
NU = p− a
z − z0 , L − z0
and may be integrated twice, subject to the initial conditions Mz0 = 0 and Mz = −MU at z = z0 , to give NU Mz = p − a
(z − z0 )3 − MU . 6(L − z0 )
The conditions Mz = MU at the builtin ends z = z0 lead to s
z0 = L −
12MU , p0 − (NU /a)
and z0 > 0 if p0 > p1 . After unloading, the inner hinge circles must be assumed to move, their location being, say, z = z¯(t). The equation of motion for z < z¯(t) reduces ¨ = −NU /a. Continuity of the velocity at t = t0 gives the midsection to µ∆ radial velocity for t0 < t < t1 as 1 NU ˙ ∆(t) = p0 t 0 − t , µ a
where t1 is the time at which the hinge circles coalesce at the midsection. For z > z¯(t) the equation of motion is Mz00 = −
NU z − z¯ ˙ z¯˙ L − z . − µ∆ a L − z¯ (L − z¯)2
Integrating subject to Mz0 = 0 and Mz = −MU at z = z¯ and substituting Mz = MU at z = L gives ˙ z¯˙ = − µ∆
NU MU (L − z¯) − 12 . a L − z¯
˙ as a function of time, we find the the differential equation Substituting for ∆ for z¯(t) is separable and can be written as dt (L − z¯)d¯ z =− , t¯ − t (L − z¯)2 + 3L2 /ω 2 where t¯ = (p0 a/NU )t0 . We can integrate the equation subject to z¯(t0 ) = z0 , obtaining ¯ t − t0 2 (L − z¯)2 + 3L2 /ω 2 = . t¯ − t (L − z0 )2 + 3L2 /ω 2
Section 7.1 / Dynamic Loading of Structures
433
We finally find t1 as
t1 = t0 1 +
p0 a − 1 1 − NU
s
3 + ω 2 (1 − z0 /L)2 . 3 + ω2
For t > t1 , the velocity field may again be assumed to be of the form (7.1.10) (mode form). Calculation of the permanent deformation may be carried out by analogy with the preceding examples. Details may be found in the paper by Hodge [1955] (see also Hodge [1956]). As the reader can see, there are a great many similarities between the dynamic shell and plate problems formulated according to the rigid–perfectly plastic model, and these in turn resemble the beam problems. The comments expressed previously concerning the validity of the travelinghinge solution may therefore be expected to be applicable to structural impact problems in general.
Exercises: Section 7.1 1. Formulate Martin’s inequality (7.1.2) in terms of generalized stresses to give a bound on the permanent deflection for (a) beams and (b) plates. 2. Determine the motion due to impact loading of a freeended rigid– perfectly plastic beam by a concentrated force at the center if (a) the force has the constant value Fm for 0 < t < t0 and is removed at t = t0 , and (b) the force rises linearly from zero to Fm at t = t0 /2 and then declines linearly to zero at t = t0 . 3. Analyze the motion of a rigid–perfectly plastic cantilever struck by a mass m that is uniformly distributed over a length a at the free end of the beam. In particular, find the stopping time ts and compare with the bound (7.1.1). Show that the solution reduces to that of Parkes as a/L → 0. 4. Analyze the motion of a rigid–perfectly plastic beam struck by a concentrated mass m at midspan when the beam is (a) simply supported and (b) clamped. 5. Analyze the motion of a rigid–perfectly plastic circular Tresca plate of radius a that is suddenly loaded by a pressure p uniformly distributed over the circle r < b (where b < a) when the plate is (a) simply supported and (b) clamped. 6. Analyze the motion of a simply supported rigid–perfectly plastic circular Tresca plate that is struck by a concentrated mass m at the center.
434
Chapter 7 / Dynamic Problems
7. Compare the stopping time ts found in the text for a long clamped cylindrical shell under a moderate impulsive pressure with the bound (7.1.1). 8. Analyze the motion of a long clamped cylindrical shell under a high pressure for t > t1 . Find the stopping time ts and compare with (7.1.1). 9. Analyze the motion of a clamped cylindrical shell under a pressurepulse loading. Study various cases. 10. Analyze the motion of an infinitely long cylindrical shell suddenly loaded by a ring load.
Section 7.2 7.2.1
OneDimensional Plastic Waves
Theory of OneDimensional Waves
In studying the propagation of longitudinal stress and strain waves in a thin bar, it is common to represent the problem by a “onedimensional” approximation in which the only nonvanishing stress component is assumed to be the longitudinal one, and the contribution of the transverse displacement to the deformation and the inertia is ignored. It is known from elastic bar theory that this approximation yields good results at points of the bar whose distance from the bar ends is more than a few diameters; near the ends, threedimensional corrections are necessary. We let x denote the Lagrangian coordinate along the bar axis and u(x, t) the corresponding displacement. The conventional (“engineering”) strain ε(x, t) and velocity v(x, t) are then given by ε=
∂u , ∂x
v=
∂u , ∂t
and satisfy the kinematic compatibility relation ∂ε ∂v = . ∂t ∂x
(7.2.1)
The equations of motion, in the absence of body force, reduce to ∂σ ∂v =ρ , ∂x ∂t
(7.2.2)
where σ is the nominal (“engineering”) stress and ρ is the mass density in the undeformed state.
Section 7.2 / OneDimensional Plastic Waves
435
The equations governing the problem of torsional motion of a thinwalled circular tube are exactly the same as the preceding ones if u and v are interpreted as the circumferential displacement and velocity (uθ and vθ ), respectively, and ε and σ as the conventional shear strain and shear stress (γzθ and τzθ ). Except for some comments concerning finite strain, the following theory applies to the torsional problem as well.
Shock Fronts A shock front is said to occur at a point x = α(t) of the bar if the velocity v is discontinuous there. We suppose that the shock front is moving at a finite speed c in the positive xdirection (say from left to right), that is, c = α0 (t) > 0, and we designate the values of v just to the right (in front) of the shock and just to the left of (behind) the shock by v + and v − , respectively. The jump in v is defined as [v] = v − − v + . Similar definitions apply to ε and σ. It is readily apparent that with v a discontinuous function of x and of t, its partial derivatives with respect to both variables are in effect infinite at the shock front. By Equation (7.2.2), the same is true of ε and σ. Relations among the jumps in velocity, strain, and stress may be derived by treating the shock front as a thin zone in which these quantities change very rapidly, their partial derivatives having large constant values. If the shock thickness is h, then, approximately, ∂v . [v] = ±h , ∂x for a front moving to the left and to the right, respectively, with similar relations for ε and σ. Another approximation for the jump may be obtained by following it along the time axis. Since v − is the earlier and v + the later value, and since the duration of the shock passage at a given point is h/c, it follows that . h ∂v [v] = . c ∂t Applying these approximations to Equations (7.2.1)–(7.2.2), we obtain the shock relations 1 [ε] = ± [v] , [σ] = ±ρc[v] , (7.2.3) c where the + and − signs apply to fronts moving to the left and to the right, respectively. Eliminating [v] , we are left with the shockspeed equation ρc2 =
[σ] . [ε]
(7.2.4)
436
Chapter 7 / Dynamic Problems
Impact of a Rigid–Plastic Bar As an application of the shock relations (7.2.3), we study the problem of longitudinal impact of a bar treated as rigid–plastic. Suppose that the bar, of length L, is moving rigidly at a speed v0 in the direction of its axis until, at time t = 0, it squarely strikes a rigid target. The situation at t > 0 is shown in Figure 7.2.1; it is assumed that plastic deformation takes place only in an infinitely narrow zone at x = ξ(t), where x is measured from the free end [so that ξ(0) = L], with the remaining portions of the bar rigid. In
ξ(t)
At rest

v¯(t)
x
Shock front
Figure 7.2.1. Impact of a rigidplastic bar on a rigid wall. particular, the portion near the target, x > ξ(t), is assumed to have come to rest, while the portion near the free end is moving with a uniform velocity: v(x, t) = v¯(t), x < ξ(t), v(x, t) = 0, x > ξ(t). The section x = ξ(t), since the velocity is discontinuous there, is the location of a shock front moving in the negative xdirection with a speed c = −ξ˙ with respect to the undeformed material. For convenience, stress and strain will be taken as positive in compression, so that the signs in Equations (7.2.3) are reversed. We begin by assuming the bar as rigid–perfectly plastic, so that it is at yield at the shock front. The true stress, then, equals σY at x = ξ(t) and is continuous there. The nominal stress is also σY ahead of the front, but it equals σY /(1− ε¯) behind the front if ε¯ is the strain there. The discontinuities at the front are therefore [σ] =
σY σY ε¯ − σY = , 1 − ε¯ 1 − ε¯
[ε] = ε¯,
[v] = −¯ v,
and the shock relations are v¯ ε¯ = − , ξ˙
σY ε¯ ˙v , = −ρξ¯ 1 − ε¯
from which, on the one hand, ρξ˙2 =
σY 1 − ε¯
(7.2.5)
Section 7.2 / OneDimensional Plastic Waves
437
while, on the other hand, ρ¯ v2 =
σY ε¯2 , 1 − ε¯
(7.2.6)
and upon differentiating, !
σY ε¯2 ρ¯ v d¯ v= d . 2 1 − ε¯
(7.2.7)
In addition, the equation of motion of the undeformed portion is ρξ(t)v¯˙ (t) = −σY , so that ρ¯ v v¯˙ = −
ξ˙ σY v¯ = σY ε¯ . ξ ξ
(7.2.8)
Combining (7.2.7) and (7.2.8) gives !
dξ 1 ε¯2 2 = d . ξ ε¯ 1 − ε¯
(7.2.9)
If the initial impact velocity is v¯(0) = v0 , then the initial strain at the impact end is obtained in terms of v0 through (7.2.6), namely, ε20 ρv02 = . σY 1 − ε0 Equation (7.2.9) may now be integrated, giving 2
ln
ξ L
=
1 1 1 − ε¯ − − ln . 1 − ε¯ 1 − ε0 1 − ε0
If ξ0 is the value of ξ where ε¯ = 0, then √ ξ0 = L 1 − ε0 exp −
ε0 . 2(1 − ε0 )
and the shock front stops when ξ(t) = ξ0 , so that the portion 0 < x < ξ0 remains undeformed. The preceding analysis is equivalent to that of G. I. Taylor [1948], who based it on a different approach. By means of some approximating assumptions Taylor derived a formula for the dynamic yield stress in terms of the impact speed and the specimen dimensions before and after impact. For a bar made of workhardening material, the problem was treated by Lee and Tupper [1954]. The geometry and notation are the same as in the preceding treatment. If the conventional stressstrain relation is given by σ = F (ε) and the initial yield stress is σE , then the material just ahead of
438
Chapter 7 / Dynamic Problems
the shock front may be assumed to be about to yield, so that σ = σE there, while immediately behind the front the stress is σ ¯ = F (¯ ε). The stress jump is therefore [σ] = σ ¯ − σE . From the shock relations we obtain, first, ρξ˙2 =
σ ¯ − σE , ε¯
which may be contrasted with (7.2.5), and second, ρ¯ v 2 = (¯ σ − σE )¯ ε. Proceeding as before, we obtain 2
dξ d[(¯ σ − σE )¯ ε] = . ξ σE ε¯
The initial strain at the impact end is related to the impact speed v0 by means of ρv02 = (σ0 − σE )ε0 , where σ0 = F (ε0 ). The relation between ε¯ and ξ, which provides the distribution of permanent strain along the bar, is obtained as 2
ξ ln L
Z
ε¯
= ε0
d{[F (ε) − σE ]ε} , σE ε
provided that ε¯ is positive; setting ε¯ = 0 gives ξ0 , which defines, as before, the extent of the undeformed portion. The result was used by Lee and Tupper [1954] in order to predict the permanent deformation of steel specimens, and experiments performed by them showed fairly good agreement.
7.2.2
Waves in ElasticPlastic Bars
Taking the elasticity of the bar into account changes the nature of the problem drastically. In an elastic solid, disturbances cannot be propagated at a speed faster than the elastic wave speed. It would therefore be impossible for the entire portion of the bar ahead of the plastic shock front to move as a rigid body from the moment of impact; an elastic front has to intervene. Moreover, when an elastic wave of compression reaches the free end, it is reflected as a tension wave and will bring about unloading when it reaches the plastically deforming material. At a section of the bar where the material is elastic, with Young’s modulus E, we have [σ] /[p ε] = E, so that the shock speed is just the elastic barwave speed ce = E/ρ, independent of the local state variables. The same is true when the behavior is elasticplastic, provided that the stress change across the shock represents unloading.
Section 7.2 / OneDimensional Plastic Waves
439
Donnell Theory To understand the nature of a front of loading into a plastic state, it is simplest to begin, following an approach due to Donnell [1930], by considering a material with a “bilinear” stressstrain relation (Figure 7.2.2). We σ
E0
σE
1
E 1
ε
Figure 7.2.2. Bilinear stressstrain diagram. return to the convention of stress and strain as positive in tension. If the initial state is stressfree, then any disturbance involving a stress increase up to the yield stress σE will be propagated at the aforementioned elastic speed ce . On the other hand, p stress increases above σE will travel at the slower “plastic” speed cp = E 0 /ρ. Thus in a semiinfinite bar occupying the halfline x > 0 in which at t = 0 a stress σ0 > σE is applied at the left end, we distinguish three regions, whose time dependence is shown in Figure 7.2.3: 0 : ce t < x σ = 0, I : cp t < x < ce t σ = σE , II : 0 < x < cp t σ = σ0 . The values of strain and velocity in each of the regions can be obtained from the shock relations (7.2.3); they are shown in Figure 7.2.3.
Finite Bars If the bar is of finite length, say L, and is supposed to occupy the interval 0 < x < L, then a front propagating to the right from x = 0 will, upon reaching the end x = L, be reflected as one propagating to the left. The nature of the reflected front depends on the end condition at x = L, and if the bar is elasticplastic, on the intensity of the incident front. End conditions are assumed as being of two kinds: (a) free, characterized by σ = 0, and (b) fixed , characterized by v = 0 if the frame of reference is stationary with respect to the fixed end. Consider, now, an elastic shock front, with a stress −σ0 and zero velocity behind it, moving into a region of zero stress and velocity −v0 (so that from the shock relations, σ0 = ρce v0 ) until it reaches a free right end. This is the problem of an elastic bar traveling freely to the left, at a speed v0 , until it
440
Chapter 7 / Dynamic Problems t σ = σ0 σ0 − σE σE + ε= E E0 σE σ 0 − σE v=− − ρce ρcp
σ = σE σE ε= E σE v=− ρce
! !
!! !!
II
! I !! ! ! !! ! 0 !! ! !
σ=ε=v=0
x
Figure 7.2.3. Semiinfinite bar of bilinear material: regions in xtplane. impinges upon a fixed rigid obstacle.1 Behind the reflected front the stress must be zero, so that it is a front of unloading, and therefore, by the shock relations, the velocity behind it will be +v0 . When the reflected front reaches x = 0, at the time t = 2L/ce after the initial impact, it will in turn be reflected to the right. If this end is regarded as a fixed end, then, in order to have v = 0 behind the second reflected front, the stress there must be +σ0 , that is, a tensile stress. Unless the bar somehow fuses with the obstacle, there is nothing to transmit a tensile stress between them, and therefore the assumption that the left end is fixed for t > 2L/ce must be abandoned in favor of the one that the end is free. In this case, the state behind the second reflected front has σ = 0 and v = +v0 ; that is, the bar rebounds from the obstacle. The rebound time is consequently 2L/ce . If the bar is elasticplastic, with a compressive yield stress σE , then the def preceding results are valid as long as σ0 ≤ σE , that is, if v0 ≤ σE /ρce = vE . If v0 > vE , and if the material is modeled by a bilinear stressstrain relation as on the previous page, then an elastic and a plastic shock front propagate from the impact end at the respective speeds ce and cp , and the results for the semiinfinite bar hold until the initial elastic front, with σ = −σE and v = vE − v0 behind it, reaches the free end. The reflected front, being one of unloading, is elastic, the stress behind it being zero and the velocity 2vE −v0 . def
Let α = cp /ce . The reflected elastic and initial plastic fronts meet at point A (Figure 7.2.4), with xA = 2αl/(1 + α) and tA = 2L/(1 + α)ce . 1
This problem was studied by Lenskii [1948] and De Juhasz [1949].
Section 7.2 / OneDimensional Plastic Waves
441
From this point, fronts may propagate both to the left and to the right. We assume, first, that only elastic fronts propagate, leaving behind them a region with σ = −σ1 and v = v1 . The strain cannot be uniform in this region, since plastic deformation has taken place to the left of A but not to the right of A. Thus a stationary discontinuity front, at which only the strain is discontinuous, forms at A. t
hhh ( (((
Strain
discontinuity
(( (((( ( ( ( (((
( (((( hhhh( σ=0 A (((( σ = −σ0 hhhhh v = 2vE − v0 h hhh v=0 h h hhh hhhh hhh hhhh σ = −σ0 ((( v = vE − v0 ( ( (( ( ( ( ((( σ=0 ((( ( ( ( (( v = −v0 ( ( ( ( ((((
0
L
x
Figure 7.2.4. Finite bar of bilinear material: wave reflection and intersection. The shock relations along the rightward and leftward fronts, respectively, are σ1 = ρce (v1 − 2vE + v0 ),
σ1 − σ0 = −ρce v1 .
Noting that σ0 = σE + ρcp (v0 − vE ), we obtain from these relations the solutions σ1 = 21 ρce (1 + α)(v0 − vE ) and v1 = 21 [(3 − α)vE − (1 − α)v0 ]. In order to justify the assumption that only elastic fronts propagate from A (in other words, that the plastic front is absorbed at A), we must have σ1 < σE , the condition for which is v0 < [(3 + α)/(1 + α)]vE . Let us assume that this last condition is met, and that the leftward elastic front is reflected from the impact end as though rebound occurred, as with the elastic bar, at t = 2L/c. The rebound velocity is found to be 2vE −v0 ; but this is positive only if v0 < 2vE . This, then, is the condition for rebound at t = 2L/ce . It can be ascertained that no further plastic deformation occurs, and therefore the bar is left with a permanent deformation of ε0 − σ0 /E to the left of point A. If v0 > 2vE , then the bar remains in contact with the obstacle at least until the next front reaches the left end. If 2vE < v0 < [(3 + α)/(1 + α)]vE , then the compressive stress holding them together is ρce (v0 − 2vE ).
442
Chapter 7 / Dynamic Problems
If v0 > [(3 + α)/(1 + α)]vE , then the plastic front continues to the right beyond A. Ahead of it, we have σ = −σE and v = 3vE − v0 . If the stress and velocity behind it are again denoted −σ1 , v1 , then the shock relations are σ1 − σE = ρcp (v1 − 3vE + v0 ), σ1 − σ0 = −ρce v1 , yielding v1 = 2αvE /(1 + α). It is clear that the numerical problem of determining the rebound time becomes more complex as the impact velocity increases. Some solutions are shown in Figure 7.2.5.
K´arm´an–Taylor–Rakhmatulin Theory It is not difficult to extend the Donnell theory to materials whose stressstrain curve consists of more than two line segments, provided that the overall curve is convex downward. Such a curve may in turn be regarded as an approximation to one that is smooth beyond the yield stress (Figure 7.2.6). It is clear that as the segments become shorter, the jumps in the field quantities at the plastic shock fronts become smaller. If the smooth curve is seen as the limit of the segmented one, then it follows that in a bar made of a material described by the smooth curve, no plastic shock fronts can be propagated. The theory that was developed independently by Taylor [1946, 1958], von K´arm´an (see K´arm´an and Duwez [1950]) and Rakhmatulin [1945] during World War II is based on complementing the basic field equations (7.2.1)– (7.2.2) with the constitutive equation σ = F (ε).
(7.2.10)
While its form is that of a nonlinear elastic stressstrain relation, Equation (7.2.10) is assumed in this theory to hold only during an initial loading process, unloading being linearly elastic. An initial yield stress σE may be incorporated if F (ε) = Eε for ε < ε0 , where ε0 = σE /E (here it is assumed that the initial loading curves are the same in tension and compression). The function F (·) is assumed to be continuously differentiable, with F 0 (ε) > 0, and convex in the sense that εF 00 (ε) ≤ 0. A solution to the system of equations (7.2.1), (7.2.2), and (7.2.10) that may be valid for some problems, at least in a certain region of the xtplane, can be obtained by assuming that the three variables σ, v, ε depend on x and t only through the combination c = x/t, that is, that they are constant along lines of slope c emanating from (0, 0). (Such a solution is sometimes called a “similarity” solution.) Since ∂c/∂x = 1/t and ∂c/∂t = −c/t, Equations (7.2.1)–(7.2.2) become dv = −c dε,
dσ = −ρc dv.
(7.2.11)
Section 7.2 / OneDimensional Plastic Waves
t
t ce + cp (v0 − vE ) σ1 = ρ 2 1 v1 = [(3 − α)vE − (1 − α)v0 ] 2
vr 0, X vr = (1 − α)vE + αv0 X + X tr XX XXXX XX XXXXXXX XXX X X X ρce v0 −2σE , 0 XX 0, vr 1 t0 X X 0, 2vE −v0 σ0 , 0 XXX XX XXX XXX σE , vE −v0 0, −v0 x
0, 2vE −v0
t0 XX1 0, 2v −v 0 E σ0 , 0 XXX XX XXX XXX 1 σE , vE −v0 cp ce 1 0, −v0 0
443
v0 , A being constant, the resulting equation for g(σ, ε) is just the onedimensional version of the Hohenemser–Prager model [Equation (3.1.3)]. The use of constitutive equations of the form (7.2.16) is not limited to materials that are viscoplastic in the classical sense, that is, those that are characterized by a static yield stress below which the behavior is elastic. It is used in creep models such as the Bailey–Norton–Nadai law [see Equation (2.1.6)], with g(σ, ε) = Bσm ε − σ/E−n sgn σ. A generalized constitutive equation that includes both the rateindependent and the Malvern models as special cases was proposed in the early 1960s by Simmons, Hauser, and Dorn [1962], Cristescu [1964], and Lubliner [1964]. This equation has the form ∂ε ∂σ = f (σ, ε) + g(σ, ε) ∂t ∂t
(7.2.17)
for loading (σ∂σ/∂t > 0); for unloading, f (σ, ε) is replaced by 1/E, or if finite strains must be taken into account, (1 − ε)2 /E. The Malvern theory corresponds to the special case f (σ, ε) ≡ 1/E, and the KTR theory is recovered if f (σ, ε) = 1/F 0 (ε) and g(σ, ε) ≡ 0. Explicit calculations by Lubliner [1965] and by Lubliner and Valathur [1969] show that solutions of impact problems according to the generalized theory tend to those of the KTR theory if the bar is short, the impact is strong, and if the viscoplastic relaxation time is long, while under the converse conditions the results of the Malvern theory are approached.
448
Chapter 7 / Dynamic Problems
7.2.4
Application of the Method of Characteristics
Characteristic Relations The three equations (7.2.1), (7.2.2), and (7.2.17) form a system of partial differential equations for the unknown variables σ, v, and ε. (Note that in using these equations we are returning to treating stress and strain as positive in tension.) As in Section 5.1, it is simpler to consider first a single firstorder partial differential equation of the form A
∂v ∂v +B = C, ∂x ∂t
where A, B, and C are functions of x, t, and v. Rewriting the equation as ∂v A ∂v B dt + dt = C dt, ∂x B ∂t
we find that the lefthand side is proportional to dv = (∂v/∂x) dx+(∂v/∂t) dt if dx = c dt, where c = A/B; the characteristic direction is thus defined by dx/dt = c. Along a characteristic, then, dx dt dv = = . A B C If a discontinuity in v, resulting from the intersection of two characteristics of the same family, should propagate, then it forms a shock front, as discussed in 7.2.1. Any discontinuity in ∂v/∂t or ∂v/∂x that is propagated through the xtplane must (as discussed in 5.1.1) be across a characteristic, and dx/dt = c is just the speed with which the front carrying the jump is propagated. If v is the velocity, then a front across which the acceleration ∂v/∂t is discontinuous is called an acceleration wave. The system formed by Equations (7.2.1)–(7.2.2) and (7.2.17) is equivalent to
λ1
∂v ∂σ ρ − ∂t ∂x
+ λ2
∂ε ∂v − ∂t ∂x
+ λ3
∂ε ∂σ −f − g = 0, ∂t ∂t
where λ1 , λ2 , λ3 are arbitrary multipliers. Let us regroup the terms of this equation so that it takes the form ∂σ ∂σ ∂v ∂v ∂ε λ1 + λ3 f + λ2 − λ1 ρ − (λ2 + λ3 ) + λ3 g = 0. ∂x ∂t ∂x ∂t ∂t
The determination of the characteristics of the system is tantamount to finding the values of dx/dt for which the bracketed terms in the last equation are proportional, respectively, to dσ, dv, and dε, where dσ =
∂σ ∂σ dx + dt ∂x ∂t
Section 7.2 / OneDimensional Plastic Waves
449
and likewise for dv and dε. The possible values of dx/dt must satisfy dx λ1 λ2 0 . = =− = dt λ3 f λ1 ρ λ 2 + λ3 One way that all these equations can be obeyed is if (a) λ1 = λ2 = 0, λ3 arbitrary (let λ3 = 1). Two other possibilities are given by (b) λ2 = −λ3 and s
(c)
λ1 =± λ2
f . ρ
In case (a) we have dx = 0. dt In cases (b) and (c), dx λ1 =− = ±c, dt λ2 f
√ where c = 1/ ρf . If f is positive, then at each point there exist three distinct characteristic directions, which accordingly define three families of characteristic curves in the xtplane. Since the number of characteristic directions equals the number of unknown variables, the system of equations is hyperbolic, as in 5.1.1. Along an infinitesimal characteristic segment of family (a) we have dx = 0, and therefore changes in the unknown variables are given by Equation (7.2.17), that is, f dσ − dε + g dt = 0
along dx = 0.
(7.2.18a)
Along characteristic segments of families (b) and (c), respectively, we obtain the relations g dσ = ρc dv − dt along dx = c dt, (7.2.18b) f g dσ = −ρc dv − dt along dx = −c dt. (7.2.18c) f
Viscoplastic Bars For a bar made of an elasticviscoplastic material governed by (7.2.16) (with infinitesimal strains), the characteristic relations (7.2.18) become 1 dσ − dε + g dt = 0 E dσ = ρce dv − Eg dt
along dx = 0, along dx = ce dt,
dσ = −ρce dv − Eg dt along dx = −ce dt.
450
Chapter 7 / Dynamic Problems
Since the characteristics are straight, the numerical integration of these equations is quite straightforward. For certain simple forms of the function g, the equations may be solved analytically. Examples include solutions by Sokolovskii [1948] and by Kaliski and Wlodarczyk [1967] for g(σ, ε) =< σ − σY > (sgn σ)/η (the Hohenemser–Prager model), and by Cristescu and Predeleanu [1965] for g given by 1 g(σ, ε) = η
E0 1+ σ − E 0 ε − σE sgn σ , E
σ > σE ,
with g = 0 for σ < σE .
RateIndependent Bars; Unloading Wave Since the KTR theory corresponds to g == 0, it is clear that Equations (7.2.11) representing the “similarity” solution are just the characteristic relations along characteristics of family (c), these characteristics being curved. The lines x = ct along which the state variables are constant are the characteristics of family (b). The characteristic network for the problem of constantvelocity impact on a semiinfinite bar made of a rateindependent material is shown in Figure 7.2.8(a). t
t Unloading wave
v v0
A AA A A A A A A % A % (c) A % A % A % (b) A % % (a) % x % (a)
BBN X X tm
v v m vE
X X X X X X X X XX X X X X x (b)
Figure 7.2.8. Characteristic networks for impact on a semiinfinite bar made of a rateindependent material: (a) constantvelocity impact; (b) impact velocity rising to a peak and declining. Suppose, now, that the impact is not sudden, but that the boundary condition at x = 0 has the form v(0, t) = v0 (t), where v0 (0) = 0 and, for t > 0, v0 is a continuous function that increases with t until it reaches a maximum value vm at t = tm , after which it decreases. As before, we may suppose the characteristics of family (a) to be straight lines along which σ, v, and ε are constant. Rather than all of them emanating
Section 7.2 / OneDimensional Plastic Waves
451
from (0, 0), however, each one originates from a point on the taxis such that v = v0 (t). We may integrate the characteristic relations along families (b) and (c) to obtain Z ε
c(ε)dε,
v=
σ = F (ε).
0
The second of these equations, however, is valid only in a loading process, that is, only as long as ∂σ/∂t > 0. Since σ and v are monotonically related, at x = 0 this condition prevails only for t < tm . What happens then? As first demonstrated by Rakhmatulin [1945], a front behind which ∂σ/∂t ≤ 0, called an unloading wave [see Figure 7.2.8(b)], begins to propagate into the plastically deforming region of the bar. Since in this region ∂σ/∂t > 0, across this front the stress rate ∂σ/∂t, and therefore also the strain rate ∂ε/∂t and the acceleration ∂v/∂t, are discontinuous. An unloading wave is therefore an acceleration wave. The calculation of the unloading wave in the xtplane must be performed step by step. Its speed, say cu , is initially c(εm ), where εm is the strain at (0, tm ). An example of a graphic construction, due to Rakhmatulin and Shapiro [1948], is shown in Figure 7.2.9 (taken from Cristescu [1967]) for a bar in which the stress at the end of the bar first increases monotonically, then remains constant for a while, and finally decreases monotonically to zero. As can be seen, the speed of the unloading wave increases as the wave t
−σ
t
!S ! !! 4 P Y H 3 ``` HH ` ...... . . . . . . . . . . . ........ 2 Unloading wave ...................................................................... . . . . . . . . 1............................... .. Constantstate region ..... ...................... . ............. . ... 0 Y σ m σE
0
x
Figure 7.2.9. Approximate construction of unloading wave (Cristescu [1967]). propagates. It was shown by Lee [1953] that the unloadingwave speed is bounded by c(ε) ≤ cu ≤ ce . A proof of this result is given in Section 7.3, in which the general theory of elasticplastic acceleration waves is studied. In his first paper, Rakhmatulin [1945] erroneously showed the unloading wave as attaining speeds faster than that of the elastic wave (see the discussion by Bodner and Clifton [1966]). More information on wave propagation in elasticplastic and elasticviscoplastic bars can be found in the books by Cristescu [1967], Chapters II
452
Chapter 7 / Dynamic Problems
and III, and Nowacki [1978], Chapter III.
Exercises: Section 7.2 1. Discuss how a shock front might form in an elasticplastic bar whose stressstrain curve beyond the initial yield stress σE is given by σ = σE {1 + [(ε − σE /E)/α]2 }. Consider the limit of a rigid–plastic bar (E = ∞). 2. For a given impact velocity v0 , find the distribution of permanent strain following impact in a rigid–plastic bar of length L when the stressstrain relation beyond the initial yield stress is given by F (ε) = σE [1 + (ε/α)1/m ]. Letting αp= 1 and m = 5, plot the strain distributions for various values of v0 / σE /ρ. 3. Repeat Exercise 2 for the stressstrain relation of Exercise 1 with α = 1. 4. An elasticplastic bar with linear workhardening, of initial length L, strikes a rigid obstacle at t = 0. Find the rebound time in terms of L/ce and α = cp /ce when v0 /vE is 3, 4, and 5. 5. A semiinfinite elasticplastic bar with linear workhardening (with tangent modulus E 0 in the plastic range) is subjected at time t = 0 to a stress σ0 > σE which remains constant until t = t0 , whereupon it is removed. Discuss the motion of the bar for various ranges of σ0 . 6. Repeat Exercise 5 for bars with the stressstrain relations of Exercises 1 and 2. 7. A semiinfinite viscoplastic bar with the constitutive equation (7.2.16) is subjected to a suddenly applied stress or velocity. Find the equation governing the decay of the stress discontinuity along the initial shock front. Show that the decay is exponential if g(σ, ε) is a linear function of its arguments for σ > σE .
Section 7.3
ThreeDimensional Waves
Threedimensional waves in rateindependent elasticplastic solids appear to have been studied first by Craggs [1957], who found relations for the speeds of plastic waves on the basis of the characteristics of the governing differential equations. As in the onedimensional case, the characteristic speeds coincide with those of acceleration waves, and in this section only the accelerationwave approach is followed. Furthermore, only rateindependent elasticplastic solids are discussed. In elasticviscoplastic solids
Section 7.3 / ThreeDimensional Waves
453
the wave speeds are those of elastic waves, while the study of specific dynamic boundaryvalue problems must, as a rule, be pursued numerically, except when the constitutive model is so simple that analytical methods, analogous to those used for linearly viscoelastic solids, may be used; examples of both approaches are given in the book by Nowacki [1978]. Acceleration waves in elasticplastic solids were first investigated by Thomas [1958, 1961] for perfect plasticity, and with greater generality by Hill [1962] and Mandel [1962].
7.3.1
Theory of Acceleration Waves
General Theory The general theory of acceleration waves is due to Hadamard [1903]; a modern exposition may be found in the monograph by Truesdell and Toupin [1960]. It is presented here in a simplified form suitable for infinitesimal deformations. We consider an acceleration wave moving in x1 x2 x3 space at the speed c. The unit normal vector to the wave surface, pointing in the direction of wave motion, will be denoted n. The jump operator [·] will be used as previously defined, and the superposed dot will denote ∂/∂t. A timedependent field φ is assumed to be continuous across the wave but to have possibly discontinuous derivatives. At time t, φ has the value φ(x1 , x2 , x3 , t) at a point of the wave front. At an infinitesimally later time t + dt, the given point will have moved to xi + ni c dt, i = 1, 2, 3, and φ will accordingly have the value φ(x1 , x2 , x3 , t) + dφ, where ˙ dφ = φ,i ni c dt + φdt. The continuity of φ requires [dφ] = 0, or ˙ . cni [φ,i ] = −[φ] Since, however, it is only the component of delφ along n that undergoes a jump, [φ,i ] must be proportional to ni , and therefore, since nj nj = 1, ˙  nj . c[φ,j ] = −[φ] The last result is known as the Hadamard compatibility condition. When applied to the velocity field v, the condition yields c[vi ,j ] = −[v˙ i] nj . When applied to the stress field σ and combined with the momentumbalance equation (1.3.1), it gives [σ˙ ij] nj = −ρc[v˙ i] .
454
Chapter 7 / Dynamic Problems
If, finally, the material is characterized by an effective tangent modulus ten¯ such that sor C [σ˙ ij] = C¯ijkl [ε˙ij] , then combining all the results of this paragraph yields the eigenvalue problem (Qik − ρc2 δik )[v˙ k] = 0, where
def Qik = C¯ijkl nj nl
(7.3.1)
defines the acoustic tensor Q. The eigenvalues of Q, if positive, equal ρc2 ˙  or with c the wave speed, while the eigenvectors are the directions of [v] polarization directions.
Elastic Waves ¯ is If the material is linearly elastic, then the tangent modulus tensor C just the elastic modulus tensor C, and the corresponding acoustic tensor will be denoted Qe : Qeik = Cijkl nj nl . (7.3.2) If the material is also isotropic, then C is given by Equation (1.4.10), and Qe is given by Qeik = (λ + µ)ni nk + µδik . One eigenvector is obviously n, with the corresponding eigenvalue being λ + 2µ, so that the wave speed is s
ce1
=
λ + 2µ = ρ
s
1−ν ce , (1 + ν)(1 − 2ν)
p
where ce = E/ρ is the elastic barwave speed defined in the preceding section. Since the polarization direction coincides with that of propagation, a wave of this nature is called longitudinal ; it is also known a dilatational wave or a Pwave. Any vector perpendicular to n is also an eigenvector of Q and corresponds to the degenerate eigenvalue µ. The polarization being perpendicular to the wave normal, the wave is called transverse (also a shear wave or an Swave), and its speed is r µ e c2 = . ρ As in the bar studied previously, the elastic accelerationwave speeds in threedimensional solids are independent of the local field variables, so that all disturbances, including sufficiently weak shocks, travel at these speeds. A shock is “sufficiently weak” if it does not entail temperature and/or density changes large enough to affect the elastic moduli.
Section 7.3 / ThreeDimensional Waves
455
ElasticPlastic Waves We now consider an acceleration wave propagating in a standard elasticplastic solid as described in Section 3.2, with a yield function f . If f < 0 at the wave front, then the solid is behaving elastically, and the wave is an elastic one. It will therefore be assumed that f = 0 at the wave front. Then the relation (3.2.10) between stress rate and strain rate, with the normality rule (3.2.7) incorporated, may be written, following Hill [1959], in the form 1 σ˙ ij = Cijkl ε˙kl − Cijmn mmn , l
(7.3.3)
where
mij = s
∂f ∂σij
,
∂f ∂f ∂σkl ∂σkl
g = Cpqkl mpq ε˙kl ,
l = h + Cklmn mkl mmn ,
h being a plastic modulus, not exactly the same as in Section 3.2, but to be specified more precisely later. Note that m is a unit tensor, that is, mij mij = 1. Applying the jump operator to Equation (7.3.3) yields 1 [σ˙ ij] = Cijkl [ε˙kl] − Cijmn mmn [] . l We may now write [] = η[g] , where η is a real number that depends on the ranges of g + and g − . Several cases may be distinguished: (a) (b) (c) (d)
g+ g+ g+ g+
> 0, > 0, ≤ 0, ≤ 0,
g− g− g− g−
>0: ≤0: >0: ≤0:
η = 1, 0 < η < 1, 0 < η < 1, η = 0.
In addition, we may consider the situation where the material ahead of the wave is about to yield (i.e., g + > 0), but is still elastic (i.e., σ˙ + = C · ε˙ + ). Since g − > 0 also, we have η=
g− , g− − g+
and thus obtain two additional cases: (e) g − > g + : η > 1, (f) g − < g + : η < 0.
456
Chapter 7 / Dynamic Problems
The waves represented by these cases can be categorized as follows, according to Mandel [1962]: case (a) represents a plastic wave, with the material deforming plastically on both sides; case (b) an unloading wave; and case (d) an elastic wave. Case (c), which was not considered by Mandel, can be called a reloading wave. Cases (e) and (f) represent loading waves; the former will here be called strong and the latter weak . ¯ may now be expressed as The effective tangent modulus C C¯ijkl = Cijkl − ηNij Nkl , √ where Nij = Cijkl mkl / l. The acoustic tensor Q accordingly may be written in the form Qij = Qeij − ηdi dj , def
where Qe is given by (7.3.2), and di = Nik nk defines a vector d that Hill [1962] calls the “traction” exerted by N on the wave front.
Analysis of Wave Speeds The analysis to be presented is based on that of Mandel [1962]. Since Q is symmetric, it has real eigenvalues and mutually perpendicular eigenvectors. Whenever such an eigenvalue —psay A — is positive, it represents a a wave propagated at the speed c = A/ρ. The symmetry of Q is due to the assumption of an associated flow rule; the propagation of acceleration waves in nonstandard elasticplastic materials was also studied by Mandel [1964], whose conclusions are summarized later. In what follows, the eigenvalues of Q and Qe will be denoted Aα and Aeα (α = 1, 2, 3), respectively, with the ordering A1 ≥ A2 ≥ A3 and Ae1 ≥ Ae2 ≥ Ae3 . If a Cartesian basis is chosen along the eigenvectors of Qe , then the characteristic equation of Q is F (A) = 0
(7.3.4)
where F (A) = det(Q − IA) Ae − ηd2 − A −ηd1 d2 1 1 e −ηd1 d2 A2 − ηd22 − A = −ηd1 d3 −ηd2 d3
−ηd1 d3 −ηd2 d3 Ae1 − ηd23 − A
= (Ae1 − A)(Ae2 − A)(Ae3 − A) − η[d21 (Ae2 − A)(Ae3 − A) + d22 (Ae1 − A)(Ae3 − A) + d23 (Ae1 − A)(Ae2 − A)]. The character of the roots of Equation (7.3.4) depends on η. The simplest case is η = 0, corresponding to an elastic wave. In this case, of course, Aα = Aeα (α = 1, 2, 3).
Section 7.3 / ThreeDimensional Waves
457
If η > 0, as in cases (a)–(c) and in case (e), then F (Ae1 ) = −ηd21 (Ae1 − Ae2 )(Ae1 − Ae3 ) ≤ 0. Similarly, F (Ae2 ) ≥ 0, F (Ae3 ) ≤ 0, and F (−∞) = +∞. Consequently,1 A3 ≤ Ae3 ≤ A2 ≤ Ae2 ≤ A1 ≤ Ae1 . Furthermore, the Aα decrease monotonically with η. If Apα denotes the value of Aα for η = 1 (plastic wave), and Auα a value of Aα for 0 < η < 1 (unloading and reloading), then we have the inclusion Apα ≤ Auα ≤ Aeα ,
α = 1, 2, 3.
Here we see the bounding of the wave speed of an unloading wave, previously obtained by Lee [1953] for waves in a thin bar.2 The speeds of strong loading waves, case (e), are even slower than those of plastic waves. The inclusions are p Asl 3 ≤ A3 ,
p Ae3 ≤ Asl 2 ≤ A2 ,
p Ae2 ≤ Asl 1 ≤ A1 .
In fact, Asl 3 may be zero, in which case the surface does not propagate. In a weak loading wave, case (f), η is negative and therefore the nature of the roots changes drastically. The ordering of the wave speeds is p Ae3 ≤ Awl 3 ≤ A2 ,
p Ae2 ≤ Awl 2 ≤ A1 ,
Ae1 ≤ Awl 1 .
The existence of waves propagating faster than elastic waves (in a bar) was apparently first noted by Lee [1953]. Mandel [1962] gave, as an example of such a wave moving at an infinite speed, the loading wave in a finite bar following reflection from a fixed end. An analysis of plastic waves in a nonstandard material, also due to Mandel [1964], shows that (a) the eigenvectors of Q are not mutually perpendicular, (b) Ap3 may be negative (representing a slip or rupture surface rather than a wave), and (c) Ap1 may be greater than Ae1 . While soils are usually modeled as nonstandard in static problems, theories of waves in soils have typically been based on standard elasticplastic models, for example by Grigorian [1960] and by Chadwick, Cox, and Hopkins [1964].
Isotropically Elastic Materials If the material is elastically isotropic, with the modulus tensor given by (1.4.10), and if in addition it is plastically incompressible (tr ε˙ p = 0), so that mkk = 0, then Cijkl mij mkl = 2µmij mij = 2µ, 1 It was also shown by Mandel [1962] that A3 > 0 for η ≤ 1, except that Ap3 may be zero if the material is perfectly plastic. 2 As pointed out in the preceding section, Rakhmatulin’s [1945] finding of an unloading wave propagating faster than the elastic wave is erroneous.
458
Chapter 7 / Dynamic Problems l = h + 2µ,
g = 2µmkl ε˙kl ,
and Nij = √
2µ mij . h + 2µ
If plastic isotropy is also assumed, then the hardening modulus h can be related very simply to the uniaxial tangent modulus as well as to the tangent modulus in shear. Recalling the definition of g and multiplying every term of Equation (7.3.3) by mij , with contraction implied, we obtain
1 2µh Cijkl mij mkl g = mkl ε˙kl . h + 2µ h + 2µ
mij σ˙ ij = 1 −
In a quasistatic uniaxial test, the lefthand side is just m11p σ˙ 11 . Moreover, 1 mij = 0 for i! = j and m22 = m33 = − 2 m11 , so that m11 = 2/3, and r
mkl ε˙kl =
2 (ε˙11 − ε˙22 ). 3
Consequently, σ˙ 11 =
2µh (ε˙11 − ε˙22 ). 2µ + h
Plastic incompressibility further implies that σ˙ 11 = (3λ + 2µ)(ε˙11 + 2ε˙22 ). Eliminating ε˙22 , we obtain the tangent compliance λ + µ + 2µ(3λ + 2µ)/3h 1 2 ε˙11 = = + , σ˙ 11 (3λ + 2µ)µ E 3h so that h = 23 H, where H = dσY /dεp is the uniaxial tangent plastic modulus. It can also be easily shown that h is twice the shearing tangent plastic modulus dτY /dγ p . The eigenvector of Qe corresponding to the fastest elastic wave (the longitudinal wave) is of course n. If this is identified with e1 , then d is given by 2µ mi1 . di = δik Nk1 = √ h + 2µ Since any vector perpendicular to n is also an eigenvector of Qe , we are free to choose e2 and e3 in the tangent plane of the wave; let us choose them so that d3 = 0. The eigenvalue problem now reads
λ + 2µ − ηd21 − A −ηd1 d2 0 ˙ = ˙ . −ηd1 d2 µ − ηd22 − A 0 [v] 0 = (Q − AI)[v] 0 0 µ−A (7.3.5)
Section 7.3 / ThreeDimensional Waves
459
Obviously, one eigenvector is e3 , with the corresponding eigenvalue A2 = µ = Ae2 = Ae3 (necessary because Ae3 ≤ A2 ≤ Ae2 ). Hence, at any η, an elastic transverse wave can propagate. If η > 0, then we also have A3 ≤ Ae2 ≤ A1 ≤ Ae1 , a result first derived by Craggs [1957]. The waves corresponding to A1 and A3 are in general neither longitudinal nor transverse, unless d1 d2 = 0. When neither d1 nor d2 is zero, the waves are called longitudinal–transverse.
7.3.2
Special Cases
Purely Longitudinal and Transverse Waves (a) If d2 = 0, then A3 = µ and the polarization is along e3 . In this case both transverse waves are elastic, while for the longitudinal wave we obtain A1 = λ + 2µ − ηd21 = λ + 2µ − η
4µ2 m2 . h + 2µ 11
The tensor m can be shown to have the same form as in the quasistatic uniaxial test: m13 = 0 because d3 = 0 by choice of basis, m12 = 0 because d2 = 0 by hypothesis, m23 = 0 because [ε˙23]p= 0, and m22 = m33 = − 12 m11 from the resulting symmetry; hence m11 = 2/3, and A1 = λ + 2µ −
4ηµ . 3(1 + h/2µ)
(7.3.6)
Note that for h = 0 (perfect plasticity) and η = 1 (plastic wave) we have A1 = λ + 23 µ = K, the elastic bulk modulus. In this case the longitudinal wave may be said to propagate as though the material were a fluid. (b) If d1 = 0, then, by contrast, it is the longitudinal wave that is elastic (A1 = λ + 2µ), and in addition to the elastic transverse wave with A2 = µ, there is a transverse wave with A3 = µ − ηd22 = µ − η
4µ2 m2 . h + 2µ 12
It can easily be shown √that this case is equivalent to quasistatic simple shear, so that m12 = 1/ 2, and ηµ A3 = µ − . (7.3.7) 1 + h/2µ For η = 1 (plastic wave), A3 reduces to the tangent modulus in shear, µh/(2µ + h). If h = 0 (perfect plasticity), then A3 = (1 − η)µ, so that a transverse plastic wave (η = 1) or a transverse strong loading wave (η > 1) cannot be propagated.
Longitudinal–Transverse Waves In an isotropic and homogeneous halfspace, say x1 > 0, whose boundary x1 = 0 is subject to timevarying tractions (or displacements) that are
460
Chapter 7 / Dynamic Problems
uniform over the plane (i.e., independent of x2 and x3 ), all the field variables may be assumed to be functions of x1 and t only, and the wave is said to be plane. A plane wave is longitudinal if the traction or displacement is purely normal, and transverse if the traction or displacement is purely tangential. If the boundary tractions or displacements include both normal and tangential components, then the wave is longitudinal–transverse. The propagation of longitudinal–transverse plane waves in an elasticperfectly plastic halfspace was studied by Bleich and Nelson [1966], and in an elasticplastic halfspace with workhardening by Ting and Nan [1969]; for further references, see Nowacki [1978], Section 22. Here, we limit ourselves to finding expressions for the wave speeds through a direct application of Equation (7.3.5). If the tangential traction is in the x2 direction, then the halfspace can be assumed to be in a state of plane strain, so that, if the material is isotropic, σ13 = σ23 = 0. Furthermore, all field quantities, including the velocity, can be assumed to be independent of x2 , so that ε˙22 = 0. The L´evy–Mises flow rule requires that σ22 = σ33 , and the stressdeviator tensor is given by
s τ 0 0 , s = τ − 12 s 0 0 − 21 s where s = written as
2 3
(σ11 − σ22 ) and τ = σ12 . The Mises yield criterion may be 3 2 s + τ 2 = k2 . 4
(7.3.8)
The “traction” vector d has the components s
d1 =
2 µ s, h + 2µ k
s
d2 =
2 µ τ, h + 2µ k
d3 = 0.
The characteristic equation is, accordingly, 2µ2 s2 λ + 2µ − A − η h + 2µ k 2
!
!
2µ2 τ 2 4µ4 s2 τ 2 2 µ−A−η −η = 0. h + 2µ k 2 (h + 2µ)2 k 4
Upon multiplying the equation by 2k(h + 2µ)/µ, we may rewrite it as 3s2 (A − µ){A − [K + 34 (1 − η)µ]} h +4τ 2 (A − λ − 2µ)[A − (1 − η)µ] + 2k 2 (A − λ − 2µ)(A − µ) = 0. µ It can easily be ascertained that the special cases τ = 0 and s = 0 lead to Equations (7.3.6) and (7.3.7), respectively. For a plastic wave (η = 1) in an
Section 7.3 / ThreeDimensional Waves
461
elasticperfectly plastic medium (h = 0) the equation reduces to the result of Bleich and Nelson [1966]: 3s2 (A − µ)(A − K) + 4τ 2 A(A − λ − 2µ) = 0. A problem closely related to that of longitudinal–transverse waves plane waves in a halfspace is that of longitudinal–torsional waves in a long thinwalled cylindrical tube. This problem was studied by Clifton [1966, 1968] and T. C. T. Ting [1969].
Spherical Radial Wave Purely longitudinal waves arise when the loading is spherically or cylindrically radial, such as that produced by the explosion of a point charge or a line charge in an infinite medium. The cylindrical problem is relatively complicated, since the condition of plane strain must be enforced, and the problem depends on the yield criterion chosen. The spherical problem is fairly simple; it was first treated by Lunts [1949]. In an isotropic and plastically incompressible elasticplastic solid, a spherically symmetric state of deformation requires εpθ = − 21 εpr , and is equivalent to a state of uniaxial stress equal to σr − σθ . The yield criterion may be written as σr − σθ  = σY (εpr ), where σ = σY (εp ) is the uniaxial relation between yield stress and plastic strain. If, now, H is again the uniaxial plastic modulus, then ε˙pr =
1 <sgn (σr − σθ )(σ˙ r − σ˙ θ )> H
when the yield criterion is obeyed. It will be assumed that the loading is compressive, that is, that σr − σθ = −σY . If v denotes the radial velocity, and if (·)0 = ∂(·)/∂r, then the radial and tangential strain rates are given by σ˙ r − 2ν σ˙ θ − , E H (1 − ν)σ˙ θ − ν σ˙ r v = + . r E 2H
v0 =
(7.3.9)
The equation of motion is σr0 + 2
σr − σθ = ρv. ˙ r
Applying the jump operator to this equation leads to [σr0 ] = ρ[v] ˙  . If, as 2 before, A = ρc , where c is the wave speed, then the Hadamard compatibility conditions give [v 0] = ρ[σ˙ r] /A. Since the velocity itself is continuous at
462
Chapter 7 / Dynamic Problems
an acceleration wave front, application of the jump operator to Equations (7.3.9) produces the two homogeneous linear equations for [σ˙ r] , [σ˙ θ] :
1 1 1 [σ˙ r] − + − H E A
1 ν − + 2H E
[σ˙ r] +
1 2ν + H E
1 1−ν + 2H E
[σ˙ θ] = 0,
[σ˙ θ] = 0,
if it is assumed that the wave is a compressive plastic wave, that is, σθ −σr = σY and σ˙ θ − σ˙ r > 0. Setting the determinant of the two equations equal to zero gives E + 2(1 − ν)H E A= . 3E + 2(1 + ν)H 1 − 2ν Since h = 23 H, it can easily be seen that this equation is equivalent to (7.3.6) with η = 1.
Cylindrical Shear Wave A purely transverse wave will be propagated cylindrically if, for example, a rigid axle, embedded in an infinite medium, suddenly has a torque applied to it. If the medium is isotropic, then it may be assumed that the only velocity component is the circumferential velocity vθ = v(r, t) and the only stress component is σrθ = σθr = τ (r, t). The equation of motion is τ0 + 2
τ = ρv, ˙ r
from which [v 0] = [τ˙ ] /A. If the shear strain is γ, then γ˙ = v 0 −
v τ˙ 3 = + , r µ H
so that [v 0] =
and thus A=
1 3 + µ H
[τ˙ ] ,
µH , H + 3µ
a result equivalent to (7.3.7) with η = 1. The propagation of the wave was studied by Rakhmatulin [1948].
Exercises: Section 7.3 1. Show that in an elastically isotropic material, the plastic modulus h is twice the tangent plastic modulus in shear. 2. Find the eigenvalues A1 and A3 of Equation (7.3.5) in the general case.
Section 7.3 / ThreeDimensional Waves
463
3. Show that the state of stress in a purely transverse wave is that of simple shear. 4. Using suitable assumptions, establish the governing equations of combined longitudinal–torsional wave propagation in a long thinwalled elasticplastic cylindrical tube. 5. For a Mises material with linear workhardening, find explicit expressions for the wave speeds of longitudinal–transverse plastic waves in terms of the ratio of normal stress to shear stress at the wave. 6. Find the speed of a spherically radial elasticplastic wave as a function of η.
464
Chapter 7 / Dynamic Problems
Chapter 8
LargeDeformation Plasticity Section 8.1
8.1.1
LargeDeformation Continuum Mechanics
Continuum Deformation
As a model of mechanical behavior, plasticity theory is applicable primarily to those solids that can experience inelastic deformations considerably greater than elastic ones. But the resulting total deformations, and the rotations accompanying them, may still be small enough so that many problems can be solved with smalldisplacement kinematics, and this is the situation that has, with a few exceptions, thus far been addressed in this book. However, when strains or rotations become so large that they cannot be neglected next to unity, the mechanician must resort to the theory of large or finite deformations. Since the reference and displaced configurations of a body, as discussed in Section 1.2, may be quite different, it is appropriate to use a notation that makes the difference apparent, a notation based on that introduced by Noll [1955] and made current by the monograph of Truesdell and Toupin [1960]. A material point is denoted simply X, and its Lagrangian coordinates are denoted XI (I = 1, 2, 3); a point in the current or displaced configuration is denoted x, and its Cartesian coordinates (sometimes called Eulerian coordinates) are xi (i = 1, 2, 3). Different indices are used for the two coordinate systems because the corresponding bases, the Lagrangian basis (eI ) and the Eulerian basis (ei ), are, in principle, independent of each other. Whenever direct notation is used for tensors in this chapter, vectors are treated as column matrices and secondrank tensors as square matrices; thus uT v is used for the scalar product u · v, while AB denotes the secondrank tensor with components Aik Bkj . Furthermore, the scalar product of two secondrank tensors is A : B = tr (AT B). If Γ is a fourthrank tensor, 465
466
Chapter 8 / LargeDeformation Plasticity
then Γ : A denotes the secondrank tensor with components Γijkl Akl . In particular, a fourthrank tensor with components ∂Uij /∂Vkl will be denoted ∂U/∂V, and the secondrank tensor with components ∂Uij /∂Vkl Akl will be denoted (∂U/∂V) : A.
Deformation Gradient The motion of the body is described by the functional relation x = χ(X, t). When χ is continuously differentiable with respect to X, then the deformation gradient at X is the secondrank tensor F(X, t) whose Cartesian components are ∂χi FiI = . ∂XI Note that these components are evaluated with respect to both bases simultaneously; in the terminology of Truesdell and Toupin [1960], the deformation gradient is a twopoint tensor . If, in a neighborhood of the material point X, the function χ(X, t) is invertible — in other words, if the material points in the neighborhood are in onetoone correspondence with their displaced positions — then, by the implicit function theorem of advanced calculus, the matrix of components of F(X, t) (the Jacobian matrix) must be nonsingular, that is, J(X, t) 6= 0, def where J(X, t) = det F(X, t) is the Jacobian determinant. If we consider only displaced configurations that can evolve continuously from one another, then since J = 1 when the displaced and reference configurations coincide, we obtain the stronger condition J(X, t) > 0. −1 (X, t) The inverse of F(X, t), denoted F−1 (X, t), has the components FIi −1 = ∂XI /∂xi x=χ(X, t) . Note that F is also a twopoint tensor, but of a different kind from F: while the components of the latter (FiI ) are such that the first index refers to an Eulerian and the second to a Lagrangian basis, −1 in the former it is the reverse (FIi ).
Local Deformation Consider two neighboring material points X and X0 = X + u, where u is a “small” Lagrangian vector emanating from X. If the displaced positions of X and X0 are respectively given by x and x0 , then, F being continuous, we have (in the matrixbased direct notation that is used throughout this chapter) x0 = x + F(X, t)u + o(u) as u → 0. Since a rigidbody displacement does not change distances between points,
Section 8.1 / LargeDeformation Continuum Mechanics
467
let us compare the distance between x and x0 with that between X and X0 : x0 − x =
q
=
q
=
q
(x0 − x)T (x0 − x) uT FT (X, t)F(X, t)u + o(u2 ) uT C(X, t)u + o(u),
def
where C = FT F is known, in the Noll–Truesdell terminology, as the right Cauchy–Green tensor . The notation will henceforth be simplified by writing F for F(X, t) and so on. The components of C are given by CIJ = χi ,I χi ,J , where (·),I = ∂(·)/∂XI . C is a Lagrangian tensor field which, moreover, is symmetric (C = CT ) and positive definite (uT Cu > 0 for any u 6= 0).
Stretch and Strain The stretch at (X, t) along a direction u is defined by χ(X + hu, t) − χ(X, t) = λu = lim h→0 hu
s
uT Cu . uT u
We have λu = 1 for every u if and only if C = I; then the displacement is locally a rigidbody displacement. If u(α) (α = 1, 2, 3) are the eigenvectors def of C and if λα = λu(α) , then the λ2α are the eigenvalues of C, and the λα def
1
(the principal stretches) are the eigenvalues of U = C 2 . A strain is a measure of how much a given displacement differs locally from a rigidbody displacement. In particular, a Lagrangian strain is a measure of how much C differs from I. The following Lagrangian strain tensors are commonly used: (a) the Green–SaintVenant strain tensor1 already mentioned in Section 1.2, E = 12 (C − I), with eigenvalues 21 (λ2α − 1); (b) the conventional strain tensor Ee = U − I, with eigenvalues λα − 1 (the principal conventional strains); and (c) the logarithmic strain tensor El = ln U, with eigenvalues ln λα (the principal logarithmic strains). Note that all three strains may be regarded as special cases of (1/k)(Uk − I), with (a), (b), and (c) corresponding respectively to k = 2, k = 1 and the limit as k → 0. Furthermore, 1 k 1 (λ − 1) = [(1 + λ − 1)k − 1] = λ − 1 + o(λ − 1), k k so that Ee El 1
)
= E + o(E),
Often called simply the Lagrangian strain tensor.
468
Chapter 8 / LargeDeformation Plasticity
where E denotes some measure of the magnitude (a norm) of E. In other words, the different Lagrangian strain tensors are approximately equal when they are sufficiently small. For large strains the Green–SaintVenant strain tensor is analytically the most convenient, except in cases where the principal directions u(α) are known a priori. Since U is symmetric and positive definite, we can form the twopoint tensor R = FU−1 . Note that RT R = U−1 FT FU−1 = U−1 U2 U−1 = I, that is, R is orthogonal. Also, det U = J, so that det R = J/J = 1, and consequently, R is a proper orthogonal tensor, or a rotation. The decomposition F = RU is the right polar decomposition of F, and U is called the right stretch tensor ; this is why C is called the right Cauchy–Green tensor. R is usually called simply the rotation tensor . If the displacement is locally a rigidbody one, then we simply have F = R. To study the general case, let us consider points near X given by X(α) = X + hu(α) , where u(α) is, as above, an eigenvector of C. The displaced images of these points are x(α) = x + hv(α) + o(h), where v(α) = Fu(α) = RUu(α) . Since, however, u(α) is also an eigenvector of U, it follows that Uu(α) = λα u(α) , and therefore v(α) = λα Ru(α) , so that R represents the rotation of the eigenvectors of C. For an arbitrary vector u, Uu is not in general parallel to u. In fact, if we consider the ellipsoid centered at X, given by uT Cu = r2 , with principal semiaxes r/λα , we see that its displaced image is approximately the sphere of radius r centered at x. The ellipsoid given by the preceding equation is called the reciprocal strain ellipsoid . We may also ask what is the effect of the displacement on the sphere of radius r, centered at X, in the reference configuration. If x + v is the displaced image of X + u, then v = dotFu, so that uT u = dotvT B−1 v (where B = FFT ), and vT B−1 v = r2 defines an ellipsoid centered at x with principal semiaxes λα r; this ellipsoid is called simply the strain ellipsoid . The tensor B−1 is called the Finger deformation tensor , while B is called
Section 8.1 / LargeDeformation Continuum Mechanics
469
(again in the terminology of Truesdell et al.) the left Cauchy–Green tensor . It is an “Eulerian” tensor, and its eigenvalues are also λ2α . Its name derives, as may be surmised, from the left polar decomposition of F (see Exercise 1). It can easily be shown that B = RCRT . The most commonly used “Eulerian” strain tensor is the Almansi strain tensor Ea = 21 (I − B−1 ). It is easy to show that E = FT Ea F, so that Ea = RU−1 EU−1 RT . Hence, in order for Ea to be approximately equal to E (i.e. to have Ea = E + o(E)), it is necessary not only for E but also for R − I to be small. In many treatments the right Cauchy–Green tensor C is given another definition, namely, as a metric tensor . If the Lagrangian coordinates XI are used to describe points in the displaced body, then they are no longer Cartesian coordinates, since the surfaces XI = constant are not necessarily planes. An infinitesimal vector dx in the displaced body has the square of its magnitude given by dx · dx = CIJ dXI dXJ . Hence C is often called the metric tensor in the displaced (strained) body. The identity I is accordingly regarded as the metric tensor in the unstrained body. The analysis of continuum deformation based on metric tensors is usually carried out by using curvilinear coordinates to begin with (see, e.g., Green and Zerna [1968], Eringen [1962], Marsden and Hughes [1983]). For our purposes, its main usefulness is in the derivation of compatibility conditions, that is, the finitedeformation analogue of Equation (1.2.4), and to that end Cartesian coordinates are adequate. The result is usually given as the vanishing of a fourthrank tensor called the Riemann–Christoffel tensor or the curvature tensor , being the necessary (locally also sufficient) condition for a symmetric positive definite tensor field C to be derivable from a configuration χ. It can be shown that the result is equivalent to the symmetric secondrank tensor equation eIKM eJLN [EKL ,M N − 12 CP−1Q (ELP ,M +EM P ,L −ELM ,P )(EKQ ,N +EN Q ,K −EKN ,Q )] = 0, (8.1.1) which can be seen to reduce to (1.2.4) for sufficiently small strains. A fundamental difference between the Lagrangian and the Eulerian deformation and strain tensors must be emphasized. The Lagrangian tensors transform according to the usual rules (Section 1.1) under a rotation of the Lagrangian basis, while they are invariant under a rotation of the Eulerian basis. To see the invariance, let (e∗i ) denote the rotated Eulerian basis, with e∗i = Qij ej , Q being orthogonal. Since x∗i = Qij xj , it follows that χ∗i (X, t) = Qij χj (X, t), and hence FiI∗ = Qij FjI . These relations may be written as x∗ = Qx, χ∗ (X, t) = Qχ(X, t), and F∗ = QF. Consequently, C∗ =
470
Chapter 8 / LargeDeformation Plasticity
FstarT F∗ = FT QT QF = C. Since the Eulerian basis is, in a sense, fixed in space, invariance under its rotation is related to the isotropy of space itself, and is invoked in the formulation of fundamental physical principles. Conversely, Eulerian tensors are invariant under a rotation of the Lagrangian basis; such a rotation may represent, for example, a rotation of the given body in space. This kind of invariance may, accordingly, be used to establish material isotropy — the fact that the mechanical response of a body does not depend on its orientation. Eulerian tensors transform according to the usual rules under a timeindependent rotation of the Eulerian basis; but only the ones called objective do so when the rotation is timedependent. The objectivity of tensors is discussed in 8.1.2.
Area and Volume Deformation Consider again a material point X and two neighboring points X0 = X + hu0 , X00 = X + hu00 , defined by two vectors u0 , u00 and a small real number h. The vector area of the triangle formed by the three points is 1 A0 = h2 u0 × u00 , 2 or, in components 1 A0I = h2 eIJK u0J u00K . 2 0 The displaced positions of X, X and X00 are x, x0 = x + hv0 + o(h) and x00 = x + hv00 + o(h), respectively, where v0 = Fu0 and v00 = Fu00 . The displaced area is 1 A = h2 v0 × v00 + o(h2 ) 2 or . Ai = 21 h2 eijk vj0 vk00 = 12 h2 eijk FjJ FkK u0J u00K = 41 h2 eijk (FjJ FkK − FjK FkJ )u0J u00K = 14 h2 eijk FjJ FkK (u0J u00K − u0K u00J ) = 41 h2 eijk FjJ FkK eIJK eILM u0L u00M =
1 2 eijk eIJK FjJ FkK
1 2 0 00 2 h eILM uL uM
−1 = (det F)FIi A0I .
In direct notation, A = JFT −1 A0 + o(A0 ). If, now, X000 = X + hu000 is a fourth point, then the volume of the tetrahedron in the reference configuration is V0 = 31 hA0 · u000 = 13 hAT0 u000 . Since the displaced position of X000 is x000 = X + hFu000 + o(h), the displaced volume is 1 V = hAT Fu000 + o(h3 ) = JV0 + o(V0 ). 3
Section 8.1 / LargeDeformation Continuum Mechanics
471
The Jacobian determinant is thus seen as having the important property of measuring the ratio between displaced and referential infinitesimal volumes, that is, dV =